Пожалуйста, ознакомьтесь с примечаниями транскриптора в конце этого текста.

Новое оригинальное оформление обложки, включенное в эту электронную книгу, является общественным достоянием.

ПОЛИТИЧЕСКАЯ И КОММЕРЧЕСКАЯ ГЕОЛОГИЯ И МИНЕРАЛЬНЫЕ РЕСУРСЫ МИРА

McGraw-Hill Book Co. Inc.

ИЗДАТЕЛИ КНИГ ДЛЯ

Coal Age ▽ Electric Railway Journal Electrical World ▽ Engineering News-Record American Machinist ▽ Ingeniería Internacional Engineering & Mining Journal ▽ Power Chemical & Metallurgical Engineering Electrical Merchandising

ПОЛИТИЧЕСКАЯ И КОММЕРЧЕСКАЯ ГЕОЛОГИЯ И МИНЕРАЛЬНЫЕ РЕСУРСЫ МИРА

СЕРИЯ ИССЛЕДОВАНИЙ СПЕЦИАЛИСТОВ

ДЖОЗАЙЯ ЭДВАРД СПУРР, редактор

Первое издание Второе издание

Авторские отчисления, полученные от продажи этой книги, будут переданы в образовательное учреждение для финансирования дальнейших исследований по направлениям, представленным в данном томе.

McGRAW-HILL BOOK COMPANY, Inc. НЬЮ-ЙОРК: 370 СЕВЕНТ-АВЕНЮ ЛОНДОН: 6 & 8 БОВЕРИ-СТРИТ, E. C. 4 1920

Авторское право, 1920 г., McGraw-Hill Book Company, Inc.

THE MAPLE PRESS YORK PA.

ПРЕДИСЛОВИЕ

Цель данной серии исследований — пролить свет на огромное значение коммерческого контроля над сырьевыми ресурсами со стороны различных держав или граждан этих держав посредством инвестированного капитала. Вопрос внутренней и внешней государственной политики Соединенных Штатов тесно связан с этим. Многим из нас, кто был занят (как и все авторы этих работ) изучением проблем минеральных ресурсов во время войны, казалось, что наше правительство никогда не осознавало огромного политического значения коммерческого доминирования, и особенно контроля над минеральными богатствами; в то время как другие, более опытные нации, осознали это и тем самым глубоко затронули интересы Америки и ее политику, причем сама Америка не осознавала этого обстоятельства.

С быстрым ростом населения мира, а также разведкой и эксплуатацией доселе нетронутых природных ресурсов конкуренция за это богатство стала и будет становиться еще более острой. В прошлые века война, эпидемии и голод сдерживали рост населения Земли; и за последние несколько лет все эти мрачные призраки вернулись в полной мере, что наводит на мысль о возможности постоянного возврата к старым первобытным временам. Тем не менее, современная наука и организация, если их не подавят масштабные социальные потрясения, будут защищать жизнь, как это было в недавнем прошлом, так что мир находится на пути к перенаселению. Все мы, подобно Германии, жаждем своего «места под солнцем» и своей доли комфорта и власти. Из всех фундаментальных потребностей для этого ничто не является в такой степени фиксированной и невосполнимой величиной, как металлы; они составляют базис и фундамент нашей современной цивилизации и власти над человеком и силами природы. Другие сырьевые ресурсы имеют растительное или животное происхождение; они размножаются и воспроизводят себя в последовательных воплощениях согласно закону жизни; они рождаются магическим образом из воздуха и воды, используя минимум земных недр, и верно возвращают свои долги воздуху, воде и земле с уходом каждого поколения и наступлением нового. В минеральном царстве есть намек на подобный закон роста, но он настолько медленный, что эфемерный человек не имеет к нему личного интереса; для всех его целей и по всем его стандартам измерения он инертен, и эти богатства, будучи однажды добытыми и использованными, никогда больше не будут доступны. Сокровища коммерчески ценных месторождений руд были причудливо спрятаны природой по всей земле, здесь и там, без какого-либо географического или широтно-долготного правила и с полным пренебрежением к равенству. Потребности или желания нации в минеральных богатствах не имеют установленной связи с ее фактическими минеральными запасами; то, что ей нужно, часто находится на территории другой нации, которая в этом не нуждается. Так рождается торговля, и нация, которая должна обладать соответствующим металлом или рудой, поддерживает свою торговлю и помогает ей закрепить свои претензии на постоянный контроль над соответствующими месторождениями посредством законодательства, дипломатии и, если потребуется, войны. В случае войны металлический приз достается сильнейшему — обычно той нации, которая ранее, в силу своих потребностей, осуществляла лишь коммерческий контроль, но которая в результате испытания силой теперь откровенно заявляет о своем суверенитете.

Осознали ли мы, американцы, эти силы? Безусловно, нет, я бы сказал. Многие ли осознают, что вопрос Эльзас-Лотарингии не является и не был сентиментальным, а представлял собой борьбу за крупнейшие месторождения железа в Европе и вторые по величине в мире, которые дали Германии ее огромный рост и мощь и теперь могут передать это богатство и мощь Франции? Что спор между Польшей и Германией по поводу Верхней Силезии — это не вопрос национальности, чувств или даже территории, а касается крупнейшего угольного бассейна Европы, а также крупных месторождений свинца и цинка? Если Польша получит это, она может соперничать с Германией в богатстве и значимости; если Германия потеряет это, она может опуститься до положения второстепенной державы, теперь, когда ей также пришлось отдать Эльзас-Лотарингию. Выносить такой вопрос на голосование местного населения — это все равно что подбрасывать монету; но многие ли из нас поняли это? Население перемещается и меняется, растет или сокращается, может быть в одно время преимущественно польским, а в другое — преимущественно немецким; но угольные месторождения неизменны. Чтобы прояснить эти вещи, нам следовало бы вместо «Силезии» говорить «Уголь», вместо «Эльзас-Лотарингии» — «Железо» и так далее.

Причина, по которой мы не осознали эти факты, заключается в нашем собственном огромном минеральном богатстве, настолько обильном, что лишь недавно американский капитал и предпринимательство сочли необходимым отправиться во внешний мир, как это давно сделали европейские нации. Их природные богатства были ограничены, поэтому они стали знакомы с теми фундаментальными принципами и законами, о которых мы не подозревали. Из этого возникла европейская внешняя политика, защита их национальной торговли и национального капитала в зарубежных предприятиях и, следовательно, дома; государственное участие в деловых объединениях, как в Германии, Англии, Франции и Италии; в то время как Соединенные Штаты были заняты «борьбой с трестами» и пренебрегали защитой своих инвесторов в зарубежных странах. Это иллюстрирует разницу между европейской дипломатией и американской наивностью. Насколько хорошо это сыграло на руку иностранным державам, объяснять не нужно. Зрелище того, как Соединенные Штаты поддерживают доктрину Монро о защите латиноамериканских республик, с которыми они не предприняли решительных шагов для объединения мощными узами торговли, должно было вызвать насмешку у тех европейских коммерческих наций, таких как Германия, которые укрепляли себя в этих странах посредством теснейших коммерческих, а следовательно, и политических связей.

Этот том просто берет на себя изучение реальной ситуации в отношении распределения и владения минеральными ресурсами в мире, и автором каждой главы является известный специалист.

Сначала рассматривается вопрос о нефти, источнике энергии и света, ключе к господству в воздухе, которая, благодаря своему жидкому и легко транспортируемому состоянию, имеет чрезвычайное значение в будущем. Далее рассматриваются великий топливный минерал — уголь, и его союзник — великий металлический минерал — железо, которые должны использоваться вместе для производства железа и стали, основы всех наших механических достижений. Затем следуют те металлы, которые незаменимы в сталеплавильном производстве и при изготовлении особо твердых или прочных сталей. Они имеют большое значение и включают марганец, хром, никель, вольфрам, ванадий, сурьму, молибден, уран и цирконий. Радий тесно связан с ураном и рассматривается вместе с ним. Тесно связаны с цирконием торий и мезоторий, и поэтому их рассмотрение следует непосредственно за цирконием.

Следующая большая группа — это основные металлы, помимо железа и ферросплавных металлов: медь, свинец, цинк, олово, ртуть и алюминий. Руды алюминия используются не только как источники металла, но и для производства огнеупорных материалов и абразивов. Поэтому они классифицируются частично как металлические, а частично как неметаллические минералы; и далее следуют другие неметаллические минералы, используемые также для абразивов, огнеупорных материалов и других целей — такие минералы, как наждак и корунд, магнезит, графит, слюда и асбест.

Следующая большая группа — это минеральные удобрения: фосфатные породы, калий, нитраты и азот, а также пирит и сера, все из которых необходимы для сельского хозяйства.

Последняя группа — это драгоценные металлы: золото, серебро и платина, необходимые для чеканки монет и в искусстве.

Эти различные исследования по сути являются одновременно исчерпывающими и элементарными: вместе они составляют почти первый вклад в ту область исследований — связь геологии с промышленностью, торговлей и политической экономией, — которую они охватывают; и естественно, что начинания должны быть довольно грубыми. Более того, многие главы были написаны за год или более до публикации тома, и хотя они были обновлены настолько, насколько это было возможно за короткое время, сами авторы считают их недостаточно полными. Поэтому извинения за недостатки и возможные неточности вполне уместны. Тем не менее, считается, что том заслуживает публикации и что сделанное здесь начало гораздо лучше, чем полное отсутствие такового.

Джозайя Эдвард Спурр.

CONTENTS

| Page
| Preface | v
Chapter |
I. | Petroleum, by John D. Northrop | 1
II. | Coal, by George S. Rice and Frank F. Grout | 22
III. | Iron, by E. C. Harder and F. T. Eddingfield | 55
IV. | Manganese, by D. F. Hewett | 90
V. | Chromium, by E. C. Harder | 109
VI. | Nickel, by C. S. Corbett | 129
VII. | Tungsten, by Frank L. Hess | 142
VIII. | Vanadium, by R. B. Moore | 163
IX. | Antimony, by H. G. Ferguson and D. A. Hall | 172
X. | Molybdenum, by R. B. Moore | 191
XI. | Radium and Uranium, by R. A. F. Penrose, Jr. | 201
XII. | Zirconium, by H. C. Morris | 209
XIII. | Monazite, Thorium, and Mesothorium, by R. B. Moore | 216
XIV. | Copper, by F. W. Paine | 223
XV. | Lead, by Frederick B. Hyder | 261
XVI. | Zinc, by Frederick B. Hyder | 294
XVII. | Tin, by James M. Hill | 317
XVIII. | Mercury, by F. L. Ransome | 337
XIX. | Bauxite and Aluminum, by James M. Hill | 349
XX. | Emery and Corundum, by Frank J. Katz | 356
XXI. | Magnesite, by R. W. Stone | 363
XXII. | Graphite, by H. G. Ferguson, Frank F. Grout, and George D. Dub | 372
XXIII. | Mica, by Durand A. Hall | 380
XXIV. | Asbestos, by Oliver Bowles | 388
XXV. | Phosphate Rock, by R. W. Stone | 402
XXVI. | Potash, by Hoyt S. Gale and A. W. Stockett | 411
XXVII. | Nitrogen, by Chester G. Gilbert | 421
XXVIII. | Pyrite and Sulphur, by A. G. White | 447
XXIX. | Gold, by John E. Orchard | 462
XXX. | Silver, by F. W. Paine | 495
XXXI. | Platinum, by James M. Hill | 506
XXXII. | Who Owns the Earth? by J. E. Spurr | 522

ПОЛИТИЧЕСКАЯ И КОММЕРЧЕСКАЯ ГЕОЛОГИЯ И МИНЕРАЛЬНЫЕ РЕСУРСЫ МИРА

ГЛАВА I НЕФТЬ Автор: Джон Д. Нортроп [1]

[1] В эту статью, подготовленную в июне 1918 года г-ном Нортропом, были включены определенные примечания и дополнения; например, информация, предоставленная Э. Расселом Ллойдом из Геологической службы США; А. Г. Уайтом и У. Э. Пердью из Бюро горной промышленности и другими. (Дж. Э. С.)

ВВЕДЕНИЕ Автор: Дж. Э. Спурр

Уголь и железо являются основой промышленной цивилизации, и их следует рассматривать в первую очередь при любой попытке проанализировать владение и контроль между нациями над мировыми минеральными ресурсами. Однако родственным углю по растущему значению является более легкое, жидкое и летучее минеральное вещество — нефть, значение которой огромно и до сих пор не полностью определено. Будучи более легко транспортируемой, чем уголь, и дающей рафинированные продукты, взрывное действие которых в двигателях внутреннего сгорания обеспечивает большую мощность по отношению к весу, чем когда-то считалось возможным, нефть и ее продукты, помимо их огромного прямого экономического значения, могут в автомобилях, подводных лодках и самолетах, а также благодаря многочисленным другим применениям, стратегически контролировать, с националистической точки зрения, более инертные основы цивилизации. Более того, использование сырой нефти в качестве топлива, особенно для судов, имеет жизненно важное значение в наши дни, когда существуют масштабные конкурентные планы по расширению мировой торговли и установлению силы и готовности военно-морских флотов. Великие морские державы должны иметь для своих нефтетопливных судов бункеровочные станции под собственным контролем во всех частях мира, где они хотят, чтобы их торговля доминировала, а их военно-морские силы эффективно защищали их интересы.

Признание некоторыми сильными и агрессивными национальностями этого критического фактора привело к ситуации, которая, возможно, не имеет аналогов в минеральной истории мира. Уголь и железо всегда были решительно статичными в плане контроля — они оставались в значительной степени под надзором и руководством стран, в которых они встречаются. Транспортные расходы, сочетание месторождений железа и угля и другие факторы препятствовали тому, чтобы эти минералы, несмотря на их огромное значение, полностью использовались как мировой товар. Напротив, нефть становится универсальной, подобно золоту, в своем признании и применимости; но, в отличие от золота, она в высшей степени необходима для прогресса современной цивилизации. Текучесть этого минерала, его следствием является удивительно дешевая транспортировка и обработка по трубопроводам, полнота, с которой он может быть использован, — все это в совокупности делает его в будущем решающим фактором коммерческого и политического контроля. Более того, эта текучесть формы и легкость применения облегчают контроль над нефтью со стороны крупных коммерческих организаций, таких как Standard Oil of America и других в различных частях мира; и даже делают ее мировой контроль осуществимым и вероятным. Признавая эту тенденцию, многие нации, такие как Англия, Франция, Голландия, Аргентина и Мексика, предприняли шаги, направленные на частичную национализацию своих нефтяных ресурсов, чтобы защитить себя от иностранной коммерческой агрессии в этом отношении. Англия зашла дальше всех в этом направлении и достигла, и агрессивно стремится в другие страны, чтобы обеспечить, посредством коммерческого контроля, подкрепленного там, где необходимо, политическим давлением, мировую империю нефти, чтобы служить ее всемирной колониальной империи. Соединенные Штаты, с другой стороны, доминировали в мировой нефтяной промышленности благодаря своим собственным огромным ресурсам, разрабатываемым интересами, которые выросли без сознательной государственной помощи или даже вопреки государственной и народной оппозиции, и достигли и обеспечили себе плацдармы в других странах.

В прошлом развитие минеральных ресурсов мира приводило к большим изменениям в политическом суверенитете. Важными, как они были, события, которые могут возникнуть в результате националистической конкурентной эксплуатации и контроля над мировыми запасами нефти, обещают превзойти по значимости все подобные изменения прошлого. Восприятие проблемы и необходимости, а также преимущество инициативы, естественно, принадлежат тем нациям с ограниченной территорией и ресурсами, которые стали великими благодаря торговле и эксплуатации ресурсов других стран. Такой нацией, например, является Англия, страна, которая, к счастью, является естественным союзником Соединенных Штатов. Напротив, в Соединенных Штатах, нации, до сих пор озабоченной только развитием своих собственных огромных ресурсов, коммерческое предпринимательство в зарубежных странах не было подкреплено никакой фиксированной национальной политикой, и, действительно, часто рассматривалось как недостойное. В новой международной эре, которая была инициирована Мировой войной, однако, эта политика китайской самодостаточности и изоляции не может безопасно продолжаться, и Соединенные Штаты должны не только ясно осознавать тенденции и движения других национальностей, но и рассмотреть, как лучше направить свои собственные коммерческие и политические планы, чтобы поддержать свою независимость и мощь. Такая политика естественно привела бы к международным соглашениям относительно распределения и раздела нефтяных земель, ресурсов и добычи, и, вероятно, ничто другое не способствовало бы больше продвижению откровенного понимания между нациями и устранению препятствий на пути к постоянному миру.

Далее следует статья г-на Нортропа:

ИСПОЛЬЗОВАНИЕ НЕФТИ

В своем сыром или полурафинированном состоянии нефть широко используется в качестве топлива под локомотивными и морскими котлами и в небольшой степени в двигателях внутреннего сгорания дизельного типа. Определенные сорта нефти используются в сыром состоянии в качестве смазочных материалов.

Основное использование нефти — для производства рафинированных продуктов, число и применение которых легион. Продукты самой легкой плотности, эфирные, используются в качестве анестетиков в хирургии. Бензины являются универсальным топливом для двигателей внутреннего сгорания, а нафты широко используются в качестве растворителей и для смешивания с сырым газовым бензином при производстве коммерческого бензина. Группа керосина включает в себя множество продуктов, используемых в первую очередь в качестве осветительных средств, но во все возрастающих количествах — в качестве топлива для сельскохозяйственных тракторов. Смазочные масла и консистентные смазки, полученные из нефти, незаменимы для работы всех типов машин. Воски, полученные из нефти парафинового основания, используются во многих формах в качестве консервантов и источников освещения, а за последние три года стали незаменимыми компонентами хирургических повязок при лечении ожогов. Нефтяной кокс из-за своей чистоты пользуется спросом для использования в определенных металлургических процессах и для производства аккумуляторных углей и электродов для дуговых ламп. Топливные масла, полученные как побочные продукты нефтепереработки, удовлетворяют топливные потребности многих промышленных предприятий, железных дорог и океанских пароходов. Дорожные масла, как следует из названия, используются для уменьшения пыли на улицах и шоссе; а искусственный асфальт, продукт определенных типов нефти, во многих местностях вытеснил использование других форм асфальта для дорожных покрытий.

Заменители.

— Для нефти в качестве топлива под котлами для выработки пара существует множество заменителей, включая дерево, древесный уголь, уголь, торф, природный газ, искусственный газ и электричество; в качестве топлива в двигателях внутреннего сгорания некоторыми продемонстрированными заменителями являются природный газ, искусственный газ, бензол и спирт, а в двигателях дизельного типа могут быть использованы определенные растительные и рыбьи жиры.

Для осветительных целей в качестве заменителей керосина могут использоваться животные жиры, масла, дистиллированные из угля, природный газ, искусственный газ, ацетиленовый газ и электричество.

Для определенных типов смазки приемлемы тщательно очищенные растительные и минеральные масла, но для смазки высокоскоростных подшипников и для всей смазки в условиях высокой температуры и пара удовлетворительных заменителей минеральных смазочных материалов, полученных из нефти, не известно.

Заменители нефтяного асфальта доступны в форме природных асфальтов, битуминозных пород и остатков каменноугольной смолы. Для вазелина можно использовать животные жиры и растительные масла, а для парафинового воска озокерит мог бы удовлетворить такие существенные требования, которые не могли быть удовлетворены охлаждением или растительными и животными маслами.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Вероятные изменения в практике, которые, как ожидается, повлияют на нефтяную промышленность в течение следующих десяти лет, включают повышенную зависимость производителей нефти от геологических исследований перед бурением, разработку методов более глубокого бурения, чем это практически возможно сейчас, и более эффективное управление отдельными скважинами и целыми объектами с целью максимального извлечения при минимальных затратах более высокого процента нефти, изначально присутствующей в недрах.

Тенденция к объединению отдельных добывающих, транспортных, перерабатывающих и маркетинговых интересов в сильные единицы, способные конкурировать на внутренних и внешних рынках на относительно равных условиях друг с другом и с уже существующими объединениями эквивалентной силы, несомненно, будет усиливаться, и с растущей силой отдельных единиц придет эффективный и тщательный поиск нефти во всех частях мира.

В нефтепереработке вероятно, что будут разработаны и усовершенствованы методы извлечения большего количества легких продуктов из низкосортной нефти и преобразования менее продаваемых продуктов нефти в продукты наибольшего текущего спроса. Более того, считается, что двигатели внутреннего сгорания будут модифицированы таким образом, чтобы успешно работать на нефтепродуктах с меньшей летучестью, чем бензин. Использование нефти в качестве железнодорожного, морского и промышленного топлива суждено колоссально увеличиться в следующем десятилетии.

Хотя сланцево-нефтяная промышленность является важным вкладчиком в поставки нефти Великобритании, в последние годы она мало привлекала внимания за пределами Шотландии. Исследования Геологической службы США показали, что Соединенные Штаты содержат огромные месторождения горючих сланцев в Юте, Колорадо, Вайоминге и Неваде, многие из которых в среднем имеют более высокое содержание нефти, чем шотландские сланцы. Усилия, уже начатые по разработке методов извлечения сланцевой нефти в коммерческих масштабах в Соединенных Штатах, несомненно, приведут к созданию сланцево-нефтяной промышленности в этой стране в течение следующих двух или трех лет. Будущий рост этой отрасли будет в значительной степени зависеть от скорости снижения внутренней добычи нефти.

ГЕОЛОГИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Коммерческие скопления нефти повсеместно ограничены пластами осадочного происхождения. В Соединенных Штатах нефть добывается в коммерческих целях из пластов всех периодов от кембрия до четвертичного, причем наиболее продуктивными источниками являются пласты каменноугольной и третичной систем. Геологический возраст основных источников добычи нефти в каждой из других нефтедобывающих стран мира указан в следующей таблице:

Таблица 1. — Геологический возраст нефтеносных формаций

Country | System
North America
Canada | Silurian and Devonian
Mexico | Cretaceous and basal Tertiary
Alaska | Tertiary (?)
West Indies
Trinidad | Tertiary
Cuba | Cretaceous and pre-Cretaceous
South America
Colombia | Cretaceous and Tertiary
Venezuela | Cretaceous and Tertiary
Peru | Tertiary
Argentina | Jurassic, Cretaceous and Tertiary
Europe
Russia | Tertiary
Roumania | Tertiary
Galicia | Tertiary
Italy | Tertiary
Germany (Alsace) | Tertiary and pre-Tertiary
Asia
India | Tertiary
Turkestan | Tertiary
Persia | Tertiary
Africa
Algeria | Tertiary
Egypt | Tertiary
Oceania
Japan | Tertiary
Dutch East Indies | Tertiary
New Zealand | Cretaceous and Tertiary

Из вышеприведенной таблицы можно сделать вывод, что существует прямая связь между распределением третичных пород и запасами нефти, но в Соединенных Штатах, которые производят две трети текущих мировых запасов, поиск нефти под научным руководством охватил весь диапазон стратиграфической колонки и обнаружил нефть в значительных количествах в породах каждой геологической системы моложе кембрия.

Тот факт, что выходы нефти и другие поверхностные признаки нефти, как правило, более выражены в относительно более молодых мезозойских пластах, чем в более старых палеозойских формациях, и дальнейший факт, что геологическая разведка нефти и газа в странах, отличных от Соединенных Штатов, была ограничена в основном районами, содержащими наиболее выраженные признаки нефти, способствуют объяснению преобладания третичной системы в вышеприведенной таблице и указывают на ошибочность попыток оценить мировые запасы нефти только на основе стратиграфических данных.

Несмотря на широкий геологический диапазон нефти, ее наличие в конкретных пластах, формациях, группах, сериях или системах отнюдь не является универсальным. Напротив, ее наличие ограничено конкретными местностями, в которых выполняются определенные переменные отношения, до сих пор мало изученные, которые включают (1) состав, последовательность и содержание органического вещества в осадках; (2) природу и степень метаморфизма, которому они подверглись; (3) их структуру; и (4) степень их насыщения соленой водой. Поскольку наиболее детальной геологической работы недостаточно для обеспечения основы для соответствующей оценки многочисленных вовлеченных факторов, и поскольку только относительно небольшой процент площадей осадочных пород в мире был изучен геологически в значительных деталях, любая оценка будущих поставок нефти в мире является особенно рискованной.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Географическое распределение нефти относительно так же широко, как и ее геологический диапазон. Нефтяные месторождения, имеющие в настоящее время коммерческое значение, расположены, в порядке их важности как вкладчиков в мировую добычу нефти в 1917 году, в Соединенных Штатах, России, Галиции, Мексике, Голландской Ост-Индии, Индии, Персии, Японии и Формозе, Румынии, Перу, Тринидаде, Аргентине, Египте, Германии, Канаде, Венесуэле и Италии. Небольшие количества нефти также были зарегистрированы в Гватемале, Гондурасе, Коста-Рике, Панаме, Гаити, Пуэрто-Рико, Боливии, Чили, Испании, Аравии, Китае, Австралии, Папуа, Филиппинских островах, Нигерии, Бельгийском Конго, Золотом Береге, Мадагаскаре и других местах. Географическое распределение нефти в мире показано на прилагаемой карте. (Таблица I.)

Таблица I. — Географическое распределение добывающих нефтяных месторождений мира. Автор: Джон Д. Нортроп.

По мнению автора, наиболее заметное развитие мировых запасов нефти в следующем десятилетии произойдет в странах, граничащих с Карибским морем и Мексиканским заливом. Тенденция в этом направлении безошибочна. С 1913 по 1917 год годовая добыча нефти в Мексике увеличилась с 21 000 000 баррелей до 56 000 000 баррелей, и потенциал будущей добычи в этой стране оказался почти непостижимым. Продукция, изначально считавшаяся ценной только как источник мазута, теперь дает, благодаря современным методам переработки, все более важные проценты осветительных масел и бензина. Единственными препятствиями для колоссально увеличенной добычи являются нестабильные политические условия и неадекватные средства морского транспорта. Эти препятствия, несомненно, будут преодолены в течение следующих нескольких лет, и, если не произойдет непредвиденных обстоятельств, Мексика вскоре займет второе место среди нефтедобывающих стран мира. [2] Судя по результатам разведочных работ, уже проведенных в Венесуэле и Колумбии, обе эти страны суждено внести заметный вклад в мировые поставки нефти в течение следующего десятилетия. Недавно Колумбия предоставила достаточно доказательств способности поставлять высококачественную нефть из скважин большой индивидуальной мощности, чтобы оправдать усилия крупных интересов, владеющих там концессиями, по преодолению неблагоприятных природных условий, которые так долго преграждали путь к эксплуатации. В Венесуэле уже проведено достаточно буровых работ, чтобы доказать, что ресурсы тяжелой нефти с асфальтовым основанием в этой стране велики, а недавняя установка современного нефтеперерабатывающего завода для обработки этих масел на острове Кюрасао, у побережья Венесуэлы, обеспечила рынок, необходимый для активного освоения месторождений.

[2] Мексика занимала второе место в 1918 и 1919 годах.

На Тринидаде добыча нефти превышает 1 500 000 баррелей в год и удвоилась за последние несколько лет. С увеличением возможностей для океанской транспортировки нефти, которые становятся доступными, обеспечен большой объем добычи.

Не ожидается, что Куба станет важным производителем нефти, и нынешние знания о нефтяных ресурсах стран Центральной Америки не таковы, чтобы оправдать веру в то, что нефтяные месторождения существенного значения будут развиты в какой-либо из них.

Ожидается, что добыча нефти в Соединенных Штатах достигнет своего максимума в течение следующих двух или трех лет и будет неуклонно снижаться после этого, хотя ожидается, что эта страна останется ведущей нефтедобывающей страной мира на большую часть, если не на все, предстоящее десятилетие.

Что касается тех нефтедобывающих стран Северной и Южной Америки, которые еще не были упомянуты, никаких существенных изменений в их нынешнем статусе не ожидается.

Считается, что нефтяные ресурсы России (включая Азиатскую Россию) достаточны, чтобы гарантировать сохранение этой страной позиции ведущего производителя нефти в Восточном полушарии далеко за пределами следующего десятилетия. В течение последних нескольких лет добыча велась во все более сложных условиях, и, как следствие, не было никакой меры ни текущей производственной мощности, ни потенциала. Относительно будущего России как источника нефти Арнольд [3] говорит: «Такие обширные территории, как в Европейской, так и в Азиатской России, дают безошибочные доказательства наличия нефти в больших количествах, что именно на эту страну, среди стран Европы и Азии, будущее должно смотреть в поисках поставок».

[3] Арнольд, Ральф: «Мировые поставки нефти»: Отчет Американского горного конгресса, 19-я ежегодная сессия, 1917 г., стр. 485-486.

Поскольку Россия наделена нефтяными запасами, как доказанными, так и перспективными, огромной величины, окончательная позиция этой страны как ведущего нефтепроизводителя мира кажется разумно обеспеченной. Ее ближайшее будущее слишком тесно зависит от прогресса выхода из политической суматохи, чтобы гарантировать прогноз.

Считается, что нефтяные месторождения как Румынии, так и Галиции прошли свой максимальный выход, и возможности открытия новых месторождений существенного значения в этих странах не считаются достаточно большими, чтобы оправдать прогноз чего-либо, кроме умеренного снижения добычи в будущие годы. Никаких существенных изменений в статусе незначительных нефтяных месторождений Италии или Эльзаса не ожидается в какое-либо время в будущем.

Что касается ситуации в Азии, автор полагает, что следующее десятилетие станет свидетелем устойчивого роста добычи нефти в Индии и вероятного развития одного или нескольких важных нефтяных месторождений в Персии и, возможно, месторождений в Малой Азии, Туркестане и Китае. В Океании тот же период, несомненно, станет свидетелем существенного увеличения добычи нефти в Японии и на Формозе, а также в Голландской Ост-Индии, вместе с возможным открытием новых месторождений в Папуа. Африка, несомненно, получит значительное внимание со стороны нефтяных операторов в следующие десять лет, но на основе имеющихся доказательств результаты, полученные в этот период, вероятно, не будут достаточно большими, чтобы повлиять на нефтяную ситуацию в мире.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ ДОБЫЧИ

Статус политического контроля над мировым объемом добычи нефти в 1917 году, определенный по лучшим имеющимся на данный момент данным, указан в следующей таблице.

Прилагаемая диаграмма (Рисунок 1) показывает долю мировой добычи нефти, вносимую ежегодно каждой из основных добывающих стран в каждый из последних десяти лет.

Таблица 2. — Политический контроль над мировой добычей нефти в 1917 году

Source
of production
Quantity of
production
(barrels)
Percentage
of total
Country
exercising
political
control

United States | 335,315,601 |  66.17 | United States
Russia |  69,000,000 |  13.62 | Russia
Mexico |  55,292,770 |  10.91 | Mexico
Dutch East Indies |  12,928,955 |   2.55 | Holland
India | 8,078,843 |   1.59 | Great Britain
Persia |   6,856,063 |   1.36 | Persia
Galicia |   5,965,447 |   1.18 | Poland (?)
Japan and Formosa |   2,898,654 |   0.57 | Japan
Roumania |   2,681,870 |   0.55 | Roumania
Peru |   2,533,417 |   0.50 | Peru
Trinidad |   1,599,455 |   0.32 | Great Britain
Argentina |   1,144,737 |   0.23 | Argentina
Egypt |   1,008,750 |   0.20 | Great Britain
Germany |     995,764 |   0.20 | Germany
Canada |     205,332 |   0.04 | Great Britain
Venezuela |     127,743 |   0.03 | Venezuela
Italy |      50,334 |   0.01 | Italy
Cuba |      19,167 | ... | Cuba
| 506,702,902 | 100.00 |

Рис. 1. — Доля мирового объема добычи нефти, вносимая ежегодно каждой из главных добывающих стран, 1908-1917 гг.

Помимо контроля, осуществляемого Великобританией через ее протекторатные отношения над нефтяными ресурсами Египта, контроль над нефтяными ресурсами различных стран осуществляется главным образом в силу государственного суверенитета. Этот политический контроль пропорционален силе правительства в стране, осуществляющей его. Недавние события, в результате которых британское правительство становится мажоритарным акционером корпорации, контролирующей нефтяные ресурсы Персии, практически передают политический контроль, а также коммерческий контроль над персидской нефтью от Персии к Англии. Недавний предпринятый Мексикой твердый политический контроль над ее огромными нефтяными ресурсами зависит для своего успеха от ее дипломатической способности в отношениях с более сильными правительствами Англии и Соединенных Штатов, чьи граждане приобрели коммерческий контроль, которому угрожает новая и решительная националистическая политика Мексики.

КОММЕРЧЕСКИЙ КОНТРОЛЬ ДОБЫЧИ

Коммерческий контроль над мировой добычей нефти, насколько вовлечены нации, определяется в основном посредством прямого владения землями, арендой и концессиями или посредством контроля через холдинговые корпорации дочерних компаний, владеющих правами собственности, арендой, правами на недра или концессиями на нефтяные земли. За исключением Аргентины, где внутренняя нефтяная промышленность принадлежит государству и управляется им; Германии, где правительство участвует непосредственно в финансировании нефтяных предприятий через Deutsche Bank; и Персии, где британское правительство владеет существенной долей в компании, владеющей и управляющей обширными концессиями, коммерческий контроль над нефтяной промышленностью определяется почти полностью объединениями частного капитала, действующими в своих собственных интересах.

Таблица 3. — Национальность и степень контроля доминирующего интереса

Country
Production
in 1917
(barrels)
Nationality
of dominant
interests
Approximate
extent of
control by
dominant
interests
(per cent.)

United States | 335,315,601 | United States |  96 |
Russia | 69,000,000 | British-Dutch |  40 | +
Mexico | 55,292,770 | United States |  65 |
Dutch East Indies | 12,928,955 | British-Dutch | 100
India |  6,078,843 | British | 100
Persia |  6,856,063 | British | 100
Galicia |  5,965,447 | German | 100
Japan and Formosa |  2,898,654 | Japanese | 100
Roumania |  2,681,870 | British-Dutch |  36
Peru |  2,533,417 | United States |  70
Trinidad |  1,599,455 | British |  80
Argentina |  1,144,737 | Argentinian | 100
Egypt |  1,008,750 | British-Dutch | 100
Germany and Alsace |   995,746 | German | 100
Canada |   205,332 | United States[4] |  80 | -
Venezuela |   127,743 | British-Dutch |  80 | (?)
Italy |    50,000 | French |  96 |

[4] Через контроль над перерабатывающими мощностями.

Насколько известно автору, Канада является единственной страной, в которой нефтяная промышленность может считаться контролируемой иностранными (США) интересами, причем этот контроль осуществляется в силу существенной монополии на трубопроводные и перерабатывающие мощности.

Предыдущая таблица показывает, согласно лучшей имеющейся информации, национальность и приблизительную степень контроля, осуществляемого доминирующим интересом в каждой из основных нефтедобывающих стран мира в 1917 году.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ РЕСУРСОВ

Прилагаемая диаграмма (Рисунок 2) графически показывает приблизительный коммерческий контроль над мировой добычей нефти в 1917 году.

Рис. 2. — Приблизительный коммерческий контроль над мировой добычей нефти в 1917 году.

Коммерческий контроль над нефтяной промышленностью в Соединенных Штатах находится в руках так называемой «группы компаний Standard Oil» через их контроль над большинством крупных трубопроводных систем страны, вероятно, 75 процентами перерабатывающих мощностей и существенной частью фактической добычи. Другие внутренние интересы, имеющие важные доли в контроле над нефтяной промышленностью в Соединенных Штатах, включают Southern Pacific Railroad Co., Cities Service Co. (интересы Доэрти), General Petroleum Corporation, Gulf Oil Corporation, Ohio Cities Gas Co., Cosden & Co., Sinclair Oil & Refining Corporation, The Sun Co., the Texas Co., the Tide Water Oil Co. и Union Oil Co. Иностранные интересы в Соединенных Штатах включают чисто британские компании, которые контролируют добычу около 2 000 000 баррелей в год; британско-голландские компании, представленные синдикатом Royal Dutch-Shell, которые контролируют добычу около 9 000 000 баррелей в год, вместе с перерабатывающими и маркетинговыми мощностями; и франко-бельгийские компании, контролирующие годовую добычу около 1 000 000 баррелей. Помимо очень вероятного владения отдельными немцами акциями компаний, занятых в одной или нескольких фазах нефтяной промышленности Соединенных Штатов, автору не известно об организованном немецком интересе в какой-либо фазе внутренней промышленности.

Коммерческий контроль над нефтяной промышленностью России в условиях, существующих сейчас в Центральной Европе, в значительной степени является предметом спекуляций. Насколько удалось установить, доминирующий контроль находится в руках чисто британских, франко-британских и британско-голландских (синдикат Royal Dutch-Shell) интересов. Некоторые из вторых названных интересов тесно связаны с дополнительной группой капиталистов, представленной фирмой Nobel Bros., имеющей большое значение, текущий контроль над которой отнюдь не ясен из литературы, доступной по этому вопросу. Хотя изначально шведские, финансовые интересы, вовлеченные сейчас в Nobel Bros., как полагают, включают представителей финансовых групп в Англии, Франции и Германии, причем контроль, вероятно, находится у англо-шведских интересов. До войны прямой немецкий интерес в российской нефти включал контроль через Deutsche Bank через бельгийскую компанию (Petrole de Grosny) важной добывающей и перерабатывающей компании A. I. Akverdoff & Co., контроль над которой сейчас находится в британских или британско-голландских руках. Как и в Соединенных Штатах, значительная часть фактической добычи нефти в России распределена между большим количеством индивидуально слабых компаний, доминируемых через контроль над трубопроводными или перерабатывающими мощностями одной или другой из основных групп.

Значительное значение в российских нефтяных делах в свое время имел Европейский нефтяной союз, организованный для борьбы на мировых рынках с трестом Standard Oil. Этот союз включал, среди прочих, таких важных нефтяных операторов, как Nobel Bros., интересы Ротшильдов (сейчас Dutch-Shell), Mantaschoff (сейчас Russian General Oil Corporation) (британская) и Deutsche Bank, последний из которых контролировал Akverdoff и Spies в России, вместе с важными компаниями в Румынии и Галиции. Насколько этот союз контролировал дела своих компаний-членов, не очевидно из имеющихся данных, и его текущее влияние на компании, работающие сейчас в России, неопределенно.

Условия в России делают невозможным любое определенное заявление о нефтяной ситуации. Декрет правительства большевиков от 20 июня 1918 года о национализации нефтяной промышленности объявил собственностью государства все движимое и недвижимое имущество, используемое в этой промышленности и принадлежащее ей. Торговля нефтью была объявлена государственной монополией и была делегирована главному нефтяному комитету топливного отдела Высшего совета народного хозяйства. Поскольку основные районы добычи сейчас находятся под британским военным контролем, этот декрет неэффективен.

Коммерческий контроль над нефтью в Мексике разделен между интересами Соединенных Штатов, британскими и британско-голландскими интересами, которые контролировали около 65, 30 и 2 процентов, соответственно, добычи в 1917 году. Интересы Соединенных Штатов включают группу Доэни, работающую главным образом как компании Huasteca и Mexican Petroleum; Standard Oil Co. of New Jersey, работающую как Penn-Mex Fuel Co.; интересы Sinclair, работающие как Freeport and Mexican Fuel Oil Co.; Texas Co.; Gulf Co.; Southern Pacific Railroad; и другие. Британские интересы представлены Пирсонами, работающими как Mexican Eagle Oil Co.; а британско-голландские интересы — La Corona Petroleum Co. и Chijoles Oil, Ltd., контролируемыми синдикатом Royal Dutch-Shell. Не известно, чтобы исключительно немецкие интересы владели существенной частью какой-либо важной компании, работающей в Мексике.

Ранее концессии свободно предоставлялись иностранным лицам и компаниям для эксплуатации месторождений полезных ископаемых, а нефтяные земли продавались местными владельцами иностранцам. Статья 27 конституции 1917 года прямо запрещает кому-либо, кроме мексиканских компаний, приобретать напрямую или эксплуатировать напрямую нефтяные земли в Мексике.

Все недавние концессии на эксплуатацию нефтяных объектов содержат положение, гласящее, что концессия будет объявлена недействительной, если какие-либо права будут переданы какому-либо иностранному правительству. Положения и намерение серии президентских декретов, изданных 19 февраля 1918 года, 8 июля 1918 года, 31 июля 1918 года и 1 августа 1918 года, заключаются в национализации всех нефтяных земель и разрешении их разработки только мексиканскими гражданами или компаниями, которые соглашаются считать себя мексиканскими и далее соглашаются не призывать к защите своих правительств. Законопроект был представлен в декабре 1918 года для выполнения статьи 27 новой конституции, но до сих пор никаких действий по этому вопросу предпринято не было. Декреты и законодательство, вытекающие из статьи 27, были опротестованы основными нефтяными компаниями, работающими в Мексике, и их соответствующими правительствами.

Коммерческий контроль над нефтяными ресурсами Голландской Ост-Индии находится в руках синдиката Royal Dutch-Shell и является по сути абсолютным по причине ограничений, содержащихся в Законе о горном деле Нидерландской Ост-Индии и последующих дополнениях к нему относительно иностранного приобретения прав на горные разработки в Ост-Индском архипелаге. Фактический контроль находится в руках Bataafsche Petroleum Maatschappij, которая имеет капитал в 56 000 000 долларов, разделенный на пять акций, три из которых принадлежат Royal Dutch Petroleum Co., а две — Shell Transport Trading Co. (британская). Чисто британские интересы контролируют незначительную добычу нефти в Британском Северном Борнео и в Сараваке.

Лицензии на разведку и концессии предоставляются только голландским подданным и голландским компаниям. Официально заявляется, что целью этих ограничений не является исключение иностранного капитала; это именно их эффект, и из-за экономической монополии, которую Royal Dutch-Shell сейчас имеет в нефтяной промышленности Голландской Ост-Индии, любому новому предприятию было бы очень трудно закрепиться.

Коммерческий контроль над нефтяными ресурсами Индии осуществляется Burma Oil Co. через ее доминирование в добыче, нефтеперерабатывающих заводах и трубопроводных мощностях, а также по причине соглашений о маркетинге со своим основным конкурентом, British Burma Petroleum Co., обе из которых контролируются британским капиталом. Burma Oil Co. связана с группой британских финансистов, если не контролируется ею напрямую, один или несколько из которых заинтересованы в компаниях на Тринидаде и в Персии.

Во время войны нефтяная промышленность Румынии временно находилась полностью под контролем немецких и австрийских интересов. Продвинутая стадия развития нефтяных месторождений до войны и преднамеренный ущерб, большая часть которого невосполнима, нанесенный месторождениям британскими отрядами в 1916 году, когда захват месторождений австро-германскими силами стал неизбежным, считаются, однако, лишившими Германию значительной части плодов ее завоевания, так как считается сомнительным, что румынские месторождения когда-либо снова смогут давать нефть по довоенной ставке 12 000 000 баррелей в год.

Американский нефтяной институт заявляет, что «Румыния рассматривает создание государственной монополии как на добычу, так и на распределение на руинах монополии, которую Германия пыталась установить там, но была вынуждена перемирием отказаться от нее».

До войны голландские, или, скорее, британско-голландские (Dutch-Shell) интересы контролировали около 30 процентов годовой добычи нефти в Румынии, немецкие интересы — около 26 процентов, интересы Соединенных Штатов (Standard Oil Co. of New Jersey) — около 18 процентов, французские интересы — около 16 процентов, чисто британские интересы — около 6 процентов, а бельгийские и румынские интересы — остальное.

Через австрийское «Society Gaz» и немецкое «Deutsche Erdoel Aktien-gesellschaft» немецкие интересы доминировали в нефтяной промышленности Галиции годами через прямой контроль над более крупными добывающими и перерабатывающими интересами и по причине того, что более мелкие разрозненные интересы зависели почти полностью от двух ведущих компаний, Galizische Karpathen Petroleum A. G. (контролируемой Society Gaz) и Premier Oil & Pipe Line Co. (контролируемой Deutsche Erdoel A. G., которая, в свою очередь, контролируется Diskonto und Bleichroeder, филиалом Deutsche Bank) для своих транспортных и перерабатывающих мощностей. Британский и голландский капитал были вовлечены в галицийские месторождения до войны, но, как полагают, не в контролирующей степени ни в одной из доминирующих компаний.

Нефтяная промышленность Японии контролируется полностью японскими интересами и в преобладающей степени одной компанией, Nippon Oil Co. Насколько известно автору, никакие иностранные интересы не участвуют каким-либо образом в развитии или контроле японской нефтяной промышленности.

Коммерческий контроль над нефтяной промышленностью Перу осуществляется Standard Oil Co. of New Jersey через ее дочернюю компанию Imperial Oil Co. of Canada. Этот контроль охватывает около 70 процентов годовой добычи, остальные 30 процентов разделены в соотношении 27 к 3 между британскими и итальянскими интересами соответственно. Насколько известно, никакие другие интересы не вовлечены.

Интересы, занятые в нефтяной промышленности Тринидада, включают финансовые группы чисто британские, контролирующие около 57 процентов добычи; британско-голландские интересы (Dutch-Shell), контролирующие около 23 процентов, и интересы Соединенных Штатов (General Asphalt Co.), контролирующие остальное. Ведущим оператором на Тринидаде является Trinidad Leaseholds, Ltd., британская компания, которая в 1917 году произвела около 42 процентов объема добычи нефти, приписанного Тринидаду в том году.

Коммерческий контроль над нефтяными ресурсами Нижнего Эльзаса находился в руках Vereinigte Pechelbronner Oelbergwerke Gesellschaft и Deutsche Tiefbohr A. G. Считается, что обе эти компании контролируются Deutsche Bank через Deutsche Erdoel A. G. и Diskonto und Bleichroeder. Незначительная добыча нефти в Ганновере, несомненно, находится под тем же финансовым контролем, хотя данных, которые оправдали бы положительное заявление на этот счет, нет под рукой.

Нефтяные запасы Аргентины, которые включают единственные районы, из которых нефть добывается в коммерческих целях в этой стране, эксплуатируются государством через Нефтяную комиссию Комодоро-Ривадавия. Считается, что немецкие интересы были вовлечены в две или три безуспешные попытки в последнее десятилетие получить нефть на участках, прилегающих к государственным запасам в районе Комодоро-Ривадавия.

Нефтяная промышленность в Египте контролируется полностью британско-голландским капиталом, работающим как Anglo-Egyptian Oilfields, Ltd., дочерняя компания синдиката Royal Dutch-Shell, через Anglo-Saxon Petroleum Co., причем последняя названная компания является преимущественно британской.

Коммерческий контроль над нефтяной промышленностью в Канаде осуществляется фактически Standard Oil Co. of New Jersey через ее дочернюю компанию Imperial Oil Co. of Canada. Этот контроль осуществляется через виртуальную монополию на трубопроводные и перерабатывающие мощности, а также благодаря тому, что добывающие интересы, хотя и британские и канадские, являются индивидуально мелкими и неорганизованными.

Добыча нефти в Италии, которая невелика, представляет собой объем производства двух компаний: Petroli d’Italia, в которой преобладает французский капитал, и Petrolifera Italiana, которая, как полагают, является по сути итальянской.

Финансовые группы, заинтересованные в нефти в Венесуэле, включают синдикат Royal Dutch-Shell (британско-голландский), General Asphalt Co. (Соединенные Штаты) и группу британских финансистов, которые контролируют объекты на Тринидаде, а также наиболее важную группу компаний, помимо Nobel и Dutch-Shell, в России.

Интересы Соединенных Штатов, включая Standard Oil Co., интересы Доэрти, Texas Co., Gulf Corporation и Island Oil Transport Corporation, занимают доминирующее положение в поисках нефти в Колумбии. Сообщается, что английская компания Venezuelan Oil Concessions, Ltd., работающая в Венесуэле, получила концессию на разведку нефти в северо-западном районе Британской Гвианы.

Интересы Sinclair (Соединенные Штаты) особенно активны в поиске нефти в Коста-Рике и Панаме; также, насколько известно, компания Sun Co. (Соединенные Штаты) изучает возможности добычи нефти в других республиках Центральной Америки.

Интересы Пирсона (британские) приложили значительные усилия в поисках нефти в Алжире и Марокко, и, как сообщается, в первой из этих стран американские интересы (Э. Э. Смит) недавно пытались получить нефтяные концессии у французского правительства.

Британские интересы, включая британское правительство, контролируют обширные нефтяные концессии в Персии, откуда в настоящее время добывается нефть в неустановленных объемах.

Наиболее перспективная нефтяная территория Персии недавно была закрыта для американской деятельности путем предоставления концессии площадью около 500 000 квадратных миль британской компании Anglo-Persian Oil Co., большая часть голосующих акций которой принадлежит британскому правительству. Срок действия этой концессии истекает в 1961 году. О важности этой нефтяной территории свидетельствует ее заявленная потенциальная мощность в 30 000 000 баррелей в год при наличии огромных неразработанных запасов.

Насколько известно, интересы Соединенных Штатов (Standard Oil Co. of New York) по-прежнему сохраняют контроль над правами на добычу нефти в некоторых провинциях Китая, где активная разведка в двух или трех районах несколько лет назад, как сообщалось, дала неблагоприятные результаты.

Нефть в небольших количествах добывается в Новой Зеландии исключительно британскими интересами.

ПОЛОЖЕНИЕ ВЕДУЩИХ ДЕРЖАВ

Соединенные Штаты.

Что касается вероятного развития нефтяной промышленности в ближайшее десятилетие, Соединенные Штаты, благодаря предприимчивости и дальновидности финансовых интересов отечественного происхождения, по-видимому, занимают прочные позиции. Интересы Соединенных Штатов практически безраздельно господствуют в коммерческом контроле над минеральными ресурсами Западного полушария, доминируя в нефтяной промышленности Соединенных Штатов, Канады, Мексики и Перу, владея значительными долями в Тринидаде и Венесуэле, а также в перспективных нефтеносных районах Центральной Америки и Колумбии. Их единственными конкурентами являются британские и британско-голландские интересы, которые контролируют ситуацию с нефтью в Тринидаде и не только прочно закрепились в Соединенных Штатах, Мексике и Венесуэле, но и агрессивно стремятся расширить свои владения в этих странах и закрепиться в других местах. Если Соединенные Штаты не примут меры, такие как федеральное управление магистральными трубопроводами, чтобы ограничить агрессию иностранного капитала в этой стране, и не выработают твердую, дальновидную государственную политику по защите инвестиций своих граждан в нефтяные активы в других странах, особенно в странах Латинской Америки, они могут стать свидетелями того, как их коммерческое превосходство в нефтяных делах пойдет на убыль и исчезнет, в то время как они все еще остаются крупнейшим политическим участником мировых поставок нефти.

В отличие от ярко выраженной националистической и преднамеренно агрессивной государственной политики, принятой Великобританией, Францией, Голландией и некоторыми другими странами, Соединенные Штаты никогда не принимали никакой политики, основанной на признании важности политического и коммерческого контроля над нефтью. Американские компании не могут владеть и управлять нефтяными землями в Британской империи, во французских владениях или голландских колониях, но единственные американские ограничения на иностранную деятельность в нефтяной промышленности — это те, которые распространяются на все полезные ископаемые, содержащиеся в государственных землях. Только американские граждане или те, кто заявил о своем намерении стать американскими гражданами, могут подавать заявки на патенты на такие земли. Однако после подачи заявки нет никаких ограничений на передачу полученных таким образом прав на недра.

Великобритания.

Британские и британско-голландские интересы легко доминируют в нефтяной ситуации в Восточном полушарии благодаря превосходству в нефтяной промышленности России, Персии, Индии и Голландской Ост-Индии. Считается, что доминирование в нефтяной ситуации только в одной России равносильно господству в нефтяной ситуации во всем Восточном полушарии на большую часть следующего столетия. Сила нынешнего положения Великобритании в мировых нефтяных делах заключается в сильной государственной политике и в широком охвате британских нефтяных инвестиций, охватывающих практически каждую страну, где нефть является важным продуктом, и почти каждую страну, где она является продуктом потенциальной важности. Общая политика Британской империи, по-видимому, заключается в контроле над всей разработкой нефти и ограничении операций иностранного капитала. В Австралии для эксплуатации нефтяных земель требуются лицензии, и только компании, зарегистрированные в Соединенном Королевстве или британском владении, могут получать такие лицензии. Генерал-губернатор имеет право преимущественной покупки всей добываемой нефти и в случае войны может взять под контроль все нефтяные активы. В Канаде, в тех западных провинциях, где полезные ископаемые являются собственностью Короны, земли с нефтью и природным газом могут сдаваться в аренду только британским компаниям. Аналогичное ограничение существует в Бирме. В Бирме монополия на нефтяную промышленность на 99 лет была предоставлена Burma Oil Co. в 1865 году. Это предоставление, по-видимому, было продиктовано страхом перед Standard Oil Co. из Соединенных Штатов, поскольку соглашение между компанией и правительством предусматривает, что первая не должна объединяться с другими нефтяными компаниями. Постановления аналогичного действия существуют в других британских колониях, где есть нефть; на Барбадосе британское правительство имеет право преимущественной покупки всех нефтяных остатков; в Британской Гвиане небританские компании могут владеть землями только по специальной лицензии губернатора; в Британском Гондурасе вся нефть зарезервирована за Короной; в Южной Нигерии, на Золотом Берегу, Тринидаде и Тобаго британское правительство имеет право преимущественной покупки всей нефти.

Недавнее предоставление концессии, равносильной монополии, в наиболее перспективном нефтяном районе Персии (регионе, который, по мнению многих нефтяных экспертов, вероятно, станет одним из самых важных в мире) британской компании, контролируемой непосредственно (через владение акциями) британским правительством, свидетельствует об агрессивной политике Англии за пределами своих собственных владений по обеспечению и удержанию под государственным контролем нефтяных земель во всех частях земного шара.

Насколько известно, самые известные нефтяные территории в Венесуэле уже покрыты концессиями, которые практически все контролируются прямо или косвенно британскими интересами, главным образом синдикатом Dutch-Shell.

Насколько можно судить, германские интересы фактически доминируют в нефтяной промышленности в Галиции и у себя на родине. Будет ли Германия вынуждена полагаться на свои собственные нефтяные ресурсы или на них, подкрепленные ресурсами Галиции, она, очевидно, будет иметь недостаточные запасы, и, как следствие, германские интересы, вероятно, будут особенно агрессивны в поисках нефти в Месопотамии, Африке и Южной Америке.

Франция.

С тех пор как контроль над нефтяными интересами Ротшильдов перешел в руки синдиката Royal Dutch-Shell (британско-голландского), влияние французских финансов в нефтяных делах стало незначительным, за исключением Галиции и Италии, где его сила была невелика. Французский капитал, несомненно, будет участвовать в усилиях по определению нефтяных запасов стран Варварийского берега, французских зависимых территорий, но он вряд ли будет сильно вовлечен в организованные усилия по контролю над мировой ситуацией в отношении нефти.

Французское горное законодательство гласит, что нефть и газ принадлежат государству и могут эксплуатироваться на основе концессий, площадь и срок действия которых являются предметом переговоров между заявителем и властями. Насколько известно, французское правительство не желает предоставлять нефтяные концессии, кроме как компаниям, большинство акций которых принадлежит французским гражданам. Компания, зарегистрированная недавно для разработки алжирских нефтяных месторождений, содержит в своем учредительном договоре положение о том, что 60 процентов ее акций должны принадлежать французским гражданам.

Япония.

Японские инвестиции в мировую нефтяную промышленность еще не достигли значительных размеров за пределами самой Японии, хотя японское правительство официально осознает важность японских инвестиций в нефтяные активы в Мексике, особенно в Нижней Калифорнии и Соноре; Китае; и, несомненно, в России. Следовательно, в ближайшем будущем можно ожидать крупных вложений японского капитала в нефтяную промышленность в одной или всех этих странах.

РЕЗЮМЕ

Нефть в сыром или полурафинированном состоянии используется в качестве топлива в локомотивных и морских котлах, а также в качестве смазочного материала. Однако основное использование нефти заключается в производстве многочисленных рафинированных продуктов. Некоторые из наиболее важных продуктов и их использование следующие: эфир — как анестетик в хирургии; бензин — как топливо в двигателях внутреннего сгорания; нафта — как растворители и в производстве коммерческого бензина; керосин — как осветительное средство и топливо для сельскохозяйственных тракторов; смазочные масла; воски — как консерванты, осветительные средства и хирургические повязки при лечении ожогов; нефтяной кокс — в металлургических процессах и в производстве угольных электродов для батарей и дуговых ламп; тяжелые котельные топлива; дорожные масла; искусственные асфальты — для дорожных покрытий. Использование нефти и продуктов ее переработки в качестве топлива, смазочного материала и для освещения можно считать необходимым. Известны заменители для большинства этих видов использования, но они либо неэффективны, либо труднодоступны.

Наиболее продуктивные источники нефти находятся в осадочных пластах каменноугольного и третичного периодов. Поскольку самая детальная геологическая работа недостаточна для обеспечения надлежащей оценки многочисленных факторов, участвующих в залегании нефти, и поскольку лишь относительно небольшой процент площадей осадочных пород по всему миру был изучен геологически с какой-либо заметной детальностью, трудно оценить будущие запасы нефти или предсказать, что крупные скопления будут обнаружены в каком-либо конкретном регионе.

Основные страны, вносящие вклад в мировую добычу нефти, располагаются в следующем общем порядке важности: Соединенные Штаты, Россия, Мексика, Голландская Ост-Индия, Румыния, Индия, Персия и Галиция. Другие страны производят менее 2 процентов от годового общего объема. Самое большое изменение, которое, вероятно, произойдет в географическом распределении добычи, — это увеличение объема добычи в странах, граничащих с Карибским морем и Мексиканским заливом, а также на персидских и месопотамских месторождениях. Мексика сейчас занимает второе место после Соединенных Штатов, и страны Южной Америки обещают стать более важными участниками мировой добычи, чем они есть сейчас. Ожидается, что Россия в конечном итоге станет одним из главных производителей нефти.

В течение следующего десятилетия, благодаря улучшенным методам добычи и дальнейшему объединению добывающих, транспортных, нефтеперерабатывающих и маркетинговых компаний в сильные единицы, объем добычи, несомненно, будет больше и будет производиться более экономично. При переработке нефти вероятно, что улучшенные методы позволят извлекать больший процент более легких продуктов из низкосортной нефти. Двигатели внутреннего сгорания модифицируются таким образом, чтобы работать на нефтепродуктах с меньшей летучестью, чем бензин. Ожидается, что использование нефти в качестве топлива в железнодорожных и морских котлах значительно возрастет в следующем десятилетии. По мере истощения добывающих месторождений огромные залежи горючих сланцев в западной части Соединенных Штатов будут разрабатываться как источник нефти.

Насколько известно, политический контроль над нефтяными ресурсами мира определяется государственным суверенитетом (см. Таблицу I, стр. 7). В нормальное время Соединенные Штаты политически контролируют более 66 процентов текущей добычи нефти. Россия и Мексика занимали второе и третье места в 1917 году, контролируя 13,6 процента и 10,9 процента соответственно. Оставшиеся 9 процентов контролировались Великобританией, Голландией, Персией (принадлежащей британскому правительству), Румынией, Австро-Венгрией, Японией, Перу, Германией, Аргентиной и Италией в указанном порядке.

Таблица, показывающая национальную принадлежность и приблизительный масштаб коммерческого контроля, осуществляемого доминирующими интересами в каждой из основных нефтедобывающих стран, и Рис. 2 (стр. 12) являются наилучшими возможными резюме коммерческого контроля. Капитал Соединенных Штатов является верховным в коммерческом контроле над нефтяной промышленностью Западного полушария. Британские и британско-голландские интересы легко доминируют в нефтяной ситуации в Восточном полушарии. Франция больше не осуществляет контроль над какими-либо важными месторождениями. Японские интересы, контролирующие в настоящее время все нефтяные месторождения Японии, могут, как ожидается, сделать крупные инвестиции в нефтяные месторождения Мексики, Китая и России.

ГЛАВА II УГОЛЬ Джордж С. Райс и Фрэнк Ф. Граут

ИСПОЛЬЗОВАНИЕ УГЛЯ

Уголь является одним из самых важных полезных ископаемых. Он обеспечивает энергию и тепло, а его дистилляция дает большое количество полезных материалов, таких как газ для освещения и топлива, взрывчатые вещества, аммиак, анилиновые красители и т. д. Кокс, который представляет собой битуминозный уголь с удаленными путем дистилляции более летучими компонентами, используется для плавки металлических руд; и, таким образом, близость месторождений высококачественного коксующегося угля и железной руды определила расположение центров сталелитейной промышленности, которые являются самой движущей силой нашей современной машинной цивилизации. Рядом с такими угольными районами естественным образом развивались другие производства всех видов, поскольку уголь был дешево доступен для получения энергии и составлял практически единственный источник энергии в регионах, где дешевая гидроэлектроэнергия недоступна. Около 66 процентов добываемого угля идет на производство энергии, включая транспорт; около 12 процентов — на коксование и побочные продукты; и около 22 процентов — на отопление зданий.

Коммерческий уголь бывает трех разновидностей: (1) антрацит (пенсильванский антрацит в народе называют твердым углем) и полуантрацит, содержащий высокий процент фиксированного углерода и относительно низкий процент летучих компонентов (от 3 до 12 процентов); (2) битуминозный (в Соединенных Штатах его двусмысленно называют «мягким углем»), содержащий меньше фиксированного углерода и больше летучих веществ (от 12 до 40 процентов); и (3) лигнит, содержащий еще меньшую долю фиксированного углерода и большую долю воды. Из битуминозных углей некоторые хорошо коксуются, но многие — нет, поэтому хорошие коксующиеся угли высоко ценятся. Антрацит, поскольку он не дает дыма, пользуется большим спросом для отопления домов; в то время как битуминозный уголь в основном используется для производства энергии, включая топку локомотивов и пароходов. Лигниты, как правило, используются только там, где недоступны лучшие сорта угля.

Уголь впервые начали использовать для отопления еще до появления паровой энергии, а железо плавили на древесном угле, а не на коксе, как в настоящее время.

Бункеровка судов требует лучших сортов битуминозного угля, с низким содержанием золы и предпочтительно высоким содержанием фиксированного углерода, поскольку использование низкосортных углей потребовало бы перевозки больших объемов, оставляя меньше места для груза. Однако ни одна страна, имеющая достаточно угля для бункеровки судов, не должна зависеть от иностранных поставок; низкое качество угля просто снизило бы эффективность и, таким образом, увеличило бы расходы.

Заменители.

Доля угля, используемого для получения энергии, в отличие от того, что используется для тепла и угольных продуктов, увеличивается и сейчас составляет две трети от общего объема. Как источник энергии, действительно нет полной замены углю. Все великие промышленные нации, такие как Англия, Германия и Соединенные Штаты, развивали свою промышленность на основе больших запасов угля. Некоторые страны широко используют гидроэлектроэнергию, но для большинства это недостаточный заменитель. Древесина и другие виды топлива редко бывают достаточными для поддержания промышленности, построенной на поставках угля. Нефть успешно заменяется в некоторых отраслях промышленности, особенно в судоходстве, но важность угольных станций, несомненно, сохранится.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Техника добычи угля во многих районах, а также развитие производства тепла, энергии и угольных продуктов развиты недостаточно. Используются расточительные методы, в основном в результате конкуренции и отсутствия сотрудничества и организации среди производителей. Однако пропагандируется экономия. На многих шахтах установлено трудосберегающее оборудование. Ряд электростанций был построен рядом с устьем шахты, а энергия распределяется электрически, что исключает расходы на перевозку угля. Центральные отопительные и энергетические установки, которые могут эффективно сжигать уголь, несомненно, станут более популярными и многочисленными через несколько лет. Можно ожидать, что государственный контроль и законодательство ускорят эти изменения. В Европе техника добычи угля, за исключением врубовых машин, развита дальше, чем в Соединенных Штатах, в том, что касается добычи всего угля и поддержания поверхности.

Усовершенствования в коксовых печах могут вскоре сделать возможным производство какого-либо вида кокса практически из любого битуминозного угля. Хотя не весь кокс может быть удовлетворительным для современной практики доменных печей, любой будущий недостаток кокса, вероятно, будет компенсирован развитием электрической плавки, поэтому серьезность металлургической потребности сомнительна. Доля коксовых печей с улавливанием побочных продуктов, которые обеспечивают более дешевый кокс за счет получения других товарных продуктов, увеличивается.

ГЕОЛОГИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Угли встречаются в осадочных отложениях нескольких геологических эр: палеозойской, мезозойской и третичной. Палеозойская эра, охватывающая каменноугольный период, является безусловно самой важной с точки зрения качества и доступности своих угольных ресурсов; но более низкосортные и главным образом лигнитные угли мезозойской и третичной эр имеют большое местное значение, и существуют огромные запасы, которые по количеству превышают в целом более высококачественные угли более ранних периодов.

Геологическое распределение угля описано в «Угольных ресурсах мира», самом важном и всеобъемлющем сборнике по запасам угля, который когда-либо составлялся и который был предпринят Исполнительным комитетом Двенадцатого международного геологического конгресса, состоявшегося в Канаде в 1913 году. Поскольку сборник был составлен при содействии геологических служб и горных геологов различных стран мира, он цитируется в этой статье как авторитетный источник по геологическому распределению и ресурсам.

Географическое распределение основных угольных бассейнов мира показано на Таблице II.

В Северной Америке наиболее важные угли в центральной и восточной части относятся к палеозойскому возрасту, но в регионе Скалистых гор огромные количества угля встречаются в меловых (мезозойских) пластах. В провинции Мексиканского залива и в провинции Северных Великих равнин Соединенных Штатов, которая простирается до Канады, находятся угли триасового (мезозойского) возраста, которые в настоящее время относительно неважны.

В пластах эоценового периода третичной эры имеются крупные залежи бурого лигнита, местами превращенного горообразовательными силами в битуминозный и полубитуминозный уголь, а также немного антрацита в сложных условиях добычи. Такие локально измененные пласты встречаются в штате Вашингтон, в Британской Колумбии и на Аляске.

Ограниченные угольные ресурсы Южной Америки, в тех месторождениях к востоку от Анд и в южной и восточной Бразилии, относятся к палеозойскому возрасту. Небольшие площади третичных углей встречаются в южной Аргентине и в Чили.

Ключ к Таблице II.

Мировые запасы угля на 1916 год — Угольные бассейны закрашены сплошным черным цветом.

1. Страны, обладающие запасами угля первой величины (от 4 000 000 миллионов до 1 000 000 миллионов тонн): Соединенные Штаты (3 527 000 миллионов), Канада (1 234 000 миллионов) и Китай (1 500 000 миллионов).

2. Страны, обладающие запасами угля второй степени величины (от 500 000 миллионов до 100 000 миллионов): Британские острова (189 533 миллиона), Германия (до войны) (423 356 миллионов), Сибирь (173 879 миллионов) и Австралия (165 572 миллиона).

3. Страны, обладающие запасами угля третьей степени величины (от 80 000 миллионов до 16 000 миллионов тонн): Франция (до войны) (17 583 миллиона), Аляска (16 293 миллиона), Колумбия (27 000 миллионов), Австро-Венгрия (до войны) (55 553 миллиона), Россия в Европе (до войны) (60 106 миллионов), Индия (79 001 миллион), Индокитай (20 000 миллионов) и Южная Африка (56 200 миллионов).

4. Страны, обладающие запасами угля четвертой степени величины (от 16 000 миллионов до 6 000 миллионов тонн): Испания (8 768 миллионов), Япония (7 970 миллионов), Бельгия (11 000 миллионов), Шпицберген (8 750 миллионов).

5. Страны, обладающие запасами угля, но меньшей величины (менее 4 000 миллионов тонн): Бразилия, Аргентина, Чили, Перу, Эквадор, Венесуэла, Гренландия, Голландия, Дания, Швеция, Италия, Болгария, Турция, Греция, Румыния, Малая Азия, Персия, Аравия, различные острова Малайзии и различные страны Африки. Угольные бассейны показаны черным цветом — страна не заштрихована.

Таблица II. — Географическое распределение угольных месторождений мира и относительные запасы. Ф. Ф. Граут.

В Европе основные угольные месторождения встречаются в каменноугольной системе, либо в верхней, либо в нижней ее части. Нижний карбон является основной серией, в которой встречаются угли в Шотландии, тогда как наиболее важные угли в Англии и Уэльсе залегают в породах верхнего карбона. В северной Франции, в Бельгии и в Вестфалии, Германия, средние каменноугольные пласты содержат наиболее важные запасы. Мезозойские угли встречаются в северной Австралии и в центральной Франции. Лигниты или бурые угли средней Европы местами очень важны в Германии; угли Австрии встречаются в многочисленных небольших, но мощных месторождениях третичного возраста.

Рис. 3. — Добыча угля в основных угледобывающих странах, 1880-1916 гг.

Основные угольные ресурсы Африки находятся в южной части континента и в основном в отложениях, возраст которых варьируется от каменноугольного до триасового.

В Азии угольные бассейны не очень хорошо определены. Есть примечательные угольные бассейны в Индии и Китае. В Китае важные угли встречаются в верхнем карбоне. Угли нижнего карбона встречаются к востоку от Урала, а также в Туркестане. В Японии важны мезозойские угли. Третичные угли широко распространены в Азии, но не являются высококачественными и не имеют значения.

Можно с уверенностью сказать, что геологическая разведка охватила мир настолько хорошо, что дальнейшее развитие вряд ли раскроет угольные ресурсы большой величины, не известные сейчас с той или иной точностью. Оценки ресурсов некоторых регионов, несомненно, будут пересматриваться много раз, особенно оценки запасов в средней части Африки, в Южной Америке и Китае.

ДОБЫЧА УГЛЯ В МИРЕ В 1913 ГОДУ

Поскольку великая Мировая война началась 31 июля 1914 года, последние нормальные цифры добычи относятся к 1913 году. Следующая таблица мировой добычи угля за 1911-1914 годы взята из «Минеральных ресурсов» Геологической службы США, причем составителем сборника г-н Лешер из Службы называет г-на Уильяма Г. Грея, статистика Американского института железа и стали, и профессора Г. А. Рауша, редактора «Минеральной индустрии».

Добыча (1880-1916 гг.) основных угледобывающих стран мира показана графически на Рисунке 3.

Таблица 4. — Мировая добыча угля (в коротких тоннах)

Country | 1911 | 1912 | 1913 | 1914
United States | 496,371,126 |  | 534,466,580 |  | 569,960,219 |  | 513,525,477 |
Great Britain | 304,518,927 |  | 291,666,299 |  | 321,922,130 |  | 297,698,617 |
Germany | 259,223,763 |  | 281,979,467 |  | 305,714,664 |  | 270,594,952 |
Austria-Hungary | 54,960,298 |  | 56,954,579 |  | 59,647,957 |  |  |
France | 43,242,778 |  | 45,534,448 |  | 45,108,544 |  |  |
Russia | 29,361,764 |  | 33,775,754 |  | 35,500,674 |  |  |
Belgium | 25,411,917 |  | 25,322,851 |  | 25,196,869 |  |  |
Japan | 19,436,536 |  | 21,648,902 |  | 23,988,292 |  | 21,700,572 |
India | 13,494,573 |  | 16,471,100 |  | 18,163,856 |  |  |
China | 16,534,500 |  | 16,534,500 |  | 15,432,200 | [5] |  |
Canada | 11,323,388 |  | 14,512,829 |  | 15,115,089 |  | 13,597,982 |
New South Wales | 9,374,596 |  | 10,897,134 |  | 11,663,865 |  | 11,644,476 |
Transvaal | 4,343,680 |  | 8,119,288 | [6] | 5,225,036 |  |  |
Spain | 4,316,245 |  | 4,559,453 |  | 4,731,647 |  |  |
Natal | 2,679,551 |  | See note 6 |  | 2,898,726 |  |  |
New Zealand | 2,315,390 |  | 2,438,929 |  | 2,115,834 |  |  |
Holland | 1,628,097 |  | 1,901,902 |  | 2,064,608 |  |  |
Chile | 1,277,191 |  | 1,470,917 |  | 1,362,334 |  |  |
Queensland | 998,556 |  | 1,010,426 |  | 1,162,497 |  | 1,180,825 |
Mexico | 1,400,000 | [5] | 982,396 |  |  |  |  |
Bosnia and Herzegovina | 848,510 |  | 940,174 |  | 927,244 |  |  |
Turkey | 799,168 |  | 909,293 |  |  |  |  |
Italy | 614,132 |  | 731,720 |  | 772,802 |  |  |
Victoria | 732,328 |  | 664,334 |  | 668,524 |  |  |
Orange Free State (Orange River Colony) | 482,690 |  |  |  | 609,973 |  |  |
Dutch East Indies | 600,000 | [5] | 622,669 |  | 453,136 |  |  |
Indo-China | 460,000 | [5] | 471,259 |  |  |  |  |
Serbia | 335,495 |  | 335,000 |  |  |  |  |
Sweden | 343,707 |  | 397,149 |  | 401,199 |  |  |
Western Australia | 300,000 | [5] | 330,488 |  | 351,687 |  |  |
Peru | 300,000 | [5] | 307,461 |  | 301,970 |  |  |
Formosa | 280,999 |  | 306,941 |  |  |  |  |
Bulgaria | 270,410 |  | 324,511 |  |  |  |  |
Rhodesia | 212,529 |  | 216,140 |  | 237,728 |  |  |
Roumania | 266,784 |  |  |  |  |  |  |
Cape Colony (Cape of Good Hope) | 89,023 |  | See note 6 |  | 67,481 |  |  |
Korea | 138,508 |  |  |  |  |  |  |
Tasmania | 70,000 | [5] | 59,987 |  | 61,648 |  | 68,130 |
British Borneo | 100,000 | [5] |  |  | 49,762 |  |  |
Spitzbergen | 44,092 |  |  |  |  |  |  |
Brazil | 16,535 |  |  |  |  |  |  |
Portugal | 10,000 | [5] | 16,938 |  | 27,053 |  |  |
Venezuela | 10,000 | [5] | 12,000 | [5] | 13,355 |  |  |
Switzerland | 8,267 |  |  |  |  |  |  |
Philippine Islands | 2,000 | [5] | 2,998 |  |  |  |  |
Unspecified | 1,016,947 | [5] |  |  |  |  |  |
Total | 1,309,565,000 | [7] | 1,377,000,000 | [7] | 1,478,000,000 | [7] | 1,346,000,000 |

[5] Оценочно.

[6] Трансвааль включал Наталь и Капскую колонию.

[7] Приблизительно.

Таблица 5. — Запасы

Общие запасы угля в миллионах метрических тонн были оценены по континентам следующим образом:

Continent | Millions of tons
North America | 5,073,000
Asia | 1,280,000
Europe | 784,000
Australia and Oceania | 170,000
Africa | 58,000
South America | 32,000

Страны, имеющие наибольшие запасы на довоенной основе, следующие:

Country | Millions of tons
United States (half lignite) | 3,527,000
Canada (three-fourths lignite) | 1,234,000
China | 996,000 to 1,500,000
British Isles | 190,000
Siberia (largely lignite) | 173,000
Germany (including Upper Silesia and the Saar) | 423,000
New South Wales | 118,000
India | 79,000
Russia including Dombrova field (Poland) | 60,000
Austria (chiefly in Bohemia, Silesia and Galicia) | 54,000
France | 17,600

Рис. 4. — Запасы угля основных добывающих стран согласно «Угольным ресурсам мира», в миллионах метрических тонн. Квадраты даны в масштабе: линии, показывающие относительную добычу, даны не в том же масштабе, что и квадраты.

Запасы основных продуктивных угольных бассейнов графически показаны на Рисунке 4.

Распределение угольных месторождений мира и оценочные запасы в этих месторождениях показаны на Таблице II.

ОБЩАЯ МИРОВАЯ СИТУАЦИЯ

Районами, имеющими уголь для экспорта, были главным образом Британские острова, Соединенные Штаты и Германия; сюда можно было бы включить также Новый Южный Уэльс, Британскую Южную Африку, Японию, Французский Индокитай, Канаду, Новую Зеландию и Шпицберген. Китай с его большими запасами может стать экспортером в будущем; или, если его промышленность будет развиваться, может найти применение своему углю внутри страны.

Антрацит хорошего качества в больших количествах встречается только в Пенсильвании и Южном Уэльсе. Более бедные запасы известны в Германии, Франции, Италии, Индокитае, а также в штатах Колорадо и Нью-Мексико.

Коксующиеся угли в больших количествах встречаются в восточной части Соединенных Штатов, Германии и Соединенном Королевстве и широко используются для коксования. Меньшие количества кокса производятся во Франции, Бельгии и старой Австрии. Относительно очень малые количества производятся в Канаде, Чили, Новом Южном Уэльсе, Японии и Испании.

Запасы угля страны не имеют прямой связи с ее текущей добычей, поскольку последняя, которая должна развиваться в конкуренции с другими странами, зависит от относительной легкости транспортировки и близости месторождений железной руды, которые делают производство стали и другие отрасли промышленности экономически целесообразными.

Великобритания особенно благоприятна благодаря наличию высококачественного угля в непосредственной близости от прибрежных портов, как на севере Англии, в Шотландии и Уэльсе. Поэтому Великобритания стала крупным экспортером угля. Сначала уголь для отопления доставлялся морем из Ньюкасла в Лондон; затем уголь перевозился в европейские порты, а в конечном итоге — во все части мира. Наличие легко разрабатываемых месторождений железа на севере Англии и открытие того, что железо можно плавить с помощью кокса, быстро ускорило развитие угольной промышленности в Великобритании, так что к середине девятнадцатого века Великобритания заняла лидирующее положение.

Ни одна другая страна не обладает высококачественным углем в таком количестве в непосредственной близости от побережья, и этот факт позволил Великобритании оставаться крупным экспортером. Среднее расстояние перевозки экспортного угля от шахты до судна составляет менее 20 миль. В Германии уголь для морского экспорта должен перевозиться на расстояние от 118 до 168 миль; в Соединенных Штатах — от 150 до 375 миль, за исключением углей Вашингтона, которые находятся в пределах 40 миль от морского побережья, но их количество невелико, а качество посредственное.

После войны с Францией в 1871 году, когда Германия аннексировала Эльзас и Лотарингию, угольная промышленность Германской империи развивалась с огромной быстротой, главным образом благодаря открытию — на основе исследований Томаса из Великобритании — метода использования высокофосфористых железных руд германской и французской Лотарингии, а также близости этих месторождений железной руды к высококачественным битуминозным углям Вестфалии. Угольная промышленность также развивалась путем поощрения экспортной торговли с соседними странами, которые имеют небольшие угольные ресурсы или не имеют их вовсе, причем эта торговля почти полностью осуществлялась по железной дороге.

Однако длительная железнодорожная перевозка и соответственно высокая стоимость добычи сдерживали морской экспортный бизнес Германии, несмотря на попечительскую заботу правительства. С передачей практически всех своих месторождений железа и важных месторождений калийных солей в Лотарингии, а также права собственности на свои угольные шахты в Сааре Франции, и возможной потерей своих угольных и цинковых месторождений в Верхней Силезии в пользу Польши, баланс коммерческого процветания также может быть передан.

Ни одна другая страна, кроме Соединенных Штатов, Канады, Австралии и Китая, не имеет запасов для обширной экспортной торговли. В Канаде угли в основном находятся внутри страны, а те, что находятся недалеко от побережья, как на острове Ванкувер и в Новой Шотландии, ограничены в количестве и трудны для добычи, поэтому экспортный бизнес вынужденно ограничен.

Одним из изменений, которое кажется вероятным, является быстрое увеличение добычи угля в Китае. Ресурсы огромны, запасы высших сортов угля не превзойдены ни одной страной, кроме Соединенных Штатов. Амбициозные и агрессивные японцы, благодаря своему стратегическому соседскому расположению, дали все основания полагать, что они воспользуются возможностью для разработки такого ресурса. Может быть вопросом, как скоро будет освоен китайский уголь, но великие перемены неизбежны, когда начнется освоение. Некоторые из угольных бассейнов находятся так близко к побережью и имеют угли такого хорошего качества, что позволяют широко развивать экспортный бизнес на Востоке.

Австралия, особенно в Квинсленде и Новом Южном Уэльсе, обладает значительными угольными ресурсами по сравнению с потребностями небольшого населения. В Новом Южном Уэльсе угли превосходны и находятся рядом или близко к гаваням, поэтому уголь широко поставляется для бункеровки и экспортной торговли в южную часть Тихого океана и стал важным фактором в океанской торговле этой части мира.

Крупным фактором в угольной торговле Тихого океана является перевозка угля в качестве обратного груза. Это также важно в торговле с Южной Америкой. Южная Африка во время войны отправляла значительное количество угля в западное Средиземноморье, но ее уголь не может быть крупным фактором в океанской торговле в нормальное время.

Из всех континентов Южная Америка является самой бедной угольными ресурсами. В Бразилии, Чили и других южноамериканских странах есть уголь, но до него трудно добраться, и месторождения, известные до сих пор, не дают надежды на то, что смогут удовлетворить потребности стран, в которых они находятся. Общая годовая добыча Южной Америки составляет менее двух миллионов тонн, в основном из Чили. Вероятно, что в течение следующего поколения Южная Америка будет продолжать импортировать уголь, как и в прошлом, в объеме 15 миллионов тонн или более в год, хотя разработки в Бразилии сейчас многообещающи для будущего снабжения этой страны. Оценки запасов см. в Таблице 5.

Резюме.

В качестве резюме можно сказать, что Соединенные Штаты лидируют в мире по угольным ресурсам; более того, их ресурсы наиболее доступны, благодаря их малой глубине залегания, общему ненарушенному (геологическому) состоянию и их доступности через железнодорожные системы. Это особенно верно для Аппалачского региона, который содержит безусловно лучший уголь, находится ближе всего к побережью и, следовательно, наиболее доступен для океанской торговли. С другой стороны, среднее расстояние перевозки до экспортных пунктов, как уже отмечалось, намного больше, чем у Великобритании, и больше, чем у Вестфалии; но, чтобы компенсировать это, уголь добывался и может добываться дешевле, чем в Вестфалии или Великобритании. Ресурсы Верхней Силезии велики, и уголь легко добывается, но вся добыча будет необходима для Центральной Европы. Что касается как качества, так и количества, пенсильванский антрацит уникален; тем не менее, внутренние потребности будут продолжать сдерживать обширный экспорт. Паровые и коксующиеся угли Соединенных Штатов, доступные для отгрузки, в среднем немного хуже соответствующих углей Великобритании, но превосходят немецкие угли.

Общие ресурсы Великобритании, возможные, фактические и вероятные, составляют всего 190 000 миллионов тонн, в отличие от 423 000 миллионов тонн в старой Германской империи и 3 838 000 миллионов тонн в Соединенных Штатах.

Вероятная будущая добыча.

Возможное истощение угольных ресурсов, конечно, важно при рассмотрении будущего, но можно с уверенностью сказать, что ни в одном из основных разрабатываемых сейчас месторождений ресурсы не истощены настолько, чтобы добыча из них сократилась еще как минимум на одно поколение.

Из великих угледобывающих стран Великобритания с ее растущим темпом добычи наиболее близко подходит к точке окончательного истощения, но эта точка по-разному оценивается от ста до нескольких сотен лет в будущем, многое зависит от того, будет ли при лучших методах использования добыча продолжать расти такими же темпами, как в прошлом. Тем временем некоторые районы в Великобритании с более мелкими угольными пластами будут истощены гораздо раньше, а оставшийся уголь станет все труднее добывать из-за увеличивающейся глубины добычи, что, в свою очередь, вызовет постоянно растущую стоимость.

Хотя истощение угля — это отдаленная перспектива, есть явные признаки приближающегося истощения определенных сортов угля. Было подсчитано, что добыча американского антрацита серьезно сократится через 60-100 лет. Вероятно, это приведет к изменению практики, использованию кокса и других методов отопления домов. Если темпы добычи продолжат расти, высококачественный американский паровой уголь, Нью-Ривер и аналогичные сорта, вероятно, будут исчерпаны чуть более чем через 150 лет. Американский коксующийся уголь лучшего качества Коннеллсвилл имеет столь же короткий срок службы. Британский уголь аналогичного высокого качества может прослужить дольше американского, так как темпы добычи менее быстры, даже если общие запасы американского угля должны прослужить гораздо дольше, чем британские.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

В ряде стран установлена государственная собственность на угольные шахты; как, например, в частях Пруссии, Австралии, Чили и Болгарии. В других неразработанные угольные земли по-прежнему в значительной степени принадлежат правительству, как на Аляске и в западной части Соединенных Штатов. В некоторых странах правительство сохраняет контроль над всеми правами на полезные ископаемые, просто сдавая собственность в аренду и предоставляя концессию на добычу. Многие правительства имеют департамент или администрацию шахт. В каждой стране, конечно, в чрезвычайной ситуации суверенное государство будет осуществлять контроль над угольными ресурсами в полной мере, насколько это необходимо. Там, где государство владеет шахтами и поощряет организацию, как в Германии, более радикальное регулирование военного времени осуществляется легко. Вполне возможно, что уголь со временем будет повсеместно считаться общественным достоянием.

В Англии движение к национализации шахт, в котором участвуют как шахтеры, так и правительство, по-видимому, делает успехи.

Колонии Англии превосходят все остальные по объему угольных ресурсов. Уголь есть в Австралии, Канаде, Индии, Новой Зеландии, Южной Африке, Родезии, Ньюфаундленде, Южной Нигерии и Британском Северном Борнео — общее количество во много раз больше, чем на Британских островах. Колонии и владения Франции, Дании, Португалии, Соединенных Штатов и Японии имеют относительно небольшое количество угля.

На угольные ресурсы, наряду с другим сырьем, повлияли некоторые торговые договоры. Однако ни одной нации не было обеспечено постоянное преимущество в торговле посредством торгового договора. Почти все такие договоры заключаются на короткие сроки и возобновляются. Если они не устраивают одну из сторон, они вскоре исправляются. Можно упомянуть различные неформальные или молчаливые соглашения. Когда во время войны не хватало судов, Англия и Соединенные Штаты разделили угольный бизнес Южной Америки в соответствии с требованиями судовой экономии. Германия заключила соглашения о поставках угля в Австро-Венгрию и Швейцарию в период войны. У Англии были соглашения с Францией, Испанией, Португалией и Италией, эти соглашения менялись в зависимости от условий, относительно поставок английского угля.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Хотя владение шахтами в большинстве стран номинально открыто как для граждан, так и для иностранцев, исключения и ограничения стремятся сохранить контроль в руках граждан. Например, невозможно, чтобы иностранцы контролировали какую-либо горнодобывающую компанию в Японии. Концессии в Голландии и голландских колониях ограничены голландскими подданными, а в Боливии — боливийскими гражданами. Законодательство, предложенное после начала Мировой войны, может привести к аналогичному положению во владениях Великобритании и ее союзников.

В мирное время отношения между двумя странами могут в значительной степени определяться владением собственностью; владельцы собственности в иностранной стране могут сильно влиять на политику двух правительств по отношению друг к другу. В чрезвычайных ситуациях политический и коммерческий контроль подвергаются испытанию, и результатом становится либо тупик, либо победа одного над другим.

Важным коммерческим отношением, оказывающим политическое влияние, является регистрация компаний по законам разных стран. Горнодобывающие компании в Китае, такие как Kailan Mining Administration, организуются в Гонконге для получения британской защиты и, таким образом, подпадают под британский контроль, несмотря на то, что бельгийские деньги финансируют компанию. Некоторые компании, организованные в Японии, также могут владеть китайскими угольными шахтами.

Поскольку относительно немногие регионы мира имеют уголь сверх своих собственных потребностей, большинство из них зависят от импорта. Если страна с углем также контролирует пароходные линии, она может полностью контролировать угольную ситуацию в импортирующей стране. Англия, имеющая около половины общего мирового судоходства и хорошие запасы портового угля, была в состоянии доминировать в экспорте угля, вплоть до обработки излишков американского угля. В течение последних трех или четырех лет нехватка судов придала повышенное значение американскому и японскому судоходству, но англичане по-прежнему оказывают сильное влияние. Их доки и складские помещения — лучшие, а их судов по-прежнему много.

Права на железнодорожные перевозки по Национальным линиям в Мексике дают определенную степень контроля над угольной промышленностью. Национальные линии принадлежат государству и имеют специальное соглашение, предоставляющее права на использование путей двум компаниям: American Smelting and Refining Co. и компании Peñoles, находящейся в германской собственности. Поскольку мексиканское железнодорожное сообщение было нарушено, германская компания работает с использованием собственных вагонов и локомотивов. Она имеет много коксовых печей и большие запасы угля и была главным конкурентом американской компании в мексиканской металлургии.

Никакой патент вряд ли ограничит угольную промышленность, за исключением побочных продуктов кокса. До войны продукты каменноугольной смолы в значительной степени разрабатывались немцами, которые патентовали свои процессы во многих странах, но не предлагали такой защиты иностранным изобретениям путем патентов в Германии. Они ограничивали производство в основном своими германскими заводами и экспортировали продукции на сумму около 50 000 000 долларов в год.

Во время войны эти патенты в Соединенных Штатах были взяты под контроль Управляющим по делам собственности иностранцев, и американские отрасли промышленности, возникшие в результате этого, могут быть защищены на постоянной основе. Другие союзные страны предприняли те же шаги, чтобы освободиться от германского контроля, который сдерживал развитие промышленности коксовых побочных продуктов в негерманских странах.

В Германии крупные горнодобывающие компании обычно владеют правами на уголь. Единственным правительством, которое добывало уголь в коммерческих масштабах и для коммерческих целей, является Германия, и даже там государственная добыча покрывала лишь небольшую часть общего объема добычи Германской империи. Шахты Саарского угольного бассейна и группа шахт в Верхнесилезском бассейне, принадлежащие прусскому правительству, были единственными крупными государственными шахтами в мире, и теперь, согласно условиям Мирного договора, право собственности на Саарские шахты перейдет к Франции. (Подробности приведены на стр. 39).

С другой стороны, правительство осуществляло тихий, но реальный контроль над всей германской угольной промышленностью. Через владение шахтами Koenigen Louise оно действовало как член Верхнесилезского угольного синдиката. Ранее, через владение шахтами Саара, оно также было членом Вестфальского угольного синдиката, но, будучи членом или нет, оно практически одобряло операции синдиката и установление цен заранее; также оно сотрудничало с синдикатом при перевозке угля последнего по государственным железнодорожным системам. В некоторых неразработанных угольных бассейнах Германии, северном продолжении Вестфальского бассейна, прусское правительство сохраняет большинство прав на уголь.

Рейнско-Вестфальский угольный синдикат является классическим примером крупного взаимосвязанного торгового объединения. Капитализированный в 571 000 долларов, он покрывал огромную капитализацию отдельных членов. Шахты имеют голоса пропорционально добыче, которая, в свою очередь, ограничена на определенные периоды. Цены устанавливаются, и уголь продается для синдиката как единого целого, но другие дела оставлены компаниям. Синдикат в целом является членом транспортного и экспортного объединения и распоряжается своей продукцией через объединение угольных дилеров. Несколько мелких объединений взаимосвязаны и практически слиты в более крупную организацию — Kohlen Kontor. Таким образом, объединение обладало исключительной властью изучать различные проблемы отрасли и стало очень мощным. Оно поддерживает исследовательский отдел и галерею для испытания взрывов недалеко от Дортмунда. В ряде стран германские компании через контроль над рекламными контрактами смогли влиять на редакционную политику ведущих газет, даже во время войны. Более половины германского угля, добытого до и во время войны, было синдикатным углем. Все 600 других германских картелей не были столь умеренны в своих действиях и правилах, как угольный синдикат. Когда угольный синдикат, однако, в одно время обнаружил, что не может обеспечить свой германский рынок углем, сообщается, что он покупал низкосортный британский уголь для своих клиентов, чтобы они сами не получали хороший британский уголь и не отказывались возвращаться к германским поставкам.

Картелем предпринимались усилия по поглощению и контролю внешней торговли углем, где политические и финансовые причины делали это целесообразным, и поэтому эти усилия были совершенно несоразмерны внутренней ценности торговли. Когда планировалось захватить такую торговлю, использовалась изобретенная немцами система «демпинга», при которой уголь продавался за границей дешевле, чем его можно было продать или произвести дома, а разница покрывалась экспортными бонусами. Этот германский демпинг стал настолько серьезным в некоторых странах, таких как Канада, Новая Зеландия и Южная Африка, что были введены специальные импортные пошлины для противодействия ему. Когда это было желательно, синдикат приобретал угольные шахты за границей, включая даже завод в Южном Йоркшире в Англии, угольные шахты Гераклеи в Турции и многие шахты в Австралии.

В Великобритании существует мощное угольное объединение, Cambria, тесно связанное с крупными судоходными компаниями. Важным торговым активом в этой организации, как и в германском картеле, является банковская связь, благодаря которой объединение может предлагать долгосрочный кредит.

Угольные синдикаты упоминаются в Бельгии. Некоторая центральная организация, интересующаяся углем, известна в Италии, России, Австро-Венгрии, Швеции, Греции, Аргентине, Чили и Эквадоре.

СИТУАЦИЯ ВО ФРАНЦИИ, АНГЛИИ И СОЕДИНЕННЫХ ШТАТАХ

Франция имеет модифицированную форму собственности на угольные ресурсы: она принадлежала ранее Короне, а теперь Республике. Правительство предоставляет концессии на добычу полезных ископаемых и взимает роялти. Считается, что полезное ископаемое не принадлежит владельцу поверхности или первоначальному владельцу поверхности, как это имеет место во всех других важных странах. Предоставляемые концессии являются либеральными и на большие площади. Роялти или арендная плата невелика и в настоящее время выплачивается на основе определенной суммы за единицу площади (гектар) в концессии, но основные доходы, получаемые обществом, поступают через процент от чистой прибыли, то есть прибыли, доступной для дивидендов. В условиях, сложившихся во Франции, система кажется исключительно справедливой, и предприятия были прибыльными как для операторов, так и для страны. Книги компании открыты для проверки правительственными чиновниками, а годовые отчеты публикуются в деталях. Система фактически делает правительство партнером в бизнесе.

В Великобритании большая часть прав собственности на уголь принадлежит владельцам майоратных имений, а роялти составляют один шиллинг за тонну и выше.

В Соединенных Штатах существует как частная, так и государственная собственность. На большей части территории страны права на уголь принадлежат крупным эксплуатирующим компаниям, хотя в антрацитовом районе Пенсильвании удачливые владельцы поверхности земли или их правопреемники получают значительные роялти — от 25 до 50 центов за тонну. На Среднем Западе большинство операторов выкупили права на уголь у владельцев поверхности. При аренде роялти относительно невелики — от 2 до 6¹⁄₄ центов за тонну. Операторы в Скалистых горах, как правило, сами владеют добываемым углем. Правительство продало права на уголь, но государственные школьные земли в Колорадо и Вайоминге, как правило, сдавались в аренду с роялти около 10 центов за тонну. В Оклахоме «Пять цивилизованных племен» до недавнего времени под контролем правительства сдавали свои земли и права на уголь в аренду примерно по 10 центов за тонну, но сейчас эти права распродаются.

В штате Вашингтон значительная часть освоенного в настоящее время района битуминозного угля принадлежит компании Northern Pacific Railway, которая получила эти земли в качестве грантов при строительстве железной дороги. Роялти составляет около 15–25 центов за тонну.

На Аляске, в битуминозных месторождениях Матануска и Беринг-Ривер, а также в месторождении лигнита Ненана, правительство предложило уголь для целей аренды по 2 цента за тонну на первый период с ограничениями, предусматривающими рациональное использование угля и разумные цены для потребителей. Некоторые участки были освоены в месторождениях Матануска и Беринг-Ривер, но, поскольку пласты сильно деформированы, а угольные залежи трудно проследить, прогресс идет медленно, и добыча едва началась. Временно Комиссия по железным дорогам Аляски разрабатывает несколько шахт в Чикалуне и Эска-Крик, чтобы обеспечить поставки угля до начала разработки других шахт арендаторами. Конгресс, открывая угольные земли в месторождениях Матануска и Беринг-Ривер для аренды, зарезервировал участки площадью не более 7680 акров и 5120 акров соответственно для нужд Военно-морского флота.

Соединенные Штаты по-прежнему владеют обширными площадями земель с залежами угля и лигнита в западных штатах. Большинство этих земель удалены от железных дорог и труднодоступны, но они содержат огромные запасы. В настоящее время, за исключением Аляски, правительство сдает в аренду только одну шахту — шахту Гебо в Гебо, штат Вайоминг, но недавно было осуществлено расширение системы аренды, аналогичной той, что действует на Аляске.

В Соединенных Штатах антрацитовая промышленность хорошо организована, а ее связи с железными дорогами делают ее исключительно эффективной и мощной. Битуминозный уголь, напротив, настолько широко распространен как на государственных, так и на частных землях, что ни одна частная организация не пыталась взять отрасль под свой контроль. Подобный контроль всегда встречал противодействие со стороны Конгресса и широкой общественности.

За исключением периода войны, ни Великобритания, ни Соединенные Штаты не пытались осуществлять какой-либо контроль над коммерческой добычей и продажей угля. Каждая страна создала топливную администрацию, и уголь отгружался по указаниям правительства и оплачивался по ценам, установленным этой администрацией. В Соединенных Штатах этот государственный контроль практически исчез с окончанием войны, но в Англии «Угольный контроль» (Coal Control) пока сохраняется, и существует тенденция к тому, что правительство на данный момент сохранит сильное руководящее влияние на различные «ключевые» отрасли. Безусловно, в конечном счете, добыча угля является общественно значимой услугой, и правительство должно осуществлять соответствующий надзор и регулирование, оставляя при этом свободу для частной инициативы.

Из важных угледобывающих стран только Германская империя более или менее открыто поддерживала угольную промышленность в мирное время и в некоторой степени контролировала ее. Во Франции существовал лишь косвенный контроль через правительственный надзор за концессиями и налогообложение доходов, а также через негласное знание о деятельности французского угольного синдиката, который, по крайней мере внешне, занимается сбором и распространением информации и проводит расследования безопасности на шахтах. В Соединенных Штатах, Великобритании и других странах была разрешена свободная конкуренция. Свободная конкуренция не кажется серьезной проблемой в таких странах, как Франция, где запасы угля ограничены, но она имела более или менее серьезные финансовые последствия там, где запасы угля были очень велики. В Германии до формирования синдикатов в угольной промышленности были периоды перепроизводства и серьезной финансовой депрессии; в другие, более редкие периоды наблюдалось большое процветание. В Великобритании были похожие времена депрессии и процветания, но в целом бизнес был прибыльным.

В Соединенных Штатах, за исключением антрацитового района, где более двадцати лет операции находились в руках сравнительно немногих компаний, депрессия и процветание быстро сменяли друг друга. Статистические данные, полученные в ходе переписи, показывают, что средняя прибыль в битуминозной промышленности до 1917 года была меньше, чем в любой другой крупной отрасли, и это имело негативные последствия для оптимального развития угольных ресурсов. У компаний, как правило, было мало или совсем не было излишков для надлежащего развития в неурожайные годы; поэтому они добывали только лучший или самый толстый уголь, а в короткие периоды большого процветания многие шахты, не принадлежащие напрямую железным дорогам и сталелитейным компаниям, эксплуатировались так, что это приводило к «сжатиям» (squeezes) и большим потерям угля. Более того, эти условия были также неблагоприятны для рабочей силы; во времена процветания открывалось слишком много новых шахт из-за огромных и легкодоступных ресурсов, а во времена депрессии количество рабочих дней у шахтеров сокращалось настолько, что их ежемесячный или годовой заработок был достаточно низким, чтобы сделать их жизнь тяжелой. Среднее количество рабочих дней в году с 1901 по 1915 год составляло 213. Система ограниченного государственного контроля над торговыми объединениями представляется весьма выгодной как для операторов, так и для шахтеров и должна обеспечить стабильные поставки угля потребителям и стабильные цены при разумной прибыли.

Что касается торговых отношений между Соединенными Штатами и другими странами в отношении поставок топлива, то, за исключением возможного соглашения о невыплате субсидий судам, перевозящим уголь, любая попытка заключения общего соглашения по такой жизненно важной необходимости, как уголь, представляется неразумной, за исключением случаев предотвращения дублирования сложных установок для хранения и перевалки угля в портах, требующих небольших объемов, и предотвращения разорительной конкуренции путем систематического «демпинга» излишков угля с целью вытеснения конкурента с рынка.

Из всех континентов Южная Америка обладает наименьшими запасами угля. Хотя уголь есть в Бразилии, Чили и других южноамериканских странах, до него трудно добраться, и известные на данный момент месторождения не дают оснований полагать, что они смогут удовлетворить потребности стран, в которых они находятся.

Влияние войны на ситуацию с углем.

— Сразу после начала войны в Европе 31 июля 1914 года германские вооруженные силы атаковали и продвинулись на восток через российскую Польшу, быстро захватив важное Домбровское месторождение, которое является продолжением Верхнесилезских угольных бассейнов. Германские войска также продвинулись на запад через бельгийские угольные бассейны и далее через продолжение этих бассейнов на севере Франции, одновременно захватив важные месторождения железной руды Брие к северу от Вердена.

Экономический эффект от этих наступлений имел огромное значение, так как позволил захватить все продуктивные угольные шахты Бельгии, самые продуктивные угольные шахты России и большую часть угольных бассейнов северной Франции. Захваченные французские угольные и железные рудники производили половину добычи угля во Франции (20 миллионов тонн из 40 миллионов тонн) и 95 процентов (20 миллионов тонн) добычи железной руды. Естественно, в этих условиях Франция была вынуждена полагаться на Англию и Соединенные Штаты для удовлетворения военных и экономических потребностей в железе, опираясь главным образом на Великобританию в вопросе необходимых поставок угля. Великобритания во время войны продолжала поставлять уголь в Италию, а также в Испанию и другие нейтральные страны.

Перемирие положило конец германской оккупации угольных бассейнов Бельгии и северной Франции. С другой стороны, французы взяли под контроль важный Саарский угольный бассейн, а союзники оккупировали германскую территорию, доходящую до Рейна и за Рейн в некоторых предмостных укреплениях; эта оккупация включала надзор за шахтами в бассейнах угля и бурого лигнита близ Ахена и Кельна, а также на западной окраине Вестфальского бассейна на левом берегу Рейна.

Мирный договор передает французам важные железорудные ресурсы бывшей германской Лотарингии, которые вместе с импортом из французской Лотарингии были основными источниками железной руды для германских металлургических заводов, а также право собственности на Саарские угольные шахты.

Условия, на которых передаются Саарские шахты, и будущее управление этим районом указаны в следующих выдержках из договора:

«В качестве компенсации за разрушение угольных шахт на севере Франции и в качестве частичной оплаты общей суммы репараций, причитающихся с Германии за ущерб, возникший в результате войны, Германия уступает Франции в полное и абсолютное владение, с исключительными правами на эксплуатацию, свободными от всех долгов и обременений любого рода, угольные шахты, расположенные в Саарском бассейне».

Это исключает ту часть Саарского бассейна в Лотарингии, которая принадлежала Франции до 1870 года и которая теперь возвращается Франции с некоторыми незначительными исправлениями границы. Договор далее уточняет: «все залежи угля, расположенные в пределах Саарского бассейна, станут полной и абсолютной собственностью французского государства. * * * Право собственности французского государства будет применяться не только к залежам, которые являются свободными и на которые еще не были предоставлены концессии, но также и к залежам, на которые концессии уже были предоставлены, кем бы ни были нынешние владельцы, независимо от того, принадлежат ли они Прусскому государству, Баварскому государству, другим государствам или органам, компаниям или частным лицам. * * * Стоимость имущества, таким образом уступленного французскому государству, будет определена Репарационной комиссией. * * * Эта стоимость будет зачтена Германии в частичную оплату суммы, причитающейся в качестве репараций. Германия должна будет возместить убытки владельцам или заинтересованным сторонам, кем бы они ни были».

Что касается управления территорией Саара, то по истечении пятнадцатилетнего периода населению будет предложено выразить свои желания, и тогда «Лига Наций решит, под чей суверенитет будет передана территория, принимая во внимание пожелания жителей, выраженные путем голосования». В промежуточный период территория будет управляться комиссией из пяти членов, выбранных Советом Лиги Наций.

В дополнение к передаче права собственности на шахты и полезные ископаемые в Саарском бассейне, Германия предоставляет следующие опционы на поставку угля нижеуказанным подписантам настоящего договора:

«Германия обязуется поставлять Франции семь миллионов тонн угля в год в течение десяти лет (подразумевается, что это должно обеспечить топливом территорию Эльзас-Лотарингии, возвращенную Франции). Кроме того, Германия обязуется ежегодно поставлять Франции в течение периода, не превышающего десяти лет, количество угля, равное разнице между годовой добычей до войны угольных шахт Нор и Па-де-Кале, разрушенных в результате войны, и добычей шахт того же района в течение соответствующих лет; такая поставка не должна превышать двадцати миллионов тонн в любой год из первых пяти лет и восьми миллионов тонн в любой год из последующих пяти лет. Подразумевается, что будет проявлено должное усердие при восстановлении разрушенных шахт в Нор и Па-де-Кале».

Помимо снабжения Франции углем, «Германия обязуется поставлять Бельгии восемь миллионов тонн угля ежегодно в течение десяти лет»; Италии — от четырех с половиной до восьми с половиной миллионов тонн ежегодно; а также Люксембургу — «количество угля, равное довоенному годовому потреблению германского угля в Люксембурге».

Цены, которые должны быть уплачены за уголь по этим опционам, должны быть следующими:

(a) Для наземной доставки, включая доставку баржами, — германская цена у шахты для германских граждан плюс фрахт до французской, бельгийской, итальянской или люксембургской границ, при условии, что цена у шахты не превышает цену у шахты британского угля для экспорта. В случае бельгийского бункерного угля цена не должна превышать голландскую бункерную цену. Железнодорожные и баржевые тарифы не должны быть выше самых низких аналогичных ставок, действующих в Германии.

(b) Для морской доставки — германская экспортная цена франко-борт (f.o.b.) в германских портах или британская экспортная цена франко-борт (f.o.b.) в британских портах, в зависимости от того, какая из них ниже.

«Заинтересованные союзные и ассоциированные правительства могут потребовать поставки вместо угля металлургического кокса в пропорции 3 тонны кокса на 4 тонны угля».

Германия обязуется поставлять Франции в течение каждого из трех лет после вступления в силу настоящего договора,

Benzol | 35,000 | tons
Coal tar | 50,000 | tons
Sulphate of ammonia | 30,000 | tons

Цена, уплачиваемая за кокс и за упомянутые товары, должна быть такой же, как цена, уплачиваемая германскими гражданами при тех же условиях отгрузки.

Право собственности на Саарские шахты является весьма желанным дополнением к угольным ресурсам Франции; и Саарский бассейн, поскольку он способен к дальнейшему развитию, может в будущем сделать Францию более самодостаточной в отношении добычи угля.

Требование поставлять уголь Франции во время восстановления французских шахт, разрушенных немцами, является весьма справедливым соглашением. Германия поначалу, из-за падения добычи в Вестфальских бассейнах, заявляла, что не может поставлять уголь, но эта ситуация, несомненно, со временем исправится, тем более что Франция держит козыри в руках благодаря контролю над железными рудами, необходимыми для крупных металлургических и сталелитейных заводов Рейнского района. Тем временем есть надежда, что Великобритания при содействии Соединенных Штатов сможет восполнить дефицит в потребностях в угле.

Проблемы, связанные с российскими угольными бассейнами, сложны, но, по крайней мере, Домбровский угольный бассейн, по-видимому, находится в руках новой Польши, и это дает угольные ресурсы, оцениваемые в 2525 миллионов тонн, с добычей до войны, вероятно, превышавшей 7 миллионов метрических тонн в год.

Согласно условиям мирного договора, плебисцит определит политический контроль над Верхнесилезскими угольными бассейнами.

Вероятные изменения в торговле углем.

— В мировой морской торговле углем наиболее вероятным изменением является то, что Соединенные Штаты будут в большей степени снабжать Южную Америку, причем их уголь будет замещать уголь Великобритании. Океанское расстояние заметно в пользу Соединенных Штатов, особенно на западном побережье Южной Америки для судов, проходящих через канал. Учитывая расширение судоходных возможностей Соединенных Штатов, есть все основания полагать, что экспорт угля в Южную Америку будет поровну разделен между Соединенными Штатами и Великобританией.

В настоящее время очевидно, что британская угольная промышленность находится в тяжелом положении, и публицисты выражают серьезную тревогу по поводу возможной потери большей части экспортной торговли и сокращения внутренних отраслей из-за значительного снижения добычи, сопровождающегося быстрым ростом себестоимости.

В 1913 году Великобритания добыла 287 000 000 длинных тонн и экспортировала 77 000 000 длинных тонн угля. Во время войны, из-за большого числа шахтеров, ушедших на военную службу, добыча значительно сократилась, но ожидалось, что она быстро восстановится с подписанием перемирия и возвращением шахтеров. Однако рабочие волнения, приведшие к забастовкам и прогулам, сдерживали добычу, и 16 июля 1919 года вступило в силу так называемое решение Сэнки (Sankey award). Это решение сократило рабочий день шахтеров с восьми до семи часов, исключая время, затрачиваемое на подъем и спуск, но включая время, затрачиваемое на дорогу до рабочего места. Ставки были повышены так, что шахтер получал за день при семичасовом рабочем дне больше, чем раньше при восьмичасовом, а Контролер повысил цену на уголь на шесть шиллингов за тонну, чтобы компенсировать возросшие расходы.

Сэр Ричард Редлэнд, главный инспектор шахт, предсказал, что добыча в 1919 году составит 230 000 000 тонн, а в 1920 году — 217 000 000 тонн, что на 70 000 000 тонн меньше, чем добыча 1913 года. По-видимому, со временем, используя дополнительные смены, Великобритания может восстановить свою прежнюю добычу, хотя, очевидно, при значительно возросших затратах; так что если стоимость в Соединенных Штатах не вырастет соответственно, есть все шансы, что эта страна сможет успешно конкурировать в экспортном бизнесе не только в Южной Америке, но и в портах Средиземноморья.

В настоящее время спрос на уголь поступает в Соединенные Штаты не только из этих частей света, но и из Скандинавии, Швейцарии, Дании и Нидерландов. Однако из-за близости Великобритания должна быть в состоянии взять на себя топливные потребности Северной Европы.

В Тихом океане маловероятно, что ни штат Вашингтон, ни территория Аляска будут производить уголь в таком количестве и по такой цене, чтобы добыча могла стать общим фактором в торговле на Тихоокеанском побережье. Потребности Аляски, Вашингтона и прилегающих штатов поглотят местную добычу; а Калифорния продолжит импортировать в балласте больше или меньше угля с острова Ванкувер, из Британской Колумбии, Китая, Японии, Новой Зеландии и Австралии.

Непосредственные изменения в Азии, скорее всего, будут связаны с развитием шахт во внутренних районах Китая и в Индии для удовлетворения внутренних потребностей, а не с масштабным экспортом, хотя, как уже говорилось, возможно, что Китай постепенно выйдет на рынки Тихоокеанского побережья.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ НАЦИЙ

Соединенные Штаты.

— Соединенные Штаты обладают лучшими запасами угля среди всех стран — около 3 527 000 миллионов из общего мирового запаса в 7 900 000 миллионов тонн — и хорошими запасами каждого из нескольких классов угля. В течение многих лет не будет опасности дефицита, за исключением антрацита, хорошего коксующегося угля и высокосортного энергетического угля, которые сейчас активно добываются. Около 600 000 000 тонн в год, или почти 40 процентов мировой годовой добычи, добывается в Соединенных Штатах.

В отличие от запасов и добычи, экспорт в 1913 году составлял лишь около 12 процентов от экспорта угля из всех стран; и большая часть американского экспорта идет в Канаду по железной дороге. Морским путем Соединенные Штаты отправили лишь 4 процента. Эта небольшая доля в международной торговле объясняется удаленностью нашего угля от морских портов, отсутствием организации и соответствующих судоходных организаций; и, кроме того, относительной независимостью Соединенных Штатов, которым из большинства стран требуется лишь небольшое количество импорта в качестве обратного груза для судов, перевозящих уголь. Мы используем наш уголь дома, но преимущество экспорта значительного количества угля для его влияния на расширение торговых отношений с другими странами становится сейчас очевидным.

С большими запасами и малым экспортом угля коррелирует замечательное развитие внутренних отраслей промышленности, использующих наш собственный уголь. Судя по кривым добычи (показанным на рисунке 3), кажется, что в течение столетия Соединенные Штаты превзойдут всю Европу по добыче угля. Поскольку наши отрасли промышленности шли в ногу с добычей угля, наше потребление угля примерно отражается кривой добычи. Следовательно, кажется, что Соединенные Штаты, вероятно, станут центром производства и богатства; и с этим придет столь же определенный постоянный рост населения и мощи.

Вторым великим мировым источником угля, вероятно, станет Китай. Конечно, европейская добыча велика, но она будет разделена между несколькими державами. Основная часть мировой энергии и промышленности на следующее столетие настолько определенно локализована угольными месторождениями (и в большинстве случаев сопутствующим железом), что роль, которую Соединенные Штаты должны играть в мировой программе, ясна. Следует соблюдать всяческую осторожность, чтобы китайские ресурсы контролировались державами, которые не будут злоупотреблять ими, чтобы сделать мир «небезопасным для демократии».

Война открыла несколько иностранных рынков, особенно в Южной Америке, для угля из Соединенных Штатов. Некоторые из этих рынков могут стать постоянными, но валлийский уголь, скорее всего, по-прежнему будет доминировать в морской торговле. У Соединенных Штатов есть угольные станции так далеко, как Манила и острова Самоа, но мало угля доходит до них из этой страны. Американский уголь снабжает наши правительственные угольные станции на Аляске; Гавайи; наши внутренние порты, как на Атлантике, так и на Тихом океане; Кубу; Пуэрто-Рико; никарагуанские порты; порты Панамского канала; Масатлан, Мексика; и некоторые южноамериканские порты. По-видимому, не было предпринято никаких попыток создать стратегические порты по всему миру, которые могут потребоваться, если нынешний рост американского судоходства должен поддерживаться под американским флагом.

Никакой иностранный контроль не оказывал влияния на добычу или обработку угля в Соединенных Штатах. Владение угольными шахтами иностранцами было возможно, но, по-видимому, не стало значительным.

Американские угольные ресурсы настолько велики, что ни одна отдельная организация, иностранная или отечественная, не смогла доминировать в этой ситуации. Отсутствие сильного торгового объединения позволило (в 1916 году) комбинации британских грузоотправителей установить цену на бункерный уголь в атлантических портах, так что шахты получали за него даже меньше, чем за промышленный уголь. Это было результатом конкурентных торгов и отсутствия организации здесь, но ожидается, что организация теперь будет развиваться.

С начала войны развитие отраслей промышленности, основанных на каменноугольной смоле, было замечательным. Однако есть признаки нездоровой конкуренции в этой стране, и правительство должно быть осторожным, чтобы внутренние распри снова не открыли дверь для германского контроля.

Англия.

— Британские острова имеют лишь одну сороковую часть от общего мирового запаса угля, но он лучшего, чем в среднем, качества. Высокосортный энергетический уголь в изобилии, и есть достаточный запас коксующегося угля. Годовая добыча, 300 миллионов тонн, составляет около одной пятой мировой добычи и уступает только Соединенным Штатам. Англия до войны экспортировала около одной четверти добычи, причем зарубежный экспорт из Англии был в шесть раз больше, чем из любой другой страны мира. Уголь составлял около трех четвертей всего английского экспорта. Угольные шахты находятся недалеко от морских портов, и ставки океанского фрахта низки, потому что спрос на импорт дает обратные грузы в Англию со всех частей света. Большие запасы угля есть также в колониях, особенно в Индии, Австралии и Южной Африке.

Угольный бизнес и судоходство Великобритании развивались вместе. Около одной четверти отгружаемого угля идет на бункеровку. В 1916 году Англия владела 40 процентами мирового судоходства и экспортировала почти 70 процентов мирового морского угля. Поддержание судоходства требует бункеровочных портов по всему миру. Угля из Уэльса и британских колоний было достаточно, чтобы снабжать их все, и они составляют, безусловно, самую стратегическую систему, которой обладает любая страна.

Англия, Гибралтар, Греция, Мальта, Суэц, Порт-Саид, Аден, Маскат, Коломбо, Сингапур, Бомбей, Гонконг, Шанхай, Сидней, острова Фиджи, Ванкувер, Вальпараисо, Сент-Люсия, Ямайка, Галифакс, Ньюфаундленд, остров Святой Елены, Бермудские острова, Кейптаун и Дурбан и другие опоясывают земной шар. Франция, Япония, Голландия и Соединенные Штаты имеют по несколько станций, но нет такой всеобъемлющей системы. Германские предложения условий мира (во время войны) признавали важность этих станций, указывая, что Англия должна отказаться от Адена, Мальты и подобных портов.

Торговые соглашения между Великобританией и другими странами были таковы, что предоставляли режим «наибольшего благоприятствования» обеим сторонам, даже с Германией, где не действовал никакой формальный договор. Политика свободной торговли Англии хорошо установлена, и на этой основе коммерческий рост Англии был очень велик. Исследования, проведенные после начала войны, показывают, что Германия воспользовалась свободой в британских странах и защитой у себя дома. Например, германский капитал контролировал некоторые угольные шахты в Южном Йоркшире через г-на Стиннеса, одного из крупнейших компонентов германского Kohlen Kontor. Эта организация имела филиалы в Ньюкасле, Кардиффе, Глазго, Халле и многих иностранных портах. Французы также приобрели английскую угольную шахту до войны — угольную шахту Стоунхолл в Лиддене, недалеко от Дувра.

Австралийские колонии и, вероятно, другие обнаружили, что германские финансисты владели и контролировали большинство шахт, когда разразилась война. Потребовалось некоторое время, чтобы уничтожить это влияние. В начале войны британские настроения, казалось, призывали к действиям против всей такой германской коммерческой агрессии, и на Союзной экономической конференции в Париже в июне 1916 года были предложены планы защиты посредством тарифов и исключения иностранной собственности в союзных странах. Совсем недавно, кажется, британский план состоит в том, чтобы сохранить за британцами определенные ключевые отрасли любой ценой и при любых затратах, но не отказываться от свободной торговли и никоим образом не уменьшать объем торговли.

Коммерческий контроль над экспортной торговлей валлийским энергетическим углем в значительной степени находится в руках Cambria Coal Combine, но в этой торговле есть несколько других крупных объединений. Антрацитовая промышленность Англии не так хорошо организована, как американская.

Коммерческий контроль над углем, экспортируемым из Уэльса, в значительной степени находится в руках крупных объединений британских грузоотправителей, по соглашению с Cambria. Даже когда война мешала судоходству, по оценкам, две трети южноамериканской торговли углем находились под британским контролем.

Многочисленных примеров британского финансового контроля над углем в странах, отличных от британских колоний, не отмечалось. Британский капитал инвестирован в несколько шахт в Сибири, и существуют обширные владения в Китае.

Германия.

— Запасы угля в Германии до войны были больше, чем в Англии, если считать возможные запасы, и были хорошего качества. Германия ранее контролировала 70 процентов угля на континенте. Австрийский уголь контролировался, и на уголь Шпицбергена были заявлены права, хотя сейчас он находится под британским и норвежским контролем.

Хотя самые важные месторождения коксующегося угля на континенте находятся в Вестфалии, месторождения Бельгии и северной Франции очень важны для общего контроля над ситуацией с углем. Нельзя предположить, что эти важные угольные бассейны были захвачены немцами по другим причинам или что немцы включили уголь и железо случайно. В 1911 году Rhenish Westphalian Zeitung советовала, чтобы французская Лотарингия и Люксембург были подчинены так же тщательно, как Вестфалия. В 1915 году шесть величайших ассоциаций деловых людей в Германии подали петицию Канцлеру с просьбой рассмотреть контроль над углем (и железом) северной Франции как военную, так и экономическую необходимость.

Годовая добыча угля в Германии до войны составляла около одной пятой общего мирового объема, вплотную приближаясь к добыче Великобритании. В первые годы войны добыча угля несколько снизилась. По экспорту угля Германия уступала только Британским островам, но ни одна страна не экспортирует морским путем и одной шестой того, что экспортирует Великобритания. До войны Германия основала около четырнадцати «Kohlen depots» за рубежом и имела большое количество судов. Эти бункеровочные порты были захвачены союзниками.

Примером германского промышленного проникновения является случай с Киао-Чау, Китай. В 1899 году в Берлине была сформирована Shantung Eisenbahn Gesellschaft со штаб-квартирой в Циндао. Она получила исключительные права на 5 лет на поиск полезных ископаемых в зоне 10 миль по обе стороны железной дороги и на приобретение заявок. Китайским шахтам не разрешалось применять современные методы и конкурировать, если они не покупали германские материалы и не нанимали германских специалистов. Разработанные шахты производили хороший пароходный уголь и достаточно хороший кокс, так что планировалась доменная печь. Немцы потеряли контроль, когда разразилась война, и эти права перешли, согласно условиям мирного договора, к Японии. Германский капитал, который был инвестирован несколько лет назад в Chung Hsing Coal Co., был выкуплен в 1908 году.

Франция.

— До войны Франция занимала пятое место в списке мировых производителей угля, но в течение многих лет нуждалась в большем количестве угля, чем производила. Возможно, во Франции можно было бы добывать достаточно угля при больших разработках, но импортировать его было дешевле. Французский капитал был инвестирован в некоторые иностранные угольные месторождения. Компания под французским контролем владела угольной шахтой Стоунхолл, недалеко от Дувра. До войны французская компания была одним из крупнейших операторов в Турции и постоянно приобретала новые шахты. Французская компания владела важной угольной шахтой в Домбровском бассейне, ныне части Польши.

Франция поддерживала правительственные угольные станции для судоходства в Индокитае, на Таити, островах Общества, Мартинике и Мадагаскаре; но не предпринималось попыток снабжать их полностью французским углем или быть независимыми от других угольных станций.

Италия.

— Италия имеет скудные запасы низкосортного угля, и нормальная добыча незначительна. Импорт был большим, причем поставки из Великобритании в 1914 году составили 10 000 000 тонн.

Россия.

— Россия имеет несколько важных угольных бассейнов. Добыча составила 31 000 000 тонн в 1915 году и 23 000 000 тонн в 1916 году, так что Россия, включая провинцию Украина, занимала пятое или шестое место среди мировых производителей. Если спрос на уголь вырастет под влиянием промышленной стабильности, вся добыча будет потребляться в России. Около двух третей добычи было получено в Донецком бассейне. Половина этого — коксующийся уголь.

Япония.

— Япония имеет на главном острове Хонсю достаточно угля, чтобы позволить значительный экспорт. Запасы в Корее и на Формозе менее обильны. Во всем японском угле очень мало угля хорошего коксующегося качества.

Когда война сократила количество британских судов в северной части Тихого океана, японские суда поставляли японский уголь на ряд новых угольных станций, и британцам может быть трудно вернуть свое прежнее положение в бункеровке там. Японский уголь теперь доходит также на запад до Коломбо, Цейлон.

Японское законодательство предписывает японский контроль над политикой горнодобывающих компаний, хотя допускаются некоторые иностранные финансовые интересы. Япония контролирует часть угля, добываемого в Китае, и, предъявляя настойчивые требования, усиливает свой контроль в этой стране. Если ей дать свободу действий, Япония будет в состоянии осуществлять промышленный и военный контроль в Азии почти так же тщательно, как Соединенные Штаты могут в Америке. Английские и бельгийские интересы имеют некоторое количество китайского угля и, таким образом, являются единственной реальной конкуренцией в настоящее время японскому контролю.

Китай.

— За пределами Соединенных Штатов Китай обладает самыми большими запасами угля среди всех стран мира. Уголь различается по качеству и сорту; часть его превосходна, но добыча достигла лишь около 18 000 000 тонн в год. Некоторые районы экспортируют, а другие импортируют уголь. Страна могла бы легко быть независимой, если бы были внутренние средства распределения. Мог бы быть даже большой экспорт, если бы добыча началась до другого промышленного развития. Коксующийся уголь доступен только в определенных районах, в основном на юге.

Крупнейшим и лучше всего оснащенным производителем является Kailan Mining Administration, управляющая британскими и китайскими объектами. Собственность компании в основном находится в бельгийских руках, но регистрация осуществлена по законам Гонконга, так что компания находится под британским контролем.

Основные производители в Китае:

Таблица 6. — Основные производители угля в Китае

Company | Tons a year | Control
Kailan Mining Administration | 3,000,000 | British and Chinese
Funshun Collieries | 2,000,000 | Owned by the South Manchuria Railway Co. (Japanese)
Pingshieng Collieries | 1,000,000 | Chinese
Pekin Syndicate | 500,000 | British
Pingshihu | 300,000 | Japanese
Lincheng | 800,000 | Belgian

Горнодобывающая компания Шаньдуна, производящая 400 000 тонн в год, ранее принадлежавшая немцам, теперь управляется японской военной организацией. Таким образом, только один из крупных производителей находится под китайским контролем, хотя многие мелкие шахты разрабатываются китайцами. Китайский закон, призванный предотвратить иностранный контроль такого рода, неэффективен. Он требует, чтобы доля в горнодобывающей промышленности, принадлежащая иностранцам, была не более половины; но если иностранная компания владеет половиной акций и финансирует китайскую половину за счет займа, иностранный контроль может быть полным. Существует дальнейший контроль над добычей через владение железными дорогами. Все крупные производители должны отгружать уголь по железной дороге, а иностранным государствам разрешено финансировать железные дороги. Трудность осуществления правительством адекватного политического и коммерческого контроля, когда оно предоставляет концессии таким образом, очевидна.

Общие горнодобывающие дела в Китае контролируются Бюро горнодобывающих дел. Любое конкретное предприятие контролируется комиссаром по финансам в каждой провинции. Однако сомнительно, будет ли правительственный контроль достаточно сильным, чтобы перевесить коммерческий и финансовый контроль и дипломатическое давление извне. Те компании, которые зарегистрированы по законам Гонконга, могут рассчитывать на британскую защиту. Японские требования к Китаю были очень настойчивыми, и говорят, что около трети добычи в стране сейчас контролируется Японией.

В целом, Китай, кажется, принимает небольшое участие в контроле над своим собственным углем. Возможность для других держав получить финансовые, а через это и промышленные выгоды, может быть вовлечена в проблему финансирования центрального правительства.

Таблица 7. — Добыча, экспорт и импорт за 1913 год [8] Миллионы метрических тонн

Country | Kind of coal | Production | Exports | Imports | Remarks (1919)
United States | Anthracite |  85   |  4.1 | ... | Resources greater than those of any other country; can easily increase ocean exports with more shipping available. Present exports chiefly to Canada. Value of coal-tar products imported in 1913, $10,962,000.
Bituminous | 432   | 18.0 |  1.4
Coke |  42   |  1.0 |  0.1
Bunker coal | ... | (7.7) | ...
Great Britain | Anthracite |   5   | ... | ... | Chief coal-exporting country; before war had virtual monopoly of ocean exports. Export control imperiled by shortage from labor conditions.
Bituminous | 282   | 73.4 | ...
Coke |  20.5 |  1.2 | ...
Briquettes | ... |  2.1 | ...
Bunker coal |  | (21.0) | ...
German Empire | Bituminous | 191   | 34.6 | 10.5 | Coal needed for Central Europe. Exports by rail and canal. Distance from seaports prevents oversea exports. Westphalia has largest coking coal resources in Europe. Ownership of Saar mines transferred to France by Treaty of Peace.
Lignite |  87   | ... |  7  
Coke |  32   |  6.4 |  0.6
Coal Briquettes |   5.8 |  2.3 |  0.3
Lignite Briquettes |  21.4 |  0.9 |  0.1
Saar District (Included under German Empire, above) | Bituminous |  17.0 |  |
Coke |   2.0 |  |
Upper Silesia (Included under German Empire, above) | Bituminous |  49.1 |  |  | Nationality of Upper Silesia to be determined by plebiscite; coal production vital to eastern Germany, Poland and Austria.
Lignite |   2.3 | ... | ...
Coke |   3.1 | ... | ...
Austria-Hungary | Bituminous |  17.6 |  0.7 | 13.7 | Austria, already deficient in bituminous coal, under the Peace Treaty loses practically all coal fields to Poland and Czecho-Slovakia.
Lignite |  36.4 |  7.0 | ...
Austria (Included under Austria-Hungary, above) | Bituminous |  16.3 | ... | ... | Hungary always lacked enough bituminous coal, and under any political control must continue to import coal from Upper Silesia.
Lignite |  27.4 | ... | ...
Coke |   2.6 | ... | ...
Hungary (Included under Austria-Hungary, above) | Bituminous |   1.3 |  |  |
Lignite |   9.0 |  |
Coke |   0.2 |  |

France
Bituminous
 40.0
 1.3
18.7
France consumed in 1913 (millions of tons)

Coal
51.2

Coke
6.9

Briquettes
4.8

62.9

Deficit 21 millions tons in 1913. Addition of Saar production (17,000,000 tons) will not cancel the deficit, as the needs of the local district and those of former German Lorraine will absorb that or more. Mines wrecked by Germany produced 20,000,000 tons; Germany to supply equivalent amount until mines rehabilitated. France must continue indefinitely to import coal and coke.

Lignite |   0.8 | ... | ...
Coke |   4.0 |  0.2 |  3.0
Briquettes |   3.7 |  0.1 |  1.1
Russia (Included in above is the Dombrova field of Poland) | Bituminous chiefly |  32.3 | ... |  8.1 | Russia, with poorly developed fields and great future needs, has imported from Great Britain and Germany; through loss of the Dombrova field (extension of Upper Silesian basin) needs more coal than can produce and is unlikely ever to be an exporting country.
Bituminous (Some brown coal) |   7.0 |  |
Belgium | Bituminous |  22.8 |  4.9 |  8.9 | Belgium has high-grade steam coals and some coking coal; beds are deep and difficult to mine. Its exports to Holland and France probably will in future continue to be exceeded by imports from Westphalia and Great Britain.
Coke |   3.5 |  1.1 |  0.4
Briquettes |   2.6 |  0.6 |  1.1

[8] Составлено Джорджем С. Райсом.

Таблица 8. — Страны Европы, в значительной степени зависящие от импорта топлива. Добыча и импорт, 1913 [9] Миллионы метрических тонн

Country | Kind of coal | Production | Imports | Remarks (1919)
Holland | Bituminous | 2.0 | 12.0 | Holland, in the small Limbourg basin, has an extension of the Aix-la-Chapelle basin of Germany. The output is increasing, but as the basin is small Holland will import from Westphalia, Belgium and Great Britain or America.
Italy | Anthracite and Lignite | 0.7 | 10.  | Italy has insignificant and poor resources in thin anthracite beds and in lignite deposits; has depended on Great Britain for imports, but now the United States is furnishing some coal. Water-power developments are large; opportunity for further development.
Spain | Bituminous | 4.3 |  3.6 | Spain has a number of small coal basins. It must continue to import.
Sweden | Bituminous | 0.4 |  4.8 | Sweden has a few thin impure beds, but has relied on imports from Great Britain.
Norway |  |  |  2.3 | Norway has no coal resources and has imported coal from Great Britain.
Switzerland |  |  |  1.6 | Switzerland has no coal worthy of mention; it has relied on imports from Westphalia. Since the armistice, Switzerland has imported coal from the United States, but this movement is abnormal.

[9] Составлено Джорджем С. Райсом.

Выводы.

— Что касается политического контроля, то три великих национальных или расовых фактора вырисовываются в будущем угольной промышленности и в развитии богатства и мощи: европейский, в котором доминирует Англия; американский, в котором доминируют Соединенные Штаты; и азиатский, в котором доминирует Япония. Усилия Англии во время войны временно обескровили ее и уменьшили хватку ее экспортной угольной и бункеровочной торговли, но условия в конце 1919 года указывали на то, что восстановление может быть быстрым. Однако немедленный рост добычи угля для использования дома, с последующим прогрессом в сталелитейной и других отраслях, будет наибольшим в Соединенных Штатах из-за наших гигантских ресурсов. На Востоке, однако, есть признаки развития китайского угля и роста сопутствующих отраслей в масштабах, которые со временем могут превзойти таковые любой страны, кроме Америки, и перенести основную часть богатства и мощи к двум великим цивилизациям по обе стороны Тихого океана — новейшей, американской, и старейшей, китайской и японской. Война и урегулирования после войны оказались для Японии чистым благом и возможностью и позволили ей настолько укрепиться в Китае и Корее, что она является не только преобладающей державой на Востоке, но может претендовать на сферу влияния и широкий протекторат над Азией, гораздо более эффективный, чем американская Доктрина Монро.

Принимая во внимание национальную внутреннюю экономику, а также внешнюю и внутреннюю эффективность, Соединенные Штаты явно пренебрегут основной функцией правительства, если не будут осуществлять эффективный надзор и регулирование угольной промышленности. Эта отрасль является национальной; каждый гражданин имеет в ней интерес и право ожидать ее управления для высшего блага всех.

Таблица 9. — Добыча и импорт топлива южноамериканскими странами в 1913 году [10] Миллионы метрических тонн

Country | Production | Imports | Remarks (1919)
Argentina |  | 4.0  | Argentina has no coal resources. Imports chiefly from Great Britain; Cardiff coal.
Brazil |  | 2.2  | Brazil has coal, but it is inaccessible for transportation.
Chile | 1.23 | 0.6  | Chile has some coal, but does not mine enough high-grade coal for its needs; has imported from Great Britain.
Colombia |  |  | Colombia has some undeveloped coal resources; has imported a little coal from time to time from the United States.
Peru | 0.28 | 0.02 | Peru has small coal resources and mines a little coal, practically enough for its needs.
Uruguay |  | 0.8  | Uruguay has no coal resources and imported some in the past, chiefly from Great Britain.
Total South America | 1.51 | 7.6  |

[10] Составлено Джорджем С. Райсом.

Таблица 10. — Добыча, экспорт и импорт угля в 1913 году основными странами Азии и Австралии [11] Миллионы метрических тонн

Country | Kind of coal | Production | Exports | Imports | Remarks (1919)
Japan | Bituminous | 21.8 | 3.5 | ... | Japan does not have large coal resources and coal is not of high grade, but deposits are advantageously located for exporting.
India | ... | 16.5 | ... | ... | India has considerable good coal, but this will be needed for domestic purposes and bunkering.
China | Bituminous | 14.0 | ... | about 2.0 | Coal is imported from Japan, but China has great coal resources, and these are being developed by Japanese, British and American capital. Germany had large interests, which have reverted, it is understood, to Japan.
Indo-China | ... |  0.4 | ... | ... | Indo-China has some coal, both anthracite and lignite.
Siberia | ... | ... | ... | ... | Little is known of the coal resources of Siberia. There are many indications of lignite deposits.
New South Wales | ... | 10.5 | 6.0 | ... | New South Wales has large resources of good coal. One-half of the 6 million tons exported goes to other Australian states; the other half to Pacific ports.
New Zealand | ... |  1.9 | ... | ... | New Zealand has small coal basins, but they are close to the sea, permitting ready export.
Queensland | ... |  1.1 | ... | ... | Queensland, Victoria, and Western Australia have considerable coal resources, but not of grade or quality to be a factor in export trade.
Victoria | ... |  0.6 | ... | ...
Western Australia | ... |  0.3 | ... | ...

[11] Составлено Джорджем С. Райсом.

ГЛАВА III ЖЕЛЕЗО Э. К. Хардер и Ф. Т. Эддингфилд

ИСПОЛЬЗОВАНИЕ ЖЕЛЕЗА

Использование железной руды настолько хорошо известно, что их перечисление вряд ли необходимо. Из железной руды производят чугун, ковкое железо и сталь. Путем добавления одного или нескольких других элементов, главным образом кремния, углерода, хрома, никеля, марганца, ванадия, серы и фосфора, в количествах менее 5 процентов и обычно менее 1 процента, можно контролировать и придавать чугуну или стали в желаемой степени различные качества, такие как твердость, вязкость, эластичность, долговечность, хрупкость, плотность, пористость, выносливость, сопротивление окислению или коррозии, ковкость и плавкость.

Использование продуктов железной руды настолько распространено, что трудно найти предметы, которые не содержали бы их в той или иной форме. Помимо использования в качестве металла, железо входит в состав красок (особенно красных, желтых и синих), химикатов различных видов, лекарств, красящих веществ в стекле и керамике, а в форме зеркального гематита оно используется в ювелирных изделиях. Значительное количество железной руды также ежегодно потребляется в качестве флюса при плавке серебряных, медных, свинцовых и других металлосодержащих руд.

Железо и его продукты используются шире, чем любой другой металл; и годовое производство чугуна составляет от 94 до 96 процентов от общего количества всех металлов, производимых в мире, и в нормальное время в среднем составляет около 80 000 000 тонн ежегодно.

ГЕОЛОГИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Железные руды связаны со многими различными классами горных пород — осадочными, магматическими и метаморфическими. Там, где они связаны с осадочными породами, руды могут быть результатом прямого осаждения или могут быть более поздними замещениями осадочных пластов магматическими или метеорными железосодержащими водами. Многие месторождения железных руд, связанные с осадочными породами, образовались путем обогащения исходных железосодержащих пластов либо путем растворения и транспортировки соединений железа, либо путем удаления других сопутствующих минеральных компонентов.

Среди тех важных месторождений железных руд осадочного происхождения, которые претерпели незначительное или вообще не претерпели дальнейшего обогащения после отложения, за исключением, возможно, непосредственно на поверхности, можно назвать железные руды типа Клинтон в восточной части Соединенных Штатов, железные руды Вабана в Ньюфаундленде, «минеттовые» руды Лотарингского района на севере Франции, в Люксембурге и южной Германии, оолитовые пласты сидерита в районе Кливленда на севере Англии и гематитовые руды Минас-Жерайс в Бразилии. Наиболее важными из осадочных железных руд, которые являются результатом дальнейшего обогащения после отложения, являются руды района озера Верхнее в Соединенных Штатах.

Железные руды, связанные с магматическими породами, в основном имеют глубокое происхождение, обычно образовавшись из растворов, которые сопровождали или следовали за внедрением пород, с которыми связаны руды. Эти руды делятся на два основных класса: (1) Связанные с кремнистыми магматическими породами; и (2) связанные с основными магматическими породами. Руды, связанные с кремнистыми магматическими породами, состоят либо из гематита, либо, чаще, из магнетита. Они встречаются в граните, сиените и монцоните, а также в гнейсе, полученном из них в результате метаморфизма. Многие важные месторождения руд в разных странах принадлежат к этому классу, среди них магнетитовые и гематитовые месторождения шведской Лапландии и центральной Швеции, магнетитовые тела Адирондака и северного Нью-Джерси в восточной части Соединенных Штатов, различные магнетитовые и гематитовые тела в Калифорнии и других местах в западной части Соединенных Штатов, смешанные гематитовые и магнетитовые месторождения южного побережья Кубы, большинство тел железной руды в Чили и недавно освоенные железные руды Маньчжурии. Как класс, железные руды, связанные с кремнистыми магматическими породами, занимают второе место по важности после железных руд осадочного происхождения.

Месторождения железных руд, связанные с основными магматическими породами, почти все относятся к особому типу, известному как титаномагнетиты. Эти руды состоят из смеси магнетита и ильменита в различных пропорциях и поэтому содержат переменное количество титана. Многие крупные месторождения руд этого класса найдены в разных частях мира, среди наиболее крупных — определенные рудные тела в Вайоминге, в районе Адирондака и других местах в Соединенных Штатах, а также несколько месторождений в Норвегии и в северной и южной Швеции.

Важная группа месторождений железных руд возникла в результате минерального замещения вдоль контакта осадочных пород с магматическими интрузиями. Эти руды обычно встречаются в известняках недалеко от интрузивных масс гранита, монцонита, сиенита или диорита, но могут быть найдены и внутри самих магматических пород, вблизи контакта. Они редко связаны с более основными магматическими породами. Эти руды известны как магматические контактные руды, и их происхождение приписывается железосодержащим растворам, которые сопровождали или следовали за внедрением магматических пород, с которыми связаны руды. Такие руды чрезвычайно широко распространены, встречаясь практически на каждом континенте. Локально существуют обширные месторождения, как в районе Корнуолл в Пенсильвании, в западной части Соединенных Штатов и Британской Колумбии, в Чили, а также в Китае и Японии. Однако магматические контактные руды дали лишь относительно небольшой процент от общего мирового производства железной руды.

Существуют также широко распространенные месторождения замещения в осадочных породах, которые не связаны с магматическими породами. Считается, что они образованы обычными метеорными водами, которые растворяют рассеянные минералы железа из определенных пластов или масс породы и переотлагают минерал в другом месте в более концентрированной форме. Такие месторождения руд могут быть грубо пластообразными и напоминать пластовые месторождения, или они могут быть очень нерегулярными. Большинство месторождений этого типа состоят из сидерита, который заместил известняк, но существуют также месторождения гематита и лимонита, образованные замещением. Среди важных месторождений этой группы — сидеритовые руды Бильбао, Испания, в значительной степени измененные в лимонит вблизи поверхности; сидеритовая руда Эйзенерца, Штирия; и гематитовые месторождения близ Хартвилла, Вайоминг. Небольшие месторождения сидерита, гематита и лимонита этого типа найдены во многих частях мира.

Помимо уже упомянутых классов железных руд, широко распространенные железные руды встречаются как остаточные продукты, полученные в результате выветривания либо магматических, либо осадочных пород. Эти руды были образованы путем концентрации железосодержащих материалов, первоначально рассеянных в породах, продуктами выветривания которых они сейчас являются. Они в основном находятся в форме лимонита и встречаются либо как крупные тела относительно чистой руды, либо как агрегаты нерегулярных масс различных размеров, заключенных в глинах. К этому классу относятся бурые железные руды, связанные с глиной в Аппалачском регионе Соединенных Штатов, лимонитовые руды частей России и подобные руды в Корее. В этот класс следует также включить обширные лимонитовые месторождения, полученные в результате выветривания серпентина, которые были недавно освоены вдоль северного побережья Кубы, а также латеритные месторождения железной руды, найденные во многих тропических странах. Лимонитовые руды, связанные с глинами, плавились с древних времен из-за их доступности и легкости, с которой их можно было плавить примитивными методами. Однако они дали решительно незначительный процент мирового производства железной руды.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Железная руда, потребляемая миром, была получена главным образом из четырех великих стран-производителей железа: Соединенных Штатов, Германии, Франции и Великобритании.

Другими странами, добывающими значительные количества железной руды, в порядке их значимости являются: Испания, Россия, Швеция, Люксембург, Австро-Венгрия, Куба, Ньюфаундленд и Алжир. Обычный годовой объем добычи в каждой из этих стран превышает один миллион тонн. Небольшие количества железной руды добываются во многих других странах.

Таблица 11. — Добыча железной руды в основных странах-производителях, 1910–1917 гг., в брутто-тоннах [12]

Country | 1910 | 1911 | 1912 | 1913 | 1914 | 1915 | 1916 | 1917
North America: |  |  |  |  |  |  |  |
Canada[13] | 231,623 | 187,807 | 192,753 | 274,673 | 218,620 | 355,457 | 245,693 | 192,210
Cuba[13] | 1,462,498 | 1,163,714 | 1,397,797 | 1,582,431 | 821,110 | 827,448 | 712,716 | 553,485
Newfoundland[13] | 1,108,762 | 1,171,992 | 1,251,968 | 1,433,858 | 566,000 | 775,403 | 903,625 | 788,820
United States | 57,014,906 | 43,876,552 | 55,150,147 | 61,980,437 | 41,439,761 | 55,526,490 | 75,167,672 | 75,288,851
South America: |  |  |  |  |  |  |  |
Chile | ... | 28,150 | 6,546 | 13,878 | 62,506 | 144,783 | 55,281 | 4,921
Venezuela[14] | ... | ... | 12,100 | 57,225 | 2,400 |  |  |
Europe: |  |  |  |  |  |  |  |
Austria-Hungary | 4,592,572 | 4,779,851 | 4,997,311 | 5,233,055 | 3,939,248 | [15]1,218,367 | ([16]) | ([16])
Belgium | 121,024 | 148,130 | 164,734 | 147,048 | 81,063 | 4,646 | 29,951 | 16,732
France | 14,375,984 | 16,376,967 | 18,858,668 | 21,572,835 | ([16]) | ([16]) | ([16]) | ([16])
Germany | [17]28,257,579 | [17]29,408,812 | [17]33,180,258 | 26,771,598 | ([16]) | ([16]) | ([16]) | ([16])
Greece | 527,040 | 493,106 | 424,835 | 308,640 | 294,573 | 154,951 | 83,647 | 62,366
Italy | 542,578 | 367,900 | 572,900 | 593,618 | 695,124 | 669,262 | 927,406 | 978,174
Luxemburg | ([18]) | ([18]) | ([18]) | 7,215,514 | 4,926,980 | 6,040,765 | 6,643,689 | 4,436,682
Norway | 100,834 | 217,051 | 401,665 | 535,869 | 641,790 | 706,379 | 865,700 | ([16])
Portugal | 3,307 | 19,233 | 28,947 | 48,392 | 6,532 | ([16]) | ([16]) | ([16])
Russia | ([19]) | ([19]) | ([19]) | 7,947,191 | ([16]) | ([16]) | ([16]) | ([16])
Spain | 8,530,310 | 8,635,523 | [20]8,990,743 | 9,703,177 | 6,710,357 | 5,527,552 | 5,762,733 | 5,461,857
Sweden | 5,465,234 | 6,056,868 | 6,595,044 | 7,357,845 | 6,482,904 | 6,774,909 | 6,876,278 | 6,119,263
United Kingdom | 15,226,015 | 15,519,424 | 13,790,391 | 15,997,328 | 14,867,582 | 14,235,012 | 13,494,658 | 14,845,734
Asia: |  |  |  |  |  |  |  |
China | [21]130,472 | [21]109,542 | [21]201,561 | [22]416,342 | [22]488,258 | 537,047 | 274,078 | 299,465
Chosen (Korea) | 104,627 | 96,902 | 121,224 | 139,370 | 179,062 | 206,510 | 241,412 | ([16])
India | 54,626 | 366,212 | 580,029 | 370,845 | 441,674 | 390,270 | 411,758 | 413,273
Japan | 132,921 | 144,001 | 168,479 | 168,897 | 134,193 | 133,933 | 156,263 | ([16])
Philippine Islands | 148 | 216 | 347 | 546 | 392 | ([16]) | ([16]) | ([16])
Africa: |  |  |  |  |  |  |  |
Algeria | 1,048,228 | 1,057,087 | 1,171,252 | 1,327,320 | 1,097,101 | 805,547 | 923,598 | 1,048,722
Morocco | 186,149 | ([16]) | ([16]) | ... | ... | ... | ... | ...
Madagascar | ([23]) | ([23]) | 22 |  |  |  |  |
Natal | 50 | ... | ... | ... | ... | ... | ... | ...
Togoland | ([16]) | 394 | ([16]) |  |  |  |  |
Tunis | 327,756 | 397,638 | 470,866 | 584,649 | 244,528 | 281,304 | 361,593 | 596,261
Australia: | 157,821 | 122,361 | 113,989 | [24]90,712 | 177,938 | 370,887 | 390,108 | [25]328,310

[12] Берчард Э. Ф., «Железная руда, чугун и сталь»: Геологическая служба США «Минеральные ресурсы», 1915 и 1917 гг., с дополнениями и исправлениями. (Приведенные выше цифры, насколько это возможно, основаны на официальных отчетах, а там, где они отсутствуют, — на данных технической прессы.)

[13] Отгрузки.

[14] Экспорт в Соединенные Штаты.

[15] Только для Венгрии.

[16] Статистические данные отсутствуют.

[17] Включает Люксембург.

[18] Включено в состав Германии.

[19] Россия произвела 2 936 024 длинные тонны чугуна в 1910 г.; 3 536 417 длинных тонн в 1911 г. и 4 131 890 длинных тонн в 1912 г.

[20] Includes 1,563 long tons of argentiferous iron ore.

[21] Экспорт.

[22] Только из месторождений Тайе.

[23] Мадагаскар произвел около 8 длинных тонн железа в 1910 г. и 1,5 длинные тонны в 1911 г.

[24] Для Южной Австралии и Квинсленда.

[25] Только для Южной Австралии.

Таблица 12. — Чугун, произведенный в основных странах в 1850, 1890, 1900 гг. и с 1910 по 1916 г., в брутто-тоннах [26]

Country | 1850 | 1890 | 1900 | 1910 | 1911 | 1912 | 1913 | 1914[27] | 1915[27] | 1916[28]
United States | 563,755 | 9,202,703 | 13,789,242 | 27,303,567 | 23,649,547 | 29,726,937 | 30,966,152 | 23,332,244 | 29,916,213 | 39,434,797
Germany | 350,000 | 4,584,882 | 8,381,373 | 14,559,509 | 15,404,648 | 17,586,521 | 19,004,022 | 14,162,147 | 11,603,874 | 13,000,000
Great Britain | 2,300,000 | 7,904,214 | 8,959,691 | 10,217,022 | 9,718,638 | 8,889,124 | 10,481,917 | 9,005,898 | 8,793,659 | 9,047,983
France | 405,653 | 1,931,188 | 2,669,966 | 3,974,478 | 4,309,498 | 4,870,913 | 5,227,378 | 3,500,000 | 4,000,000 | 5,000,000
Russia | 227,555 | 912,561 | 2,889,789 | 2,992,058 | 3,531,807 | 4,133,000 | 4,474,757 | 4,190,000 | 3,638,000 | 4,300,000
Austria-Hungary | 250,000 | 910,685 | 1,472,695 | 2,153,788 | 2,056,839 | 2,276,141 | 2,335,170 | 1,500,000 | 1,929,000 | 2,000,000
Belgium | 144,452 | 775,385 | 1,001,872 | 1,822,821 | 2,072,836 | 2,307,853 | 2,318,767 | 1,500,000 | 500,000 | 1,000,000
Canada | ... | 19,439 | 86,090 | 740,210 | 824,368 | 912,878 | 1,015,118 | 705,972 | 825,420 | 1,069,541
Sweden | 150,000 | 483,155 | 518,263 | 594,385 | 624,367 | 688,757 | 728,103 | 629,608 | 755,000 | 750,000
Spain | ... | 176,598 | 289,315 | 367,423 | 402,209 | 396,872 | 418,061 | 400,000 | 421,000 | 440,000
Italy | ... | 14,094 | 23,569 | 347,657 | 298,144 | 373,960 | 420,011 | 379,028 | 389,000 | 454,923
Japan | ... | ... | ... | 186,794 | 200,000 | 200,709 | 236,491 | 295,428 | 312,957 | 379,574
Other countries[28] | 10,000 | 80,000 | 100,000 | 200,000 | 250,000 | 350,000 | 250,000 | 200,000 | 200,000 | 500,000
Total | 4,401,415 | 26,994,904 | 40,181,865 | 65,459,712 | 63,342,901 | 72,713,565 | 77,876,347 | 59,800,325 | 63,284,123 | 77,000,000

[26] «Металлическая статистика», 1914–1918 гг., с некоторыми дополнениями и изменениями.

[27] Частично оценочные данные.

[28] В значительной степени оценочные данные.

Более двух пятых от общего годового объема добычи железной руды в мире приходится на Соединенные Штаты, причем более 80 процентов американской продукции обычно добывается в районе озера Верхнее. Таким образом, этот район является, безусловно, самым важным районом добычи железной руды в мире, ежегодно производя более 30 процентов от общемирового объема железной руды.

Германия и Франция по значимости следуют за Соединенными Штатами как страны-производители железной руды, при этом около 80 процентов руды, добываемой в этих двух странах, получают из Лотарингских железорудных месторождений, расположенных на границе. Годовой объем добычи на этих месторождениях, который включает также руды Люксембурга, составляет около 25 процентов от мирового производства. Таким образом, Лотарингский район и район озера Верхнее вместе производят несколько более половины от общего объема железной руды, ежегодно добываемой в мире.

Железная руда, производимая в Великобритании, добывается главным образом в районе Кливленд на севере Англии; этот район обеспечивает около 40 процентов британского общего объема, что эквивалентно примерно 2,6 процента мирового годового производства. Для сравнения, район Бирмингема в Алабаме и Криворожский район на юге России, которые по значимости следуют за Лотарингским и Верхнеозерным районами, обеспечивают около 3,5 процента и 3,2 процента соответственно от мирового годового производства.

Table 13.—Production and Movement of Iron Ore and Production of Pig Iron, 1913[29]
Gross Tons

Production
of
iron ore
Iron ore
imports
Iron ore
exports
Apparent
consumption
(in part
stocks)
Production
of
pig iron

United Kingdom | 15,997,328 | 8,028,532 | 21,223 | 24,004,637 | 10,260,315
Canada | 307,634 | 2,110,828 | 126,124 | 2,292,338 | 1,015,118
Belgium | 149,450 | 4,400,000 | ... | 4,549,450 | 2,484,690
France | 19,160,407 | 1,410,424 | 10,066,627 | 10,504,264 | 5,311,316
Italy | 603,116 | 7,666 | 20,000 | 590,772 | 426,755
Russia | 8,077,000 | ... | 565,000 | 7,512,000 | 4,557,000
Austria | 3,039,324 | 942,312 | 106,071 | 3,875,565 | 1,757,864
Hungary | 2,059,000 | ... | 700,000 | 1,359,000 | 623,000
Germany (including Luxemburg) | 35,941,285 | 14,019,045 | 2,613,158 | 47,347,172 | 19,291,920
Spain | 9,861,668 | ... | 8,907,202 | 954,466 | 424,774
Sweden | 7,475,571 | ... | 6,440,000 | 1,035,571 | 730,257
United States | 61,980,437 | 2,594,770 | ... | 64,575,207 | 30,966,152
Algeria | 1,349,000 | ... | 1,350,000 |  |
Chile | 70,000 | ... | 65,000 |  |
Cuba | 1,500,000 | ... | 1,582,431 |  |
Newfoundland | 1,605,900 | ... | 1,605,920 |  |

[29] Консультативный совет, Департамент научных и промышленных исследований: «Отчет об источниках и добыче железа и других металлосодержащих руд, используемых в черной металлургии», Лондон, 1918 г., стр. 12.

Таблица 11 показывает мировое производство железной руды с 1910 по 1917 г.

Таблица 12 показывает производство чугуна в 1850, 1890, 1900 гг. и с 1910 по 1916 г.

Таблица 13 показывает производство и перемещение железной руды, а также производство чугуна за 1913 год.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Соединенные Штаты.

— Основными железными рудами Соединенных Штатов являются обширные докембрийские месторождения гематита в районе озера Верхнее; пластовые ископаемые руды клинтонского типа в Алабаме и других южных штатах; месторождения магнетита в Нью-Йорке, северном Нью-Джерси и юго-восточной Пенсильвании; лимонитовые руды восточных и южных штатов; а также смешанные гематитовые и магнетитовые руды Запада. Соединенные Штаты являются крупнейшим производителем железной руды в мире и ежегодно дают более двух пятых мировых поставок. Более 80 процентов продукции поступает из района озера Верхнее, а большая часть остального — из Алабамы, Нью-Йорка и Пенсильвании. В 1917 году в Соединенных Штатах было добыто 75 000 000 тонн железной руды, из которых 63 000 000 поступило из региона озера Верхнее, 7 000 000 — из Алабамы, 1 000 000 — из Нью-Йорка и около 500 000 тонн из каждого штата: Пенсильвании, Нью-Джерси, Теннесси, Вирджинии и Вайоминга; в 1918 году общий объем производства составил 69 000 000 тонн, из которых 60 000 000 поступило из района озера Верхнее, 6 000 000 — из Алабамы, 900 000 — из Нью-Йорка, 500 000 — из Пенсильвании и по 400 000 тонн из Теннесси, Вирджинии, Нью-Джерси и Вайоминга.

В следующей таблице представлены приблизительные запасы железной руды в основных районах Соединенных Штатов:

Таблица 14. — Запасы железной руды в Соединенных Штатах в брутто-тоннах [30]

| Millions of tons.
Lake Superior District (hematite) | 3,500
Birmingham District (fossil hematite) | 355
Tennessee and Virginia (fossil hematite) | 100
Adirondack District (non-titaniferous magnetite) | 40
Adirondack District (titaniferous magnetite) | 90
Northern New Jersey and Southeastern New York (magnetite) | 15
Southeastern Pennsylvania (magnetite) | 40
Appalachian region (magnetite) | 50
Northeastern Texas (limonite) | 260
Western United States (magnetite and hematite) | 100
Other Districts | 150
Total | 4,700

[30] Kemp, J. F.: “The Iron-Ore Resources of the World,” Stockholm, 1910 (with minor revisions).

Крупнейшей единой железоделательной и сталелитейной промышленной компанией в Соединенных Штатах является United States Steel Corporation, которая контролирует следующие компании по производству железа и стали: Carnegie Steel Co., Illinois Steel Co., Indiana Steel Co., American Steel & Wire Co., American Sheet & Tinplate Co., National Tube Co., The National Tube Co. of Ohio, Minnesota Steel Co., The Lorain Steel Co., Tennessee Coal, Iron & Railroad Co. и Shelby Steel Tube Co., имеющие в общей сложности 124 доменные печи с годовой мощностью около 18 000 000 тонн чугуна. Большинство доменных печей находится в Пенсильвании, Огайо, Иллинойсе и Алабаме.

С United States Steel Corporation связана компания Oliver Iron Mining Co., которая производит около 43 процентов железной руды, ежегодно добываемой в районе озера Верхнее, что эквивалентно почти 37 процентам всей железной руды, ежегодно добываемой в Соединенных Штатах. Tennessee Coal, Iron & Railroad Co. является основным производителем железной руды в Алабаме.

Следующей по значимости после United States Steel Corporation как производитель железа и стали является Bethlehem Steel Corporation с ее дочерними компаниями: Bethlehem Steel Co., Pennsylvania Steel Co., Maryland Steel Co., Jurugua Iron Co., Spanish-American Iron Co. и Bethlehem Iron Mines Co.

Предприятия Bethlehem Steel Corporation имеют общую мощность по производству чугуна 3 060 000 тонн в год на 23 доменных печах. Семь печей находятся в Южном Вифлееме, штат Пенсильвания, семь — в Стилтоне, штат Пенсильвания, четыре — в Лебаноне, штат Пенсильвания, три — в Корнуолле, штат Пенсильвания, и четыре — в Спэрроус-Пойнт, штат Мэриленд. Bethlehem Steel Corporation владеет крупными месторождениями железной руды на Кубе и в Чили. Большая часть руды, потребляемой в ее печах в настоящее время, поступает с Кубы, из района озера Верхнее и из Корнуолла, штат Пенсильвания.

Третьей по значимости среди компаний по производству железа и стали в Соединенных Штатах является недавно организованная Midvale Steel & Ordnance Co., контролирующая Worth Brothers, Midvale Steel Co., Remington Arms Co., Cambria Steel Co. и другие. Совокупная мощность по производству чугуна 14 доменных печей, контролируемых Midvale Steel & Ordnance Co., составляет 2 420 000 тонн чугуна. Три доменные печи находятся в Коутсвилле, штат Пенсильвания, и одиннадцать — в Джонстауне, штат Пенсильвания. Эта компания владеет важными месторождениями железной руды на Кубе и в районе озера Верхнее.

Четыре другие крупные компании производят более миллиона тонн чугуна в год: Republic Iron & Steel Co. с расчетной общей мощностью 11 доменных печей в Огайо и Алабаме в 1 430 000 тонн чугуна и 2 500 000 тонн руды с ее шахт в районе озера Верхнее и в Алабаме; Lackawanna Steel Co. с годовой мощностью в 1918 году на девяти доменных печах в Лакаванне, штат Нью-Йорк, в 1 440 000 тонн чугуна; Jones & Laughlin Co. из Питтсбурга с мощностью 1 920 000 тонн на 11 доменных печах; и McKinney Steel Co. с восемью печами в Огайо, Нью-Йорке и Пенсильвании и годовой мощностью 1 205 000 тонн чугуна. Последние три названные компании имеют обширные железные рудники в районе озера Верхнее.

Важными компаниями по производству железа и стали, производящими несколько менее миллиона тонн чугуна в год, являются: Youngstown Sheet & Tube Co. с годовой мощностью 990 000 тонн чугуна на шести доменных печах, все из которых находятся в Янгстауне, штат Огайо; недавно организованная Steel & Tube Co. of America, имеющая шесть доменных печей в Чикаго и его окрестностях с годовой мощностью по чугуну 900 000 тонн; Colorado Fuel & Iron Co., важный западный производитель железа и стали, имеющий шесть доменных печей недалеко от Пуэбло, штат Колорадо, с годовой мощностью 625 000 тонн чугуна и владеющий рудниками железной руды в Нью-Мексико, Вайоминге и Колорадо; и Schloss-Sheffield Steel & Iron Co. из Алабамы с семью доменными печами и мощностью по чугуну 530 000 тонн. Многие другие предприятия с меньшей мощностью разбросаны по восточной и центральной части Соединенных Штатов. Насколько известно, практически весь бизнес по производству железа и стали в Соединенных Штатах находится в руках американского капитала.

Германия.

— «Минеттовые» руды немецкого Лотарингского района до войны составляли, безусловно, крупнейший запас железной руды Германии и являются основным источником текущих поставок. Следующими по значимости среди немецких запасов руды являются бурые гематиты, залегающие к северу от Гарца, а третьими и четвертыми по значимости — месторождения районов Лан и Дилль в Рейнской области и месторождения Зигера. Все эти районы находятся в западной и юго-западной Германии, и все они, за исключением Лотарингии, расположены в регионе к востоку от Рейна в Ганновере, Вестфалии, Гессен-Нассау и Рейнской Пруссии.

Лотарингский район находится на французской границе и является частью крупного рудного бассейна Люксембурга и северной Франции. Месторождения осадочного происхождения юрского периода включают обширные пласты оолитового лимонита толщиной до 20 футов, прослоенные мергелем и известняком. В пределах толщи осадочных пород от 75 до 150 футов обнаружено семь основных пластов руды, наиболее важный из которых известен как «Серый пласт». Тоннаж [31] «минеттовой» руды, доступной в немецком Лотарингском районе, оценивается в 1830 миллионов [32] по сравнению с 300 миллионами в Люксембурге и 2975 миллионами [33] в северной Франции. «Минеттовые» руды содержат в среднем от 30 до 40 процентов металлического железа и от 0,3 до 0,7 процента или более фосфора.

[31] Запасы руды в этой главе указаны в метрических тоннах, если не указано иное.

[32] Айнеке Г. и Колер В.: «Мировые ресурсы железной руды», Стокгольм, 1910 г.

[33] Нику Л., там же.

Месторождения районов Зальцгиттер и Ильзеде к северу от гор Гарц представляют собой пласты конгломерата бурого железняка со средней толщиной от 20 до 30 футов, состоящие из лимонитовой гальки в глинистом или известковом цементе. Эти месторождения занимают много квадратных миль, а запасы оцениваются в 248 миллионов тонн. Руды содержат от 30 до 40 процентов железа и в среднем от 0,7 до 0,8 процента фосфора.

Руды региона Лан и Дилль — это в основном красные гематиты, залегающие в обширном осадочном пласте. Они содержат около 48 процентов железа, от 0,2 до 0,3 процента фосфора и отличаются высоким содержанием кремнезема. Запасы оцениваются примерно в 135 миллионов тонн.

В Зигере железные руды — это в основном карбонаты, содержащие от 38 до 40 процентов металлического железа и от 6 до 9 процентов марганца. Они образуют нерегулярные месторождения, обильно разбросанные по всему региону, а доступные запасы оцениваются примерно в 100 миллионов тонн.

Общие фактически доступные запасы железной руды в Германии (не включая запасы Люксембурга) оцениваются в 2540 миллионов тонн, а вероятные дополнительные запасы — в 1067 миллионов тонн. Однако Лотарингия содержит подавляющую часть этих объемов, поэтому передача этой провинции Франции сокращает доступные запасы Германии до 28 процентов от довоенного уровня, а ее вероятные дополнительные запасы — наполовину, в целом сокращая ее ресурсы железной руды до одной трети от прежнего объема.

Насколько известно, немецкий бизнес по производству железа и стали находится в руках немецких капиталистов, которые, кроме того, имеют важные активы в виде железной руды во Франции, Испании, Швеции и других странах. Среди важных фирм по производству железной руды и чугуна в Германии — Gutehoffnungshütte, de Wendel & Co., Krupp, Gebrüder Stumm, Aschener Hütten Aktien Verein, Rombacher Hüttenwerke, Thyssen & Cie. и другие. Все эти фирмы имели крупные запасы руды в Лотарингском районе к началу войны.

Франция.

— Железные руды Франции делятся на три отдельные группы: «минеттовые» руды районов Брие, Лонгви, Крюсн и Нанси; силурийские руды в Нормандии; и жильные месторождения в восточных Пиренеях.

«Минеттовые» руды северной Франции являются частью упомянутого выше великого бассейна «минеттовых» руд Франции, Люксембурга и Германии. В 1913 году они обеспечили около 91 процента от общего объема производства Франции. Железные руды Нормандии и Бретани имеют осадочное происхождение и состоят из гематита или карбоната, либо их смеси. С глубиной содержание карбоната увеличивается. Месторождения железной руды в восточных Пиренеях состоят как из гематита, так и из сидерита и являются высококачественными, составляя единственный значительный источник бессемеровской руды во Франции. Содержание железа в рудах Нормандии и Бретани варьируется от 30 до 50 процентов; в рудах Пиренеев — от 51 до 57 процентов. Последний диапазон включает кальцинированный сидерит.

Добыча железной руды во французской Лотарингии в 1913 году составила около 19 500 000 тонн; в Нормандии и Бретани — около 1 500 000 тонн, а в восточных Пиренеях — около 500 000 тонн, что в сумме дает более 21 000 000 тонн для Франции.

В следующей таблице показан относительный объем добычи железной руды на различных железорудных полях Франции и Германии за последние три нормальных года перед войной:

Table 15.—Production of Iron Ore in France and Germany, 1911 to 1913
Metric tons

District | 1911 | 1912 | 1913
German Lorraine | 17,734,576 | 20,050,245 | 21,135,554
Luxemburg | 6,059,797 | 6,553,930 | 7,331,050
French Lorraine, including Briey, Longwy and Nancy | 14,878,000 | 17,235,125 | 19,499,166
Germany, outside of Lorraine | 6,968,000 | 7,167,000 | 7,472,000
France, outside of Lorraine | 1,584,000 | 1,925,000 | 1,686,000

Доступные запасы в различных районах французского месторождения «минеттовых» руд оцениваются следующим образом: [34]

Таблица 16. — Запасы руды во французском месторождении «Минетт»

| Million tons
Briey | 2,000
Crusnes | 500
Longwy | 275
Nancy | 200
Total | 2,975

[34] Нику Л.: «Мировые ресурсы железной руды», Стокгольм, 1910 г.

Список действующих компаний во Франции показывает значительное число немецких компаний среди преобладающих французских. Немецкие или предположительно немецкие компании произвели в 1913 году шесть с половиной миллионов тонн железной руды, или одну треть от всего объема производства. В регионе Нормандии и Бретани две немецкие компании обеспечили 11 процентов от всего производства; а в восточных Пиренеях одна немецкая компания произвела 20 процентов. В общей сложности немецкий капитал контролировал более одной трети железоделательной и сталелитейной промышленности Франции в 1913 году. Остальная часть, по-видимому, находилась в руках французского капитала.

Наиболее важными фирмами по производству железа в Лотарингском районе в последние годы были de Wendel & Co., Gutehoffnungshütte, Société des Hauts Fourneaux et Fonderies de Pont-a-Moussons, Société des Forges et Acieries de la Marine et d’Homecourt, Société Anonyme des Acieries de Longwy, Société des Acieries de Micheville и Société des Mines d’Ammermont Dommery. Первые две фирмы являются преимущественно немецкими и контролировали земли не только в немецкой Лотарингии, но и во французской Лотарингии. Таким образом, железорудные земли Лотарингского района даже после передачи территории Франции будут в значительной степени принадлежать фирмам, контролируемым Германией. Политически, однако, Франция будет иметь контроль над объемом добычи.

Великобритания.

— Железные руды, добываемые в Великобритании, поступают главным образом с Кливлендских холмов в Йоркшире, а также из Линкольншира, Нортгемптоншира, Камберленда, Стаффордшира, Лестершира, Шотландии и Ланкашира, в порядке их значимости. Более одной трети от общего объема производства приходится на Кливлендские холмы. Руда с Кливлендских холмов, из Линкольншира, Нортгемптоншира, Лестершира и Шотландии представляет собой пластовый оолитовый сидерит среднего и нижнего юрского периода; руда из Камберленда и Ланкашира — это гематит с исключительно низким содержанием фосфора, встречающийся в карманах в каменноугольных и силурийских известняках; а руда в Стаффордшире — это сидерит разновидностей «черный пласт» и «глинистый пласт», встречающийся в угольных пластах.

В следующей таблице показано производство железной руды в Соединенном Королевстве в 1915 году:

Таблица 17. — Производство железной руды в Соединенном Королевстве в 1915 году

| Long tons
Cleveland Hills | 4,746,293
Lincolnshire | 3,149,079
Northamptonshire | 2,517,150
Cumberland | 1,323,408
Staffordshire | 703,231
Leicestershire | 685,137
Scotland | 375,241
Lancashire | 333,086
Other Great Britain and Ireland | 402,387
Total | 14,235,012

Значительная часть железной руды в Великобритании в настоящее время не может разрабатываться с прибылью, и большая часть руды, которая была товарной несколько лет назад, теперь не может разрабатываться из-за возросших затрат на транспортировку, рабочую силу и, в особенности, на топливо. Фактические запасы руды товарного качества оцениваются в 1300 миллионов тонн; общие запасы были оценены Г. Луи в 39 500 миллионов тонн. [35]

[35] Луи Г.: «Мировые ресурсы железной руды», Стокгольм, 1910 г.

В 1915 году Соединенное Королевство произвело 14 000 000 тонн железной руды. В том же году было импортировано почти 7 000 000 тонн, из которых 4 000 000 поступило из Испании и от половины до одного миллиона из Алжира и Норвегии из каждой, что составило в общей сложности более 20 000 000 тонн, выплавленных в Соединенном Королевстве. Общее производство чугуна составило почти 9 000 000 тонн, из которых почти 7 000 000 тонн было произведено в Англии, 1 000 000 тонн в Шотландии и почти 1 000 000 тонн в Уэльсе. Ирландия чугун не производит. Железоделательная и сталелитейная промышленность Великобритании, насколько имеется информация, находится в руках британских подданных.

Эккель [36] рассматривает ситуацию с железной рудой в Великобритании следующим образом:

Положение Великобритании в отношении ресурсов железной руды своеобразно — возможно, более любопытно, чем удовлетворительно. Вопрос можно резюмировать, сказав, что у Англии все еще есть несколько сотен миллионов тонн высококачественной руды, которая была бы востребована где угодно; что у нее есть, кроме того, возможно, вдвое большее количество низкокачественной руды, пригодной для разработки из-за близости к углю и рынкам сбыта; и что в Англии, Шотландии и Уэльсе есть тысячи миллионов тонн руды, которые сейчас не подлежат разработке, но могут стать пригодными в будущем при условии, что к тому времени останется какая-либо другая веская причина для производства стали в Великобритании. Это последнее ограничение может быть неприятным, но оно действительно является сутью всего вопроса, и, по-видимому, оно было упущено из виду британскими геологами, обсуждавшими эту тему. Люди не производят железо из низкокачественных руд просто для того, чтобы использовать руды; а при растущей стоимости кокса и сужающемся экспортном рынке возникает очень серьезный вопрос, будут ли вообще когда-либо использованы эти британские карбонаты. Продолжительность существования британской сталелитейной промышленности будет определяться ее запасами угля, а не запасами местных руд; ибо до тех пор, пока кокс и рынки сбыта это оправдывают, руду можно выгодно импортировать. Если другие условия не оправдывают импорт руды, они, безусловно, не оправдают использование этих гипотетических резервных тоннажей.

[36] Эккель Э. К.: «Железные руды, их залегание, оценка и контроль», стр. 320, 1914 г.

Испания.

— Испания богата запасами железной руды, но железоделательная и сталелитейная промышленность получила здесь слабое развитие. Годовое производство железной руды в Испании в последние годы перед войной составляло около 9 000 000 тонн, из которых более 8 000 000 тонн экспортировалось. Потребление железной руды испанскими доменными печами составляло около 800 000 тонн в год.

Основные железные руды Испании залегают в северо-западной части, в провинциях Бискайя, Овьедо, Луго и Сантандер; в северо-восточной части, в провинциях Теруэль и Гвадалахара; и в юго-восточной части, в провинциях Гранада, Альмерия, Мурсия, Севилья и Уэльва.

Железные руды Бильбао в Бискайе относятся к бессемеровскому сорту, и в течение многих лет большие объемы экспортировались в Англию для использования на бессемеровских заводах в дополнение к рудам из Кливлендского и других районов Англии. Благодаря своему превосходному качеству они пользуются постоянным спросом, и английская железоделательная и сталелитейная промышленность в значительной степени зависела от этих и других высококачественных руд Испании. В более поздние годы Германия также проявила интерес к железорудным месторождениям Бильбао, и в последние годы перед войной Германия забирала более одной трети от общего объема производства Испании, включая также большие объемы руды из южной Испании. Испанские интересы владеют важными месторождениями на юго-востоке Испании и в районе Бильбао.

Большая часть руды юго-восточной Испании является высококачественной, богатой железом и с низким содержанием фосфора. Почти вся она бессемеровского качества, а некоторая имеет очень низкое содержание фосфора; последняя широко экспортируется для использования в производстве чугуна с низким содержанием фосфора. Соединенные Штаты в прошлые годы в значительной степени зависели от Испании в отношении этого сорта руды, импортируя более 100 000 тонн ежегодно.

В Испании имеется ряд доменных печей и сталелитейных заводов, основные из которых находятся в Бильбао, в провинции Бискайя. В Бискайе ежегодно производится более 300 000 тонн чугуна, что составляет примерно три четверти от общего объема производства чугуна в Испании.

Европейская Россия.

— В Европейской России [37] основные месторождения железной руды распределены по четырем главным районам: Уральские горы, центральная Россия, южная Россия и Кавказ.

[37] Богданович К.: «Мировые ресурсы железной руды», Стокгольм, 1910 г.

В Уральских горах руды по большей части связаны с изверженными породами. Наиболее важные месторождения находятся в окрестностях горы Благодать, в северных районах Урала, и возле горы Магнитной, на Южном Урале. Руды в основном магнетитовые и лимонитовые и поступают из чрезвычайно большого количества мелких рудников. В центральной России, на широко разбросанных территориях, имеются месторождения известковых руд, глинистых железняков и болотных руд. Многие из месторождений являются тонкими и не могут разрабатываться с прибылью. Единственные сколько-нибудь важные запасы в южной России разделены между тремя центрами: Кривой Рог, Донецкий бассейн и Керченский полуостров. Безусловно, самыми важными месторождениями являются магнетито-гематитовые руды в районе Кривого Рога. Железняки угольных пластов в Донецком бассейне и лимонит Керченского полуострова имеют второстепенное значение. Рудники Кривого Рога интенсивно разрабатываются, а их запасы оцениваются примерно в 86 миллионов тонн товарной руды. Рудники контролируются в основном следующими тремя компаниями: Брянское общество, Криворожское железорудное общество и общество «Провиданс».

В следующей таблице показано производство железной руды в различных частях России в 1912 году:

Таблица 18. — Добыча железной руды в России

| Long tons
Southern Russia | 5,679,000
Ural | 1,817,000
Central Russia | 286,000
Other Russia and Siberia | 6,000
Total | 7,788,000

Запасы руды в России можно резюмировать по районам следующим образом:

Запасы железной руды в России

| Millions of tons
Ural | 282
Central Russia | 789
Southern Russia | 536
Caucasus | 14
Total | 1,621

Эккель [38] рассматривает ситуацию с железной рудой в России следующим образом:

На первый взгляд отмеченные запасы руды кажутся вполне удовлетворительными, и пока данные не будут изучены более критически, трудно объяснить, почему относительно большая производственная мощность Московского и других центрально-российских районов настолько не соответствует сравнительно небольшой добыче руды в этой области. На самом деле, однако, большие общие запасы руды, приписываемые центральной России, в действительности менее важны, чем кажутся, из-за качества руды и малой мощности рудных тел. С международной точки зрения месторождения руды южной России требуют наибольшего внимания; ибо они расположены так, что представляют интерес для иностранных конкурентов, в то время как общий тоннаж запасов высок, а качество многих руд превосходно.

[38] Эккель Э. К.: «Железные руды, их залегание, оценка и контроль», 1914 г., стр. 326.

Фактические доступные запасы руды товарного качества в России оцениваются в 865 миллионов тонн.

До революции большая часть российской железоделательной и сталелитейной промышленности контролировалась синдикатами. [39] Старейший из них состоял из производителей среднего листа (1902 г.); затем последовали производители двутавровых балок и U-образного железа (1903 г.), осей и бандажей (1904 г.), железных труб (1906 г.), рельсов (1907 г.), а также сортового железа и обручей. Эти шесть синдикатов были впоследствии объединены в один, официально называвшийся «Общество для продажи изделий русских металлургических заводов», но общеизвестный как «Продамета» по своему телеграфному адресу. Существовали отдельные синдикаты по проволоке, проволочным гвоздям и кровельному железу. «Продамета» состояла, по последним сведениям, из девятнадцати заводов, из которых шестнадцать находятся в южной России, и по одному — в Петрограде, Москве и на Урале. «Продамета» прекратила свое существование в конце 1915 года, но была временно продлена на один год, а в конце 1916 года снова была продлена на аналогичный период. Совокупный капитал восемнадцати заводов составлял 198 400 000 рублей, а их чистая прибыль за 1915–1916 гг. — 76 200 000 рублей.

[39] Ежегодник металлического рынка Ironmonger, Лондон, 1918 г.

Швеция.

— Железорудные месторождения Швеции являются одними из самых важных в Европе и в течение последних десяти-пятнадцати лет обеспечивали большой объем добычи, который шел главным образом в Англию и Германию. Относительно небольшое количество железной руды используется на шведских заводах по выплавке железа. Железные рудники центральной Швеции активно разрабатываются примерно с начала XII века, тогда как рудники шведской Лапландии были освоены недавно. В настоящее время около половины объема добычи железной руды в Швеции поступает из шведской Лапландии, а другая половина — из центральной Швеции.

Запасы железной руды в шведской Лапландии оцениваются в 1128 миллионов тонн. Руды в основном магнетитовые, связанные с изверженными породами, и демонстрируют значительную разницу в содержании фосфора. Некоторые месторождения или части месторождений состоят из руд с умеренно низким содержанием фосфора, тогда как другие имеют достаточно высокое содержание, чтобы получать специальный бонус от немецких сталелитейных заводов, производящих высокофосфористый шлак для нужд удобрений. Практически все руды шведской Лапландии экспортируются. В последние годы общий объем производства составлял около 3 500 000 тонн ежегодно. Основные рудники разрабатываются компанией Trafikaktiebolaget Grängesberg Oxelosund, в которой английский и немецкий капитал участвует совместно со шведским правительством. Шведское правительство контролирует объем добычи на рудниках и получает крупную сумму в виде роялти с добытой руды. Месторождения, из которых в настоящее время добывается руда, — это Кируна, Елливаре и Туоллуварра, причем первые два эксплуатируются упомянутой выше фирмой, а последнее является независимым предприятием.

Запасы руды в центральной и южной Швеции оцениваются в 140 миллионов тонн, включенных в большое количество относительно небольших месторождений. Большинство рудников центральной Швеции контролируется мелкими шведскими операторами. Некоторые рудники, однако, такие как Блотберг, в значительной степени находятся под немецким контролем, а крупнейший из них, Гренгесберг, эксплуатируется той же фирмой, которая контролирует месторождения шведской Лапландии. Некоторые руды центральной Швеции, такие как руды Даннеморы, Норберга, Строссы и Стрипы, имеют очень низкое содержание фосфора и используются в производстве специального железа с низким содержанием фосфора; другие, такие как руды Гренгесберга и Блотберга, содержат более 1 процента фосфора.

Австро-Венгрия.

— Железные руды бывшей Австро-Венгерской империи — это в основном низкокачественные водные силикаты железа, требующие обжига, крупные месторождения карбоната железа и некоторое количество лимонита. Общие вероятные запасы руды оцениваются в 940 миллионов тонн, из которых около 560 миллионов являются очень низкокачественными.

Основными источниками, из которых в прошлом в Австро-Венгерской империи получали отечественную железную руду, являются месторождения шамозит-гематита в Нучице и других местах Богемии; пласты сидерита в Эрцберге, Штирия, оцениваемые в более чем 200 миллионов тонн руды; месторождения сидерит-лимонита на склонах Карпат; и месторождения различных руд в северной и центральной Боснии.

Безусловно, крупнейшим из месторождений является Эрцберг, принадлежащее и эксплуатируемое Oesterreichische Alpinen Montan Gesellschaft, предположительно австрийской компанией. Богемские месторождения, также важные, в значительной степени находятся под контролем Prager Eisen Industrie Gesellschaft. Карпатские месторождения в значительной степени контролируются местными частными лицами и фирмами, среди которых герцог Филипп Саксен-Кобург-Готский-Кохари. Таким образом, основные месторождения в значительной степени находились под австро-венгерским контролем.

В результате войны и распада Австро-Венгерской империи богемские месторождения, оцениваемые в 35 100 000 тонн высококачественной руды и 221 800 000 тонн низкокачественной руды, перейдут под контроль Чехословакии, тогда как боснийские руды с оценочными запасами в 21 500 000 тонн отойдут Югославии. Австрия сохранит контроль над крупным месторождением Эрцберг в Штирии, а руды Карпатского региона останутся под венгерским контролем.

Алжир, Тунис и Марокко.

— Железные руды Марокко, Алжира и Туниса в северной Африке — это в основном высококачественный гематит. Тоннаж запасов Алжира и Туниса оценивается Нику в 100–150 миллионов тонн, и около 30–40 миллионов тонн зафиксировано на испанской территории Риф, Марокко.

Месторождения Марокко и Алжира почти все находятся недалеко от северного побережья, и руды отгружаются из различных небольших портов, таких как Мелилья, Бенисаф, Арзеу, Алжир, Бужи и Бона. Месторождения Туниса находятся в 180–200 километрах к юго-западу от Туниса, порта отгрузки, с которым они соединены железной дорогой.

Основные рудники Эль-Рифа, Марокко, принадлежат Sociedad Española de Minas de Riff. Немецкие интересы, компания «Netta Company», владели крупной концессией, но после войны эти интересы контролируются компанией из Бильбао.

Североафриканские месторождения важны как источник высококачественной руды с низким содержанием фосфора для европейских доменных печей. Вся добытая руда экспортируется, а годовой объем отгрузок составляет около 1 500 000 тонн.

Куба.

— На Кубе есть две основные группы месторождений железной руды — магнетитовая и гематитовая руда на южном побережье и бурая руда, или лимонит, на северном побережье. Все они находятся недалеко от восточной оконечности острова. Руды Фирмезы и Дайкири на южном побережье представляют собой смесь магнетита и гематита, содержащую в среднем около 58 процентов железа и 0,03 процента фосфора. Они связаны с изверженными породами. Определение тоннажа затруднено из-за нерегулярности рудных тел, и оценки запасов варьируются от 5 до 9 миллионов тонн. Бурая руда северного побережья — это гидратированный бурый гематит, продукт латеризации серпентина. Высушенная руда содержит в среднем около 46 процентов железа, 0,01 процента фосфора и 1,7 процента хрома. Тоннаж запасов, оцениваемый до 3000 миллионов тонн, в основном содержится в трех крупных месторождениях: Камагуэй, Майари и Моа.

Основные месторождения Кубы принадлежат и эксплуатируются Bethlehem Steel Co. Важные неразработанные месторождения принадлежат Buena Vista Iron Co. (Midvale Steel & Ordnance Co.), United States Steel Corporation, Guantanamo Exploration Co. и Eastern Steel Co.

Ньюфаундленд.

— Основные железные руды Ньюфаундленда — это пластовые оолитовые гематиты, содержащие в среднем от 50 до 52 процентов металлического железа. Запасы руды Ньюфаундленда оцениваются в пределах от 3250 до 3500 миллионов тонн, что делает их одними из крупнейших и, безусловно, самыми компактными запасами железной руды в мире. Объем добычи руды составлял от 1 000 000 до 1 500 000 тонн ежегодно, за исключением периода войны, когда производство снизилось. Эти месторождения важны как из-за своего размера, так и из-за своего расположения. Руду можно легко доставить в американские или европейские порты по стоимости за единицу железа, значительно более низкой, чем любая конкурирующая руда, поэтому рынок практически неограничен.

Руды в основном экспортировались в Сидней, Новая Шотландия, и в Филадельфию, в то время как около 10 процентов шло в Голландию (Германию). Содержание фосфора слишком высоко для нормальной экономической практики основной мартеновской плавки, если руды используются в чистом виде, но не слишком высоко для литейного производства или для процесса томасовской плавки, разработанного в Европе.

Месторождения железной руды Вабана принадлежат и разрабатываются Dominion Iron & Steel Co. и Nova Scotia Steel & Coal Co., двумя канадскими фирмами. Обе компании эксплуатируют сталелитейные заводы недалеко от Сиднея, Кейп-Бретон.

Норвегия.

— Основные железные руды Норвегии — это низкокачественный магнетит и зеркальный гематит, значительную часть которых можно выгодно обогащать. Они встречаются в северной части, к северу от Полярного круга. Небольшие месторождения высококачественных руд, состоящие в основном из магнетитовых линз, встречаются в южной Норвегии.

Месторождения Сидвариангер на крайнем севере, недалеко от границы с Финляндией, по оценкам, содержат 100 миллионов тонн низкокачественного магнетита. Руда перерабатывается на крупном обогатительном заводе, построенном норвежской компанией, но контролируемом шведским и немецким капиталом. Концентраты содержат 70 процентов железа и 0,02 процента фосфора. Месторождения Дандерланд на Ранненфьорде, недалеко от Полярного круга, по оценкам, содержат 80 миллионов тонн смешанного низкокачественного зеркального гематита и магнетита.

In 1914 Norway produced 652,273 tons of iron ore, of which seven-eighths came from the Sydvaranger deposit.

Италия.

— Самыми важными железными рудниками в Италии являются гематитовые рудники на острове Эльба, которые в последние годы давали от 500 000 до 1 000 000 тонн руды ежегодно. Десять или двенадцать крупных рудных тел обнаружены в восточной части острова, все они находятся под контролем компании Elba Company, которая получила концессию, дающую ей исключительные права на добычу железа на острове. Важные, но пока малоразработанные месторождения магнетита найдены в долине Аоста, Пьемонт, а месторождения лимонита найдены на острове Сардиния. Они давали очень небольшой объем продукции. Незначительные месторождения железной руды встречаются в Ломбардии, в Апеннинах центральной Италии и в других местах. Общие запасы железной руды в Италии оцениваются примерно в 25 миллионов тонн.

В Италии есть несколько важных заводов по выплавке железа, среди которых доменные печи Elba Company на острове Эльба, печи Piombino в Пьомбино, на материке напротив Эльбы, и печи Ilva в Баньоли, недалеко от Неаполя. Кроме того, есть несколько небольших предприятий в северной Италии.

Железорудные месторождения и производство железа в Италии контролируются коммерческими организациями, в основном итальянскими, но частично английскими. Итальянское правительство осуществляет контроль над месторождениями руды путем предоставления концессий на сравнительно короткие сроки.

Соглашения, заключенные между итальянскими производителями о рациональном разделении труда, привели к формированию синдиката следующих фирм: Ilva, Elba, Siderurgica di Savona, Metallurgica di Lestre, Ferriere Italiane и сталелитейный завод Piombino. Эти фирмы обязались поддерживать синдикат в течение одиннадцати лет, начиная с июля 1911 года. Делами организации руководила компания Ilva. «В 1916 году компании-участницы продлили свое соглашение до 1930 года, но компания Ilva перестала руководить делами синдиката, а отношения между синдикатом и немецким Stahlwerks Verband были расторгнуты и заменены англо-итальянскими отношениями». [40]

[40] Ежегодник металлического рынка Ironmonger, 1918 г.

Была создана еще одна организация под названием «Societa Ferro ed Acciaio», объединение сталелитейных заводов.

Италия важна как производитель железной руды и как производитель изделий из железа. Она была способна обеспечивать свои собственные потребности в железной руде в течение многих лет и при нынешних темпах может продолжать делать это, вероятно, еще двадцать лет. По-видимому, нет тенденции к расширению в другие области для контроля над иностранными месторождениями руды.

Италия произвела 593 000 тонн железной руды в 1913 году; 669 000 тонн в 1915 году; и 927 000 тонн в 1916 году. В 1915 году было произведено 408 000 тонн чугуна и 87 000 тонн было импортировано.

Греция.

— Хромосодержащие железные руды встречаются в восточной Греции и на прилегающих островах. Они содержат от 46 до 52 процентов железа, от 2 до 3 процентов хрома и около 0,10–1,00 процента никеля и кобальта. Обычное годовое производство железной руды в Греции составляло около 400 000 тонн.

Канада.

— Небольшие месторождения железной руды встречаются в Нью-Брансуике и Новой Шотландии. В Онтарио есть два основных района железной руды — хребты Атикокан и Мичипикотен. Руда в первом — магнетит, а во втором — гематит и сидерит с некоторым количеством лимонита. Руды западной Британской Колумбии — это в основном магнетит. Основные месторождения находятся на островах Тексада и Ванкувер, где руда отличного качества, содержащая в среднем 63 процента железа, 0,02 процента фосфора и от 4 до 10 процентов кремнезема. Низкокачественная магнетитовая руда найдена на руднике Мус-Маунтин, Онтарио, и подвергается обогащению.

В Канаде имеется ряд доменных печей, среди которых печи Dominion Iron & Steel Co., Сидней; Nova Scotia Steel & Coal Co., Сидней-Майнс, и Londonderry Iron & Mining Co., Лондондерри, все из которых используют руды из Ньюфаундленда и Новой Шотландии; Algoma Steel Corporation, Су-Сент-Мари, Онтарио; Steel Company of Canada, Гамильтон, Онтарио; Canadian Furnace Co., Порт-Колборн, Онтарио; Canada Iron Foundries, Мидленд, Онтарио; Standard Iron Co., Дезеронто и Парри-Саунд, Онтарио; и Atikokan Iron Co., Порт-Артур, Онтарио, которые используют в основном озерные руды Соединенных Штатов и Канады. Moose Mountain Co. из Селлвуда, Онтарио, имеет завод по магнитному обогащению и брикетированию, использующий руду с рудника Мус-Маунтин. В мае 1920 года была образована British Empire Steel Corporation, вторая по величине в мире, путем слияния девяти сталелитейных, угольных, судостроительных и транспортных компаний.

В 1912 году Канада произвела 156 000 тонн железной руды и изготовила 906 000 тонн чугуна. [41] В 1918 году она изготовила 1 066 071 тонну чугуна. Железные рудники Канады в значительной степени находятся в канадской, а частично в американской собственности.

[41] Совет по торговле, «Отчеты о железе и стали», Лондон, 1905–1918 гг.

Китай и Маньчжурия.

—Имеется мало информации о масштабах месторождений железных руд Китайской империи. Основным районом добычи является Дайе, расположенный к югу от реки Янцзы в провинции Хубэй, где вдоль контакта известняка и интрузивного сиенита залегает серия рудных тел, состоящих из смеси гематита и магнетита. По оценкам, месторождения содержат около 40 миллионов тонн руды. [42] Компания Han-Yeh-Ping Iron & Steel Co., в значительной степени контролируемая Японией, владеет этими месторождениями и сталелитейным заводом Ханьян близ Ханькоу. Сообщается, что железная руда, аналогичная руде Дайе, встречается ниже по течению Янцзы в Тунлине, в провинции Аньхой, а также вдоль побережья близ Амоя, провинция Фуцзянь. Месторождения близ Амоя, как утверждается, содержат около 25 миллионов тонн.

[42] Бейн, Г. Ф.: «Заметки о ресурсах железных руд Китая», Trans. Am. Inst. Min. Eng., 1918.

Значительный интерес представляют смешанные гематит-магнетитовые руды Цзиньлинчжэня, близ Цзяочжоу, провинция Шаньдун. Сообщается, что серия рудных тел, некоторые из которых достигают 100 футов в ширину, залегает вдоль контактной зоны протяженностью два километра. [43] Месторождения эксплуатировались немцами и в настоящее время осваиваются японцами.

[43] Керт, В.: «Ресурсы железных руд мира», Стокгольм, 1910.

В провинциях Чжили и Цзянси отмечены осадочные пласты оолитовой руды некоторого распространения, однако они являются низкосортными.

Пластовые сидеритовые руды, подобные рудам каменноугольных отложений Англии, в течение многих лет добывались в провинции Шаньси и плавились в местных печах. В провинции Хунань также ведется добыча этого типа руды.

Основными железными рудами Маньчжурии являются магнетиты, залегающие в виде серии месторождений в поясе северо-западного — юго-восточного простирания к югу и юго-востоку от Мукдена, в Южной Маньчжурии. Они переслаиваются со сланцами, гнейсами и порфирами. В этом поясе находятся месторождения Аньшань, которые в настоящее время разрабатываются японскими интересами, связанными с Южно-Маньчжурской железной дорогой, и месторождения Мяоэргоу, эксплуатируемые китайско-японской компанией Pen-hsi-hu Coal & Iron Co., Ltd. Сообщается, что южно-маньчжурский магнетитовый пояс содержит запасы, составляющие около 500 миллионов тонн. [44] Большая часть руды является низкосортной.

[44] Ван, К. Ф.: «Месторождения угля и железа района Бэньсиху, Маньчжурия», Trans. Am. Inst. Min. Eng., 1918.

Индия.

—В Индии встречаются железные руды четырех типов [45]: (1) линзы зеркального гематита с некоторым количеством магнетита, залегающие в кварц-гематитовых и кварц-магнетитовых сланцах серии Дхарвар и других более древних породах; (2) гранулы магнетита и гематита, рассеянные в граните и сланцах; (3) глинистые железняки в каменноугольных отложениях Бенгалии; и (4) латеритные руды.

[45] де ла Туш, Ф. Э.: «Ресурсы железных руд мира», Стокгольм, 1910.

Гематит-магнетитовые линзы, переслаивающиеся с железистыми сланцами, являются наиболее важными из индийских руд, хотя их эксплуатация началась лишь недавно. Компания Tata Iron & Steel Co. владеет основными месторождениями этого типа, включая Майюрбхандж в Бенгалии, где в настоящее время ведется добыча, и крупными неосвоенными месторождениями округа Райпур, Центральные провинции. Важные месторождения этого типа также встречаются в Южной Индии.

Магнетит и гематит, образовавшиеся в результате разрушения сланцев и гранитов, в настоящее время используются компанией Bengal Iron & Steel Co. из Баракара. Они представляют собой поверхностные скопления железных песков и встречаются в различных частях Индии. Глинистые железняки, рассеянные в сланцах, ранее использовались компанией Bengal Iron & Steel Co., но их запасы истощены. Латеритные железные руды, залегающие на поверхности, широко распространены, но не освоены.

Основной железоделательной и сталелитейной компанией Индии является индийская фирма Tata & Sons. Ее завод, ведущий добычу с 1912 года, находится в Сакчи, Бенгалия, и включает три доменные печи с общей ежемесячной производительностью 24 000 тонн чугуна. Имеются также обширные коксовые печи, мартеновские печи и станы. Планируется множество расширений. Компания Bengal Iron & Steel Co., работающая в течение тридцати лет, имеет три небольшие доменные печи в Баракаре с ежемесячной производительностью 12 000 тонн. Сталелитейный и прокатный цеха, построенные этой компанией, были заброшены.

В индийской сталелитейной промышленности планируется несколько новых проектов, среди которых Indian Iron & Steel Co., английская фирма, строящая завод близ Асанола на Восточно-Индийской железной дороге.

Добыча железных руд в 1915 году составила 390 270 тонн, производство железа и стали в 1914 году составило 504 564 тонны, а в 1915–1916 годах — 584 775 тонн. Общий импорт железа и стали в 1914–1915 годах составил 698 635 тонн, а в 1915–1916 годах — 424 597 тонн.

Япония и Корея.

—Железная руда, используемая на японских заводах, частично поступает с отечественных рудников, а частично — с корейских, маньчжурских и китайских. Железная руда, добываемая в Японии, поступает в основном из группы месторождений Камаиси в северной части острова Хонсю. Эти рудники дают более половины общего годового объема добычи железной руды в Японии, остальная часть поступает в основном с рудников Сеннин и Курики, также расположенных в северной части Хонсю; месторождений Абута и других болотных руд на Хоккайдо, а также месторождений черных песков в Тюгоку, в южной части Хонсю. Месторождения Камаиси, Сеннин и Курики состоят из магнетита и гематита, ассоциированных с осадочными породами вблизи магматических интрузий. Запасы железной руды в Японии оцениваются Иноуэ [46] примерно в 60 миллионов тонн.

[46] Иноуэ, К.: «Ресурсы железных руд мира», Стокгольм, 1910.

Корейские железные руды, используемые в Японии, поступают в основном из поверхностных лимонитовых месторождений провинции Хванхэдо, примерно в 100 милях к северо-западу от Сеула, которые активно разрабатываются уже 10 лет или более. Недавно в Кенджипо, Корея, были созданы контролируемые японцами доменные печи, использующие руду с железного рудника Кенджипо, расположенного в том же районе, что и рудники Хванхэдо. Чугун, производимый этим заводом, отправляется в Японию для использования на японских сталелитейных заводах.

Китайская железная руда, используемая в Японии, поступает с рудников Дайе в провинции Хубэй. Часть руды с этих рудников идет непосредственно в Японию, а часть — на заводы Ханьян близ Ханькоу для переработки в чугун и стальную продукцию, которые также отправляются в Японию. Компания Han-Yeh-Ping Iron & Steel Co., владеющая как рудниками Дайе, так и заводами Ханьян, является китайским предприятием, капитал которого в настоящее время в значительной степени контролируется японскими банковскими фирмами.

Значительный интерес в настоящее время представляет освоение японцами месторождений железной руды Цзиньлинчжэнь на полуострове Цзяочжоу, провинция Шаньдун. Эти месторождения эксплуатировались немцами непосредственно перед войной и недавно были переданы японцам, которые продолжают их освоение.

Два важных контролируемых японцами проекта по производству железа и стали в настоящее время развиваются в Маньчжурии. Более старым из них является завод компании Pen-hsi-hu Colliery & Mining Co. в Бэньсиху, к юго-востоку от Мукдена, где производится чугун из руды, получаемой с соседних магнетитовых рудников Мяоэргоу. Чугун отправляется в Японию. Другим маньчжурским предприятием является железоделательный и сталелитейный завод Аньшань в Шахэкоу, к югу от Мукдена. Руда поступает с железных рудников Аньшань, а чугун и стальная продукция, производство которой планируется в будущем, будут отправляться в Японию. Также планируется отправка маньчжурской руды в Японию.

На странице 77 приведены данные о добыче и импорте железной руды в Японию за последние годы:

Table 19.—Production and Importation of Iron Ore into Japan, 1914 to 1916
(Metric tons)

Year
Produc-
tion
Importation from
Total
including
other
countries

Korea | China
1914 | 136,385 | 163,747 | 300,305 | 465,754
1915 | 136,121 | 204,101 | 311,310 | 516,132
1916 | 158,815 | 192,225 | 282,149 | 474,955

Значительное количество чугуна импортируется в Японию из Британской Индии, Великобритании и других стран.

Основные железоплавильные заводы в Японии следующие: Императорский сталелитейный завод, Явата; Железоделательный завод Камаиси, Камаиси; Железоделательный завод Ваниси, Танбури; Железоделательный завод Сеннин, Вака; Железоделательный завод Курики, Кисэн. Все они контролируются японцами, причем первый является государственным заводом Японии.

Польша.

—В Польше основными месторождениями железной руды являются лимонитовые месторождения в Вислинском районе, содержащие от 22 до 50 процентов железа. Добыча в 1912 году составила 289 000 длинных тонн. Ресурсы оцениваются в 300–800 миллионов тонн.

Бельгия.

—Добыча железной руды в Бельгии в последние годы составляла около 150 000 тонн ежегодно, из которых более половины приходилось на пласты руды «минетт» в юго-восточной части вдоль французской границы, а остальная часть поступала частично из пластов оолитового гематита девонского возраста в бассейнах Намюра и Льежа, а частично — из месторождений болотной руды в северной части. В прошлом наибольшая добыча приходилась на Намюрский бассейн, и там до сих пор имеются крупные запасы этих оолитовых гематитовых руд. Общие запасы железной руды в Бельгии оцениваются примерно в 62 500 000 тонн.

Железная руда, добываемая в Бельгии, обеспечивает лишь очень малую часть потребностей бельгийской железоделательной и сталелитейной промышленности, при этом большая часть руды импортируется из Франции.

Португалия.

—Крупнейшими месторождениями железной руды в Португалии являются месторождения Монкорво в северо-восточной части. Руда представляет собой пластовое осадочное месторождение низкого качества, а предполагаемый запас составляет 45 миллионов тонн. Небольшие месторождения магнетита и бурого гематита встречаются в южной части в провинции Алентежу. В 1913 году Португалия добыла 48 342 тонны железной руды.

Турция и Болгария.

—Незначительные месторождения магнетита и гематита встречаются в Болгарии и бывшей европейской части Турции, а в западной части Малой Азии известно несколько важных рудных тел. [47] Крупнейшее из этих месторождений находится в холмах Берут, в 90 милях к северо-западу от залива Искандерун. Сообщается, что оно способно давать 300 000 тонн ежегодно.

[47] Эдвардс, Г. М.: «Заметки о рудниках в Османской империи», Trans. Inst. Min. Met., том 23, 1913–14.

Другие важные месторождения найдены близ Аязмата, на материке напротив острова Митилини, а также близ Тиреболи и Трабзона на Черном море. Единственным действующим рудником является рудник близ Аязмата.

Чили.

—Разрозненные месторождения железной руды встречаются в Чили в прибрежном горном районе; основные месторождения простираются на расстояние около 150 миль параллельно побережью, некоторые из них находятся к северу, а некоторые — к югу от Кокимбо. Рудные тела находятся на расстоянии от 10 до 40 миль от побережья. Большинство из них заключено в виде линз в гранитных породах; некоторые залегают в осадочных породах вблизи контакта с магматическими породами.

Печи и сталелитейный завод были построены французским синдикатом 10–15 лет назад в южной части Чили. Завод проработал всего несколько месяцев, по-видимому, из-за отсутствия рынка сбыта продукции. Железная руда добывалась на месторождении Тофо, а в качестве топлива использовалась сырая древесина.

Из чилийских месторождений крупнейшее, Альгарробо, принадлежит совместному голландско-немецкому синдикату, контролируемому Wm. H. Müller & Co. и Gutehoffnungshütte. Тофо, следующее по величине после Альгарробо, находится в аренде у Bethlehem Steel Co. Большинство других месторождений принадлежат чилийцам. Тоннаж чилийской руды, контролируемый представителями разных национальностей, примерно следующий:

| Millions of tons (long tons)
German |  50
American |  40
Chilean (in part English) |  50
Total | 140

Железная руда добывалась в Тофо в течение 1914, 1915 и 1916 годов и экспортировалась в Соединенные Штаты. В 1915 году было отгружено около 153 000 тонн. Во время войны добыча практически прекратилась.

Бразилия.

—Месторождения железной руды в Минас-Жерайс, Бразилия, являются одними из самых важных в мире. Рудные тела, которые до сих пор практически не освоены, лежат на площади примерно 100 квадратных миль, центр которой находится в 225 милях по прямой линии к северу от Рио-де-Жанейро. Основными рудами являются гематиты, ассоциированные в виде пластов и линз с ламинированным железистым кварцитом, известным как «итабирит», который покрывает многие квадратные мили. Переслаивающиеся пласты и линзы руды являются высококачественными, содержат до 69 или 70 процентов металлического железа и в среднем от 0,003 до 0,025 процента фосфора. Почти все руды этого типа относятся к бессемеровскому или низкофосфористому сорту. Существуют также обширные площади недавно образовавшихся поверхностных руд, состоящих из смеси гематита и лимонита с умеренно высоким содержанием фосфора; они содержат в среднем от 55 до 65 процентов металлического железа.

Из-за удаленности от побережья и высокой стоимости транспортировки только высококачественные пластовые руды в настоящее время считаются доступными. Центральная железная дорога Бразилии проходит через район железных руд до порта Рио, в 310 милях от южной границы района, но, к сожалению, из-за крутых уклонов она не может использоваться для масштабной транспортировки железных руд. Поскольку месторождения угля, пригодного для производства железа, в Бразилии, насколько известно, отсутствуют, месторождения Минас-Жерайс до настоящего времени давали мало руды.

Основные месторождения железной руды в Минас-Жерайс принадлежат Itabria Iron Ore Co., St. John del Rey Gold Mining Co., Ltd., Brazilian Iron & Steel Co. и Compania Metallurgica, причем первые две являются английскими, третья — американской, а четвертая — бразильской. Deutsch-Luxemburgisches Bergwerks und Hütten Aktiengesellschaft (немецкая), Société Anonyme Franco-Bresiliene (французская), Jules Bernard, Mathiew Goudchaux et Cie (французская), Minas Geraes Iron Syndicate (американская) и другие владеют местными месторождениями. В следующей таблице показан приблизительный тоннаж руды, контролируемый каждой национальностью:

Таблица 20.—Бразильская железная руда, контролируемая представителями разных национальностей

| Millions of tons (long tons)
Bessemer | Non- Bessemer
English | 145 |   300
American | 160 |   420
French |  21 |    15
German |  40 |    10
Brazilian |   44 |   400
Total | 410 | 1,145

Железные руды, подобные рудам Минас-Жерайс, и магнетитовые месторождения второстепенного значения отмечены в других частях Бразилии.

Мексика.

—Мексика имеет важные месторождения железной руды в штатах Нижняя Калифорния, Коауила, Дуранго, Герреро, Мичоакан и Оахака. Крупнейшим железоделательным и сталелитейным заводом в Мексике является завод Compañia de Aciero y Fierro de Monterey в штате Нуэво-Леон, работающий на испанском капитале. Этот завод производит от 50 000 до 100 000 тонн чугуна в год. Руда поступает из Коауилы, а кокс — с близлежащих угольных месторождений. В Дуранго находится древесноугольная печь, которая простаивает уже много лет. Она принадлежит Durango Iron & Steel Co. (американская). Небольшие железоделательные предприятия существуют в Идальго, Пуэбле, Веракрусе и Оахаке. Самым известным из мексиканских месторождений железной руды является «Железная гора» (Серро-де-Меркадо) близ города Дуранго — крупное тело магнетита. В Нижней Калифорнии имеются важные месторождения железной руды в нескольких местах. Они принадлежат International Development Co., американской фирме со штаб-квартирой в Лос-Анджелесе, Калифорния. Месторождения в Герреро, Мичоакане и Оахаке, как сообщается, являются обширными.

Южная Африка.

—В Южной Африке встречаются различные месторождения низкосортной железной руды. В Трансваале имеются кремнистые осадочные гематиты и магнетиты в железистых сланцах различных возрастов, титанистые магнетиты, ассоциированные с основными магматическими породами, и местные глинистые пластовые руды; а как в Капской колонии, так и в Трансваале имеются латеритные поверхностные руды. 15-тонная доменная печь была построена в течение последнего года или двух близ Претории компанией Pretoria Iron Mines Co., Ltd. с целью производства чугуна из местных руд. Это первая попытка создания железоделательной промышленности в Южной Африке.

Австралия, Тасмания и Новая Зеландия.

—В Австралии и Новой Зеландии имеются некоторые важные месторождения железной руды, но лишь немногие из них освоены. Большая часть железной руды, добываемой в Австралии, использовалась в качестве флюса на медеплавильных, свинцовых, цинковых и других плавильных заводах; небольшое количество использовалось на двух местных железоделательных и сталелитейных заводах — заводе Broken Hill Proprietary Co. в Ньюкасле, Новый Южный Уэльс, и заводе Eskbank Iron Works в Литгоу, примерно в 75 милях к западу от Сиднея, Новый Южный Уэльс. Первый является более важным, имея в настоящее время в эксплуатации две доменные печи, а также сталеплавильные печи, рельсопрокатный и листопрокатный станы.

Среди важных австралийских месторождений железной руды — гематитовые руды Кумбинг-Парк близ Каркоара и Кадии близ Миллторпа, оба в Новом Южном Уэльсе, запасы которых оцениваются в 42 миллиона тонн руды; гематитовые месторождения района Мерчисон, примерно в 400 милях к северо-востоку от Перта, Западная Австралия, где одно единственное месторождение — Вилги-Миа — по оценкам, содержит более 25 миллионов тонн; марганцовистое железорудное месторождение Айрон-Монарх, оцениваемое в 20 миллионов тонн руды, и соседнее гематитовое месторождение Айрон-Ноб объемом в один миллион тонн, оба примерно в 40 милях от Порт-Огасты, в вершине залива Спенсер, Южная Австралия; и гематитовые месторождения горы Левиафан, оцениваемые в 10 миллионов тонн, расположенные примерно в 250 милях от Нормантона, на заливе Карпентария, Квинсленд. Многочисленные более мелкие и менее важные рудные тела встречаются во всех провинциях.

Руды Кумбинг-Парк использовались на заводе Eskbank Iron Works, где в 1916 году было произведено 90 200 тонн. Руда содержит в среднем около 55 процентов железа. Месторождение Айрон-Монарх осваивается компанией Broken Hill Proprietary Co., и руда будет использоваться на печах в Ньюкасле.

Важное месторождение железной руды, оцениваемое в 23 миллиона тонн добываемой руды, по сообщениям, находится на реке Блайт, в северо-западной части Тасмании, примерно в 6,5 милях от побережья. В последнее время ходят слухи о возможной эксплуатации этого месторождения.

В Новой Зеландии крупные месторождения лимонита встречаются в районе Нельсон, в северной части Южного острова. Основная группа месторождений, известная как Парапара, оценивается примерно в 64 миллиона тонн. Титанистые магнетитовые пески, исчисляемые миллионами тонн, как сообщается, встречаются в юго-западной части Северного острова близ Нью-Плимута.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ НАЦИЙ

Общее положение.

—Основными странами-производителями железа и стали в мире являются, в порядке их значимости: Соединенные Штаты, Германия, Великобритания, Франция, Россия, Австро-Венгрия и Бельгия. Годовое производство чугуна в этих странах в 1913 году варьировалось от 2 300 000 тонн в Бельгии до 30 900 000 тонн в Соединенных Штатах. Нормальное потребление железной руды этими странами в последние годы перед войной и их недавний максимальный годовой объем производства приведены ниже:

Таблица 21.—Максимальный годовой объем добычи и нормальное потребление железной руды основными странами-производителями железа и стали

Countries | Consumption (long tons) | Production (long tons)
United States | 62,000,000 | 75,288,851
Germany | 40,600,000 | [48]33,987,112
Great Britain | 19,000,000 | 15,997,328
France | 12,300,000 | 21,572,835
Russia | 8,900,000 | 9,362,746
Belgium | 6,800,000 | 164,734
Austria-Hungary | 5,200,000 | 5,233,055

[48] Включает добычу Люксембурга.

Цифры потребления представляют собой металлическое железо, потребленное в пересчете на железную руду, и получены на основе данных о добыче и импорте железной руды, а также импорте чугуна и сырых форм железа и стали. Экспорт железной руды, чугуна и сырых форм железа и стали не рассматривается как часть потребления стран.

Сравнение потребления и добычи показывает, что Соединенные Штаты, Франция, Россия и Австро-Венгрия были самодостаточными в том, что касалось сырьевых ресурсов для их железоделательной и сталелитейной промышленности. Великобритания и Германия зависят от иностранных государств в отношении небольшого процента своих потребностей. Бельгия производит очень малый процент от своего потребления железной руды, будучи почти полностью зависимой от иностранных источников, главным образом Франции и Германии, в отношении своих потребностей в железной руде.

В ряде стран, добывающих много железной руды, железоделательная и сталелитейная промышленность все еще находится в зачаточном состоянии. Железная руда из этих стран почти вся экспортируется в крупные страны-производители железа и стали. В следующей таблице показаны недавний максимальный годовой объем добычи и нормальное годовое потребление в некоторых из них:

Таблица 22.—Максимальный годовой объем добычи и нормальное потребление железной руды в ряде стран

Countries | Consumption (long tons) | Production (long tons)
Spain | 1,000,000 | 9,705,963
Sweden | 700,000 | 6,878,318
Cuba | ... | 1,585,431
Newfoundland | ... | 1,433,858
North Africa | ... | 1,349,000

Таким образом, значительные количества железной руды доступны из этих стран для потребления в странах, которые вынуждены импортировать железную руду и железную продукцию.

Ниже показано производство чугуна и стали в 1913 году в основных странах-производителях железа и стали в мире.

Table 23.—Pig-Iron and Steel Output of the Chief Producing Countries, 1913

Countries | Pig iron (long tons) | Steel (long tons)
United States | 30,966,152 | 31,300,874
Germany | 19,004,022 | 18,659,000
Great Britain | 10,481,917 | 7,664,000
France | 5,227,378 | 4,349,000
Russia | 4,474,757 | 4,750,000
Austria-Hungary | 2,335,170 | 2,641,000
Belgium | 2,318,767 | 2,475,000
Canada | 1,015,118 | 1,044,000
Sweden | 728,103 | 574,000
Spain | 418,061 | 359,000
Italy | 420,011 | 897,000
Japan | 236,491 | 251,000

Соединенные Штаты.

—Соединенные Штаты в течение многих лет имели в районе озера Верхнее основные месторождения железной руды в мире. В последние годы район озера Верхнее обеспечивал более двух пятых мирового объема добычи железной руды. В 1917 году в Соединенных Штатах было произведено 75 288 851 брутто-тонна железной руды, 38 647 397 брутто-тонн чугуна и 45 060 607 брутто-тонн стали по сравнению с 61 980 437 тоннами железной руды, 30 966 152 тоннами чугуна и 31 300 874 тоннами стали в 1913 году. Импорт железной руды в 1917 году составил 971 663 тонны, а сырых форм железа и стали — 306 189 тонн по сравнению с 2 594 770 тоннами железной руды и 250 592 тоннами сырых форм железа и стали, импортированными в 1913 году. Экспорт железной руды из Соединенных Штатов в 1917 году составил 1 132 313 тонн, а сырых форм железа и стали — 4 744 527 тонн по сравнению с 1 042 151 тонной железной руды и 1 278 131 тонной сырых форм железа и стали, экспортированными в 1913 году.

Эти цифры указывают на то, что в нормальное время Соединенные Штаты потребляют около 85 процентов внутреннего объема добычи железной руды при производстве готовой продукции из железа и стали. Пятнадцать процентов экспортируется либо в виде железной руды, либо в виде сырых форм железа и стали, которые перерабатываются в готовую продукцию в других странах. Из готовой продукции из железа и стали, произведенной в этой стране, сами Соединенные Штаты потребляют большую часть. Однако большие количества изделий из железа и стали, а также оборудования экспортируются и в другие страны.

Железная руда, экспортируемая из этой страны, — это в основном руда с озера Верхнее, которая идет на канадские заводы. Импортируемая железная руда — это в основном кубинская руда, которая используется на заводе Sparrow’s Point корпорации Bethlehem Steel Corporation. Этот завод имеет мощности для использования только той руды, которая прибывает морским путем, и работал почти исключительно на иностранных рудах. Кубинские железные рудники в значительной степени находятся под контролем этой компании, и в будущем ожидается увеличение их добычи.

Корпорация Bethlehem Steel Corporation также разработала обширное месторождение железной руды в Чили, откуда в первые годы Мировой войны осуществлялись некоторые поставки. В последнее время оно простаивало из-за нехватки транспортных мощностей. В будущем ожидаются крупные поставки из Чили.

Значительное количество шведской руды в последние годы импортировалось корпорацией Bethlehem Steel Corporation для дополнения своих поставок кубинской руды. Однако во время войны компания Trafikaktiebolaget Grängesberg Oxelosund сократила поставки руды и в конечном итоге полностью отказалась от экспорта руды в Соединенные Штаты. Эти поставки возобновились вскоре после прекращения военных действий в Европе.

Определенные высококачественные низкофосфористые железные руды, которые не присутствуют в Соединенных Штатах в достаточном количестве для удовлетворения внутренних потребностей, в прошлые годы импортировались из Испании, Северной Африки и в небольшой степени из Швеции. Во время войны, когда нехватка транспортных мощностей потребовала тщательного поиска источников высококачественных низкофосфористых руд в стране, выяснилось, что Соединенные Штаты в той или иной степени зависят от иностранных источников таких руд.

В Соединенных Штатах есть ряд рудников, таких как рудник Лион-Маунтин в Нью-Йорке и рудник Крэнберри в Северной Каролине, которые производят ограниченное количество высококачественной низкофосфористой руды. Несколько рудников на хребте Меномини, Мичиган, производят очень кремнистую низкофосфористую руду, которая может быть использована для частичного дополнения высококачественных руд. Значительное количество низкофосфористого пиритного остатка с заводов серной кислоты и удобрений также используется для производства низкофосфористого железа. Большая часть пирита, дающего этот остаток, импортируется из Испании, часть имеет отечественное происхождение, а часть поступает из Канады. В целом Соединенные Штаты обеспечивают около 60 процентов материала, необходимого для производства своего нормального объема низкофосфористого чугуна.

Определенные разработки, находящиеся в процессе реализации, делают вероятным, что больший процент руды, используемой для этой цели, может поставляться с отечественных рудников. Основным предприятием является то, которое планирует обогащение кремнистой магнетитовой руды восточной части хребта Месаби. Эксперименты дали высококачественный продукт, и планируются работы в коммерческих масштабах.

Запасы обычных сортов железной руды в Соединенных Штатах велики, и дефицита такой руды в течение многих лет не ожидается. Они легко могут обеспечить значительно возросшее потребление. Крупнейшие запасы находятся в районе озера Верхнее и в юго-восточных штатах, но крупные нетронутые запасы встречаются и в западных штатах. Железные руды в регионе Тихоокеанского побережья остаются неосвоенными из-за отсутствия достаточного спроса на чугун и сырые формы железа и стали на Тихоокеанском побережье. Несомненно, этот спрос в будущем возрастет, и там будут созданы железоделательные и сталелитейные производства.

Запасы руды в районе озера Верхнее велики. Однако качество добываемой руды постепенно снижается, и возможно, что через несколько лет придется использовать железные руды озера Верхнее со средним содержанием значительно ниже 50 процентов. В настоящее время среднее содержание руд, добываемых в районе озера Верхнее, составляет около 51 процента.

Ясно, что дефицит обычных сортов железной руды в Соединенных Штатах вряд ли возникнет. Однако запасы высококачественных руд постепенно истощаются, и высококачественные руды из иностранных государств будут находить все более готовый рынок сбыта. Американский капитал контролирует крупный запас высококачественной железной руды в Бразилии. Большая часть бразильской руды содержит около 68 процентов металлического железа и очень мало фосфора, что делает ее чрезвычайно желательным сырьем для производства специального железа и для смешивания с низкосортными отечественными рудами. Несомненно, большая часть бразильской руды пойдет в Европу, так как британские и другие иностранные владения этой рудой обширны. Однако весьма желательно, чтобы определенная доля этой руды направлялась на американские заводы.

Германия.

—Годовое потребление железной руды в Германии непосредственно перед войной составляло около 40 миллионов тонн, а максимальный годовой объем добычи в это время, включая более 7 миллионов тонн из Люксембурга, составлял лишь около 34 миллионов длинных тонн. Поэтому для снабжения немецких заводов необходимо было импортировать более 6 миллионов тонн железной руды из иностранных государств. Более 58 процентов железной руды, добываемой в Германии, поступало из Лотарингского района. Добыча на немецких железных рудниках за пределами Лотарингского района составила 6 906 809 тонн в 1913 году. Производство чугуна в том году составило 19 004 022 тонны.

Довоенный импорт железной руды в Германию был значительным, составив почти 14 миллионов тонн в 1913 году; против этого экспорт составил несколько более 2 миллионов тонн.

Железная руда, импортируемая из Швеции, — это в основном высокофосфористая руда с рудников шведской Лапландии и центральной Швеции. Она особенно приспособлена для производства чугуна для томасовского процесса, широко используемого в Германии. Большинство руд из Лотарингского района имеют содержание фосфора, слегка недостаточное для томасовского процесса; и шведские высокофосфористые руды, фосфориты и фосфатные шлаки местами смешиваются с лотарингской рудой для повышения содержания фосфора.

Значительное количество низкофосфористой железной руды, используемой при производстве низкофосфористого чугуна, также импортируется из Швеции, а большее количество этой руды импортируется из Испании. Этот материал используется в Германии для производства чугуна, который будет использоваться при изготовлении стали в кислой мартеновской печи.

Поскольку Германия потеряла лотарингские железорудные месторождения, оставшиеся отечественные железные рудники смогут обеспечить менее 20 процентов потребностей в железной руде для немецких заводов. Однако вероятно, что Германия продолжит получать большую часть своих поставок с лотарингских месторождений, в которых немецкие владения в настоящее время преобладают над французскими и, вероятно, будут преобладать и в дальнейшем.

Великобритания.

—Соединенное Королевство производило от 10 до 14 процентов железа и стали в мире ежегодно в течение последних 10 лет или более и, по-видимому, потребляло в нормальное время около 50 процентов продукции и экспортировало 50 процентов, главным образом в британские владения. Во время войны около 75 процентов британского производства потреблялось внутри страны, а 25 процентов экспортировалось, в основном во Францию. Пятьдесят процентов произведенной продукции из железа и стали было получено из руд, добытых в Великобритании, и 50 процентов — из импортных руд. Таким образом, в нормальных условиях внутренний объем добычи железной руды примерно равен внутреннему спросу на железо, тогда как во время войны внутренний спрос на железо был больше, чем внутреннее предложение руды. Великобритания зависит от внешних источников в отношении одной трети своего предложения железной руды, и это составляет источник около половины железной продукции.

Железная промышленность в Великобритании до войны слабо контролировалась торговцами, которые выступали посредниками между производителем и потребителем, что не работало в пользу потребителя. [49] Британские производители имели мало интересов за рубежом и сами были недостаточно организованы для успешной работы. Если бы источники иностранной железной руды были отрезаны, ситуация могла бы стать критической и чрезвычайно затруднительной до тех пор, пока не была бы расширена отечественная горнодобывающая промышленность. Чтобы справиться с этим условием, комитет Совета по торговле Великобритании рекомендовал консолидацию железных интересов путем формирования синдиката для закупки и распределения железных руд и, в частности, для приобретения интересов за рубежом. Этот синдикат должен был бы создать торговые агентства и организовать транспортировку и торговлю, подобно организации W. H. Müller & Co. из Гааги. Комитет рекомендовал, чтобы эти операции поддерживались правительством и чтобы все ресурсы Британской империи находились под контролем правительства, особенно в отношении предоставления концессий иностранцам и введения ограничений в пользу отечественных производителей. Недавно сообщалось, что железные интересы организовались по указанным направлениям.

[49] Британский Совет по торговле, «Отчеты о железе и стали», Лондон.

Франция.

—Годовое потребление железной руды во Франции для производства чугуна и сырых форм железа и стали составляет около 12 миллионов тонн в нормальных условиях. Производственная мощность железных рудников Франции составляет более 21 миллиона, оставляя излишек в 9 миллионов тонн руды, ежегодно доступный для экспорта. Более 90 процентов железной руды, производимой во Франции, добывается на лотарингских железных рудниках.

Большая часть руды, экспортируемой из Франции в прошлом, шла на немецкие доменные печи. Многое шло в Бельгию. Импорт железной руды невелик, в основном это высококачественная руда из Швеции, в которой Франция испытывает недостаток. Французские владения в Северной Африке имеют крупные запасы высококачественной руды, но основная часть добываемой там руды шла в Англию и Германию.

В результате войны та часть лотарингских железорудных месторождений, которая находилась в границах спорных провинций Эльзас и Лотарингия, была передана Франции, которая таким образом получила контроль над всей добычей великих лотарингских железорудных месторождений, за исключением части, включенной в Люксембург. Добыча на лотарингских железорудных месторождениях, включая часть, которая ранее принадлежала Германии, составляла почти 48 миллионов тонн ежегодно, из которых около 7 миллионов тонн добывается в Люксембурге. За пределами Лотарингского района Франция производит около 1 500 000 тонн руды. Таким образом, если только производство железа и стали во Франции значительно не расширится, будет добываться много железной руды для экспорта.

Россия.

—В 1913 году Россия занимала шестое место по добыче железной руды и пятое по производству чугуна, производя около 4,5 процента мировой добычи железной руды и 6 процентов чугуна.

Запасы железной руды в России оцениваются примерно в 1 600 миллионов тонн, часть из которых, особенно в центральной России, экономически нерентабельна для добычи. Район южной России важен из-за своих крупных запасов, большого объема добычи и своего расположения. Это особенно верно в настоящее время из-за потребности Германии в железной руде для будущего использования.

Добыча железной руды в России выросла с примерно 2 миллионов тонн ежегодно в 1891–1893 годах до 7 или 8 миллионов тонн ежегодно в 1913–1917 годах. Южная Россия (почти исключительно Криворожский район) произвела почти 7 миллионов тонн в 1913 году, но к 1916 году добыча в этом регионе сократилась вдвое, а разница была восполнена за счет других регионов. [50] В период с 1913 по 1917 год Россия производила около 4 миллионов тонн чугуна ежегодно, из которых 3 миллиона тонн приходилось на Южную Россию, а большая часть остального — на Уральский регион.

[50] Консультативный совет, Департамент научных и промышленных исследований, «Отчет об источниках и добыче железа и других металлосодержащих руд, используемых в железоделательной и сталелитейной промышленности», 1918. Также Британский Совет по торговле, «Отчеты о железе и стали», Лондон; и Ironmonger Metal Market Year Book, 1918.

В 1916 году Центральный военно-промышленный комитет оценил ежемесячные потребности всей страны в 300 000 тонн чугуна для военных целей и в 80 000 тонн для нужд гражданского населения, что составило общее годовое потребление около 4 500 000 тонн, или лишь около половины нормального потребления. В 1917 году общая добыча в стране, по оценкам, составила лишь 30 процентов от этих минимальных потребностей.

Ситуация в России настолько нестабильна, что заявление о текущих условиях в сталелитейной промышленности не имеет ценности. Однако разумно предположить, что ситуация с железом и сталью существенно не изменится в отношении операций и контроля. Более того, можно с уверенностью предсказать, что Польша будет развиваться быстрее как производитель железной руды в будущем, так как в прошлом она была ограничена запретами на экспорт руды.

Бельгия.

—Бельгия была незначительным производителем железной руды, но была сравнительно крупным импортером железной руды и производителем чугуна. Страна занимала шестое место как производитель чугуна в 1913 году, в котором она произвела 147 048 тонн руды и импортировала 4 400 000 тонн. [51]

[51] Совет по торговле, «Отчеты о железе и стали», Лондон.

Бельгийские железоделательные заводы были сильно повреждены немцами во время войны, и, вероятно, пройдет некоторое время, прежде чем промышленность снова достигнет положения, которое она занимала до войны. Однако страна предлагает хороший рынок сбыта для железных руд Франции и в будущие годы должна стать более крупным производителем изделий из железа и стали.

Бельгия практически зависит от внешних источников в отношении поставок руды, но удобно расположена как рынок сбыта для руд из многих стран. Общие запасы железной руды в стране оцениваются в 62 500 000 тонн, чего недостаточно, чтобы продержаться 10 лет при текущем уровне потребления.

Австро-Венгрия.

—Бывшая Австро-Венгерская империя давала в последние годы от 2 до 3 процентов мировой годовой добычи железной руды и около 2 процентов производства чугуна; поэтому она имела второстепенное значение в железной промышленности. Запасы руды оцениваются в 284 миллиона тонн доступной руды и 807 миллионов тонн дополнительной вероятной руды.

Текущие нестабильные условия, вероятно, приведут к значительным изменениям в эксплуатации и контроле железных рудников и заводов. В конечном итоге потрясения могут стимулировать железную промышленность, но результат не должен существенно изменить международное положение.

Япония.

—Железоделательная и сталелитейная промышленность Японии невелика по сравнению с промышленностью Соединенных Штатов, Германии, Великобритании и других ведущих стран-производителей железа и стали. Общие запасы железной руды, вероятно, составляют не более 60 миллионов тонн, или меньше, чем добывалось ежегодно в районе озера Верхнее в последние годы. Однако сталелитейная промышленность быстро расширяется, и в настоящее время доменные печи, сталеплавильные печи и сталелитейные заводы строятся в Японии, Корее, Маньчжурии и Китае японскими интересами.

Добыча железной руды в Японии совершенно неадекватна для снабжения этой расширяющейся промышленности. Добыча железной руды в Японии в последние годы составляла в среднем около 150 000 тонн ежегодно, тогда как потребление сырых, полусырых и промышленных изделий из железа и стали составляет примерно 1 500 000 тонн. Таким образом, чтобы удовлетворить свои потребности со своих собственных производственных мощностей, Японии потребовалось бы около 3 миллионов тонн железной руды ежегодно. По сравнению с этим, общее потребление железной руды в Японии, как импортной, так и отечественной, составляет менее 700 000 тонн. Остальная часть железа и стали, требуемая в Японии, импортируется в виде чугуна и сырых и промышленных изделий.

Япония прилагает большие усилия для освоения месторождений железной руды в соседних странах, особенно в Китае, Маньчжурии и Корее; и добыча из этих источников, которая идет на контролируемые японцами заводы, быстро растет. Среди более недавних японских железоделательных и сталелитейных предприятий в этих странах — доменные печи и сталелитейный завод, строящиеся в Аньшане, к югу от Мукдена, в Маньчжурии; доменные печи в Бэньсиху, к юго-востоку от Мукдена, в Маньчжурии; и доменные печи в Кенджипо, в Корее. Последние два из этих заводов в настоящее время производят чугун, который отправляется в Японию. В будущем на всех трех заводах, вероятно, будут построены сталелитейные цеха. Месторождения железной руды разрабатываются в связи со всеми из них. Помимо использования на местных доменных печах, железная руда отправляется в Японию с этих рудников. В Китае наиболее важным железоделательным и сталелитейным предприятием является предприятие в Ханьяне, в провинции Хубэй. Эта операция была начата компанией Han-Yeh-Ping Iron & Steel Co. как китайское предприятие в связи с рудниками Дайе в той же провинции. Однако эта компания столкнулась с финансовыми трудностями, и потребовался японский капитал, чтобы работа могла продолжаться. В настоящее время под японским руководством происходит значительное расширение завода. Железная руда с рудников Дайе и чугун с завода в Ханьяне отправляются в Японию для использования на японских железоделательных и сталелитейных заводах.

Сомнительно, что при быстром расширении японской железоделательной и сталелитейной промышленности рудники в Китае, Маньчжурии и Корее смогут развиваться достаточно быстро, чтобы обеспечить необходимое сырье. Ходят слухи, что в настоящее время осваивается несколько месторождений железной руды в восточном Китае, включая месторождение Цзиньлинчжэнь, и они могут дать некоторое дополнительное предложение. Железные рудники Индии также могут быть призваны поставлять Японии больше железной руды, чем они делали это в прошлом. Единственные другие важные месторождения железной руды, известные в других местах на Востоке, находятся на Филиппинских островах. Эти месторождения, как сообщается, довольно важны, и они выгодно расположены для снабжения японских заводов. Они контролируются американцами.

Текущее расширение японской железоделательной и сталелитейной промышленности таково, что возникает вопрос, будет ли потребление железной продукции в Японии достаточным, чтобы поглотить весь объем производства. Кажется очень вероятным, что Япония ищет возможности для крупного экспортного рынка продукции из железа и стали. Японцы могут быть амбициозны не только в том, чтобы вытеснить европейские и американские товары на Востоке, но могут даже попытаться обеспечить рынок на Тихоокеанском побережье Соединенных Штатов и Канады. Вполне вероятно, что японские промышленные изделия смогут конкурировать в западной части Соединенных Штатов с изделиями, произведенными в восточных штатах и облагаемыми высокими транспортными тарифами. С другой стороны, существует активное движение за создание железной промышленности на Тихоокеанском побережье, и есть надежда, что заводы, созданные там, смогут производить изделия из железа и стали по достаточно низкой цене, чтобы позволить им конкурировать с японской продукцией на Востоке.

ГЛАВА IV МАРГАНЕЦ Д. Ф. Хьюитт

ПРИМЕНЕНИЕ МАРГАНЦА

Сплавы марганца имеют важное значение в производстве стали мартеновским и бессемеровским способами, на долю которых приходится 99 процентов общего объема производства в Соединенных Штатах. В этой стране при выплавке тонны стали среднего качества используется около 14 фунтов металлического марганца в виде сплавов, что эквивалентно примерно 40 фунтам высокосортной руды. Широко применяются два сплава: ферромарганец и зеркальный чугун (шпигель). Ферромарганец, содержащий от 70 до 80 процентов марганца, в основном используется при производстве мартеновской стали с содержанием углерода менее 0,30 процента, тогда как зеркальный чугун, содержащий от 20 до 32 процентов марганца, применяется при производстве бессемеровской стали с содержанием углерода более 0,30 процента. Первая группа низкоуглеродистых сталей используется для изготовления конструкционных профилей, листового металла, прутков, проволоки и т. д., а вторая группа высокоуглеродистых сталей — для изготовления рельсов, поковок и т. д.

Для производства ферромарганца с содержанием марганца от 70 до 80 процентов требуется так называемая «высокосортная» руда, содержащая более 35 процентов марганца и менее 5 процентов железа и 15 процентов кремнезема. Для производства зеркального чугуна с содержанием марганца от 20 до 32 процентов требуется так называемая «низкосортная» или железистая марганцевая руда, содержащая от 10 до 35 процентов марганца, от 20 до 35 процентов железа и менее 20 процентов кремнезема, хотя местами зеркальный чугун получают путем смешивания высокосортной марганцевой руды с железной рудой.

Ряд других сплавов, таких как силикомарганец, ферросилиций и ферроуглеродтитан, могут использоваться в качестве частичных заменителей ферромарганца, но, хотя они могут найти более широкое применение в условиях дефицита, они являются продуктами электропечей, и при нормальных условиях их стоимость является запретительно высокой.

Очень чистый оксид марганца используется при производстве обычных сухих батарей, выпуск которых значительно увеличился в связи с широким использованием двигателей внутреннего сгорания. Ежегодно в Соединенных Штатах для этой цели расходуется около 25 000 тонн. Используемый таким образом оксид марганца не потребляется, но истощается из-за потери кислорода. В условиях высоких цен оксид может быть регенерирован путем обработки или смешивания с новым рафинированным материалом.

Небольшие количества марганцевой руды используются при производстве многих химических продуктов и пигментов.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Любое рассмотрение потребности в марганцевой руде и ферромарганце, а также зависимости от иностранных источников поставок должно учитывать степень, в которой низкосортная руда и зеркальный чугун могут использоваться в качестве заменителей высокосортной руды и ферромарганца. Так, хотя и Германия, и Соединенные Штаты обладают лишь незначительными запасами высокосортной руды, обе страны располагают необычайно большими запасами низкосортной руды. В недавних условиях в Соединенных Штатах доля общего объема марганца, используемого в виде зеркального чугуна, за три года увеличилась с 10 до примерно 18 процентов. Компетентные органы подсчитали, что эта замена может быть дополнительно увеличена почти до 70 процентов при незначительных изменениях в практике и скромном дополнении оборудования. Некоторые компетентные инженеры далее утверждают, что за счет других изменений в практике значительная часть марганца, необходимого в настоящее время в виде сплавов, может быть исключена путем добавления низкосортной марганцевой руды на ранних стадиях процесса плавки и рафинирования.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Хотя концентрированные массы, полезные для промышленности, встречаются довольно редко, марганец широко распространен по всей Земле; он входит в состав около 100 минералов, и большинство обычных горных пород, как магматических, так и осадочных, содержат от 0,1 до 2 процентов марганца.

Современные требования к сортности таковы, что марганцевые руды в основном представлены оксидами. Карбонат, родохрозит, содержит достаточно марганца, чтобы позволить использовать его при производстве 80-процентного ферромарганца, но лишь в немногих местах эти массы достаточно велики, чтобы служить основой для масштабной добычи. Обычный силикат содержит 43 процента марганца, но содержание кремнезема в нем настолько высоко (23 процента), что он не может быть использован в чистом виде при производстве обычных сплавов.

Обычные оксиды марганца отлагаются в самых разных условиях, которые встречаются вблизи поверхности Земли. Крупные массы оксидов отлагались в мелководных морских бассейнах, в мелководных пресноводных бассейнах и в других условиях в относительно тонком слое выветрелых пород, который встречается по всему миру. Хотя большинство этих крупных масс сформировалось в приповерхностной зоне, где подстилающие невыветрелые породы необычайно богаты марганцем, некоторые крупные массы оксидов накапливаются при особо благоприятных условиях за счет концентрации небольших количеств марганца, рассеянного в обычных горных породах.

Для целей геологического изучения месторождения оксидов марганца можно разделить на две группы: (1) месторождения, производные от более или менее локализованных масс карбонатных или силикатных материалов, как правило, с содержанием марганца более 5 процентов, которые, по-видимому, не имеют связи с поверхностью Земли; и (2) месторождения, первоначально отложившиеся вблизи поверхности в виде локализованных тел оксидов.

К первой группе относятся зоны карбонатных или силикатных пород в контакте с интрузивными магматическими породами, подобные тем, что встречаются в Бразилии и Индии. Эти зоны содержат марганцовистые карбонаты (смешанные с железом, известью и магнезией) и силикаты (спессартин или марганцевый гранат, пьемонтит или марганцевый эпидот и, возможно, родонит или марганцевый пироксен). В результате выветривания таких пород образовались крупные тела высокосортных оксидов.

Марганец также встречается в жилах или прилегающих вмещающих породах в регионах, куда внедрялись магматические породы. Жилы обычно содержат родохрозит, марганцовистый сидерит или родонит, ассоциированные с кварцем и металлическими сульфидными минералами, включая алабандин, сульфид марганца. Такие жилы известны в Филипсбурге и Бьютте, штат Монтана; Силвертоне, штат Колорадо, и в других местах. В таких регионах, если вмещающие породы, прилегающие к трещинам, представлены известняком или доломитом, они могут быть в значительной степени замещены марганцовистым сидеритом или другими карбонатами, которые при выветривании образуют крупные тела оксидов марганца, местами смешанные с оксидами железа. Такие тела известны в Ледвилле, штат Колорадо.

Марганец, существующий в отложениях, преимущественно глинистых, но частично карбонатных, может локально мигрировать после того, как отложения оказываются слегка погребенными, и образовывать зоны марганцовистых карбонатных и силикатных конкреций, параллельных напластованию. Там, где, как в округе Бейтсвилл, штат Арканзас, эти зоны обнажаются в результате эрозии, марганец дополнительно концентрируется в виде масс оксидов в остаточной глине.

Метаморфические породы, такие как сланцы, местами, как в Испании, Ньюфаундленде, Калифорнии и Вашингтоне, содержат обширные линзы родонита или другого силиката с родохрозитом или без него, примерно параллельные напластованию. Происхождение этих линз, которые обычно находятся довольно далеко от магматических интрузий, неясно. Некоторые из них считаются материалами, отложившимися во время осадконакопления, другие, как полагают, представляют собой концентрации, возникшие во время метаморфизма, когда осадочные породы были глубоко погребены.

Ко второй упомянутой выше группе (марганцевые месторождения, первоначально сконцентрированные вблизи поверхности в виде оксидов) относятся обширные месторождения оксидов, переслаивающиеся с морскими отложениями, как в Кавказском регионе, Россия. Другие, переслаивающиеся с вулканическим материалом, туфами и лавовыми потоками, известны в Средиземноморском регионе и в Чили. В Индии важные пласты оксидов переслаиваются с кварцитом и сланцем.

Многие месторождения оксидов недавно сформировались и, вероятно, формируются в настоящее время в болотах во многих регионах, особенно в Нью-Брансуике, Канада. Они не являются важными источниками добычи.

Хотя, по-видимому, не существует простой закономерности, определяющей распределение марганца в невыветрелых породах, есть основания полагать, что накоплению оксидов марганца в коре выветривания благоприятствуют климатические условия, вызывающие необычайно полное или глубокое разрушение пород. Хотя несколько месторождений оксидов марганца обнаружены в пределах поясов недавнего оледенения, а некоторые не имеют отношения к выветриванию, большинство важных месторождений встречается в районах, которые в настоящее время или в недавнем прошлом отличались теплым влажным климатом, и есть основания подозревать, что такие районы дадут и другие важные месторождения.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Северная Америка.

— В Соединенных Штатах распространение марганцевой руды можно наиболее четко описать, сгруппировав районы по сортности руды: (1) высокосортная, содержащая 35 процентов или более марганца, которая обычно используется для производства высокосортного сплава, ферромарганца, и (2) низкосортная, железистая марганцевая руда, обычно используемая для низкосортного ферросплава, зеркального чугуна. Страна испытывает дефицит природных запасов первой, но обладает обильными ресурсами второй, которая под давлением необходимости могла бы в значительной степени заменить высокосортную руду, импортируемую в настоящее время в основном из-за рубежа.

Следующие районы в Соединенных Штатах дают высокосортную руду:

В Филипсбурге, штат Монтана, находятся тела карбоната марганца, замещающие кембрийский известняк вблизи жил и контактов с магматическими породами. Они выветрились до состояния оксидов на глубину около 200 футов от поверхности. В Бьютте, штат Монтана, жилы в граните содержат карбонат и силикат марганца, местами выветрелые до оксидов.

В долине Шенандоа в Вирджинии, а также в аналогичных долинах в Теннесси и Джорджии остаточные глины, образовавшиеся из определенных кембрийских известняков и силурийских сланцев и песчаников, содержат тела оксидов марганца на глубинах от 200 до 250 футов от поверхности. Многие небольшие месторождения также встречаются в Арканзасе, Аризоне, Калифорнии, Неваде и Юте.

The total production of the United States from 1838 to 1918 was 893,734 tons, and the maximum was 305,869 tons in 1918.

Среди основных районов, дающих руду более низкого сорта (от 10 до 35 процентов марганца), наиболее примечательным является район Кайюна в Миннесоте, где пласты железо-марганцевого карбоната докембрийского возраста выветрились до оксидов на глубину от 250 до 500 футов от поверхности и содержат рудные тела с содержанием марганца от 7 до 20 процентов и железа от 25 до 50 процентов. Отдельные месторождения варьируются от 50 000 до 7 500 000 тонн каждое. С момента первых поставок в 1913 году объем добычи по 1918 год включительно составил 1 666 677 тонн руды с содержанием марганца более 5 процентов.

Крупные месторождения низкосортной марганцевой руды также встречаются в районе Ледвилл в Колорадо, где нерегулярные тела железо-марганцевого карбоната замещают магнезиальный известняк каменноугольного периода и выветрились до оксидов на глубину до 850 футов. С 1885 по 1918 год общий объем добычи составил 3 202 678 тонн материала, большая часть которого содержала от 15 до 30 процентов марганца.

Другие месторождения железистой марганцевой руды эксплуатировались в округе Игл, Колорадо; районе Пайоче, Невада; районе Силвер-Сити, Нью-Мексико; а также в Арканзасе, Джорджии и Вирджинии.

В Канаде крупные месторождения кремнистых марганцевых руд встречаются на Ньюфаундленде, а также имеется несколько небольших месторождений в Нью-Брансуике, Альберте и Британской Колумбии.

В Коста-Рике марганец встречается в четырех районах вблизи Плайя-Реаль, полуостров Никоя, в форме оксидов, которые, по-видимому, переслаиваются с осадочными породами. Наиболее продуктивные месторождения принадлежат гражданам Соединенных Штатов и Кубы; другие полностью принадлежат кубинцам. Они начали эксплуатироваться в 1916 году, и к концу 1918 года в Соединенные Штаты было экспортировано 18 000 тонн.

На Кубе марганец добывается вблизи Сантьяго и Буэйсито в провинции Орьенте. Вблизи Сантьяго оксиды марганца встречаются в виде линзовидных или нерегулярных тел в туфе, глине и известняке. Другие месторождения отмечены в провинциях Санта-Клара и Пинар-дель-Рио. Рудники, которые были источником более 90 процентов экспорта, принадлежат совместно гражданам Кубы и Соединенных Штатов, а остальные рудники — кубинцам.

С 1888 по 1910 год было экспортировано 266 621 тонна. В 1915 году, после четырех лет простоя, рудники были вновь открыты, и импорт в Соединенные Штаты с 1915 по 1918 год включительно составил 163 189 тонн. [52]

[52] Данные о добыче приведены в длинных тоннах, если не указано иное.

В Мексике марганцевые руды найдены в четырех милях к северу от города Чиуауа и к югу от Паломаса в штате Чиуауа. Предполагается, что месторождения принадлежат коренным мексиканцам. Марганец также встречается вблизи залива Консепсьон, Нижняя Калифорния, где рудники принадлежат коренным мексиканцам, но находятся в аренде у американцев. Из обоих этих районов в 1917 году было добыто и экспортировано в Соединенные Штаты 1 500 тонн.

В Республике Панама, вблизи Номбре-де-Диос и Мадинги, имеются нерегулярные линзы оксидов марганца в разложившихся осадочных пластах. Вблизи Номбре-де-Диос эксплуатировалось семь групп месторождений. Пять из них эксплуатировались американцами, одна — местными владельцами и одна — французами. Месторождения Номбре-де-Диос дали 50 000 тонн руды с 1871 по 1902 год, в основном за последние шесть лет. Месторождения Мадинги были открыты в 1916 году, и в течение 1916 и 1917 годов в Соединенные Штаты было экспортировано 11 000 тонн.

Южная Америка.

— Крупнейшие месторождения марганцевой руды в Южной Америке находятся в Бразилии, особенно в важном горнодобывающем штате Минас-Жерайс.

В районе Лафайет в этом штате оксиды марганца встречаются в виде широких линзовидных тел, которые, по-видимому, не имеют определенного расположения или ассоциации, за исключением того, что большинство из них ограничено сланцами или гнейсами. Месторождения залегают в комплексе гранитов, гнейсов и кристаллических сланцев; оксиды марганца, вероятно, являются производными марганецсодержащих карбонатных и силикатных минералов. Наиболее продуктивная область, известная как Морру-да-Мина, размером 2500 футов в длину и 1000 футов в ширину, содержит четыре отдельных тела длиной от 320 до 1300 футов и шириной от 48 до 320 футов. Здесь оксиды марганца сохраняются на глубине 410 футов от поверхности.

The area has yielded about 1,000,000 tons of ore and the reserves are probably between 7,000,000 and 10,000,000 tons.

В том же штате Минас-Жерайс, в районах Мигель-Бурнье и Ору-Прету, оксиды марганца переслаиваются с железистыми осадочными породами докембрийского возраста.

В штате Баия район Назарет содержит тела оксида марганца в мощной приповерхностной зоне сильно выветрелых сланцеватых пород. Оксиды, вероятно, являются производными линз марганцевого граната в сланцах. Крупнейшее месторождение дало 70 000 тонн руды. Марганцевые месторождения также отмечены вблизи Бом-Фин в том же штате.

Другие месторождения марганцевой руды в Бразилии отмечены в штатах Мараньян и Мату-Гросу.

Известные марганцевые месторождения Минас-Жерайс лежат в пределах площади около 30 квадратных миль, центр которой находится примерно в 300 милях к северу от Рио-де-Жанейро. Руда легко добывается открытым способом, но существующие транспортные и погрузочные мощности практически ограничивают годовой экспорт 550 000 тонн.

Большинство важных месторождений в районах Лафайет-Мигель-Бурнье и Ору-Прету принадлежат местным бразильцам. В 1915 году немецкая компания разрабатывала часть месторождения Морру-да-Мина в течение шести или семи лет и произвела в общей сложности 200 000 тонн руды. В течение 1915 года бельгийская компания эксплуатировала рудник Кокуруту вблизи Ору-Прету и отгружала 2 000 тонн ежемесячно. Крупнейшее месторождение района Назарет принадлежит американцу, а неразработанные месторождения вблизи Туриасу принадлежат норвежцам.

С начала развития отрасли в 1894 году по 1918 год из Бразилии было экспортировано 4 660 000 тонн марганцевой руды. С 1900 по 1913 год годовой экспорт варьировался от 99 000 до 250 000 тонн, но с устранением российских источников в 1914 году экспорт вырос до 503 130 тонн в 1916 году, 532 855 тонн в 1917 году и 393 388 тонн в 1918 году. В октябре 1917 года экспортная пошлина на марганцевую руду была повышена с 0,85 до 3,00 долларов за метрическую тонну. Еще до войны значительная часть бразильского экспорта направлялась в Соединенные Штаты. Направления экспорта 1913 года были следующими: Соединенные Штаты — 60 процентов; Германия — 18 процентов; Великобритания — 16 процентов; Франция — 6 процентов.

В Чили марганцевые руды встречаются в Корраль-Кемада и близлежащих районах в штате Кокимбо. В этих районах пласты оксидов марганца переслаиваются с песчаником, сланцем и вулканическими потоками. Марганец также найден в районе Каррисаль в штате Атакама, где пласты оксидов марганца перемежаются со сланцами и известняком. С 1885 года, когда начались исследования, по 1905 год экспорт марганцевых руд из чилийских портов составил 549 716 тонн, при этом максимальный экспорт за один год составил 50 871 тонну в 1892 году.

В Уругвае месторождения железистой марганцевой руды, по сообщениям, содержащие 80 500 000 тонн, встречаются в Сапукае, департамент Ривера.

Европа.

— В бывшей империи Австро-Венгрии основной марганцевый район находится вблизи Дорна-Ватра в Буковине. Здесь имеются линзы карбоната и силиката марганца в сланцах, которые выветрились до оксидов вблизи поверхности. Месторождения принадлежат Буковинской греческой церкви. Среднегодовая добыча с 1906 по 1912 год составляла 13 600 тонн. Другие месторождения отмечены в Богемии, Истрии, Штирии, Венгрии и Боснии. С 1901 года добыча в Австро-Венгрии варьировалась от 18 000 до 25 000 тонн ежегодно.

В Бельгии, вблизи Шеврона в провинции Льеж, железистые оксиды марганца образовались в результате выветривания карбонатов марганца и железа. С 1901 года годовая добыча в мирное время варьировалась от 2 000 до 15 000 тонн.

Во Франции марганец встречается главным образом вблизи Романеша в департаменте Сона и Луара, где несколько тел оксидов марганца залегают в разломе между осадочными породами и гранитом. Месторождение известно с 1823 года, и добыча в 1901 году составила 9 500 тонн. Другие французские месторождения исследовались в департаментах Верхние Пиренеи, Арьеж, Алье, Од и Ньевр. Годовая добыча довольно устойчиво снижалась с 22 000 тонн в 1901 году до 6 000 тонн в 1913 году. Владение французскими марганцевыми месторождениями, по-видимому, в основном французское, возможно, при некоторой поддержке английского капитала.

В Германии марганцевая руда лучшего типа, содержащая более 30 процентов металла, встречается в Саксен-Гота, Центральная Германия, в небольших жилах карбонатов марганца и железа, выветрелых вблизи поверхности до оксидов. Руда аналогичного сорта встречается в небольших количествах в Гессене и Вальдеке в Рейнской Пруссии.

Марганцовистая железная руда, содержащая от 12 до 30 процентов марганца, встречается в Гессен-Нассау, Рейнская Пруссия, где оксиды марганца и железа образуют нерегулярные плоские линзы, залегающие в глинах, образовавшихся в результате выветривания подстилающего девонского известняка. В период с 1907 по 1911 год девять месторождений давали от 262 000 до 283 000 тонн ежегодно.

Марганцовистая железная руда (содержащая менее 12 процентов марганца) встречается в Зигерланде и Нассау, Рейнская Пруссия. Жилы крупные и содержат марганцовистый сидерит; они прорезают девонские отложения. Эти месторождения в основном принадлежат основным металлургическим заводам Рейнской Пруссии. В период с 1907 по 1911 год годовая добыча варьировалась от 2 200 000 до 2 600 000 тонн.

В Великобритании основные месторождения находятся в Северном Уэльсе. Встречаются жилы карбоната и силиката марганца, а также переслаивающиеся линзы. Материал содержит от 20 до 36 процентов марганца. Другие месторождения отмечены в Девоншире, Корнуолле и Шропшире. Максимальная добыча в Великобритании, составившая около 23 000 тонн, была достигнута в 1906 году, когда два рудника в Северном Уэльсе дали 19 300 тонн.

Марганец встречается в Греции, в западной части острова Милос, где конкреции и массы оксидов марганца рассеяны в пластах туфов плиоценового возраста. Максимальная добыча в 15 000 тонн была зафиксирована в 1902 году. С тех пор объем производства неуклонно снижался до 550 тонн в 1913 году. Марганец также встречается на полуострове Кассандра, который ранее входил в состав европейской Турции. Жила, разрабатывавшаяся главным образом на серебросодержащий галенит, дает оксиды марганца из приповерхностной зоны. Максимальная добыча в 52 000 тонн была достигнута в 1902 году, после чего неуклонно снижалась до 12 000 тонн в 1910 году.

В Италии марганец есть в Тоскане, где нерегулярные тела оксидов марганца и железа встречаются в триасовых известняках. Другие месторождения в Лигурии и на Сардинии недавно дали немного руды. Из максимальной добычи в Италии в 18 147 метрических тонн (от 18 до 45 процентов марганца) в 1916 году 14 072 метрические тонны были получены из месторождений в Тоскане. Обычно годовая добыча варьировалась от 1 600 до 4 700 тонн.

В Португалии марганец есть в Алентежу. Месторождения, которые, как сообщается, представляют собой линзы и жилы в силурийских кварцитах, принадлежат португальской компании.

Россия содержит самые важные марганцевые месторождения в Европе, если не в мире. Основной горнодобывающий район находится вблизи Чиатуры, в Кутаисской губернии, на южной стороне Кавказских гор, в южной России. Слои оолитовых зерен оксидов марганца переслаиваются с горизонтальными песчаниками и сланцами нижнеэоценового возраста. В пределах зоны мощностью от 4,5 до 7,5 футов, в среднем около 6,5 футов, семь отдельных слоев очень чистого оксида марганца составляют около 40 дюймов в толщину, а остальное — низкосортный материал и песок. По оценкам, площадь от 120 до 143 квадратных километров первоначально была подстилаема пластом оксидов, но около половины было удалено эрозией. Оценки запасов варьируются от 23 000 000 тонн до нескольких сотен миллионов тонн.

Рудники эксплуатируются примитивным, неэффективным способом, и извлекается едва ли две трети руды. Число фактических производителей варьировалось от 183 в 1902 году до 376 в 1906 году, но сократилось до 96 во время политических волнений в 1908 году. Руда сортируется вручную, а низкосортный материал промывается на примитивных установках. От 20 до 25 процентов экспортируемого материала было сконцентрировано путем промывки.

В 1902 году существовало 5 000 концессий, из которых 3 750 принадлежали 14 лицам, каждое из которых владело от 25 до 500 концессий; остальные принадлежали 300 крестьянам и мелким торговцам. К 1912 году была сформирована ассоциация производителей, чтобы позволить владельцам коллективно взаимодействовать с экспортерами. Крупные инвестиции были также сделаны немецкими капиталистами как в рудники, так и в неразработанные территории. Gelsenkirchen Gesellschaft, немецкая фирма, была сформирована частично с целью добычи, но главным образом для покупки и экспорта руды в Германию. В 1912 году эта фирма, хотя и добывала лишь немного руды, экспортировала почти треть от общего объема. Немецкие группы также создали необходимые финансовые агентства для содействия экспорту руды, а также для предоставления кредитов операторам рудников. В 1913 году из 16 экспортных фирм только 3 были российскими.

Продукция рудников Чиатурского района перевозится до Чиатуры (от 1,3 до 3,3 миль), грузится на узкоколейные вагоны для транспортировки до Шорапани (25 миль), а затем перегружается на вагоны для отправки в Поти или Батум (107 миль), порты экспорта. Крупные запасы, варьирующиеся от 1 030 000 тонн в 1912 году до 1 525 000 тонн в 1908 году, хранятся в Чиатуре, Поти и Батуме. С 1910 по 1912 год распределение экспорта выглядело следующим образом: Голландия (для Германии) — от 30 до 43 процентов; Англия — от 22 до 23 процентов; Бельгия (в основном для Германии) — от 15 до 21 процента; Германия (напрямую) — 5 процентов; Франция — от 4 до 6 процентов; Соединенные Штаты — от 4 до 10 процентов; Австрия — от 4 до 10 процентов. Примерно в 1913 году российским правительством была введена экспортная пошлина в размере 40 центов за длинную тонну.

По оценкам, с 1848 по 1914 год включительно это месторождение дало около 11 000 000 тонн промытой руды товарного качества. Максимальная добыча в 1 300 000 тонн была достигнута в 1913 году.

Другим важным марганцевым горнодобывающим регионом является Никопольский район в Екатеринославской губернии, к северу от Черного моря. В этом районе пласт оксидов марганца залегает между глинами и песчаниками олигоценового возраста. Этот пласт имеет мощность от 1 до 5 футов, в среднем около 3 футов. По оценкам, он простирается на площади 20 квадратных километров (7,5 квадратных миль) и содержит 7 400 000 тонн марганцевой руды. Руда добывается и промывается примитивным способом для очистки от прилипшей глины.

Месторождения в этом районе, вероятно, в значительной степени принадлежат русским, хотя французский капитал заинтересован в одной компании, а немецкий — в другой. В период с 1901 по 1910 год от 80 до 90 процентов продукции потреблялось в южной России, а остальная часть экспортировалась. С 1886 года, когда месторождения начали эксплуатироваться, добыча довольно устойчиво росла до максимума в 271 000 тонн в 1907 году, а затем снизилась до 173 000 тонн в 1910 году. Общая добыча в районе составляет около 1 800 000 тонн.

Марганцевые месторождения также известны в Подольской и Терской областях, а также в Тифлисской, Эриванской, Елизаветпольской и Пермской губерниях.

Основные марганцевые месторождения Испании находятся на южном склоне Сьерра-Морены, в провинции Уэльва. Вертикальные линзовидные тела карбоната и силиката марганца с небольшим количеством пирита, граната и слюды переслаиваются со сланцами палеозойского возраста. Известно около ста тел, многие из которых имеют длину 500 футов и ширину 100 футов, тогда как самое крупное имеет длину 3 300 футов и ширину 330 футов. Марганцевые минералы выветрились до оксидов на среднюю глубину 65 футов и максимальную глубину 250 футов. С 1881 по 1905 год, когда оксидные руды были почти исчерпаны, было отгружено около 700 000 тонн. С 1906 по 1910 год было добыто около 125 000 тонн смешанного карбоната и силиката.

Марганец также найден в районе Ковадонга, провинция Овьедо, где крупные валуны оксида марганца встречаются в глине, образовавшейся в результате выветривания подстилающего известняка. Эти месторождения дали 3 800 тонн в 1915 году. Другие продуктивные месторождения встречаются в провинциях Севилья и Теруэль. Месторождения также известны в провинциях Сьюдад-Реаль, Мурсия и Альмерия.

В Швеции марганцевые руды есть к северу от Филипстада в Вермланде, где таблитчатые тела оксидов марганца переслаиваются с доломитом и магнетитом. Эти месторождения дали 7 607 тонн из общего объема 7 733 тонны в 1915 году, что стало максимальной зафиксированной добычей в Швеции.

Азия.

— В Индии, на восточном побережье в округах Визагапатам и Ганджам, Мадрас, находится уникальная группа пород, известная как серия кодуритов, содержащая марганцевый гранат, марганцевый пироксен, калиевый полевой шпат, апатит и кварц. Эти породы, предположительно магматического происхождения, подверглись глубокому выветриванию, и марганец сконцентрировался в виде оксидов в приповерхностной зоне. Марганцевые рудные тела были исследованы только до глубины 100 футов, но ожидается, что они будут простираться до 500 футов. Крупнейшее рудное тело, исследованное на руднике Гарбхам, имеет длину 1 600 футов и ширину 100 футов, и с 1896 по 1913 год дало 736 192 тонны руды. Месторождение Кодур дало 370 382 тонны руды с 1892 по 1913 год. Добыча началась в 1892 году, достигла максимума в 111 501 тонну в 1906 году и медленно снизилась до 44 127 тонн в 1913 году.

Марганец также встречается в округах Балагхат, Бхандара, Чиндвара и Нагпур в Центральных провинциях; округах Нарукот и Панч-Махал, Бомбей; округе Джабуа, Центральная Индия; и округе Гангпур в Бихаре и Ориссе. Эти округа образуют пояс, который простирается от Бароды на западном побережье через северную Индию почти до Калькутты на востоке, на расстояние 700 миль. В этих округах пласты оксидов марганца с марганцевым гранатом и родонитом образуют тип породы, известный как гондит, который переслаивается с кварцитом и слюдяным сланцем. Эти породы считаются отложениями группы Дхарвар (архей). Оксиды марганца могли отложиться как осадочные породы или представлять собой результат выветривания силикатов. Рудные тела представляют собой линзы и пласты. Крупнейшее отдельное месторождение, Балагхат, имеет форму полого корыта, имеет длину 1 3/4 мили и мощность от 45 до 50 футов, и с 1901 по 1913 год дало 725 248 тонн руды. В 1913 году тринадцать отдельных месторождений дали более 100 000 тонн каждое, в диапазоне от 101 721 до 725 248 тонн.

С 1901 года, когда месторождения этого типа начали эксплуатироваться, темпы добычи неуклонно росли до максимума в 697 035 тонн в 1913 году. В течение 1907 года пятьдесят два отдельных месторождения дали 598 437 тонн.

Там, где породы дхарварского возраста (архей), такие как слюдяные сланцы, которые, по-видимому, не содержат марганецсодержащую серию гондитов, глубоко выветрились, оксиды марганца и марганцовистого железа образуют нерегулярные, но местами обширные месторождения на гребнях холмов. Эти месторождения подстилаются бесплодными глинами, которые представляют собой остаток подстилающих пород. Крупнейшее месторождение дало 160 000 тонн руды за три года, с 1906 по 1908 год, но, вероятно, почти исчерпано. Основные месторождения этого класса находятся в районе Сандур-Хиллз, Мадрас; районе Шимога, Майсур; и районе Белгаум, Бомбей; которые лежат в пределах области диаметром менее 100 миль в юго-западной Индии. С 1905 года, когда месторождения этой группы начали исследоваться, добыча увеличилась до максимума в 11 353 тонны в 1909 году, затем снизилась до 62 770 тонн в 1913 году. Общий выход этой группы к концу 1913 года составил всего 765 401 тонну.

Что касается коммерческого контроля над марганцевыми месторождениями, то недавно принятый закон запрещает иностранцам владеть более чем миноритарной долей в месторождениях полезных ископаемых в Индии. До этого, в течение 1907 года, последнего года, за который имеются полные данные и в котором было добыто 899 055 тонн, весь объем был получен с рудников, принадлежащих проживающим в стране англичанам или местным жителям, за исключением 21 500 тонн, добытых компанией Carnegie Steel Co. из Питтсбурга, США.

Годовая добыча марганцевой руды в Индии неуклонно росла с 1892 года, когда были осуществлены первые поставки, до 1907 года, когда было отгружено 899 055 тонн; с тех пор она варьировалась от 450 000 до 815 000 тонн. Общая добыча по 1916 год включительно составила 8 748 000 тонн.

Индийские руды транспортируются в порты отгрузки по железной дороге на расстояния от 56 миль для округа Визагапатам до 783 миль для округа Чиндвара, в результате чего транспортные расходы высоки. Порты экспорта в порядке объема обработанного тоннажа: Бомбей, Мормугао, Калькутта и Визагапатам. Направления экспорта в 1913 году были следующими: Соединенное Королевство — 36 процентов; Бельгия (в основном в Германию) — 26 процентов; Соединенные Штаты — 15 процентов; Франция — 14 процентов; Германия — 2 процента; другие — 7 процентов.

В Японской империи, на островах Муцу, Этиго, Уго и Нато, имеются нерегулярные линзовидные тела довольно чистых оксидов марганца, которые залегают более или менее параллельно напластованию метаморфизованных палеозойских отложений. Ниже уровня грунтовых вод оксиды переходят в родонит и, вероятно, являются производными этого минерала. Рудные тела невелики, но известно их много, и они являются источником небольшой, но регулярной добычи. На островах Муцу, Ного, Хоккайдо и Уго многие нерегулярные, но местами крупные месторождения оксидов марганца ассоциированы с сильно измененными вулканическими туфами и лавовыми потоками третичного возраста. Большинство месторождений в Японии, по-видимому, принадлежат местным жителям на правах мелкого владения. Максимальная добыча в 18 076 тонн зафиксирована в 1913 году, но с 1900 года диапазон обычно составлял от 5 000 до 15 000 тонн.

На Филиппинских островах марганец встречается на островах Илокос-Норте, Масбате, Булакан, Пангасинан и Тарлак, главным образом в виде прожилков и валунов оксидов в выветрелых магматических породах. На Илокос-Норте максимальная добыча в 3 000 тонн была достигнута в 1916 году.

Африка.

— На Золотом Берегу Западной Африки (британская колония), вблизи Дагвина, находится несколько месторождений марганца, крупнейшее из которых имеет длину 400 футов и ширину 70 футов. Концессия принадлежит британской геологоразведочной компании. Месторождение было открыто в 1914 году; и с начала разведки в 1916 году по 7 ноября 1917 года в Англию было отгружено 28 465 тонн.

В Бельгийском Конго марганцевая руда есть в долине реки Верхняя Фунгве и в южной Катанге. Месторождения слишком удалены от океана, чтобы оправдать разведку, но, по сообщениям, они крупные. В Южно-Африканском Союзе (британский) несколько марганцевых месторождений обнаружено вдоль морского побережья, в пределах 30 миль к востоку и западу от Кейптауна. Из семи известных месторождений крупнейшее, по оценкам, содержит 15 000 тонн. В Египте, на Синайском полуострове, имеются крупные месторождения марганцовистого железа, а также небольшие марганцевые месторождения, но ни одно из них не эксплуатировалось. В Тунисе имеются месторождения, которые, как сообщается, содержат от 4 000 000 до 5 000 000 тонн марганцовистой железной руды, а также несколько марганцевых месторождений, которые дали 5 800 метрических тонн марганцевой руды в 1917 году.

Хотя известные месторождения марганца в Африке немногочисленны и относительно неважны, континент представляет собой необычайную перспективу для открытия месторождений, которые внесут значительный вклад в мировые поставки. Поскольку влажный тропический климат больших территорий способствует необычайному разрушению пород и поверхностной концентрации оксидов марганца, разведка, вероятно, покажет наличие многих месторождений, и там, где геологические условия коренных пород благоприятны, могут быть найдены крупные тела.

Австралазия.

— В Австралии имеются месторождения марганцевой руды в Новом Южном Уэльсе, Квинсленде, Южной Австралии и Виктории.

В Новой Зеландии месторождения марганцевой руды встречаются в районе Темс, Окленд.

Месторождения марганцевой руды известны на Борнео, в заливе Маруда.

Рис. 5. — Годовой объем добычи марганцевой руды в основных странах-производителях.

Рис. 6. — Процент марганцевой руды, добываемой основными странами-производителями.

Сообщается, что на Яве недавно были обнаружены крупные месторождения высокосортной руды.

Некоторые статистические данные о добыче марганца представлены графически на рисунках 5 и 6.

РАЗВИТИЕ И ИЗМЕНЕНИЯ В ГЕОГРАФИЧЕСКОМ РАСПРЕДЕЛЕНИИ В БЛИЖАЙШЕМ БУДУЩЕМ

Известные ресурсы марганца в России, Индии и Бразилии настолько велики и легко доступны для эксплуатации и сбыта, что мало шансов на то, что они будут вытеснены в качестве основных источников мировых поставок в течение многих лет. С начала войны в 1914 году было открыто и доведено до стадии производства несколько важных новых районов, особенно Золотой Берег Западной Африки, западная Коста-Рика и Ява. Хотя месторождения на Яве, по сообщениям, велики и могут стать важным фактором в мировой торговле, все, что известно о других месторождениях, не дает больших надежд на то, что они смогут конкурировать с уже существующими источниками.

По-видимому, существует неплохой шанс, что экваториальный пояс, а также некоторые другие части Земли могут дать дополнительные важные марганцевые месторождения.

Распределение марганцевых месторождений мира показано на Таблице III.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Таблица добычи за 1913 год на странице 105 показывает долю каждой страны в общем объеме и известную степень коммерческого контроля.

В отличие от месторождений некоторых других важных минералов, большинство марганцевых месторождений по всему миру принадлежат местным жителям или резидентам соответствующих стран, в которых они находятся.

Немецкие компании приобрели участки в Чиатурском и Никопольском районах, Россия, и районе Келуз (Лафайет), Бразилия. По-видимому, хотя одна из этих компаний добывает немного руды, основной целью была стабилизация неорганизованной отрасли путем финансовой помощи.

В Индии трудно провести различие между компаниями, состоящими из проживающих в стране англичан и местных индийцев, которые были созданы для эксплуатации рудников с целью получения прибыли, и компаниями, состоящими из англичан-нерезидентов, которые стремятся обеспечить поставки руды для английского или другого потребления. По-видимому, в Бразилии или России нет английского капитала.

Одна французская компания владела двумя действующими рудниками в Индии в 1907 году, но нет никаких записей об операциях в 1913 году. Французский капитал заинтересован в нескольких компаниях, работающих в Никопольском районе, Россия. Бельгийская компания эксплуатирует один рудник в районе Келуз, Бразилия.

Таблица III. — Географическое распределение основных марганцевых месторождений мира. Д. Ф. Хьюитт.

Таблица 24. — Добыча и коммерческий контроль марганца

Country | Long tons | Manganese content (per cent.) | Per cent. of total production | Commercial control (estimated per cent.)
North America |  |  |  |
United States | 4,048 | 40+ |  0.16 |  | United States, 100
South America |  |  |  |
Brazil | 120,368 | 38-48 |  5.10 |  - |  | Brazil, 80
Belgium, 5
Germany, 15
Europe |  |  |  |
Austria-Hungary | 34,986 | ? |  1.5  |  | Austria-Hungary, 100
Bosnia-Herzegovina | 5,709 | ? |  0.2  |  | ?
France | 7,610 | 30+ |  0.3  |  | France, 100
Germany | 748 | 30+ |  0.03 |  | Germany, 100
Italy | 1,596 | 18-45 |  0.07 |  | Italy, 100
Russia | 1,289,370 | 41-48 | 55.4  | - |  | Russia, 65
Germany, 30
France, 5
Spain | 21,254 | 29+ |  0.9  |  | ?
Sweden | 3,938 | ? |  0.15 |  | ?
United Kingdom | 5,393 | 30+ |  0.21 |  | England, 100
Asia |  |  |  |
India | 815,047 | 42-54 | 35.0  | - |  | English and native, 90
United States, 10
Japan | 18,516 | ? |  0.8  |  | Japan, 100
Oceania |  |  |  |
Australia | 27 |  |  |  | ?
Total | 2,328,110 |  |  |

Компания Carnegie Steel Co. из Питтсбурга, штат Пенсильвания, США, владеет и разрабатывает несколько месторождений в Индии. Хотя американцы владеют месторождениями в районе Назарет, Бразилия, в Панаме и Коста-Рике, а также некоторыми на Кубе, нет никаких записей об американском владении какими-либо из наиболее важных месторождений Бразилии или России.

С 1902 по 1914 год около половины ферромарганца, используемого в Соединенных Штатах, производилось в этой стране из иностранной руды, а половина импортировалась из Англии, где он производился из импортной руды. Эта тенденция обусловлена ограничениями доменной плавки сплава и разницей в стоимости рабочей силы в Соединенных Штатах и Англии, но не представляет собой определенного контроля, поскольку ферромарганец может быть произведен в любой современной доменной печи, используемой для производства чугуна. Однако для плавки с максимальной эффективностью при производстве ферромарганца доменная печь должна работать непрерывно в течение длительных периодов и, следовательно, производить от 20 000 до 35 000 тонн сплава ежегодно. Хотя можно без перерыва перейти от производства ферромарганца к зеркальному чугуну, а затем к чугуну, это изменение вызывает потери. Поэтому мелким сталелитейным заводам в Соединенных Штатах выгоднее покупать импортный ферромарганец, чем производить то, что им нужно.

ПОЛОЖЕНИЕ ВАЖНЫХ НАЦИЙ В ОТНОШЕНИИ ПОСТАВОК МАРГАНЦА

Соединенные Штаты.

— Хотя с 1885 по 1890 год месторождения в Соединенных Штатах обеспечивали половину или более необходимой высокосортной марганцевой руды, с 1890 по 1916 год внутренняя добыча довольно устойчиво снижалась до пренебрежимо малого минимума, в то время как импорт иностранной руды и ферромарганца неуклонно рос в соответствии с темпами общего производства стали. С другой стороны, в период, закончившийся около 1908 года, когда темпы производства стали бессемеровским способом (при котором широко используется зеркальный чугун) превышали темпы мартеновского способа, годовой внутренний вклад зеркального чугуна, производимого в основном из отечественных руд, значительно превышал импорт. Таким образом, еще до эксплуатации крупных месторождений низкосортных руд Миннесоты, которые были источником большей части добычи с 1916 года, Соединенные Штаты продемонстрировали независимость от иностранных поставок низкосортной руды и сплавов.

Опыт и информация, полученные во время войны, главным образом в течение 1918 года, убедительно показывают, во-первых, в отношении металлургии, что 20-30-процентный зеркальный чугун, а также 60-70-процентный ферромарганец вместо 80-процентного могут быть использованы для производства удовлетворительных сортов мартеновской стали без заметного ущерба для темпов производства или качества продукта; и во-вторых, в отношении добычи руды, что известные отечественные месторождения могут поставлять в течение как минимум пяти, а вероятно, десяти или более лет гораздо больше низкосортной руды, чем необходимо для производства зеркального чугуна, и в течение как минимум пяти, а возможно, десяти лет около одной трети высокосортной руды, необходимой для производства сплава с содержанием марганца от 60 до 80 процентов. Читателю следует, однако, отметить, что способность рудников удовлетворять спрос в значительной мере определяется ценами, предлагаемыми за продукт, которые в течение 1918 года были примерно в пять раз выше тех, что преобладали до войны. Вне всякого сомнения, при довоенных ценах Соединенные Штаты не могут обеспечить более нескольких процентов высокосортной руды, необходимой для производства ферромарганца.

Граждане Соединенных Штатов не проявляли большого интереса к приобретению иностранных месторождений марганцевой руды. Совместно с кубинцами они контролировали рудники, обеспечивавшие значительную часть добычи на Кубе, а примерно в 1907 году одна компания, Carnegie Steel Co., приобрела несколько месторождений в Индии. Однако эта компания, по-видимому, закупает руду в дополнение к продукции своих собственных рудников. Только в 1917 году американцы вышли на бразильские месторождения; тогда крупнейшие залежи относительно неважного района Баия были приобретены группой из Филадельфии.

Англия.

— До войны Англия получала около 50 процентов марганцевой руды из Индии, 40 процентов из России, 3 процента из Бразилии и небольшие количества из Испании и Португальской Индии. Некоторое количество низкосортной руды также поступало из Испании, Алжира и Греции. Внутренняя добыча едва составляла 1 процент от объема импорта. Однако экспорт ферромарганца, главным образом в Соединенные Штаты, был эквивалентен 35–45 процентам от общего объема импорта руды. Двумя последствиями войны стали исключение России как источника руды, при этом дефицит восполнялся за счет Индии, и значительное сокращение экспорта ферромарганца. В отличие от Соединенных Штатов и Германии, в Великобритании, по-видимому, нет месторождений низкосортных руд, способных восполнить потребности в высокосортной руде.

Англия полностью контролирует 90 процентов индийской добычи, вероятно, посредством владения со стороны проживающих там англичан и коренных индийцев. С другой стороны, Англия, по-видимому, не имеет никакого прямого или косвенного контроля над добычей в Бразилии, России или другими важными источниками поставок.

Франция.

— Из необходимой марганцевой руды Франция импортирует от 35 до 45 процентов из Индии, от 40 до 55 процентов из России, около 10 процентов из Испании и несколько процентов из Бразилии, а собственная добыча составляет около 2 процентов. Однако отечественное сырье содержит 30 процентов марганца или меньше. Кроме того, Франция время от времени как импортирует, так и экспортирует небольшое количество ферромарганца.

Насколько позволяют судить имеющиеся данные, французы практически не делали иностранных инвестиций в марганцевые месторождения, за исключением Никопольского района в России. Компания с французским названием добыла около 1300 тонн в Индии в 1907 году из общего объема в 899 055 длинных тонн.

Германия.

— Положение Германии в отношении марганца очень похоже на положение Соединенных Штатов. В течение четырех лет до 1914 года Германия импортировала от 48 до 68 процентов от общего объема поступлений из России, от 25 до 35 процентов из Индии, от 3 до 7 процентов из Бразилии, а также небольшие количества из Испании, Греции и Швеции. Внутренняя добыча руды с содержанием марганца более 30 процентов незначительна. Германия, вероятно, экспортирует небольшие количества ферромарганца в Швецию и другие европейские страны, а время от времени экспортировала сплавы в Соединенные Штаты.

Однако, подобно Соединенным Штатам, Германия обладает обширными месторождениями железистой марганцевой руды с содержанием марганца от 12 до 30 процентов; и с 1908 по 1913 год она добывала от 260 000 до 330 000 метрических тонн такого материала, а также от 2 300 000 до 3 000 000 тонн с содержанием марганца от 5 до 7 процентов. Почти не вызывает сомнений, что, хотя Германия благодаря накопленным запасам марганцевой руды и захватам в Бельгии обладала в 1914 году как минимум двухлетним запасом, она смогла поддерживать довольно постоянный уровень производства стали в течение четырех лет за счет адаптации процессов для экономии высокосортной руды и использования низкосортной.

Немцы, по-видимому, приобретали марганцевые месторождения только в России и Бразилии, и они давали лишь малую часть ежегодного импорта. Однако в Чиатурском районе России, где большинство месторождений принадлежит местным жителям, около 1910 года была основана немецкая компания Gelsenkirchen Gesellschaft, которая, как сообщается, является дочерним предприятием компании Krupp, для покупки собственности, а также для торговли с производителями и предложения им финансовой помощи. Сообщается, что эта компания в одиночку экспортировала около трети продукции района. По имеющимся сведениям, немцы владеют частью одной из нескольких компаний, работающих в Никопольском районе России.

РЕЗЮМЕ

Обзор промышленности марганцевой руды, включая особенности месторождений, их географическое распределение и структуру собственности, позволяет сделать несколько определенных выводов:

1. Поверхностные выходы большинства марганцевых месторождений дают достоверную информацию о размерах и качестве залежей, а наиболее ценная руда встречается в приповерхностной зоне глубиной едва ли более 100 футов.

2. За исключением России и Испании, наиболее продуктивные рудники являются открытыми карьерами, и добыча осуществляется быстро и легко с минимальными затратами. Обширные подготовительные работы перед началом добычи требуются редко.

3. Страны, обладающие самыми крупными и богатыми месторождениями, имеют обильные и дешевые трудовые ресурсы.

4. Производственная мощность известных месторождений настолько превышает мировой спрос на руду для производства стали, что если какой-либо отдельный источник временно исключается, спрос может быть полностью удовлетворен за счет оставшихся источников по ценам, которые лишь незначительно выше ранее преобладавших.

5. Стоимость материала в местах добычи относительно низка среди сырьевых минералов и составляет от одной трети до одной восьмой от продажной цены в пунктах потребления. Очевидно, что транспортные расходы составляют значительную часть конечной цены.

6. Разработка большинства месторождений приносит так мало прибыли и поэтому является настолько рискованной, что лишь немногие иностранцы владеют месторождениями в основных странах-производителях.

7. Единственный случай коммерческого контроля — контроль немцами Чиатурского района в России, которые предлагают естественный рынок сбыта, — по-видимому, был установлен для противодействия местным политическим беспорядкам, а не для устранения конкурирующих потребителей.

8. Ни одна страна, вносящая значительный вклад в мировое производство стали, за исключением России, не обладает внутренними месторождениями марганцевой руды, достаточными для удовлетворения своих потребностей, и все они должны импортировать руду из довольно отдаленных источников. Однако Соединенные Штаты и Германия обладают внутренними месторождениями железистой марганцевой руды, которые в условиях острого дефицита, вероятно, позволили бы им стать независимыми от иностранных источников.

ГЛАВА V ХРОМ Автор: Э. К. Хардер

ПРИМЕНЕНИЕ ХРОМА

Хромит является основной рудой, из которой получают металлический хром и хромовые продукты. Теоретический состав хромита представлен формулой FeO Cr2O3, что соответствует 32 процентам закиси железа и 68 процентам оксида хрома. Однако во многих рудах закись железа частично замещается магнезией (до 30 процентов), а оксид хрома — глиноземом и оксидом железа (до 20 процентов). Таким образом, состав хромита значительно варьируется. Процентное содержание оксида хрома может составлять всего 10 процентов; содержание закиси железа может варьироваться от 10 до 50 процентов. Другими распространенными минералами хрома являются пикотит (хромистая шпинель), уваровит (хромистый гранат), хромдиопсид и крокоит (хромат свинца).

Хромовая руда потребляется главным образом в производстве специальных сталей и при дублении кожи. Специальные стали включают хромистую сталь, хромоникелевую сталь, хромовольфрамовую сталь и хромованадиевую сталь. Металлический хром добавляется в такую сталь в виде феррохрома — сплава хрома и железа, содержащего от 60 до 70 процентов металлического хрома. Хромистая сталь прочна и трудно поддается излому. Она быстро закаливается, имеет мелкозернистую структуру и волокнистый излом; она не ломается легко при ударе и из-за своей твердости с трудом или вовсе не поддается резке обычными станками. Металлический хром присутствует в ней в количестве от 1 до 5 процентов. Специальные стали, содержащие хром, используются для изготовления орудий, броневых плит, бронебойных снарядов, деталей автомобилей, станков, прутьев для тюрем, сейфов, взломостойких сейфов, обуви, столовых приборов, щек дробилок, штамповочных молотов, пружин и других изделий, где необходимы твердость и прочность. Во время войны, когда возникла угроза значительного дефицита хромита, в хромистых сталях использовалось меньше хрома, а вместо него применялись некоторые другие упрочняющие материалы. Однако результаты, как говорят, были неудовлетворительными.

Феррохром, используемый в производстве хромистых сталей, производится в электрической печи путем плавки смеси хромита, угля или кокса, извести и плавикового шпата или кремнезема в надлежащих пропорциях.

Много хромовой руды используется в сталелитейной промышленности в качестве огнеупорных материалов для футеровки мартеновских печей. Часть используемой таким образом руды сначала перерабатывается в хромовый кирпич, а часть используется в сыром виде. Хромовый кирпич применяется в мартеновских печах в качестве футеровки вдоль шлаковой линии между магнезитовым подом печи и стенками и сводом из динасового кирпича. Хромовый кирпич также используется для покрытия портов газовых печей. Он желателен для этих целей благодаря своей нейтральной реакции, которая снижает износ из-за коррозии. Кусковой или дробленый хромит используется для ремонта подов мартеновских печей, особенно носка или вершины пода, при этом руда либо забивается на место в виде кусков, либо измельчается, смешивается с небольшим количеством воды или дегтя и глины, а затем утрамбовывается. Использование кускового хрома при ремонте таких печей желательно из-за быстроты, с которой можно отремонтировать печи, и из-за большей износостойкости хромита. Количество хромита, используемого для этой цели, варьируется от 2 до 10 фунтов на тонну произведенной стали. Магнезит использовался для замены хромита при ремонте печей, но оказался более дорогим и менее износостойким.

Хромовый кирпич в небольших объемах используется в электрических печах для производства стали, в поясе вдоль шлаковой линии и в зоне вокруг выпускных отверстий. Он также используется в печах для производства стали дуплекс-процессом.

Хромовый кирпич, помимо использования в сталеплавильных печах, применяется для футеровки печей для выплавки меди, никеля и других металлов. В этих печах он используется в подах и вокруг выпускных отверстий. Магнезитовый кирпич, а также бокситовый кирпич использовались для замены хромитового кирпича в этих целях.

Химикаты хрома, используемые для дубления, — это главным образом бихроматы натрия или калия. Около половины бихроматов, производимых в Соединенных Штатах, обычно используется для дубления, остальная часть — для красок, пигментов, сухих красителей и красителей в лакокрасочной, полиграфической, гравировальной и текстильной промышленности. Хромовый желтый, хромовый оранжевый и хромовый черный используются в ситцепечатании и крашении. Оксид хрома, или хромовая зелень, является несмываемым пигментом, используемым при печати банкнот. Различные другие хромовые цвета используются для красок и пигментов, а также в керамическом искусстве. Второстепенных применений химикатов хрома множество.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Хромит во всем мире ассоциируется с основными изверженными породами, такими как перидотит или пироксенит, или с продуктами изменения этих пород, такими как серпентин, тальковый сланец и родственные породы. Месторождения хромита обычно имеют форму линз, гнезд или неправильных масс, которые могут встречаться по отдельности или группами. Помимо нахождения в виде крупных тел, хромит встречается как второстепенный компонент этих пород, будучи широко рассеянным в них в виде мелких вкраплений и частиц. Считается, что хромит, образующий промышленные месторождения, отделился от расплавленной массы основной изверженной породы путем сегрегации и образовал отдельные тела внутри массы породы во время остывания. Большинство месторождений хромита находятся вдоль границ интрузивных массивов недалеко от контакта с более древними породами, в которые они внедрены. Вероятно, это связано с образованием периферийных трещин во время остывания изверженной массы, при этом хромит вытеснялся в эти отверстия. Действие конвекционных токов в расплавленной магме также могло привести к локализации тел хромита вблизи границ массы. Однако тела хромита довольно обильны и в других частях изверженных массивов, часто встречаясь на больших расстояниях от граничащих пород.

В результате выветривания хромитсодержащей изверженной породы тела хромита высвобождаются и встречаются в виде рыхлых масс в образующихся остаточных глинах. Такие тела в глине имеют промышленное значение во многих местах. Разрушение хромитсодержащих пород приводит к высвобождению рассеянных вкраплений и частиц хромита, которые могут переноситься и впоследствии откладываться вдоль потоков, вытекающих из хромитсодержащих районов. Таким образом образуются скопления хромитовых песков. Помимо хромита, эти пески обычно содержат значительные количества других тяжелых минералов, таких как магнетит, ильменит, гранат и рутил, и хромит в них, как правило, не является доступным для промышленного использования.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Мировые поставки хромита были получены главным образом из следующих источников, перечисленных примерно в порядке их важности:

Новая Каледония; Южная Родезия; западная и южная Малая Азия; Уральские горы, Россия; восточная Греция, прилегающие острова, Македония и Сербия; Белуджистан и Майсур, Индия; Квебек, Канада; штаты Атлантического и Тихоокеанского побережья, Соединенные Штаты; штат Баия, Бразилия; Орьенте, Куба; Япония; Босния и Герцеговина; Австро-Венгрия; и Гватемала.

Географическое распределение наиболее важных месторождений хромита показано на Пластине IV.

Другие страны, в которых известны месторождения хромита, но в которых добывалось мало руды или она не добывалась вовсе: Шетландские острова, Шотландия; Норвегия; Швеция; Силезия; Португалия; Новый Южный Уэльс, Австралия; Новая Зеландия; Трансвааль; Тоголенд; и Ньюфаундленд.

В Таблице 25 показана добыча хромита в основных странах-производителях с 1905 по 1917 год.

Австралазия.

— Значительные количества хромита встречаются на острове Новая Каледония в южной части Тихого океана, а в меньших количествах — в Австралии, Новой Зеландии и на Тасмании.

Пластина IV. — Географическое распределение месторождений хромита в мире. Автор: Э. К. Хардер.

Таблица 25. — Мировая добыча хромита в 1905–1917 гг. в длинных тоннах [53]

| 1905[54] | 1906 | 1907 | 1908 | 1909 | 1910 | 1911 | 1912 | 1913 | 1914 | 1915 | 1916 | 1917
United States | 22 |  | 107 |  | 290 |  | 359 |  | 598 |  | 205 |  | 120 |  | 201 |  | 255 |  | 591 |  | 3,281 |  | 47,035 |  | 43,725 |
Canada[55] | 7,657 |  | 8,068 |  | 6,425 |  | 6,451 |  | 2,205 |  | 267 |  | 140 |  | ... |  | ... |  | 121 |  | 11,008 |  | 24,545 |  | 32,457 | [56]
Cuba[57] | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | 34 |  | 17 | [58]
Guatemala[57] | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | 179 | [58]
Brazil[57] |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |
Great Britain (Shetland Islands) | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | 100 |  |  |  |  |  |  |
Norway | ... |  | ... |  | 105 | [56] | ... |  | ... |  | ... |  | ... |  | 113 | [56] | ... |  | 80 | [56] | 344 | [56] |  |  |  |
Sweden | ... |  | ... |  | ... |  | ... |  | ... |  | 31 |  |  |  |  |  |  |  |  |  |  |  |  |  |  |
Austria-Hungary (Bosnia and Herzegovina) | 183 |  | 315 |  | 305 |  | 492 |  | 327 |  | 315 |  | 246 |  | 197 |  | 300 | [56] | 474 | [56] |  | [59] |  | [59] |  |
Greece[60] | 8,759 |  | 11,348 |  | 11,545 |  | 4,281 |  | 9,448 |  | 9,311 |  | 4,542 |  | 6,209 |  | 6,242 | [56] | 6,947 | [56] | 10,255 | [56] | 9,724 | [56] |  | [59]
Serbia[61] | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  | ... |  |  | [59] |  | [59] |  | [59]
Russia | 26,620 |  | 16,708 |  | 25,940 |  | 10,777 |  | 21,857 |  | 14,157 |  | 1,218 | [56] | 20,934 |  | 21,401 |  |  | [59] |  | [59] |  | [59] |  | [59]
Turkey[62] (mainly Asia Minor) | ... |  | 23,404 |  | 21,111 |  | 28,394 |  | 11,364 |  |  | [59] | 11,993 |  | 16,823 | [63] |  | [59] |  | [59] |  | [59] |  | [59] |  | [59]
Rhodesia | ... |  | 3,256 |  | 8,017 |  | 11,927 |  | 22,875 |  | 39,287 |  | 46,753 |  | 61,840 |  | 62,365 |  | 48,235 |  | 60,617 | [56] | 79,350 | [56] |  | [59]
India | 2,708 |  | 4,375 |  | 7,274 |  | 4,745 |  | 9,250 |  | 1,737 |  | 3,804 |  | 2,890 |  | 5,580 | [56] | 5,887 | [56] | 3,768 | [56] | 20,160 | [56] |  | [59]
Japan | ... |  | ... |  | ... |  | ... |  | ... |  | 2,091 |  | 1,500 |  | 1,591 |  |  | [59] | 2,075 | [56] | 2,932 | [56] | 8,149 | [56] |  | [59]
New South Wales | 52 |  | 15 |  | 30 |  | ... |  | ... |  | ... |  | 148 |  | 23 |  |  |  |  |  |  |  |  |  |  |
New Caledonia | 75,717 |  | 82,910 |  | 56,461 | [56] | 24,970 | [56] | 39,368 |  | 39,368 |  | 34,447 |  | 41,325 |  | 62,352 |  | 41,336 | [56] | 65,941 | [56] | 74,115 | [64] | 41,230 | [56]

[53] Цифры, если не указано иное, были получены из «Минеральных ресурсов Соединенных Штатов, 1914» и последующих лет, Геологическая служба США (цифры первоначально получены главным образом из британской статистической публикации «Шахты и карьеры: Общий отчет со статистикой», ч. 4, Лондон).

[54] Figures for 1905 taken direct from Mines and Quarries, 1905 and 1906.

[55] Минеральное производство Канады, 1916, Министерство горнодобывающей промышленности Канады, Горнодобывающее отделение.

[56] Минеральная промышленность, 1917.

[57] Exports from Cuba, Guatemala, and Brazil in 1918 were respectively 8,820 tons, 1,193 tons, and 17,854 tons.

[58] Экспорт.

[59] Недоступно.

[60] Добыча в Салоникском районе включена в состав Турции до 1914 года.

[61] Нынешние сербские месторождения находились во владениях Турции до войны.

[62] Экспорт из Турции за финансовые годы, начинающиеся с марта.

[63] В отчете «Шахты и карьеры» добыча в Турции в 1912 году указана как 145 тонн.

[64] Ежегодник государственного деятеля, 1918, Лондон.

Серпентин в массах, внедряющихся в метаморфические породы и осадочные отложения, возраст которых варьируется от архейского до мезозойского, в изобилии встречается по всему острову Новая Каледония, и хромит неизменно ассоциируется с ним как второстепенный компонент. Местами встречаются крупные массы довольно чистого хромита, обычно в виде линзовидных тел в серпентине, но локально — в виде неправильных масс в остаточной глине, образовавшейся в результате разложения серпентина.

На Новой Каледонии известны месторождения хромита трех типов: скальный хром, состоящий из твердых рудных тел в серпентине; остаточный хромит в виде неправильных тел или разрозненных масс, часто дезинтегрированных, в красной остаточной глине, образовавшейся в результате выветривания серпентина; и хромитовый песок и гравий в поверхностных наносах и аллювиальных отложениях. Руды первых двух классов имеют промышленное значение на Новой Каледонии и присутствуют на большинстве рудников. Руды последнего типа не разрабатываются.

Из этих новокаледонских месторождений месторождение Маунт-д'Ор в южной части острова было первым, которое было обнаружено и разработано Гарнье в 1866 году. Позже эксплуатировались месторождения Нго-Бэй и другие, расположенные дальше на юг. Добыча и экспорт новокаледонского хромита начались в начале 80-х годов и продолжались в небольших объемах до 1902 года, при этом добыча велась главным образом на месторождениях Маунт-д'Ор и Нго-Бэй.

В 1902 году Л. Бернхайм сформировал компанию Société le Chrome, в которой французский капитал был в значительной степени заинтересован. Эта компания управляла рудниками в северной и южной частях острова. Она разработала месторождения Тьебаги недалеко от порта Пагумен, которые сейчас являются одними из самых важных в Новой Каледонии. Экспорт хромита вскоре увеличился, и постепенно новокаледонская руда заменила турецкую руду на рынке. В 1911 году была создана лондонская компания Chrome Co., Ltd., которая приобрела у Société le Chrome рудники Тьебаги и другие. В то же время она получила право от Rhodesia Chrome Mines Co., Limited на продажу родезийской руды, тем самым обеспечив практически монополию на мировую торговлю хромитом. Компания Chrome Co., Ltd. контролируется французскими и английскими интересами. Крупнейшими акционерами являются Chalas & Sons, Finsbury Pavement House, Лондон, E. C. Ранее были немецкие акционеры. Л. Бернхайм, по-видимому, не связан с Chrome Co., Ltd., но говорят, что он до сих пор владеет месторождениями хромита в Новой Каледонии. Помимо деятельности Chrome Co., Ltd., на острове существует ряд независимых предприятий. Они находятся в основном под контролем жителей острова.

Африка.

— Важные месторождения хромита в Южной Родезии находятся недалеко от города Селукве, который соединен железной дорогой с портом Бейра. Они встречаются разбросанными по территории, состоящей из сланца и серпентина. Было нанесено на карту сто двадцать тел хромита, но единственными, которые были разработаны, являются десять тесно сгруппированных крупных тел на хромитовом руднике к северо-западу от Селукве. Одно из самых крупных тел имеет ширину 180 футов и длину 240 футов. Руды высокосортные, в среднем содержат от 48 до 51 процента оксида хрома.

Недавно широкую огласку получило открытие того, что, как сообщается, является одними из крупнейших месторождений высокосортного хромита в мире в холмах Умвукве в районе Ломагунди, в 30 милях от Банкет-Джанкшен, Южная Родезия. Сообщается, что руда встречается на большой территории в виде тел в серпентине. Сообщается, что было обнаружено более двух миллионов тонн. Месторождения были открыты Альбертом Пиком из Умвукве-Ранч и принадлежат братьям Пик, которые, как говорят, предложили их Имперскому правительству на особых условиях.

Хромит в Родезии впервые начали добывать в 1905 году, руда поступала с участков возле Селукве, принадлежащих Bechuanaland Exploration Company, Ltd. Добыча неуклонно росла, сначала медленно, но более быстрыми темпами после 1910 года, когда рудники Селукве были переданы Rhodesia Chrome Mines, Ltd. В 1910 году сообщалось о подаче заявок на хромитовые участки в районе Хартли, а в 1911 году хромит был обнаружен в Виктории. Поставки из Селукве прекратились в августе 1914 года после объявления войны, но возобновились в декабре и увеличились в течение 1915 и 1916 годов. В 1917 году было сообщено об открытии крупных и ценных месторождений хромита в районе Ломагунди (уже упоминалось). До 1916 года вся добыча родезийского хромита поступала с рудников Селукве компании Rhodesia Chrome Mines, Ltd. Однако в 1917 году на рынок вышла другая компания, Rhodesia Metals Syndicate, Ltd., которая добывает значительные объемы руды.

Азия.

— До того как Турция потеряла большую часть своих европейских владений после Балканских войн, месторождения хромита в районах Косово, Ускюб и Монастир в Сербии и Салоникском районе Греции находились в ее границах. Теперь же у нее остались только месторождения Малой Азии.

Месторождения хромита широко разбросаны по многим частям Малой Азии, и говорят, что их сотни. Наиболее важные месторождения сгруппированы в три района: в регионах Брусса и Кутахья к югу от Мраморного моря, где находятся важные месторождения Дагхарди; недалеко от Макри, Денизлу и вокруг залива Адалия в юго-западной части полуострова, а также на соседнем острове Родос; и недалеко от Мерсины, Аданы, Алеппо и в других местах в регионе вокруг залива Александретта к северо-востоку от острова Кипр. Менее значительные месторождения отмечены в вилайетах Ангора и Кастамуни в северо-центральной части Малой Азии, а также недалеко от Бейрута и Дамаска в Сирии. Все рудные тела встречаются в более или менее сланцеватом и разложившемся серпентине в группах линзовидных или неправильных тел.

Хромитовые рудники Малой Азии производили значительные количества руды. Примерно с 1870 года, когда Турция начала вытеснять Соединенные Штаты в качестве основного мирового производителя хромита, и почти до 1900 года Малая Азия поставляла основную часть хромита для мирового потребления. Большая часть добытой руды поступала с рудников в регионе Брусса на южных и юго-западных склонах Мизийского Олимпа и с рудников региона Макри. Месторождения Брусса и Кутахья, как говорят, давали в среднем около 20 000 тонн ежегодно в течение многих лет, из которых рудник Дагхарди, как говорят, давал почти три четверти. Это месторождение состоит из высокосортной руды, содержащей в среднем от 51 до 55 процентов оксида хрома, и, по оценкам, содержит около 10 000 000 тонн руды. Вероятно, это некоторое преувеличение, хотя, несомненно, месторождение является крупным и важным.

Хромитовые рудники в регионе Макри давали значительную часть продукции Малой Азии, но большая часть руды, добытой в последние годы, была низкосортной, с содержанием оксида хрома до 40 процентов. Хромит недалеко от Денизлу и тот, что недалеко от залива Адалия, с другой стороны, как говорят, очень богат, некоторые месторождения содержат руду, в среднем достигающую 56 процентов оксида хрома.

Большинство хромитовых рудников Малой Азии, вероятно, сейчас находятся под контролем турецкого правительства, вернувшись к нему десять или пятнадцать лет назад, когда усиление конкуренции со стороны новокаледонского хромита на внешних рынках привело к закрытию многих рудников. Налоги как на разрабатываемые, так и на неразрабатываемые минеральные объекты в Турции настолько высоки, что если рудники не приносят постоянных и существенных доходов, они не могут удерживаться частными лицами.

Политика Турции заключалась в том, чтобы не позволять ее минеральным объектам попадать в руки иностранцев. Поэтому даже в то время, когда эксплуатация месторождений хромита была наиболее активной, рудники, хотя во многих местах и разрабатывались иностранными фирмами, в значительной степени принадлежали турецкому правительству или турецким подданным, которые сдавали их в аренду. Так, в 1904 году основные месторождения недалеко от Бруссы принадлежали чиновнику Порты и эксплуатировались J. W. Whittal & Co., английской фирмой в Константинополе, в то время как другие месторождения в том же районе разрабатывались Patterson & Canghellari, английской компанией, расположенной в Смирне. Знаменитое месторождение Дагхарди в регионе Кутахья в то время принадлежало турецкому морскому министру и эксплуатировалось турком по имени Рагит-бей.

В районе Макри ряд низкосортных месторождений в 1904 году находился под контролем Patterson & Co. из Смирны, а рудники недалеко от залива Адалия контролировались французским синдикатом. Некоторые крупные месторождения недалеко от Денизлу, во внутренних районах, к северу от Макри, как говорят, остаются неразработанными из-за отказа турецкого правительства разрешить добычу.

Месторождения хромита в регионе, окружающем залив Александретта, разрабатывались в небольших масштабах как турками, так и иностранцами. Среди операторов в регионе упоминаются Дуриан-эфенди, турок, представляющий Оттоманский банк; Хюсни Херикизаде-эфенди, турок из Аданы; братья Надер из Мерсины; Alfred Keun & Co. из Смирны; братья Протопацци из Смирны и Mavrommati & Sons из Мерсины, обе, вероятно, греческие фирмы; Лоизидес из Мерсины; и Хаджи Кемаль-бей из Константинополя. Дуриан-эфенди также упоминается как человек, эксплуатировавший хромитовые рудники недалеко от Бейрута.

Наиболее важные месторождения хромита в Индии находятся в северной части Белуджистана, но рудники районов Мадрас и Майсур в южной Индии также давали значительные количества руды. Небольшая добыча велась в Бенгалии. Месторождения Белуджистана крупные, а руда богатая, большая ее часть содержит в среднем почти 55 процентов оксида хрома. Одно месторождение, как сообщается, имеет длину 440 футов и ширину 5 футов. Рудные тела представляют собой сегрегации в серпентине. Проблема транспортировки сложна, так как руды находятся далеко от побережья, а средства наземного транспорта развиты плохо. Тем не менее, эти рудники обеспечивают стабильную добычу с момента их открытия в 1903 году. Самая большая добыча была в 1907 году, когда выход превысил 7000 тонн. С тех пор наблюдается снижение из-за конкуренции со стороны Новой Каледонии и Родезии.

Рудные тела хромита разрабатывались в Мадрасе еще в 1861 году, и небольшие количества руды добывались с перерывами. Руды ассоциируются с магнезитовыми жилами в серпентине. С 1907 года в Мадрасе зафиксирована стабильная добыча, которая в последнее время увеличилась. Важные месторождения хромита найдены в Майсуре. Эти месторождения в последние годы давали более 2000 тонн руды ежегодно, которая, как сообщается, отправлялась в Соединенные Штаты. Месторождения хромита в Бенгалии, как говорят, небольшие и неважные. В Бомбее крупное тело низкосортного хромита, как говорят, имеет размеры 1000 на 300 футов и в среднем содержит 34 процента оксида хрома.

До 1910 года добыча хромита в Японии была спорадической и неважной, но с 1910 года добыча стала стабильной и растущей. Основные месторождения хромовой руды находятся в юго-западной части, рудники Вакамацу в Хоки являются наиболее важными. Руда, как говорят, содержит в среднем около 40 процентов оксида хрома. Также сообщается о наличии хромита в северной части Японии. Японские месторождения хромита небольшие и быстро истощаются.

Основные месторождения хромита в России находятся в южной части Уральских гор и ассоциируются с серпентином и мыльным камнем. Месторождения классифицируются по трем типам: крупные зернистые массы в серпентине, мелко рассеянный хромит в серпентине и хромитовый песок в платино- и золотоносных россыпях. Характерным проявлением тел хромита на Урале являются сегрегации внутри областей дунита, в значительной степени измененного в серпентин. Платина в виде рассеянных зерен ассоциируется с хромитом в дуните в нескольких местах. Недавно о месторождениях хромита сообщалось в северной части Кавказских гор.

Европа.

— Месторождения хромита на Балканском полуострове можно сгруппировать в четыре основных района: центральная Сербия; южная Сербия; Салоники в восточной Македонии; и Магнесия, южная Фессалия и соседние острова. Месторождения хромита встречаются в серпентине, образовавшемся в результате изменения перидотита.

Хромитовые рудники Сербии и Македонии в течение многих лет давали небольшую добычу, приписываемую европейской Турции, которая до последней Балканской войны охватывала все хромитсодержащие районы. Многие месторождения центральной Сербии плохо расположены с точки зрения транспортировки, руда перевозится на телегах до железнодорожных станций, а оттуда по железной дороге до побережья. В восточной Македонии некоторые рудники относительно близки к побережью, и руда перевозится на телегах в Салоники. Рудники Сербии и Македонии разрабатывались частично частными лицами, а частично теми же фирмами, которые добывали хромовые руды Малой Азии, такими как Patterson & Co., Whittal & Co. и другими.

Хромитовые рудники Магнесии, Фессалии и прилегающих островов в восточной Греции давали более или менее непрерывную добычу в течение последних 30 или 40 лет. Однако добываемая руда была в основном низкосортной, большая ее часть содержала в среднем от 30 до 40 процентов оксида хрома. Говорят, что она в основном используется для огнеупорных целей. До 1908 года большая часть греческой добычи хромита поступала с рудников Магнесии, но в последнее время большая часть руды поступала с рудников южной Фессалии. Рудники в Греческом архипелаге также поставляли некоторое количество руды. Ежегодная добыча в Греции варьировалась от нескольких сотен тонн до более чем 15 000 тонн. В течение последних 20 лет она редко опускалась ниже 5000 тонн.

Хромистая железная руда в значительных количествах добывается в Греции, большая ее часть экспортируется. В 1913 году разрабатывалось десять или более рудников. Добыча составляла в среднем более 100 000 тонн ежегодно. Рудники эксплуатируются частично греческими, а частично французскими и британскими фирмами.

Хромистые железные руды, добываемые в бывшей Австрийской империи, поступали главным образом из центральной части Боснии, но хромитовые рудники в Верхней Штирии и те, что находятся на румынской границе, также давали заметную добычу, при этом руда была низкосортной. Месторождения Боснии находятся в серпентине. Руда хорошего качества и добывалась для использования в качестве футеровки печей. На левом берегу реки Дунай и вблизи него в Банате, Венгрия, находится обширная область серпентина, содержащая хромит в виде скоплений. Месторождения разрабатывались в незначительной степени.

Северная Америка.

— В Канаде хромитсодержащие области значительного размера встречаются в южной части провинции Квебек, где расположены почти все продуктивные хромитовые рудники Канады. Руда встречается в серпентине в виде неправильных масс и карманов без определенной формы, размер которых достигает 75 футов по длинной оси, редко достигая 100 футов. Количество высокосортной руды в квебекских месторождениях хромита невелико, но низкосортные рудные тела, которые при нормальных рыночных условиях не могут быть добыты с прибылью, многочисленны и имеют большие размеры. Низкосортные руды варьируются по содержанию оксида хрома от менее 20 процентов до 35 или 40 процентов. Почти вся добытая канадская руда экспортировалась в Соединенные Штаты. С 1910 по 1914 год добыча хромовой руды на рудниках Квебека была незначительной из-за стоимости добычи низкосортных руд и отсутствия рынка сбыта для них. Когда цена на хромит выросла в конце 1914 года, американские фирмы начали активные разработки в этом районе, и впоследствии компанией Mutual Chemical Co. были построены два концентратора. Добыча канадского хромита, как сырой руды, так и концентратов, в военный период была примечательной: добыча выросла со 121 длинной тонны в 1914 году до 47 035 длинных тонн в 1916 году и 43 725 длинных тонн в 1917 году.

Основными американскими фирмами, заинтересованными в разработке канадских месторождений хромита в течение последних нескольких лет, были Mutual Chemical Co., Harbison-Walker Refractories Co., Electrometallurgical Co. и Quebec Asbestos & Chrome Co. Последняя компания приобрела один из концентраторов, построенных Mutual Chemical Co., и обеспечила значительный выпуск как сырой руды, так и концентратов. Канадские фирмы также произвели значительное количество руды.

С окончанием войны и падением цены на хромит канадские рудники были в значительной степени заброшены. Однако возможно, что некоторые американские фирмы, которые добывают руду для использования на своих собственных заводах, могут продолжить работу в небольшом масштабе.

Когда Соединенные Штаты были основной страной-производителем хромита в мире, добыча велась в восточной части Соединенных Штатов и главным образом в Мэриленде. Хромитовый рудник Вуд и соседние месторождения в округах Балтимор и Харфорд обеспечивали большую часть добычи. Меньшие количества добывались в Северной Каролине и Пенсильвании.

Основные месторождения хромита в Соединенных Штатах, которые обеспечивали почти всю руду, добытую в последние годы, находятся в Калифорнии и Орегоне. Недавно месторождения некоторого размера были найдены в Монтане, но они еще не достигли стадии добычи. Месторождения хромита в Калифорнии по большей части сгруппированы в четыре основных района: регион гор Кламат на северо-западе Калифорнии и юго-западе Орегона; Береговой хребет в западно-центральной Калифорнии; хребет Сьерра-Невада на значительной части своей протяженности; и район Сан-Луис-Обиспо на юго-западе Калифорнии.

Хромовые руды Калифорнии и Орегона образуют линзы или неправильные тела в серпентине и родственных породах. Многие рудные тела встречаются в сравнительно свежем перидотите и дуните, и тесная связь между хромитом и ассоциированным пироксеном или оливином хорошо видна. Местами массы хромита встречаются также в мантии остаточного материала, образовавшегося в результате изменения серпентина и других пород. Большинство хромовых руд Тихоокеанского побережья являются низкосортными, немногие содержат более 45 процентов оксида хрома. Были построены обогатительные фабрики для переработки руды из тел, достаточно крупных, чтобы оправдать такие расходы. На некоторых заводах качество руды таким образом повышалось до более чем 52 процентов. Локально были найдены небольшие тела высокосортной руды.

Хромитовые рудники восточных Соединенных Штатов начали разрабатываться около 1827 года и продолжали эксплуатироваться около сорока лет. Месторождения Калифорнии начали разрабатываться около 1870 года, но никогда не давали большой добычи до тех пор, пока война не подняла цену на хромит до беспрецедентных цифр, и руду можно было добывать с прибылью, несмотря на высокие затраты и высокие тарифы на перевозку до центров потребления. Хромитовые рудники Соединенных Штатов всегда разрабатывались и контролировались американским капиталом. В Калифорнии руда добывалась главным образом частными лицами, работающими на небольших разрозненных месторождениях. Несколько крупных фирм, таких как California Chrome Co., Adams & Maltby Co., L. H. Butcher Co. и Union Chrome Co., работали в более крупных масштабах в военный период.

Месторождения хромита были известны на Аляске в течение ряда лет, но только когда война принесла высокие цены, стало возможным добывать их с прибылью. Месторождения, имеющие значение в настоящее время, находятся недалеко от юго-западной оконечности полуострова Кенай. Около 1000 тонн руды, содержащей от 46 до 49 процентов оксида хрома, было добыто в 1917 году.

Южная Америка, Центральная Америка и Куба.

— Насколько известно, в Южной Америке встречается только один важный хромитсодержащий район, он находится в штате Баия, Бразилия. Одно месторождение в этой местности разрабатывалось компанией E. J. Lavino & Co. из Филадельфии, и сообщается об открытии нескольких соседних месторождений. Первые поставки руды были сделаны в феврале 1918 года, и к 1 июля 1918 года 12 620 тонн было отправлено в Соединенные Штаты. Сообщается, что месторождения принадлежат Newman & Co., фирме американских экспортеров в Баие. Они сданы в аренду E. J. Lavino & Co. из Филадельфии.

Южная Америка, за исключением Бразилии, не имеет известных месторождений хромита, имеющих значение. В Колумбии, как сообщается, хромовая руда существует недалеко от Антиокии, и говорят, что хромистый чугун производился доменной печью недалеко от Медельина. В Венесуэле, как говорят, хромовая руда встречается на полуострове Коро.

Важные месторождения хромита лежат вдоль северного побережья Кубы в провинциях Камагуэй и Орьенте. Небольшое месторождение найдено в северо-западной части провинции Матансас. Наиболее важные месторождения на Кубе — это месторождения на руднике Каледония, к югу от залива Нипе и к северо-востоку от железных рудников Маяри компании Bethlehem Steel Co. По оценкам, эти месторождения содержат около 40 000 тонн руды, готовой к добыче. Они принадлежат и разрабатываются компанией Bethlehem Steel Co., которая начала эксплуатацию весной 1918 года. Поставки в течение 1918 года составили 8820 тонн. Вторыми по важности после месторождений на руднике Каледония являются месторождения вдоль побережья, к северо-востоку от Баракоа, известные как месторождения Кайогуан и Потоси, где, по оценкам, имеется около 35 000 тонн руды. Месторождения находятся на северном краю пересеченной горной цепи, образующей восточную оконечность Кубы. Участки Кайогуан принадлежат интересам Брэди (американским), а участки Потоси — компании Harbison-Walker Refractories Co. из Филадельфии.

В провинции Камагуэй месторождения найдены к северо-востоку от города Камагуэй. Они состоят главным образом из масс руды в остаточной глине и наносов на поверхности. Подстилающая порода — серпентин. Месторождения Камагуэя принадлежат частично Университету Лихай, а частично кубинцам. Оценочные запасы составляют 20 000 тонн.

Эксплуатация месторождений хромита на Кубе началась осенью 1917 года и продолжалась весной и летом 1918 года. Только рудник Каледония добывал руду. Все месторождения хромита ассоциируются с областями серпентина.

Хромистые железные руды, которым суждено сыграть важную роль в американской черной металлургии, найдены в Маяри, Камагуэе и Моа, вдоль северо-восточного побережья Кубы. Запасы измеряются сотнями миллионов тонн. В настоящее время добываются только месторождения Маяри.

Месторождения хромита были разработаны во внутренних районах Гватемалы в 1917 году, и поставки начались осенью. Месторождения принадлежали и эксплуатировались International Railways of Central America, американской компанией, и расположены в холмах в 100 милях вглубь страны от Пуэрто-Барриос. Руда находится в серпентине. Она очень чистая и особенно желательна для химических целей. Среднее содержание оксида хрома в поставках в течение 1918 года составляло 58 процентов, что делает эту руду самой высокосортной из тех, что поступали на американский рынок. Руда использовалась компанией Grasselli Chemical Co. Из-за расстояния от железной дороги эти руды очень дороги в добыче, и только благодаря высоким ценам, выплачиваемым за хромит во время войны, они были разработаны.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ НАЦИЙ

Страной, которая лидирует в производстве продуктов хрома, таких как феррохром и химикаты хрома, являются Соединенные Штаты. В нормальное время Соединенные Штаты потребляют более одной трети мирового годового потребления хромита. В 1913 году хромит, используемый производителями феррохрома и химикатов хрома в Соединенных Штатах, составил 65 000 тонн. Из-за войны потребление заметно увеличилось до 1917 года, когда оно составило почти 130 000 тонн. Нормальное потребление хромита в Англии составляет около 25 000 тонн, а во Франции — примерно 35 000 тонн. Эти объемы не сильно увеличились в последние годы. Германия является важным производителем продуктов хрома, обычно потребляя 30 000 тонн хромита ежегодно. Россия и бывшая Австрийская империя использовали, возможно, по 5000 тонн каждая ежегодно. Норвегия и Швеция используют небольшие количества. Потребление в России было главным образом в производстве химикатов хрома, а в бывшей Австрийской империи — главным образом для огнеупорных целей. В Норвегии и Швеции производятся небольшие количества феррохрома.

Соединенные Штаты.

— Соединенные Штаты, хотя и являются крупнейшим в мире потребителем хромита, не являются важным производителем этого минерала в нормальное время. В течение 30 лет, предшествовавших войне, годовая добыча никогда не превышала 4000 длинных тонн сырой руды, а в течение последних 15 лет, предшествовавших войне, самая большая годовая добыча составила 598 длинных тонн в 1909 году. Добыча в 1913 году составляла менее 1 процента от внутренних потребностей.

Поэтому поставки хромита в Соединенные Штаты поступали главным образом из иностранных источников, и этими источниками были в основном Малая Азия, Родезия и Новая Каледония. До 1905 года Турция в Азии была основным источником поставок. С тех пор, однако, Родезия и Новая Каледония в значительной степени заменили Турцию на американском рынке хрома.

Хотя многочисленные месторождения хромита встречаются в западных Соединенных Штатах и локально в восточных штатах, эти месторождения обычно небольшие и разрозненные или низкосортные. Из-за их физического характера, малого размера, разрозненного появления или расстояния от центров потребления отечественный хромит не мог быть поставлен потребителям в требуемом качестве или по цене, по которой мог быть поставлен хромит из богатых иностранных месторождений. По этой причине американские месторождения хромита оставались неразработанными, и руда не добывалась, за исключением небольших количеств, которые потреблялись для огнеупорных целей на соседних металлургических заводах.

Когда в 1914 году, в начале войны, цена на хромит выросла, добыча была немедленно стимулирована, что видно по быстрому увеличению выпуска с 591 длинной тонны сырой руды в 1914 году до около 82 350 длинных тонн сырой руды в 1918 году, что эквивалентно около 66 554 тоннам руды в пересчете на 50-процентный оксид хрома. Однако даже этот значительно увеличенный внутренний выпуск удовлетворил лишь немногим более половины американских потребностей, при этом общее количество хромовой руды, потребленной в 1918 году, составило около 104 000 длинных тонн в пересчете на 50-процентный оксид хрома. Если бы рынок хромита сохранился, однако, отечественные рудники обеспечили бы гораздо большую долю потребностей в 1919 году. Потребление хромита в Соединенных Штатах в 1913 году составило 65 000 тонн руды, содержащей 50 процентов оксида хрома. С этого уровня оно выросло до около 127 000 тонн в 1917 году, что представляет собой максимальное годовое потребление на данный момент.

В следующей таблице представлены данные о добыче и импорте хромита в пересчете на 50-процентный оксид хрома за период с 1913 по 1918 год, а также общее количество, доступное для потребления в эти годы. Хромит из Соединенных Штатов не экспортируется.

Таблица 26. — Добыча и импорт хромита, Соединенные Штаты, 1913–1918 гг.

| Production (long tons) | Imports (long tons) | Total available for consumption (long tons)
1913 |    230 |  65,180 |  65,410
1914 |    530 |  74,578 |  75,108
1915 |  2,756 |  73,762 |  76,318
1916 | 39,509 | 110,849 | 150,358
1917 | 36,729 |  64,978 | 101,707
1918 | 66,554 |  92,678 | 159,232

Цены, выплачиваемые за хромит отечественного производства в Соединенных Штатах в последние годы, варьировались от среднего значения 11,19 доллара за тонну в 1913 году до примерно 24,00 долларов за тонну в 1917 году.

Когда во второй половине 1917 года возникла потребность в увеличении объемов морских перевозок, были приняты меры по сокращению импорта хромита из отдаленных стран, таких как Турция, Новая Каледония и Родезия, увеличению импорта из близлежащих источников, таких как Бразилия, Куба и Канада, а также по стимулированию максимальной добычи на отечественных рудниках. В результате в 1918 году импорт хромита из Бразилии составил 17 854 длинные тонны сырой руды, а из Кубы — 8 821 длинную тонну сырой руды. Ранее на Кубе добыча велась лишь в объеме 34 длинных тонн в 1916 году и 17 длинных тонн в 1917 году. В Бразилии до 1918 года добыча не велась. Импорт из Канады составил 20 949 длинных тонн сырой руды в 1918 году по сравнению с 19 021 длинной тонной в 1917 году и 12 220 длинными тоннами в 1916 году. В начале 1918 года Советом по военной торговле (War Trade Board) были введены различные ограничения с целью сокращения импорта хромита из стран, расположенных далеко за океаном.

Разработка отечественных запасов хромита означает истощение ограниченных ресурсов, высокую себестоимость добычи, использование руд более низкого качества и снижение эффективности потребления. При свободном доступе к высококачественным иностранным рудам рынок для отечественных руд исчезает, и отечественная промышленность по добыче хромита не может существовать в сколько-нибудь значительных масштабах. Если первостепенное значение имеет сохранение мировых сырьевых ресурсов или их наилучшее использование, то отечественной промышленности по добыче хромита следует позволить прийти в упадок, а более дешевые и высококачественные иностранные руды должны заменить отечественный хромит. Опыт последних нескольких лет показал, что месторождения хромита в Соединенных Штатах, дополненные импортом из Канады, Бразилии и Кубы, могут в значительной степени удовлетворять внутренние потребности в течение ограниченного периода.

Соединенные Штаты контролируют лишь небольшую часть мировых запасов хромита. Американские фирмы владеют основными кубинскими месторождениями и контролируют бразильские месторождения на правах аренды. Таким образом, Соединенные Штаты в значительной степени зависят от доброй воли Франции и Англии в вопросе бесперебойных поставок хромовой руды, поскольку эти две страны совместно контролируют большую часть запасов хромита в Родезии и Новой Каледонии. Турция контролирует большинство, если не все, месторождения хромита в Малой Азии, но из-за их изолированного положения в Средиземноморье на эти месторождения нельзя было полагаться как на источник снабжения в случае необходимости. То же самое относится к месторождениям Уральского региона в России.

Основными фирмами-потребителями хромита в Соединенных Штатах являются Electrometallurgical Co., вероятно, крупнейший в мире производитель феррохрома; Mutual Chemical Co. и National Electrolytic Co., крупные производители соединений хрома; а также Harbison-Walker Refractories Co., American Refractories Co. и различные сталелитейные заводы, использующие хромит в качестве огнеупорного материала.

Великобритания.

— До войны Великобритания ежегодно потребляла около 25 000 тонн хромита, большая часть которого использовалась компанией Blackwell & Sons, Ltd. для производства феррохрома. Однако феррохрома, производимого в Англии, недостаточно для удовлетворения потребностей британской сталелитейной промышленности, и значительная его часть импортируется из Франции.

За исключением незначительных проявлений на Шетландских островах, на Британских островах нет месторождений хромита, поэтому Великобритания полностью зависит от зарубежных источников снабжения. С другой стороны, британские колонии богаты месторождениями хромита, и до тех пор, пока британские суда имеют свободу передвижения по океану, они будут иметь доступ к наиболее важным месторождениям хромита в мире.

Благодаря своей богатству и крупным размерам, наиболее важными из всех месторождений, контролируемых Великобританией, являются месторождения Родезии. В настоящее время разрабатывается только одно из многих месторождений в этом районе, а запасы в нетронутых рудных телах, несомненно, велики и, возможно, сопоставимы с запасами Новой Каледонии.

Добыча на родезийских хромовых рудниках в последние годы составляла в среднем около 60 000 тонн в год, или около 35 процентов мировой добычи, и, несомненно, объем производства мог бы быть значительно увеличен при освоении других известных месторождений. Однако даже текущий объем добычи более чем вдвое превышает фактические потребности Великобритании в хромите. Эти потребности, однако, не отражают нужды в металлическом хроме или соединениях хрома, и если бы Франция прекратила поставки феррохрома в Великобританию, английской сталелитейной промышленности потребовалось бы гораздо большее количество сырья — хромита.

Помимо месторождений хромита в Южной Африке, важные месторождения хромита встречаются и в других британских колониях, в частности в Британской Индии и Канаде. В Британской Индии в течение многих лет ежегодно добывалось от 2 000 до 10 000 тонн хромита, в основном в Белуджистане, в северо-западной части страны, но небольшая добыча велась также в Майсуре, в южной части. В ранние годы Индия обеспечивала более значительную часть мировых поставок хромита, чем в настоящее время. Транспортировка является серьезной трудностью при разработке этих месторождений, и когда были освоены новокаледонские и родезийские руды, значение индийских руд снизилось.

Канадские месторождения, хотя и имеют значительные размеры и удобный доступ к восточным американским рынкам, не разрабатывались интенсивно или непрерывно из-за низкого качества руд. Путем обогащения можно получить продукт среднего и высокого качества, но методы обогащения дороги и повышают стоимость материала до такой степени, что он не может конкурировать с другими рудами, представленными на рынке. Таким образом, стоимость добычи как индийских, так и канадских руд такова, что в нормальных условиях трудно найти для них рынок сбыта, но в случае необходимости из этих источников можно получить значительный тоннаж.

Другими британскими колониями, в которых существуют месторождения хромита, являются Новый Южный Уэльс, Тасмания и Новая Зеландия. Насколько известно, месторождения в этих странах невелики, и только месторождения в первом из них обеспечили небольшую добычу.

Помимо контроля над месторождениями хромита во многих частях мира через свои колониальные владения, Великобритания контролирует месторождения через британские фирмы, имеющие иностранные активы. Так, компания Chrome Co., Ltd., представляющая смешанные британские и французские интересы, контролирует не только добычу хромита в Родезии, но также владеет и управляет большинством важных новокаледонских рудников.

В прошлом Великобритания получала большую часть своих поставок хромита из Родезии, Новой Каледонии и Турции. Хотя в Родезии добывается более чем достаточно хромита для удовлетворения британских потребностей, Англия разрешала экспортировать большую часть родезийской руды в другие страны и импортировала иностранную руду для части собственных нужд. Вероятно, большая часть родезийской продукции до войны направлялась в Соединенные Штаты. Значительная часть руды, потребляемой в Англии, поступала из Турции, где английские фирмы в течение многих лет проявляли интерес к добыче хромита. Большая часть индийской продукции, вероятно, использовалась в Великобритании, но часть ее направлялась во Францию.

Франция.

— Во Франции известно несколько месторождений хромита, но они не имеют коммерческого значения. Поэтому Франция, как и Англия, полностью зависит от зарубежных источников поставок хромита. Однако, в отличие от Англии, у Франции есть только одна колония, Новая Каледония, содержащая важные месторождения хромита; но, к счастью, эта колония содержит достаточно руды, чтобы стать одним из основных мировых источников хромита.

Хотя компания Chrome Co., Ltd., которая контролирует основные новокаледонские месторождения хромита и является крупнейшим поставщиком, представляет как английский, так и французский капитал, Франция посредством политических рычагов может контролировать добычу хромита на острове. Хотя в прошлом, вероятно, большая часть хромита, используемого во Франции, поступала из этого источника, Франция также использовала родезийские и турецкие руды, а также, вероятно, в значительной степени российские руды, в то время как много новокаледонской руды направлялось в Германию, Соединенные Штаты и Великобританию.

Основными французскими фирмами, производящими феррохром, являются Société Electrometallurgique Française в Ла-Пра, Société La New Metallurgie в Жифре, Société Anonyme Electrometallurgique в Альбервиле, Keller, Leleux et Cie в Ливе, Société Electrometallurgique de Saint Beron в Сен-Бероне, Ch. Betrolus в Бельгарде и Rochette Frères в Эпьере.

Германия.

— За исключением неважных низкосортных месторождений в Силезии, Германия не имеет запасов хромита в своих границах. Как потребитель хромита Германия по значимости стоит в одном ряду с Францией, причем большая часть потребляемой руды используется в производстве феррохрома, основными производителями которого были заводы Круппа. Однако в изобилии производятся и хромовые химикаты. Неизвестно, чтобы какая-либо из бывших колоний Германии имела месторождения хромита, за исключением Тоголенда, но месторождения в Тоголенде не освоены и считаются неважными.

В прошлом Германия получала хромит из Новой Каледонии, Родезии, Турции, Греции и, вероятно, России. Из-за длительной железнодорожной перевозки из России и плохого состояния развития промышленности в Турции руды из этих двух стран в годы, непосредственно предшествовавшие войне, в значительной степени заменялись рудами из-за рубежа. Таким образом, все четыре крупные страны-потребителя хромита в основном ориентировались на Новую Каледонию и Родезию как на свои источники снабжения.

Во время войны, когда зарубежный хромит был недоступен, Германия благодаря своим отношениям с Турцией получила возможность приобретать хромит из Малой Азии, а также, вероятно, с хромитовых рудников в Сербии, Венгрии, Боснии и Герцеговине. Таким образом, в случае необходимости, когда обычные зарубежные источники снабжения были отрезаны, Германия через свои отношения с соседними странами смогла получить по суше достаточное количество хромита для удовлетворения своих потребностей в боеприпасах. Если бы война продолжилась, Германия, несомненно, развила бы хромитовые ресурсы Урала, и они вместе с месторождениями Малой Азии, даже при их текущем состоянии разработки, могли бы обеспечивать Германию неопределенно долго.

Вероятно, что германский контроль стал значимым на рудниках Малой Азии во время войны. Благодаря относительно небольшим улучшениям транспортной инфраструктуры, таким как строительство железнодорожных веток к основным месторождениям, хромитовые рудники Малой Азии могли бы быть возрождены до такой степени, чтобы позволить рудам конкурировать с родезийской и новокаледонской рудой и снова поставить их в число крупных мировых производителей. Месторождения велики, и по запасам они сопоставимы с месторождениями Родезии и Новой Каледонии.

Россия.

— Россия независима в том, что касается ее потребностей в хромите. Из ее добычи, составляющей около 20 000 тонн в год, отечественная промышленность потребляет менее одной четверти, а остальное доступно для экспорта в страны, менее обеспеченные ресурсами хромита.

Большая часть хромита, используемого в России, идет на производство хромовых химикатов. Российский бихроматный завод в Елабуге, к востоку от Казани, основанный в 1892 году, потреблял около 2 000 тонн руды ежегодно.

РЕЗЮМЕ

Политический и коммерческий контроль над основными месторождениями хромита в мире обобщен в следующей таблице:

Таблица 27. — Политический и коммерческий контроль над месторождениями хромита

Country | Political control | Predominant commercial control
New Caledonia | French | French-British
Rhodesia | British | British
Asia Minor | Turkish | Turkish
Ural Mountains, Russia | Russian | Russian-British
Greece | Grecian | Uncertain
Serbia | Serbian | Uncertain
India | British | Probably British
Canada | British | United States-Canadian
United States | United States | United States
Brazil | Brazilian | United States
Cuba | Cuban | United States
Japan | Japanese | Japanese
Austria-Hungary | Austrian | Uncertain
Guatemala | Guatemalan | United States

Великобритания и Франция производят в своих колониальных владениях достаточно хромита для собственных нужд и для экспорта, но Соединенные Штаты, крупнейший в мире потребитель, должны зависеть, за исключением времени чрезвычайных ситуаций, от импорта, в основном из Новой Каледонии и Родезии.

Различные страны время от времени играли важную роль в удовлетворении мирового спроса на хромит. Одна страна за другой вытеснялись с рынка по мере появления более дешевых или более качественных сортов хромита. Временами эти изменения были вызваны обнаружением более крупных тел руд более высокого качества, чем те, что добывались ранее, а в других случаях они были вызваны тем, что дешево транспортируемые руды заменяли руды, неудобно расположенные по отношению к центрам потребления.

Так, в начале девятнадцатого века и примерно до 1830 года Уральский горный регион России обеспечивал большую часть мировых потребностей в хромите, которые были невелики. Около 1830 года в восточной части Соединенных Штатов, особенно в Мэриленде, были сделаны важные открытия хромита, и Соединенные Штаты вскоре вытеснили Россию как ведущего производителя хромита. После этого в течение многих лет Соединенные Штаты продолжали лидировать в добыче хромита примерно до 1870 года, когда отечественные месторождения постепенно приблизились к истощению, а важные месторождения, открытые в европейской Турции и Малой Азии, начали интенсивно разрабатываться.

Малая Азия была основной страной-производителем хромита примерно с 1870 года до начала двадцатого века. Месторождения продолжали разрабатываться довольно стабильно из-за их богатства и больших размеров, хотя они были неудобно расположены с точки зрения транспортировки. Только некоторые месторождения, такие как месторождения в регионах Макри и Александретта, находились настолько близко к побережью, что руду можно было перевозить на мулах или верблюдах в порты отгрузки. Из более крупных месторождений, таких как Дагарди, руду приходилось перевозить животными на железнодорожные станции, часто на расстояние многих миль, а затем по железной дороге к побережью. Из-за этих трудностей турецкая руда была в значительной степени заменена рудой из важных новокаледонских и родезийских месторождений, как только они были освоены.

В Новой Каледонии рабочая сила дешева, а все месторождения находятся недалеко от побережья. С помощью парусных судов и трампов, которые взимают низкие ставки и часто требуют такие тяжелые материалы, как хромит, в качестве балласта, эту руду можно доставлять в пункты потребления с относительно небольшими затратами. Родезийские месторождения хромита не так доступны с побережья, но они велики и богаты, а тарифы на железнодорожные перевозки до порта отгрузки исключительно низки. По этой причине родезийская руда смогла успешно конкурировать на рынке с новокаледонской рудой, и эти два источника, таким образом, в последние годы совместно удовлетворяли большую часть потребностей основных стран в хромите.

Во время войны из-за ненормальных условий, возникших вследствие нехватки транспортных мощностей, существовала значительная неопределенность относительно того, будет ли возможно обеспечить американских потребителей хромита импортными рудами. Под влиянием значительно более высоких цен добыча хромита в Соединенных Штатах увеличилась с 255 длинных тонн сырого хромита в 1913 году до примерно 82 350 тонн в 1918 году, в основном в Калифорнии, Вашингтоне и Орегоне. Это производство было больше, чем годовая добыча сырой руды из любого отдельного источника (за исключением 82 910 тонн из Новой Каледонии в 1906 году) с момента начала промышленности по добыче хромита. Это производство, конечно, не могло продолжаться без быстрого истощения американских запасов хромита и не представляет собой нормального развития.

ГЛАВА VI. НИКЕЛЬ. Автор: К. С. Корбетт

ПРИМЕНЕНИЕ НИКЕЛЯ

Никель используется главным образом в производстве специальных сталей. По оценкам [65], около 60 процентов всей добычи никеля идет на выплавку стали в нормальное время и больше — в условиях войны. Никелевые стали являются наиболее важными из всех легированных сталей и наиболее часто используемыми [66]. Они применяются там, где требуется необычайная прочность на разрыв. Никель-хромовые стали используются в производстве броневых плит.

[65] Отчет Королевской комиссии по никелю Онтарио, 1917 г., стр. 300.

[66] Брэдли Стоутон: «Металлургия железа и стали», 1911 г.

Обычные никелевые стали обычно содержат около 3,5 процента никеля. «Высоконикелевые стали, содержащие до 40 процентов никеля, используются для специальных целей, где важны немагнитные свойства, устойчивость к коррозии и, прежде всего, отсутствие расширения или сжатия, или любое желаемое расширение или сжатие при изменении температуры» [67].

[67] Отчет Королевской комиссии по никелю Онтарио, 1917 г., стр. 301.

Цветные никелевые сплавы нашли широкое применение, и, вероятно, около 20 процентов мировой добычи никеля идет на их производство. Безусловно, наиболее важными являются сплавы, образованные из никеля и меди. Один из них, обычно называемый «купроникелем», содержит приблизительно 80 процентов меди и 20 процентов никеля и широко используется для оболочек пуль и других военных целей. Другой, ставший хорошо известным под торговой маркой «монель-металл», содержит 29 процентов меди, 67 процентов никеля, около 2,5 процента железа и небольшое количество марганца. Он производится непосредственно из штейна Садбери. Монель-металл используется главным образом там, где необходим прочный, не подверженный коррозии металл, например, в частности, в гребных винтах судов.

По оценкам, около 2 процентов добычи никеля используется для гальванопокрытий. В значительной степени никелирование предотвращает коррозию покрываемого металла.

Никель также используется для аккумуляторов; для чеканки монет; в качестве катализатора при отверждении масел или жиров (твердые жиры используются для производства мыла); для кухонной утвари; и в качестве пигмента для окрашивания керамических изделий. Сомнительно, чтобы на эти последние цели уходило более 3 процентов мировой добычи никеля.

Медь придает стали свойства, несколько схожие с теми, что придает никель, в частности, повышая прочность на разрыв. Кремний также придает стали схожие свойства, увеличивая, прежде всего, вязкость и прочность на разрыв. Значительная доля хрома делает сталь высокоустойчивой к коррозии. Однако не известно ничего, что могло бы заменить никель в специальных сталях, имеющих нулевой или заранее определенный коэффициент расширения, таких как «инвар» или «платинит».

Никель обладает необычайной способностью придавать свой белый цвет сплавам меди; отсюда его использование в чеканке монет. Другие белые металлы, которые могли бы быть использованы вместо него, менее распространены и более дороги. Нет другого распространенного металла или сплава, обладающего хорошим цветом, большой прочностью и устойчивостью к коррозии, которыми обладают монель-металл и подобные сплавы никеля и меди.

Соли никеля используются в качестве заменителей металлов платиновой группы в качестве катализаторов при отверждении масел и жиров.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Добыча никеля в довольно крупных масштабах началась только после открытия рудников в Новой Каледонии в 1875 году. Для обработки этих руд в Англии и континентальной Европе были построены плавильные и аффинажные заводы. Поскольку руды относятся к силикатному типу и не содержат меди, они легко поддавались обработке обычными процессами плавки с флюсами для удаления пустой породы, а затем нагреванием с древесным углем для восстановления до металлического состояния. Был получен чистый металл, который нашел хороший рынок сбыта.

Добыча медно-никелевых руд в районе Садбери началась в 1887 году. Из-за наличия меди вместе с никелем в этих рудах пришлось разрабатывать новые процессы аффинажа и преодолевать торговые предубеждения против продукта. На это ушли упорные усилия в течение нескольких лет. Только одна из первых компаний, начавших работать в районе Садбери, сохранилась до настоящего времени. Это Canadian Copper Co., производственная дочерняя компания International Nickel Co.

Для обработки медно-никелевых руд были разработаны три новых процесса аффинажа. Orford Copper Co. (дочерняя компания International) использует процесс с сульфатом натрия (salt cake process). Этот процесс представляет собой сплавление с сульфидом натрия, при котором сульфид меди концентрируется в верхней части, а сульфиды никеля — в нижней части расплава. Повторное сплавление «верхов» и «низов» обеспечивает хорошее разделение.

У компании Mond был процесс еще до того, как у нее появились рудники. Этот процесс основан на летучести никеля путем пропускания оксида углерода над штейном, который был предварительно подвергнут обжигу и выщелачиванию от содержания меди. Образуется карбонил никеля, Ni(CO)4, и металлический никель осаждается при разложении этого продукта, так что полученный никель является чистым.

Процесс Гибинетта, процесс, основанный на электролизе, был впервые разработан на заводе Orford Copper Co. на штейне Садбери. Он использовался для низкосортных руд во Фредериктауне, штат Миссури, а затем позже для норвежских руд в Кристиансанне. Он будет использоваться на новом аффинажном заводе British-American Co. в Онтарио.

Монель-металл производится непосредственно из штейна Садбери с удалением небольшого количества меди. Он известен как естественный сплав, в отличие от сплава, полученного путем объединения чистых металлов.

Увеличение использования никельсодержащей железной руды для выплавки стали уменьшит количество никеля, которое придется добавлять при производстве такой стали. Это, вероятно, будет скомпенсировано увеличением использования таких сталей.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Анализы изверженных пород показывают, что никель присутствует в средней изверженной породе в количестве 0,020 процента [68]. О его встречаемости Кларк говорит [69]: «Очень часто обнаруживается в изверженных породах, вероятно, как составляющая оливина. * * * Присутствие никеля особенно характерно для магнезиальных изверженных пород, и в них он обычно ассоциируется с хромом». О меди он говорит: «Минутные следы этого металла часто обнаруживаются в изверженных породах, хотя они редко определяются количественно». По оценкам [70], медь присутствует в средней изверженной породе в пропорции около 0,010 процента, или только около половины содержания никеля, а цинк и свинец присутствуют в еще меньшей пропорции. Несмотря на это большее обилие никеля, месторождения меди, свинца и цинка, пригодные для разработки, гораздо более распространены, и добыча их соответственно больше. «Таким образом, можно сказать, что никель менее поддается концентрации агентами, которые способствуют образованию месторождений, пригодных для разработки, чем другие упомянутые металлы (медь, свинец и цинк)» [71].

[68] Ф. У. Кларк, «Данные геохимии», Бюллетень 616, Геологическая служба США, 1916 г., стр. 27.

[69] Там же, стр. 18.

[70] Отчет Королевской комиссии по никелю Онтарио, 1917 г., стр. 95.

[71] Там же.

Из вышесказанного можно сделать вывод, что никелевые месторождения, имеющие значение, вероятнее всего, будут встречаться в связи с изверженными породами, особенно основными. Это действительно так; фактически, единственные известные никелевые месторождения коммерческой или перспективной коммерческой ценности встречаются в ассоциации с основными изверженными породами. Никеленосные металлогенические провинции мира можно сказать, что они лежат внутри петрографических провинций. Харкер говорит [72]: «Изучение пород, принадлежащих к одному великому периоду магматической активности, и их фактического распределения позволяет нам выделить области большей или меньшей протяженности, внутри которых породы представляют большую или меньшую степень родства, причем закон заключается в том, что более выраженная специализация идет с более узкой локализацией». На основе этого закона и факта, отмеченного Кларком и упомянутого выше, никеленосные металлогенические провинции могут быть ограничены более тесно, чем просто областями основных изверженных пород. Можно сказать, что они примерно совпадают с областями основных изверженных пород, характеризующихся минералами группы оливина, причем эти минералы образовались в результате высокого содержания магния в магме породы.

[72] Альфред Харкер, «Естественная история изверженных пород», 1909 г., стр. 89.

Никелевые руды встречаются там, где была необычная сегрегация элемента в изверженной породе во время затвердевания. В некоторых местах для превращения породы в руду потребовалась дальнейшая концентрация путем выветривания. В других местах концентрации путем выветривания оказалось недостаточно, чтобы сделать никель ценным сам по себе, но она повысила содержание железа в породе, а вместе с ним и содержание никеля, до такой степени, что сделала руду ценной в первую очередь как железную руду и дополнительно ценной из-за содержания в ней никеля.

Никель уникален среди менее редких металлов тем, что один район содержит количество доступной, пригодной для разработки руды, намного превышающее количество во всех других известных месторождениях мира вместе взятых. Это район Садбери в Онтарио. Никелевые руды там были сегрегированы из огромной массы изверженной породы, внедренной в условиях, благоприятных для широкой сегрегации, и впоследствии подвергшейся эрозии настолько, что стали доступны крупные рудные тела.

В тех никелевых рудах и никеленосных железных рудах, где выветривание было необходимым агентом для концентрации никеля и железа в достаточной степени, чтобы сделать их коммерчески ценными, исходными месторождениями были никеленосные изверженные породы — то есть они были похожи на породы, связанные с никелевыми месторождениями сульфидного типа, но содержали гораздо меньше никеля. Никелевые месторождения региона Новой Каледонии, которые занимают второе место по продуктивности после месторождений района Садбери, относятся к этому типу. Кубинские никеленосные железные руды лучше всего иллюстрируют месторождения железных руд этого типа.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Никеленосные рудные месторождения мира можно разделить на два основных типа — сульфидный тип, в котором выветривание не имело первостепенного значения, и гарниеритовый или латеритный тип, в котором выветривание изменило и сконцентрировало никель, а также хром и железо исходной породы. Кроме того, никель встречается в некоторых местах с рудами драгоценных и полудрагоценных металлов в жилах. Никель может быть извлечен из таких руд в качестве побочного продукта, но руды никогда не добываются в первую очередь из-за содержания в них никеля. Краткие описания известных месторождений, сгруппированные по типам, которые следуют ниже, были взяты из описаний мировых никелевых месторождений в отчете Королевской комиссии по никелю Онтарио. Приведено несколько прямых цитат из текста отчета.

Месторождения сульфидного типа.

— Район Садбери расположен в юго-восточном Онтарио, Канада. В своих общих чертах геология этого района относительно проста. Огромная масса никеленосной породы была внедрена в виде «лакколитового пласта» или силла вдоль несогласной плоскости контакта между горизонтально залегающими осадочными породами и подстилающим комплексом древних пород. Во время внедрения и остывания, или, возможно, вскоре после этого, подстилающие породы центральной части лакколита, покрывающие резервуары, из которых пришла магма, просели. Длительные периоды эрозии затем выровняли регион до тех пор, пока все, что осталось от силла, не заняло синклинальный бассейн длиной почти 40 миль и шириной от 10 до 15 миль. Все вовлеченные породы имеют докембрийский возраст.

Лакколитовый пласт имеет толщину приблизительно 10 000 футов. При остывании он дифференцировался на два вида пород — микропегматит, породу гранитной группы, образующую теперь верхнюю часть силла, и норит, габбровую породу, образующую нижнюю часть. Переход между этими двумя породами довольно резкий. В основании силла, в некоторых местах залегающего между норитом и подстилающей породой, а в других местах полностью внутри подстилающей породы, находятся рудные тела, состоящие из пирротина, пентландита и халькопирита. Это сегрегированные продукты норита, которые в некоторых местах затвердели в основании силла, а в других были внедрены в виде даек в подстилающие породы или в ранее затвердевшие части норита. Они представляют собой коммерческие рудные тела там, где сульфиды составляют преобладающую часть породы.

Рудные тела классифицируются как «маргинальные» и «смещенные» (offset). Маргинальные месторождения встречаются вдоль контакта норита с подстилающей породой. Часто они залегают полностью внутри пород, прилегающих к нориту. Смещенные месторождения встречаются там, где разломы пересекают крылья складки, образуя зоны слабости, в которые была внедрена руда или минерализованный норит.

Никельсодержащим минералом является пентландит; медьсодержащим — халькопирит. Другой сульфид, пирротин, является сульфидом железа. Добываемые на сегодняшний день руды содержат в среднем около 3,5 процента никеля и 2 процента меди.

С момента открытия района в 1887 году до конца 1916 года было добыто и выплавлено почти десять с половиной миллионов тонн руды Садбери; и из этого было произведено около 285 000 тонн никеля. По оценкам, запасы руды составляют, вероятно, не менее 100 000 000 тонн. В 1916 году было добыто и выплавлено более полутора миллионов тонн руды.

Рудник Алексо расположен в 150 милях прямо к северу от Садбери. Руда встречается на контакте большой массы перидотита (теперь измененного в серпентин) с подушечной лавой, в которую внедрился перидотит. Руда состоит из сульфидных минералов, сегрегированных из интрузивной массы. Она бывает двух типов: один — массивная, чистая сульфидная руда, занимающая трещины в дайкоподобных отношениях, другой — вкрапленная сульфидная руда в перидотите, прилегающем к сульфидным рудным массам. Рудное месторождение имеет доказанную длину 700 футов, вскрыто на глубину 120 футов, а бурение показало, что руда простирается на глубину 240 футов. Среднюю ширину можно принять приблизительно за 10 футов. К концу 1916 года было добыто 34 650 тонн руды, и было разведано более этого количества. В 1915 году было отгружено около 12 000 тонн руды, содержащей в среднем около 4,9 процента никеля и 0,6 процента меди. В этом месторождении, вероятно, доступно несколько сотен тысяч тонн.

Никелевые рудные месторождения Норвегии минералогически похожи на месторождения Садбери. Месторождения невелики, содержание металла в них низкое, и по сравнению с месторождениями Садбери и Новой Каледонии они не имеют большого значения. К 1909 году в Норвегии было добыто и выплавлено около 400 000 тонн никелевой руды. Ручная сортировка руды содержала от 1,4 до 1,7 процента никеля.

Месторождения, подобные норвежским, были найдены в Швеции, но в последние годы они не разрабатывались. В скандинавских странах, очевидно, существует никеленосная металлогеническая провинция, и там еще могут быть найдены важные рудные месторождения.

В Соединенных Штатах, недалеко от Гэпа, округ Ланкастер, штат Пенсильвания, находится месторождение никелевой руды сульфидного типа, которое встречается как сегрегация из 300-футовой дайки амфиболита. Оно периодически разрабатывалось на медь в течение всего 18-го века. Никель был обнаружен в руде в 1852 году, и, по оценкам, до 1882 года было произведено 4 000 000 фунтов никеля. Появление руд Новой Каледонии и Садбери привело к закрытию рудника. Добываемая руда содержала от 1 до 3 процентов никеля и около одной трети этого количества меди.

Рядом с Джулианом, округ Сан-Диего, Калифорния, находится сульфидное никелевое месторождение, которое никогда не было коммерчески продуктивным. Анализы показывают, что руда содержит почти 3 процента никеля или более.

Небольшое месторождение в Тасмании дало несколько тысяч тонн богатой руды. Алмазное бурение показало, что руды осталось мало.

Никель-медные сульфиды были найдены в связи с крупным интрузивом основной изверженной породы в хребте Инсизва, Южная Африка. Рентабельной руды найдено не было.

Никелевые сульфидные месторождения неизвестного значения встречаются в Индии и в Юго-Западном Китае. Небольшие месторождения, которые разрабатывались, когда никель был в дефиците, встречаются в Италии, Шотландии, Германии и Австрии.

Месторождения гарниеритового и латеритного типов.

— Около одной трети поверхности острова Новая Каледония занято серпентином, являющимся продуктом выветривания основной изверженной породы. «Руда, ноумеаит или гарниерит, встречается как гидратированный силикат никеля и магнезии и лучше всего может быть описана как продукт изменения серпентина, в котором магнезия и железо были замещены никелем. * * * Месторождения, пригодные для разработки, всегда встречаются на седловинах отрогов от главного горного хребта, на высотах от 400 до 2 500 футов, причем последняя высота является более распространенной. * * * Замещение серпентина никелем следует по трещинам и разломам в серпентине, а неразложившиеся блоки и валуны серпентина, как правило, покрыты оболочкой руды, которую приходится отбирать вручную». Руды отбираются вручную, чтобы довести их до сорта, выгодного для обработки. В прошлом не считалось экономичным плавить руду с содержанием никеля ниже 4,5 процента, а также отгружать руду с содержанием значительно ниже 6,5 процента.

Рудные тела обычно содержат менее 250 000 тонн руды. Крупнейший из когда-либо разрабатывавшихся рудников произвел менее 600 000 метрических тонн (2 204 фунта) руды. Вероятно, все еще остается столько же неразведанной руды, сколько было добыто за сорок лет производства — эквивалентно 160 000 тонн никеля. Это было бы равно примерно четырехлетнему объему добычи района Садбери при уровне производства 1916 года. «Существуют крупные тела низкосортных руд, которые еще не удалось найти целесообразным для обработки».

Три крупных пластовых месторождения никеленосной железной руды встречаются на возвышенных плато на Кубе. Это типичные латеритные (остаточные) месторождения. Средняя глубина руды составляет 15 футов, а совокупный тоннаж трех месторождений оценивается в полтора-три миллиарда тонн. Содержание никеля варьируется от примерно 0,6 процента до 2,1 процента и показывает прогрессивное обогащение сверху вниз. Хром также присутствует и показывает аналогичное обогащение. Присутствие никеля и хрома в железных рудах значительно повышает их ценность для производства специальных сталей.

Железная руда на острове Себоэкоэ, лежащем у юго-восточного побережья Борнео, содержит заметные количества никеля и хрома. По меньшей мере 300 000 000 тонн руды содержится в месторождении, которое представляет собой пористый лимонит толщиной около 15 футов, залегающий поверх серпентина.

В Соединенных Штатах никелевые месторождения гарниеритового типа встречаются в Северной Каролине и Орегоне. Попытки добывать эти руды никогда не были успешными.

Небольшие никелевые месторождения гарниеритового типа встречаются в Египте, Германии (прусская Силезия), Греции, на Мадагаскаре, в России и Испании. Никеленосные железные руды встречаются в Греции, и считается, что хромистые железные руды на острове Миндао на Филиппинах могут при дальнейшей разведке оказаться никеленосными.

Никель в жилах.

— Никель встречается с другими металлами, драгоценными или полудрагоценными, в некоторых жильных месторождениях и извлекается как побочный продукт при обработке руд из них. Он заметно присутствует в месторождениях в Кобальте, Онтарио, и был найден в жильных месторождениях в Соединенных Штатах, Франции, Германии, Австрии, Мексике и Южной Америке. Несколько сотен тонн извлекается ежегодно при аффинаже меди, производимой в Соединенных Штатах.

К типу жильных месторождений никельсодержащей руды относятся месторождения галенита, рассеянные в доломите в юго-восточном Миссури. Сульфиды железа, меди, никеля и кобальта встречаются вместе с галенитом. Много лет назад никель извлекался электролитическим путем из штейна этих руд.

РАЗВИТИЕ И ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРОСТРАНЕНИИ

В 1900 году Новая Каледония поставляла 65 процентов мирового производства, а Онтарио — 35 процентов. С тех пор мировое производство увеличилось в шесть раз, и Онтарио к концу 1916 года производил 80 процентов всего объема. Это показывает тенденцию развития отрасли. Недавние открытия руды в районе Садбери и строительство новых плавильных и аффинажных заводов в Онтарио для обработки руд указывают на растущее доминирование этого района в отрасли. Новая Каледония не имеет крупных рудных тел и находится слишком далеко, чтобы успешно конкурировать с Онтарио, хотя работа там будет продолжаться.

Рис. 7. — Рафинированный никель, произведенный из руд Новой Каледонии и Онтарио, за пятилетние периоды; суммы указаны за указанный календарный год.

Статистика добычи и запасов руды в Онтарио и Новой Каледонии показана графически на рисунках 7 и 8.

Изолированные рудные тела никеля сульфидного типа — то есть сегрегации из основных изверженных пород, как в Садбери — были найдены в ряде широко разнесенных мест. Существует отчетливая вероятность того, что существуют и другие, которые могут быть обнаружены. Такие неоткрытые месторождения могли бы даже содержать больше доступной руды в совокупности, чем общее количество добытых и нетронутых руд района Садбери, но в свете современных знаний это кажется отдаленной возможностью.

Другие месторождения новокаледонского и кубинского типов, вероятно, будут обнаружены, но сомнительно, чтобы оставались неоткрытыми столь же крупные месторождения этих типов. В них никель остался в материале, оставшемся в качестве остатка от частичного или полного выветривания путем растворения исходной никеленосной породы. Этот материал лежит на поверхности и покрывает относительно широкие площади. Поэтому тела его обычно нетрудно обнаружить. Кажется, что они встречаются наиболее обильно в теплых широтах, где выветривание путем растворения наиболее легко происходило в условиях, благоприятных для сохранения остатка.

Рис. 8. — Добыча никеля и содержание никеля в запасах в Онтарио, Новой Каледонии и Норвегии.

Настоящие известные месторождения никеля и никеленосных железных руд примерно указывают на местоположения, возможно, всех или почти всех никеленосных металлогенических провинций мира. Именно в этих провинциях наиболее вероятно обнаружение новых месторождений. Широкое распространение этих провинций указано в следующем утверждении в Отчете Комиссии по никелю Онтарио:

Хотя конкуренции не следует опасаться (то есть для Онтарио), было бы бесполезно пытаться перекрыть поставки никеля почти любой из великих наций. * * * Почти каждая важная страна имеет запасы никелевой руды, которые могут быть разработаны, если спрос велик, тем самым обеспечивая высокую цену.

Считается вероятным, что никеленосная металлогеническая провинция восточной Канады, которая включает район Садбери, содержит величайшие неизвестные никелевые месторождения, точно так же, как она содержит величайшее известное, и это по трем причинам. Первая и самая очевидная причина заключается в том, что великие никелевые рудные тела района Садбери, изолированное рудное тело Алексо, в 150 милях к северу от района, и заметное содержание никеля в жилах Кобальта и других близлежащих районов указывают на необычно высокое содержание никеля в исходной магме, из которой были получены основные изверженные породы. Вторая причина заключается в том, что мантия ледниковых отложений эффективно скрывает большие площади подстилающей породы и препятствует легкому обнаружению. Третья заключается в том, что дикая и неустроенная природа страны препятствует человеческой деятельности, благодаря которой могли бы быть сделаны случайные или другие открытия.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Никелевые месторождения Садбери и рудное тело Алексо в восточном Онтарио находятся под политическим контролем Британской империи; никелевые месторождения Новой Каледонии контролируются политически Францией, так как Новая Каледония является французской колонией; а никелевые месторождения Норвегии и Кубы находятся под политическим контролем этих правительств. Другие месторождения мира, как было отмечено, коммерчески неважны.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Владение рудниками и неразведанными рудными телами в районе Садбери разделено между британскими и американскими интересами. В настоящее время руду добывают две компании, и ожидается, что третья вскоре начнет добычу.

Первой крупной компанией в этой области была Canadian Copper Co. Это дочерняя компания International Nickel Co., более 90 процентов акций которой принадлежит Соединенным Штатам. Canadian Copper Co. владеет следующими рудниками: Copper Cliff, Evans, Stobie, Crean Hill, Vermilion, Creighton, No. 1, No. 2, No. 3, No. 4, No. 5 и No. 6. Четыре из них разрабатывались в 1917 году — Crean Hill, Vermilion, Creighton и No. 2. В декабре 1916 года президент Canadian Copper Co. дал следующие оценки запасов рентабельной руды в трех объектах этой компании: 10 000 000 тонн в Creighton; 2 000 000 тонн в Crean Hill; и 45 000 000 тонн в No. 3.

Mond Nickel Co. контролируется британскими интересами. Она владеет следующими рудниками: Garson, Worthington, Levack, Victoria и Kirkwood. Levack имеет доказанные запасы хорошей руды в количестве 4 500 000 тонн. Запасы других рудников не указаны.

British-America Nickel Corporation, Ltd. имеет 20 000 000 долларов обыкновенных акций, из которых 14 500 000 долларов принадлежат британскому правительству на имя Алана Андерсона, доверительного управляющего. К концу 1916 года эта компания имела 11 000 000 тонн пригодной для разработки руды, подготовленной к добыче. Ее рудники — Murray, Gertrude, Elsie, Blue Lake и Frood Extension. Запасы только Murray оцениваются в 9 000 000 тонн.

В юго-восточной части района недавно в ходе алмазного бурения, проведенного компанией E. J. Longyear Co. из Миннеаполиса, было обнаружено рудное тело длиной 7500 футов, мощностью от 10 до 120 футов и простирающееся как минимум на глубину 1020 футов в одном месте. Эта компания и ее партнеры, все американцы, осуществляют коммерческий контроль над этим рудным телом. Запасы руды в данном месторождении оцениваются в 6 000 000 тонн выше горизонта 500 футов. Несколько скважин были пробурены на большую глубину, где также была обнаружена руда. Оценить запасы этого месторождения ниже глубины 500 футов не представляется возможным.

Компания Alexo Mining Co. Ltd., разрабатывающая месторождение Алексо к северу от района Садбери, является канадским предприятием. Оценка количества руды в этом месторождении отсутствует, однако оно невелико по сравнению с месторождениями района Садбери. Общий объем может составлять несколько сотен тысяч тонн.

Крупнейшими и наиболее важными владельцами земель, содержащих никель, в Новой Каледонии, в относительном порядке значимости их активов, являются: (1) La Société le Nickel, компания, ведущая добычу на острове в течение многих лет. (2) The International Nickel Co., представленная в Новой Каледонии двумя своими дочерними компаниями: The Nickel Corporation и La Société Minière Caledonienne. International не ведет добычу на острове, но некоторые из ее земель разрабатываются на правах аренды лицами, связанными с La Société le Nickel. (3) Les Hauts-Fourneaux de Noumea. [73]

[73] Отчет Комиссии по никелю Онтарио, 1917 г., стр. 253.

Компания La Société le Nickel находилась под контролем французских Ротшильдов во время открытия месторождений в Садбери. Г-н Ф. Э. Мерри, английский металлург, в своих показаниях Комиссии по никелю Онтарио сообщил, что к началу войны немцы осуществляли контроль над этой компанией. Германская фирма Krupp также приобрела некоторую никелевую собственность в Новой Каледонии.

The International Nickel Co., второй по величине владелец никелевых земель в Новой Каледонии, является той же американской фирмой, которой принадлежит Canadian Copper Co.

Компания Les Hauts-Fourneaux de Noumea принадлежит, по крайней мере с начала войны, французским интересам.

По словам г-на Мерри, никелевые рудники и плавильные заводы Норвегии также находились преимущественно под контролем той же германской группы, которая получила контроль над Le Nickel. Она работала под названием «Metallgesellschaft». Один недавно открытый рудник и плавильный завод находились под английским контролем.

Никеленосные железные руды Кубы полностью принадлежат американским компаниям, главным образом сталелитейным, в частности Bethlehem Steel Co.

Все три компании, добывающие или готовящиеся к добыче никеля в районе Садбери, владеют собственными плавильными и рафинировочными заводами. International плавит свою руду в Канаде и рафинирует ее в Соединенных Штатах. У нее есть новый рафинировочный завод в Порт-Колборне, Онтарио. Mond Nickel Co., которая плавит руду в Канаде и рафинирует ее в Англии, запустила рафинировочный завод в Канаде. British-American Nickel Corporation построила в Канаде как плавильный, так и рафинировочный завод.

United States Nickel Co. управляет рафинировочным заводом в Нью-Брансуике, штат Нью-Джерси. Les Hauts-Fourneaux de Noumea и эта компания принадлежат одним и тем же интересам. У них есть плавильный завод в Нумеа, Новая Каледония, а также рафинировочный завод в Гавре, Франция.

La Société le Nickel имеет плавильный завод в Тио, Новая Каледония, и рафинировочные заводы в Гавре (Франция), а также в Эрдингтоне и Керкинтиллохе (Британские острова).

Ни один процесс рафинирования не доминирует в мировой никелевой промышленности. Две компании, производящие никель из руд Садбери, используют совершенно разные процессы рафинирования, которые они контролируют индивидуально; а компания British-America, которая вскоре начнет производство, будет использовать третий процесс — процесс Хибинетта, электролитический процесс, на который она имеет исключительные права в Северной Америке. Orford Copper Co., дочерняя компания International, использует так называемый «солевой» процесс, но также производит некоторое количество никеля электролитическим путем.

Процесс, используемый United States Nickel Co. в Нью-Брансуике, штат Нью-Джерси, заключающийся во флюсовании и восстановлении из штейна, произведенного на плавильном заводе в Нумеа, не пригоден для сульфидных руд, содержащих медь.

Руды, добываемые в Норвегии, плавятся и рафинируются в Норвегии по процессу Хибинетта.

Очевидно, что мировые ресурсы никеля контролируются несколькими компаниями. Главная из них — International Nickel Co., которая имеет крупнейшие активы в Садбери и вторые по величине активы в Новой Каледонии. Mond и British-America являются следующими по значимости, а La Société le Nickel занимает четвертое место. E. J. Longyear Co. и ее партнеры не стремятся стать производителями никеля и готовы продать свои активы. Чтобы новая компания добилась успеха, ей пришлось бы разработать собственный процесс рафинирования. Альтернативой было бы продать активы или объединиться с фирмой, контролирующей процесс рафинирования. В Америке нет давальческих плавильных или рафинировочных заводов. Компания Mond покупает руду Алексо, поскольку высокое содержание магния делает ее хорошим флюсующим материалом при плавке руд Садбери.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ ДЕРЖАВ

Соединенные Штаты.

— Хотя Соединенные Штаты обладают незначительными месторождениями никелевой руды и поэтому практически не осуществляют политического контроля над добычей никеля, американский капитал играет важную, если не ведущую роль в этой отрасли. Из четырех компаний, владеющих месторождениями в районе Садбери, две являются американскими, и именно они обладают, несомненно, крупнейшими запасами в этом районе. Одна из них, International Nickel Co., имеет вторые по величине активы в Новой Каледонии.

Великобритания.

— Из всех стран Великобритания занимает наиболее сильную политическую позицию в отношении никелевой промышленности, поскольку район Садбери находится в Канаде. Она использовала этот контроль в стремлении локализовать бизнес по рафинированию никелевых руд Онтарио в Канаде, в результате чего International Nickel Co. переносит свои операции по рафинированию из Нью-Джерси на свой новый рафинировочный завод в Онтарио.

В коммерческом отношении британский капитал контролирует две другие компании, имеющие активы в Садбери. В одной из них — British-America Nickel Corporation — правительство само имеет контрольный пакет акций.

Политика британского правительства в отношении никелевых руд Садбери, которые обеспечивают британцам подавляющий политический контроль над мировым никелем, весьма показательна, поскольку демонстрирует, что правительство осознает необходимость как коммерческого, так и политического контроля, чтобы извлечь все коммерческие и стратегические преимущества из своей удачи. Во время войны, еще до вступления в нее Соединенных Штатов, в Канаде и Англии вызвало большое возмущение то, что германская подводная лодка «Deutschland» загрузила в Нью-Йорке груз, частично состоящий из металлического никеля, при этом предполагалось, что это изначально был канадский никель. Прямое участие британского правительства в промышленности Садбери, сделавшее правительство практически доминирующим фактором, а также перенос операций по рафинированию американской компании International Nickel Co. из Нью-Джерси в Онтарио знаменуют собой энергичную и агрессивную националистическую политику, которая достигла своей цели без особых промедлений.

Франция.

— Франция владеет островом Новая Каледония и осуществляет политический контроль над находящимися там никелевыми месторождениями. Две из трех основных компаний, владеющих месторождениями руды в Новой Каледонии, предположительно находятся под контролем французских интересов. Более крупная из них, La Société le Nickel, долгое время контролировалась французскими Ротшильдами. Позже сообщалось, что она перешла в руки немцев.

Германия.

— Германия не осуществляет политического контроля ни над какими важными никелевыми месторождениями. До войны германская фирма Krupp приобрела некоторые никелевые активы в Новой Каледонии. Сообщается, что германская группа Metallgesellschaft к началу войны контролировала La Société le Nickel, а также рудники и плавильные заводы Норвегии.

ГЛАВА VII ВОЛЬФРАМ Фрэнк Л. Хесс

ПРИМЕНЕНИЕ ВОЛЬФРАМА [74]

[74] Если не указано иное, в этой главе используется короткая тонна (2000 фунтов), а под «вольфрамовой рудой» понимаются материалы, содержащие 60 процентов WO3.

Основными направлениями использования вольфрама являются: легирующая добавка в быстрорежущую инструментальную сталь, изготовление нитей накаливания для ламп, мишени и катоды для рентгеновских трубок, а также электрические контакты для двигателей внутреннего сгорания или любых устройств, где требуется прерывистый электрический контакт. Другие области применения включают пилы и некоторые другие виды стали, в качестве компонента стеллита, в вольфрамо-железном сплаве для клапанов автомобильных и авиационных двигателей, для кенотронов и аналогичных приборов, в марганцево-хромо-вольфрамо-железном сплаве для волочильных матриц, в проволочной сетке, люминесцентных экранах для рентгеновских лучей, протравах и других химических веществах.

Заменители.

— Использование вольфрама в быстрорежущих сталях является таким же стандартом, как использование дрожжей в хлебе, и, несмотря на усердные поиски, неизвестно ни одного заменителя, который мог бы удовлетворительно его заменить. Согласно сообщениям, в Англии и Франции молибден использовался для замены около половины вольфрама в некоторых быстрорежущих инструментальных сталях, но это, по-видимому, не является предпочтительным методом и применяется только тогда, когда получение вольфрама затруднено. В Соединенных Штатах эта практика нашла мало сторонников. Следующая цитата из Mining Journal (Лондон) от 25 мая 1918 г., стр. 318, показывает, что эти настроения не чужды и за рубежом:

Производство ферромолибдена, как сообщается, было начато в Швеции, где нехватка ферровольфрама вынудила использовать этот заменитель.

В течение 1917 года 104 (метрические?) тонны молибденита были отправлены из Норвегии в Германию, где, вероятно, использовались так же, как в Швеции. Генри Э. Вуд сообщил об обнаружении молибдена в стали германской каски. Когда в начале 1916 года цена на вольфрам была чрезмерно высокой, было проведено множество экспериментов по поиску заменителя, но, по-видимому, без полного успеха, хотя в последнее время на рынок было выпущено несколько сталей-заменителей, содержащих кобальт и хром, специально предназначенных для литых фрез и других многолезвийных инструментов, а также были предложены кобальт-хромо-молибденовая сталь и урановая сталь для токарных инструментов. Стеллит, кобальт-хромо-вольфрамовый сплав, в котором содержится лишь от одной трети до половины того количества вольфрама, что используется в быстрорежущей стали, стал более популярным, а коперит, никель-циркониевый сплав, также является конкурентом, но торговля этим списком заменителей не оказала заметного влияния на спрос на вольфрамовые стали.

Изменение способа использования вольфрамовой стали, при котором тонкая пластина быстрорежущей стали припаивается к более обычной стальной полосе для формирования режущей кромки токарного инструмента, сделало спрос на вольфрам меньшим, чем он был бы при соблюдении старой практики изготовления всего инструмента из быстрорежущей стали.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

О каких-либо поразительных изменениях в металлургии вольфрама не известно, но наблюдается постоянное совершенствование технологии, улучшение качества ферровольфрама, смещение мест восстановления и значительное изменение способов использования. Расточительный, небрежный спрос на руды высокой концентрации и большой чистоты, обычный до войны, уступил место более просвещенной и разумной практике, вплоть до того, что фирмы как в этой стране, так и в Англии специализируются на использовании низкосортных или нечистых руд, хотя, по-видимому, здесь прогресс был гораздо значительнее, чем за рубежом. Одна фирма, Chemical Products Co. (Вашингтон, округ Колумбия), была организована специально для покупки руд, содержащих менее 60 процентов триоксида вольфрама (WO3), требуемых другими американскими фирмами, а также руд, содержащих серу, медь, мышьяк, висмут, олово, сурьму, фосфор или другие примеси, против которых возражало большинство потребителей. Две фирмы, Black Metal Reduction Co. и Tungsten Products Co., обе из Боулдера, штат Колорадо, были организованы для обработки таких материалов, как хвосты, содержащие всего 1 процент триоксида вольфрама, и они заявили, что способны оплачивать золото и серебро в руде.

Несколько фирм производят триоксид вольфрама или вольфрамовую кислоту (H2WO4) для производителей ферровольфрама. Фирмы также производили искусственный шеелит (CaWO4) для той же отрасли, используя в процессе руды низкого качества. Порошкообразный ферровольфрам, получаемый путем химического осаждения железо-вольфрамовой соли из раствора и восстановления ее до металлического порошка, содержащего от 4 до 11 процентов железа, производился несколькими фирмами и, по-видимому, создал спрос на порошкообразный ферровольфрам, поэтому фирмы теперь мелко измельчают массивный ферровольфрам. Также заявляется о более совершенной работе печей, что значительно снижает потребление тока и обеспечивает извлечение 90–96 процентов вместо обычных 80 процентов. Несколько фирм производят ферровольфрамовый порошок и вольфрамовый порошок в железных трубах или других железных контейнерах вместо графитовых тиглей, использовавшихся до войны.

При обогащении вольфрамовых руд в этой стране наблюдается тенденция к отказу от неэкономичного метода получения концентратов с очень высоким содержанием триоксида вольфрама (более 60 процентов WO3). Мало кто из операторов действительно знает, каково содержание в исходном сырье, и определение потерь — это лишь догадки. Некоторые из наиболее осторожных операторов на месторождении Боулдер перед закрытием в начале 1919 года производили высококачественный продукт с содержанием ближе к 50 процентам, чем к 60 процентам триоксида вольфрама, и низкосортный продукт с содержанием около 20 процентов триоксида вольфрама, не пытаясь повысить его содержание. Эта практика значительно сокращает потери. Когда в 1916 году возник острый дефицит вольфрамовой руды, потребители были вынуждены принимать концентраты более низкого качества, и некоторые соответственно улучшили свою металлургию. Это изменение облегчило продажу 50-процентных концентратов. Даже в Англии принимались руды с содержанием 60–65 процентов, тогда как ранее требовалось содержание 67,5 или 70 процентов WO3.

Раньше шеелит продавался на 50 центов за единицу дешевле других вольфрамовых минералов, даже несмотря на отсутствие вредных примесей, но с переходом от кустарных методов к более вдумчивой, тщательной и научной практике он стал продаваться с премией. Гюбнерит, по-видимому, до сих пор продается в Англии вместе с «вольфрамитом» и как «вольфрамит», но в этой стране он должен продаваться в соответствии со своим составом, поскольку для большинства металлургов марганец нежелателен, хотя по крайней мере одна фирма сейчас производит ферровольфрам из гюбнерита без каких-либо предубеждений или трудностей. Этот рост знаний и техники привел к тому, что цены на вольфрамовые минералы расположились примерно в следующем порядке: шеелит, ферберит, вольфрамит и гюбнерит. Это относится к вольфраму, используемому в производстве вольфрама и ферровольфрама для сталелитейной промышленности. Шеелит в этой стране не востребован для производства нитей накаливания.

До войны Соединенные Штаты импортировали значительные количества германского ферровольфрама, но металлурги утверждают, что ферровольфрам, производимый сейчас в этой стране, превосходит любой германский. В настоящее время, конечно, германская экспортная торговля мертва. Англия, ранее являвшаяся мелким производителем, теперь производит большие количества ферровольфрама и вольфрамового порошка на ряде заводов. Один из производителей, High Speed Steel Alloys, Ltd., Уиднес, недалеко от Ливерпуля, «находится под государственной поддержкой и принадлежит 31 ведущему потребителю Шеффилда». [75] В процитированной статье говорилось, что объем производства составлял 500 тонн вольфрама в год. Thermo-Electric Ore Reduction Corporation, [76] Лутон, в то же время производила 140 тонн вольфрама в месяц. Произведенный ферросплав содержал 80 процентов, а порошок — 98 процентов металлического вольфрама. Только одна компания в Соединенных Штатах производила до 60 тонн вольфрама в месяц в тот же военный период. Thermo Electric Ore Reduction Corporation владела рудниками, на которых рассчитывала ежегодно добывать 4000 длинных тонн концентратов, содержащих 65 процентов оксида вольфрама. В Англии есть по меньшей мере семь других производителей вольфрама или ферровольфрама.

[75] Mining Journal, Лондон. «High Speed Steel Alloys, Ltd., Посещение заводов с инспекцией», том 115, 25 ноября 1916 г., стр. 779.

Джулиус Л. Ф. Фогель впоследствии написал статью (Min. Jour., Лондон, том 20, стр. 16, янв. 1919 г.), в которой говорит, что государственная помощь, хотя и предлагалась, не была принята. Это заявление подтверждает государственную политику.

[76] Mining Journal. «Thermo-Electric Ore Reduction Corporation, Ltd., Посещение заводов в Лутоне», том 115, стр. 797, 2 декабря 1916 г.

Во Франции до войны было несколько заводов по производству ферровольфрама, и считается, что они все еще работают.

В начале войны около половины вольфрама, используемого в Соединенных Штатах, вводилось в сталь в виде ферровольфрама и около половины — в виде вольфрамового порошка. Эта практика изменилась, так что теперь более трех четвертей используемого вольфрама вводится в виде ферровольфрама, в основном, по-видимому, из-за того, что ферросплав теперь производится в более чистой форме, а отчасти из-за того, что вольфрамовый порошок некоторое время было невозможно получить. Одно время вольфрамовые руды добавляли в шихту, и вольфрам легировался непосредственно со сталью; фактически, вольфрамовые стали впервые были изготовлены именно таким способом, хотя этот процесс был запатентован в этой стране как новый. От этой практики, по-видимому, отказались из-за попадания в сталь примесей, которые могут быть удалены при предварительном производстве вольфрама или ферровольфрама.

В производстве вольфрамовых сталей произошло значительное изменение благодаря расширению использования электропечей. Один крупный производитель, Latrobe Electric Steel Co., производит всю свою быстрорежущую инструментальную сталь таким способом. Vanadium Alloys Steel Co., один из крупных производителей, производит большую часть своей стали в электропечи, и считается, что Crucible Steel Co. и некоторые другие сталелитейные компании производят часть или всю свою сталь таким образом.

Удаление олова, меди и других примесей из ферровольфрама путем измельчения и химической обработки позволило использовать нечистые руды при производстве высококачественного ферровольфрама в электропечи.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Вольфрам, даже в большей степени, чем олово, встречается почти исключительно в гранитных породах. В некоторых местах вольфрамовые руды встречаются в вулканических, осадочных или метаморфических породах, но, как постулируется в отношении некоторых оловянных месторождений, многие из этих месторождений можно объяснить предположением, что они находятся недалеко по вертикали над подстилающим гранитом.

Среди самих месторождений существует значительное разнообразие типов, и их можно классифицировать следующим образом: сегрегационные месторождения, пегматитовые жилы, жилы, месторождения замещения, контактово-метасоматические месторождения и россыпи.

Сегрегационные месторождения немногочисленны и не имеют большого значения; они представляют собой месторождения, в которых вольфрамит сегрегирован в граните, подобно биотиту или роговой обманке. Близким типом является присутствие вольфрамовых минералов в аплитовом граните, и это почти незаметно переходит во второй тип — пегматиты.

Пегматиты также имеют сравнительно небольшое значение, но дают определенные количества вольфрамовых минералов. Пегматиты также переходят в следующий тип — жилы, которые до сих пор давали большую часть вольфрамовых минералов в мире. Тесно связаны с жилами четвертый тип — месторождения замещения, в которых вмещающие породы вдоль жил, хотя жилы могут быть очень маленькими, замещаются различными минералами, включая вольфрамовые. Единственными известными крупными примерами являются месторождения вольфрамита близ Лида, Южная Дакота, которые были значительными производителями при высоких ценах Великой войны.

Среди месторождений замещения следует отметить также такие месторождения, как в горах Дип-Крик, Юта, где растворы, следовавшие по трещинам в монцоните, заместили породу массой полевого шпата, кварца, турмалина, апатита, шеелита, вольфрамита (очень мало), висмута, меди и молибденовых минералов, которые при других условиях без колебаний были бы названы пегматитом.

Тесно связаны с месторождениями замещения контактово-метасоматические месторождения, пятый тип. Они лишь недавно начали приобретать коммерческое значение, но обещают стать одними из крупнейших, если не самыми крупными производителями в этой стране и, возможно, в других странах. Они относятся к известному типу — известняки или известковые породы, которые были прорваны гранитами, принесшими большие количества водных или газообразных растворов кремния, железа, алюминия и магния, с меньшим содержанием хлора, фтора, калия и серы, и, в данном случае, вольфрама. В Большом Бассейне обширные площади известняков, простирающиеся от северо-западной Юты до Сьерра-Невады и вокруг их южной оконечности, были таким образом прорваны и метаморфизованы. Некоторые крупные месторождения шеелита уже эксплуатировались в этом регионе, а другие еще предстоит разрабатывать. Подобные месторождения встречаются в Корее, Японии и Тасмании и, вероятно, существуют, хотя еще не открыты, в Китае, на Малайском полуострове и в других странах. Вольфрамовым минералом в таких месторождениях неизменно является шеелит.

Россыпи, шестой тип, образуются из всех видов месторождений, но их ценность во многом зависит от местных условий. Они являются как остаточными, так и аллювиальными месторождениями и были крупными производителями вольфрамовых минералов, особенно вольфрамита. Очень большая доля бирманской добычи приходилась на полу-остаточные и речные россыпи, а китайская добыча в 1918 году, самая большая из когда-либо произведенных любой страной за один год, почти полностью велась из россыпей.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Распространение вольфрамовых руд далеко не так широко, как распространение гранитных пород, и некоторые регионы с большими площадями гранита почти не имеют вольфрамовых минералов. Среди таких регионов — Скандинавский полуостров, обширные территории Канады, восточная часть Соединенных Штатов и Бразилия.

Известные крупные вольфрамовые месторождения мира сгруппированы вдоль берегов Тихого океана — не всегда близко к нему, но где-то в великих горных массивах, параллельных его окраине, причем западный берег гораздо богаче восточного. В 1918 году 92 процента мирового вольфрама поступало с берегов Тихого океана, 61 процент — из Азии, Австралии и Океании, и 31 процент — из Северной и Южной Америки. Только Восточная Азия дала 56 процентов. Существует только один значительный вольфрамоносный район, не расположенный близ Тихого океана, — это Иберийский полуостров, в основном в Португалии, но частично в Испании. Из менее чем 8 процентов, произведенных не вокруг Тихого океана, этот район дал почти 5 процентов. Конечно, есть небольшие месторождения в Англии, Германии и других местах вблизи Атлантического океана, но вместе они производят менее 3 процентов мировых вольфрамовых руд. Огромный континент Африка имеет лишь незначительные известные месторождения; никаких существенных месторождений не найдено на границах Арктического, Антарктического или Индийского океанов, за исключением узкого Малайского полуострова, разделяющего Индийский и Тихий океаны, и лишь незначительные месторождения известны в Сибири.

Рассматриваемый как единая металлогеническая провинция, регион, обеспечивающий наибольшую добычу, находится в Юго-Восточной Азии; он включает Малайский полуостров, Бирму, Шанские государства, Сиам, Тонкин и Юго-Восточный Китай. Второй по величине производящей металлогенической провинцией является Кордильерская, включающая Боливию и прилегающие тесно связанные районы Перу, Аргентины и Чили, за которыми следуют Соединенные Штаты и Мексика. [77] Португалия, Испания и Италия образуют четвертую провинцию, к которой тесно примыкают корнуоллско-французские производящие районы. Австралия, включая Тасманию, является следующей по значимости и представляет собой отдельную провинцию, практически все руды которой находятся в хребтах восточной части континента. Япония и Корея также образуют довольно четкую провинцию, которая может продолжаться в Маньчжурию. Мексика, как было указано, должна быть включена в ту же провинцию, что и западные Соединенные Штаты. Существует множество небольших, более или менее изолированных районов, таких как Коннектикут, Новая Шотландия, Манитоба и т. д., которые в настоящее время не имеют большого значения и не дают никаких обещаний будущего величия.

[77] Можно вполне справедливо возразить, что идея металлогенической провинции значительно растянута, чтобы включить месторождения Боулдера и Блэк-Хилс вместе с месторождениями юго-западных штатов и Мексики, но для удобства они здесь сгруппированы таким образом — с откровенным признанием допущенной вольности.

ПРОИЗВОДСТВО ПО СТРАНАМ

Мировое производство вольфрамовых руд по металлогеническим провинциям и политическим территориям показано в следующей таблице:

Таблица 28. — Мировое производство вольфрамовой руды, 1913–1918 гг., по металлогеническим провинциям и политическим территориям [78] В коротких тоннах (2000 фунтов) концентратов, содержащих 60 процентов WO3.

Province and area | 1913 | 1914 | 1915 | 1916 | 1917 | 1918
Africa |  |  |  |  |  |
South African province: |  |  |  |  |  |
Rhodesia | 4 | ... | ... | 2 | 12 | 37
Union of South Africa | ... | ... | ... | 1 | 9 | 19
| 4 | ... | ... | 3 | 21 | 56
Asia |  |  |  |  |  |
Chino-Malayan province: |  |  |  |  |  |
Burma | 1,891 | 2,605 | 2,963 | 4,166 | 5,018 | 4,919
China | ... | ... | ... | [79]120 | [79][80]1,500 | [80]11,662
Dutch East Indies (Billiton and Singkep) | 7 | 1 | 7 | 52 | [81]61 | [81]61
Federated Malay States | [80]252 | [80]292 | [80]326 | 578 | 794 | 398
French Indo-China (Tonkin) | [80]101 | 119 | 220 | 183 | 422 | [82]450
Siam | ... | 301 | 475 | 584 | 800 | [82]800
Unfederated Malay States: |  |  |  |  |  |
Johore[80] | ... | ... | 2 | 25 | 2 | 1
Kedah | 32 | 27 | 14 | 19 | 139 | 582
Trengganu[80] | 94 | 160 | 161 | 303 | 225 | 691
Indian province: |  |  |  |  |  |
India (excluding Burma) | ... | ... | ... | 47 | 69 | 45
Japo-Korean province: |  |  |  |  |  |
Chosen (Korea) | ... | ... | 74 | 613 | 992 | [82]1,102
Japan | 272 | 215 | 411 | 770 | 808 | [79]651
| 2,649 | 3,720 | 4,653 | 7,460 | 10,830 | 21,362
Australia |  |  |  |  |  |
Australian province: |  |  |  |  |  |
New South Wales | [80]191 | [80]220 | [80]93 | [80]296 | [80]274 | [79]325
Northern Territory[79] | 217 | 159 | 366 | 401 | 427 | 614
Queensland | 402 | 270 | 468 | 415 | 406 | 298
South Australia | ... | ... | ... | 1 | ... | ...
Tasmania | 76 | 53 | 106 | 119 | 270 | 416
Victoria | 1 | ... | 16 | 1 | 25 | 4
Western Australia[80] | 1 | 1 | ... | 4 | 1 | 5
| 888 | 703 | 1,049 | 1,237 | 1,403 | 1,662
Europe |  |  |  |  |  |
Erzgebirgan province: |  |  |  |  |  |
Austria | 57 | 62 | [82]75 | [82]150 | [82]150 | [82]150
Germany | [80]318 | [82]100 | [82]150 | [82]351 | [82]200 | [82]200
Franco-Cornish province: |  |  |  |  |  |
England | 204 | 229 | 370 | 441 | 270 | 338
France | 301 | [82]200 | [82]200 | [81]182 | [81]182 | [81]182
Iberian province: |  |  |  |  |  |
Italy | ... | ... | ... | 9 | 1 | ...
Portugal | 1,241 | 735 | 1,029 | 1,563 | 1,742 | [82]1,300
Spain | 186 | 149 | 208 | 468 | 491 | 4,741
Russian province: |  |  |  |  |  |
Russia | ... | ... | ... | 36 | [79]108 | [82]150
Scandinavian province: |  |  |  |  |  |
Norway | 3 | 4 | ... | 1 | [82]10 | [82]10
| 2,310 | 1,479 | 2,032 | 3,201 | 3,154 | 7,071
North America |  |  |  |  |  |
American province: |  |  |  |  |  |
Alaska | ... | ... | ([83]) | 47 | 32 | 12
United States | 1,537 | 990 | 2,332 | 5,876 | 6,112 | 5,056
Canadian province: |  |  |  |  |  |
Southeastern Canada | ... | ... | ... | ... | ... | 13
Southwestern province: |  |  |  |  |  |
Mexico | ... | ... | ... | 13 | 207 | 165
| 1,537 | 990 | 2,332 | 5,936 | 6,351 | 5,246
Oceania |  |  |  |  |  |
Oceanic province: |  |  |  |  |  |
New Zealand[80] | 248 | 228 | 217 | 298 | 181 | 190
South America |  |  |  |  |  |
Brazilian province: |  |  |  |  |  |
Brazil | ... | ... | ... | [80]7 | ... | ...
Cordilleran province: |  |  |  |  |  |
Argentina[80] | 679 | 499 | 201 | 963 | 1,251 | 724
Bolivia[80] | 339 | 330 | 947 | 3,624 | 4,646 | 4,082
Chile | ... | ... | 10 | 2 | ... | ...
Peru | 357 | 235 | 455 | 587 | 471 | 295
| 1,375 | 1,064 | 1,613 | 5,183 | 6,368 | 5,101
Total | 9,011 | 8,184 | 11,896 | 23,318 | 28,308 | 40,688

[78] Цифры, не сопровождающиеся ссылками на сноски, взяты из официальных источников или других достоверных публикаций. Во всех случаях исходные количества были приведены к эквиваленту в концентратах, содержащих 60 процентов WO3.

[79] Цифры частично официальные, частично оценены Геологической службой США.

[80] Экспорт.

[81] Цифры оценены союзниками, когда предлагалось распределить вольфрамовые руды мира между собой.

[82] Цифры оценены Геологической службой США.

[83] Менее половины тонны.

РАЗВИТИЕ И ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРОСТРАНЕНИИ В БЛИЖАЙШЕМ БУДУЩЕМ

Азия.

— Рост добычи в Восточной Азии был поразительным. В 1913 году он составлял 2497 тонн, а в 1918 году, как уже говорилось, 20 228 тонн — более 56 процентов мирового производства. Как и везде, производство должно снизиться, пока не будут использованы накопленные запасы в центрах переработки, затем производство снова возобновится. Аллювиальные месторождения Китая отнюдь не исчерпаны, жилы едва затронуты, вольфрамоносная площадь велика и лишь частично разведана, а та разведка, которая была проведена, велась почти исключительно на россыпи; рабочая сила дешева, и большой будущий объем производства обеспечен. Более либеральные идеи торговли и управления постепенно укореняются в Китае, и в конечном итоге образованные китайцы или подготовленные иностранцы будут разрабатывать месторождения; объем производства в течение долгого времени будет большим, хотя, возможно, он никогда больше не будет таким большим, как в 1918 году.

Насколько можно судить, легко разрабатываемые россыпи и верхние части жил в Бирме довольно быстро истощаются, [84] и поэтому приходится все больше прибегать к добыче тех частей жил, которые находятся ниже уровня грунтовых вод и в более твердых породах, а это, вероятно, будет означать уменьшение, а не увеличение объема производства. Сиам, по-видимому, должен дать увеличение производства, так как рудники сравнительно новые, и еще должны быть возможности для открытий. Федеративные Малайские Штаты и нефедеративные штаты (Джохор, Кедах и Тренгану) должны производить в ближайшем будущем по крайней мере столько же, сколько в прошлом — при наличии спроса и равной цены.

[84] Торговая палата Бирмы и Горная палата Тавоя, «Меморандум сэру Джорджу Барнсу», Mining Jour., Лондон, том 121, 1918, 4 мая, стр. 261.

Австралазия.

— Как и другие британские владения, Австралия работала в условиях препятствия в виде сравнительно низкой фиксированной цены на вольфрамовые руды во время войны. Эта цена, сначала 55 шиллингов за единицу длинной тонны c.i.f. Лондон, позже была повышена до 60 шиллингов. В течение первой части войны цена, выплачиваемая в Австралии, составляла в среднем менее половины цены, выплачиваемой в Соединенных Штатах, и лишь немногим более половины той, что выплачивалась в регионах, отличных от британских провинций. В результате австралийская добыча вольфрама не увеличилась во время войны так, как могла бы, если бы цены были выше. Сливки известных месторождений сняты, за исключением Тасмании, где контактово-метасоматические месторождения на острове Кинг увеличили тасманийскую добычу в четыре раза. Вольфрамовые минералы, добываемые в Австралии, — это в основном вольфрамит с меньшими количествами гюбнерита и шеелита. Гюбнерит, по-видимому, редко признается таковым на британском рынке, а весь продается как вольфрамит. За исключением контактово-метасоматических месторождений на острове Кинг, Тасмания, разрабатываемые месторождения — это в основном жилы, с некоторыми пегматитами.

В Новой Зеландии производство — это исключительно шеелит; оно значительно увеличилось во время войны до последнего года — 1918-го, когда, по-видимому, из-за нехватки квалифицированной рабочей силы, оно упало до самого низкого уровня с 1909 года. Вероятнее всего, в настоящее время произойдет остановка производства.

Южная Америка.

— В Боливии рост производства был значительным. Месторождения, по-видимому, представляют собой исключительно жилы и производные россыпи. Жилы тесно связаны с оловянными месторождениями, и во многих жилах олово и вольфрам ассоциированы, но многие вольфрамовые месторождения содержат мало олова или не содержат его вовсе. Добываемые вольфрамовые минералы — это ферберит, вольфрамит, шеелит и немного гюбнерита. В некоторых жилах минералы смешаны, а в других — полностью разделены. Рудники находятся в восточной Кордильере Анд и по обе ее стороны на протяжении почти 400 миль от точки близ Пуэрта-Акоста на северо-западе до Чорольке на юго-востоке. Расходы на добычу во время войны значительно выросли в связи с ростом цен в других частях мира. Заработная плата не достигла больших высот, но стоимость материалов значительно возросла. Транспортные условия всегда плохи в большей части Боливии и сильно увеличивают расходы. Из-за обстоятельств объем производства чрезвычайно чувствителен к снижению спроса или цен, и поэтому он быстро упал после перемирия, но если высокие цены вернутся, он, вероятно, снова быстро вырастет. Некоторые современные заводы были установлены на рудниках до или как раз когда было подписано перемирие, и когда мировые запасы вольфрама будут использованы и снова появится спрос, некоторое количество руды будет производиться даже при цене менее 10 долларов за единицу, хотя средняя стоимость, по-видимому, составляет около 12 долларов за единицу на руднике. [85]

[85] Хазелтайн, Росс, консул Соединенных Штатов, Ла-Пас. Отчет от 14 мая 1919 г.

Добыча в Перу, как она ведется сейчас, по-видимому, зависит от высоких цен, и при таких ценах могла бы, вероятно, оставаться на уровне 1916 года в течение нескольких лет. Месторождения Уаура, как сообщается, велики, хотя и низкосортны, и при надлежащем управлении могут давать много руды даже при более низких ценах. Во время войны они находились под контролем германских фирм и, вероятно, остаются таковыми до сих пор.

Северная Америка.

— До 1911 года Соединенные Штаты были ведущей страной по производству вольфрама, но в том году их обогнала Бирма, которая удерживала лидерство до 1916 года, когда Соединенные Штаты снова стали основным добытчиком вольфрамовой руды. В 1918 году Китай вышел на рынок с чрезмерно высокими ценами с объемом производства, который превысил почти на 1000 тонн мировое производство любого года до 1915-го. Северная Америка увеличила объем производства с 1549 тонн в 1913 году до 6512 тонн в 1917 году, но откатилась почти на 1000 тонн (до 5406 тонн) в 1918 году. В Соединенных Штатах снижение производства было вызвано почти исключительно падением цены и лишь частично истощением месторождений. На вольфрамовом месторождении Боулдер, штат Колорадо, некоторые из лучших рудных тел отработаны, и стоимость добычи значительно возросла из-за обеднения других, и то же самое верно для некоторых других мест, но кажется возможным, что в стране в целом производство может быть доведено примерно до уровня, который был раньше, при условии столь же высоких цен, благодаря открытию контактово-метасоматических месторождений Большого Бассейна.

В Мексике вольфрамовые месторождения, по-видимому, являются продолжением месторождений южной Аризоны. Насколько известно, все мексиканские месторождения содержат шеелит, местами частично замещенный купротунгститом. Известные разрабатываемые месторождения в районе Сахуарипа в Соноре описываются как жилы, содержащие шеелит с медными минералами, и пегматитовая жила, в которой находятся крупные массы шеелита и молибденита.

Европа.

— Европейское производство увеличилось примерно на 50 процентов в период между 1913 и 1918 годами, в основном в Португалии, и объем добычи вольфрамовых руд в Португалии, по-видимому, не достиг своего максимума. Эксплуатировались как россыпи, так и жилы, и, по-видимому, есть россыпной материал, который еще предстоит разрабатывать, а также жилы, которые, как говорят, далеки от истощения. Официальная статистика производства, представленная Португалией в течение большей части войны, объявляется инженерами, знакомыми с ситуацией, слишком заниженной из-за того, что руда контрабандой вывозилась в Испанию и на суда, направляющиеся в Англию. С другой стороны, в 1918 году Англия и Франция возражали против поставок португальской руды в Соединенные Штаты, но не хотели платить эквивалентные цены. Поэтому португальское правительство издало приказ, запрещающий экспорт вольфрамовой руды, за исключением фиксированных цен, приближающихся к текущим американским ценам. Американские владельцы не могли успешно разрабатывать свои рудники в условиях британско-французского эмбарго, в результате чего объем производства был, вероятно, намного меньше, чем в 1917 году. Несмотря на неопределенность, официальные оценки использовались, насколько они доступны, так как лучших цифр нет под рукой.

Что касается испанской добычи, то предсказания затруднены, поскольку данные о рудниках скудны. Кажется вероятным, что при аналогичных ценах от английских и французских месторождений можно ожидать примерно такого же объема производства, как в прошлом. Английская добыча уменьшилась в 1917 году и увеличилась лишь немного в 1918 году. Точных данных из Франции нет. Германские и австрийские месторождения, вероятно, эксплуатировались так интенсивно во время Мировой войны, что от них следует ожидать меньшего, чем они производили до сих пор.

Резюме.

— Основными изменениями в распределении производства в течение следующих нескольких лет, по-видимому, будут: дальнейшее развитие в Корее; возможное развитие в Маньчжурии; развитие месторождений в Южном Китае и Сиаме; дальнейшее развитие в Боливии; тенденция в Соединенных Штатах к значительному увеличению производства из месторождений Большого Бассейна; и развитие как жил, так и контактово-метасоматических месторождений в Мексике. Производство, возможно, снизится на месторождениях Атолия и Боулдер в Соединенных Штатах; а также в Австралии, Японии, Германии и Австрии.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Фактический контроль над мировыми месторождениями вольфрама значительно отличается от того, что указано производством в пределах политических территорий. Фактический контроль справедливо достигается посредством обычной конкурентной покупки, владения месторождениями гражданами (иногда правительствами) и посредством коммерческого союза. Контроль через владение банками и транспортными линиями может быть справедливым, а может осуществляться путем принуждения и коммерческого бандитизма, захвата портов для угольных и ремонтных станций — методы, которые являются лишь усовершенствованиями, развившимися со времен, когда «Они искали свои состояния за границей как им было угодно, корона не беспокоила их никакими запросами, чтобы смутить их поиск испанских кораблей с сокровищами или их торговлю пиратским полотном и шелками». [86]

[86] Вильсон, Вудро. «История американского народа», том 1, стр. 25.

Table 29.—Actual Control of the World’s Tungsten Output in 1917 and 1918.
In Short Tons of 2,000 Pounds

| 1917 | 1918

Quantity
Percent-
age of
world’s
output
Quantity
Percent-
age of
world’s
output

British: |  |  |  |
Possessions |  |  |  |
Burma and Shan States |  4,600 |  |  4,870 |  |
Federated Malay States |    853 |  |    920 |
Trengganu |    350 |  |    350 |
Johore and Kedah |    200 |  |    582 |
India |     75 |  |     46 |
Australia |  1,404 |  |  1,662 |
New Zealand |    241 |  |    146 |
England |    265 |  |    330 |
South Africa |     24 |  |     37 |
|  8,012 | 28.4 |  8,943 |  | 24.9
Obtained through trade and political pressure |  |  |  |
Japan and Korea (including ores for France) |    790 |  | None |  |
China and Hongkong (including ores for France) |  1,105 |  |    900 |
Siam |    600 |  |    600 |
Billiton and Singkep |     60 |  |     60 |
Argentina |  | - | (including ores for France) |  2,035 |  |    950 |
Bolivia
Peru
Portugal |    960 |  |    800 |
Spain (including ores for France) |    446 |  |    425 |
|  5,996 | 21.3 |  3,735 |  | 10.4
Total ores under British control | 14,008 | 49.7 | 12,678 | 35.3
French: |  |  |  |
France |    182 |  |    180 |  |
Tonkin |    422 |  |    450 |
Siam |    170 |  |    190 |
Portugal |    650 |  |    440 |
Bolivia (See Great Britain) | ? |  | ? |
Argentina (See Great Britain) | ? |  | ? |
|  1,424 |  5.3 |  1,260 |  |  3.5
German: |  |  |  |  |
Germany |    200 |  |    200 |
Austria |    150 |  |    150 |
Norway | ? |  |  |
Portugal | ? |  | ? |
Spain | ? |  | ? |
|    350 |  1.2 |    350 |  |  1  
American: |  |  |  |
Mexico |    340 |  |    326 |  |
Peru |  | - |  |  4,320 |  |  4,680 |
Bolivia
Argentina
Japan and Korea (including some Chinese ore) |  1,010 |  |  1,650 |
China and Hongkong |    395 |  |  9,300 |
Portugal |    130 |  |     60 |
Siam |     30 |  |     12 |
Domestic production |  6,144 |  |  5,068 |
| 12,369 | 43.9 | 21,150 |  | 59  
Japanese: (Quantity smelted only) |  |  |  |
China | ? |  |    300 |  | - |  1.3
Norwegian: |  |  |
Norway |     10 |  |     10
Russian: |  |  |
Russia |    110 |  |    150
Total | 28,178 |  | 35,832 |  |

Из-за тесных отношений между некоторыми иностранными правительствами и частными фирмами — как это иллюстрируется интересом германского правительства к фирмам по производству красителей, калия и судоходным компаниям, а также участием британского правительства в компаниях по добыче никеля и производству ферровольфрама — не представляется возможным провести черту между государственными и частными месторождениями. В странах со слабыми правительствами месторождения, принадлежащие британским подданным, по всем намерениям и целям являются британскими; но иностранные месторождения, принадлежащие американцам, не обязательно находятся под американским контролем; на самом деле, вместо того чтобы помогать и поощрять наших пионеров во внешней торговле, мы склонны преследовать их и разрушать их бизнес драконовскими таможенными законами.

По сути, предыдущая таблица лишь показывает, куда направляются руды разных стран для обработки; это, конечно, только обобщение, так как торговые условия постоянно меняются. Например, японские электропечи начинают плавить вольфрамовые руды, хотя в настоящее время только в объеме от 10 до 15 тонн содержащегося вольфрама в месяц, но вполне вероятно, что объем производства может быть значительно увеличен. Хотя Япония могла бы контролировать распоряжение своей рудой, ей приписывается контроль только над ее плавлеными рудами. Точное распределение руд из Аргентины, Боливии, Перу, Португалии и Испании не может быть приведено.

Британский контроль.

— Во время войны британское правительство требовало и получало все вольфрамовые руды, производимые в его колониях и владениях. Это ограничение было позже снято в отношении Канады, и новое правило разрешило Канаде отправлять вольфрамовые руды другим странам Антанты, но поскольку Канада не была производителем, предоставленная лицензия ничего не значила, кроме как облегчение чувств канадцев. Однако в Манитобе были обнаружены месторождения шеелита, которые одно время казались потенциальными производителями. Номинально Сиам оставался свободным от британского контроля, поскольку находился в той или иной степени в зоне влияния французов, но в Бангкоке, по-видимому, оказывалось дипломатическое давление. Сиамские руды в основном содержат некоторое количество олова и отправлялись в Сингапур для разделения; и как только они попадали во владения британцев, конечно, их нельзя было экспортировать. Английский контроль над сиамскими поставками, однако, кажется таким же полным, как если бы руды поступали из английской провинции. Г-н Нассуэр из Siamese American Trading Co. дал показания перед Тарифной комиссией в Сан-Франциско 28 июня 1918 года, что его компания хотела отправить руду в Соединенные Штаты, но британский посланник в Сиаме не давал разрешения. Компания обратилась с этим вопросом в наш Государственный департамент и в конце концов получила разрешение на отправку 10 тонн.

В феврале 1918 года Chemical Products Co. из Вашингтона, округ Колумбия, выразила протест Государственному департаменту в Вашингтоне в связи с британским вмешательством в экспорт вольфрамовой руды из Сиама в Соединенные Штаты, заявив, что компания работает в условиях, специфичных для нее, поскольку использует дорогостоящий процесс, разработанный для обработки низкосортных руд, которые можно получить по гораздо более низкой цене, чем обычные сорта на рынке; что она заключила соглашение с американцем, разрабатывающим вольфрамовые рудники в Сиаме, о покупке его вольфрамовой руды, только чтобы обнаружить, что благодаря контролю над портовыми привилегиями в Сингапуре и Гонконге британцы эффективно запретили ей или любой другой американской фирме получать этот материал. Конечно, это, как и другие упомянутые инциденты, происходило в тени отчаянной войны, когда следовало ожидать строгости, но запрошенные поставки предназначались союзнику из страны, не находящейся открыто под контролем Великобритании. Несомненно, сейчас таких возражений не было бы, но инциденты показывают эффективность этих методов контроля над торговлей.

В Южном Китае, где Гонконг является портом для провинций Гуандун и Гуанси, а также частей южной части провинций Цзянси и Хунань, британцы некоторое время осуществляли контроль над экспортом руд, производимых в этих районах, [87] отказываясь разрешить переотправку руд, если они не были отправлены в Англию.

[87] Андерсон, Джордж Э.: Генеральный консул США, Гонконг, Китай. «Вольфрам из Южного Китая». Commerce Reports, 9 ноября 1917 г., стр. 546.

Иностранцам, включая, конечно, американцев, не разрешается владеть горнодобывающей собственностью в Бирме, Федеративных и нефедеративных Малайских Штатах или Австралии — на территории, производящей почти все вольфрамовые руды Британской империи.

В Аргентине небольшие вольфрамовые рудники принадлежат английским компаниям. [88]

[88] Шарп, Ралстон К.: «Вольфрамовые месторождения в Аргентине». Mining Magazine, Лондон, том 18, май 1918 г., стр. 230–233.

В Боливии английское и французское правительства во время войны арендовали рудники напрямую и вступили в прямую конкуренцию с американскими бизнесменами, занимающимися покупкой или добычей вольфрамовых руд.

Британские торговцы постоянно стремятся усилить свой контроль над боливийскими вольфрамовыми рудами. В настоящее время англичане, по-видимому, имеют полный контроль над финансовой системой Боливии, насколько это касается иностранной валюты. Американец, интересующийся вольфрамовым рудником в Боливии, сообщил автору, что почти невозможно вести дела с английскими банками, потому что они настаивают на том, что если они оказывают коммерческие услуги, даже за плату, получатель должен покупать только английское горнодобывающее оборудование. Вашгерд, который для обогащения вольфрамовой руды устарел в других странах, как говорят, до сих пор используется на боливийских фабриках под английским контролем. Если горняки не хотят иметь дело через английские банки, они вынуждены переводить деньги в Нью-Йорк и обратно с большими затратами. Американские банковские интересы, представленные в Боливии, по-видимому, консервативны в авансировании денег под поставки руды, тогда как германские и английские представители, как говорят, авансируют до 80 процентов рыночной стоимости отгружаемых руд. Горнодобывающие корпорации, контролируемые английскими фирмами, отправляют руду в Англию, и американцы не могут конкурировать за продукцию. Такой фирмой является Aramayo Francke Mines, Ltd., которая произвела 2050 длинных тонн оловянных концентратов, 226 тонн вольфрамитовых концентратов и значительное количество висмута за год, закончившийся 31 мая 1916 года. Контроль над боливийскими рудниками со стороны англичан пока не опасен для американских интересов, за исключением банковской системы, но полный контроль может перейти к ним, к немцам или французам через американское тарифное законодательство.

В Португалии английские компании контролируют ряд месторождений, и, как утверждают по меньшей мере два американца [89], английское правительство через своих представителей в Лиссабоне в течение более чем двух лет препятствовало переходу прав собственности к американским компаниям. Thermo Electric Ore Reduction Corporation, Ltd., по-видимому, является основным английским владельцем португальских вольфрамовых рудников.

[89] Личные сообщения.

В Голландской Ост-Индии, как считается, британцы контролируют текущую добычу вольфрамита в объеме около 5 тонн в месяц.

Французский контроль.

— Французский контроль над месторождениями вольфрама невелик. Он включает в себя добычу во Франции и Тонкине, часть добычи в Португалии и сравнительно небольшую долю в Боливии. Во время войны Англия и Франция пытались установить контроль в Португалии. Цены, предлагаемые англичанами и французами, были значительно ниже рыночных цен в Нью-Йорке, и португальское правительство вмешалось, подняв цены до уровня, несколько более низкого, чем в Соединенных Штатах, но на 20 процентов выше цен, предлагаемых Англией и Францией.

Японский контроль.

— Япония имеет в своих границах значительное количество месторождений вольфрама в южной части островов, но все они невелики. В Корее были обнаружены и активно разрабатываются важные месторождения, особенно в течение последних двух лет. Считается, что месторождения в Маньчжурии контролируются японцами; о них мало что известно, и если они существуют, то, вероятно, невелики. Японские руды в течение нескольких лет в значительной степени поступали в Соединенные Штаты. Как уже говорилось, японские фирмы построили электрические печи, в которых восстанавливается часть вольфрамовых руд, вероятно, эквивалентная 25–35 тоннам концентратов в месяц с содержанием 60 процентов WO3.

Американский контроль.

— Соединенные Штаты полностью контролируют месторождения вольфрама в своих границах и на Аляске. Американцы, работающие в Мексике, добывали от 200 до 300 коротких тонн шеелитовых концентратов в год на месторождениях в округе Сауарипа, Сонора. Говорят, что вольфрамит поставлялся из Синалоа в Соединенные Штаты, но его реальное происхождение неизвестно. Контактово-метаморфические месторождения примерно в 60 милях к юго-западу от Накозари содержат 0,7 процента WO3 и 1–2 процента меди. Они принадлежат американцам, но в настоящее время не разрабатываются.

В Боливии американцам принадлежат некоторые из наиболее важных вольфрамовых рудников. Американские фирмы, которые, как известно, владеют там вольфрамовыми объектами: W. R. Grace & Co. (местный адрес: Ла-Пас), Stewart, Wilson & Hepburn (Оруро), Easley Inslee (Ла-Пас) и C. Dillon (Оруро). Их общая добыча оценивается примерно в 1600 тонн из общего объема добычи в стране, превышающего 4000 тонн.

В Южном Китае американские фирмы в значительной степени развили торговлю вольфрамом, так что через этот источник Соединенные Штаты (или, скорее, американский капитал) контролируют, если им не препятствуют, годовой объем добычи, возможно, в 9000 коротких тонн вольфрамовых концентратов.

В Сиаме одна или две компании из Соединенных Штатов пытались добывать вольфрам, но английское влияние во время войны затруднило отправку даже небольших партий руды в эту страну.

Поскольку Соединенные Штаты предлагали более высокие цены, чем другие страны, и поскольку более прямой и короткий торговый путь делал торговлю с этой страной выгодной для японцев, в 1918 году США в значительной степени контролировали японскую добычу вольфрамовой руды. Эта торговля, вероятно, была несколько сокращена и будет еще больше уменьшена за счет строительства электрических печей в Японии. Приведенная ниже таблица показывает вольфрамовые руды, импортированные для потребления в Соединенные Штаты в 1918 году, но дает слабое представление о рудах, отгруженных из стран происхождения; китайские руды поступают с задержкой в три месяца, а южноамериканские — примерно в два месяца. В таблице указаны только руды, фактически полученные в течение года. Таблица 29 более точно показывает руды, отгруженные в Соединенные Штаты в течение года.

Считается, что китайские руды содержат в среднем 67,5 процента WO3, а другие руды — 65 процентов WO3.

Таблица 30. — Вольфрамсодержащие руды, импортированные в Соединенные Штаты в 1918 году, по странам, указанным в портах ввоза, и по вероятным странам происхождения.

As listed at ports | Probable origin and equivalent in 60 per cent. WO₃
Country | Quantity, short tons | Value | Country | Quantity, short tons | Value

Argentina
536
$
730,722
South America, including:
Argentina
Bolivia
Chile
Colombia
Costa Rica
Ecuador
Panama
Peru
Salvador
4,181
$
3,746,299

Bolivia | 88 | 122,357
Canada | 56 | 115,863
Chile | 1,251 | 1,209,864
China | 2,384 | 2,068,636
Colombia | 56 | 65,124
Costa Rica | 18 | 19,081

Ecuador
6
9,979
China, including:
Hongkong,
“Other British East Indies;”
also Canada
6,811

5,708,616

France | 29 | 3,400
Hongkong | 3,595 | 3,511,046
Japan | 1,361 | 1,700,332 | Japan | 1,474 | 1,700,332
Mexico | 264 | 224,247 | Mexico | 286 | 224,247
“Other British East Indies” | 19 | 13,071 | Portugal, including: France | 61 | 21,160
Panama | 37 | 40,614
Peru | 1,827 | 1,488,516 | Siam | 12 | 8,583
Portugal | 27 | 17,760
Salvador | 40 | 60,042 | Unaccounted for | 157 | 142,981
Siam | 11 | 8,583
Unaccounted for | 145 | 142,981
| 11,750 | $ | 11,552,218 |  | 12,882 | $ | 11,552,218

Если бы другие правительства не чинили препятствий, эта страна импортировала бы еще большие количества руды, поскольку она платит более высокие цены и более либеральна в отношении примесей.

Таблица показывает, что Соединенные Штаты импортировали 36 процентов мировой добычи вольфрама; это количество в дополнение к внутренней добыче составляет в сумме 17 921 тонну, или 50 процентов мирового производства. Из-за задержки поставок из Южной Америки и Китая южноамериканские руды, полученные в январе и феврале, относились к добыче 1917 года, как и китайские руды, прибывшие до конца марта. Вычитание руд, прибывших из этих двух регионов в течение первых двух и трех месяцев 1918 года соответственно, и добавление руд, прибывших за аналогичный период в 1919 году, делает количество руды, контролируемой Соединенными Штатами в 1918 году (как показано на стр. 153), эквивалентным 21 131 тонне концентратов с содержанием 60 процентов WO3, или 59 процентам мирового производства. Все эти руды контролировались благодаря частной инициативе американских фирм, которые предлагали лучшие цены и лучшие условия, чем можно было получить за рубежом. Вероятно, в будущем можно было бы обрабатывать большую долю, если бы не возникло вмешательство изнутри наших собственных границ. В настоящее время предлагается ввести тариф в размере 10 долларов за единицу на вольфрамовые руды без учета чистоты или качества, с соответствующим высоким тарифом в 1 доллар за фунт, плюс действующие в настоящее время 15-процентные адвалорные пошлины на металл в любой форме — элемент, сплав или соль; такой законопроект был принят Палатой представителей. Его сторонники полагают, что цена, составляющая сейчас около 7 долларов за единицу в Нью-Йорке, поднимется до 17 долларов за единицу.

В дальнейшем объемы вольфрамовой руды будут значительно меньше, чем в 1916, 1917 и 1918 годах, и будут ограничены потребностями мирного времени, если не возникнет какая-либо непредвиденная война. По оценкам правительства на январь 1920 года, у Англии был запас на два года, и Франция, вероятно, обеспечена не хуже. У Соединенных Штатов, вероятно, имелось в наличии количество, эквивалентное почти 8000 тонн руды с содержанием 60 процентов WO3. Производители инструментальной стали рассчитывали на потребление 7500 тонн в течение 1919 года, но из-за отсутствия рынка сбыта руды эта цифра была слишком завышена; вероятно, 4000 тонн — достаточно большая величина, поэтому в течение почти двух лет вряд ли будет рынок для новых поставок, за исключением случаев, когда руда может закупаться спекулятивно. В течение этого времени рудники повсюду должны оставаться бездействующими, пока снова не возникнет спрос, за исключением тех рудников, которые необходимы для снабжения вольфрамом Германии, Австрии и России, а также небольшого количества, требуемого Швецией, Норвегией и Италией. Если промышленность Германии, Австрии и России восстановится настолько, что они смогут покупать и использовать вольфрам, Германия вернет себе часть утраченной торговли за счет руд, которые будут охотно предлагаться странами-производителями, нуждающимися в рынке сбыта. Торговцы Англии, Франции и Соединенных Штатов будут рады продавать вольфрам и ферровольфрам, но Германия, несомненно, будет стремиться к получению сырья, чтобы максимально использовать свою многочисленную безработную рабочую силу. Если будет принят такой тарифный закон, как предлагаемый сейчас, Соединенные Штаты отрежут себя от иностранных поставок и положат конец своему контролю над какой-либо значительной их частью. Однако, если высокая цена будет поддерживаться, искусственно или иным образом, разработка других легированных сталей для использования в многолезвийных инструментах может достичь точки, когда потребуется не так много вольфрама.

Германский контроль.

— У Германии не было значительных месторождений вольфрама у себя дома и на удерживаемых ею иностранных территориях, но в 1913 году ее контроль через деловые альянсы охватывал около двух третей мировой добычи вольфрамовой руды. В том году, согласно официальным немецким данным, было импортировано 5295 коротких тонн вольфрамовых руд. Большая часть этого объема, вероятно, содержала 65 процентов или более WO3, что эквивалентно, скажем, 5736 тоннам концентратов с содержанием 60 процентов WO3. Добавление 106 тонн саксонских концентратов, произведенных в том году, показывает, что Германия переработала в общей сложности примерно 5840 тонн из мировой добычи в 8864 тонны, или около 66 процентов от общего объема. Соединенные Штаты в том же году произвели 1537 тонн и импортировали 449 тонн неизвестного содержания, но все это, вероятно, было эквивалентно более чем 2000 тоннам руды с содержанием 60 процентов WO3, оставляя лишь около 1000 тонн для других стран, большая часть которых, по-видимому, перерабатывалась во Франции. Эту торговлю Германия потеряла, когда вместе с Австрией начала Мировую войну. С прекращением всех океанских поставок в Германию большая часть иностранных руд стала ей недоступна, но, несомненно, в течение некоторого времени после начала войны небольшие количества просачивались через Швецию и Норвегию. Небольшая добыча Австрии была доступна всегда, и говорят, что значительное количество руды контрабандой перевозилось через границу Португалии в Испанию, оттуда по воде к западной границе Италии, в Швейцарию, а оттуда отправлялось прямо в Германию. Значительная часть испанской продукции, как говорят, также попадала в Германию таким путем, а «искалеченные» подводные лодки, заходившие в испанские порты, как сообщается, перевозили грузы вольфрама для Германии. На основе имеющихся данных невозможно подтвердить или опровергнуть эти сообщения, и при их изложении их сомнительность полностью признается, но такие возможности должны быть приняты во внимание.

В странах Антанты и Соединенных Штатах немецкие интересы были взяты под контроль правительствами, но в Южной Америке немецкие фирмы по-прежнему сохраняют некоторый контроль над вольфрамсодержащими объектами. В Боливии четыре немецкие фирмы, как говорят, имеют добычу около 600 метрических тонн руды в год. В Перу то, что считается большей частью месторождений вольфрама, контролируется фирмами, которые считаются немецкими: E. y W. Hardt и Carlos W. Weiss y Cia. В Аргентине основным производителем является Hansa Mining Co., немецкое предприятие. Его добыча, как говорят, составляет около 500 тонн концентратов в год, но даже эта продукция, по имеющимся сведениям, поступала в Соединенные Штаты во время войны. Если Соединенные Штаты введут запретительный тариф, Германия может легко восстановить значительную часть своего контроля над мировой торговлей вольфрамом.

ПРОИЗВОДСТВЕННЫЕ ПРЕДПРИЯТИЯ И ПРОЦЕССЫ

Распространение знаний, особенно касающихся электрических печей, делает контроль над торговлей вольфрамом с помощью секретных процессов или превосходного мастерства чрезвычайно трудным и, насколько это касается Соединенных Штатов, Великобритании и Франции, дает мало преимуществ кому-либо одному. Япония, возможно, находится в несколько менее выгодном положении. Плавильные заводы строятся так легко, быстро и дешево, что не дают больших шансов на монополию. Дешевая энергия, высокий технический уровень и знания, оригинальность и смелость в экспериментах, превосходная организация, щедрое отношение к производителям, честный продукт, продаваемый честно, хорошие транспортные возможности и широкие разумные законы — вот элементы, которые обеспечат контроль. Соединенные Штаты могут получить этот контроль благодаря разумным усилиям, но эгоистичные законы могут еще легче разрушить контроль над большей частью мировой торговли, свести наш вольфрамовый бизнес к провинциальному масштабу и сделать продукт дорогим на все времена.

ЧТО ОЗНАЧАЕТ КОНТРОЛЬ В СОЕДИНЕННЫХ ШТАТАХ

В годы хорошей конъюнктуры перед Мировой войной Соединенные Штаты использовали эквивалент 3000–4000 коротких тонн концентратов с содержанием 60 процентов WO3 в год. Когда началась война, наступило затишье, пока атакованные страны переводили дух и готовились к долгой борьбе. После того как планы были составлены и производство боеприпасов началось в широком масштабе, спрос на вольфрам колоссально вырос. Все виды руд принимались по баснословным ценам. Руды, содержащие олово, фосфор, серу и висмут, которые раньше не рассматривались производителями стали, принимались с жадностью, и началась большая борьба за месторождения. В октябре 1918 года Соединенные Штаты использовали вольфрамовые руды со скоростью 20 000 тонн в год. Тем временем разведка обнаружила так много новых месторождений, и они эксплуатировались так активно, что в странах Антанты накопились большие запасы руд. С другой стороны, в этой стране многие из известных месторождений показали признаки истощения, ряд из них после непродолжительной прибыльной работы стал полностью неработоспособным, и вполне вероятно, что некоторые из месторождений, которые казались самыми богатыми, никогда больше не будут давать много продукции. Среди новых открытий были контактово-метаморфические месторождения Большого Бассейна в Калифорнии, Неваде и северо-восточной Юте. Они были частично освоены, и некоторые из них многообещающие, но неравномерность контактово-метаморфических месторождений руды общеизвестна.

В 1916 году при ценах от 15 до 93,50 долларов за единицу Соединенные Штаты произвели 5969 тонн концентратов; в 1917 году, все еще под влиянием бума 1916 года, при ценах около 25 долларов за единицу — 6144 тонны; а в 1918 году, при ценах, все еще составлявших в среднем около 25 долларов за единицу, — 5041 тонну, хотя в декабре добыча была невелика. При цене 17 долларов за единицу, которой, по мнению сторонников тарифов, можно достичь с помощью тарифа в 10 долларов за единицу, кажется маловероятным, что Соединенные Штаты смогут рассчитывать на добычу более 3000 тонн в год в течение следующих трех лет. Существуют, конечно, возможности как большей, так и меньшей добычи. Если бы произошла еще одна великая война, событие, которое не выходит за рамки воображения, Соединенные Штаты, вероятно, начали бы с использования вольфрама со скоростью 20 000 тонн концентратов в год. Если бы цена не была еще более экстравагантной, чем самая высокая цена в 1916 году (93,50 доллара за единицу), Соединенные Штаты не смогли бы произвести и половины необходимых им концентратов, а время, необходимое для достижения даже такого объема добычи, было бы слишком долгим для безопасности. Конечно, такая добыча была бы намного лучше, чем никакой, но для безопасности Соединенные Штаты должны иметь в пределах досягаемости запас по крайней мере на год.

Тихий океан, вокруг границ которого находятся крупнейшие месторождения вольфрама, многими рассматривается как следующий крупный театр военных действий, и как бы жизненно необходимы они ни были, получение поставок вольфрамовых руд может стать невозможным из-за блокирования торговых путей. Поэтому представляется гораздо более правильным, чтобы вместо того, чтобы поощрять быстрое истощение наших собственных запасов, которые и так слишком скудны, мы использовали богатые низкоценовые руды, добываемые сейчас на Востоке. Эти дешевые руды мы можем получить в торговле по первому требованию, и для правительства было бы одной из лучших форм национального страхования жизни создать запас в 10 000 тонн этих руд, пока их можно достать.

Часто приводится аргумент, что, установив высокий тариф на вольфрамовые руды, мы добьемся такого развития наших собственных месторождений, что при необходимости можно будет быстро наладить добычу; также утверждается, что при наличии потребности мы найдем больше руд. Оба аргумента ложны. Имеется в виду не развитие, а извлечение. Никто не будет открывать вольфрамовый рудник, чтобы руды просто лежали на случай дня нужды страны. Нахождение новых руд — это вероятность, но их количество — вопрос совершенно открытый. Немногие вольфрамовые рудники Соединенных Штатов могут прибыльно работать при нынешней цене около 7 долларов за единицу, и рудники сейчас закрыты. Число лиц, зависящих от добычи американских вольфрамовых руд, невелико, вероятно, менее 900 человек в мирное время. В настоящее время большинство вольфрамовых шахтеров уже получили другую работу, и практически все могли бы получить работу с не меньшей выгодой на других рудниках, многие из которых испытывают нехватку рабочей силы, так что больших трудностей не возникло бы. С точки зрения национальной экономики Соединенные Штаты не могут позволить себе упустить шанс покупать дешевые вольфрамовые руды, пока они доступны. Помимо вопроса страхования и даже выживания во время другой войны, не покупать южноамериканские руды — значит выбросить южноамериканскую торговлю. В некоторой степени это верно и для китайских и японских руд.

Металлургия вольфрама, как и других металлов, постоянно совершенствуется, и если наши руды некоторое время останутся в земле, они будут иметь большую абсолютную ценность при добыче, так как будет меньше отходов при переработке. Если наши руды будут добываться сейчас при искусственно завышенной цене, мы всегда будем платить высокую цену за вольфрамовые руды, ибо когда наши будут использованы, руды в других странах уменьшатся в количестве и вырастут в цене; цены будут выше, и нам придется покупать по повышенной ставке. С другой стороны, удерживая наши рынки открытыми для дешевых руд из любого источника, мы будем на равных с другими странами и всегда будем иметь резерв дорогостоящих руд, доступных в чрезвычайной ситуации.

Существует только один урожай руды. Сознательно передать все дешевые вольфрамовые руды мира нашим конкурентам, предоставляя им это преимущество в производстве быстрорежущих сталей, с помощью которых они конкурируют в иностранной торговле с нашими сталями и со всеми продуктами, в которых они используются; поощрять раннее истощение наших собственных месторождений этого незаменимого металла; и принуждать нас всегда использовать дорогостоящие руды — это были бы экономические преступления.

ГЛАВА VIII ВАНАДИЙ Р. Б. Мур

ПРИМЕНЕНИЕ ВАНАДИЯ

Основное применение ванадия — в стали. Он используется там, где требуются большая вязкость и сопротивление кручению, например, в деталях автомобилей, шестернях, поршневых штоках, трубах, котельных листах, трансмиссионных валах, болтах, стволах орудий, орудийных щитах и любых видах поковок, которые должны выдерживать тяжелый износ. Содержание ванадия в таких сталях варьируется от 0,1 до 0,4 процента. Ванадий иногда используется в некоторых вольфрамовых сплавах для производства быстрорежущей инструментальной стали, причем введение небольшой доли ванадия значительно снижает долю вольфрама, необходимую для придания таким сплавам желаемой твердости и вязкости.

Арнольд привел несколько иллюстраций влияния ванадия на стали различных типов:

Одна простая углеродистая сталь, содержащая около 1 процента углерода, имела предел текучести 35 тонн на квадратный дюйм, максимальное напряжение 60 тонн на квадратный дюйм, относительное удлинение 10 процентов на 2 дюйма и уменьшение площади поперечного сечения на 10 процентов. Добавление к этой стали около 0,6 процента ванадия повысило предел текучести с 35 до 65 тонн, максимальное напряжение с 60 до 86 тонн на квадратный дюйм, при этом относительное удлинение составило 7 процентов, а уменьшение площади поперечного сечения — 8 процентов.

Сталь, содержащая 0,25 процента углерода и 3,3 процента никеля, имела предел текучести 33 тонны, максимальное напряжение 42 тонны на квадратный дюйм, относительное удлинение 26 процентов на 2 дюйма и уменьшение площади поперечного сечения 53 процента. Практически идентичная сталь, содержащая дополнительно около 0,25 процента ванадия, имела предел текучести 50 тонн вместо 33 и максимальное напряжение 68 вместо 42 тонн на квадратный дюйм. Относительное удлинение составило 17 процентов на 2 дюйма, а уменьшение площади поперечного сечения — 36 процентов.

Сталь, содержащая 0,25 процента углерода и около 1 процента хрома, имела предел текучести 27 тонн и максимальное напряжение 41 тонну на квадратный дюйм, при относительном удлинении 36 процентов на 2 дюйма и уменьшении площади поперечного сечения 55 процентов. Добавление 0,25 процента ванадия повысило предел текучести с 27 до 40, а максимальное напряжение с 41 до 55 тонн на квадратный дюйм. Относительное удлинение было снижено с 36 до 26 процентов, а уменьшение площади поперечного сечения — с 55 до 53 процентов.

Таким образом, ванадий отличается от вольфрама тем, что оказывает чрезвычайно благотворное влияние не только на инструментальную, но и на конструкционную сталь. Арнольд показал, что ванадий, по-видимому, не образует двойного карбида с железом, а постепенно забирает углерод из карбида железа до тех пор, пока при наличии около 5 процентов ванадия Fe3C не может существовать, и присутствует только карбид ванадия V4C3, содержащий 15 процентов углерода; этот компонент является постоянным, по крайней мере в инструментальных сталях, содержащих от 5 до 14 процентов ванадия. Микрографический анализ таких сплавов привел к открытию трех новых компонентов, а именно: ванадиевого перлита, ванадиевого харденита и ванадиевого цементита.

Хромованадиевые стали — это последняя разработка в области конструкционных легированных сталей, получившая обширный рынок сбыта. Почти все эти стали производятся в мартеновских печах; сплавы хрома и ванадия добавляются незадолго до разливки. По своим физическим свойствам эти стали очень похожи на хромоникелевые стали, но имеют большее сужение площади поперечного сечения при заданном пределе упругости, чем последние. Большая часть производимых хромованадиевых сталей идет на нужды автомобилестроения. Некоторые производители предпочитают такие стали из-за их большей свободы от поверхностных дефектов, особенно швов, которые склонны иметь стали, содержащие никель, если слитки хоть немного некачественные. Эти стали почти всегда используются в термообработанном состоянии, но даже в автомобилях некоторые рамы, поковки и валы изготавливаются из стали в ее естественном состоянии.

Некоторое количество хромованадиевой стали, как говорят, используется в броневых плитах средней толщины, которые не подвергаются поверхностной закалке, но обладают высокой стойкостью, придаваемой термической обработкой.

Ванадий также в некоторой степени используется в производстве бронз, в медицине и при крашении.

Заменители.

— Утверждалось, что несколько заменителей, главным образом титан и молибден, придают стали свойства ванадия. Оба этих металла придают стали некоторые свойства, которые обычно ассоциируются с ванадием, но ни один из них не заменяет ванадий полностью.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Primos Chemical Co. (см. далее) имеет свой собственный запатентованный метод обработки роскоэлита, руды, найденной в Ньюмайре, штат Колорадо. Этот метод заключается в обжиге руды с солью, содержащей немного пирита, и является методом, который в некоторой степени применим к большинству ванадиевых руд, не содержащих свинца. American Vanadium Co. имеет секретный процесс обработки своих перуанских руд. Этот метод не был опубликован. Обработка ванадинитовых, купродесклуазитовых и карнотитовых руд изучалась Геологической службой США в Голдене, штат Колорадо. Любое изменение в практике, которое произойдет, вероятно, будет касаться главным образом обогащения ванадинита и обработки этого минерала и купродесклуазита.

ГЕОЛОГИЧЕСКОЕ И ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Перуанские месторождения.

— Крупнейшие месторождения ванадия в мире и самые важные до недавнего времени контролировались American Vanadium Co. из Питтсбурга, штат Пенсильвания, которая в 1919 году была поглощена Vanadium Products Corporation, связанной с Bethlehem Steel Corporation. Эти месторождения находятся в Минасрагре, Перу, в 20 милях от Серро-де-Паско. Район расположен вдоль западного края широкой антиклинали в юрско-триасовых и меловых породах. Разрез показывает, что серия в этой местности состоит из зеленых сланцев, тонких пластов известняка и красных сланцев. Ванадий встречается только в красных сланцах. Само месторождение представляет собой линзообразную массу шириной 28 футов и длиной 350 футов. Руда содержит несколько минералов. Минерал, составляющий большую часть месторождения, называется «квискеит»; это черное углеродистое вещество, содержащее серу. Существует также меньшее количество коксоподобного материала. Ни один из них не содержит ванадия. Ванадий находится в основном в южной части рудного тела, и на глубине до 20 футов он в значительной степени находится в форме красного ванадата кальция, который имеет более яркий цвет, чем ванадат кальция в Колорадо и Юте, и содержит до 50 процентов оксида ванадия. Он встречается в небольших карманах и заполняет трещины и разломы в тонком сланце. Ниже этого сланца находится «материнская жила», которая имеет толщину от 9 до 30 футов, простирается на большую часть длины месторождения и содержит до 10 процентов оксида ванадия и почти столько же серы. На восточной и южной сторонах, ниже «материнской жилы», находится твердый сине-черный ванадиевый сланец, содержащий до 13 процентов оксида ванадия и 4–5 процентов серы. Патронит, основной ванадиевый минерал, зеленовато-черного цвета и содержит от 19 до 24,8 процента оксида ванадия, а местами 50–55 процентов связанной серы. Патронит первоначально почти достигал поверхности и наиболее распространен в северной половине линзы. Все рудное тело почти полностью окружено порфировыми дайками и содержит два или три интрузивных тела. Эти месторождения контролируются American Vanadium Co. и ее преемником, Vanadium Products Corporation, через концессию от перуанского правительства. Они велики, но отнюдь не неисчерпаемы, и, поскольку они полностью локальны, вряд ли будут продублированы. Подобные месторождения неизвестны ни в Перу, ни в какой-либо другой части мира.

В 1917 году American Vanadium Co. переработала 5236 брутто-тонн руды, из которых извлекла 2 122 005 фунтов ванадиевой кислоты. Из этой ванадиевой кислоты компания произвела 4 925 014 фунтов феррованадия. Компания не закупала руду в этой стране, а полагалась исключительно на свою перуанскую добычу.

Другие иностранные месторождения.

— Месторождения в Перу — единственные месторождения, имеющие какое-либо коммерческое значение за пределами Соединенных Штатов. Ванадий встречается в Южной Австралии в ассоциации с карнотитом и другими урановыми минералами. Небольшие количества оксида ванадия получаются как побочный продукт при переработке этих руд.

Ванадий также ассоциируется с урановыми минералами в Андижанском районе, Среднеазиатская Россия. Ванадий обычно встречается в виде туранита, или ванадата меди; ферганита, ортованадата урана; и в виде нескольких других новых минералов. Количество руды представляется достаточно большим, и этот район может в конечном итоге стать источником как урана, так и ванадия.

Свинцовые руды Мексики содержат некоторое количество ванадия, наиболее известные месторождения находятся в северо-восточной части штата Чиуауа. Другие месторождения сообщаются в Сакатекасе, Гуанахуато, Сан-Луис-Потоси и Идальго.

Месторождения в Соединенных Штатах.

— Основные месторождения ванадия в Соединенных Штатах находятся в металлогенической провинции, охватывающей южный и юго-западный Колорадо, юго-восточную Юту и части Аризоны и Нью-Мексико. Уран и радий характеризуют ту же провинцию.

Вероятно, крупнейшие месторождения ванадия, обнаруженные до сих пор в Соединенных Штатах, находятся в юго-западном Колорадо, в округе Сан-Мигель. Эти месторождения были посещены Рэнсомом и Спенсером в 1899 году, и их описание вместе с примечаниями к химическим анализам и составу роскоэлита, сделанными Хиллебрандом, было опубликовано в 1900 году. Флек и Френч также описали эти месторождения. Флек и Холдейн позже опубликовали дополнительные описания с примечаниями о горных работах. Хесс в 1912 году опубликовал отличное описание этих месторождений с примечаниями о возможном происхождении и т. д.

Согласно Кроссу и Пьюрингтону, вмещающая порода состоит из юрских и триасовых отложений, делимых на три формации: Долорес внизу, Ла-Плата выше и Мак-Элмо над Ла-Платой. Последняя состоит из двух мощных пластов светлого песчаника, разделенных тонким пластом известняка. Ванадийсодержащая порода — это нижний песчаник. Он светло- или тускло-зеленого цвета, мелкозернистый. Иногда в трещинах и разломах встречаются пятна карнотита, но содержание урана слишком мало, чтобы его стоило сохранять.

Согласно Хиллебранду, зеленый ванадиевый минерал, которому песчаник обязан своим цветом, не является хлоритом, а тесно связан со слюдой, роскоэлитом. Добываемая руда имеет среднее содержание 1,5 процента V2O5. Эти низкосортные месторождения роскоэлита могут разрабатываться с прибылью, потому что они велики и легко разрабатываются.

Несомненно, эти месторождения ощутили на себе последствия довольно большой добычи последних нескольких лет, и среднее содержание руды сейчас, вероятно, по крайней мере на полпроцента ниже по V2O5, чем было несколько лет назад. Все еще остается значительное количество нетронутой руды, которая в среднем содержит 1 процент или немного меньше. Британское правительство в течение нескольких лет, согласно сообщениям, было заинтересовано в получении контроля над месторождениями ванадия.

Primos Chemical Co. с заводами в Ньюмайре, штат Колорадо, и Примосе, штат Пенсильвания, разрабатывает эти месторождения и в 1917 году произвела следующую продукцию:

Переработано 60 907 000 фунтов руды; из этого было произведено 496 731 фунт ванадия в форме ванадата железа с содержанием около 34 процентов металлического ванадия. Из этого было произведено 417 770 фунтов содержащегося ванадия в форме обычного 40-процентного феррованадия. В 1918 году, по июль включительно, эта компания добыла 17 449 000 фунтов руды, из которых было произведено 149 343 фунта содержащегося ванадия в форме ванадата железа и 133 666 фунтов содержащегося ванадия в форме 40-процентного феррованадия.

В 1919 году Primos Chemical Co. была поглощена недавно организованной Vanadium Products Corporation.

Ванадиевая руда была обнаружена в округе Уэрфано, штат Колорадо, недалеко от хребта Сангре-де-Кристо. Жила, как говорят, хорошо выражена и имеет ширину от 1 до 4 футов. Ряд анализов показывает содержание V2O5 от 2 до 7 процентов, а другие — от 2 до 4 процентов меди. Руда тяжелая, черная и полосчатая; она содержит небольшие количества оксида урана, но должна классифицироваться как ванадиевый, а не урановый минерал. Коммерческой добычи до настоящего времени не было.

В округе Игл, в 7 милях к юго-востоку от города Игл, была найдена серебряная руда, содержащая ванадий. Она была обнаружена в основном на руднике Lady Bell. Руда, темно-зеленоватый песчаник, похожий по внешнему виду на более темные типы роскоэлитовой руды, найденной в округе Сан-Мигель, содержала от 25 до 1000 унций серебра на тонну. Рудник был в значительной степени выработан на серебро, ванадий терялся в процессе плавки. Однако все еще остается значительное количество ванадиевой руды, так как низкосортная серебряная руда не добывалась и не перерабатывалась.

Значительное количество ванадия получается как побочный продукт при переработке карнотитовой (уран и радий) руды. Трудно сказать, каков выход из этой руды, но вероятно, что он составляет в среднем около 200 000 фунтов оксида ванадия в год. Это производится пятью или шестью действующими радиевыми компаниями. Эти месторождения находятся в юго-западном Колорадо, вокруг долины Парадокс, и в юго-восточной Юте, простираясь до Сан-Рафаэль-Свелл, к юго-западу от Грин-Ривер, Юта.

Существует значительное количество руды с содержанием от половины до 1 процента оксида урана, которая содержит от 4 до 10 процентов оксида ванадия. В прошлом эта руда не добывалась, потому что извлечение из нее радия не окупалось. При сильном спросе и высокой цене на ванадий, по крайней мере, более высокие сорта этой руды могли бы добываться с прибылью. В определенных местах к северу от долины Парадокс имеется значительное количество такой руды; к сожалению, эти месторождения несколько разбросаны, и некоторые из них потребовали бы не только долгой перевозки на повозках, но и транспортировки на ослах до дорог. Только руду более высокого качества можно было бы обрабатывать таким образом с прибылью, а трудность заключается в том, чтобы получить достаточное количество, оправдывающее строительство перерабатывающего завода.

Автору сказали, что существуют месторождения этого же типа руды на горе Темпл, в 40 милях к югу от Грин-Ривер, Юта.

Небольшое ванадинитовое месторождение, содержащее следы вульфенита, было найдено недалеко от станции Клайнфелтер, на главной линии железной дороги Санта-Фе, недалеко от восточной границы округа Сан-Бернардино, Калифорния. Руда в основном состоит из кальцита и является низкосортной, составляя в среднем, вероятно, от 1 до 2 процентов оксида ванадия.

Месторождение ванадинита в округе Сьерра, Нью-Мексико, на железной дороге Atchison, Topeka & Santa Fe, разрабатывалось в течение короткого периода в 1912 и 1913 годах. Помимо ванадия, жилы содержат галенит, карбонаты меди, барит, флюорит и другие минералы. Руда перерабатывалась на мельнице рядом с рудником, но все предприятие было безуспешным, вероятно, из-за того, что руда была очень низкосортной, и из-за металлургических трудностей. Существует ряд других месторождений ванадинита в Нью-Мексико, но ни одно из них не было коммерчески освоено каким-либо образом.

Ванадинит встречается в значительном количестве мест в Аризоне, часто в ассоциации с вульфенитом, или молибдатом свинца. Действительно, одна из трудностей производства как ванадия, так и молибдена из ванадинита и вульфенита заключается в том, что эти два минерала часто настолько тесно связаны, что из-за незначительной разницы в удельном весе их нелегко разделить механическими методами. На руднике Mammoth в Аризоне верхние уровни богаче ванадинитом, чем вульфенитом, но на нижних уровнях верно обратное. Несомненно, значительное количество ванадинита можно было бы добыть на этом руднике и других в окрестностях, но сомнительно, можно ли это сделать с прибылью, даже при высокой цене на ванадий.

United States Vanadium Co. имеет рудник в 4 милях от Рэй-Джанкшен, Аризона, и на руднике небольшую мельницу для концентрации руды, которая является низкосортной, и производит ванадий из концентратов. Количество руды, которое можно получить с этого рудника, несколько сомнительно. В этом и заключается проблема с ванадинитом в целом; он существует на обширной территории, но все месторождения низкосортные и, по-видимому, не являются обширными в какой-либо одной местности.

Одним из наиболее многообещающих месторождений с точки зрения увеличения добычи ванадия является рудник Shattuck в Бисби, Аризона, где большая жеода, или полость, выстлана ванадиевым минералом, вероятно, купродесклуазитом. Руда содержит около 8–10 процентов оксида ванадия, в дополнение к меди и свинцу. Это кажется одной из лучших возможностей для увеличения добычи ванадия в этой стране. Станция Геологической службы США в Голдене, Колорадо, провела металлургическое исследование обработки этой руды.

Таблица V. — Географическое распределение месторождений ванадия в мире.

Распределение месторождений ванадия в мире показано на Таблице V.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ НАЦИЙ

Соединенные Штаты исключительно удачливы в отношении ванадиевых продуктов, так как они практически являются единственным производителем ванадия в мире, а перуанские месторождения находятся под контролем американской компании. Поэтому Англия, Франция, Германия, Япония и другие страны вынуждены покупать у американских компаний.

РАЗВИТИЕ И ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРЕДЕЛЕНИИ В БЛИЖАЙШЕМ БУДУЩЕМ

Большая часть ванадия, использовавшегося в этой стране, поступала с рудников American Vanadium Co. в Перу, но Primos Chemical Co. произвела такое количество ванадия из своих заявок в Ньюмайре, округ Сан-Мигель, Колорадо, которое по крайней мере имело тенденцию создать некоторую реальную конкуренцию American Vanadium Co. Как уже говорилось, эти заявки далеко не так богаты или продуктивны, как были, но они, вероятно, пригодны еще на несколько лет. На руду из Перу можно рассчитывать, вероятно, еще несколько лет при примерно нынешнем уровне добычи. То же самое относится к карнотитовой руде, и вполне вероятно, что добыча ванадия из карнотита может в некоторой степени увеличиться, так как спрос на радий силен, и может последовать увеличение переработки карнотита более низкого качества. Поскольку этот низкосортный материал обычно содержит больше ванадия, добыча ванадия из этого источника может увеличиться.

Ванадинит может оказаться источником ванадия, хотя сомнительно, можно ли произвести большое количество из этого минерала. Как уже говорилось, купродесклуазит, вероятно, является лучшим источником для немедленного увеличения добычи.

Что касается иностранных стран, кроме Перу, Россия — единственная, которая может производить сколько-нибудь значительное количество ванадиевых руд, и, несомненно, такая добыча не будет получена до тех пор, пока промышленные условия не станут более стабильными.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

American Vanadium Co. владеет своими рудниками в Перу через концессию от перуанского правительства. Таким образом, по крайней мере две трети мировой добычи ванадия практически находятся в руках перуанского правительства, хотя компания, осуществляющая деятельность, — американская.

Ранее American Vanadium Co. была единственным производителем ванадиевых продуктов и феррованадия в мире. Цена на ванадий тогда составляла около 5,00 долларов за фунт металлического ванадия в составе феррованадия. Позже на рынок вышла Primos Chemical Co., и American Vanadium Co. снизила цену. Из-за больших запасов руды, которые Primos Chemical Co. имела в Колорадо, результатом стало просто снижение цены на феррованадий. Несомненно, если бы не эта конкуренция, цена на ванадий в тот период была бы выше, чем она была, и если бы не Primos Chemical Co., American Vanadium Co. имела бы практически монополию на всю добычу ванадия, так как добыча из карнотита была недостаточно велика, чтобы серьезно повлиять на рынок. Как бы то ни было, эти две компании контролировали более 90 процентов поставок руды, и поэтому недавняя смена владельца на Vanadium Products Corporation позволит последней устанавливать цену, а также регулировать потребление и тем самым продлевать доступность полезного металла, который в противном случае, вероятно, скоро был бы исчерпан. Основные месторождения ванадия в Чиуауа, Мексика, контролируются поместьем Мадеро (мексиканским).

Это доминирование в контроле над источниками поставок сделало контроль через владение перерабатывающими заводами, патентами и секретными процессами менее важным.

ГЛАВА IX СУРЬМА Х. Г. Фергюсон и Д. А. Холл

ПРИМЕНЕНИЕ СУРЬМЫ

Следующая сводка применения сурьмы взята из «Минеральных ресурсов Соединенных Штатов», 1918 г. [90]

[90] Бастин, Э. С.: «Сурьма в 1918 году», «Минеральные ресурсы Соединенных Штатов», 1918 г. Геологическая служба США, 1919 г.

Применение в мирное время. — Металлическая сурьма в чистом виде имеет мало промышленных применений. В форме мелкого порошка, известного как «железная чернь», она используется для придания вида полированной стали изделиям из папье-маше или керамики. Для этих целей она осаждается действием металлического цинка в кислом растворе солей сурьмы. Сурьма легко сплавляется с большинством тяжелых металлов, и сплав тверже, чем два чистых металла. Большинство этих сплавов обладают свойством небольшого расширения при затвердевании. Типографский сплав — это сплав сурьмы, свинца и олова; баббит, антифрикционный или подшипниковый металл — это обычно сплав сурьмы, олова и меди. Британский металл, также известный как «белый металл», — это сплав сурьмы, олова и меди с некоторым количеством цинка и, редко, небольшими количествами других металлов. Он используется при изготовлении дешевой домашней посуды, чайников и ложек. Сплавы сурьмы находят незначительное применение в аккумуляторных пластинах, игрушках, кабельных оболочках и сифонных головках. Свинцово-сурьмяный сплав, или твердый свинец, используется при изготовлении кислотостойких клапанов.

Белый оксид сурьмы, главным образом тетраоксид (Sb2O4), используется для изготовления непрозрачной белой эмали и других санитарно-технических изделий. В этом применении оксиды сурьмы конкурируют с оксидом олова. Оксид сурьмы, главным образом триоксид, используется в качестве красящего агента в производстве стекла, так как он более легкоплавок, чем тетраоксид, и не придает стеклу непрозрачности. Оксиды сурьмы далее используются в качестве пигментов для красок.

Красные сульфиды сурьмы используются при вулканизации и окрашивании красной резины, а также в качестве пигментов для красок. Природный трисульфид сурьмы, антимонит, входит в состав безопасных спичек или состава, который наносится на спичечную коробку.

Антимонат свинца, содержащий избыток оксида свинца, известный как «неаполитанская желтая», используется в масляных красках, а также в стекольной и керамической промышленности. Соль сурьмы, рвотный камень (двойной тартрат сурьмы и калия), и фторид сурьмы используются в качестве протрав при крашении. Рвотный камень и триоксид сурьмы применяются в медицине.

Военное применение. — Сурьмянистый свинец, содержащий от 12 до 13 процентов сурьмы, используется в производстве шрапнельных пуль. Меньшие количества ликвационного сульфида сурьмы используются в капсюлях снарядов. Для этой последней цели, как утверждается, материал должен содержать менее 2 процентов примесей, нерастворимых в соляной кислоте. Сульфид сурьмы в виде порошка используется в заряде некоторых снарядов для создания при взрыве белого дыма, который полезен при определении дальности.

Во время войны Германия в некоторой степени использовала сурьму в качестве заменителя более важных металлов при производстве валюты, но нехватка самой сурьмы не позволила этому применению стать значительным.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Геологическое распространение промышленного сурьмяного сырья зависит, за немногими исключениями, от распространения основного рудного минерала — антимонита (сульфида сурьмы). Сервантит, сернармонтит и валентинит представляют собой оксиды сурьмы, образующиеся непосредственно в результате разложения антимонита вблизи поверхности, и вместе с другими продуктами окисления составляют основные руды некоторых районов. Самородная сурьма, также являющаяся продуктом окисления сульфидов, встречается редко и еще реже выступает в качестве рудного минерала. Джеймсонит, сульфид сурьмы и свинца, встречается часто и является основной рудой одного важного месторождения в Мексике. Сурьма также извлекается при рафинировании сурьмянистого свинца.

Антимонит встречается в кварцевых жилах и связанных с ними месторождениях. Многие важные месторождения сурьмы в мире находятся в более или менее тесной генетической связи с изверженными породами третичного периода. С глубиной руда часто сменяется пиритом. Несколько важных месторождений связаны с интрузивными породами, сформировавшимися на значительной глубине, и, вероятно, имеют контактово-метаморфическое происхождение.

Несмотря на большое разнообразие форм месторождений и характера вмещающих пород, антимонит проявляет отчетливую склонность к образованию метасоматических залежей в известняках. Основными жильными минералами являются кварц и кальцит. Из других сульфидов наиболее распространен пирит, но в качестве акцессорных минералов часто присутствуют киноварь, реальгар, халькопирит, галенит и сфалерит. Характерной чертой месторождений антимонита является относительная редкость других сульфидов; верно и обратное: важные сульфидные месторождения других металлов редко содержат антимонит. Исключением из общего правила является киноварь, сульфид ртути, который является характерным минералом некоторых антимонитовых жил. Аналогичным образом антимонит является одним из минералов, наиболее часто ассоциирующихся с месторождениями киновари.

Несколько наиболее важных сурьмяных районов обязаны своей добычей этого металла наличию извлекаемых количеств золота. Это справедливо для некоторых месторождений Франции, Венгрии, Австралии и Южной Африки.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ, А ТАКЖЕ ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Хотя сурьма в разное время добывалась во многих местах по всему миру, лишь в немногих странах месторождения были разработаны в значительных коммерческих масштабах. При нормальных условиях потребления потенциальное предложение сурьмяной руды значительно превышает спрос. Вследствие этого интенсивно эксплуатировались только те месторождения, которые можно было разрабатывать с низкими затратами, которые были выгодно расположены по отношению к рынкам сбыта или содержали значительные количества других минералов, главным образом золота.

Страны-производители сурьмы в мире можно разделить на три группы следующим образом:

1. Основные страны-производители в порядке значимости: Китай, Франция и Алжир, а также Мексика.

2. Страны, в которых производство в нормальное время нестабильно, но потенциальные запасы значительны, и производство становится важным при высоких ценовых уровнях: бывшая Австрийская империя, Боливия, Австралия (Виктория), Бирма, Южная Африка, Италия, Испания и Малая Азия.

3. Страны, в которых нормальное производство невелико и в которых известные запасы, вероятно, менее значительны: Соединенные Штаты и Аляска, Канада, Перу, Германия, Турция (Малая Азия), Сербия, Португалия, Борнео, Индокитай и Япония.

На таблице VI показано географическое распространение основных месторождений сурьмы в мире.

Статистические данные о производстве в различных странах настолько противоречивы, что невозможно дать более чем приблизительное сравнение между важными производителями. Насколько можно судить, добыча сурьмяной руды в 1913 году, последнем году, для которого имеются хотя бы приблизительно полные статистические данные, составила около 20 000 метрических тонн извлекаемой сурьмы. Потребление оценить еще труднее, так как таможенные данные разных стран сильно различаются. В следующей таблице показана относительная значимость основных стран-производителей и стран-потребителей в процентах от мирового производства в 1913 году:

Таблица 31. — Процент производства и потребления сурьмы

Country | Percentage of production | Percentage of consumption
Austria-Hungary |   4 |  |   4
France |  24 |  20
Germany | (small) |  20
Italy |   2 |   2
United Kingdom |   0 |  12
Serbia |   1 |   0
Asia Minor |   1 |   0
Japan |   0 |  | -  |  10
China |  51
Algiers |   1 |  |   0
United States |   0 |  32
Mexico |  11 |   0
Australia (Victoria) |   4 | (small)
All other |   1 | (small)
| 100 |  | 100

Таблица VI. — Географическое распространение месторождений сурьмы в мире. Авторы: Х. Г. Фергюсон и Д. А. Холл.

В последующем обсуждении мировых ресурсов сурьмы политический контроль в значительной степени обозначен заголовками стран, под которыми обобщены основные черты коммерческого контроля над производством, осуществляемого через владение рудниками и перерабатывающими заводами, а также через торговые интересы.

Северная Америка.

Соединенные Штаты.

— Месторождения сурьмы встречаются во многих местах в Соединенных Штатах, но в мирное время сравнительно высокие затраты на добычу в этой стране не позволяют конкурировать с китайскими и мексиканскими рудниками. До войны осуществлялось небольшое производство сурьмянистого свинца из отечественных руд, а также небольшое количество сурьмы извлекалось в качестве побочного продукта при рафинировании свинца, но, за исключением этого, страна полностью зависела от импортной сурьмы.

Высокие цены после начала войны вызвали быстрый рост добычи сурьмяных руд. Добыча сурьмяной руды на рудниках в 1915 году составила около 5000 коротких тонн, содержащих 2100 коротких тонн металла, а в 1916 году — 4500 коротких тонн, содержащих около 1770 коротких тонн металла. Более низкие цены 1917 года отразились на снижении добычи в том году, которая составила 1060 коротких тонн руды, содержащей 390 тонн металла. Производство в 1918 году составило 190 тонн, содержащих около 50 тонн металла.

Основными штатами-производителями в порядке значимости были Невада, Калифорния, Аляска, Вашингтон, Орегон, Айдахо и Арканзас. Юта и Аризона дали незначительные количества. В Неваде основным производителем был рудник Сазерленд в округе Гумбольдт. В Калифорнии большая часть продукции была получена с двух рудников в округах Иньо и Керн, эксплуатируемых компанией Western Metals Co. из Лос-Анджелеса; руда отправлялась на плавку в Сан-Педро, недалеко от Лос-Анджелеса. В Вашингтоне сурьма добывалась на объекте компании Gold Creek Antimony Mining & Smelting Co. в округе Оканоган. В Орегоне основным производителем был рудник Джим Дэнди недалеко от Бейкер-Сити. В Арканзасе один объект в округе Севьер дал заметное количество руды в 1916 году, а также небольшое количество металлической сурьмы на местном перерабатывающем заводе. На Аляске добыча велась в основном в районе Фэрбенкса, руда отправлялась на плавку в Лос-Анджелес и Сиэтл.

Владение рудниками в Соединенных Штатах не играет важной роли в нынешнем контроле над мировыми ресурсами, поскольку производство в нормальных условиях незначительно. Возможно, что с развитием новых способов применения сурьмы и ростом спроса на этот металл запасы в этой стране приобретут коммерческое значение.

Около 40 процентов мексиканской добычи сурьмы контролируется в Соединенных Штатах. Во время войны в Сан-Луис-Потоси был построен плавильный завод, принадлежащий американцам. Руды с рудников этого региона также отправлялись компании Western Metals Co. в Лос-Анджелесе. Американская компания Antimony Corporation владеет крупным месторождением джеймсонита (сульфида сурьмы и свинца) в Мексике, которое представляет собой важный резерв, еще не введенный в эксплуатацию. Месторождения сурьмы на севере Мексики во время войны разрабатывались на американский капитал. До 1914 года только одна компания в Соединенных Штатах пыталась заниматься плавкой сурьмы. Однако во время войны наблюдалась значительная активность, и несколько компаний занялись плавкой иностранных и отечественных руд. Основными источниками поставок были Китай, Боливия и Мексика. Успех всех этих предприятий был лишь временным, так как в нормальных условиях высокая стоимость производства в этой стране препятствует успешной конкуренции с китайским и японским металлом. Американские плавильные интересы в настоящее время практически не контролируют мировую сурьму, и ожидать этого в ближайшем будущем не приходится. Плавильные мощности страны оцениваются в 6000–7000 тонн металла в год, все они сейчас простаивают. Одна компания, Antimony & Compounds Co. of America, тесно связана с французской компанией La Lucette.

Канада.

— Производство сурьмы в Канаде было крайне нестабильным. В периоды высоких цен получали значительную продукцию, при этом годами максимальной добычи были 1898 год с отгрузкой 1344 коротких тонн руды и 1907 год с 2016 коротких тонн. Добыча прекратилась в 1910 году и не возобновлялась до 1915 года. В 1915 году было произведено 1341 тонна руды с содержанием 40 процентов металла; в 1916 году — 885 тонн руды с содержанием 42 процентов металла; и 361 тонна в 1917 году.

Основной производственный район находится в Уэст-Горе, Новая Шотландия, где руда, помимо содержания сурьмы, имеет содержание золота от 2 до 4 унций на тонну. Другими регионами, где добывалась сурьмяная руда, являются Нью-Брансуик (округ Йорк), Британская Колумбия, Квебек и территория Юкон. В Британской Колумбии (район Слокан) и на территории Юкон (Чифтейн-Хиллс) также разрабатываются сурьмянистые свинцовые руды. Руды Новой Шотландии, которые обеспечивали основную часть добычи, с 1915 года экспортировались в Англию; более ранняя продукция шла в Германию. Небольшое производство рафинированной сурьмы было получено главным образом как побочный продукт при рафинировании свинца на плавильном заводе компании Consolidated Mining & Smelting Co. в Трейле, Британская Колумбия; небольшое количество сурьмы также выплавлялось из сурьмяных руд компанией New Brunswick Metals, Ltd. (ранее Canadian Antimony Co.) в Лейк-Джордже, Нью-Брансуик. Канада, по-видимому, находится примерно в том же положении, что и Соединенные Штаты в отношении добычи сурьмы. Высокие цены, сохраняющиеся в течение длительного периода, приведут к значительному росту производства, но при ценах мирного времени ожидать какой-либо продукции не приходится.

Мексика.

— Месторождения сурьмы существуют во многих частях Мексики, и в течение многих лет велась значительная добыча. Как и в других странах, объем производства значительно увеличился в течение 1915 и 1916 годов. Производство металлической сурьмы за 1917 год составило 2141 метрическую тонну. В 1914 году в Англию было экспортировано 1543 длинные тонны сурьмяного сырья и регулюса; в 1918 году экспорта в Англию не было, но 1449 коротких тонн руды и 2660 тонн металла были отправлены в Соединенные Штаты.

Основные рудники находятся в Сьерра-Каторсе, в штатах Сан-Луис-Потоси и Керетаро. Руды представляют собой смесь сульфидов и оксидов и содержат от 5 до 50 процентов сурьмы.

В 1900 году в Уэдли был построен плавильный завод с годовой мощностью 6000 тонн металла, и большая часть продукции ранее направлялась в Англию, но с 1915 года она реализуется в Соединенных Штатах. Плавильный завод и наиболее важные рудники принадлежат английской компании Cookson’s через дочернее предприятие Republican Mining & Metal Co. Американские интересы владеют другими объектами в том же регионе, и во время войны компания International Mining & Metal Co. построила плавильный завод в Сан-Луис-Потоси. В западной Соноре, недалеко от Калифорнийского залива, имеются месторождения окисленных руд, которые обеспечивали значительную часть руды, импортируемой в Соединенные Штаты. Они принадлежат американскому капиталу.

Крупное месторождение свинцово-сурьмяной руды (джеймсонита) в Зимапане, Идальго, принадлежащее американской фирме The Antimony Corporation, еще не достигло стадии эксплуатации. Другие месторождения, возможно имеющие значение, известны в штатах Герреро, Дуранго, Сонора, Мехико, Нижняя Калифорния и других местах.

Политические беспорядки в течение последних нескольких лет препятствовали получению объема сурьмы, соразмерного с вероятной мощностью месторождений. Производство, вероятно, будет поддерживаться в будущем, даже в периоды низких цен.

Южная Америка.

Боливия.

— Добыча в Боливии до войны была незначительной, но под влиянием высоких цен в 1915 и 1916 годах было произведено большое количество высококачественной руды. Эта руда отправлялась главным образом в Англию, пока в 1918 году не было введено эмбарго на боливийскую руду. Руда высококачественная, отгружаемая руда содержит в среднем более 50 процентов сурьмы, но жилы небольшие и становятся непродуктивными на небольшой глубине. Возможно, что известные месторождения были в значительной степени исчерпаны; и хотя спрос, столь же высокий, как в 1916 году, мог бы привести к новым важным открытиям, маловероятно, что Боливия сможет стать важным производителем при нормальных условиях цен.

Экспорт руды составил 17 923 метрические тонны в 1915 году (по сравнению со 186 тоннами в 1914 году); 22 748 тонн в 1916 году; и 18 340 тонн в 1917 году; но в 1918 году, по причинам, указанным выше, поставки упали до 3070 тонн. От 75 до 90 процентов руды направлялось в Англию, а большая часть остального — в Соединенные Штаты, за исключением примерно тысячи тонн в год во Францию.

Перу.

— Во время сурьмяного бума 1906–1907 годов в Перу добывалось небольшое количество сурьмы. Дальнейшего производства не было до 1915 года, когда было добыто 522 тонны высококачественной руды. В 1916 году производство выросло до 1876 тонн 60-процентной руды. Производство 1917 года составило 902 тонны. Хотя месторождения известны во многих частях республики, более 90 процентов добычи приходится на департамент Пуно на юге Перу. До настоящего времени прибыльная добыча была возможна только в периоды высоких цен, но месторождения, как говорят, обширны, и возможно, что улучшение транспортных условий привело бы к некоторому производству в нормальных условиях.

Европа.

Австро-Венгрия.

— Наиболее важными месторождениями сурьмы старой Австрийской империи являются месторождения Венгрии и Богемии. Другие, менее значительные, находятся в Крайне, в Австрии. Венгерские месторождения в 1913 году дали 11 017 тонн руды, содержащей 1038 тонн металла; для остальной части Австрии добыча составила 1270 тонн руды, но только 89 тонн металла. Низкое содержание сурьмы в венгерских месторождениях компенсируется содержанием золота, и эти месторождения работали гораздо более регулярно, чем месторождения других частей империи. Насколько известно, запасы довольно велики, но ожидать значительного увеличения производства вряд ли стоит.

Производственная мощность как венгерских, так и богемских месторождений, вероятно, достаточна для удовлетворения местных потребностей в нормальное время и позволяет иметь излишки для экспорта, когда экономические условия благоприятны. До войны экспорт регулюса направлялся в Германию, а небольшие количества руды экспортировались во Францию и Англию. Во время войны Центральные империи, вероятно, в значительной степени зависели от австро-венгерских месторождений в плане поставок сурьмы. Все рудники находились в ведении правительства. Известно, что некоторые заброшенные рудники возобновили работу.

Франция.

— Франция является наиболее важной страной-производителем сурьмы в Европе, а также контролирует важные продуктивные месторождения в Алжире и Индокитае.

Французские месторождения многочисленны, но по большей части невелики. Самым важным из них является Ла-Люсетт в Майенне, где антимонит, ассоциированный с золотоносным пиритом, добывался в течение многих лет. Считалось, что это месторождение приближается к истощению, но, как сообщается, недавние работы позволили выявить новые рудные тела. Компания La Lucette недавно расширила свои владения в других частях Франции, приобрела объекты в Алжире и Трансваале, а в 1911 году арендовала плавильный завод в Барселоне для переработки руд, закупаемых за рубежом. Компания La Lucette также в некоторой степени связана с американской фирмой Antimony & Compounds Co. of America. Неразработанные месторождения известны в Тунисе, Марокко, Французской Гвинее и на Мадагаскаре.

Французский контроль над иностранными поставками не имеет большого значения. Помимо своих владений в Трансваале, компания La Lucette закупает некоторые иностранные руды. В 1913 году 4440 тонн сурьмяной руды было импортировано из Китая и 205 тонн из Турции. Иностранный контроль над французскими месторождениями ограничен несколькими компаниями. Итальянская компания Minière Fonderie d’Antimonio владеет концессиями во Франции и на Корсике, добыча на которых до войны составляла около 3500 тонн руды в год. Крупная бельгийская плавильная компания Société de la Vieille Montagne владеет самым продуктивным алжирским месторождением — рудником Хамман-Н’Байльс; а один неважный алжирский рудник до войны принадлежал немецкой фирме Beer, Sondheimer & Co.

В 1913 году Франция произвела 20 872 метрические тонны руды с содержанием металла около 32 процентов. Выпуск продукции плавильных заводов в 1913 году составил 6390 тонн регулюса и оксида. Франция обычно является экспортером металлической сурьмы, средний годовой экспорт за период 1910–1914 годов составлял около 2000 метрических тонн. Основными покупателями были Соединенные Штаты, Германия, Италия, Нидерланды и Россия. Согласно последней информации, избыточное производство сурьмы во Франции сейчас настолько велико, что промышленность вряд ли сможет продолжать существовать на рентабельной основе, если производители не придут к соглашению между собой. Однако ясно, что для эффективности любое соглашение между французскими производителями должно либо поддерживаться высокими защитными тарифами, либо быть расширено за счет включения их основных иностранных конкурентов.

Германия.

— В Германии добыча сурьмы слишком мала, чтобы существенно повлиять на мировой рынок, но в нескольких местах существуют возможности добычи при достаточно высокой цене на сурьму. Один завод в районе Эйфель в 1915 году производил от 25 до 30 тонн регулюса и от 60 до 70 тонн оксида в месяц. Однако существовало производство сурьмянистого свинца на плавильных заводах, которое может составлять 1000 тонн или более сурьмы в год. Это получается частично из немецких руд, особенно свинцово-цинковых, а частично из руд иностранного происхождения.

Интерес Германии к рынку сурьмы заключается главным образом в плавке и посредничестве. Среднегодовой импорт за 1910–1913 годы был следующим: руда — 3668 тонн; металл — 3398; соли — 668. Экспорт в среднем составлял: руда — 566 тонн; металл — 331; соли — 1226. Основными покупателями металла были Соединенные Штаты и Россия; а солей — Россия и Англия.

Немецкий интерес к иностранным месторождениям не был обширным. Metallgesellschaft, по-видимому, имела некоторую связь с итальянской компанией Minière Fonderie d’Antimonio, владеющей рудниками в Италии и Франции, а Beer, Sondheimer & Co. была зарегистрирована как владелец одного алжирского рудника.

Великобритания.

— Хотя месторождения ранее разрабатывались в Корнуолле, Девоне и других местах, с 1892 года в Англии сурьма не добывалась, но до войны Англия была главным центром плавки в мире, и несколько марок британской сурьмы, таких как Cookson’s и Hallett’s, имели мировую репутацию. Месторождения значительной важности существуют во многих британских владениях.

Компания Cookson & Co. из Ньюкасла контролирует рудники в районе Каторсе, Сан-Луис-Потоси, Мексика, и управляет плавильным заводом, продукция которого до 1915 года отправлялась в Англию для дальнейшего рафинирования, когда поставки были в значительной степени перенаправлены в Соединенные Штаты.

Англия через свои плавильные интересы играла важную роль в мировой торговле сурьмой. Семь плавильных заводов в Англии рафинируют руду и сырые металлы, которые поступают главным образом из Китая, а также из Мексики, Австралии и Венгрии, а во время войны — в больших количествах из Боливии и Испании. Лучшие британские марки считались более чистыми, чем другие сорта, и до войны практически монополизировали американские рынки.

Британские торговые интересы оказывали важное влияние как на обеспечение сырьем британских плавильных заводов, так и на получение рынков сбыта для британского металла. До 1914 года компания Chinese Eastern Antimony Co., дочернее предприятие Cookson & Co., имела контракты на продукцию Wah Chang Mining & Smelting Co., самого важного производителя сурьмы в Китае. В 1914 году компания Wah Chang создала независимое торговое агентство в Соединенных Штатах. Во время высокого спроса на сурьму в 1915 и 1916 годах британские интересы обеспечили большую часть продукции боливийских рудников и полностью контролировали промышленность этой страны.

Италия.

— Италия является третьим важным производителем сурьмы в Европе. Основные месторождения находятся в южной части острова Сардиния. Однако во время войны тосканские месторождения были вновь открыты, и также было небольшое производство на Сицилии. Качество руды низкое, вероятно, в среднем менее 25 процентов, и производство, которое составляло 7609 тонн руды в 1900 году, упало в 1913 году до 1822 тонн. Военные условия стимулировали промышленность, и в 1915, 1916 и 1917 годах производство составляло в среднем более 5000 тонн в год, хотя импорт металлической сурьмы также увеличился, составив: 191 тонну в 1914 году; 825 в 1915 году; 155 в 1916 году; и 1247 в 1917 году.

Низкое содержание металла в руде, а также тот факт, что в сардинских месторождениях кальцитовая пустая порода затрудняет извлечение, делают вероятным, что в условиях мирного времени и цен Италия не станет важным фактором в мировом производстве сурьмы.

Главная производственная компания, Minière Fonderie d’Antimonio, до войны была тесно связана с немецкой Metallgesellschaft, и самая богатая сардинская руда отправлялась в Германию на плавку. Помимо рудников в Италии, эта компания владела несколькими продуктивными месторождениями во Франции.

Португалия.

— В Португалии производится небольшое количество сурьмяной руды: 100 тонн в 1912 году и 19 тонн в 1913 году. Экспорт в 1916 году превысил 4000 тонн.

Россия.

— Месторождения сурьмы и серебросодержащих свинцово-сурьмяных руд известны на Урале и находились в стадии разработки в 1912 году. Месторождения сурьмы также встречаются в Амурской области и во многих местах Сибири. В 1915 году в Англию из России было импортировано 67 тонн регулюса. Возможно, однако, что это представляет собой сухопутную перевозку китайского материала.

Сербия.

— Сербия содержит несколько месторождений сурьмы, представляющих значительные перспективы. Однако производство было небольшим. Данные после 1912 года отсутствуют. Выпуск регулюса и оксида, который составлял 4725 метрических тонн в 1904 году, снизился до 297 метрических тонн в 1912 году. Большая часть продукции ранее отправлялась в Соединенные Штаты. Заводы на двух рудниках способны обеспечить значительный выпуск, если условия будут этому способствовать. Однако маловероятно, что сербские месторождения будут играть важную роль в определении контроля над мировым производством.

Испания.

— Месторождения сурьмы известны во многих местах Испании. Большинство из них нестабильны и неоднократно разрабатывались и забрасывались. Однако некоторые из них дают определенные надежды на продолжение добычи. Годовое производство едва превышало 500 метрических тонн руды, даже под влиянием военных условий (516 тонн в 1916 году и 502 тонны в 1917 году). Производство на плавильных заводах в 1916 году составило 425 тонн. Вскоре после начала войны работали три плавильных завода, самый важный из которых эксплуатировался французской компанией La Lucette.

До войны Испания ежегодно импортировала 800 тонн сурьмяной руды из Франции, а более 100 тонн солей сурьмы ежегодно экспортировалось в Германию.

Азия.

Борнео.

— Британское Борнео ранее было производителем значительной важности, и много руды экспортировалось в период между 1859 и 1894 годами, главным образом в Англию. Затем месторождения оставались бездействующими до 1914 года, когда было экспортировано 870 тонн руды; в 1915 году экспорт составил около 360 тонн. Вероятно, что при ценах мирного времени значительного производства ожидать не стоит, хотя страна в значительной степени не исследована. Компания Borneo (британская), по-видимому, была основным, если не единственным производителем.

Китай.

— Обладая всеми своими огромными минеральными ресурсами, Китай смог занять важное положение на мировых рынках лишь в отношении немногих металлов. Из них сурьма является самым ярким примером, так как с 1908 года более 50 процентов общего мирового производства сурьмы приходится на Китай. В 1913 году добыча оценивалась в эквиваленте 10 800 тонн металлической сурьмы, при том что общемировой показатель составлял около 20 000 тонн. Поскольку китайская промышленность была хорошо налажена, она смогла быстро отреагировать на огромный спрос военного времени. Экспорт увеличился с 14 361 короткой тонны регулюса и сырой сурьмы и 4795 тонн руды в 1913 году до 38 142 тонн и 8667 тонн соответственно в 1917 году.

Сурьма встречается на широко разбросанных территориях в центральных и южных провинциях, но главным образом в провинциях Хунань, Юньнань, Гуйчжоу и Гуанси. В Хунани месторождения эксплуатировались наиболее интенсивно, вероятно, 90 процентов всей добычи Китая приходится на регион вокруг Чанша, центра плавильной промышленности. Здесь, в районе Хай-Кэн-Шань, в 1915 году около 70 компаний добывали сурьму вдоль выхода месторождений на поверхность. Руда, примечательная своей чистотой, встречается в виде карманов и гнезд, главным образом антимонита, в плоском пласте доломитового известняка. Несколько местных плавильных заводов производят ликвационный сульфид, и выпуск продукции в районе составляет около 1000 тонн сырой сурьмы в месяц, содержащей в среднем около 70 процентов металлической сурьмы. Все производство регулюса контролируется компанией Wah Chang Co. В районе Панши руда встречается в виде жильных трещин в сланцах, глинистых сланцах и кварцитах. Выпуск продукции составляет около 400 тонн 30-процентной руды в месяц, вся она отправляется компании Wah Chang Co. в Чанша для переработки.

Единственный район в Юньнани, где сурьма является предметом коммерческих сделок, находится недалеко от Чицуня на Тонкин-Юньнаньской железной дороге. Компания Pao Hua Co., связанная с Wah Chang Co., владеет заводом, построенным французами, и производит высококачественный регулюс.

Компания Wah Chang Mining & Smelting Co. практически контролирует производство сурьмяной руды, регулюса и сырой сурьмы в провинции Хунань. Эта компания управляет плавильными заводами в Чанша и владеет рудниками с низкосортной рудой. Она обладает полной монополией, предоставленной пекинским правительством, на производство регулюса в Хунани и владеет патентными правами в Китае на печь Херреншмидта, наиболее успешное средство восстановления низкосортных сурьмяных руд. Сами рудники в основном принадлежат местным жителям и разрабатываются кустарным способом.

До войны экспорт китайской сурьмы находился главным образом в руках английских, французских и нескольких немецких фирм. Компания New Chinese Antimony Co. (также известная как Chinese Eastern Antimony Co.), дочернее предприятие Cookson & Co. из Англии, имела контракт на всю продукцию Wah Chang Co. Этот контракт был расторгнут вскоре после начала войны, хотя Wah Chang Co. в течение года после этого выплачивала процент со всех продаж компании New Chinese Antimony Co. Компания Wah Chang Trading Co. была организована как прямое торговое агентство в Нью-Йорке и создала крупный бизнес в этой стране.

При нынешнем высоком уровне заработной платы и цен на материалы трудно понять, как эта страна может конкурировать с Китаем в производстве сурьмы. Неблагоприятные условия обмена валюты из-за высокой цены на серебро, вероятно, почти удвоили стоимость производства в Китае, и заработная плата в этой стране выросла. Несмотря на это, однако, Китай может производить сурьму гораздо дешевле, чем это возможно в Европе или Америке; и, вероятно, также дешевле, чем в Японии.

Китайская сурьма до войны страдала от недостатка рекламы, будучи в значительной степени вытесненной с рынка этой страны британским металлом, но теперь она прочно утвердилась на наших рынках, и ее качество оказалось равным лучшим английским сортам.

Индия.

— После войны небольшие количества сурьмы производились в Бирме и Майсуре. Общая добыча индийской руды составила 1040 тонн в 1916 году и 130 тонн в 1917 году. Самым продуктивным регионом был округ Амхерст в Бирме. Здесь запасы руды, как говорят, значительны, но труднодоступность района сделала производство невозможным, за исключением периодов высоких цен. Добыча в Майсуре составила всего 26 тонн в 1916 году.

Индокитай.

— Во Французском Индокитае имеются продуктивные месторождения, возможно имеющие значение в будущем. В 1916 году они дали 1437 тонн сурьмяной руды с содержанием металла 642 тонны. Плавильные заводы эксплуатировались фирмой Schön & Rhay, перерабатывалась как местная, так и китайская руда. В 1914 и 1915 годах 883 и 630 тонн сурьмяной руды были экспортированы во Францию.

Япония.

— С момента разработки китайских месторождений в Японии добывалось очень мало сурьмяной руды, хотя, как и в большинстве других стран, во время войны наблюдалось возобновление разработки. Плавка китайских руд в Японии стала чрезвычайно важной; и производство на плавильных заводах, которое составляло всего 32 тонны в 1914 году, выросло до 8189 тонн в 1915 году и до 10 633 тонн в 1916 году. В 1917 году оно составило 6562 тонны. Производство металла и сырой сурьмы из отечественных руд составило всего 186 тонн в 1915 году и 286 тонн в 1916 году. Вероятно, что до тех пор, пока в Китае доступна дешевая руда, ожидать значительного производства из японских месторождений не приходится.

Японская собственность в китайских рудниках, вероятно, невелика, так как практически вся китайская сурьма, купленная Японией, была приобретена на открытом рынке в виде сырой сурьмы и руды. С 1914 года Япония играет важную роль в плавке китайской руды и штейна, и в этом отношении она занимала второе место после Китая. Однако до этого времени производство было незначительным. Китай сейчас находится в положении, позволяющем напрямую обеспечивать большую часть мировых потребностей в металле, значительно расширив свои мощности по переработке сурьмяных руд, и сомнительно, смогут ли японские плавильные заводы долго успешно конкурировать.

Турция.

— Добыча сурьмы в Турецкой империи ведется в Восточной Малой Азии в вилайетах Брусса и Смирна. Продуктивный район Алчар, ранее находившийся в европейской части Турции, отошел к Сербии после последней Балканской войны. Месторождения кажутся богатыми и способными к дальнейшему развитию. Плохое управление, отсутствие транспортных условий и чрезмерные экспортные пошлины, по-видимому, сдерживали производство. Некоторые рудники были собственностью Султана, и разработка затруднялась чрезмерными роялти. Большинство рудников, по-видимому, принадлежат или арендуются греками. Месторождения сурьмяных руд, ассоциированные с серебросодержащими свинцовыми рудами, сообщаются в окрестностях Карахисара в Армении. В 1914 году концессия на них принадлежала Asia Minor Mining Co., предположительно британской корпорации. Неразработанные месторождения, возможно имеющие значение, встречаются на островах Митилена и Хиос, которые сейчас находятся в греческой собственности.

Информации о производстве мало. В 1911 году рудник Джинли-Кая произвел 1500 тонн 50-процентной руды. Добыча в Малой Азии в 1912 году сообщается как 677 тонн руды. Экспорт сурьмяной руды из Турции в Великобританию был следующим: 1910 год — 303 (метрические) тонны; 1911 год — 773 тонны; 1912 год — 1108 тонн; и в 1913 году — 408 тонн. Некоторое количество руды также отправлялось в Австрию, а в 1913 году 205 тонн ушло во Францию. Кажется вероятным, что при хорошем управлении и улучшенных транспортных условиях можно было бы получить увеличенное производство из этого региона даже при ценах мирного времени, так как, согласно лучшей имеющейся информации, месторождения велики, а большая часть руды высококачественная.

Африка.

Алжир.

— Алжирские месторождения, вероятно, способны к значительному развитию, что показывает реакция на возросший спрос в 1915 и 1916 годах. Руды почти все окисленные и содержат различные редкие сурьмяные минералы. До войны основная добыча состояла из антимоната железа, добываемого вместе со свинцовыми и цинковыми рудами в Хамман-Н’Байльс. Во время войны были разработаны крупные месторождения оксидов, которые поставляли сурьму со скоростью 300 тонн в месяц в начале 1918 года. В 1912 году было произведено 4661 тонна руды; в 1913 году — 582 тонны; в 1914 году — 1100 тонн; в 1915 году — 9022 тонны, и в 1916 году — 28 473 тонны. По-видимому, добываемая руда содержит около 40 процентов сурьмы (металлическое содержание).

Рудник Хамман-Н’Байльс принадлежит крупной бельгийской плавильной компании Société de la Vieille Montagne; а компания La Lucette (французская) владеет продуктивными месторождениями оксидов Айн-Керма. До войны немецкая фирма Beer, Sondheimer & Co. была указана как владелец одного из менее важных рудников.

Британская Южная Африка.

— В Британской Южной Африке известно несколько месторождений сурьмы, наиболее перспективными из которых, по-видимому, являются месторождения хребта Мурчисон в северном Трансваале. Здесь золотоносный антимонит встречается в виде жил и метасоматических залежей в известняке на значительной площади. Добываемая руда содержит от 3 до 6 пеннивейтов золота и от 7 до 10 процентов сурьмы. Продажи и отгрузки концентрированной и сырой сурьмы были следующими: 1913 год — 48 тонн; 1914 год — ничего; 1915 год — 91 тонна; 1916 год — 722 тонны; и 1917 год — 617 тонн.

Главный рудник хребта, United Jack, был приобретен в 1917 году компанией La Lucette (французской). В 1916 году в районе было четыре действующих рудника. Месторождения сурьмы в районе Стейнсдорп, недалеко от границы со Свазилендом, находились в стадии разработки в 1916 году, а месторождения сурьмы известны в районе Форбс-Риф в Свазиленде. Сурьмяные руды встречаются на значительной части Южной Родезии, и этот район, вероятно, был бы способен к значительному выпуску продукции при лучших транспортных условиях и сохранении высоких цен. Добыча руды в 1916 и 1917 годах составила 38 и 15 тонн. Некоторые рудники, такие как Hope Fountain недалеко от Булавайо, являются главным образом золотодобывающими, сурьма является побочным продуктом.

Австралия.

— Единственным районом добычи сурьмы, имеющим какое-либо значение в Австралии, является район Костерфилд в штате Виктория. Здесь антимонит и оксиды сурьмы встречаются в кварцевых жилах, прорезающих ордовикские сланцы. Сурьмяные концентраты, которые содержат в среднем около 48 процентов сурьмы, а также около 2¹⁄₂ унций золота на тонну, отправляются в Англию. Годовое производство довольно регулярно составляет от 2500 до 3000 тонн концентратов.

Таблица 32. — Мировое производство сурьмы (1912–1917) Приблизительное содержание извлекаемого металла в добытой руде, метрические тонны; сурьмянистые свинцовые руды не включены

| 1912 | 1913 | 1914 | 1915 | 1916 | 1917 | Principal financial control
United States | 0 |  | 0 |  | 0 |  | 1,760 |  | 1,420 |  | 310 |  | United States
Canada | 0 |  | 0 |  | 0 |  | 420 |  | 300 |  | 120 |  | Great Britain
Mexico | 3,500 |  | 2,340 |  | 1,570 |  | 200 | [91] | 450 | [91] | 2,730 |  | Great Britain and United States
Bolivia | 40 |  | 30 |  | 70 |  | 7,170 |  | 9,100 |  | 7,340 |  | Great Britain
Peru | 0 |  | 0 |  | 0 |  | 260 |  | 930 |  | 450 |  | Peru
Austria-Hungary | 1,350 |  | 840 |  |  | [92] |  | [92] |  | [92] |  | [92] | Hungary
Germany | 0 |  | 0 |  |  | [92] | 700 | [91] |  | [92] |  | [92] | Germany
France | 2,290 |  | 5,170 |  |  | [92] |  | [92] |  | [92] |  | [92] | France
Italy | 310 |  | 360 |  | 110 |  | 720 |  | 1,080 |  | 960 |  | Italy
Spain | 170 |  | 0 |  | 0 |  | 100 |  | 170 |  | 160 |  | France
Portugal | 40 |  | 10 |  |  | [92] |  | [92] | 1,000 | [91] |  | [92] | ?
Serbia | 300 |  | 250 | [91] |  | [92] |  | [92] |  | [92] |  | [92] | ?
Algiers | 940 |  | 180 |  | 320 |  | 2,740 |  | 8,940 |  |  | [92] | France
British S. Africa | 0 |  | 30 |  | 0 |  | 50 |  | 380 |  | 300 |  | Great Britain and France
China | 10,800 |  | 11,000 |  | 15,900 |  | 10,500 |  | 42,800 |  | 31,000 |  | China (Japan), Great Britain?
Japan | 70 |  | 20 |  | 30 |  | 180 |  | 280 |  |  | [92] | Japan
India | 0 |  | 0 |  | 0 |  | 0 |  | 400 |  | 50 |  | Great Britain
Indo-China | 110 |  | 0 |  | 0 |  | 160 |  | 510 |  |  | [92] | Great Britain
Borneo | 0 |  | 0 |  | 300 |  | 120 |  |  | [92] |  | [92] | Great Britain
Asia Minor | 270 |  | 240 |  |  | [92] |  | [92] |  | [92] |  | [92] | Turkey (Greece)
Victoria | 580 |  | 960 |  | 890 |  | 1,300 |  | 1,320 |  |  | [92] | Great Britain
New South Wales | 30 |  | 10 |  | 20 |  | 320 |  | 310 |  | 150 |  | Great Britain
Queensland | 0 |  | 0 |  | 0 |  | 80 |  | 80 |  |  | [92] | Great Britain
West Australia | 0 |  | 0 |  | 0 |  | 0 |  | 20 |  | 10 |  | Great Britain
Total | 20,800 |  | 21,440 |  | 24,400 | [93] | 35,400 | [93] | 78,700 | [93] | 54,300 | [93] |

[91] Неполные данные; фактическое производство, вероятно, больше.

[92] Данные отсутствуют.

[93] Итоговые показатели за 1914–1917 годы включают оценки производства стран, по которым данные отсутствуют.

Район Хиллгроув в Новом Южном Уэльсе ранее имел значительную важность, максимальный годовой объем добычи составил 2450 тонн руды в 1906 году. Недавнее производство было незначительным, и хотя под влиянием военных цен произошел очень большой рост, стоимость продукции 1917 года составила лишь около 5 процентов от стоимости продукции штата Виктория. Незначительные количества сурьмяной руды недавно добывались в Квинсленде и Западной Австралии. Новая Зеландия дала небольшое количество во время бума 1906 и 1907 годов, но с 1910 года производство не регистрировалось.

Imports of antimony ore into Great Britain from Australia in 1915 amounted to 3,854 tons.

Статистические данные о производстве (1912–1917) приведены в предыдущей таблице.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ НАЦИЙ

Соединенные Штаты.

— Соединенные Штаты являются крупнейшим потребителем сурьмы в мире, требующим в нормальных условиях от 7000 до 8000 тонн нового металла, большая часть которого до войны поступала из Англии. Потребление во время войны было примерно вдвое больше этого количества и обеспечивалось главным образом за счет Востока, Южной Америки и Мексики. Соединенные Штаты должны оставаться зависимыми от иностранных источников поставок, если на импорт не будут наложены гораздо более высокие тарифы. Даже при таких условиях сомнительно, чтобы отечественные рудники оказались способны удовлетворить более чем малую часть потребностей страны.

Китайская и японская сурьма в значительной степени заменила британский продукт с 1914 года и настолько прочно утвердилась, что, вероятно, продолжит удерживать американские рынки. Китайская сурьма, в частности, показала себя во всех отношениях равной лучшим британским сортам. При несколько более высоком уровне цен импорт руды из Мексики и Южной Америки может быть осуществлен перерабатывающими заводами в этой стране, поскольку опыт, накопленный несколькими компаниями во время войны, сделал возможным производство высококачественного металла.

Англия.

— Данные о фактическом потреблении сурьмы в Англии отсутствуют. Судя по балансу импорта и экспорта, нормальное потребление составляет около 4500 тонн в год. Во время войны потребление было колоссально увеличено для производства боеприпасов. Английские плавильные заводы полностью зависят от иностранных руд, большая часть которых в прошлом поступала из Китая, с меньшими количествами из Мексики и Австралии. Положение отрасли, по крайней мере в том, что касается экспортной торговли, находится под угрозой из-за сильных позиций китайской промышленности, приобретенных во время войны, что особенно представлено деятельностью Wah Chang Mining & Smelting Co. Две трети английского экспорта сурьмы направлялись в Соединенные Штаты до 1914 года. Не кажется вероятным, что Англия сможет полностью вернуть этот рынок, который сейчас полностью доминируется китайской и японской сурьмой.

Франция.

— Франция — единственная мировая держава, обладающая важными ресурсами сурьмы в своих границах. Включая свои алжирские рудники, она полностью независима от внешних поставок. Поскольку некоторые из французских месторождений содержат значительные количества золота, а основной алжирский рудник содержит свинец и цинк, производство сурьмы во Франции, вероятно, будет продолжать иметь некоторое значение, и вероятно, что она продолжит экспортировать сурьму, как и до войны, хотя, вероятно, в меньшей степени.

Германия.

— Германия до 1914 года потребляла около 20 процентов мирового годового производства сурьмы. Ее собственные ресурсы сурьмы незначительны, а немецкие интересы в иностранных месторождениях не были широко распространены, а скорее заключались в плавке и посредничестве, при этом сырье поступало главным образом из Китая, а металл и соли экспортировались в Соединенные Штаты, Россию и Великобританию. Во время войны Германия в значительной степени опиралась на Венгрию в плане поставок сурьмы, но известно, что этот источник не мог адекватно удовлетворить спрос.

Япония.

— Фактическое потребление сурьмы в Японии никогда не было большим и до войны ограничивалось главным образом производством коробок, подносов и других изделий из «белого металла». Во время войны ее значение в торговле сурьмой основывалось на способности удовлетворять значительную часть потребностей союзников, главным образом России, а позже Соединенных Штатов и Канады. Как долго после войны она сможет сохранить свои позиции — неизвестно. Благоприятные фрахтовые ставки для японских грузоотправителей и тот факт, что нынешняя высокая цена на серебро и вытекающие из этого условия обмена валюты неблагоприятно влияют на китайское производство, могут позволить Японии оставаться фактором в торговле сурьмой.

НЕДАВНИЕ УСЛОВИЯ В ПРОМЫШЛЕННОСТИ

Из-за очень высоких цен на сурьму в 1915 и 1916 годах, вызванных значительно возросшим спросом на сурьму для производства боеприпасов, несколько стран стали крупными производителями. Наиболее важными среди них были Боливия, Мексика и Алжир, но Виктория и Соединенные Штаты, Перу, Бирма и Испания также внесли существенные вклады. За возможным исключением Алжира — чьи основные рудники дают значительное количество свинца и цинка и расположены недалеко от французских перерабатывающих заводов — и Мексики, ни одна из этих стран не будет важным фактором в производстве сурьмы при обычных низких ценах, преобладающих на этот металл.

Внезапное окончание войны застало воюющие стороны с большими запасами сурьмы на руках; англичане, согласно цифрам, опубликованным Британским министерством боеприпасов 1 марта 1919 года, имели 4325 длинных тонн регулюса. Есть основания полагать, что у других союзников были запасы того же порядка величины, и если это так, то к 1 апреля 1919 года должно было быть доступно около годового запаса, так как потребление сурьмы в 1913 году составляло всего около 20 000 тонн. Кроме того, имелись большие запасы сплавов и сурьмянистого свинца, и, несомненно, больше будет получено в результате спасательных операций. Поэтому можно ожидать, что до тех пор, пока они не будут поглощены, производство сурьмы будет даже меньше, чем в довоенные годы. В настоящее время стимулов для добычи мало. Затраты на добычу выросли повсюду. Китай, крупнейший производитель, сталкивается с особенно трудной ситуацией, так как более высокая цена на серебро привела к удвоению затрат на рабочую силу и местные материалы. Если цены на серебро останутся высокими после того, как спрос на первичную сурьму восстановится, другие страны-производители сурьмы, не находящиеся на серебряной основе, будут иметь соответствующее преимущество перед Китаем в вопросе производства.

РЕЗЮМЕ

Потребление сурьмы в мирное время ограничено скорее относительно узкими сферами ее применения, нежели недостатком потенциальных запасов. Как следствие, стабильная добыча поддерживалась только в тех районах, где эксплуатационные расходы невелики, рынки сбыта легкодоступны или месторождения содержат другие ценные металлы. Однако современная война создает особый спрос на сурьму — для производства шрапнели, — что требует количества сурьмы, во много раз превышающего необходимое для обычных мирных целей. В ходе каждой из трех крупных войн последних двадцати лет — англо-бурской, русско-японской и Великой войны — кривые цен на сурьму и объемов ее производства резко поднимались в соответствии со спросом и столь же быстро падали после того, как потребность в боеприпасах исчезала.

Китай долгое время был важнейшим источником сурьмы и, несомненно, сохранит эту позицию на многие годы. Стабильная, хотя и менее значительная добыча велась во Франции, Австро-Венгрии и Мексике, в то время как ряд других стран производили значительные объемы в результате существенно возросшего спроса военного времени. Среди них главными были Боливия, Алжир и Австралия.

До 1914 года Англия доминировала на рынке сурьмы благодаря своим крупным интересам в области плавки, торговым соглашениям на Востоке и сбытовым агентствам в Америке — основной стране-потребителе. Однако с того времени китайские интересы стали независимыми, а Япония приобрела важное значение в сфере плавки и торговли сурьмой.

Соединенные Штаты обладают ограниченными ресурсами сурьмы, которые могут эксплуатироваться только при очень высоких ценах, и почти полностью зависят от внешних источников поставок. В прошлом эти поставки в значительной степени осуществлялись из Англии, но в последнее время — из стран Востока и Мексики.

Германия имеет незначительные собственные ресурсы сурьмы и во время войны зависела от поставок из венгерских месторождений, которые, по-видимому, были недостаточны для удовлетворения спроса. Ее интересы до войны были связаны главным образом с плавкой и посреднической деятельностью и не распространялись в значительной степени на зарубежные месторождения.

Соединенные Штаты, Франция, Германия и Великобритания обычно потребляют 85 процентов мировой сурьмы, и из них только Франция независима от внешних источников поставок.

Мировая торговля сурьмой в значительной степени контролируется несколькими компаниями, наиболее важными из которых являются: Cookson’s (британская), Wah Chang Co. (китайская) и Société de La Lucette (французская). Компания Mitsui Co. (японская), в основном через судоходные интересы, имеет значительную долю в торговле сурьмой в Китае и Японии.

ГЛАВА X МОЛИБДЕН Р. Б. Мур

ПРИМЕНЕНИЕ МОЛИБДЕНА

Молибден используется в производстве ферросплавов для изготовления стали. В виде проволоки он применяется для поддержки нити накала в лампах электрического освещения. Проволока также используется для обмотки электрических печей сопротивления и для этой цели оказалась дешевле и лучше платины благодаря более быстрому нагреву и возможности достижения более высоких температур. Металл успешно заменяет платину и платино-иридиевые сплавы в устройствах для электрических контактов. Соединения молибдена используются в химии, в частности молибдат аммония для определения фосфора. Стойкие красители различных оттенков могут быть получены на коже при использовании молибденового таната в сочетании с экстрактами кампешевого дерева. Он применялся для цветных глазурей в фарфоре, а также при окрашивании шелка и резины.

Добавление молибдена в сталь повышает предел упругости, не снижая пластичности. Молибден может заменять определенный процент вольфрама в быстрорежущей стали, как правило, одна часть молибдена заменяет от двух до трех частей вольфрама.

ГЕОЛОГИЧЕСКОЕ И ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Примерно до 1916 года практически весь производимый молибденовый концентрат поступал из Квинсленда, Нового Южного Уэльса и Норвегии. Вскоре после начала войны проявился интерес к добыче молибденита в Канаде, главным образом в провинциях Онтарио и Британская Колумбия. В течение 1917 и 1918 годов в Соединенных Штатах возник большой интерес к молибденовым рудам, и в настоящее время эта страна, вероятно, может производить молибденовый концентрат в количестве, равном, если не превышающем, объем производства остального мира вместе взятого. Некоторое количество молибдена производится Испанией и Перу.

Австралия и Норвегия.

Первая официальная запись о добыче молибденита в Квинсленде относится к 1900 году, когда объем производства составил 12,3 коротких тонны высококачественного материала. Производство постепенно выросло до 119 тонн в 1906 году и с тех пор существенно не менялось, хотя отпускные цены на концентраты значительно выросли. Основная часть материала добывалась в Вольфрам-Кэмпе, на месторождении Чиллаго, в 120 милях к юго-западу от Кэрнса, в Северном Квинсленде. Рудникам в Бэмфорде, на том же месторождении, приписывается небольшой объем добычи. Вместе с молибденитовыми рудами встречаются висмутово-вольфрамовые руды, поэтому добываются все три металла.

Добыча молибденита была впервые зафиксирована в Новом Южном Уэльсе в 1902 году; в том году объем производства составил 17 коротких тонн. Общий объем производства до конца 1914 года составил 498 коротких тонн стоимостью 264 000 долларов. Основные молибденитовые рудники находятся в Уипстике (округ Памбула), в Кингсгейте (округ Глен-Иннес) и недалеко от Дипуотера (округ Дипуотер). Молибденит также добывается в Рокки-Ривер (округ Тантафилд) и в округе Батерст. Добыча во всех этих местах была невелика — ни в один год она не превышала 100 тонн концентрата.

В Норвегии производство высококачественного молибденового концентрата составляло в среднем около 30 тонн в год с 1902 года. В 1906 году был зарегистрирован объем производства 1 129 коротких тонн. Вероятно, это относится к добытой руде, а не к произведенному концентрату.

Основные молибденитовые районы Норвегии — это провинции Листер, Мандал и Неденес на самой южной оконечности полуострова. Район Фьотланд в первой из названных провинций, вероятно, богаче молибденитом, чем любой другой из обнаруженных в Норвегии. Рудник в Кнабене в этом районе был крупнейшим и, вероятно, единственным успешным производителем в Норвегии. Этот рудник, принадлежащий компании George G. Blackwell & Sons из Ливерпуля, Англия, имел средний объем производства около 25 коротких тонн в год.

[94] Сообщается, что перешел к норвежской компании. U. S. Commerce Reports, 24 сентября 1918 г.

Таблица 33. — Производство молибденита в Квинсленде, Новом Южном Уэльсе и Норвегии

Year | Queensland | New South Wales | Norway
Weight (short tons) | Value (dollars) | Weight (short tons) | Value (dollars) | Weight (short tons) | Value (dollars)
1902 |  45.9 |  26,770 | 16.8 | 8,960 |    22 | 16,100
1903 |  26.9 |  10,220 | 32.5 | 21,960 |    34 | 21,400
1904 |  23.6 |  13,010 | 28.3 | 13,270 |    33 | 17,400
1905 |  70.8 |  41,340 | 21.7 | 12,200 |    51 | 16,300
1906 | 118.9 |  74,330 | 36.6 | 23,350 | 1,129 | 14,200
1907 |  74.0 |  41,080 | 24.2 | 17,340 |    33 | 12,900
1908 |  98.7 |  44,960 |  9.5 |  4,520 |    39 | 13,400
1909 | 103.9 |  45,120 | 31.5 | 15,810 |    33 | 12,100
1910 | 118.6 |  58,640 | 53.2 | 27,580 |  |
1911 | 111.4 |  64,610 | 23.1 | 12,610 |     2 |   800
1912 | 114.6 |  84,420 | 63.3 | 18,030 |    23 | 5,400
1913 |  74.3 |  92,460 | 88.3 | 33,100 |    13 | 3,200
1914 |  87.1 | 185,830 | 68.8 | 55,720 |  |

Производство молибденита в Квинсленде, Новом Южном Уэльсе и Норвегии по годам показано в предыдущей таблице.

Данные за более поздние годы указывают на общий объем производства в Австралии около 330 коротких тонн в год и 110 коротких тонн в Норвегии в 1916 году. В 1917 году объем производства в Норвегии был в три раза выше показателей 1916 года.

Северная Америка.

Как уже было сказано, основные месторождения молибденита в Канаде находятся в провинциях Онтарио и Британская Колумбия. Они являются низкосортными и, конечно, требуют обогащения. Канадское и британское правительства проявляли большой интерес к обогащению этих руд, и канадское правительство имеет фабрику, занимающуюся экспериментальной работой и коммерческим обогащением. Департамент горнодобывающей промышленности потратил много времени на эксперименты, полагая, что молибденит имеет важное будущее в металлургии.

Производство в 1917 году составило около 80 коротких тонн высококачественного концентрата и, несомненно, было больше в 1918 году.

Канада при надлежащей разведке может производить гораздо больше молибденита, чем сейчас.

В Соединенных Штатах имеется очень большое количество мелких молибденовых месторождений, разбросанных по западным штатам от Вашингтона до Аризоны и от Колорадо до Калифорнии. Существует два распространенных минерала — молибденит, или сульфид молибдена, и вульфенит, или молибдат свинца. Вообще говоря, молибденит встречается в северных штатах, а вульфенит — в южных, но это правило не без исключений. В Аризоне и Нью-Мексико основным минералом является вульфенит, но есть и довольно крупные месторождения молибденита, вероятно, лучшие из которых находятся на рудниках Leviathan в Медном каньоне, округ Мохаве, Аризона. Это единственное месторождение молибденита, которое разрабатывается в Нью-Мексико или Аризоне. Оно находится в горнодобывающем районе Сидар-Вэлли, примерно в трех милях к юго-востоку от Коппервилля и примерно в 25 милях к востоку от Юкки. Эта руда содержит много меди, а также небольшие следы золота и серебра. Некоторые анализы показали 2 или 3 процента MoS2 и от 1,5 до 2 процентов меди с 0,02 унции золота и от 1 до 4 унций серебра на тонну. Процентное содержание молибденита, несомненно, выше среднего, которое не превышает 1 процента. Вмещающая порода — среднезернистый серый гранит, состоящий из кварца, полевого шпата, биотита, мусковита и небольшого количества других акцессорных минералов, таких как циркон и апатит. Компания построила фабрику и успешно осуществила удовлетворительное отделение меди от молибденита.

Наибольшие возможности в Аризоне и Нью-Мексико связаны с добычей вульфенита. Этот минерал широко распространен в этих двух штатах, особенно в Аризоне, и в значительной степени ассоциирован с ванадинитом. Одной из самых больших трудностей при обогащении вульфенита было отделение его от ванадинита. Бюро горнодобывающей промышленности некоторое время работало над этой проблемой с частичным успехом.

Самое важное месторождение вульфенита находится на рудниках Mammoth и Collins в округе Пинал. Первоначально это были золотые рудники, и когда ценность молибдена стала очевидной, полковник Рэндольф, владелец рудника Mammoth, решил, что стоит переработать отвалы хвостов на вульфенит. Он переоборудовал свою фабрику для этой цели и переработал не только отвалы Mammoth, но и отвалы старого рудника Yuma в округе Пима. Общее количество концентратов, произведенных полковником Рэндольфом и другими лицами в этом районе в течение трех лет с 1916 по 1918 год, вероятно, составляет от 1000 до 1200 тонн вульфенитового концентрата. В то время как эти операции продолжались, они представляли практически единственное производство молибденовых концентратов в этой стране, за исключением очень мелких масштабов. Еще одна действующая компания — Rowley Copper Mines Co., Гила-Бенд, Аризона, руда которой представляет собой вульфенит, а основной примесью является барит. Компании удалось получить удовлетворительные концентраты, которые, однако, содержат значительное количество барита. Станция Бюро горнодобывающей промышленности в Голдене, штат Колорадо, провела некоторые испытания этого концентрата и осуществила частичное разделение барита и вульфенита.

Молибденит встречается в значительном количестве мест в Колорадо, Монтане, Вашингтоне, Неваде, Юте, Техасе и других западных и северо-западных штатах, но крупнейшее месторождение находится в Колорадо. Вообще говоря, отдельные месторождения на Западе недостаточно велики, чтобы оправдать строительство фабрики для любого из них, а поскольку месторождения широко разбросаны, трудно найти место, где заказная фабрика могла бы получать достаточное количество руды. Это одна из главных трудностей в производстве большого тоннажа молибденитовых концентратов за пределами Колорадо.

Вероятно, крупнейшие месторождения молибденита в мире находятся в Клаймаксе, штат Колорадо. Эти месторождения расположены на юго-западном склоне горы Бартлетт, округ Саммит, примерно в 15 милях от Ледвилла. Обнажения практически непрерывны по всей длине горы и местами достигают ста-двухсот футов в толщину. Руда представляет собой скорее зернистый, чем чешуйчатый молибденит, среднее содержание составляет около 8 процентов MoS2.

Существуют две действующие компании: Climax Molybdenum Co., дочерняя компания American Metal Co. из Нью-Йорка и Денвера, и Molybdenum Products Co. из Денвера. Обе эти компании построили фабрики с суточной производительностью 200 тонн. Фабрика American Metal Co. начала непрерывную работу примерно в марте 1918 года, а фабрика другой компании была завершена вскоре после этого. Обе компании заявляют, что могут увеличить мощность в короткие сроки. Автор был на руднике American Metal Co. Очевидно, что значительная часть горы состоит из молибденита, и, без сомнения, может быть добыт очень большой тоннаж. Интересы Джеклинг недавно приобрели прилегающие объекты, принадлежащие Pingree Mines Co., но в 1918 году не построили фабрику и не проводили никаких серьезных работ по освоению.

Еще одна очень большая группа месторождений молибденита находится недалеко от Эмпайра, округ Клир-Крик, Колорадо, на восточном склоне Красной горы, на высоте около 11 000–12 000 футов. Месторождения находятся в 14 милях от станции Эмпайр железной дороги Colorado & Southern и принадлежат Primos Chemical Co. из Примоса, Пенсильвания. Рудные тела состоят из трех жил низкосортной руды. Рудная зона, то есть площадь, заключенная между лежачим боком жилы № 1 и висячим боком жилы № 3 в месте пересечения туннелем, имеет ширину около 200 футов. Жилы сильно различаются по ширине и не особенно хорошо выражены, тонкие прожилки и штокверки руды уходят в боковые породы. Primos Chemical Co. разрабатывала эти рудники с перерывами в течение нескольких лет. Около трех лет назад она построила фабрику рядом с рудником, но производство было довольно прерывистым. Эта компания, вероятно, использовала все свои концентраты для производства ферромолибдена на собственных заводах в Примосе, Пенсильвания.

Небольшая фабрика была построена в Питкине, Колорадо, в связи с рудником в этом месте, принадлежащим Pennsylvania Molybdenum Mines Co. из Джонстауна, Пенсильвания. Ряд других месторождений, представляющих значительный интерес, найдены в Колорадо, особенно вокруг Брекенриджа, округ Саммит. Здесь пегматитовые жилы состоят в основном из мусковита и кварца с некоторым количеством полевого шпата и содержат биотит, халькопирит и акцессорные минералы. Трудность здесь заключается в отделении молибдена от медных минералов, а также от слюды, большая часть которой всплывает вместе с молибденитом.

Большинство разведанных молибденовых месторождений Мексики находятся в штате Сонора. В районе Сахуарипа в восточной Соноре минерал встречается вместе с шеелитом в богатых гнездах, содержащих очень крупные куски чистого минерала. Некоторое количество молибденовой руды было отправлено из медного района Монтесума в Empire Smelting & Refining Co. из Деминга, Нью-Мексико. О наличии молибдена сообщается в нескольких других местах Соноры. Рядом с Койаме и Маркесом, северо-восточная Чиуауа, рудники Compañia Minera Aurora y Anexas производят молибденовую руду. Вульфенит обильно встречается вместе со свинцовой рудой на руднике Cuchillo Parado в том же районе. Медный рудник Jibosa компании American Smelters Securities Co., недалеко от Хименеса, Чиуауа, по-видимому, содержит значительное количество оксида молибдена, молибдита. В настоящее время он не является коммерческим.

Месторождения молибденита также зарегистрированы в штатах Синалоа, Оахака, Идальго и Халиско.

ЗАПАСЫ

Поскольку добыча молибденовых руд в прошлом во всех странах была относительно небольшой, вероятно, ни одно из месторождений не было исчерпано, и можно получить увеличенный объем добычи. Это особенно относится к Соединенным Штатам. Вся работа, которая была проделана до сих пор, велась на экспериментальной основе, и, возможно, единственный рудник, чей тоннаж будет уменьшен в результате прошлой добычи, — это рудник Mammoth недалеко от Мэммота, Аризона, и нет уверенности, что этот рудник не сможет продолжать производить столько же в течение некоторого времени в будущем, сколько он производил во время своего периода эксплуатации. Каков именно объем добычи может быть получен в Соединенных Штатах, несколько неопределенно, но вполне вероятно, что месторождения в Клаймаксе, Колорадо, будут давать не менее тысячи тонн руды в день в течение нескольких лет, а возможно, и в течение многих лет. Месторождения Primos Chemical Co. недалеко от Эмпайра, Колорадо, также обширны и должны давать большой объем добычи в течение некоторого времени. Остальные упомянутые месторождения малы по сравнению с этими двумя, но общий объем добычи всех их мог бы быть большим, если бы был обеспечен стабильный рынок и построены заказные фабрики.

ОБРАБОТКА РУД

При обогащении вульфенитовых руд обычно используется какая-либо форма концентрации на столах с добавлением шламовых аппаратов. Металлургическая обработка концентратов варьируется и все еще находится на экспериментальной стадии. Существует возможность разработки процесса, который даст патентообладателю значительное преимущество перед конкурентами. Бюро горнодобывающей промышленности работало над этой проблемой и недавно разработало метод, который кажется столь же эффективным, как и любой другой, и, возможно, имеет некоторые дополнительные преимущества.

При обработке молибденита почти повсеместно используются одни и те же методы. Сначала руда измельчается до требуемой тонкости, и молибденит отделяется флотацией, в основном масляной флотацией. Металлургия концентрата, теперь более или менее стандартизированная, включает обжиг концентрата до оксида и обработку этого оксида в электрической печи для производства ферромолибдена. При небольших улучшениях эта практика, вероятно, сохранится еще некоторое время.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Политический контроль над молибденовыми месторождениями мира определяется географическим положением. В настоящее время большинство известных месторождений контролируется Соединенными Штатами и Великобританией, причем последняя контролирует месторождения в Канаде и Австралии. Британское и канадское правительства фактически имеют государственную фабрику в Канаде.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Рудники Кнабен во Фьотланде, самые известные и, вероятно, единственные успешные молибденовые рудники в Норвегии, были приобретены в 1905 году английской компанией Blackwell Developing Corporation. Позже вновь организованная норвежская компания с головным офисом в Христиании приобрела рудники по цене 2 500 000 крон.

В Мексике крупное молибденовое месторождение в районе Сахуарипа в восточной Соноре принадлежит Джорджу Фасту из Дугласа, Аризона. Lucky Tiger-Combination Gold Mining Co. из Канзас-Сити, Миссури (американская), владеет месторождениями в районе Монтесума. Другая американская компания приобрела месторождения недалеко от Позы, Сонора, примерно в 20 милях к северу от Эрмосильо. Месторождение, расположенное в 35 милях от порта Тополабампо, северо-западная Синалоа, принадлежит американцу. Compañia Minera Aurora y Anexas, эксплуатирующая молибденовые рудники недалеко от Койаме и Маркеса, северо-восточная Чиуауа, принадлежит наследникам Мадеро. Руда отправлялась Леонарду Вустеру, Эль-Пасо, Техас, агенту наследников, а также закупщику для L. Vogelstein & Co., Нью-Йорк, ранее филиала немецкого металлургического объединения.

В Соединенных Штатах во время войны неоднократно заявлялось, как в частном порядке, так и в прессе, что немецкие интересы пытаются получить контроль над молибденовыми месторождениями страны. Это было связано с тем, что American Metal Co., которая работает в Клаймаксе, Колорадо, как Climax Molybdenum Co. и имеет некоторые другие молибденовые месторождения, ранее контролировалась немецкими интересами. Это правда, что большинство акций American Metal Co. принадлежало Германии, но г-н Палмер, Управляющий имуществом иностранцев, взял на себя управление этими акциями, и дела American Metal Co. были приведены в соответствие с изменившимися условиями. Основными акционерами Primos Chemical Co. были четыре брата по фамилии Берике. До войны они имели сильные немецкие связи, но, помимо своих месторождений в Эмпайре, они не предпринимали особых усилий, чтобы получить крупные молибденовые активы в этой стране, и не стремились к объединению каких-либо действующих компаний. Primos Chemical Co. с 1919 года была поглощена Vanadium Products Corporation, аффилированной с Bethlehem Steel Corporation. Molybdenum Products Co., Денвер, Колорадо, которая владеет частью молибденового месторождения на склоне горы Бартлетт, недалеко от Клаймакса, и эксплуатирует 200-тонную фабрику, является дочерней компанией E. J. Longyear Co., инженерно-разведочной компании из Миннеаполиса, Миннесота. Обе компании принадлежат американским акционерам.

В Канаде и Австралии несомненно то, что ни один крупный интерес не имеет контроля, так как руда поступает с ряда более или менее независимых мелких рудников.

В связи с концентрацией и металлургией молибдена было выдано большое количество патентов. Ни один из них не является жизненно важным для производства; большинство из них бесполезны, и даже те, которые имеют отчетливую ценность, не обязательно дают контроль владельцу патентов или секретных процессов.

Для обеспечения стабильного спроса на молибден главным требованием является четкое знание свойств и способов использования молибденовой стали. В прошлом этого не хватало, и в настоящее время этим не обладают большинство операторов и производителей стали. Европа должна существенно помочь в восполнении этого пробела. Молибденовая сталь в настоящее время находится в том же положении, что и ванадиевая сталь несколько лет назад — она проходит испытания. Эта неопределенность вызвала очень решительный спад спроса на молибденовые концентраты весной 1918 года. Контроль над молибденом скорее придет через производство молибденовой стали, чем через процессы, связанные с производством концентратов или ферромолибдена.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ НАЦИЙ

В настоящее время Соединенные Штаты имеют самый большой потенциальный запас молибденовых руд среди всех стран мира. Кроме того, у них есть три из крупнейших и самых современных фабрик, которые обрабатывают руду с любого молибденового месторождения. Страна находится в благоприятном положении, чтобы в течение некоторого времени сравняться или превзойти любую другую страну по объему производства молибденовых концентратов.

До войны Великобритания, благодаря политическому контролю над австралийскими и канадскими месторождениями, была ведущим мировым производителем. Некоторое количество молибдена поступало из Норвегии, но объем был невелик по сравнению с объемом производства Австралии: Норвегия в 1913 году произвела всего 13 коротких тонн, а Австралия — 162,6. Как в Канаде, так и в Австралии известные месторождения не были полностью освоены, и при надлежащей разведке, вероятно, будут обнаружены новые месторождения, так что будущее производство молибдена под британским контролем обещает увеличиться. Канадское и британское правительства очень заинтересованы в развитии молибденовых ресурсов доминиона.

Франция полностью зависит от Англии и Соединенных Штатов, хотя, возможно, могла бы получать небольшое количество концентратов непосредственно из Норвегии.

Германия до войны очень интересовалась молибденом. Во время войны она, вероятно, вообще не импортировала молибденовые концентраты, и, поскольку мировое производство до этого времени было небольшим, маловероятно, что в империи в 1919 году были какие-либо запасы.

Япония, насколько известно, не имеет молибденовых месторождений и, вероятно, в настоящее время не особенно заинтересована в использовании этого металла.

Распределение основных молибденовых месторождений мира показано на Пластине VII.

Пластина VII. — Географическое распределение молибденовых месторождений мира. Р. Б. Мур.

РЕЗЮМЕ

Молибден привлекает внимание из-за своей растущей важности как металла для легирования стали. Хотя металлургия и свойства молибденовых сталей не до конца изучены, а их использование не является широко распространенным, особенно в этой стране, накапливающиеся данные свидетельствуют о том, что молибден со временем станет одним из обычных легирующих металлов. Он используется в виде проволоки в качестве опор для нитей накала ламп накаливания и в электрических аппаратах, и может стать незаменимым в производстве специальных сталей. Его нельзя легко заменить в химии, а для других применений он лучше и дешевле других материалов.

До 1915 года практически весь производимый молибден поступал из Квинсленда, Нового Южного Уэльса и Норвегии. В настоящее время более важные месторождения разрабатываются в Онтарио, Квебеке и Британской Колумбии, Канада, а также в Колорадо, Аризоне, Нью-Мексико и других западных штатах. Минерал широко распространен, и открытие дополнительных месторождений вероятно, если спрос будет достаточным для стимулирования разведки. Соединенные Штаты имеют месторождения, достаточно большие, чтобы удовлетворить все внутренние потребности, а также производить излишки для экспорта. Некоторое количество молибдена получается из Мексики, Перу и Испании, но Соединенные Штаты, Великобритания (Канада и Австралия) и Норвегия контролируют важные месторождения.

Крупнейшее молибденовое месторождение в Соединенных Штатах, расположенное в Клаймаксе, Колорадо, принадлежит Climax Molybdenum Co., дочерней компании American Metal Co. (ранее немецкой), и Molybdenum Products Co. из Денвера, американской компании. Другие месторождения в Колорадо принадлежат Primos Chemical Co., компании, которая до войны имела сильные немецкие связи, но была поглощена Vanadium Products Corporation, американской компанией. Другие производящие месторождения Соединенных Штатов принадлежат американским гражданам.

Рудники Кнабен, самые важные в Норвегии, с 1905 года принадлежали английской компании, но, согласно отчету, они были приобретены норвежской компанией. Ряд месторождений северной Мексики принадлежит американцам. Другие принадлежат наследникам Мадеро (мексиканским). Канадские и австралийские месторождения контролируются мелкими независимыми операторами. Как Соединенные Штаты, так и Великобритания имеют достаточные запасы молибдена; Франция не производит его и зависит от других стран; Германия, которая до войны очень интересовалась молибденом, вероятно, не имеет больших запасов на руках.

ГЛАВА XI РАДИЙ И УРАН Р. А. Ф. Пенроуз-младший

Радий — это металл, являющийся продуктом естественного распада металла урана. И радий, и уран являются элементами. Радий был выделен в своем металлическом состоянии, но в этой форме не используется и более известен в виде своих солей, среди которых наиболее важными с точки зрения их применения являются бромид, хлорид и сульфат.

Везде, где уран встречается в природе, радий ассоциирован с ним в определенных определяемых количествах. Однако уран может содержать только определенное максимальное количество радия в данный момент времени, и когда он достигает этой стадии, говорят, что соотношение радия и урана находится в равновесии. В этом состоянии количество радия на грамм урана, по расчетам Резерфорда, составляет 3,4 × 10⁻⁷ грамма. Это соответствует 1 грамму элемента радия на примерно 3000 килограммов элемента урана, или 1 части элемента радия на примерно 3 000 000 частей элемента урана. Урановые минералы в добытом виде обычно нечисты и содержат лишь небольшой процент элементов урана, поэтому соотношение между радием и сырой урановой рудой может составлять от 1 к нескольким или многим раз по 3 000 000.

Производство радия из урана обычно указывается в миллиграммах или граммах, и даже в самых богатых рудах обычно содержится лишь небольшая доля грамма на тонну, в то время как в обычной низкосортной руде содержится лишь несколько миллиграммов на тонну, что соответствует небольшой доле грана на тонну. Менее двадцати лет назад оценивалось, что в мире, вероятно, не было добыто и одного грамма элемента радия в виде его очищенных солей. Сегодня это количество было добыто во много раз, возможно, в сто или более раз, и находится в использовании. Ежегодное производство радия в мире сегодня, вероятно, составляет несколько граммов. Ежегодное производство урана в мире, вероятно, составляет несколько сотен фунтов.

Уникальное положение урана как источника радия в природе делает необходимым обсуждение обоих материалов вместе.

Применение радия.

Радий — это тяжелый белый металл, который очень нестабилен и быстро изменяется на воздухе. Он не используется в металлическом состоянии, а только в виде своих солей. Несколько лет назад предполагалось, что эти соли оказывают общее благотворное влияние при лечении рака и других злокачественных новообразований, но более поздние исследования, по-видимому, ограничивают их влияние только определенными формами этих недугов. Их влияние при других болезненных состояниях часто очень заметно, но полная степень области полезности радия для медицинских целей еще не была очень четко определена.

В последние годы радий стал применяться для других важных целей, особенно в светящихся красках для часов, компасов и других инструментов; и это использование настолько сильно возросло в последние годы, особенно для военных целей, что сейчас потребляет больше радия, чем используется в медицине. Соли радия более или менее светятся, если смотреть на них в темной комнате, и это качество часто усиливается добавлением некоторых других материалов, особенно сульфида цинка. Отсюда их ценность в светящихся красках. Соли радия также вызывают флуоресценцию некоторых минералов, особенно цинковых минералов виллемита и сфалерита. В Германии, где радий во время войны стал дефицитным из-за нехватки руд, из которых он извлекается, соли радия, как говорят, сохранялись для медицинских целей, а мезоторий и другие радиоактивные вещества использовались при изготовлении светящихся красок.

Применение урана.

Уран — это тяжелый белый металл, который медленно тускнеет на воздухе. Основное использование урана сегодня — как источника радия. Однако за много лет до открытия радия соединения урана использовались в небольших масштабах при окрашивании стекла и фарфора, в фотографии, в качестве реагентов для химического анализа, в качестве протрав при крашении и для других второстепенных целей. Использование металлического урана в небольших количествах в производстве стали было опробовано с некоторой степенью успеха.

РУДЫ РАДИЯ И УРАНА

Общее положение.

Основными урановыми минералами, известными в настоящее время в природе, которые, следовательно, являются основными источниками как урана, так и радия, являются карнотит и уранинит, а также нечистая аморфная форма уранинита, известная как настуран (урановая смолка). Торбернит, отунит и некоторые из более редких урановых минералов дали немного радия и урана.

Карнотит и уранинит или настуран в добытом виде обычно более или менее смешаны с другими материалами и редко встречаются в чистом виде. Уран в рудах обычно указывается в коммерческих целях для удобства в виде оксидов урана, представленных формулой UO2 + 2UO3, кратко выражаемой как U3O8. Большинство карнотитовых руд варьируется от 1 до 3 процентов U3O8; руда с содержанием 5–10 процентов считается высокосортной; руда с содержанием 20–40 процентов является удивительно богатой. Уранинит и настуран обычно содержат больше урана, чем карнотит, и даже в нечистых формах, в которых они добываются как руды, они часто показывают это более высокое содержание урана. Обычные руды уранинита и настурана содержат от 2–3 до 8–10 процентов U3O8, а руда с содержанием 20 процентов является очень высокосортной, хотя некоторая руда достигает 60 или 70 процентов.

Карнотит.

Карнотит — это аморфный, мягкий, порошкообразный материал, иногда более или менее связный и талькоподобного или воскового характера, обычно ярко-канареечного цвета, хотя иногда обесцвеченный железом, органическими веществами и другими субстанциями. По существу, это водный ванадат калия-урана. Некоторые авторитеты полагают, что карнотит — это не отдельный минерал, а смесь различных минералов.

Уранинит и настуран.

Термины уранинит и настуран часто используются как синонимы для обозначения одного и того же минерала, но более правильно термин уранинит является общим названием для всех форм минерала и особенно для более чистой и отчетливо кристаллической разновидности, а термин настуран применим к нечистой аморфной форме. Он черного или серовато-черного цвета, непрозрачен и часто имеет субметаллический блестящий или смолистый блеск. Уранинит часто удивительно лишен отличительных характеристик, поэтому его присутствие часто может быть не замечено. По этой причине кажется возможным, что этот минерал, известный сейчас лишь в сравнительно небольших количествах, когда-нибудь в будущем будет найден в большем изобилии.

Уранинит, как и карнотит, имеет несколько неопределенную формулу, но по существу является комбинацией двух оксидов урана UO2 и UO3, в которой UO2, по-видимому, действует как основание, а UO3 — как кислота. С ними часто ассоциируется ряд как более редких, так и более распространенных элементов. Относительные количества двух оксидов значительно варьируются в разных образцах, особенно в нечистой форме настурана, и никакой определенной формулы в настоящее время дать нельзя. В настуране часто присутствует заметное количество воды, возможно, иногда в химическом соединении. Несколько других минералов, гораздо более редких, чем уранинит или настуран, связаны с ними по составу, среди них клевеит, брёггерит и нивенит.

Другие руды.

Хотя карнотит, уранинит и настуран являются самыми распространенными из всех материалов радия и урана в природе и производят почти весь радий и уран в торговле, многие другие минералы содержат оба металла, и, хотя пока они известны лишь в таких ограниченных количествах, что имеют небольшую коммерческую ценность, в будущем могут быть найдены в значительных количествах. Среди них можно упомянуть тюямунит, водный ванадат кальция-урана, часто ассоциированный с водным ванадатом калия-урана, описанным выше как карнотит; отунит, водный фосфат кальция-урана; торбернит или хальколит, водный фосфат меди-урана.

ГЕОГРАФИЧЕСКОЕ И ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ РАДИЯ И УРАНА

Единственными регионами мира, которые до сих пор производили какие-либо значительные количества минералов радия и урана в коммерческом масштабе, являются Колорадо, Юта и Австрия. Корнуолл, Австралия и Германия произвели небольшое количество этих минералов. Они известны в небольших количествах во Франции и Португалии, и о них сообщалось в Индии и Германской Восточной Африке, но в этих регионах они еще не стали коммерчески важными. Они встречаются редко, насколько известно, и практически только как минералогические курьезы, в Коннектикуте, Северной Каролине, Канаде, Норвегии и многих других регионах, но в будущем могут быть найдены в больших количествах.

Минутные количества радия или продуктов его распада встречаются почти во всех породах, в атмосфере, а также в водах морей и суши, но в таких малых количествах, что они недоступны в качестве источника этих веществ. Источником всего радия в торговле в настоящее время являются определенные немногие урановые минералы, уже упомянутые. Они встречаются в формациях различных геологических возрастов, от недавних поверхностных отложений до более старых кристаллических пород, но проявляют тенденцию к определенным способам залегания, таким как в юго-западном Колорадо и юго-восточной Юте в виде пропитки в песчанике; в восточном Колорадо, Корнуолле, Австрии и Южной Австралии как один из жильных минералов в жилах других руд; в Северной Каролине, Канаде, Норвегии и Западной Австралии в пегматитовых или других полевошпатовых дайках.

РЕСУРСЫ РАДИЯ И УРАНА В СОЕДИНЕННЫХ ШТАТАХ

Общее положение.

Коммерчески важные месторождения руд радия и урана в Соединенных Штатах, насколько известно, ограничены карнотитовыми регионами юго-западного Колорадо и юго-восточной Юты, а также месторождениями настурана в округе Гилпин в восточном Колорадо. В Коннектикуте, Северной Каролине и других местах были найдены уранинит, настуран и другие урановые минералы; а недалеко от Моч-Чанка в Пенсильвании были обнаружены небольшие количества карнотита, но эти проявления, насколько известно, находятся в количествах, слишком малых, чтобы иметь коммерческую ценность.

Колорадо и Юта.

Карнотитовые месторождения юго-западного Колорадо и юго-восточной Юты являются самыми важными источниками радия и урана в мире. В Колорадо наибольшее количество руды поступило со многих рудников в округе Монтроуз, особенно в Парадокс-Вэлли, в то время как округа Меса, Сан-Мигель, Долорес, Рио-Бланко, Раутт и другие были производителями. В юго-восточной Юте руды представляют собой карнотит, как и в юго-западном Колорадо, и встречаются особенно в округах Гранд, Эмери и Сан-Хуан, но не разрабатывались в той же степени, что и в Колорадо.

Карнотит Колорадо и Юты встречается в виде пропитки в песчаниках и сланцеватых песчаниках, в основном в формациях Мак-Элмо и Ла-Плата, лежащих в верхней части юрских пластов и ниже меловых песчаников и конгломератов региона. Месторождения, по-видимому, образовались путем осаждения карнотита из раствора вдоль определенных пластов этих формаций, и материал встречается вдоль плоскостей напластования, в трещинах и небольших полостях, в виде слоев или неправильных масс шириной от доли дюйма до нескольких дюймов, а иногда как общая пропитка песчаника на несколько футов в толщину. Он кажется особенно обильным в пластах, сильно пропитанных растительными или животными остатками, и часто встречается в необычных количествах в лигнитовых или окаменелых стволах деревьев. Это явление предполагает влияние органических веществ в осаждении и сегрегации карнотита.

Породы, содержащие карнотит, лежат горизонтально или падают под небольшими углами в большинстве частей региона Колорадо; в Юте они часто лежат таким же образом, но иногда падают под крутыми углами. Там, где они появляются на поверхности, карнотит иногда пропитывает определенные пласты на несколько сотен футов или более вдоль обнажений, но чаще он встречается в виде пятен вдоль них, с небольшим количеством карнотита или его отсутствием в промежуточных пространствах. По мере того как эти обнажения прослеживаются в склоны холмов, руда кажется еще более неравномерной в своем распределении, чем на поверхности, и во многих или большинстве случаев она становится гораздо более редкой по мере того, как ее исследуют под землей, пока на расстоянии от 10 до 40 или 50 футов от поверхности она часто большей частью или полностью исчезает. Есть исключения из этой особенности, но постепенное и часто быстрое уменьшение количества и качества карнотитовой руды по мере ее прослеживания в холм общепризнано. Этот факт предполагает, что карнотит мог быть повторно растворен в песчанике и вынесен на поверхность капиллярным действием в этом засушливом климате, образуя богатые поверхностные выцветы.

Во многих карнотитовых месторождениях ванадиевые минералы встречаются независимо от ванадия в карнотите, но эта ассоциация наблюдается не всегда. Они встречаются в песчанике и часто придают ему темно-серый или черноватый цвет.

В восточном Колорадо несколько рудников недалеко от Сентрал-Сити, округ Гилпин, произвели ограниченное количество настурана. Среди них рудники Kirk, Wood, Belcher, Alps, German и Calhoun. Настуран встречается как второстепенный компонент в золотоносных жилах этой страны. Жилы пересекают старые метаморфические породы, прорванные изверженными породами. Рудники округа Гилпин сегодня производят мало, если вообще производят, настурана, и общий объем производства был небольшим, составив в общей сложности, вероятно, всего несколько тонн. Однако гораздо больше настурана было выброшено в отвалы в прежние дни, когда рудники разрабатывались для других руд и ценность урана не была признана.

Производство.

Соединенные Штаты сегодня являются, безусловно, крупнейшим производителем руд радия и урана в мире, а также крупнейшим производителем промышленных соединений радия и урана. До войны Англия, Франция и Германия, особенно Германия, импортировали большие количества американских руд и извлекали радий в очищенном состоянии в виде его различных солей, большая часть которых возвращалась в Соединенные Штаты для продажи. Сейчас, однако, американские руды почти полностью обрабатываются в Соединенных Штатах, за исключением небольшого количества, отправляемого в Англию и, возможно, во Францию. Standard Chemical Co. из Питтсбурга была пионером в этой работе, и другие быстро последовали за ней, среди них National Radium Institute из Денвера; Schlesinger Radium Co. из Денвера; Chemical Products Co. из Денвера; Cummings Chemical Co. из Лэнсдауна, Пенсильвания; Radium Luminous Materials Corporation из Нью-Йорка и другие.

До открытия радия в 1898 году урановым рудам в Америке уделялось мало внимания, хотя некоторое количество настурана отправлялось из района Сентрал-Сити, Колорадо, для использования в производстве соединений урана. Однако вскоре после открытия радия началась добыча карнотита в юго-западном Колорадо, и с 1900 по 1910 год было создано несколько компаний для разработки этих руд как в Колорадо, так и в Юте. Настуран из Сентрал-Сити также начал привлекать возобновленное внимание. В течение нескольких лет велась активная работа по его разведке, но количества до сих пор оказывались небольшими. Несколько тонн, вероятно, представляют собой общее количество, полученное с этих рудников с тех пор, как начались поиски. Тем временем, однако, производство карнотита быстро росло до 1915 года, когда оно значительно сократилось из-за ограничения поставок в Европу. Однако во второй половине 1916 года производство снова увеличилось из-за возросшего потребления руды в этой стране, а в 1918 году производство было очень активным, во многом из-за возросшего использования радия не только в медицине, но особенно в светящихся красках.

Количество руд радия и урана, добываемых в Соединенных Штатах или, по сути, где-либо еще за определенный период, трудно определить из-за различий в основаниях, на которых составляются отчеты, однако можно сказать, что тоннаж невелик по сравнению с рудами более распространенных металлов: несколько тысяч тонн — это большое количество карнотита, а всего лишь несколько тонн или фунтов — уже значительный объем настурана. Хотя добыча радиевых и урановых руд в Соединенных Штатах началась примерно в 1900 году или незадолго до этого, очень большие объемы не добывались вплоть до 1912 года, когда было добыто около 1100 тонн, состоящих главным образом из колорадского карнотита. Добыча постепенно увеличилась до нескольких тысяч тонн в год, практически весь этот объем составляет карнотит из Колорадо и Юты.

РЕСУРСЫ РАДИЯ И УРАНА В ЕВРОПЕ

Австрия.

— Самой важной рудой радия и урана в Европе в настоящее время является уранинит, или настуран, обнаруженный на рудниках Иоахимсталя в Богемии. Он встречается как второстепенный жильный минерал в некоторых серебряных жилах этого региона, пересекающих метаморфические и изверженные породы, и активно разрабатывается с момента открытия радия М. и Мм. Кюри в 1898 году. До этого времени минерал имел определенную ценность как источник соединений урана.

Эти австрийские рудники занимают второе место после рудников Соединенных Штатов как источник радия и урана, но их добыча равна лишь очень малой части добычи в этой стране. До Великой войны эта добыча в значительной степени, если не полностью, контролировалась австрийским правительством, и, поскольку говорят, что добыча продолжается до сих пор, вероятно, она по-прежнему контролируется таким же образом.

Англия.

— Вторым по значимости в Европе после уранинита, или настурана, из Иоахимсталя в качестве источника радия и урана является аналогичная руда на некоторых рудниках Корнуолла, Англия. Она встречается как второстепенный минерал в жильной породе некоторых старых оловянных и медных рудников, в жилах, пересекающих метаморфические и изверженные породы, особенно в Сент-Джасте, Сент-Айвсе, Грэмпоунд-Роуд, Сент-Остелле и других местах. Добыча и переработка руды находились под частным или корпоративным управлением, и объем добычи был невелик.

Германия.

— В Германии добыча радиевых и урановых руд всегда была незначительной. Небольшое количество таких руд добывалось в Шнееберге, Йохангеоргенштадте, Аннаберге и других местах. До войны Германия была крупным производителем готовых соединений радия и урана, но они получались в основном из импортируемых американских руд.

Другие месторождения.

— За исключением Иоахимсталя и Корнуолла, в Европе добывались лишь небольшие количества минералов радия и урана. Некоторое количество уранинита, или настурана, было найдено в других местах Австрии, таких как Пршибрам и другие, а также в небольших количествах в Норвегии. Автонит и другие урановые минералы были найдены в небольших количествах близ Отена, Франция, и близ Сабугала и Гуарды в Португалии, но значительных количеств добыто не было.

РЕСУРСЫ РАДИЯ И УРАНА В АВСТРАЛИИ, ИНДИИ И АФРИКЕ

Австралия.

— В Южной Австралии карнотит, автонит, торбернит и другие редкие урановые минералы встречаются в регионах метаморфических и изверженных пород на Рэдиум-Хилл, близ Олари, и на горе Пейнтер в хребте Флиндерс. Несколько сотен тонн руды, содержащей эти минералы, были добыты частными лицами или корпорациями. Большая часть этого сырья была отправлена в Вулвич, близ Сиднея, Новый Южный Уэльс, или в Англию для извлечения радия. С начала войны активные горные работы по добыче таких руд в регионе Южной Австралии не велись.

В Куглонге, Западная Австралия, урановый минерал фергусонит и, в меньшей степени, урановый минерал эвксенит встречаются в поверхностном обломочном материале региона. В Воджине минералы макинтошит, торогуммит и пилбарит, являющиеся гидратированными силикатами урана, тория и свинца, встречаются в альбитовом пегматитовом дайке. Значительных количеств этих руд Западной Австралии пока не добыто.

Индия и Африка.

— Сообщалось о наличии минералов радия и урана в Индии и Германской Восточной Африке, но значительных количеств пока не добыто.

ПЕРСПЕКТИВЫ БУДУЩИХ ОТКРЫТИЙ РУД РАДИЯ И УРАНА

Перспективы новых открытий минералов радия и урана в настоящее время кажутся наиболее благоприятными в регионах распространения карнотита в Колорадо и Юте. Разрабатываемые месторождения, по-видимому, являются более или менее поверхностными, и, возможно, в одном месте нельзя найти большое количество руды, однако огромная протяженность региона, в котором встречаются формации, содержащие карнотит, обеспечит колоссальное совокупное количество руды.

Увеличение числа открытий уранинита, настурана и других урановых минералов в Европе кажется возможным, даже несмотря на то, что этот континент уже был хорошо исследован на их наличие. Более того, новые открытия различных минералов радия и урана, весьма вероятно, могут быть сделаны в других частях Соединенных Штатов, помимо упомянутых, а также в менее исследованных частях мира, особенно в некоторых регионах Южной Америки, Австралии, Азии и Африки. Многие из этих минералов, особенно настуран, не имеют ярко выраженных признаков при первом наблюдении и могут быть легко пропущены много раз, прежде чем будет обнаружена их истинная природа. Отсюда и возможности будущих открытий.

ГЛАВА XII ЦИРКОНИЙ Автор: Х. К. Моррис

ПРИМЕНЕНИЕ ЦИРКОНИЯ

Еще в 1830 году была предпринята попытка использовать циркониевые кнопки, нагретые до каления, для освещения улиц Парижа. В 1885 году была запатентована калильная газовая сетка из оксида циркония, но через несколько лет она была заменена торием. Около 1900 года диоксид циркония использовался в горелке Нернста, а также применялся вместо извести и магнезии в качестве накаливаемого материала в свете Драммонда. Также сообщается, что он используется в светильниках Блерио, и предлагалось его применение в сигнальных ракетах.

За последние несколько лет д-ру К. М. Джонсону удалось наладить производство лабораторной посуды из циркониевых минералов, смешанных с другими огнеупорными материалами. Фильтрующие тигли, муфели, трубки и лодочки для сжигания, защитные трубки для пирометров и аппараты Киппа теперь имеются в продаже, конкурируя по цене с немецким фарфором и плавленым кварцем. Тигли из диоксида циркония изготавливаются из плавленого материала, измельченного в подходящей мельнице. Порошок прессуется или формуется с органическим связующим, таким как крахмал, или, возможно, еще лучше, с пластичным цементом, полученным путем измельчения плавленого материала до 20 меш, когда он становится коллоидным в присутствии воды. После сушки изделия обжигаются при очень высокой температуре (от 2300 до 2400°C) до прекращения усадки.

Плавленый диоксид циркония обладает высокой термической стойкостью; он не разрушается при нагревании докрасна и погружении в холодную воду, его коэффициент расширения составляет всего 0,00000084; а его сопротивление сжатию во много раз превышает сопротивление кварцевого стекла. Его твердость находится между твердостью корунда и кварца; удельный вес 5,89, а пористость ниже 1 процента. Его температура плавления составляет 2950°C, но 0,5 процента примесей снижают ее на 100°C. Платина с температурой плавления около 1750°C может быть расплавлена до состояния подвижной жидкости в тиглях из диоксида циркония, и утверждается, что в подобных тиглях была определена температура кипения чистого железа.

Химически диоксид циркония очень инертен, обладая высокой устойчивостью к воздействию кислот, расплавленных щелочей, плавленого кварца или расплавленного стекла. Возможно, ни один другой материал, известный химикам, не обладает таким сочетанием желательных огнеупорных свойств. Его единственная нежелательная характеристика — это склонность при определенных условиях при высоких температурах в присутствии азота или углерода превращаться в нитрид или карбид.

Поучительная статья под названием «Диоксид циркония как огнеупорный материал» Э. Х. Родда была опубликована в «Журнале Общества химической промышленности» 15 июня 1918 года.

Оксид циркония как глушитель был тщательно исследован Хартманом [95] и Грюнвальдом [96] с многообещающими результатами; и был выдан ряд иностранных патентов на использование этого оксида в белых керамических эмалях. Диоксид циркония, по-видимому, особенно подходит для производства огнеупорного кирпича, или его можно наносить в качестве футеровки или покрытия на другие, менее подходящие огнеупорные материалы. Говорят, что практика на континенте в этом направлении развита гораздо выше, чем в нашей стране, причем одним из приводимых примеров являются практические испытания мартеновской печи Сименса с подом, футерованным диоксидом циркония. После четырех месяцев непрерывной работы при высоких температурах под все еще находился в хорошем состоянии и обещал прослужить по крайней мере столько же времени без замены. Статистика, составленная по результатам этих испытаний, показала экономию около 50 процентов фактических затрат на техническое обслуживание в пользу диоксида циркония по сравнению с другими огнеупорными материалами, обычно используемыми для таких целей. Брэдфорд [97] процитировал Подшуса [98], который утверждал, что изготовил печь из чистого оксида, который сначала был расплавлен в дуговой печи, а затем измельчен; и в которой температуры от 2400° до 2500°C были получены при сжигании с помощью газа и кислорода.

[95] Хартман, Август, Zirconemail: Диссертация: Технический университет, Мюнхен, 1910.

[96] Об оксиде циркония в эмалевой промышленности: Sprechsaal, № 5, 1911.

[97] Брэдфорд, Леопольд, Бирмингемское металлургическое общество (Британское).

[98] Подшус, Zeitsch. angew. Chem., год 30, 1917, 1, стр. 17-19.

Самый важный вопрос, касающийся циркония в настоящее время, связан с замечательными свойствами, которые, как утверждают некоторые его сторонники, он придает стали. То, что немцы имели в виду это применение в течение некоторого времени, подтверждается многочисленными патентами, которые они получили на использование циркония и его сплавов.

Цирконий был получен в аморфном и графитовом состоянии; а Ведекинд получил металл чистотой 99,8 процента, напоминающий по внешнему виду белый чугун, с твердостью 7,8 (по Моосу); удельным весом 6,40; удельной теплоемкостью 0,0804; теплотой соединения 1958 калорий; и температурой плавления 1530°C.

Было создано множество сплавов циркония, и был выдан ряд иностранных и отечественных патентов, охватывающих различные сплавы, как черные, так и цветные. Утверждается, что ферроцирконий находит ограниченное применение в сталелитейной промышленности в качестве раскислителя для удаления азота и оксидов. Английский патент № 29 376 охватывает использование циркония в качестве раскислителя, при этом сплав содержит 20 процентов этого элемента и используется в количестве, равном примерно 1 проценту от веса обрабатываемой стали.

Другой сплав, содержащий от 40 до 90 процентов циркония, остальное — в основном железо, как говорят, свободен от металлоидов и оксидов, а также ковок и пластичен. Сплавы, охватываемые патентом США № 1 151 160, как утверждается, обладают высокой устойчивостью к окислению и химическим реагентам. Они имеют металлический блеск и хорошо полируются, легко поддаются ковке и пластичны, и предполагается, что они могут найти важное применение в нитях накала для электрических ламп, поскольку, как говорят, обладают свойством селективного излучения. Типичный анализ некоторых сплавов, которые, как утверждается, были произведены по этому патенту, показывает: Zr 0,65 процента, Fe 26 процентов, Ti 0,12 процента и Al 7,7 процента.

Широко распространенное утверждение о том, что цирконий использовался в Германии при производстве стали для броневых плит и бронебойных снарядов, насколько известно автору, не было подтверждено никакими записями анализов.

Использование циркония для легирования стали настолько ново, что до окончательного определения независимыми компетентными органами точных свойств, если таковые имеются, которые цирконий придает стали, следует воздержаться от суждений о его ценности для этой цели.

Карбид циркония был запатентован для нитей накала ламп электрического освещения, а также использовался в качестве абразива. При испытании в качестве пигмента диоксид циркония показал хорошую укрывистость и должен рассматриваться там, где особенно желательна защита от кислот, щелочей или газов. Основной ацетат использовался для утяжеления шелка, а чистый оксид используется в качестве заменителя субнитрата висмута в рентгенологии.

ГЕОЛОГИЧЕСКОЕ И ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Цирконий встречается в природе в коммерческих количествах в виде смешанного оксида и силиката, известного как бадделеит, иногда называемого бразилитом, и в виде силиката — циркона. Бадделеит, поставляемый в торговлю, обычно содержит от 80 до 85 процентов ZrO2. Силикат, циркон, содержит около 65 процентов ZrO2. Месторождения оксида, содержащие более высокий процент циркония, а также являющиеся более чистыми и легко восстановимыми, по всей вероятности, станут основным источником циркония.

Основные известные месторождения циркониевых руд находятся в Бразилии, Индии и Соединенных Штатах, страны названы в относительном порядке их коммерческой значимости.

Природный оксид.

— Природный оксид, бадделеит, или бразилит, встречается в коммерческих количествах только в Бразилии и описан в «Mineral Foote-Notes» Мейером [99], который пишет следующее:

[99] Мейер, Х. К., Mineral Foote-Notes, ноябрь 1916 г., стр. 29.

Существует лишь несколько коммерческих месторождений необычных руд, которые представляют более интересные геологические, а также экономические особенности, чем месторождения природного оксида циркония в Бразилии. Регион Калдас (посещенный автором в 1915 году), в котором встречаются эти месторождения диоксида циркония, расположен частично в штате Минас-Жерайс и частично в штате Сан-Паулу, примерно в 130 милях к северу от города Сан-Паулу. Это горное плато, основная высота которого составляет около 3600 футов. Поверхность волнистая, с перепадами уровней от 300 до 600 футов.

Вся территория ограничена со всех сторон хребтами, резко поднимающимися на 600–1200 футов над общим уровнем и образующими грубо эллиптическое ограждение с большой осью длиной примерно 20 миль и малой осью 15 миль. Это своеобразное расположение более высоких хребтов весьма показательно в сочетании с тем фактом, что преобладающей породой плато является фонолит, а также с наличием сильно минерализованной термальной воды, обладающей значительными лечебными свойствами [100]. Тщательная геологическая съемка этой территории с целью определения происхождения диоксида циркония не проводилась. Характер руды, однако, и формация, по-видимому, указывают на пневматолитовые процессы. Тщательное изучение взаимосвязи крупных масс крупнокристаллического нефелинового сиенита в этой области с выраженными сегрегациями эвдиалита могло бы пролить некоторый свет на этот предмет.

[100] Дерби, О. А., «Нефелиновая порода в Бразилии»: Quart. Jour. Geol. Soc., август 1887 г.

Руду диоксида циркония можно грубо разделить на два класса:

Во-первых, аллювиальные гальки размером от половины дюйма до трех дюймов в диаметре, обычно содержащие от 90 до 93 процентов оксида циркония. Эти гальки, известные как «фавас» и имеющие удельный вес от 4,8 до 5,2, встречаются вдоль русел небольших ручьев и на осыпях низких хребтов.

Во-вторых, собственно руда диоксида циркония, или зиркит (торговое название), которая варьируется по оттенку от светло-серого до сине-черного, причем материал более светлого цвета содержит более высокий процент силиката циркония, что подтверждается анализами, которые в некоторых случаях показывают минимум 73 процента оксида циркония. Сине-черная руда обычно содержит от 80 до 85 процентов оксида циркония. Однако путем тщательной сортировки производится однородный сорт, содержащий около 80 процентов.

До исследований Дерби и Ли эта руда считалась идентичной бадделеиту. Однако теперь было показано, что она представляет собой механическую смесь трех минералов, а именно: бразилита, циркона и нового, еще не названного силиката циркония, содержащего около 75 процентов оксида циркония. Этот новый минерал имеет ту же кристаллическую форму, что и циркон (67 процентов ZrO2), но легко растворяется в плавиковой кислоте, в то время как циркон не подвергается воздействию, что является характерным дифференциальным тестом. Тонко измельченный минерал при обработке слабым раствором плавиковой кислоты оставляет остаток из крошечных совершенных пирамидальных кристаллов циркона, при этом бразилит и новый силикат циркония переходят в раствор. На крайнем западном краю плато встречаются несколько крупных выходов руды, причем один или два изолированных валуна весят до тридцати тонн. Это весьма беглое обследование месторождений диоксида циркония делает небезопасным выдвижение каких-либо предположений относительно количества доступной руды. Достаточно сказать, однако, что месторождения были прослежены на расстоянии пятнадцати миль между Гаскатой и Калдасом, и если поверхностные признаки имеют какое-либо значение, то они имеют огромные масштабы.

Оксиды также были найдены в штате Монтана, а также на Цейлоне, в Швеции и Италии, но ни одно из этих месторождений не имеет коммерческого значения.

Силикат.

— Простой силикат, циркон, встречается в прибрежных и речных концентрациях монацитовых песков, ассоциированных с ильменитом, гранатом, рутилом и различными другими тяжелыми минералами, обычно встречающимися в таких местах.

Важная концентрация циркона встречается вдоль побережья Бразилии, в штатах Баия, Эспириту-Санту и Рио-де-Жанейро, где выступы пляжей защищены с севера гранитными мысами и окаймлены третичными утесами, которые прорезаны различными ручьями и лагунами, постоянно поставляющими свежий материал для концентрирующего действия приливов и волн.

Вероятно, следующее по значимости месторождение циркона находится в Индии, в пляжных песках провинции или штата Траванкор на крайнем юго-западном конце полуострова Индостан.

Следующим по значимости является месторождение в Соединенных Штатах на Пабло-Бич, Флорида, где не только пляжные пески, но и дюны, граничащие с ними, содержат заметные количества следующих минералов в относительном порядке их распространенности: ильменит, гранат, эпидот, циркон, рутил и другие тяжелые минералы, включая монацит [101].

[101] Хесс, Фрэнк Л., Письмо от 1 мая 1918 г.

Другие месторождения в этой стране, большинство из которых представляют лишь академический интерес, находятся в Колорадо, на Сент-Питерс-Доум, близ Пайкс-Пик; в Айдахо, в регионе Клируотер и в других местах в черных песках и в некоторых гранитных породах; в округе Сассекс, Нью-Джерси, на руднике Уильямс, где циркон встречается в изобилии в магнетите; в Нью-Йорке на горе Лайон, округ Клинтон; в нескольких местах близ Краун-Пойнт; в изобилии в пегматите на рудниках Олд-Ред, Майнвилл, округ Эссекс, и в многочисленных местах в округе Ориндж на юге и округе Сент-Лоуренс на севере. В Северной Каролине, в округах Берк, Макдауэлл и Резерфорд, циркон встречается в монацитовых песках, а также в округе Хендерсон близ Цирконии и в округе Фриделл близ Стерлинга.

Крупные кристаллы циркона встречаются в небольшой пегматитовой области в округе Команчи, Оклахома, в юго-западной части Национального леса Уичито. В Орегоне есть много мест, где было отмечено присутствие циркона, главным образом в черных песках, старых и современных пляжах, россыпных гравиях и т. д., то же самое верно и для Вашингтона. В Вирджинии циркон найден в пегматите в округе Аурелия и в песчанике близ Ашленда, недалеко от Ричмонда.

Циркон также встречается в Норвегии, на Уральских горах, на Цейлоне, в Австралии и Британской Южной Африке.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Важные мировые ресурсы циркония политически контролируются, в порядке их коммерческой значимости, Бразилией, Великобританией и Соединенными Штатами.

Бразилия.

— Много лет назад Джон Гордон, американский горный инженер, заинтересовался месторождениями монацитового песка на побережье Бразилии в окрестностях Прадо, Баия. Тщательное исследование всех известных месторождений монацита в мире показало, что месторождения в Бразилии являются самыми желанными, а месторождения в Траванкоре, Индия, занимают второе место по коммерческой значимости [102].

[102] См. главу XIII.

Другими фирмами, экспортирующими циркониевые минералы из Бразилии, помимо Gordon & Rogers, 141 Бродвей, Нью-Йорк, являются Suffern & Co., 135 Бродвей, Нью-Йорк; S. R. Scott & Co., 39 Бродвей, Нью-Йорк; Foote & Co., Филадельфия, Пенсильвания; P. S. Nicholson & Co., Caixa 91, Рио-де-Жанейро; E. J. Lavino & Co., здание Буллит, Филадельфия, Пенсильвания; Luiz de Rezende & Co., Руа-Овидор, Рио-де-Жанейро, Бразилия; и Час. Шпиц, также из Рио-де-Жанейро, который является агентом Société Minière, французской компании, в которой, как говорят, Rezende & Co. имеют значительную долю. Некоторое время назад фирма A. C. de Freitas & Co. из Гамбурга, Германия, имела контракт с бразильским правительством на монацитовые пески и обязалась экспортировать не менее 1200 тонн ежегодно. Сколько циркона экспортировала эта компания, неизвестно. Свойства de Freitas в настоящее время разрабатываются Société Minière (французской компанией) [103].

[103] Цифры добычи за 1902–1916 годы для Соединенных Штатов и Бразилии приведены в таблице 34.

До самого недавнего времени цирконий представлял незначительный интерес в этой стране, монацитовые пески эксплуатировались только из-за содержания в них тория, а не циркония. Однако Германия и Австрия, по-видимому, придавали большое значение пескам, содержащим цирконий, и, как показано в прилагаемой таблице, в 1913 году было добыто больше, чем за все время до этого, и практически весь материал, произведенный в том году, ушел в Германию. Это согласуется с усилиями Германии непосредственно перед войной получить вольфрам и молибден и является свидетельством подготовки задолго до начала военных действий.

Индия.

— До войны немецкие потребители монацита контролировали месторождения в Траванкоре, Индия. Этот контроль, конечно, прекратился, и контракты были аннулированы. Министерство по делам Индии решило, что в будущем все директора компании должны быть британцами по рождению и что компания должна быть готова в любое время продавать монацитовый песок британским фирмам напрямую по справедливой цене.

Соединенные Штаты.

— Вряд ли вероятно, что месторождения в Соединенных Штатах смогут конкурировать на коммерческой основе с бразильскими рудами; но если возникнет необходимость, эта страна может произвести в своих собственных границах достаточно циркония для производства многих тысяч тонн циркониевой стали. Сердечные коммерческие отношения между Соединенными Штатами и Бразилией, вероятно, защитят эту страну от любых чрезмерных ограничений на экспорт из Южной Америки.

Общие сведения.

— Все крупные заинтересованные страны имеют возможности для производства ферросплавов. Было создано множество сплавов циркония, и был выдан ряд патентов, как иностранных, так и отечественных, охватывающих различные сплавы, как черные, так и цветные. Никакие секретные процессы как таковые автору не известны.

Таблица 34. — Добыча циркониевых минералов в Соединенных Штатах и Бразилии, 1902–1916 гг. [104]

Year | United States | Brazil
Quantity (short tons) | Value | Quantity (short tons) | Value
1902 | ... | ... |    12 | $ |  3,947
1903 | 1 | ¹⁄₂ | $ |   570 |     7 |  1,947
1904 |  | ¹⁄₂ |   200 |     9 |  3,935
1905 | 4 |  |  1600 |    18 |  5,506
1906 |  | ¹⁄₂ |   248 |    26 |  5,041
1907 |  |    46 |    38 |  8,756
1908 | 0 |  |     0 |   275 | 15,151
1909 | 1 |  |   250 |   117 | 11,838
1910 | 0 |  |     0 |   128 | 23,271
1911 | 1 | ¹⁄₂ |   802 |    45 | 16,169
1912 | 0 |  |     0 |    43 | 14,772
1913 | 0 |  |     0 | 1,119 | 54,767
1914 | 0 |  |     0 |   237 | 14,903
1915 | 0 |  |     0 |     8 |  2,915
1916 | 0 |  |     0 |   104 | 16,647

[104] Адаптировано из «Минеральных ресурсов США», 1916 г., часть II, Геологическая служба США, 1917 г., стр. 377–386.

РЕЗЮМЕ

Основное использование циркониевых руд в настоящее время определяется огнеупорными свойствами оксида — диоксида циркония. Огнеупорный кирпич и фасонные изделия для футеровки печей, химическая посуда и другие изделия, устойчивые к воздействию тепла, кислот и щелочей, изготавливаются из диоксида циркония и находят ограниченный рынок сбыта.

Недавний интерес к цирконию обусловлен замечательными свойствами, которые, как говорят, он придает стали. Его реальная ценность или функция в этом направлении еще должны быть окончательно определены, и проводятся испытания Бюро горного дела, Бюро стандартов и другими организациями, чтобы установить факты.

Лучшим и наиболее доступным источником поставок в настоящее время является Бразилия, где природный оксид, бадделеит, встречается в значительных количествах в штатах Минас-Жерайс и Сан-Паулу. Месторождения не были исследованы в достаточной степени, чтобы сделать возможной какую-либо надежную оценку тоннажа, но, судя по их поверхностным проявлениям, они имеют огромные масштабы. Силикат, циркон, встречается в Бразилии, Индии и Соединенных Штатах в коммерческих количествах.

Важные месторождения циркониевых минералов контролируются Бразилией, Великобританией и Соединенными Штатами, но фактическая собственность на многие месторождения неизвестна. Это особенно верно в отношении оксидных руд.

ГЛАВА XIII МОНАЦИТ, ТОРИЙ И МЕЗОТОРИЙ Автор: Р. Б. Мур

ПРИМЕНЕНИЕ МОНАЦИТА

Практически единственным применением монацита был источник солей тория. При их извлечении извлекаются побочные продукты, такие как церий, лантан и другие редкоземельные элементы. Соли тория используются почти исключительно для производства сеток Вельсбаха, которые состоят из 99 процентов оксида тория и 1 процента оксида церия. Для этого применения не существует известного заменителя. Единственное другое применение солей тория — в обычных химических лабораториях, но это использование очень ограничено. Фторид и другие соли церия используются в связи с пламенной дугой, их присутствие дает повышенную светимость.

Мезоторий — это радиоактивный элемент, всегда встречающийся в ториевых минералах. До недавнего времени его выбрасывали при производстве нитрата тория; но сейчас он производится как побочный продукт и полезен в качестве заменителя радия в светящихся красках и для терапевтических целей.

ГЕОЛОГИЧЕСКОЕ И ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Основными источниками монацита являются Бразилия и Индия, хотя его успешно добывали в Соединенных Штатах в Каролинах и в Айдахо. Он был найден в Свазиленде, Африка, и в Австралии, а также, в ограниченной степени, в коренных породах и россыпях в Екатеринбурге, Россия.

Монацит обычно встречается в гравиях небольших ручьев или донных земель, хотя иногда его находят в почве склонов холмов. В Бразилии и Индии он встречается главным образом в пляжных песках морского побережья. Местами он встречается в виде мелких кристаллов в гнейсах, гранитах и пегматитовых породах. По мере разрушения этих пород кристаллы вымываются в ручьи и вместе с другими тяжелыми песками откладываются в руслах ручьев. На побережье Бразилии зерна монацита из кристаллических пород прибрежных гор концентрируются морскими волнами.

Соединенные Штаты.

— Месторождения Каролин охватывают площадь в несколько сотен квадратных миль к востоку от гор Блу-Ридж. В Северной Каролине самые богатые месторождения находятся в округах Кливленд, Берк, Александер, Резерфорд и Линкольн. В Южной Каролине единственные ценные месторождения находятся в округах Чероки и Гринвилл. Практически весь монацит, добываемый в Каролинах, извлекается из гравия в ручьях и донных землях, причем горняки обычно следуют по руслам ручьев. Гравий сильно варьируется по толщине, поэтому трудно сделать точную оценку среднего значения, но в целом монацитосодержащий гравий имеет толщину от 1,5 до 2,5 футов. Верхний слой почвы в донных землях имеет среднюю толщину от 3 до 6 футов и может достигать 7 футов и более.

Месторождения в штате Айдахо находятся близ Сентервилла и Айдахо-Сити. В будущем, при более благоприятных условиях цены, транспортировки и т. д., эти месторождения, возможно, станут коммерческим источником монацита. Почти все они содержат небольшие количества золота. Гравийные пласты значительно толще, чем в Каролинах, и при наличии содержания золота могли бы быть более прибыльными, если бы не более высокая стоимость рабочей силы.

Монацит был найден в Колорадо, в районе Ньюленд-Галч, в 20 милях к югу от Денвера, где он встречается в гравиях, содержащих значительное количество золота.

Бразилия.

— В Бразилии существует три вида месторождений монацитового песка: месторождения на государственных землях вдоль побережья; месторождения, лежащие за государственными прибрежными землями, которые являются частными владениями штата или принадлежат частным лицам; и внутренние месторождения. Основная часть монацита извлекается из прибрежных песков в штатах Эспириту-Санту и Баия, песок промывается с помощью осциллирующих столов или шлюзовых ящиков. Прибрежные земли являются собственностью федерального правительства на 33 метра вглубь суши, отсчитывая от точки, где морские волны омывают пляж при среднем приливе. Этот неопределенный метод разметки собственности, конечно, привел к спорам при установлении границ.

В нескольких местах вдоль побережья полосы монацитосодержащих песков лежат непосредственно за государственной землей, и некоторые из них могли бы разрабатываться с прибылью, если бы не тот факт, что было трудно доказать федеральному правительству, что эти пески не были взяты с близлежащей государственной земли. Одна французская компания эксплуатировала такие земли в штате Рио-де-Жанейро. Вдоль берегов крупных рек, таких как Параиба, находятся огромные количества черных песков со следами монацита. Близ Сапукаи такие месторождения разрабатывались французской компанией. Многие внутренние месторождения не могут эксплуатироваться из-за расходов на транспортировку продукции, так как месторождения находятся в многих милях от железной дороги.

Индия.

— Индия — новейший источник монацитовых песков, месторождения лежат на морском пляже, как и в Бразилии. Месторождения находятся в районе Траванкор близ юго-западного конца полуострова Индостан. Очень мало информации доступно относительно этих месторождений.

ИЗМЕНЕНИЯ В ПРАКТИКЕ ПЕРЕРАБОТКИ

Общий метод переработки, применявшийся до недавнего времени, включал выщелачивание концентрата концентрированной серной кислотой, тем самым переводя торий, церий и другие редкоземельные элементы в раствор и отделяя их от диоксида кремния, циркона, ильменита и других нерастворимых продуктов. С этого этапа разные компании использовали небольшие вариации в практике, такие вариации держались в строгом секрете, хотя все они включали осаждение тория в виде оксалата с помощью щавелевой кислоты.

С началом войны цена на серную кислоту поднялась в четыре-пять раз по сравнению с первоначальной стоимостью, а возросшая цена на щавелевую кислоту была практически запретительной. Вследствие этого производственные компании были вынуждены изменить всю свою процедуру и использовать химикаты, которые они могли получить по разумной цене. В этом трудном начинании компании преуспели, и по крайней мере одна компания разработала процесс, который был значительно более эффективным, чем старый.

В настоящее время мезоторий производится как побочный продукт компаниями Lindsay Light Co. и Welsbach Co., причем процесс, используемый последней компанией, был разработан Колорадской станцией Бюро горного дела США. Этот процесс дешев и чрезвычайно эффективен и, несомненно, позволит Welsbach Co. конкурировать на коммерческой основе с любым другим производителем мезотория. Конечно, поскольку процесс был разработан Бюро горного дела, он в конечном итоге станет доступным для всех, но поскольку мезоторий может быть произведен с прибылью только как побочный продукт нитрата тория, любой, кто производит мезоторий, должен сначала создать ториевую промышленность.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Важные мировые ресурсы монацита политически контролируются тремя странами: Соединенными Штатами, Великобританией (Индия) и Бразилией. Месторождения Соединенных Штатов в обычное время, вероятно, не могут успешно разрабатываться в конкуренции с иностранными месторождениями без защиты высокого тарифа.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Соединенные Штаты.

— Широко разбросанные месторождения монацита в Соединенных Штатах имеют значение только в период аномально высоких цен или во время ограничения импорта из Бразилии и Индии. Известные запасы невелики, и месторождения, вероятно, никогда не станут важным фактором на мировом рынке монацита. Насколько известно автору, все американские месторождения контролируются американским капиталом.

Производство нитрата тория в этой стране тесно контролируется двумя крупными компаниями, Welsbach Co. и Lindsay Light Co.; они владеют двумя единственными коммерческими заводами какого-либо размера в Соединенных Штатах.

Все производители сеток в Соединенных Штатах, за одним исключением, должны получать нитрат тория от одной из этих двух компаний. Поскольку эти компании обеспечивают практически все потребности в нитрате тория Англии и Франции, они контролируют ториевую промышленность. Единственным другим производителем нитрата тория в этой стране является Block Co. из Чикаго, которая использует около 15 тонн монацита в год, производя достаточно нитрата тория для собственного производства сеток. Welsbach Co. использует около 1200 тонн монацита ежегодно, а Lindsay Light Co. — около половины этого количества. Welsbach Co. имеет контракты на поставку монацита в соответствии со своими потребностями из Бразилии; Lindsay Light Co. получает весь свой монацит из Индии.

Большинство используемых процессов, включая те, что применяются Welsbach Co. и Lindsay Light Co., являются секретными. Поскольку торий можно извлечь из монацита более чем одним способом, секретный процесс не обязательно означает коммерческий контроль, если только такой процесс не является во всех отношениях эффективным и компания, владеющая им, не готова вступить в коммерческую войну.

Бразилия.

— Поскольку бразильские месторождения в течение столь многих лет были основным источником поставок монацита, история их коммерческого контроля — это практически история коммерческого контроля над монацитовой промышленностью. Около 27 лет назад Джон Гордон, американец, ныне проживающий в Нью-Йорке, нашел монацит на побережье Бразилии. Он привез большие количества в Гамбург, Германия, и смог получить монополию на монацитовый песок.

В то время производство нитрата тория, основного продукта монацитового песка, было ограничено в Европе несколькими крупными химическими фирмами в Германии и Welsbach Co. в Вене. Они не только снабжали европейский рынок нитратом тория, но и отправляли большие количества в Соединенные Штаты. Американская Welsbach Co. рано начала производить нитраты тория из песков, добытых в Каролинах, что стало возможным благодаря защитной пошлине в 6 процентов.

В 1902 году г-н Гордон согласился поставлять четырем крупным немецким производителям и австрийским производителям монацит по цене 150 долларов за тонну и с прибылью на произведенные нитраты. Таким образом, сформировалось тесное объединение, известное как Немецкая ториевая конвенция, которое не позволяло другим производителям тория приобретать какой-либо минерал, добытый г-ном Гордоном, и подняло цену на нитрат тория на 100 процентов.

В течение значительного периода г-н Гордон экспортировал песок с прибрежных земель Баии, близ Прадо, Бразилия, без вмешательства. Наконец, бразильское правительство ознакомилось с ценностью ресурсов и решило, что ни одно частное лицо или правительство штата не имеет права добывать, продавать, сдавать в аренду или вывозить какой-либо монацит на так называемых государственных землях без согласия федеральных властей. В 1908 году правительство объявило, что прибрежные земли в штате Эспириту-Санту будут сданы в аренду тому, кто предложит самую высокую цену за эксплуатацию песков. Таким образом, контракт был получен фирмой A. C. de Freitas & Co. из Гамбурга, Германия. По контракту фирма обязалась выплачивать бразильскому правительству арендную плату, равную 50 процентам от продажной цены монацитовых песков, и экспортировать не менее 1200 тонн ежегодно.

Чтобы избежать неприятностей, Немецкая ториевая конвенция позже договорилась, что половина ее поставок будет обеспечиваться г-ном Гордоном, а половина — компанией de Freitas. Новая конвенция была сформирована четырьмя немецкими химическими производителями с г-ном Гордоном и компанией de Freitas, что не позволяло фирмам в других странах, которые начали производить нитрат тория, получать сырье. Вследствие этого были предприняты большие усилия по поиску и разработке новых месторождений монацита. Высокая цена на нитрат тория сделала возможной добычу монацита в Каролинах и его экспорт в Германию, особенно одному немецкому производителю, который не входил в Немецкую ториевую конвенцию.

В конечном итоге произошло перепроизводство тория, и в 1906 году цена упала на 50 процентов. Добыча монацита сократилась во всех местах, где стоимость добычи была высокой, и производство в Каролинах и внутренних районах Бразилии практически остановилось.

В течение четырех или пяти лет, предшествовавших войне, Немецкая компания ламп накаливания из Берлина преуспела в контроле над крупнейшими производителями нитрата тория в Европе, за исключением тех, что находились во Франции. Она контролировала как английские, так и австралийские компании и стала активным конкурентом так называемой Ториевой конвенции, которая к тому времени утратила большую часть своей власти. Г-н Гордон по-прежнему имеет обширные интересы в Бразилии, но у него нет монополии. Права на экспорт из Бразилии находятся в руках Luis de Rezende & Co. (Рио-де-Жанейро), г-на Гордона и других. Luis de Rezende & Co. — это в основном французская компания, но она имеет бразильских и португальских акционеров. Компания контролирует французскую компанию Société Minière, связанную с Welsbach Co.

Как отмечалось выше, одна французская компания эксплуатировала месторождения монацита на территории непосредственно за государственными землями в штате Рио-де-Жанейро. Другая французская компания разрабатывала черные пески вдоль реки Параиба, близ Сапукаи, которые содержат следы монацита.

Индия.

— До войны немецкие производители нитрата тория осуществляли такой же жесткий контроль над месторождениями монацита в Траванкоре, Индия, как и над месторождениями в Бразилии. Лишь ограниченное количество песка продавалось производителям сеток и другим потребителям в Соединенном Королевстве, и то по цене, в девять раз превышающей цену, которую платили немецкие потребители. Такая монополия на поставки сырья сделала немецкую монополию в индустрии нитрата тория почти полной.

Согласно С. Дж. Джонстону, в выступлении на ежегодном собрании Общества химической промышленности в июле 1916 года, немцы получили фактический контроль над месторождениями монацита в Траванкоре следующим образом: аренда на разработку этих месторождений была предоставлена несколько лет назад Траванкорским Дурбаром с одобрения правительства Индии компании London Cosmopolitan Tin Mining Co., которая заключила контракт на продажу всей своей продукции немецкой фирме. Вскоре после начала войны было обнаружено, что все привилегированные акции и 11 000 обыкновенных акций Travancore Minerals Co. удерживались в доверительном управлении для компании Auer из Берлина.

Министерство по делам Индии решило, что в будущем все директора компании, разрабатывающей концессию, должны быть британцами по рождению и что компания должна быть готова в любое время продавать монацитовый песок напрямую по справедливой цене британским фирмам. Немецкие контракты были аннулированы. Вторая компания, Thorium, Ltd., получила 20-летнюю аренду на разработку 150 акров в Траванкоре для добычи монацитового песка и экспортирует песок и производит из него нитрат тория на заводах в Англии. Большое количество монацита из Траванкора было импортировано американскими компаниями.

ПОЛОЖЕНИЕ СОЕДИНЕННЫХ ШТАТОВ

Как было указано выше, легко заметить, что Соединенные Штаты зависят от Бразилии и Индии в плане поставок сырьевых ресурсов, поскольку внутренние месторождения недостаточно велики, чтобы обеспечить требуемый объем, и не могут конкурировать с иностранными месторождениями, где добыча обходится дешевле.

Среднее содержание оксида тория в концентрате, получаемом в Каролине, составляет около 3,5–4 процентов; в бразильском концентрате оно в среднем превышает 8 процентов. В таких условиях монациту из Каролины трудно конкурировать с монацитом из Бразилии или Индии. Кроме того, значительная часть доступных запасов монацита в Каролине уже выработана. Старые выработки в той или иной степени заброшены, а вся отрасль пришла в полный упадок.

В то время как эти месторождения разрабатывались, фермеры обычно самостоятельно получали концентрат в примитивных промывочных лотках. Полученный таким образом продукт содержал в среднем около 35 процентов монацита. Затем концентраты продавались на перерабатывающий завод, где их наиболее эффективно обрабатывали с помощью электромагнитных сепараторов, таких как машина Уэтерилла. Конечный продукт, полученный на этих машинах, был готов к химической обработке для извлечения тория.

Практически такая же обработка применяется к монациту из Бразилии и Индии. Поскольку получаемый концентрат имеет гораздо более высокое качество, дополнительные расходы на фрахт и пошлины, которые не ложатся на продукт из Каролины, с лихвой компенсируются. Несомненно, если на монацит из Бразилии и Индии не будет наложен очень высокий тариф, наши будущие поставки будут осуществляться из этих двух источников, по крайней мере, в течение некоторого времени. Очень сомнительно, что при высоком тарифе месторождения Каролины смогут обеспечить монацитом, необходимым в этой стране, даже в течение нескольких лет, и при самых благоприятных условиях потребуется некоторое время, возможно, от шести месяцев до года, чтобы возродить отрасль.

Союзники и практически весь мир зависят от Соединенных Штатов в отношении готовой продукции: нитрата тория и газокалильных сеток. Сохранится ли эта монополия — вопрос спорный, поскольку в Англии существует движение за поощрение производства как нитрата тория, так и газокалильных сеток.

ГЛАВА XIV МЕДЬ Автор: Ф. У. Пейн

ВВЕДЕНИЕ

Одна страна занимает выдающееся положение как крупнейший в мире производитель меди, и это Соединенные Штаты, на долю которых в 1917 году пришлось 60 процентов от общего мирового объема производства. Железо, уголь, нефть и медь являются основными сырьевыми ресурсами, которых Соединенные Штаты производят больше, чем любая другая страна, но только по меди и нефти объем производства превышает показатели всех остальных стран вместе взятых. В отношении меди это справедливо с начала девяностых годов. «Американская медь», «английское золото», «русская платина» и «чилийская селитра» — это общепринятые фразы на мировых рынках; такие же обычные, как и сами эти товары.

Ни одна другая страна не производит и в течение многих лет не производила даже одной шестой части того объема меди, который дают Соединенные Штаты. В то время как мировое производство меди увеличивалось со средним темпом 5 процентов в год в течение 10 лет до 1914 года и в три раза быстрее с тех пор, относительная значимость Соединенных Штатов не снизилась. Напротив, она росла более высокими темпами, чем общий мировой объем производства. Правда, некоторые отдельные страны с 1914 года увеличили свой объем производства быстрее, чем Соединенные Штаты, но нет никаких признаков того, что Соединенные Штаты утратят свое нынешнее доминирующее лидерство.

Благодаря масштабам медной промышленности Соединенных Штатов здесь были построены крупные перерабатывающие заводы. Американский капитал также в значительной степени вложен в медные предприятия Канады, Мексики и Южной Америки. В результате Соединенные Штаты сейчас импортируют почти треть того объема меди, который производят (18 процентов от общего мирового объема производства в 1917 году). Таким образом, американский капитал контролирует, посредством переработки в дополнение к владению рудниками, 78 процентов мирового производства меди. Этот контроль должен быть столь же сильным и в отношении продаж. Очевидно, что большая часть нашей внутренней меди, а если судить по статистике, то и вся импортируемая медь, экспортируется в готовом виде — медные слитки и прутки, латунь, электротехническое оборудование и т. д. Однако в том, что касается продаж и даже владения рудниками в Мексике и Южной Америке, существует значительный германский контроль; хотя важные рудники Канады, Мексики и Южной Америки принадлежат либо американским, либо британским, либо французским интересам, за исключением тех, что принадлежат местному иностранному капиталу.

Таблица 35. — Географический и финансовый контроль над мировыми медными рудниками (Производство в метрических тоннах)

Percentage
of
World total
Average
1916-1917
output
of copper
Country of origin
Estimated
capacity
output
of copper
Per-
centage
of
world
total
Owned
by
U. S.
capital
Owned
by
British
capital
Owned
by
German
capital
Owned
by
French
capital
Owned
by
Japanese
capital
Owned by
local capital in
producing countries

|  | Western Hemisphere |  |  |  |  |  |  |  |
59.2 |   868,903 | United States |   928,000 |  57.5 |   899,000 |  29,000 |  |  |  |  |
 3.3 |    49,168 | Canada |    58,000 |   3.6 |    28,000 |  30,000 |  |  |  |  |
 3.4 |    49,478 | Mexico |    65,000 |   4.0 |    49,000 | Idle |  |  2,500 | plus | 13,500 |  |  |
 1.0 |    14,000 | Cuba |    10,000 |   0.6 | ... | ... |  |  2,000 | plus | ... |  | ... | 8,000
 0.2 |     2,000 | Venezuela |     2,000 |   0.1 | ... |   2,000 |  |  |  |  |
 4.8 |    70,000 | Chile |   110,000 |   6.8 |    86,000 |   2,500 |  |  4,500 | plus |  9,500 | [105] | ... | 7,500
 3.  |    43,620 | Peru |    45,000 |   2.8 |    45,000 |  |  |  |  |
 0.4 |     6,000 | Bolivia |    12,000 |   0.8 |     6,000 | ... |  | ... |  |  6,000 |  |  |
75.4 | 1,103,169 | Total Western Hemisphere | 1,230,000 |  76.2 | 1,113,000 |  63,500 |  |  9,000 |  | 29,000 |  | ... | 15,500
|  | Eastern Hemisphere |  |  |  |  |  |  |  |
 3.2 |    47,500 | Africa |    58,000 |   3.6 | ... |  58,000 | [105] | ... |  | ... |  |  |
 2.5 |    36,550 | Australia |    43,000 |   2.7 | ... |  43,000 |  |  |  |  |
 7.9 |   112,900 | Japan |   125,000 |   7.7 | ... | ... |  | ... |  | ... |  | 125,000 |
 2.9 |    42,000 | Spain and Portugal |    42,000 |   2.6 | ... |  40,000 |  | ... |  | ... |  | ... | 2,000
 1.3 |    18,500 | Russia (estimated) |    18,000 |   1.1 | ... | ... |  | 18,000 | (?) |  |  |
 4.8 |    71,000 | Central Powers (estimated) |    71,000 |   4.4 | ... | ... |  | 71,000 |  |  |  |
 1.4 |    19,000 | Norway |    19,000 |   1.2 | ... |  10,000 |  | ... |  | ... |  | ... | 9,000
 0.1 |     1,000 | Sweden |     1,000 |   0.1 | ... | ... |  | ... |  | ... |  | ... | 1,000
 0.4 |     6,250 | Other countries |     6,250 |   0.4 | ... |     250 |  | ... |  |  2,000 |  | ... | (3,000) (Italy)
|  |  |  |  |  |  |  |  |  | (1,000) (China)
24.6 |   354,700 | Total Eastern Hemisphere |   383,250 |  23.8 |  |  |  |  |  | 31,500
World Total | 1,456,869 |  | 1,613,250 | 100   | 1,113,000 | 212,750 |  | 98,000 |  | 31,000 |  | 125,000 |
100% |  |  |  |  | 69[106] | 13.3[106] | 6.1[106] | 1.9[106] | 7.7[106] | 2.0%, divided as follows: Cuba, 0.5; Spain, 0.1; Norway, 0.6; Sweden, 0.05; Chile, 0.5; China, 0.05; Italy, 0.2

[105] Включает бельгийский капитал.

[106] Доля владения.

Таблица 36. — Бизнес-контроль над мировыми медными рудниками. Все цифры в метрических тоннах

Country
of
origin
Estimated
capacity
output of
refined
copper
Refined
in
the U. S.
Refined
in
British
Dominions
Refined
in
Germany
Refined
in
France
Refined
in
Japan
Refined
in
other
countries
Formerly
sold by
German
houses

Western Hemisphere |  |  |  |  |  |  |  |
United States |   928,000 |  |   928,000 | ... | ... | ... | ... | ... | ( 73,000)
Canada |    58,000 |  |    28,000 |  30,000 | ... | ... | ... | ... | ( 21,000)
Mexico |    65,000 |  |    52,000 | ... | ... | 13,000 | ... | ... | (  2,500)
Cuba |    10,000 |  |    10,000 | ... | ... | ... | ... | ... | ( 10,000)
Venezuela |     2,000 |  |     2,000 |  |  |  |  |  |
Chile |   110,000 |  |    43,000 |   2,500 | ... |  9,500 | ... | 55,000 | ( 20,000)
Peru |    45,000 |  |    45,000 |  |  |  |  |  |
Bolivia |    12,000 |  |     6,000 | ... | ... |  6,000 |  |  |
Total Western Hemisphere | 1,230,000 |  | 1,114,000 |  32,500 |      0 | 28,500 |       0 | 55,000 | (134,500)
Percent of total | 76.2%[107] |  | 69 | 2 | ... | 1.8 | ... | 3.4 (Chili copper) (U. S. owned) | (8¹⁄₄%)
Eastern Hemisphere |  |  |  |  |  |  |  |
|  |  | (or in Belgium) |  |  |  |  |
Africa |    58,000 |  |     5,000 |  53,000 | ... | ... | ... | ... | (  5,000)
Australia |    43,000 |  | ... |  43,000 | ... | ... | ... | ... | ( 43,000)
Japan |   125,000 |  |     3,000 | ... | ... | ... | 122,000 |  |
Spain and Portugal (estimated) |    42,000 |  |     2,000 |  35,000 | ... |  5,000 | ... | ... |
Russia (estimated) |    18,000 |  | ... | ... | ... | ... | ... | ... | ?
Central Powers |    71,000 | ? | ... | ... | 71,000 | ... | ... | 18,000 | ?
Norway |    19,000 |  | ... |  19,000 | ... | ... | ... | ... | ?
Sweden |     1,000 |  | ... |   1,000 | ... | ... | ... | ... | ?

Other Countries
    6,250

...
    250
...
 2,000
...
 3,000
(Italy)
 1,000
(China)

Total Eastern Hemisphere |   383,250 |  |    10,000 | 151,250 | 71,000 |  7,000 | 122,000 | 22,000 | ( 48,000)
Percentage of total | 23.8 |  |   .7 |  9.3 | 4.4 |  .4 | 7.6 | 1.4 | (3%)
Total percentage | 100% |  | 69.7 | 11.3 | 4.4 | 2.2 | 7.6 | 4.8 | (11¹⁄₄%)

[107] Соединенные Штаты контролируют продажу практически всей этой меди.

Таблица 37. — Будущая значимость нынешних стран-производителей меди, определяемая по известным запасам медной руды и капиталу, контролирующему эти запасы

Producing
country
Estimated
capacity
output
of copper
(metric tons)
Percentage
of world total
Developed reserves in terms of
years’ life at capacity output
Exten-
sion[108]
Percentage
of
total
reserves
of world

Owned by
U. S.
capital
Owned by
British
capital
Owned by
German
capital
Owned by
French
capital
Owned by
Japanese
capital
Owned by
local capital
in producing
countries

W. Hemisphere: |  |  |  |  |  |  |  |  |  |
United States |   928,000 |  57.5 | 12.4 | yrs. | 12 | .4 yrs. | ... | ... | ... | ... |   713   | 34 | .
Canada |    58,000 |   3.6 | 15   |  | 20 |  | ... | ... | ... | ... |    63.3 | 3 | .
Mexico |    65,000 |   4.0 | 5   |  | large | large | 6 yrs. | ... | ... |    20.8 | 1 | .15
Cuba and Venezuela |    12,000 |   0.7 | ... |  | ... | 3 |  yrs. | ... | ... | 3 yrs. |     2.1 | 0 | .10
Chile |   110,000 |   6.8 | 150   |  | 3 |  | ? | 5⁫  | ... | consider- able |   795.8 | 37 | .9[109]
Peru |    45,000 |   2.8 | 4   |  | ... | ... | ... | ... |  |    11.2 | 0 | .55
Bolivia |    12,000 |   0.8 | ... |  | ... | ... | 4   | ... | ... |     2.8 | 0 | .10
Total | 1,230,000 |  76.2 | ... |  | ... | ... | ... | ... | ... | 1,609.0 |
Percentage total reserves | ... |  76.8 | 73.6 |  | 2 | .4 | 0 | .1 | 0.4 | ... |  0.3  | ... | 76 | .8
Eastern Hemisphere: |  |  |  |  |  |  |  |  |  |
Africa |    58,000 |   3.6 | ... |  | 66 | [110] | ... | ... | ... | ... |   237.6 | 11 | .3
Australia |    43,000 |   2.7 | ... |  | 7 | .2 | ... | ... | ... | ... |    20   | 0 | .95
Japan |   125,000 |   7.7 | ... |  | ... | ... | ... | 6   | ... |    46.2 | 2 | .2
Spain and Portugal |    42,000 |   2.6 | ... |  | 50 |  | ... | ... | ... | 50    |   130   | 6 | .2
Russia |    18,000 |   1.1 | ... |  | 18 | (?) | 18 | (?) | ... | ... | 18    |    19.8 | 0 | .95
Central Powers |    71,000 |   4.4 | ... |  | ... | ? | ... | ... | ? |    20   | 0 | .95
Norway |    19,000 |   1.2 | ... |  | 10 |  | ... | ... | ... | 10    |    12   | 0 | .55
Sweden |     1,000 |   0.1 | ... |  | ... | ... | ... | ... | 10    |     1   | 0 | .04
Other countries |     6,250 |   0.4 | ... |  | ... | ... | ... | ... | ? |     1.4 | 0 | .06
Total |   383,250 |  23.8 | ... |  | ... | ... | ... | ... | ... |   488.0 |
Percentage total reserves | ... |  23.2 | ... |  | 18 | .4 | 0 | .95 | ... | 2.2 |  1.65 | ... | 23 | .2
World total | 1,613,250 | 100   | ... |  | ... | ... | ... | ... | ... | 2,097.0 |
Percentage of world total reserves | ... | ... | 73.6 |  | 20 | .8 | 1 | .05 | 0.4 | 2.2 |  1.95 | ... | 100 |

[108] «Расширение» является произведением «Процента от мирового итога» на «Разведанные запасы в годах эксплуатации» и дает общую конечную относительную значимость различных стран.

[109] В той мере, в какой это влияет на производство, эта высокая цифра должна быть скорректирована из-за компактности крупных запасов, удаленности от рынка и неблагоприятных условий добычи в малонаселенной стране.

[110] Катанга составляет 65/66 от этого объема.

Примечание. — Не следует придавать большого значения цифрам, указывающим на срок эксплуатации более 10 лет. Общая полная будущая стоимость за длительный период времени значительно снижается при выражении в текущей стоимости с учетом нормального дисконтирования процентов. Все страны с запасами, рассчитанными на десять или более лет, можно считать находящимися в равном положении, что касается медных ресурсов. Однако крупные запасы могут означать расширение производства (как в Чили и Африке) и быть важными именно по этой причине.

Для оценки запасов руды они были взяты в совокупности, но положение Испании по сравнению с Соединенными Штатами не ухудшилось бы, если бы ее запасы были оценены в 10 лет вместо 50 (как рассчитано выше). Ее запасы оказались того рода, который легко оконтурить, но объем добычи остается неизменным.

Таблица VIII. — Географическое распределение основных меднорудных районов мира. Автор: Ф. У. Пейн.

Таблица 35 показывает различные страны мира, производящие медь, и основные особенности финансового контроля над добывающими рудниками. Таблица 36 показывает основные особенности бизнес-контроля (контроль над переработкой и продажей), в отличие от контроля через владение рудниками. В обеих таблицах сделан прогноз будущих условий с использованием оценок производства за 1918 и 1919 годы. Эти цифры прослежены до различных форм контроля. Фактические объемы производства за 1916–1917 годы приведены для справки и проверки. Таблица 37 показывает запасы, в основном на действующих рудниках. Таблица VIII показывает расположение основных месторождений меди в мире.

СЕВЕРНАЯ АМЕРИКА

СОЕДИНЕННЫЕ ШТАТЫ

Производство.

— Максимальный объем добычи меди на рудниках в пределах Соединенных Штатов был достигнут в 1916 году и составил 1 927 850 548 фунтов. В 1917 году объем производства был ниже из-за трудовых конфликтов, но шесть ведущих штатов показали рост, и если бы Монтана достигла уровня производства 1916 года, объем производства в 1917 году составил бы 1 962 034 512 фунтов. Без хороших рынков сбыта и благоприятных условий труда производство в Соединенных Штатах не может достичь уровня, близкого к 2 000 000 000 фунтов в год.

Коммерческий контроль

Контроль через владение рудниками.

— Все продуктивные медные тела в Соединенных Штатах принадлежат американцам, за исключением небольшого числа, контролируемого английским капиталом. До войны были свидетельства германской аффилированности и потенциального контроля в медной промышленности, но это было сосредоточено на переработке и продаже металла. Соответственно, германская хватка в отрасли была высокоцентрализованной, и для ее преодоления были использованы прямые и эффективные меры.

Пять ведущих групп контролируют производство меди в Соединенных Штатах. Некоторые из них имеют дополнительные важные доли собственности в Южной Америке и Мексике, что будет обсуждаться в разделах, посвященных этим странам.

Таблица 38. — Ведущие финансовые группы, контролирующие производство меди в Соединенных Штатах

| Pounds
Group 1. Hayden-Jackling “porphyries” (closely affiliated with group 2) Utah Copper, Ray Consolidated (Ariz.), Nevada Consolidated, (Nev.) Chino (N. Mex.) and Butte & Superior (Mont.); 1917 output (custom ore not included) | 448,887,253

Group 2. Morgan-Guggenheim (American Smelting & Refining Co). Kennecott (Alaska) and a large number of smaller mines owned by Americans which have their ore treated at plants controlled by this group. The 1917 output of Kennecott and eleven of the chief customers of American Smelting & Refining plants (smaller custom shipments to smelters must be added) was
156,954,722

Group 3. Rockefeller-Ryan: Anaconda, Inspiration, North Butte, Utah Consolidated, Mountain Copper (Cal.), Balaklala (Cal.), Walker mine (Cal.), and Arizona Copper Co., 1917 output (custom ore not included) | 357,308,558
Group 4. Phelps-Dodge and affiliations: Arizona and New Mexico only. Copper Queen, Detroit, Burro Mountain, Commercial Mining Co. (Phelps-Dodge); 1917 output | 123,000,000
Calumet & Arizona—New Cornelia (Briggs-Congdon); 1917 output | 79,360,000
United Verde Extension (affiliated with each of above); total 1917 output | 63,242,784
To which must be added custom business which is important, e.g., Arizona Commercial mine, etc.; 1917 business (other custom ore not included) about | 10,000,000
Total for group 4 | 275,603,113
Group 5. Calumet & Hecla: 1917 output, Calumet & Hecla mine and subsidiaries | 168,765,033
Total 1917 output of these five leading groups[111] | 1,407,518,679

[111] За исключением мелких рудников (поставщиков давальческой руды), частично контролируемых через контракты на плавку и переработку теми же интересами.

Важные более мелкие группы можно перечислить следующим образом:

Group 6. W. A. Clark: United Verde, Elm Orlu (Mont.) and Ophir Hill (Utah); 1917 output | 88,390,038
Group 7. Adolph Lewisohn: Miami and, by sale of output, Shattuck-Arizona; 1917 output | 57,058,666
Group 8. U. S. Smelting, Refining & Mining Co. Custom ore and Mammoth mine, Cal., Utah Apex, and Tintic (Utah) mines; 1917 output | 22,600,000
Group 9. Lake mines (other than Calumet & Hecla): Copper Range Co., Mohawk, Quincy, etc.[112]; 1917 output | 99,700,000

[112] Десять различных интересов.

Существует также группа, обсуждаемая ниже, с неопределенными или неклассифицируемыми аффилиациями, принадлежащая американцам, но во многих случаях работающая по контрактам на плавку и переработку, которые заслуживают особого упоминания:

| 1917 output, pounds
Old Dominion (Ariz.), (perhaps group 4) | 25,758,381
East Butte (and custom ore), (perhaps group 9) | 18,000,000
Shannon Copper Co., (Ariz.), (independent) | 6,138,219
Penn. Mining Co. (Cal.) (independent) | 3,400,000
Cons. Arizona Smelting Co. (independent) | 5,000,000
Ducktown Sulphur, Copper & Iron Co., Ltd. (Tenn.), (English) | 5,523,573
Total unclassifiable and uncertain | 63,820,173
Total of groups 1 to 5 | 1,407,518,679
Total of groups 6 to 9 | 267,748,704
Total of all interests | 1,739,087,556
Total 1917 United States copper production (from domestic mines only) | 1,873,546,171
Balance (custom ore from small shippers)[113] | 134,458,614

[113] Этот остаток включает медь, произведенную как побочный продукт при добыче других металлов в Колорадо и на Востоке, оцениваемую в 50 000 000 фунтов, и давальческие поставки с 1000 мелких предприятий, главным образом на плавильные заводы, контролируемые группами 1, 2, 3, 4 и 6, оцениваемые в 84 458 614 фунтов.

Некоторые рудники в вышеуказанных группах принадлежат Англии, но классифицируются вместе с тем интересом, который перерабатывает и продает продукцию. В группе 2, например, указана Tennessee Copper Co., чья медь перерабатывается и продается на заводе American Smelting & Refining в Балтиморе. Однако по праву собственности это предприятие следует отнести к группе 7 (объем производства 10 547 704 фунта).

В группе 3 находятся два рудника, принадлежащих англичанам: Arizona Copper Co. (шотландская) и Mountain Copper Co. (английская). Ducktown Sulphur, Copper & Iron в последней группе (неопределенной и неклассифицируемой) также принадлежит англичанам. Совокупный объем производства этих трех английских предприятий составляет 48 000 000 фунтов. Это охватывает все предприятия, не принадлежащие американскому капиталу. Ducktown Sulphur, Copper & Iron Co., Ltd. принадлежит англичанам, но вся ее продукция (медный штейн) продается компании American Metal Co. Остальные в группе, обозначенной выше как неопределенная или неклассифицируемая, полностью принадлежат американцам, хотя их продукция продавалась компаниями American Metal Co. или L. Vogelstein, как обсуждается ниже.

Ни одна из этих групп не владеет рудниками напрямую, так как рудники принадлежат множеству акционеров, разбросанных по всей стране. Во многих компаниях президент и директора владеют очень небольшой долей акций. Что касается группы 6 и, в меньшей степени, группы 4, однако, фактическая собственность находится в очень немногих руках; но это исключение. Медные рудники Соединенных Штатов, подобно железным дорогам и крупнейшим промышленным предприятиям, таким как United States Steel Corporation и т. д., в конечном счете контролируются своими акционерами.

Суммируя на основе данных об объеме производства за 1917 год, можно обнаружить, что собственность на американские медные рудники распределяется следующим образом: американская — 97,5 процента, английская и шотландская — 2,5 процента.

Контроль через владение плавильными и перерабатывающими заводами.

— Владение плавильными заводами, которые перерабатывают внутреннюю руду, по существу идентично владению рудниками, указанному выше. Интересов, владеющих действующими плавильными заводами, меньше, чем интересов, владеющих рудниками, поскольку эффективная плавка требует крупномасштабных операций.

Электролитические перерабатывающие заводы полностью принадлежат американцам. Крупномасштабные установки, представляющие собой значительные капиталовложения, необходимы для электролитической переработки. Небольшой перерабатывающий завод не может успешно конкурировать с крупными. Средний важный медный рудник производит достаточно руды, чтобы получить около 25 000 000 фунтов в год, тогда как средний плавильный завод производит в три или четыре раза больше черновой или литейной меди, а средний электролитический перерабатывающий завод может производить более 250 000 000 фунтов ежегодно. Следовательно, существует только шесть групп (Hayden-Jackling, Morgan-Guggenheim, Rockefeller-Ryan, Phelps-Dodge, Calumet & Hecla и U. S. Smelting, Refining & Mining Co.), заинтересованных во владении перерабатывающими заводами. Ни один мелкий производитель не обладает капиталом или размером, чтобы иметь возможность выйти в эту область. Таблица 39 показывает электролитические медные перерабатывающие заводы Соединенных Штатов и их владельцев:

Таблица 39. — Владение и мощность американских медных перерабатывающих заводов

Works | Ownership, group— | 1917 capacity (pounds)
Baltimore Copper Smelting & Rolling Co. | 1 and 2 | 720,000,000
Nichols Copper Co. Independent and in part | 4 | 500,000,000
Raritan Copper Works | 3 | 460,000,000
American Smelting & Refining Co. | 1 and 2 | 288,000,000
United States Metals Refining Co. | 8 | 250,000,000
Tacoma Smelting Co. | 1 and 2 | 204,000,000
Anaconda Copper Mining Co. (new plant) | 3 | 180,000,000
Calumet & Hecla Mining Co. | 5 | 65,000,000
Anaconda Copper Mining Co. (old plant) | 3 | 65,000,000
Balbach Smelting & Refining Co.[114] (former German affiliations) | ... | 48,000,000
Total capacity |  | 2,780,000,000
|  | 1917 production (pounds)
Electrolytic copper | ... | 1,452,744,593
Secondary electrolytic copper | ... | 66,337,771
Imported copper made into electrolytic | ... | 555,000,000
Total 1917 refinery production | ... | 2,074,082,364

[114] Эта компания перерабатывает медный лом и импортные медные руды и штейн.

Перерабатывающие заводы контролируют ситуацию в очень значительной степени. Производитель меди должен получить электролитическую переработку, чтобы продать свой продукт. Озерная медь и литейная медь не требуют электролитической переработки, хотя производители литейной меди часто находятся в невыгодном положении, когда существует большая премия на электролитическую медь, а литейную медь можно продать только с большой скидкой.

Плавильные заводы не контролируют ситуацию таким же образом. В Соединенных Штатах существует большое количество давальческих плавильных заводов — 32, — которые активно конкурируют за руду; некоторые имеют много филиалов. Более того, рудник любого размера будет иметь свой собственный плавильный завод, так как капитальные вложения гораздо меньше, чем те, что требуются для электролитического перерабатывающего завода. Как показывает таблица, есть только семь групп (шесть вышеперечисленных и Balbach Smelting & Refining Co.), заинтересованных в электролитической переработке, и одна из них (самая маленькая) в значительной степени заинтересована в переработке вторичной меди или лома.

Контроль электролитических перерабатывающих заводов над производством меди в Соединенных Штатах показан цифрами за 1917 год. В том году производство электролитической меди составило 1 452 744 593 фунта; озерной меди — 238 508 091 фунт; и литейной меди — 152 293 487 фунтов. Таким образом, электролитическая медь составила 77,5 процента от общего объема.

Контроль через продажу и распределение меди в готовом виде.

— Группы, владеющие рудниками, плавильными и перерабатывающими заводами, неизменно также контролируют или владеют торговыми агентствами, которые распределяют продукт потребителю. В этих случаях контроль через продажу такой же, как контроль через владение рудниками, но он увеличивается за счет меди в рудах, поступающих на давальческие плавильные заводы.

Контроль через продажу, таким образом, идентичен контролю, показанному в Таблице 38, что касается групп 1, 2, 3, 4 и 8, если сделать определенные дополнения за счет других групп. Но каждый производитель озерной меди контролирует продажу своего продукта, потому что озерная медь не нуждается в электролитической переработке. Следовательно, в группах 5 и 9 владение рудниками и контроль через продажу идентичны. Это факт, представляющий значительный интерес, и он подтверждает факт контроля через владение перерабатывающими заводами. Группы 6 и 7 (Таблица 38) являются крупными производителями, и хотя они не владеют перерабатывающими заводами, они способны контролировать продажи своего продукта. Перерабатывающие заводы готовы перерабатывать их медь за плату и возвращать товарную медь владельцам рудников, которые осуществляют продажу на рынке. Группы 2, 3 и 7 теперь контролируют медь еще дальше, так как они владеют латунными, проволочными и прокатными заводами и т. д. Они производят часть своей продукции и продают ее как медную проволоку, готовую латунь и т. д., вместо того чтобы осуществлять продажи на латунные и проволочные заводы слитков, прутков, чушек и т. д., что является и всегда было общей практикой.

Остается рассмотреть контроль через продажу шести неопределенных групп (общий объем производства 63 820 173 фунта) и части из 134 458 614 фунтов меди, произведенной из давальческой руды. Большая часть этого, как было отмечено, сосредоточена в группах 1, 2, 3, 4 и 8.

В течение многих лет три концерна, аффилированные с германскими металлическими объединениями (Merton Co. и Metallgesellschaft из Франкфурта-на-Майне и Aaron Hirsch из Хальберштадта), были активны в медном бизнесе Соединенных Штатов. Их деятельность ограничивалась продажей меди, произведенной в этой стране, а также владением и продажей меди, произведенной в зарубежных странах, но привезенной в Соединенные Штаты для плавки и переработки. Один небольшой перерабатывающий завод принадлежит или принадлежал этой группе в Соединенных Штатах, а также два плавильных завода, перерабатывающих в основном иностранные руды. Она также владеет плавильными заводами в Мексике и Южной Америке и имела тесные связи с двумя крупными перерабатывающими заводами в Нью-Джерси, благодаря чему продавала всю электролитическую медь, произведенную одним заводом, и значительную часть продукции другого завода.

Германский контроль над американской медью.

— Точная германская собственность на эти концерны была раскрыта во время войны работой Управляющего имуществом иностранцев и была следующей: (1) American Metal Co. с выпущенным капиталом в 7 000 000 долларов, из которых германские доли составляли 3 336 000 долларов, или около 50 процентов; эти доли были взяты под контроль властями Соединенных Штатов; (2) L. Vogelstein & Co., 80 процентов акций которой принадлежали немцам (A. Hirsch & Sohn) и 15 процентов — Л. Фогельштейну, натурализованному американскому гражданину; (3) Beer, Sondheimer & Co., полностью принадлежащая немцам. Правительство конфисковало два последних названных концерна.

American Metal Co. продает медь компаний Old Dominion, East Butte, Shannon, Penn. Mining Co. и Ducktown Sulphur, Coal & Iron. Черновая медь чистотой 99 процентов закупается по контракту у первых четырех названных компаний компанией American Metal Co. Эта медь перерабатывается для American Metal Co. компанией Nichols Copper Co., а готовый продукт продается на рынке компанией American Metal Co. Ducktown Sulphur, Copper & Iron Co. продает всю свою продукцию в виде медного штейна компании American Metal Co., которая подвергает ее обработке и продает готовый продукт. Таким образом, 58 820 173 фунта контролировались через продажу компанией American Metal Co. в 1917 году. Кроме того, значительное количество внутренней давальческой руды и большое количество меди, импортируемой из Канады (Granby), Южной Америки и Мексики, обрабатывается компанией American Metal Co. таким же образом. Такая импортная медь в три раза превышает объем внутренней меди, контролируемой таким образом.

Что касается внутренней меди, эта ситуация будет исправлена. Nichols Copper Co. свободна перерабатывать эту медь и продавать ее или возвращать производителям для продажи; она делает последнее для Phelps-Dodge и Miami. Можно предположить, что контроль через продажу прекратится в отношении 58 820 173 фунтов, упомянутых выше, а также в отношении продукции Granby — около 50 000 000 фунтов.

American Metal Co. может быть продана американским интересам [115], тем самым в некоторой степени проясняя ситуацию с импортной медью. Некоторые мексиканские и чилийские предприятия, принадлежащие American Metal Co., возможно, не будут проданы, и такие предприятия можно считать, вероятно, всегда принадлежащими немцам.

[115] Сообщается, что германские доли в American Metal Co. проданы американскому синдикату, в котором участвовал Л. Фогельштейн.

American Metal Co. владеет электролитическим перерабатывающим заводом Balbach и от переработки лома и импортной меди (чилийская и японская черновая медь) на этом заводе получает и продает около 50 000 000 фунтов рафинированной меди в год.

Концерн L. Vogelstein & Co. потерял свой главный контроль над американским производством меди в 1915 году. До того времени L. Vogelstein & Co. очень тесно сотрудничала с группой 8 (United States Smelting, Refining & Mining Co.). Продукция рудников и плавильных заводов United States Smelting Refining & Mining Co. продавалась Фогельштейном, так же как и продукция ее электролитического перерабатывающего завода. Но с 1915 года это американское предприятие само продает всю медь, произведенную на собственных рудниках и плавильных заводах.

Но Фогельштейн по-прежнему контролирует продажу меди, перерабатываемой на заводе United States Metals Refining Co. [116], сверх того, что производится United States Smelting, Refining & Mining Co. на собственных рудниках и плавильных заводах. Эта оставшаяся медь состоит частично из импортной меди, а частично из продукции Consolidated Arizona Smelting Co., которая является американским предприятием. Объем производства был большим в 1917 году (около 20 000 000 фунтов), но три четверти его составляла руда с рудника United Verde Extension. United Verde Extension с тех пор завершила строительство собственного плавильного завода и больше не передает часть своей медной продукции Фогельштейну через Consolidated Arizona Smelting Co. Продукция United Verde (группа 6) также ранее продавалась Фогельштейном, но теперь продается владельцем рудника.

[116] United States Metals Refining Co. была дочерней компанией United States Smelting, Refining & Mining Co., проданной в 1920 году компании American Metal Co.

Следовательно, единственной медью, контролируемой в 1918 году Фогельштейном через продажу, было около 50 000 000 фунтов в год, продукция рудников, принадлежащих Consolidated Arizona Smelting Co. (около 5 000 000 фунтов), и импортная медь, из которой около 45 000 000 фунтов было переработано в 1917 году. Последняя контролируется Фогельштейном не только продажей продукта, но частично контрактами на плавку и частично, вероятно, что касается Южной Америки, владением рудниками. [117]

[117] Сообщается, что Л. Фогельштейн продал свои интересы компании American Metal Co. и впоследствии, в начале 1920 года, приобрел пятую долю в этой компании.

Beer, Sondheimer & Co.

никогда не была крупным фактором в медной промышленности Соединенных Штатов, хотя была очень заинтересована в цинке. Но фирма действительно контролирует продажу некоторого количества меди и владеет плавильным заводом в Норфолке. Этот плавильный завод перерабатывает импортные руды по большей части, но также получает некоторое количество меди из пиритов (серных руд), поступающих из Соединенных Штатов и Канады. Возможно, до 10 000 000 фунтов внутренней меди было продано Beer, Sondheimer & Co. в 1917 году. Компания владеет важным кубинским рудником.

Поскольку американский капитал владеет американскими медными рудниками, плавильными и перерабатывающими заводами, германские интересы смогли получить плацдарм только через торговые организации (торговля металлами), которые позже они расширили до тесных рабочих соглашений с электролитическими перерабатывающими заводами, которые были естественно заинтересованы в поиске хорошего денежного рынка для своей продукции. Тот факт, что Германия до 1914 года была крупнейшим иностранным покупателем американской меди, облегчил успешное развитие тщательно разработанных германских планов.

В будущем от таких планов можно защититься, поощряя производителей меди продавать свою собственную продукцию. Все крупные производители уже делают это, изменение в этом отношении произошло с 1914 года. Продажи на иностранных рынках теперь могут должным образом управляться в соответствии с положениями недавнего законодательства, разрешающего производителям меди вступать в объединения для продажи экспортной меди. Это противодействует старой германской системе объединения покупателей против продавцов меди, что было важным фактором, вынуждающим американских производителей позволять германским концернам продавать свой продукт. Но электролитическим перерабатывающим заводам необходимо будет сотрудничать в этой политике американского контроля продаж американской меди. Производители, чей объем производства составляет всего несколько миллионов фунтов в год, вероятно, не могут позволить себе создать свои собственные торговые агентства; такие производители будут включать всех, у кого нет плавильного завода, но кто отгружает руду на давальческие плавильные заводы. Продукция может продаваться крупными давальческими плавильными заводами, которые принадлежат американцам, или эти мелкие производители могли бы создать общее торговое агентство. Другие более крупные производители, такие как те, чья медь сейчас продается компанией American Metal Co., должны иметь возможность осуществлять свои собственные продажи. В этом они были заблокированы отсутствием перерабатывающих мощностей, за исключением условий, которые лишали их контроля над продажей своего продукта. Эту ситуацию можно исправить с помощью правил, которые ставят электролитические перерабатывающие заводы на признанную давальческую основу для всех американских клиентов. Все перерабатывающие заводы имеют примерно одинаковые затраты, и их совокупная мощность достаточна для переработки всей черновой меди, которая будет произведена. Они должны получать хорошую прибыль от бизнеса, но должно быть незаконным для перерабатывающих заводов отказываться перерабатывать черновую медь на давальческой основе и настаивать на том, что медь должна быть продана им напрямую. Давальческая система уже используется на нескольких перерабатывающих заводах и доказала свою удовлетворительность.

Как показано выше, в Соединенных Штатах есть несколько очень крупных перерабатывающих заводов, собственность на которые находится в немногих руках. Если эти перерабатывающие заводы контролируют продажу всей продукции меди, возникают несколько нежелательных особенностей. Несколько торговых агентств обрабатывают так много меди, что существует тенденция к сотрудничеству с представителями иностранных потребителей, которые могут покупать в больших количествах, и нетрудно манипулировать рынком временно, в игнорирование фактических условий спроса и предложения. Таким образом, весь объем производства меди, одного из наших великих природных ресурсов, оказывается в руках групп, которые, будучи заинтересованными в добыче, больше заинтересованы в переработке. Лучшие интересы отрасли ближе к интересам горняка, чем переработчика. Поэтому наиболее позитивное вытеснение бывшего германского контроля над медью через продажу произойдет от разрушения бывшей системы и передачи каждого звена этой системы в другие руки; а не от передачи старых звеньев целиком в негерманские руки. Продажи американской меди должны осуществляться большим количеством отдельных агентств, активно конкурирующих за внутренний рынок; это важно в интересах потребителя и страны. Но экспортный медный бизнес должен осуществляться через одно агентство или ассоциацию, представляющую все торговые агентства, как это сейчас законно, и это должно делаться в интересах производителя и страны.

Запасы медных рудников Соединенных Штатов.

— Разведанные запасы медных месторождений Соединенных Штатов полностью равны, пропорционально объему производства, таким запасам в иностранных медных месторождениях. Это гарантирует тот факт, что в течение следующих десяти лет, по крайней мере, производство меди в Соединенных Штатах сохранит свое нынешнее относительное доминирование над всеми иностранными странами.

Большая часть всех медных месторождений имеет такой глубокий характер, что ни в какое время крупные запасы не могут быть положительно разведаны, даже когда они существуют. С другой стороны, во всем мире рудники с крупными известными запасами представляют собой горизонтальные залежи, залегающие близко к поверхности, потому что только в таких случаях возможно легко и дешево оконтурить большие тоннажи руды. В Соединенных Штатах есть шесть очень важных месторождений этого типа, так называемые «порфиры». Это:

Таблица 40. — «Порфировые» медные рудники в Соединенных Штатах

Mine | Reserves (tons) | Years of life at present production
Utah Copper Co. | 200,000,000 | 31
Ray Consolidated Copper Co. | 90,000,000 | 30
Chino Copper Co. | 80,000,000 | 27
Inspiration Consolidated | 120,000,000 | 20
Nevada Consolidated | 80,000,000 | 20
Miami Copper Co. | 50,000,000 | 20
Total | 620,000,000 | 26

Эти рудники в 1917 году произвели 31,5 процента от общего объема производства Соединенных Штатов.

Рудник New Cornelia относится к аналогичному типу и уже разведал 75 000 000 тонн, но так как он новый, его объем производства в 1917 году был небольшим. Arizona Copper Co., Ltd. также относится к этому типу, как и некоторые новые разработки на предприятиях Phelps-Dodge.

Эти «порфировые» месторождения встречаются в или вблизи интрузивных магматических пород различных возрастов. Полностью одна треть производства Соединенных Штатов сейчас и будет продолжать получаться из таких месторождений. В среднем из руды извлекается около 1 процента меди.

Отличными от неглубоких и горизонтально залегающих вкрапленных руд или «порфировых медных руд» являются глубокие рудники. Два старейших и наиболее важных района глубоких рудников в Соединенных Штатах — это Бьютт, Монтана, и полуостров Кивино, Мичиган. Рудники Бьютта работают на крутопадающих жилах. Нельзя считать, что известно более пяти лет запасов руды, и, вероятно, не более 2,5 лет запасов фактически оконтурены с трех сторон. Однако нет никаких признаков скорого истощения, так как жилы прибыльны на глубине более 3000 футов, наибольшей глубине, на которую пока продвинулась добыча. Месторождения северного Мичигана находятся в докембрийских породах. Они были важными производителями меди более 50 лет, и несколько рудников достигли вертикальной глубины более 5000 футов. Конечно, не более пяти лет запасов руды полностью разведаны, но нет никаких признаков скорого истощения. Эти два района, Бьютт и Мичиган, сейчас производят около 30 процентов от общего объема производства Соединенных Штатов, меньшая доля, чем до разработки «порфиров». Среднее содержание меди в месторождениях Мичигана колеблется от 0,5 процента до 2 процентов, а в месторождениях Бьютта — от 2,5 до 5 процентов.

Определенные рудные месторождения (обычно массивные, но нерегулярные), которые расположены главным образом в Аризоне, составляют третий важный общий класс. Эти месторождения производят около одной четверти от общего объема производства Соединенных Штатов. Бисби, Джером и Глоуб (Аризона) и Кеннекотт (Аляска) являются основными местностями. Из-за нерегулярного характера месторождений и расстояния от поверхности, на котором находится руда, крупные разведанные запасы не могут быть оконтурены заранее. Такие запасы принимаются равными пяти годам.

Помимо трех классов месторождений, описанных выше, существует много более мелких месторождений, из которых наиболее отчетливым классом являются пиритовые тела, особенно в Теннесси и Калифорнии. Такие месторождения часто прибыльны, даже когда они низкого качества, потому что сера, так же как и медь, извлекается. Запасы в таких месторождениях велики: равны, скажем, десяти годам жизни. Месторождения этого класса важны в Испании, Норвегии и частично в Японии. Рудники, производящие медь как побочный продукт, также должны быть сгруппированы здесь.

Из вышеприведенного обзора была составлена таблица ниже:

Таблица 41. — Разведанные запасы медных рудников Соединенных Штатов

General group | Percentage of total output | Years of life | Extension[118]
The “porphyries” |  35 | 26   |  9.10
Deep mines |  30 |  5   |  1.50
Rich ore bodies (Arizona and Alaska) |  25 |  5   |  1.25
Pyritic ore bodies |   5 | 10   |  0.50
Others |   5 |  2   |  0.10
Average | 100 | 12.4 | 12.45

[118] «Расширение» — это Процент от общего объема производства, умноженный на Годы жизни, что дает относительную значимость каждой группы.

Известные запасы руды служат основанием для предположения, что производство меди в Соединенных Штатах будет продолжаться на текущих цифрах в течение по крайней мере десяти лет.

КАНАДА

Канадские меднодобывающие предприятия полностью контролируются американским и британским капиталом в примерно равной пропорции, при этом предполагается, что изменения, связанные со строительством новых перерабатывающих заводов и сдвигом в контроле продаж, уже вступили в силу. До настоящего времени естественным развитием событий было то, что Канада в значительной степени зависела от Соединенных Штатов в отношении перерабатывающих мощностей. Вероятно, что в будущем местный или английский контроль в этой области будет более тесным, чем до сих пор, хотя канадская медная промышленность всегда будет тесно связана с промышленностью Соединенных Штатов.

В Канаде есть три главных медных предприятия, которые контролируются капиталом Соединенных Штатов, все в Британской Колумбии, а также несколько мелких рудников в этой провинции и в других. Безусловно, крупнейшим является Granby Consolidated Mining, Smelting & Power Co. Эта компания имеет рудники в двух районах. Одно из этих предприятий почти истощено; другое — новый и энергичный производитель. Плавильные заводы работают в каждом месте. Компания Granby контролируется теми же интересами, которые владеют Nichols Copper Co. (электролитический перерабатывающий завод). Значительное количество давальческой руды перерабатывается компанией Granby, большое количество поступает с Аляски. Два других рудника — это рудники Canada Copper Co. и Howe Sound Co. Их продукция перерабатывается и продается в Соединенных Штатах американскими концернами. Разведанные запасы на этих трех рудниках велики, будучи полностью адекватными на пятнадцать лет при текущем уровне производства.

Единственным предприятием в Канаде, которое создало мощности для производства меди, готовой для потребителя, является Consolidated Mining & Smelting Co. из Трейла, Б. К. Эта канадская компания владеет и управляет своими собственными рудниками, плавильным заводом и электролитическим перерабатывающим заводом. Мощность перерабатывающего завода сейчас составляет 14 000 000 фунтов рафинированной меди ежегодно. Руды представляют собой массивные пиритовые тела без больших разведанных запасов, но вероятные запасы велики.

Английские и американские предприятия в Садбери дают почти столько же меди, сколько компания Granby, хотя их основной бизнес — производство никеля. Небольшая часть продукции перерабатывается в Уэльсе, производя медный купорос; но большая часть перерабатывалась в Нью-Джерси. В Канаде завершается строительство перерабатывающего завода, который будет перерабатывать эти медно-никелевые штейны и производить рафинированную медь. Эти медно-никелевые месторождения встречаются в докембрийских породах, и известные или потенциальные запасы очень велики. Они описаны более подробно в Главе VI.

В Онтарио и Квебеке есть ряд пиритовых рудников, где часть пирита содержит значительное количество меди. Большая часть пирита отгружается в Соединенные Штаты, где медь извлекается, перерабатывается и продается.

Производство Канады растет, и страна будет приобретать все большее значение как источник меди. Известные запасы больше пропорционально объему производства, чем в Соединенных Штатах, и, вероятно, будут важные разработки новых районов. Район северной Британской Колумбии является исключительно многообещающим.

КУБА И КАРИБСКИЙ БАССЕЙН

Объем добычи меди на Кубе увеличился в чрезвычайной степени за последние несколько лет, но нет никаких признаков того, что этот рост продолжится. Два рудника ответственны почти за весь объем производства. Один — это старый рудник около Сантьяго, El Cobre, который давал около одной четверти от общего объема производства. Он принадлежит германскому металлическому объединению, которое отгружает руду и концентраты в Норфолк, где они перерабатываются на плавильном заводе, принадлежащем Beer, Sondheimer & Co., которые всегда продавали продукцию. Рудник Matahambre в провинции Пинар-дель-Рио дает почти весь остальной объем кубинской продукции; он принадлежит кубинцам. Руда отгружается в United States Smelting, Refining & Mining Co. из Нью-Йорка и, как полагают, продается компанией L. Vogelstein & Co. Запасы медной руды на Кубе нельзя считать большими. Статистика кубинского производства противоречива: отчеты производителей, статистические органы и отчеты о торговле Соединенных Штатов не совпадают. Вся продукция отгружается в сыром виде в Соединенные Штаты для переработки.

Существуют медные месторождения в Центральной Америке [119] и в одном или двух местах в Вест-Индии за пределами Кубы. На сегодняшний день производство было незначительным, хотя будущие возможности значительны.

[119] Рудник Rosita в Никарагуа имеет 1 500 000 тонн оконтуренной руды с содержанием меди более 5 процентов. Он не был оборудован.

МЕКСИКА

Будущая значимость Мексики как производителя меди или других металлов будет определяться не только характером ее природных месторождений, но и политическими условиями. Последние существенно снизили объем производства за последние несколько лет, так что в 1917 году производство составило около 100 000 000 фунтов, вероятно, не намного больше половины того, что было бы, если бы нормальные условия сохранялись с 1912 года.

Коммерческий контроль.

— Три компании сейчас производят около трех четвертей всей меди. Две из них принадлежат американскому капиталу, и их продукт перерабатывается и продается в Соединенных Штатах. Расположенные недалеко от границы с Аризоной, они не пострадали от революции так сильно, как предприятия дальше на юг. Эти две компании — Greene Cananea Copper Co. (Ryan-Rockefeller, группа 3 Таблицы 38) и Montezuma Copper Co. (Phelps-Dodge и др.; группа 4 Таблицы 38). Разведанные запасы в Montezuma Copper Co. эквивалентны пяти годам при текущем производстве, а запасы в Cananea можно считать примерно такими же. Оба района имеют важные возможности. Рядом с Greene Cananea находится другое американское предприятие, Democrata Cananea, которое является производителем умеренного размера. Район Cananea сейчас производит более 50 000 000 фунтов в год. Другое американское предприятие, заслуживающее внимания, — Teziutlan Copper Co., Пуэбла, сейчас простаивает из-за революций. Оно имеет плавильный завод, который обычно отгружает 12 000 000 фунтов черновой меди ежегодно на электролитический завод компании Anaconda. Значительное количество меди производится на заводах American Smelting & Refining Co., которая имеет три медных плавильных завода: один в Матеуале, Сан-Луис-Потоси; один в Асарсо и другой в Агуаскальентесе, Дуранго.

Французский капитал

контролирует третье важное предприятие (среди трех наиболее важных в Мексике), которое находится на полуострове Нижняя Калифорния. Это Boleo, принадлежащее Ротшильдам; так как оно далеко удалено от центра Мексики, операции не были сильно нарушены. Рудник является старым производителем с большими потенциальными запасами, а фактические разведанные запасы будут поддерживать текущий объем производства в течение шести лет. Месторождения руды Boleo, которые являются необычного типа, представляют собой третичные осадочные породы, содержащие 3,5 процента медной руды, обычно в виде оксидов. Плавильные заводы рядом с рудником производят черновую медь и штейн, которые обычно отгружаются во Францию. Во время войны большая часть черновой меди и штейна поступала в Соединенные Штаты и переходила в руки American Smelting & Refining Co. Французские интересы также владеют Compagnie d’Inguaran, недалеко от Арио, Мичоакан. Там есть большие разведанные запасы, но предприятие простаивает из-за политических условий и отсутствия оборудования или железнодорожных соединений. Французский капитал также контролирует Magistral Ameca Co. в Халиско, где были разведаны большие запасы руды. Это предприятие также простаивает из-за политических условий.

Английский капитал

контролирует Mazapil Copper Co., которая имеет крупные заводы, включая плавильные, в Сакатекасе и Коауиле. Это одна из крупнейших медных компаний в Мексике, а также один из старейших важных рудников. Он простаивал некоторое время из-за мексиканских революций, но недавно был вновь открыт.

Подводя итог, производство в Мексике в настоящее время на три четверти контролируется американцами (из которых половину можно отнести к группе 3 и четверть к группам 2 и 4), в то время как оставшаяся четверть контролируется французами. Но текущий объем производства и известные запасы не дают верной картины будущих возможностей. Мексика может стать первостепенным производителем меди, занимая, возможно, второе место после Соединенных Штатов или равняясь с Чили и Японией среди мировых производителей. Природные ресурсы там есть, и в будущем они, несомненно, будут развиваться гораздо более широко, чем когда-либо прежде.

Германский капитал

должен быть принят во внимание, особенно деятельность American Metal Co. в Мексике, заметно более энергичная с 1914 года, чем до этого. Считается, что компания получила существенную прибыль от мексиканских горнодобывающих инвестиций в этот период и получила очень прочный плацдарм. Compañia Metallurgica de Torreon является одной из дочерних компаний American Metal Co., владеющей многообещающими рудниками, главным образом в стадии разработки, и плавильными заводами, уже оборудованными для производства 20 000 000 фунтов меди ежегодно. Плавильный завод Mapimi также принадлежит American Metal Co., как и многие другие компании. Какова будет будущая мексиканская политическая ситуация и какую роль сыграет American Metal Co. или германское металлическое объединение в мексиканской медной промышленности? Нет более уместного вопроса во всей области политического и коммерческого контроля над медными ресурсами мира, особенно учитывая, что американский капитал в значительной степени заинтересован в мексиканских медных рудниках и сделал там огромные инвестиции. Также естественной тенденцией является отгрузка большей части мексиканской меди в Соединенные Штаты для переработки и маркетинга. Американские перерабатывающие заводы с дешевым топливом и эффективными методами являются естественным пунктом назначения для мексиканской сырой меди.

ЮЖНАЯ АМЕРИКА

Южная Америка является вторым по величине меднодобывающим континентом мира, но в настоящее время значительно отстает от Северной Америки. Страны Южной Америки, производящие медь, в порядке их значимости: Чили, Перу, Боливия, Венесуэла и Аргентина.

ЧИЛИ

Чили является производителем меди быстро растущей значимости, как показывают отчеты о производстве последних лет. [120]

[120] Согласно чилийской статистике и оценке за 1917 год.

| 1914 | 1915 | 1916 | 1917
Metric tons | 44,665 | 52,341 | 71,288 | 95,000

Крупнейшие рудники Чили контролируются американским капиталом. Группа 2 Таблицы 38 (интересы Morgan-Guggenheim) контролирует Chile Copper Co., Braden Copper Co. и давальческие плавильные заводы Caldera и Carrizal. Разведанные запасы руды Chile Copper Co. являются крупнейшими среди всех известных медных месторождений в мире, а запасы Braden — одними из крупнейших известных. Группа 3 Таблицы 38 (Anaconda Copper Co.) имеет предприятие с большими разведанными запасами руды — Andes Copper Co. Этот рудник еще (1918) не производит.

Таблица 43 (стр. 243) дает данные об этих рудниках, принадлежащих американцам.

Эти три рудника по характеру близки к «порфирам» Соединенных Штатов, но они менее прибыльны, потому что внешние условия делают эксплуатацию более трудной.

Таблица 42. — Главные производители меди в Чили. Их собственность и относительная значимость

Controlled by capital of | Company | Plant capacity, 1918 (pounds a year) | Nature of product | Source of product | Remarks
United States | Chile Copper Co. | 120,000,000 | Refined copper | Mines of the Company | Capacity will be increased
Do | Braden Copper Co. |  72,000,000 | Blister copper | Do | Do
Do | A. S. & R. Co. |  24,000,000 | Blister copper and matte | Local owned mines | Caldera plant
Do | A. S. & R. Co., custom smelters |  24,000,000 |  | Do | Carrizal plant
| Total United States | 240,000,000 |  |  |
| United States properties’ reserves | 150 years |  |  |
England | Central Chile Co. |   6,000,000 | Matte | Panulcillo mine ¹⁄₃ | Balance custom ore
Do | Poderosa mine |   2,000,000 | Ore (rich) |  | Shipped to U. S.
Do | Lota custom smelter |   8,000,000 | Blister | Largely custom ore | Treat custom matte
| Total British |  16,000,000 |  |  |
| British properties’ reserves | 3 years |  |  |
France | Chanaral |  15,000,000 | Blister and matte | Mines of the company |  | - | Product treated at Balbach plant (U. S.) in 1917
Do | Naltagua |  10,000,000 | Blister | Mines of the company
| Total French |  25,000,000 |  |  |
| French properties’ reserves | 5 years |  |  |
Belgium | Catemo |  11,000,000 | Blister | Mines of the company | Refined by Balbach, 1917.
| Reserves | 5 years |  |  |
Germany | Gatico smelter |   8,000,000 | Blister | Custom ore and mines controlled. | Tributary to rich mining district.
| Guayacan smelter |   3,000,000 | Matte |  | Formerly shipped matte to England.
Chile | 6 mines with smelters |   5,000,000 | Matte | Locally owned mines | Shipped to big smelters or exported.
| Great numbers of mines | large | Ore | Locally owned mines | Shipped to big smelters or exported.
| Grand total | 308,000,000 |  |  |
| Expected output 1918-1919 | 244,000,000 (110,000 metric tons) |  |  |

Таблица 43. — Объем производства, запасы и срок эксплуатации трех медных рудников в Чили, принадлежащих американцам

Company
Output,
First six months
of 1918,
(pounds)
Ore reserves
(tons)
Life at
present output,
(years)

Chile | 50,000,000 | 350,000,000 | 200
Braden Copper Co. | 36,000,000 | 150,000,000 | 125
Andes Copper Co. | non-producing (capacity 24,000,000) | 50,000,000 | Work suspended for present

Давальческие плавильные заводы Caldera и Carrizal компании American Smelting & Refining Co. перерабатывают руды, отгружаемые с различных более мелких рудников. Завод Carrizal был закрыт. Два главных предприятия являются притоками этого завода — рудники Carrizal Alto и Astilla. Большое количество предприятий являются притоками завода Caldera, среди них: Dulcinea, Flamenco, Morado, San Juan, El Gallo и т. д. По всей северной Чили есть множество мелких медных рудников. От предприятия Braden к востоку от Вальпараисо до Chili Copper Co. к юго-востоку от Икике вся страна кажется необычайно богатой медью.

Есть пять важных чилийских рудников, контролируемых французским или британским капиталом. См. Таблицу 42. Все они являются жильными рудниками без значительного тоннажа разведанных запасов руды, и совокупный объем производства составляет почти 50 000 000 фунтов меди в год (значительная часть — из давальческой руды, отгружаемой мелкими рудниками) в виде черновой меди или штейна. Эта продукция обычно отгружается во Францию или Англию.

American Metal Co. и L. Vogelstein, представляющие германский капитал, как полагают, контролируют через продажу и переработку большую часть продукции французских, британских и бельгийских рудников. Эти концерны также владеют давальческими плавильными заводами в Чили и, вероятно, имеют интересы во многих горнодобывающих предприятиях там. Крупный бизнес по чилийским рудам, отгружаемым в Соединенные Штаты, ведется этими концернами, хотя American Smelting, Refining & Mining Co. также является важным фактором. Эти руды поступают со многих мелких рудников, хотя есть несколько важных грузоотправителей руды, один из которых принадлежит британцам. Большинство рудников по видимости принадлежат чилийцам, но большая часть финансирования, маркетинга продукции и т. д. осуществляется американскими домами с германскими аффилиациями.

По-видимому, Чили вскоре может стать вторым по величине производителем меди в мире. Американский капитал сыграл ведущую роль в освоении чилийских месторождений, поскольку американские интересы обнаружили два крупнейших месторождения и предоставили средства для их оснащения, а третье по значимости рудное тело также принадлежит американцам. Это тем более примечательно, что американский капитал до сих пор практически отсутствовал в развитии других важных отраслей промышленности Чили. Если бы не нынешние трудности с созданием производственных мощностей, вызванные нехваткой судов, высокой стоимостью оборудования и т. д., принадлежащие американцам медные рудники сегодня были бы еще более крупными производителями, чем они есть. Тем не менее, американский капитал в настоящее время полностью контролирует около семи восьмых общего объема добычи. Почти вся медь, производимая в Чили, отправляется в Соединенные Штаты. Компания Chili Copper Co. производит в Чили рафинированную электролитическую медь, и это единственная готовая рафинированная медь, производимая в Южной Америке. Braden может производить сорт меди, который не конкурирует с электролитической, но достаточно рафинирован для непосредственного использования потребителем.

ПЕРУ

Перу является одной из важных медедобывающих стран мира. Однако основные рудники расположены на экстремальных высотах, а их характер и местоположение указывают на то, что объем производства, вероятно, останется на прежнем уровне или, по крайней мере, не покажет значительного роста в ближайшие несколько лет. Существуют два важных района: Серро-де-Паско (высота 14 300 футов) и Морокоча (высота 13 700 футов).

Основные рудники этих районов в настоящее время контролируются американским капиталом и могут быть отнесены ко второй группе таблицы 38. Район Морокоча ранее контролировался англичанами, но контрольный пакет акций был недавно приобретен компанией Cerro de Pasco Copper Co. (американской). Руды в обоих районах чрезвычайно богаты, а объекты хорошо обеспечены запасами. Разведанных запасов достаточно для обеспечения четырех лет добычи, и все указывает на то, что на рудниках разрабатываются обширные и устойчивые месторождения руд. Черновая медь отправляется в компанию American Smelting & Refining Co. в Нью-Йорке для переработки и сбыта. Оба рудника имеют полностью оборудованные предприятия, включая плавильные заводы.

На заводе компании Backus & Johnson Co. в Морокоче перерабатывается некоторое количество давальческой руды и штейна с рудников, принадлежащих местным владельцам. Среди этих рудников — рудники Дж. Галливера, производящие 600 тонн штейна в год. Backus & Johnson также имеют плавильный завод и рудники в районе Касапалка. Синдикат Sayapullo (английский) разрабатывает рудник Sayapullo по опциону от перуанских владельцев. Часть этого штейна отправляется на плавильный завод в Касапалке, а остальная часть экспортируется в Соединенные Штаты. Объем добычи пока невелик; в настоящее время он составляет 800 тонн в год.

Некоторые небольшие компании отправляют руды в Соединенные Штаты: содержание меди в них составило около 4 000 000 фунтов в 1917 году. В 1919 году они поставлялись главным образом компаниям American Metal Co. и L. Vogelstein для рафинирования и продажи. Эта руда поступает из Салаверри и Трухильо (район Касапалка), Мольендо (южный район, включая Ферробамбу, см. ниже) и Кальяо. Вся черновая медь отправляется из Кальяо, за исключением небольших объемов, отправляемых компанией Backus & Johnson из района Касапалка. Американская компания разработала крупное тело низкосортной руды в Ферробамбе (провинция Котобамба), южное Перу. Объект труднодоступен, и в настоящее время работы там не ведутся.

Следующее резюме содержит некоторые важные факты, касающиеся перуанских производителей меди:

Таблица 44. — Производство меди в Перу в 1918 году

| Output | Developed Reserves | Product | Control
Cerro de Pasco | 72,000,000 | (-) | 4 years | Blister Copper | United States
Backus & Johnson | 28,000,000 | (-) | 4 years | Do | Do
Huaron (new) | 5,000,000 | (?) | 4 years | Do | French
Ore shippers | 5,000,000 |  | ? | Ore | Local
| 110,000,000 |  |  |  |

БОЛИВИЯ

В Боливии есть один важный медедобывающий район — Коро-Коро, центральная Боливия (высота 12 000 футов). Пласты песчаника содержат самородную медь и жилы сульфидов. Рудники принадлежат французскому капиталу. Плавильного завода нет, но концентраты с содержанием меди до 85 процентов экспортируются во Францию для переработки. Объем производства составляет около 12 000 000 фунтов в год. Запасы велики, но почти недоступное расположение рудников сдерживало развитие. В последнее время наблюдается большая активность, был установлен флотационный концентратор.

Некоторые боливийские оловянные и серебряные рудники производят небольшое количество меди, но за пределами Коро-Коро общее производство меди незначительно.

ВЕНЕСУЭЛА

Рудники Aroa, принадлежащие английскому синдикату, включают медный рудник и плавильный завод, производящий низкосортный штейн. Объект расположен вдоль железной дороги, которая заканчивается в порту Тукакас. В 1917 году объем производства составил 3 500 000 фунтов. Продукт был отправлен в Соединенные Штаты, где был рафинирован и продан компанией L. Vogelstein & Co.

АРГЕНТИНА

В самой западной части страны есть некоторые медные перспективы, которые на самом деле являются продолжением чилийских медедобывающих районов. Одна компания, Famatina, Ltd., является английским предприятием, у которого была неудачная история. Компания управляет единственным медным плавильным заводом в Аргентине — небольшим предприятием, которое ведет добычу нерегулярно. По последним данным, годовой объем производства составлял несколько сотен тонн черновой меди; она всегда отправлялась в Англию, но в последнее время предпринимались попытки отправки в Нью-Йорк. Эта черновая медь чрезвычайно богата серебром (6 процентов серебра).

АФРИКА

Африка является производителем меди растущего значения, почти полностью благодаря развитию одной группы месторождений (Катанга), которая настолько затмевает все остальные, что ситуация в Африке почти полностью описывается обсуждением активов компании Tanganyika Concessions, Ltd. Рудники этой компании дают сейчас три четверти производства меди в Африке, и их значение в будущем будет еще больше.

Производство меди в Африке осуществляется к югу от экватора и в шести основных районах, а именно:

Таблица 45. — Производство меди в Африке (Производство, фунты чистой меди)

District
Province and
chief mines
1917 output
1918-1919,
estimated output
Control
Reserves,
years of life
at this rate
of output

1. | Congo: Katanga[121] | 60,000,000 |  | 80,000,000 |  | English-Belgian | 100
| Bwan M’Kubwa | 4,000,000 | ? | 3,000,000 |  | English | large
2. | Transvaal: Messina | 14,000,000 |  | 12,000,000 |  | English | 1¹⁄₂
3. | Rhodesia: Falcon | 7,000,000 |  | 7,000,000 |  | English | 4
4. | Cape Colony: Cape Copper-Namaqua | 7,000,000 |  | 6,000,000 |  | English | 2
5. | Former German Southwest-Africa: Tsumeb (Otavi) | 10,000,000 | ?[122] | 15,000,000 | ? | (English since conquest of German Southwest Africa) | 4
| Khan, etc. | 2,000,000 |  | 4,000,000 | ? |  | 4
6. | Miscellaneous northern Africa not specified | 1,000,000 | ? | 1,000,000 | ? | French | ?
| Total | 105,000,000 |  | 128,000,000 |  | Almost entirely English |

[121] Каншанши включен в состав Катанги.

[122] База 1914 года. Нынешние политические условия определяют объем работ. В 1917 году в Соединенные Штаты было отправлено 1 000 000 фунтов меди в руде.

В районе 1, районе Катанга, который включает Бельгийское Конго и прилегающую территорию, компания Union Minière du Haut Katanga приобрела у Бельгийского специального комитета право собственности на весь медный пояс Катанги, но не на месторождение Каншанши в Родезии. Равные, но не полные доли участия в этой компании принадлежат Tanganyika Concessions, Ltd. и Катангийскому (бельгийскому) специальному комитету. Плавильный завод Lubumbashi компании U. M. du Haut Katanga в Элизабетвилле, недалеко от границы с Родезией, имеет семь доменных печей с суточной производительностью 2000 тонн. Перерабатываемая руда содержит 15 процентов меди и дает 96-процентную черновую медь. Прошлое производство выглядит следующим образом: 1911 г. — 996 тонн черновой меди; 1912 г. — 2492 тонны; 1913 г. — 7407 тонн; 1914 г. — 10 722 тонны; 1915 г. — 14 190 тонн; 1916 г. — 22 165 тонн; 1917 г. — 30 000 тонн. Эта медь отправляется в Англию и потребляется там и во Франции после дальнейшего рафинирования. В меди очень мало золота и серебра, поэтому она поступает на рынок в основном как рафинированная, высшего сорта и вязкая медь.

Tanganyika Concessions, Ltd. владеет концессиями в Северной Родезии, содержащими рудник Каншанши (месторождение, аналогичное месторождениям в Катанге), принадлежащий дочерней железнодорожной компании, 70 процентов которой принадлежит Tanganyika Concessions, Ltd. Там работает небольшая доменная печь. Фактическое железнодорожное сообщение с Катангой идет на север из Родезии, а оттуда к восточному побережью Африки. Планируется строительство незавершенной линии с западного побережья для соединения этих месторождений полезных ископаемых с заливом Лобито (Benguella Ry. Co.). Португальское правительство имеет небольшую долю в некоторых железнодорожных линиях на своей территории. По-видимому, английская группа (Р. Уильямс, который был партнером Сесила Родса, Т. Уайт и другие) вместе с Бельгийским специальным комитетом контролирует всю группу; но значительная доля была продана населению, в основном британским и бельгийским инвесторам.

Рудник Bwan M’Kubwa, расположенный дальше на юг на Родезийской железной дороге, представляет собой месторождение того же общего характера. Оно принадлежит британскому капиталу, причем две родезийские девелоперские компании владеют крупным пакетом акций.

Рудные тела встречаются в Катанге в районе, простирающемся на 250 миль с востока на запад и на 50 миль с севера на юг, а также в разрозненных местах в Родезии. Малахит, главным образом, и другие окисленные руды пропитывают определенные осадочные породы и образуют рудные тела, которые очень богаты (от 10 до 15 процентов меди). В Луушии сульфиды (3 процента меди в виде халькопирита) встречаются под окисленной рудой. Кобальт встречается часто; есть немного никеля, но мало золота и серебра. Разведанные запасы рудников Катанги оцениваются в 40 000 000 тонн руды с содержанием 8 процентов меди выше уровня грунтовых вод, что равно 100 годам добычи при нынешнем уровне производства; запасы рудника Bwan M’Kubwa в Родезии оцениваются в 3 000 000 тонн руды с содержанием 4 процентов меди, помимо руды более низкого качества. Запасы рудника Каншанши в Родезии в оценки не включены.

В районе 2, недалеко от границы с Родезией, находится рудник Мессина, единственный производитель меди в Трансваале. Вдоль жил в очень старых гнейсовых породах встречаются штокверки и линзы халькозина и энаргита с некоторым количеством оксида. На руднике производится немного штейна, но основной продукт — концентраты (от 45 до 50 процентов меди), все из которых отправлялись в Англию. В последнее время они частично отправляются в Соединенные Штаты. Объем производства составил около 14 000 000 фунтов в 1915 году и столько же в 1916 году. Сообщается о разведанных запасах в 208 000 тонн руды с содержанием 5 процентов меди, что составляет немногим более годового запаса. Компания является строго английской.

В районе 3 рудники Falcon в Центральной Родезии принадлежат английской компании, которая перерабатывает медно-золотую руду, встречающуюся в старых сланцах. Объем производства составил около 7 000 000 фунтов в 1916 году. Руда содержит 2 процента меди, 5 долларов золота, а запасы оцениваются в 862 000 тонн руды такого качества, или около четырех лет запаса.

Во Французском Конго, к северу от устья реки Конго, находится пояс медных месторождений длиной 60 миль, которые веками разрабатывались местными жителями. В этой местности встречаются диабазовые породы. Объем добычи очень мал.

Район 4, Капская колония, является старейшим важным производителем меди в современной Африке, но его основные месторождения, разрабатываемые с 1852 года, почти истощены. Компании Cape Copper Co. и Namaqua Copper Co. находятся к югу от реки Оранжевой в районе, расположенном в 90 милях по железной дороге от порта на западном побережье. Руда представляет собой борнит и халькопирит в нерегулярных линзах; запасы эквивалентны только двум годам добычи. Каждый рудник имеет обогатительную фабрику и плавильный завод. Дальнейшее рафинирование осуществляется на плавильном заводе Briton Ferry компании Cape Copper Co. в Уэльсе, который имеет мощность 12 000 тонн рафинированной и электролитической меди в год. Все эти компании, включая железную дорогу, являются полностью британскими. Производство меди в Капской колонии зависит от этого одного района, объем добычи в котором в 1917 году составил от 6 000 000 до 7 000 000 фунтов.

В районе 5, бывшей колонии Германская Юго-Западная Африка, медные месторождения многочисленны, и после добычи алмазов производство меди является важнейшей отраслью провинции. Основным месторождением является Цумеб в северо-восточной части страны, где в доломите встречаются массивные сульфиды свинца и меди. В 1917 году было отгружено пятьдесят тысяч тонн руды с содержанием 13 процентов меди и 40 процентов свинца. Здесь есть плавильный завод, и рудник имеет железнодорожное сообщение. Компанией, разрабатывающей эти месторождения, была Otavi Minen und Eisenbahn, но через компанию Southwest Africa Co. англичане имели долю в этом объекте. Сейчас англичане имеют контроль. Рудник Хан, второй по значимости после Цумеба, разрабатывает пегматитовую жилу в сланце. В 1914 году фабрика, перерабатывающая 50 тонн в день, отправляла в Европу 60–70-процентные концентраты. Руды представляют собой халькопирит и халькозин.

В районе 6, Северная Африка, есть некоторые месторождения меди в Алжире, Египте и Марокко. В настоящее время они не имеют значения. Де Лоне описывает их главным образом как жилы в породах гораздо более молодого возраста, чем важные месторождения Африки, расположенные к югу от экватора.

Штейн и черновая медь, производимые в Африке, обычно перерабатываются на небольших английских заводах или на плавильном заводе Briton Ferry в Уэльсе, который является предприятием значительного размера.

Общая экономическая ситуация в отношении африканских медных руд в 1917 году показана в таблице.

Таблица 46. — Производство и отгрузки меди из Африки в 1917 году

Mine | Production, (pounds) | Chief product shipped | Shipped to—
Katanga | 60,000,000 | matte and blister | England
Cape Copper-Namaqua | 7,000,000 | matte | England
Messina | 14,000,000 | concentrates, matte, hand-picked ore | England
Falcon | 7,000,000 | concentrates or ore | England
Bwan M’Kubwa | 4,000,000 |  | Katanga plants
German Southwest Africa, Otavi, Khan | 12,000,000 | ore | England or Germany
North Africa | 1,000,000 | ore | France
| 105,000,000 |  |

Значительная часть этой меди идет в Соединенные Штаты. В 1917 году, как показано ниже, общее количество меди, полученной в этой стране, составило 7,5 процента от общего объема производства в Африке.

Таблица 47. — Отгрузки в Соединенные Штаты в 1917 году

| Grade Shipped | Shipments (tons) | Copper content (pounds)
Otavi to New York | Ore (12 per cent.) | 3,900 | 1,048,000
Messina to New York | Ore (45 per cent.) |   703 |   715,000
Do | Matte (45 per cent.) |   306 |   310,000
Cape Copper to New York | Concentrates (55 per cent.) |   375 |   460,000
|  | 5,284 | 2,533,000
Katanga | Blister | ... | 5,437,000
Total |  |  | 8,000,000

АВСТРАЛАЗИЯ

Производство меди в Австралазии в настоящее время не растет. В последние годы производство (в метрических тоннах) было следующим:

1912 | 1913 | 1914 | 1915 | 1916 | 1917
16,600 | 22,900 | 37,592 | 32,512 | 35,000 | 38,100

Ранее немецкие компании по закупке и рафинированию металлов контролировали австралийскую добычу меди (как и свинца и цинка) благодаря контрактам на рафинирование и продажу. Поэтому 1914 год принес дезорганизацию в австралийскую горнодобывающую промышленность. Налогообложение военной прибыли на австралийских рудниках было суровым; а государственная помощь, предоставлявшаяся ранее, была в значительной степени отозвана. Нехватка рабочей силы, неспособность новых объектов получить железнодорожное сообщение и отсутствие государственной поддержки геологоразведки сдерживали медную промышленность с августа 1914 года. Помимо бывшего немецкого контроля, основанного на контрактах на продажу и рафинирование, вся австралийская добыча меди находится и находилась под британским контролем. Объекты принадлежат британскому и австралийскому капиталу, и нынешние соглашения о рафинировании и продаже не позволят немецким металлургическим компаниям снова закрепиться в этой области. Все прежние контракты с немецкими агентствами были аннулированы. Правительство взяло эту сторону дела в свои руки, и одним из шагов стала закупка всей продукции Австралии за первую половину 1918 года по цене от 106 до 108 фунтов стерлингов за тонну.

Ситуация с медью в Австралии в 1917 году представлена в следующей таблице:

Таблица 48. — Производство меди и рафинировочные заводы в Австралии в 1917 году

Chief mines | Production, 1917, (long tons) | Refineries
Queensland: |  |
Mount Morgan |  8,000 | [123] | Port Kembla plant, Electrolyte Refining & Smelting Co., Ltd.
Hampden Cloncurry |  8,000 | [123] | Capacity, 29,000 tons electrolyte copper per annum; 12,000 tons fire-refined copper per annum.
Other Cloncurry district mines |  4,000 | [123] | Mount Elliott completed refinery at Bowen, Queensland, in 1917; capacity 10,000 tons refined copper.
South Australia: |  |
Wallaroo & Moonta |  7,000 |  | Wallaroo & Moonta smelter, Bowen, Queensland; capacity increased from 7,000 to 10,000 tons per annum.
Tasmania: |  |
Mount Lyell |  5,000 |  | Ships to Port Kembla.
New South Wales: |  |
Great Cobar |  2,500 | [123] |
C. S. A. and Mt. Hope, etc. |  2,250 |  |
West Australia and Papua: |  |
New pyrite ore bodies of promise opened |  1,250 |  |
| 38,000 |  |

[123] Добываемые руды являются первичными, состоящими из халькопирита и халькозина. Вторично обогащенные руды вблизи поверхности были полностью выработаны.

Как уже говорилось, собственность на эти рудники является строго британской, и в настоящее время рафинирование и маркетинг являются британскими, а не немецкими. Два рафинировочных завода, оба недавно расширенные и улучшенные, теперь имеют мощность более 60 000 тонн в год, что значительно превышает текущий объем производства в стране. К концу 1917 года в Австралии была создана ассоциация Copper Producers’ Association Proprietary, Ltd. с целью продажи и отгрузки меди на кооперативной основе. Все производители меди были приглашены присоединиться. Wallaroo & Moonta, Mount Morgan, Mount Lyell и рудники Cloncurry являются членами этой ассоциации, как и компания Electrolytic Refining & Smelting Co., которая перерабатывает руды этих рудников. Компания продает свою продукцию в Англии и Австралии. Ее основные бренды — E. S. A. (электролитическая) и E. S. A. F. R. (огневого рафинирования). Эти бренды также продаются компанией Elder Smith & Co., Ltd. из Лондона и Австралии, которая имела финансовый интерес в компании Wallaroo & Moonta Co. с первых дней ее существования, а с 1915 года финансировала и продавала медную продукцию этой компании.

Недавно была создана компания Metals Products, Ltd. с заводами в Порт-Кембла, производящими медную проволоку, латунные изделия и т. д. Импорт медных и латунных изделий в Австралию должен полностью исчезнуть, если планы австралийского правительства и производителей меди не потерпят неудачу.

Старейшим рудником и одним из двух ведущих рудников в Австралазии является Wallaroo & Moonta в Южной Австралии. Это месторождение находится в докембрийском комплексе, пересеченном пегматитовыми дайками. Считается, что запасы руды достаточны: скажем, на пять лет работы при разведанной руде. В последние годы производство было очень стабильным — около 7000 тонн рафинированной меди в год. Это единственное важное медное месторождение докембрийского возраста в Австралии.

Другим ведущим рудником в Австралии является Mount Morgan в Квинсленде, который до 1910 года был одним из крупнейших золотых рудников в мире. Золото находилось в окисленной верхней части крупного низкосортного медного месторождения, которое сейчас разрабатывается открытым способом. Первичный халькозин, халькопирит и пирит с кварцем составляют рудное месторождение. Руда содержит 2,5 процента меди и концентрируется до 7 процентов. Запасы превышают 4 000 000 тонн руды с содержанием 2,5 процента меди, или 10 лет запаса.

Район Клонкерри — это обширная территория площадью 200 на 40 миль, содержащая несколько медных месторождений, которые встречаются в сланцах и представляют собой в основном небольшие богатые залежи. Будущее этого района кажется очень многообещающим. Основными рудниками являются Hampden Cloncurry, Mount Elliott, Mount Cuthbert; разведанные запасы руды обеспечивают пять лет добычи. Рудник Hampden Cloncurry имеет в запасе 300 000 тонн руды с содержанием 7 процентов меди, плавильный завод, производящий черновую медь, и железнодорожное сообщение. Район страдает от плохого климата и т. д., и особенно от условий труда. Недавние правительственные постановления (1918 г.) относительно очень короткого рабочего дня и более высокой заработной платы снижают объемы производства. Рудник Mount Elliott, имеющий месторождение в 300 000 тонн руды с содержанием 10 процентов меди, сейчас (1919 г.) простаивает из-за условий труда. Рудник Mount Cuthbert, завершивший строительство нового плавильного завода в 1917 году, имеет запасы в 150 000 тонн руды с содержанием 6,5 процента меди и железнодорожное сообщение.

Рудник Mount Lyell в Тасмании является старым и стабильным производителем. Один сорт руды содержит 0,5 процента меди и 1,25 унции серебра; другой содержит 6 процентов медной руды с таким же количеством серебра. Это вкрапленное месторождение в сланцах, недалеко от контакта с конгломератом. Магматические породы в окрестностях неизвестны. Запасы составляют 2 000 000 тонн низкосортной руды и 1 000 000 тонн высокосортной, что обеспечивает текущий объем производства на 15 лет. Значительная часть руды добывается открытым способом, и это один из самых низкосортных прибыльных рудников в мире. Руды плавят напрямую после смешивания, так что продукт, поступающий в печь, содержит 2,5 процента меди.

Рудник Great Cobar в Новом Южном Уэльсе разрабатывает медьсодержащий пирит с содержанием 2–2,5 процента меди. Cobar раньше производил от 4000 до 5000 тонн меди в год. После постройки плавильного завода мощностью 1200 тонн в 1912 году компания была передана под внешнее управление в апреле 1914 года. Считается, что запасы велики. Другие основные рудники в Новом Южном Уэльсе (C. S. A., Mount Hope, Nymagee и др.) производят вместе примерно столько же, сколько Great Cobar. Эти рудники имеют плавильные заводы и по большей части раньше имели гораздо большее значение, чем сегодня. Некоторые из них не имеют железнодорожного сообщения, и это является важным препятствием для рудников Нового Южного Уэльса, которые когда-то производили вдвое больше нынешнего объема.

В Западной Австралии недавно было разведано несколько многообещающих месторождений пиритных медных руд. Важных производителей нет, так как нет железных дорог.

Нынешние условия в Австралии, в которых наиболее важными являются условия труда, и отсутствие нового железнодорожного строительства серьезно повлияли на развитие медной промышленности, но будущее кажется многообещающим. Несколько важных месторождений оказались крупными, а рудные тела — устойчивыми. Большая часть страны не исследована, и многие хорошие проявления могли бы разрабатываться, а некоторые, вероятно, превратиться в прибыльные рудники, если бы условия были благоприятными для новых предприятий. Однако дело обстоит как раз наоборот. Компания Mount Lyell проводила разведку в северной Тасмании и недавно обнаружила на руднике Tasmania Copper Co. около 1 000 000 тонн руды, содержащей медь, цинк, золото и серебро, стоимостью от 20 до 30 долларов за тонну в валовом выражении.

Считается, что Австралия останется важным производителем меди; вероятно, ее значение будет расти. Взвешенные запасы, в пересчете на обеспечение рудой для поддержания текущего уровня производства, гарантируют, что добыча меди будет продолжаться без уменьшения в течение 7,2 лет. Эти запасы хорошо распределены между различными производителями.

АЗИЯ

ЯПОНИЯ

Медные месторождения встречаются на большой части центральной Японии. Руды, которые встречаются в третичных вулканических породах, состоят из халькопирита и пирита с содержанием 2,5–3,5 процента меди и обычно концентрируются перед плавкой. Пустая порода обычно кварцевая. Линзовидные месторождения медьсодержащего пирита в палеозойских сланцах и осадочных породах встречаются на западе и юге Японии. Эти рудники дают плавильную руду с содержанием около 3,5–4 процентов, но содержат очень мало кремнезема. Широко практикуется пиритная плавка. Более половины производства меди приходится на четыре основных рудника: Асио и Косака третичного типа; и Хитати и Беси палеозойского сланцевого типа.

Государство оставляет за собой право первоначальной собственности на все руды, включая медь. Право на их разработку предоставляется физическим или юридическим лицам японской национальности. Компании по добыче, плавке и рафинированию меди, по-видимому, полностью принадлежат японцам и следуют японской политике. Количество рудников значительно, но их собственность сосредоточена в немногих руках, а плавильная и рафинировочная промышленность еще более сконцентрирована. Японские производители продают свою медь сами, все иностранные торговые агентства являются строго японскими. Рудники в Японии, как правило, не работают как акционерные предприятия, а в основном являются семейной собственностью, унаследованной нынешними владельцами. Таблица, показывающая производство меди в Японии в 1917 году, указывает на эти факты. (См. таблицу 49.)

Благодаря условиям труда, обилию топлива рядом с рудниками и водному транспорту производство меди в Японии в последние годы быстро росло. Высокие цены и внедрение современных методов добычи и плавки были важными способствующими факторами. Нет причин ожидать, что производство в Японии сократится, но о геологических условиях известно недостаточно, чтобы можно было обсуждать перспективы на будущее. Единственный рудник, запасы которого известны, — это Беси, который имеет запасы, достаточные для 100 лет добычи при нынешнем уровне, что составляет 10 процентов от японского производства. Запасы на других рудниках не разведаны далеко вперед, но должны обеспечить несколько лет непрерывной добычи при нынешнем уровне.

Производство и экспорт японской меди в последние годы выглядят следующим образом (в метрических тоннах):

Year | 1912 | 1913 | 1914 | 1915 | 1916 | 1917
Production |  63,893 |  67,697 |  71,046 |  76,039 | 101,467 | 124,306
Exports |  30,000 |  42,000 |  45,500 |  59,500 |  62,000 |  72,000

Таблица 49. — Производство меди в Японии. Компании-производители и бренды продаваемой меди. Названные компании имеют торговые представительства в Лондоне и других зарубежных центрах потребления.

Company and chief mines owned | Smelters | Electrolytic refineries
Location | 1917 production (pounds) of refined and casting[124] and brands sold | Location | 1917 estimated capacity (pounds) and brands sold
Mitsu Bishi & Co. | Osaka | 15,000,000 | Osaka | 15,000,000
Osaruzawa |  |  |  |
Arakawa |  |  |  |
Ikuni and 6 smaller mines |  |  |  |
Brands sold |  | Arakawa, Mitsui Bishi, casting, etc. (rough copper) |  | M. B. (Mitsu Bishi)
Furukawa & Co. | Osaka (Amagasaki) | 17,000,000 | Osaka (Nikko Plant) | 67,000,000
Ashio |  |  |  |
also Ani, Furukura, Kune and 6 smaller mines |  |  |  |
Brands sold |  | Furukawa, Ani Tiles, refined Maragata Best Selected |  | F. M. (Furukawa Mines)
Fujita & Co. | Inushimo | 3,000,000 | Mosaka | 20,000,000
Kosaka (North end Honshu) |  |  |  |
Brands sold |  | Obiye casting, etc. (rough copper) |  | Kosaka
Kuhara Mining Co. |  | None | Hitach | 100,000,000
Hitachi (near Tokio) |  |  |  | Reported capacity at least 20% in excess of 1917 output.
3 smaller mines 30 per cent. custom ore |  |  |  |
Brands sold |  |  |  | H. M. (Hiatachi Mine)
Baron Sumitomo | Shikoku Island | 22,000,000 |  |
Beshi |  | Beshi Best Selected |  |
Brands sold |  |  |  |
Nippon Metals Co. of Kobe | Moji |  |  | 19,000,000
Brands sold |  | S. Z. K. (Susuki) and some casting |  |
Denkibundo Co. |  |  | Bundo | 13,000,000
Total casting rough copper and best selected sold |  | 57,000,000 |  |
Total electrolytic refining capacity[125] |  |  |  | 235,000,000
1917 output of electrolytic estimated |  | 217,000,000 |  |
Total |  | 214,000,000 or 124,306 metric tons Eng. & Mining Journal figure 1917 output. |  |

[124] Остаток плавится до катодов и подвергается электролитической обработке.

[125] Мощность завода. Очевидно, не достигнута в 1917 году.

После высоких цен на медь в 1916 году в Японию начался массовый ввоз китайских медных монет. В 1917 году одна компания заключила контракт на 200 000 тонн таких монет, которые содержат около 85 процентов меди, и уровень импорта в то время означал бы 60 000 тонн рафинированной меди в год из этого вторичного источника. Это развитие событий позволило Японии осуществлять значительный экспорт меди.

Крах России лишил Японию одного из ее крупных рынков сбыта меди. Япония, вероятно, не сможет выгодно производить большой экспортный излишек меди, если полученная цена не будет достаточно высокой по сравнению с котировками, действовавшими в 1912–1914 годах. В нормальных условиях Япония будет обеспечивать свои собственные потребности в меди, имея мало или ничего для продажи.

КОРЕЯ (ЧОСОН)

Компания Seoul Mining Co. (Коллбран и Боствик) ведет добычу на контактных месторождениях, одно из которых находится в 50 милях, а другое — в 100 милях от гавани. Это американское предприятие является доминирующим торговым и банковским домом в Корее и разрабатывает рудники, ранее эксплуатировавшиеся корейцами. Медные руды представляют собой сульфиды между известняком и гранитом. В 1917 году из Чосона в Соединенные Штаты было отправлено пятьсот тонн 60-процентных концентратов.

КИТАЙ

Текущий объем производства в Китае составляет 2000 тонн в год, а основные месторождения находятся в провинции Юньнань. Сообщается, что медные руды встречаются во многих местах, в основном это медьсодержащий пирит в очень старых сланцах или в пермском базальте. Последние месторождения слишком малы для современных методов. За последние сто лет нехватка древесины для производства древесного угля ограничила объем производства номинальным количеством. Небольшие жилы самородной меди высоко ценятся местными жителями. Руды тщательно отбираются вручную, а методы мелкого масштаба являются расточительными.

Рудник Tungschuanfu в Юньнани, главный рудник в Китае, имеет годовой объем производства около 1000 тонн меди. Район разрабатывался сотни лет и, вероятно, очень богат. Руды, представляющие собой замещения в известняке и жилы в сланце, содержат 8 процентов меди, а запасы велики. Правительственный плавильный завод Yaoki Kansu — это современное предприятие с производительностью четыре тонны меди в день.

Существует несколько других рудников, все они контролируются правительством. Сторонние инженеры дали положительные отзывы о некоторых из них, но правительство жестко регулирует добычу меди в Китае, поскольку это влияет на валюту и правительственную прибыль от чеканки медной монеты. Существуют также некоторые медные рудники, разрабатываемые вместе с контактными железными месторождениями Китая (образованными контактным воздействием диорита); а месторождения малахита в триасовом песчанике разрабатываются в нескольких точках.

ИНДИЯ

Индия не является производителем меди. Рудник Rakha Hills компании Cape Copper Co. (см. Капская колония) имеет разведанные запасы в 400 000 тонн руды с содержанием 4 процента меди, и строится плавильный завод. Индия является огромным потребителем меди, и удивительно, что она никогда не была производителем.

ЕВРОПА

Политический и коммерческий контроль над значительной частью производства меди в Европе, очевидно, крайне неопределен, как и любые цифры производства для Центральных держав и России. (См. таблицу 49.)

ИСПАНИЯ, ПОРТУГАЛИЯ, НОРВЕГИЯ И ШВЕЦИЯ

Испания является старейшим и самым стабильным производителем меди в мире. Основные месторождения контролируются английским капиталом, а их разведанные запасы обеспечивают текущее производство на 30–60 лет. Медь в значительной степени рафинируется до готового вида в Англии и поступает на рынок под различными брендами. Rio Tinto — это огромное месторождение, разрабатываемое открытыми карьерами.

Таблица 50. — Производство и контроль меди в Европе

Country and chief localities in which copper is produced
Output
1916-1917
(metric tons)
Estimated
output
1918-1919
(metric tons)
Estimated
output
1918-1919
(pounds)
Control by:
Reserves
of ore
Remarks

Financial[126] | Political | Handling of sales
Germany |  |  |  |  |  |  |  |
Mansfeld | 30,000 | 30,000 |  | ... |  | Now entirely German |  |  | Output in future should not be nearly as large.
Mitterberg, etc. | 10,000 | 10,000 |  | ... |  | Do |  |  |
Austria-Hungary | 10,000 | 10,000 |  | ... |  | Do |  |  |
Serbia, Bor, etc. | 10,000 | 10,000 |  | ... |  | Do |  |  |
Turkey, Aghano, etc. | 10,000 | 10,000 |  | ... |  | Do |  |  |
Bulgaria and Roumania | 1,000 | 1,000 |  | ... |  | Do |  |  |
Total Central Powers (est.) | 71,000 | 71,000 |  | ... |  |  |  |  |
Spain and Portugal[127] | 42,000 | 42,000 |  | ... |  |  |  |  | No statistics since 1914.
Mason & Barry | ... | ... | 5,000,000 | English | Portuguese | English | 32 years’ supply |
Rio Tinto | ... | ... | 62,000,000 | Do | Spanish | Do | Very large | 60 years’ reserves known.
Tharsis | ... | ... | 12,000,000 | Do | Do | Do | Do |
Misc. (United Alkali, Huelva, Cordoba, etc.) | ... | ... | 11,000,000 | Do | Do | Do | Do |
Miscellaneous (Calva, Los Guardos, etc.) | ... | ... | 3,000,000 | Spanish | Do | Do | Do |
Russia (See Table 52) | 18,500 | 18,000 | ? | ... | ? | ? | ? |  | 1914 output 36,340 tons.
Norway[128] (Sulitolma 40 per cent.) | 19,000 | 19,000 |  | ... | ¹⁄₂ English and ¹⁄₂ Norwegian | Norwegian |  | Important | Like Spanish deposits.
Sweden | 1,000 | 1,000 |  | ... | Swedish | Swedish | Swedish |  |
Other countries |  |  |  |  |  |  |  |
Italy | 3,000 | 3,000 |  | ... | Italian | Italian | Italian |  | Some English capital.
France | 1,000 | 1,000 |  | ... | French | French | French |  | French pyrite mines.
England | 250 | 250 |  | ... | English | English | English |  | Tin mines.

[126] Все компании имеют иностранных акционеров, но доминирующая национальность указана.

[127] Экспорт меди во Францию и Англию в виде черновой меди, сплавов, цементной меди, пиритной руды и медной руды.

[128] Экспорт меди в Англию и Швецию, главным образом в виде медьсодержащего пирита.

Примечание. Производство в Германии в 1919 году, вероятно, меньше оценки.

Медные месторождения, главным образом массивные медьсодержащие пириты, в Норвегии и Швеции аналогичны месторождениям Испании как в геологическом, так и в экономическом отношении. Их коммерческая ценность зависит не только от содержания меди, но и от извлекаемых серы и железа. Во многих случаях сера, используемая в производстве серной кислоты, имеет большую денежную ценность, чем извлекаемая медь. Поэтому экспортируемая медь из Испании, Португалии и Норвегии представлена в нескольких формах: пирит, штейн, слитковая медь из Норвегии и значительное количество цементной меди или осадков из Испании и Португалии. Пирит экспортируется в Англию, Соединенные Штаты и, возможно, немного во Францию; штейн, слитки и т. д. — в различные европейские страны. Швеция импортирует, а также производит пирит. Франция, Италия и Россия производят значительное количество пирита, а до войны Франция экспортировала пирит. В нормальных условиях медь во всем этом пирите перемещается туда и обратно по Европе, и ее трудно отследить. Таблица показывает местонахождение сырьевых ресурсов, но не место производства товарной меди. Основной импорт и экспорт пирита обычно выглядят следующим образом:

Таблица 51. — Нормальный экспорт и импорт пирита для некоторых европейских стран

Exports from— | Amount (tons) | Imports to— | Amount (tons)
Spain | 1,500,000 | England | 1,050,000
Norway | 500,000 | Sweden | 100,000
Portugal | 250,000 | United States | 1,000,000
| ... | France | 100,000
Estimated total | 2,250,000 |  | 2,250,000

ГЕРМАНИЯ

В существующих условиях текущий объем производства в Германии не может быть точно оценен. Цифры в таблице 49 являются предположениями, основанными на имеющейся информации. Месторождения Мансфельда, безусловно, являются наиболее важными, и, поскольку они находятся в сланцах, которые простираются на большой площади, запасы следует считать большими. Рудник Mitterberg, принадлежащий Круппам, имел довоенный объем производства всего 1000 тонн в год. Несколько медных месторождений в австрийском Тироле имели довоенный объем производства 1000 тонн в год.

Однако основным источником меди в Германии во время войны, должно быть, была переработка изделий, содержащих медь, которые использовались до войны. Сомнительно, чтобы 10 процентов годового производства меди в мирное время было уничтожено в процессе использования. Следовательно, во всех странах обычно существует большой запас меди в виде проволоки, латуни, деталей машин и т. д. Это то, что Германия использовала во время войны, и ее замена необходима для ее промышленного успеха в мирное время.

РОССИЯ

Производство меди в России быстро росло до войны и достигло максимума в 1913 году. Собственность на рудники и рафинировочные заводы была в значительной степени английской, но частично французской. Было проведено достаточно разработок, чтобы указать на то, что Россия, вероятно, станет крупным производителем меди, когда станет возможен последовательный промышленный прогресс. В 1918 году рудники были захвачены рабочими, и операции были почти или полностью приостановлены. Медные районы находятся на Урале, Кавказе или в Сибири. Производство меди в России (в длинных тоннах) было следующим:

1905 | 1910 | 1913 | 1914 | 1915 | 1916 | 1917
8,700 | 22,310 | 33,794 | 31,435 | 25,472 | 20,557 | 15,700
| (34,911) |  | (27,295) |

Таблица 52. — Производство меди и запасы руды в России (Все цифры в длинных тоннах)

District | Company | Original investments made by: | 1913 production | 1915 production, (estimated) | Ore reserves (developed) | Copper in ore reserves (per cent.) | Remarks
Urals | Kyshtim | British |  7,000 |  7,600 | 3,150,000 | 2.75 | Obtains gold as by-product.
Do | Bogoslovsk | Do |  4,300 |  4,100 | ... | ... | Ore hard to follow; excellent possibilities.
Do | Sissert | Do |  1,100 |  1,500 | 5,000,000 | (2³⁄₄)-4 |
Do | Tanalyk | Do |   600 |   600 |  ⁫126,000 | ... | Developing into a gold rather than a copper deposit.
Do | Verch-Isselz | Russian |  3,000 |  2,500 | large reserves | 2-3 | Massive pyrite ore.
Do | Nishni Tagilsh (Demidov) | Do |  2,000 |  1,500 |  |  |
Urals total |  |  | 18,000 | 17,800 |  |  |
Caucasus | Caucasus Copper Co. | British |  5,500 |  3,000 | 3,600,000 | 3 | Mines at Khot Eli and Katar.
Do | Allah Verde | French |  2,000 |    700 | ... | ... | Industrial & Metallurgical Co. of Caucasus.
Do | Siemens Co. | Russian |  1,500 |    800 | ... | ... | Mines at Tcherek and Kedabeck.
Caucasus total |  |  |  9,000 |  4,500 |  |  |
Siberia | Spassky | British |  4,756 |  3,450 |  ⁫543,000 | 10.7 |
Do | Miscellaneous | Do |  |    734 | ... | ... | Development companies, see below.
Do | Irkysh (Ridder) | Do | (New) | ... | 2,300,000 | 5 | 1,000,000 low-grade ore also in reserves.
Do | Russian Mining Co. | Do |    410 | ... |  ⁫500,000 | 2.6 | Ore carries other metals.
Do | Alexeieff Co. | Do |    377 | ... |  |  |
Do | Russo-Asiatic Corporation | Do |  |  |  |  |
Siberia total |  |  |  5,553 |  4,184 |  |  |
Russian chemical works |  |  |  1,358 |    811 |  |  | Ouchkoff, Kreiners, etc.
Grand total Russia |  |  | 34,911 | 27,295 |  |  |

Russian reserves insure maintenance
of 1913 maximum output for at least 15 years

Copper refineries
Capacity
per year.

Electrolytic
Kyshtim
10,000

Electrolytic
Bogoslov
6,000

Best selected (refined)
Caucasus Copper Co.
10,000

Total
26,000

Россия всегда в значительной степени зависела от иностранной меди, и существовала тарифная премия на внутреннее производство. Вполне вероятно, что в конечном итоге Россия сможет в большей степени обеспечивать себя медью, даже если потребление значительно возрастет. Таблица 52 показывает важные разведанные объекты, их производство в 1913 году (максимум) и в 1915 году (оценка), их разведанные запасы руды и национальность первоначального капитала, который сделал возможными эти разработки.

РЕЗЮМЕ

Медь, красный металл, превосходит только золото и серебро по ковкости и только серебро по электропроводности. После железа это промышленно самый важный из всех металлов, так как его стоимость за фунт намного выше, чем у свинца или цинка, а мир требует и потребляет гораздо большие количества меди, свинца и цинка, чем любых других цветных металлов.

Применений меди много, но электротехническая промышленность является крупнейшим потребителем. Латунь, бронза и другие медные сплавы занимают второе место по важности. Значительное количество медных листов, труб и других изделий используется вне электротехнической промышленности. Медь используется в чеканке монет, а в Китае она является денежным стандартом для рабочего населения.

Соединенные Штаты, производящие основную часть мировой меди, также несут ответственность за финансирование и развитие более успешных медных рудников за рубежом, чем любая другая страна. Успеху способствовало наличие в Западном полушарии основных мировых медных месторождений, а также достижения в области добычи, обогащения и металлургии, которые в значительной степени были работой инженеров Соединенных Штатов. Англия и Япония контролируют значительное производство меди, но оно мало по сравнению с тем, что контролируется Соединенными Штатами.

В потреблении меди Германия является крупным фактором. Из-за этого факта немецкие интересы и международные металлургические дома в прошлом обеспечили значительный контроль над поставками меди через контракты на рафинирование и продажу с горнодобывающими компаниями. Такой контроль основан исключительно на компаниях по рафинированию и продаже и не распространяется на владение добывающими рудниками, а лишь в небольшой степени — на владение плавильными заводами.

Чили, Мексика, Канада и Бельгийское Конго должны стать все более важными производителями меди не только из-за известных запасов, но, в случае Канады и Мексики в частности, из-за вероятности новых и важных открытий. Позиция Соединенных Штатов, включая Аляску, должна поддерживаться на нынешнем уровне, не приобретая и не теряя по сравнению с остальным миром.

ГЛАВА XV СВИНЕЦ Фредерик Б. Хайдер

ПРИМЕНЕНИЕ СВИНЦА

Свинец используется в виде металла, сплавов с другими металлами и различных химических соединений. Как металл, его основное применение — трубы для воды и коррозионных растворов; защитное покрытие электрических кабелей; листовой свинец для футеровки камер для производства серной кислоты и чанов для химических производственных процессов. При плавке свинец используется как коллектор других металлов, особенно золота и серебра, от которых он позже отделяется, в настоящее время чаще всего с использованием цинка по процессу Паркса для обессеребрения.

Свинец легко образует сплавы почти со всеми другими металлами во всех пропорциях. Его сплавы, имеющие промышленное значение, включают типографский сплав, подшипниковые или баббитовые металлы, дробь, припои, литейные металлы, некоторые латуни и легкоплавкие сплавы, используемые для защиты электрических аппаратов и в автоматических спринклерах для защиты зданий от пожара. Типографский сплав, первоначально состоявший из 83 процентов свинца и 17 процентов сурьмы, теперь часто содержит висмут, а иногда немного меди и железа. Сплав из 9 частей свинца, 2 частей сурьмы и 2 частей висмута используется для стереотипных пластин. Менее 2 процентов мышьяка добавляется к свинцу, используемому для изготовления дроби, чтобы увеличить твердость и сферичность продукта. Сурьма также придает твердость, необходимую для шрапнели и т. д. Подшипниковые металлы включают сплавы свинца и сурьмы или их сплавы с медью, оловом и цинком. Сурьма придает свинцу свойство расширения при затвердевании, необходимое для типографского сплава и литейных материалов в целом. Свинец делает латунь мягкой и легко поддающейся механической обработке. Припой обычно представляет собой сплав свинца и олова. Температура плавления варьируется в зависимости от пропорций этих компонентов и других, иногда добавляемых для специальных целей. Самый дешевый припой, находящийся в общем пользовании, состоит из 30 процентов олова и 70 процентов свинца. Припои редко содержат более 50 процентов олова. Добавление висмута, кадмия или ртути снижает температуру плавления ниже температуры кипения воды. Таким образом, можно получить предохранители, которые размыкают электрические цепи при любой желаемой температуре.

Крупнейшее применение соединений свинца — в качестве пигментов. Свинцовые белила или основной карбонат, 2(PbCO3)Pb(OH)2, потребляются наиболее широко, используются отдельно или в смеси с оксидом цинка и баритом. Свинцовый сурик (Pb3O4) используется для окраски стальных конструкций, в качестве цемента для трубных соединений и в производстве стекла. Глет, другой оксид, используется при анализе в качестве флюса, в производстве резины и при изготовлении стекла. Ацетат, карбонат и другие химические соединения используются в медицине.

Относительные количества свинца, потребленного в различных целях в 1913 году, были следующими: в пигментах, включая свинцовые белила, свинцовый сурик, глет и оранжевый минерал, — 38,0 процента; в сплавах, таких как типографский сплав, подшипниковые металлы и припои, — 29,7 процента; в трубах — 15,2 процента; в дроби — 10,4 процента; и в листах — 6,7 процента.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Самым революционным достижением в обогащении руд за последние годы стало развитие процессов масляной флотации, электромагнитной и электростатической сепарации для концентрации свинцово-цинковых руд. Эти процессы позволяют устранить нежелательное содержание цинка во многих рудах и делают его дополнительным важным фактором при эксплуатации низкосортных комплексных руд.

Процесс Murex, применяемый к переработке комплексных руд, состоит в покрытии металлических сульфидных минералов маслом и частицами магнетита и пирита, прокаленными до магнитного сульфида, а затем отделении их от пустой породы с помощью электромагнитной машины. Селективная флотация галенита по методу Листера зависит от присутствия различных солей в используемой воде. На рудниках Брокен-Хилл эти соли присутствуют в шахтных водах. После удаления галенита сфалерит может быть селективно флотирован с помощью медной соли Брэдфорда, гипосульфита Брэдфорда или процессов с сернистой кислотой.

В восстановлении свинцовых руд постоянно происходят улучшения. Они касаются главным образом механических приспособлений, таких как механические рудные поды и непрерывное обжиговое оборудование, например, Dwight-Lloyd, а также деталей конструкции печей и обращения с материалами, а не процессов или признанных принципов. Были предложены различные новые процессы, большинство из которых предназначены для того, чтобы сделать доступными руды, которые сейчас слишком низкосортны, или комплексные руды свинца и цинка, разделение которых затруднено или коммерчески невыполнимо. Эти процессы сейчас являются предметом экспериментов, с некоторыми признаками того, что могут быть найдены успешные применения. Один процесс включает улетучивание путем хлорирующего обжига сульфидных руд, осаждение дыма хлорида свинца с помощью электрического осаждения Коттрелла и плавку дыма с известью. По меньшей мере 50 процентов хлора извлекается в виде хлорида кальция, который может быть заменен солью в дальнейших операциях. При работе с окисленными рудами предлагается растворять свинец с помощью рассола, подкисленного серной кислотой, и осаждать металлическую губку путем электролиза.

Процесс Гиллиса состоит в обжиге комплексных сульфидов до низкого содержания серы, смешивании с углеродистым веществом, дистилляции в избытке воздуха и улетучивании свинца, цинка, висмута, кадмия, мышьяка и т. д. в виде оксидов и сульфатов, причем свинец — в форме сульфата, а цинк — главным образом в виде оксида. Дым улавливается и переваривается раствором ZnSO4 и свободной H2SO4 из электролитических ванн; остается PbSO4, который можно использовать в качестве пигмента или плавить. Раствор ZnSO4 подвергается электролизу в присутствии гуммиарабика в электролите, что делает цинковый осадок более плотным.

Процесс Ганлина, признанный успешным для бирманских цинково-свинцовых промпродуктов, состоит в подаче сухой измельченной руды в расплавленную ванну из Zn и NaCl в равных частях. Цинк замещает свинец и серебро, которые растворяются в виде хлоридов, при этом осаждается ZnS. Когда эта реакция завершается, свинец и серебро осаждаются в виде металлов путем добавления гранулированного спельтера в количестве 35 процентов от их веса, при этом растворенный спельтер образует ZnCl2. Свинец, содержащий серебро, сливается, остаток гранулируется, соли выщелачиваются водой, а цинксодержащая пустая порода освобождается от свинцовой дроби путем стольной сепарации, оставляя цинковую руду, свободную от свинца.

Электролитическое рафинирование стало одним из величайших достижений в отрасли; оно делает возможным получение чистого свинца из любого источника и извлечение многочисленных побочных металлов.

ГЕОЛОГИЧЕСКОЕ ЗАЛЕГАНИЕ

Цинк и свинец обычно ассоциируются в месторождениях полезных ископаемых, иногда тесно перемешаны, иногда достаточно разделены, так что преобладает один металл, но редко бывают полностью свободны друг от друга. Геологическое и географическое распределение этих двух металлов, следовательно, почти идентично. Галенит является наиболее распространенным и важным из свинцовых минералов. Церуссит, англезит и пироморфит обычно являются результатом окисления галенита, причем сульфат обычно является промежуточным состоянием при окислении до карбоната. Пироморфит и вульфенит имеют второстепенное значение. Джеймсонит — это скорее руда сурьмы, чем свинца. Сфалерит (цинковая обманка) выветривается легче, чем галенит, и поэтому цинк во многих местах переносится ниже уровня грунтовых вод быстрее и полнее, чем свинец. По этой причине некоторые рудники с увеличением глубины превращаются из преимущественно свинцовых в цинковые. Помимо эффекта такого вторичного обогащения, это изменение часто встречается в первичных рудах с увеличением глубины.

Свинцовые руды встречаются в месторождениях нескольких различных генетических типов. Многие месторождения залегают на небольшой глубине в осадочных породах, без видимой связи с магматическими породами, встречаясь в виде пластовых замещений восприимчивых слоев. В регионах со слегка нарушенными пластами рудные тела имеют тенденцию следовать за наклонными впадинами. Руды этого типа обычно содержат минералы свинца (галенит), цинка (сфалерит) и железа (пирит); многие содержат марганец и кадмий; некоторые содержат кобальт и никель; но немногие несут золото, серебро, медь или сурьму. Месторождения этого типа имеют всемирное распространение, и многие из них обширны и коммерчески важны. Большая чистота руды и простота обработки (особенно для руд в зонах окисления) привели к тому, что они были эксплуатированы первыми и наиболее широко, и доминировали в мировом производстве свинца. К этому типу относятся, наряду со многими другими, месторождения долины Миссисипи и Силезии, которые вместе дали 15 процентов мирового производства в 1913 году.

Другие важные месторождения тесно связаны с изверженными породами и характеризуются комплексными рудами. Они включают жильные месторождения, вкрапленные залежи в изверженных породах и серебряно-свинцовые замещения в известняках.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Основные месторождения свинцовых руд в мире расположены в странах, перечисленных ниже в порядке их значимости в 1913 году.

Извлекаемое содержание свинца в свинцовых рудах, добытых в мире в 1913 году [129]

Rank | Country | Short tons | Metric tons | Percentage of world’s total production
 1. | United States | 484,880 | 440,000 |  36.0
 2. | Australia | 267,169 | 242,440 |  19.8
 3. | Spain | 209,193 | 189,830 |  16.4
 4. | Germany | 79,344 | 72,000 |   5.9
 5. | Mexico | 68,343 | 62,000 |   5.1
 6. | Tunis | 31,076 | 28,200 |   2.3
 7. | Italy | 24,905 | 22,600 |   1.8
 8. | Canada | 24,244 | 22,000 |   1.8
 9. | Austria | 22,591 | 20,500 |   1.7
10. | Great Britain | 20,277 | 18,400 |   1.5
11. | Greece | 19,836 | 18,000 |   1.5
12. | Turkey-in-Asia | 15,428 | 14,000 |   1.1
13. | China | 13,995 | 12,700 |   1.0
14. | German S. W. Africa | 13,224 | 12,000 |   1.0
15. | Algeria | 12,893 | 11,700 |   1.0
16. | France | 9,587 | 8,700 |   0.7
17. | India (Burma) | 6,502 | 5,900 |   0.5
18. | Peru | 4,331 | 3,930 |   0.3
19. | Japan | 4,143 | 3,760 |   0.3
20. | Egypt | 3,196 | 2,900 |   0.2
21. | Russia | 3,083 | 2,800 |   0.2
22. | Bulgaria | 2,204 | 2,000 |   0.2
23. | Sweden | 2,094 | 1,900 |   0.2
24. | Hungary | 1,256 | 1,140 |   0.1
25. | Bolivia | 1,102 | 1,000 |   0.1
26. | Portugal | 661 | 600 |
27. | Rhodesia | 361 | 330 |
| Total | 1,345,918 | 1,221,390 | 100.0

[129] Адаптировано на основе сводных данных Адольфа Кнопфа из Геологической службы США.

Четыре района, имеющие в настоящее время первостепенное значение, — это, в порядке убывания: Брокен-Хилл в Новом Южном Уэльсе (Австралия), юго-восточная Испания, юго-восточный Миссури и Кер-д’Ален в Айдахо, на долю которых в 1913 году приходилось соответственно около 19, 16, 12 и 10 процентов мировой добычи.

Соединенные Штаты.

— Основные добывающие регионы и их доля в общенациональной добыче свинца в 1915 году представлены ниже:

Region
Percentage
of total
domestic
production

Southeastern Missouri | 33
Coeur d’Alene, Idaho | 27
Utah | 18
Joplin (in Mo., Kans., Ark., and Okla.) |  6
Colorado |  5

Что касается типов руд и характера получаемого свинца, существуют две металлогенические провинции: долина Миссисипи, включая юго-восточный Миссури и Джоплин, а также небольшой район Висконсина, производящие от 39 до 45 процентов общего объема национальной добычи в виде мягкого свинца; и Западная провинция, где руды являются комплексными, содержат драгоценные металлы, а зачастую также сурьму и медь. Весь объем продукции Западной провинции, но лишь часть мягкого свинца, подвергается обессеребрению.

Девяносто процентов руды, добываемой в юго-восточном Миссури, поступает из округов Сент-Франсуа и Мэдисон. Месторождения руд содержат преимущественно галенит и вкраплены в кембрийские известняки на обширных площадях на глубине от 100 до 550 футов. В рудах округа Мэдисон присутствуют медь, никель и кобальт, при этом медные концентраты отделяются и отгружаются почти всеми компаниями региона. Основные действующие компании (названия поглощенных ими или являющихся их дочерними предприятий указаны в скобках): St. Joseph Lead Co. (Doe Run Lead Co.), Federal Lead Co., National Lead Co. (St. Louis Smelting & Refining Co.), Desloge Consolidated Lead Co., Baker Lead Co. (St. Francois Lead Co.), Boston Elvins Lead Co., Missouri Metals Co. (Mine La Motte Co.) и Missouri Cobalt Co. (North American Lead Co.). Компания St. Joseph Lead Co. обычно является второй по величине компанией по добыче свинца в Соединенных Штатах. Ее запасы имеют консервативно оцененный срок эксплуатации 20 лет при уровне добычи 2 000 000 тонн руды, или 80 000 коротких тонн свинца, в год. В 1917 году эта компания добыла 2 485 431 тонну руды, что составляет почти половину общего объема добычи в регионе. Federal Lead Co., дочерняя компания American Smelting & Refining Co., является следующей по величине добывающей компанией в регионе. В 1915 году она добыла и переработала 1 355 000 тонн руды. National Lead Co. через свою дочернюю компанию St. Louis Smelting & Refining Co. разрабатывает три рудника близ Флэт-Ривер и располагает обогатительной фабрикой суточной мощностью 2 400 тонн. Ее плавильный завод в Коллинсвилле перерабатывает собственные концентраты, а также концентраты Baker Lead Co. и Boston Elvins Lead Co. Desloge Consolidated Lead Co. эксплуатирует три рудника и фабрику суточной мощностью 1 700 тонн; ее руды переплавляются на заводе Federal Lead Co. Missouri Metals Co. эксплуатирует рудник Mine La Motte и фабрику, перерабатывающую 700 000 тонн ежегодно (по данным на 1917 год). В 1915 году оценивалось, что этот рудник может добывать 3 000 000 тонн руды ежегодно в течение шестидесяти лет.

В регионе Джоплин, который находится преимущественно в штате Миссури, но также включает прилегающие территории в Канзасе, Арканзасе и Оклахоме, руды залегают на трех горизонтах в горизонтальных пластах известняка и кремня нижнекаменноугольного возраста. На верхнем горизонте, обычно на глубине от 100 до 150 футов от поверхности, руда встречается в глинистых кремнистых брекчиях. Рудные тела представляют собой характерные «русла» шириной до 300 футов, непрерывные на одном горизонте на протяжении нескольких сотен футов, а в редких случаях — более мили. Средний горизонт, или «пластовая залежь», на глубине от 150 до 300 футов обычно имеет мощность от 6 до 15 футов. Руда, представляющая собой смесь галенита и цинковой обманки, цементирует брекчированный кремень. Третий, самый нижний горизонт в песчанистых известняках содержит в основном вкрапленные руды и на данный момент мало эксплуатируется. В 1915 году около 4 000 000 тонн руды было добыто из верхнего горизонта и 6 500 000 тонн — из среднего горизонта, или «пластовой залежи». Среднее содержание свинца в добываемой руде составляло около 0,25 процента. Большая часть свинцовых концентратов продается на свободном рынке. Район Уэбб-Сити является наиболее важным в регионе Джоплин, а компания American Zinc, Lead & Smelting Co. — крупнейшим производителем галенита. Большая часть продукции добывается арендаторами и мелкими операторами. Район Джоплин занимает второе место по значимости. Компания A. W. C. Mining Co. является крупнейшим разработчиком «пластовой залежи». Рудники Рейвенсвуд и Ритц компании United States Smelting, Refining & Mining Co. в округе Джаспер производят 218 000 тонн руды ежегодно. Концентраты этого региона переплавляются преимущественно на заводах Eagle-Picher Lead Co. в Галене (Канзас), Джоплине (Миссури), Уэбб-Сити (Миссури) и на заводах Granby Mining & Smelting Co. в Грэнби (Миссури).

Район Кер-д’Ален находится в округе Шошон, штат Айдахо. Месторождения представляют собой метасоматические жилы, образовавшиеся в результате замещения кремнистых осадочных пород вдоль зон трещиноватости, и содержат преимущественно галенит и сидерит с примесью пирита и сфалерита. В 1915 году отгрузки сырой руды составили 95 169 тонн с содержанием свинца 35 271 короткая тонна. Остальная часть руды, или почти 96 процентов от общего объема, была обогащена до содержания свинца около 50 процентов. Выход концентратов всех видов в 1915 году составил 329 530 тонн с содержанием свинца 128 928 коротких тонн, что довело общее содержание свинца в отгрузках сырой руды и концентратов до 164 199 коротких тонн. Горнодобывающие компании образуют три группы, определяемые главным образом их связями или аффилированностью с плавильными заводами: группа Bunker Hill, включающая Bunker Hill & Sullivan Mining & Concentrating Co. и Hecla Mining Co.; группа Day, включающая Tamarack & Custer Mining Co., рудник Amazon-Manhattan и Hercules Mining Co.; и группа American Smelting & Refining, включающая Federal Mining & Smelting Co. и различных мелких производителей.

Рудники компании Bunker Hill & Sullivan Mining & Concentrating Co. на 31 декабря 1917 года имели запасы в размере 3 457 634 тонн. Рудные тела представляют собой замещения кварцитов. Добыча этой компании в 1917 году составила 493 030 тонн руды, при этом извлеченный при плавке металлический свинец составил 46 996 тонн. Компания Bunker Hill & Sullivan, продолжая отгружать собственные руды на завод American Smelting & Refining Co. в Хелене, построила собственный плавильный завод в Келлогге (Айдахо), где переплавляет руды Hecla и других компаний. Семья Дэй контролирует компании Hercules и Tamarack & Custer, плавильный завод Northport в Нортпорте (Вашингтон, ныне закрыт) и Pennsylvania Smelting & Refining Co. в Питтсбурге (Пенсильвания). Отгрузки компании Hercules в 1916 году содержали около 22 000 тонн свинца. Обе компании являются закрытыми корпорациями и предоставляют мало информации о своей деятельности. Tamarack & Custer, вероятно, обладает большими запасами руды со средним содержанием свинца около 9 процентов; она производила до 3 000 тонн товарной руды и концентратов в месяц. Federal Mining & Smelting Co. эксплуатирует несколько рудников. Одна шестая часть акций принадлежит American Smelters Securities Co., и все ее серебряно-свинцовые руды и концентраты законтрактованы компании American Smelting & Refining Co. Компания Success Mining Co., разрабатывающая два рудника, является важным производителем. Interstate-Callahan была преимущественно производителем цинка, но отгружает некоторые свинцовые концентраты на завод Ohio & Colorado Smelting Co. в Салиде.

Добыча свинца в штате Юта ведется преимущественно в районах Парк-Сити, Бингем-Каньон и Тинтик. Руды, состоящие из галенита, тетраэдрита и пирита, а местами сфалерита, с их окисленными производными, встречаются в жилах, прорезающих известняки, песчаники и сланцы преимущественно каменноугольного возраста, а также в виде пластовых залежей в известняках. Оба типа часто ассоциированы с порфирами и образуют неправильные рудные тела в контактово-метаморфизованных известняках. Во многих рудниках медь является важным компонентом руд, а содержание серебра всегда значительно.

Добыча в штате Колорадо в 1917 году составила 33 995 коротких тонн свинца, из которых 9 293 короткие тонны поступили из района Ледвилл в округе Лейк, 10 412 коротких тонн — из района Сан-Хуан в округах Сан-Хуан, Сан-Мигель и Урей, и 6 816 тонн — из района Аспен в округе Питкин. Месторождения Ледвилла находятся в хребте Москито. Основными добывающими компаниями являются Iron Silver Mining Co., Yak Mining, Milling & Tunnel Co. и ее дочерняя компания Leadville Exploration & Mining Co.; Western Mining Co.; Downtown Mines Co.; Ibex Mining Co.; и United States Smelting, Refining & Mining Co. Yak Mining, Milling & Tunnel Co. и Western Mining Co. являются дочерними предприятиями American Smelting & Refining Co. В районе Сан-Хуан основными производителями являются рудники Liberty Bell, Smuggler-Union, Tomboy, Black Bear, Iowa-Gold Tiger, Dives, Shenandoah и Silver Lake. Жилы проникают во все обломочные и изверженные породы этого региона, а руды чрезвычайно сложны. В округе Питкин компания Smuggler Leasing Co. эксплуатирует большинство действующих рудников в Аспене. Руды отличаются необычной чистотой от других металлов, кроме свинца, сурьмы и серебра.

Австралия.

— Ресурсы свинца в Австралийском Союзе сосредоточены главным образом в Новом Южном Уэльсе, Западной Австралии, Тасмании и Квинсленде. Новый Южный Уэльс был основным производителем в прошлом, но тасманские месторождения в настоящее время быстро осваиваются и оснащаются для добычи.

Самым важным источником руды в Новом Южном Уэльсе является крупная жила Брокен-Хилл, расположенная в засушливых хребтах Барьер на высоте около 1 000 футов над уровнем моря. Мощность жилы варьируется от нескольких дюймов до 400 футов, и она разрабатывалась на протяжении трех миль. Добыча началась в 1884 году и в настоящее время ведется несколькими горнодобывающими компаниями, которые в порядке значимости их добычи и запасов руды располагаются следующим образом: Broken Hill South Silver Mining Co.; Broken Hill North Mining Co.; Zinc Corporation; Sulphide Corporation; British Broken Hill Proprietary Co.; Broken Hill Proprietary Co.; Broken Hill Proprietary Co., Block 10; и Broken Hill Proprietary Co., Block 14.

Хотя самые глубокие выработки достигают 1 815 футов, руда продолжает уходить на глубину. В течение многих лет оценочные запасы руды на всех рудниках составляли около 12 000 000 тонн. Верхняя часть жилы состояла из «железной шляпы» шириной от 20 до 100 футов, сложенной кремнистым и марганцовистым лимонитом, гематитом и каолином. Под «железной шляпой» находились огромные массы церуссита, англезита, куприта и малахита с обильными включениями кераргирита, эмболита и иодирита. Между окисленными и первичными сульфидными рудами находилась тонкая зона вторичных сульфидов. Первоначальные работы в районе велись с целью получения свинцовых руд, в результате чего накопились огромные отвалы цинксодержащих руд, отсортированных при обогащении, или цинксодержащих хвостов, оставшихся после обогащения свинцовых руд. В 1903 году объем этих отвалов оценивался в 5 687 400 тонн с содержанием цинка 18,6 процента. С появлением спроса на сульфидные цинковые руды и методов масляной флотации для разделения и обогащения эти отвалы стали важными источниками цинка. Существует два класса сульфидных руд, различающихся по пустой породе: руды с силикатной пустой породой и руды с кальцитовой пустой породой. Сульфидные руды представляют собой тесную смесь галенита и цинковой обманки, содержащую серебро. Рудные тела с силикатной пустой породой содержат родонит, гранат и кварц и богаче цинком и серебром, чем руды с кальцитовой пустой породой.

Компания Broken Hill South Silver Mining Co. имеет запасы руды, оцениваемые в 3 350 000 тонн, и является крупнейшим производителем руды на месторождении. Компании Broken Hill North, Broken Hill South, Amalgamated Zinc (De Bavay), Zinc Corporation и Barrier South, Ltd. контролируются группой британских и австралийских капиталистов Гувера-Говетта-Байо.

Компания Amalgamated Zinc Co. в 1913 году переработала 498 289 тонн хвостов, содержащих 17,1 процента цинка, 3,7 процента свинца и 4,4 унции серебра, получив 140 098 тонн цинковых концентратов с содержанием цинка 48,9 процента, свинца 5,9 процента и серебра 8,5 унции на тонну. Компания Zinc Corporation, созданная фирмой Bewick, Moreing & Co., имеет запасы руды, оцениваемые в 1 504 211 тонн, со средним содержанием 14,8 процента свинца, 9,2 процента цинка и 2,5 унции серебра на тонну.

Крупнейший свинцоводобывающий район Тасмании находится на Западном побережье, где крупнейшие производители — рудник Hercules группы Dundas, а также рудники Primrose и Tasmanian Copper группы компаний Rosebery — в настоящее время контролируются компанией Mount Read-Rosebery Co., аффилированной с Mount Lyell Mining & Railway Co., Ltd. Месторождения содержат комплексные сульфидные руды, запасы которых оцениваются государственным геологическим ведомством в 1 272 500 тонн со средним содержанием 29,79 процента цинка, 8,89 процента свинца, 12,16 унции серебра и 0,17 унции золота на тонну. С тех пор эта оценка была пересмотрена в сторону большей консервативности.

В 1913 году Западная Австралия произвела 26 589 длинных тонн свинцовой руды и 125 тонн серебряно-свинцовой руды, почти полностью в районе Нортхэмптон на Западном побережье. Единственной компанией, работающей в крупных масштабах, является Fremantle Trading & Smelting Co., эксплуатирующая рудники Baddera и Narra Tarra и ранее имевшая плавильный завод во Фримантле. Район Чиллаго является крупнейшим производителем в Квинсленде, его добыча в 1913 году составила 2 550 длинных тонн свинца в слитках, главным образом на руднике Girofla компании Mungana, а частично — из свинцово-медных концентратов. Компания Chillagoe эксплуатировала небольшой плавильный завод. Общий объем производства свинца в слитках в Квинсленде в 1913 году составил 3 603 длинные тонны.

Испания.

— Испания в 1913 году добыла 314 369 коротких тонн свинцовых концентратов, из которых было выплавлено 189 559 тонн свинца в слитках. В 1915 году было экспортировано всего 1 010 коротких тонн руды или концентратов и 161 912 коротких тонн обессеребренного свинца, в основном в Англию. Более 90 процентов добычи руды приходилось на провинции Хаэн, Мурсия, Кордова и Сьюдад-Реаль. В 1913 году провинция Альмерия занимала четвертое место, но ее рудники сейчас почти истощены. Эти провинции расположены в юго-восточной части Испании и охватывают горные хребты Сьерра-Морена и Сьерра-Невада.

В провинции Хаэн выделяются два основных района — Линарес-Санта-Елена и Ла-Каролина. Много лет назад Линарес был крупнейшим свинцоводобывающим районом в мире. Жилы прорезают гранит и тонкий перекрывающий песчаник и являются очень узкими. Государственный рудник Arrayanes эксплуатировался на протяжении двух с половиной миль и до глубины 1 500 футов. Пустая порода представлена гранитом, кварцем и кальцитом. Присутствуют железный и медный колчеданы и сфалерит, но легко получить 79-процентный свинцовый концентрат. Самый глубокий рудник достигает 1 800 футов и все еще находится в богатой руде. В окрестностях Санта-Елены рудники San Fernando, Ojo Vecino и Santa Ana принадлежат местным владельцам. Рудник Caridad принадлежит французскому капиталу, а Santa Susanna — бельгийскому концерну Compagnie Real Asturienne des Mines. В районе Ла-Каролина почти вертикальные жилы прорезают силурийские кварциты и кембрийские и силурийские сланцы. Руда достигает большей мощности, чем в жилах района Линарес. Рудник Nuevo Centenillo (английская собственность) производит 27 000 коротких тонн концентратов ежегодно. Крупная жила Guindo проходит через шесть рудников, два из которых принадлежат испанским компаниям, а три — компании Guindo Co., германо-испанской корпорации с годовым объемом производства 27 000 коротких тонн концентратов. Рудник Castillo La Vieja, принадлежащий французской компании, имеет годовой объем производства 20 000 тонн товарной руды.

В провинции Мурсия важными являются районы Масаррон и Картахена. Большинство жил почти вертикальны, но многие имеют ответвления или разветвления, образующие линзовидные и пластовые залежи в осадочных породах. Этот район простирается на юго-запад вдоль побережья от Кабо-де-Палос в нескольких милях к северу от Картахены. Добыча в этой провинции неуклонно снижается.

В провинции Кордова (район Посадас) многие серебряно-свинцово-цинковые рудники разрабатывались еще римлянами и остаются прибыльными до сих пор. Близ Алькарасехоса находятся рудники Anglo-Vask и Penarroya, последний принадлежит французской компании с тем же названием.

Развитие добычи свинцовых руд в провинции Сьюдад-Реаль сдерживалось отсутствием транспортных путей. Наиболее известным является район Эль-Ойо-Сан-Лоренцо, который в 1915 году вышел на четвертое место среди свинцоводобывающих районов Испании.

Германия.

— В имперской Германии свинцоводобывающие районы в порядке их значимости располагались следующим образом: Верхняя Силезия, Рейнская Пруссия, Вестфалия, Саксония, Ганновер и Нассау. Рейнская Пруссия и Вестфалия обычно объединяются в одну металлогеническую провинцию. В Гладбахе, к востоку от Кельна в Рейнской Пруссии, находятся месторождения руд, залегающие в мульдах и бассейнах в известняках. Руда представляет собой смесь смитсонита и галенита со сланцами. Основные месторождения Вестфалии находятся в Изерлоне и Брилоне. В Изерлоне руды, содержащие каламин, галенит и цинковую обманку, встречаются в виде нерегулярных карманов. Месторождения Брилона аналогичны, но большая часть руды встречается в трещинах известняка. На долю Рейнской Пруссии и Вестфалии приходится около одной трети германской добычи свинца.

Большая часть Верхней Силезии в 1914 году находилась в границах Германии, хотя ранее была частью Польского королевства, а население оставалось преимущественно польским; однако некоторые части входили в состав старых империй России и Австрии. Довоенная добыча свинцовых руд из Российской Польши велась исключительно в пределах этой металлогенической провинции. Месторождения, содержащие свинец и цинк вместе, залегают в триасовых пластах, перекрывающих каменноугольные породы, содержащие важные пласты угля. Такое соседство руды и топлива создало идеальную базу для крупной плавильной промышленности, развившейся на местном уровне, поскольку условия позволяют переплавлять низкосортные руды.

Исторические рудники во Фрайберге, Саксония (Рудные горы), дают небольшое количество цинковой обманки в связи с обогащением галенитовых руд из замечательной серии пересекающихся жил, число которых превышает 900, хотя лишь немногие из них имеют мощность более 2 футов. Они разрабатывались до глубины 2 100 футов. Более 10 процентов добычи свинца в Германии приходится на Саксонию. Эти рудники принадлежат саксонскому правительству и эксплуатируются им; оно также владеет плавильными заводами.

Свинец преобладает над цинком в рудах Верхнего Гарца в Ганновере. Эти руды встречаются в жилах и зонах в сланцах девонского и нижнекаменноугольного возраста. Эти рудники эксплуатируются Прусским горным управлением, которое также управляет двумя плавильными заводами, при этом объем производства составляет около 10 процентов от общего объема добычи в Германии. В Нассау, в долине Лана, свинцовые руды добываются как побочный продукт вместе с концентратами цинковой обманки.

Мексика.

— В Мексике свинцовые руды добываются в нескольких штатах, наиболее важными из которых являются Чиуауа, Дуранго, Коауила, Нуэво-Леон, Сонора, Сан-Луис-Потоси и Сакатекас. Во многих районах в течение значительной части последних восьми лет работы велись с перерывами и временами приостанавливались на длительные периоды.

Район Санта-Эулалия в штате Чиуауа в значительной степени принадлежит американским компаниям, включая American Smelting & Refining Co., эксплуатирующую рудники Mina Vieja, Sin Nombre, Velardeña, San Antonio и Santo Domingo, а также El Potosi Mining Co., эксплуатирующую одноименные рудники. Рудник San Toy находится в аренде у American Metal Co., ныне очищенной от германских интересов. Santa Eulalia Mining Co. принадлежит наследникам Херста. Buena Tierra Mining Co. является британским концерном. Рудники районов Санта-Барбара и Парраль также в значительной степени находятся под американским контролем, среди многих других — Montezuma Lead Mining Co. интересов Р. С. Тауна, Granadeña Mining Co., American Smelters Securities Co. и American Zinc Extraction Co. American Smelters Securities Co. эксплуатирует рудники Tecolotes, Montezuma, San Diego, Guadalupe и Alfarena. Рудники San Francisco принадлежат британскому капиталу. В районе Сан-Исидро рудники Calera, Prieta и Buena Vista эксплуатируются компанией American Smelting & Refining Co. Рудник Lago эксплуатируется компанией C. M. de Las Plomosas (французская). В районе Парадо находятся рудники Compañia Minera Aurora y Anexas, контролируемые семьей Мадеро (мексиканская). Другими рудниками компании American Smelting & Refining Co. в Чиуауа являются Orizaba и La Union в Магистрале, Jibosa в Долоресе, La Luz и Parcionera в Кордере, Veta Grande и Veta Colorado.

Крупнейшими операторами в штате Дуранго являются American Smelters Securities Co. в Веларденье и Cia. Minera de Peñoles в Мапими; обе компании стали американскими после продажи акций American Metals Co., принадлежавших германским интересам, Управляющим по делам собственности враждебных государств.

В штате Сонора компания Carnegie Lead & Zinc Co. во время войны разрабатывала рудник близ Кананеи, но лучшая часть месторождения в настоящее время истощена.

Рудники Tiro General в штате Сан-Луис-Потоси принадлежат American Smelting & Refining Co.

Рудники Cabrilla и Paloma в районе Кабрильяс в штате Коауила принадлежат Compañia Minera de Peñoles, контролируемой American Metal Co. Район Сьерра-Мохада находится под доминирующим влиянием американских компаний, основные рудники принадлежат Consolidated Kansas City Smelting & Refining Co., дочерней компании American Smelting & Refining Co. Рудник Boquillas de Carmen был приобретен американской компанией.

В штате Нуэво-Леон месторождения, расположенные в радиусе 50 миль от Монтеррея, в Вильядаме, Вальесильо, Ладера-Оксиденталь-де-Минас-Вьехас и др., эксплуатировались германскими и американскими компаниями, включая Compañia Metalurgica Mexicana (американская), Joplin-Mexican Mining Co. (американская) и Metallgesellschaft (германская).

Другие страны.

—The output of lead ore in Tunis in 1913, almost wholly by French companies, was 56,072 metric tons. It is all exported.

Практически весь объем добычи свинцовой руды в Италии приходится на район Иглезиас на Сардинии, который в 1915 году произвел 40 829 метрических тонн руды со средним содержанием свинца 55 процентов из общего объема национальной добычи в 41 590 метрических тонн. Основными операторами являются компании Monteponi и Pertusola, первая — итальянская, вторая — английская. Остальная часть руды поступает из провинций Бергамо, Брешиа, Кунео и Гроссето, а действующими компаниями являются English Crown Spelter Co. (английская), Societa Austro-Belga и Société de la Vieille Montagne (бельгийские).

В Чехословакии наиболее важным районом является Пршибрам в Богемии. Богатые свинцовые руды когда-то добывались в Мизе, но район в настоящее время истощен. Район Иоахимсталь на протяжении столетий был важным производителем.

В Германской Австрии находятся серебряно-свинцовые горнодобывающие районы Шнееберг в Тироле и Райбль в Верхней Каринтии. В обоих районах рудники до войны принадлежали австрийскому государству и эксплуатировались им. Мисс в Каринтии является одним из основных источников руды в последние годы.

Свинцовые рудники Великобритании в 1916 году произвели 17 083 тонны обогащенной свинцовой руды. Крупнейшим оператором является Weardale Lead Co., эксплуатирующая рудники Boltsburn и Stanhopeburn и переплавляющая собственные, а также некоторые давальческие руды.

В Греции единственным важным свинцовым месторождением является Лаврион, который разрабатывался в крупных масштабах в античные времена. В настоящее время он контролируется и эксплуатируется французской компанией Compagnie Française des Mines de Laurium.

Добыча свинца в Канаде ведется преимущественно в Британской Колумбии, причем наиболее важные производители находятся в районе Слокан. Крупнейшим оператором является Consolidated Mining & Smelting Co. of Canada, Ltd., владелец также плавильного завода Trail. Эта компания эксплуатирует рудник Sullivan и другие рудники и за год, закончившийся 30 сентября 1917 года, произвела 29 542 тонны свинцовой руды на руднике Sullivan и от 1 100 до 1 500 тонн на нескольких других. Сообщалось, что рудник Sullivan имеет запасы в 3 500 000 тонн галенито-сфалеритовой руды. Многочисленные более мелкие предприятия в том же районе отгружают руду на завод Trail, который произвел около 22 000 тонн свинца за год, закончившийся 30 сентября 1917 года.

Важнейшими свинцово-серебряными рудниками Азиатской Турции являются рудники в Ходжа-Гернише (Балия), принадлежащие Société des Mines de Balia-Kara-Aidin (французская), которые дают около 12 000 тонн свинца ежегодно. Существует государственный рудник в Булгардаге, производящий свинец, золото и серебро. Английская компания Asia Minor Mining Co. производит около 3 000 тонн руды ежегодно.

В Китае десять свинцовых рудников в провинции Хунань контролируются китайцами. Wah Chang Mining & Smelting Co., Ltd. эксплуатирует рудники Тьен-Фор-Тай. Рудник Шуй-Ко-Шань, контролируемый Горным управлением Хунани, разрабатывающий месторождение в известняках, в 1913 году произвел 51 561 нетто-тонну руды, из которой было получено 3 762 тонны свинцовых концентратов и 12 275 тонн цинковых концентратов. С 1913 года добыча была увеличена, но возможности месторождения ограничены. Японцы пытались установить контроль над этим рудником, но безуспешно. Свинец в слитках, производимый в Китае, потребляется преимущественно внутри страны. Единственный современный свинцовый плавильный завод находится в Чанша и принадлежит японцам.

Добыча свинца в Юго-Западной Африке (бывшей германской) велась главным образом на месторождении Цумеб в районе Гроотфонтейн в горах Отави. Руды, экспортированные в 1913-14 финансовом году, составили 48 000 длинных тонн со средним содержанием 13 процентов меди, 25 процентов свинца и 7,7 унции серебра. Руда представляет собой крупнокристаллический агрегат серебросодержащего галенита и халькозина с незначительным количеством других минералов. Otavi Mines & Railway Co. владеет этим рудником и эксплуатирует его; в 1913-14 годах руда экспортировалась в Соединенные Штаты для плавки.

В 1913 году вся добыча свинцовой руды в Алжире велась в департаменте Константина и составила 21 442 тонны. Практически весь объем добычи обеспечивался французскими компаниями.

Свинцовая руда добывается в нескольких разрозненных районах Франции, главным образом на юге. Среди рудников — рудники Chaliac et Chassezac (Ардеш) компании Société Metallurgique et Minière des Cevennes, произведшие 2 200 метрических тонн в 1913 году; рудники Société Civile des Mines des Malines; рудник La Londe компании Société des Mines des Bormettes; рудник Société des Mines de Bleymard, произведший 2 470 тонн галенитовой руды в 1913 году; а также рудники Pierrefitte (Верхние Пиренеи), Peybrune и Bulard de Sentein-Saint Lary (Арьеж). Все они, по-видимому, являются французскими компаниями, за исключением Pierrefitte, который находится под английским контролем.

В Бирме основные месторождения — это рудники Бодуин в Северных Шанских штатах, соединенные в настоящее время с Бирманской железной дорогой из Рангуна. Рудные тела, представляющие интерес в настоящее время, являются почти вертикальными залежами в полевошпатовых песчаниках (риолитовых туфах или окремненных риолитах) и риолитовой серии. Считается, что рудное тело Chinaman и меньшее по размеру рудное тело Shan были единым целым, хотя сейчас разделены сбросом. Оценочные запасы на 31 декабря 1917 года составляли 4 033 000 тонн свинцово-цинковой руды с содержанием 24,7 унции серебра, 27,4 процента свинца, 19,1 процента цинка и 0,4 процента меди; а также 105 000 тонн медно-серебряной руды с содержанием 21,0 унции серебра, 19,9 процента свинца, 8,8 процента цинка и 8,9 процента меди. С тех пор геологоразведочные работы значительно увеличили эти запасы. Кроме того, оценивается наличие 1 600 000 тонн низкосортной руды со средним содержанием 5,1 унции серебра, 7,5 процента свинца, 4,8 процента цинка и 0,2 процента меди на тонну, с отличными перспективами дальнейшего расширения. Большой тоннаж руды из «железной шляпы», содержащей 4 или 5 унций серебра, 4-5 процентов свинца и немного цинка, добывается дешево и доступен в качестве кремнистого флюса. Основными компонентами руд являются галенит и сфалерит с небольшим количеством пирита и халькопирита. Вся руда является серебросодержащей.

Свинцовые и цинковые концентраты пригодны для обычных методов плавки. В Сакчи при содействии индийского правительства строится завод по дистилляции цинка и производству серной кислоты для переработки табличных цинковых концентратов. Ожидается, что его первоначальная мощность в 25 000 тонн концентратов будет увеличена до 75 000 тонн. Компания эксплуатирует свинцовый плавильный завод в Нам-Ту, в 11 милях от рудников, используя смесь руды и древних шлаков. Предлагается переработка промпродуктов по процессу Ганлина, и 100-тонная установка строится в Эйвонмуте, Англия. Можно ожидать, что месторождения Бодуин станут важным фактором в мировой добыче свинца в ближайшем будущем. Они принадлежат Burma Mines, Ltd., английской корпорации, представляющей интересы Р. Тилдена Смита-Говетта-Гувера и часть американского капитала.

Добыча свинца в Перу в значительной степени представлена древними высокосвинцовыми шлаками из района Серро-де-Паско, департамент Хунин, отгружаемыми на заводы American Smelting & Refining Co. в Соединенных Штатах. Свинец встречается как второстепенный компонент медных месторождений.

Месторождения свинцовых руд в Японии полностью принадлежат японцам и эксплуатируются ими. Во время войны импортировались и переплавлялись австралийские концентраты и китайская руда: 10 666 коротких тонн первых с содержанием 56 процентов свинца в 1915-16 финансовом году и 9 829 коротких тонн вторых в 1916 году. Компания Fujita, ведущая добычу в Японии, Корее и на Формозе, производит 382 короткие тонны свинца ежегодно. Ее основной рудник — Косака на северной оконечности Хонсю, главного острова Японии. Руда представляет собой комплексную сульфидную смесь свинцовых, цинковых, железных и медных минералов. Годовой объем добычи этого рудника составляет около 335 коротких тонн свинца. Mitsui Mining Co., Ltd. является крупнейшим производителем, объем производства которой в 1915 году составил 3 561, а в 1916 году — 8 098 коротких тонн свинца в слитках. Это количество полностью получено из цинково-свинцового рудника Камиока в провинции Хида, представляющего собой контактово-метаморфическое месторождение в линзах известняка, заключенных в архейских гнейсах близ контакта с кварцевыми порфирами.

Единственным месторождением, эксплуатируемым в Египте, является известное еще древним месторождение Гебель-Росас, ныне эксплуатируемое французской компанией Compagnie Française des Mines de Laurium. Что касается бывшей Российской империи, то добыча свинца в Российской Польше и на Кавказе невелика, причем объем производства в 1913 году поступал главным образом с Кавказа и обеспечивался компанией «Эльборусс» и Compagnie d’Alagir (бельгийская).

На Алтае в Сибири цинково-свинцово-серебряное месторождение Змеиногорское, ранее принадлежавшее Russian Mining Corporation (британская), в настоящее время принадлежит российской компании Altai Mines, Ltd., хотя часть капитала, вероятно, является британской. Нерчинский район в восточной Сибири включает множество известных месторождений. Акатуевское, Кадаинское, Алгачинское и Кличкинское месторождения являются жильными, тогда как многие месторождения Зерентуйского рудника, Газимурской долины, Култуминское и Мальцевское представляют собой линзовидные массы вкрапленной руды. На Кадаинских месторождениях два массивных вкрапленных рудных тела залегают в доломитах между двумя жилами. Эти месторождения контролировались Кабинетом Его Императорского Величества, и их эксплуатация серьезно рассматривалась британским и американским капиталом незадолго до революции. Месторождениями наибольшей важности в настоящее время в Сибири являются месторождения Ridder Mining Co., контролируемой Irtysh Corporation из Лондона, которая разработала два рудника, Риддерский и Сокольный, на одной и той же минерализованной зоне. Месторождения представляют собой замещения комплексной сульфидной рудой членов согласной серии сланцев, туфов и изверженных силлов. В 1916 году запасы оценивались в 945 000 тонн с содержанием 31,2 процента цинка, 18,1 процента свинца, 1,5 процента меди, 9,7 унции серебра и 0,47 унции золота; а также 2 229 000 тонн со средним содержанием 6,7 процента цинка, 3,5 процента свинца, 0,5 процента меди, 1,7 унции серебра и 0,7 унции золота на тонну. Другие известные минерализованные зоны не были разработаны, но возможности объекта огромны, ограничиваясь главным образом общими социально-политическими и экономическими условиями.

Небольшое количество свинца производится в Болгарии на нескольких мелких месторождениях, содержащих тесные смеси свинцовых, медных и цинковых минералов; обычно преобладает либо цинк, либо медь.

Самым важным свинцовым месторождением в Швеции является Сала в Вестманланде, где неправильные массы и жилы галенита и цинковой обманки с незначительным количеством пирита и др. встречаются в известняках. Аналогичные месторождения встречаются в Лофасе и Гулдмедсхюттане.

В Венгрии нет важных свинцовых рудников, хотя галенит встречается в некоторых разрабатываемых жилах, особенно в Шемнице, где крупные рудники являются собственностью венгерского государства.

Большая часть руды из Боливии, экспортируемой в Соединенные Штаты, поступает с рудника Махо, который в 1912 году произвел 884 тонны свинца. Этот рудник находится на юге Боливии в районе Ла-Киака.

Важнейшим свинцоводобывающим районом в Португалии является Мерлота близ реки Гвадиана, где встречаются серебросодержащий галенит и окисленные руды. Другими районами являются Вила-Реал, Визеу, Авейру, Порталегри и Бежа. Месторождения аналогичны месторождениям Испании.

Единственным важным месторождением в Родезии (Южная Африка) является Родезия Брокен-Хилл. Крупные рудные тела, насколько они разведаны, почти полностью окислены. Одно рудное тело оценивается в 250 000 длинных тонн руды со средним содержанием 26 процентов свинца и 22,5 процента цинка; другое рудное тело оценивается в 300 000 длинных тонн со средним содержанием 32 процента цинка, с небольшим содержанием свинца, но большим количеством оксида железа и карбоната. Эти рудные тела контролируются британским капиталом. При разработке коммерческого метода переработки возникли значительные трудности. Отчеты указывают, что это месторождение имеет большие масштабы, чем принято считать.

Самое важное свинцовое месторождение Бельгии, или, вернее, нейтрального района Морене, прилегающего к Бельгии, принадлежало бельгийской компании Société de la Vieille Montagne в Морене. Оно было истощено в 1882 году.

Изменения в географическом распределении добычи в ближайшем будущем.

— Никаких заметных изменений в довоенном уровне добычи руд странами Европы или Северной Африки не ожидается после восстановления нормальных условий. Большинство районов в этих странах эксплуатировались долгое время и прошли свой пик добычи; многие приближаются к истощению. Возможным исключением из этого утверждения является провинция Сьюдад-Реаль в Испании, которая энергично осваивается компанией Penarroya. Раздел Австро-Венгрии существенно не повлияет на контроль над свинцовой промышленностью.

Соединенные Штаты останутся крупнейшим источником свинца в мире, и единственное ожидаемое изменение — это незначительное увеличение относительной важности добычи твердого свинца в западных штатах.

Главным новым фактором в добыче станут рудники Бодуин в Бирме, которые осваиваются в крупных масштабах для производства 300 000 тонн руды ежегодно.

Недавние разработки на Алтае в юго-западной Сибири доказали наличие огромных тел комплексных цинково-свинцовых руд. Их географическая изоляция будет препятствовать тому, чтобы они стали важным фактором на мировом рынке в течение длительного периода, несмотря на их большие размеры и отличное качество. Масштабы их эксплуатации будут определяться главным образом тем, насколько сильно российский рынок будет затронут внутренними социальными и политическими условиями. Потеря польского промышленного региона с его рынком, защищенным жесткими тарифами, существенно ограничивает круг видимых рынков сбыта.

В будущем, но не в ближайшее время, ожидается, что в регионе Анд в Южной Америке будут развиваться месторождения комплексных свинцовых руд, подобные месторождениям западных штатов США.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Политический контроль над мировыми ресурсами свинца до начала войны в 1914 году, по-видимому, был второстепенным фактором в отрасли и проявлялся главным образом через введение протекционистских тарифов или бонусов, призванных стимулировать внутреннюю добычу, плавку и рафинирование. Такие меры привели к созданию свинцовоплавильной промышленности в Британской Колумбии и послужили стимулом к развитию Алтайского района в Сибири. Как будет подробно описано далее, рост международных коммерческих отношений позволил германским интересам создать организации, которые, хотя и не были всеобъемлющими, обеспечивали эффективный контроль над отраслью.

Однако во время Мировой войны политическая юрисдикция в значительной степени использовалась для восстановления контроля граждан над национальными ресурсами. Это движение было особенно заметно в Британской империи, где в настоящее время существует совместный политический и коммерческий контроль. Иностранные интересы были устранены правительственными мерами, и правительство сохраняет долю в контроле через свое участие в маркетинговых организациях или финансовое участие в перерабатывающих предприятиях. Во Франции консорциум Société Minerais et Metaux, организованный по инициативе правительства, является арбитром отрасли и включает все важные французские компании как внутри страны, так и за рубежом. В Соединенных Штатах Управляющий по делам собственности враждебных государств активно занимался устранением всех интересов враждебных иностранцев.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Медь, свинец и цинк образуют отдельный класс с точки зрения промышленного использования и объемов производства, занимая после железа, которое значительно превосходит их, место наиболее важных цветных металлов. Общий годовой объем производства каждого из них во всем мире значительно превышает миллион тонн.

Table 53.—Ore Production, Smelting, and Consumption of Lead in 1913
(Tons of 2,000 Pounds)

Country | Recoverable lead content of ores and concentrates | Primary pig lead | Recoverable lead in ores and pig lead
Mine production | Exports | Imports | Smelter production | Imports | Exports | Consumption | Net imports | Net exports
Net tons | Per cent. [130] | Net tons | Per cent. [130] | Net tons | Per cent. [130] | Net tons | Per cent. [131] | Net tons | Per cent. [131] | Net tons | Per cent. [131] | Net tons | Per cent. | Net tons | Per cent. [132] | Net tons | Per cent. [132]
Algeria | 12,900 |   1.0 | 12,900 |   1.0 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 12,900 |   1.3
Australia | [133]244,500 |  19.7 | 132,000 |  10.6 | ... | ... | 112,500 |   9.0 | ... | ... | 101,900 |   8.1 | 10,600 |   0.8 | ... | ... | 233,900 |  18.7
Austria-Hungary | 23,800 |   1.9 | ... | ... | 2,800 |   0.2 | 26,600 |   2.1 | 12,500 |   1.0 | ... | ... | 39,100 |   3.0 | 15,300 |   1.2 | ... | ...
Belgium | ... | ... | ... | ... | 56,000 |   4.5 | 56,000 |   4.5 | ... | ... | 8,700 |   0.7 | 47,300 |   3.7 | 47,300 |   3.8 | ... | ...
Bolivia | 1,100 |   0.1 | 1,100 |   0.1 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 1,100 |   0.1
Bulgaria | 2,200 |   0.2 | 2,200 |   0.2 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 2,200 |   0.2
Canada | 18,800 |   1.5 | ... | ... | ... | ... | 18,800 |   1.5 | 6,400 |   0.5 | ... | ... | 25,200 |   2.0 | 6,400 |   0.5 | ... | ...
China | 14,000 |   1.1 | 14,000 |   1.1 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 14,000 |   1.1
Egypt | 3,200 |   0.3 | 3,200 |   0.3 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 3,200 |   0.2
France | 9,600 |   0.8 | ... | ... | 21,300 |   1.7 | 30,900 |   2.5 | 87,700 |   7.0 | ... | ... | 118,600 |   9.1 | 109,000 |   8.7 | ... | ...
German S. W. Africa | 13,200 |   1.0 | 13,200 |   1.0 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 13,200 |   1.0
Germany | 79,300 |   6.4 | ... | ... | 120,300 |   9.7 | 199,600 |  15.9 | 46,800 |   3.7 | ... | ... | 246,400 |  19.1 | 167,100 |  13.4 | ... | ...
Great Britain | 20,300 |   1.6 | ... | ... | 13,300 |   1.1 | 33,600 |   2.7 | 177,400 |  14.1 | ... | ... | 211,000 |  16.4 | 190,700 |  15.2 | ... | ...
Greece | 20,300 |   1.6 | ... | ... | ... | ... | 20,300 |   1.6 | ... | ... | 20,300 |   1.6 | ... | ... | ... | ... | 20,300 |   1.6
Holland | ... | ... | ... | ... | ... | ... | ... | ... | 10,500 |   0.8 | ... | ... | 10,500 |   0.8 | 10,500 |   0.1 | ... | ...
India (Burma) | 6,500 |   0.5 | [134]2,200 |   0.2 | ... | ... | 4,300 |   0.3 | ... | ... | 4,300 |   0.3 | ... | ... | ... | ... | 6,500 |   0.5
Italy | 24,900 |   2.0 | [134]1,000 |   0.1 | ... | ... | 23,900 |   1.9 | 12,000 |   1.0 | ... | ... | 35,900 |   2.8 | 11,000 |   0.1 | ... | ...
Japan | 4,200 |   0.3 | ... | ... | ... | ... | 4,200 |   0.3 | 17,000 |   1.3 | ... | ... | 20,400 |   1.6 | 17,000 |   1.3 | ... | ...
Mexico | 68,300 |   5.5 | 7,100 |   0.6 | ... | ... | 61,200 |   4.9 | ... | ... | 61,200 |   4.9 | ... | ... | ... | ... | 68,300 |   5.5
Norway | ... | ... | ... | ... | ... | ... | ... | ... | 500 | ... | ... | ... | 500 | ... | 500 | ... | ... | ...
Peru | 4,300 |   0.3 | 4,300 |   0.3 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 4,300 |   0.3
Portugal | 600 | ... | 600 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 600 | ...
Rhodesia | 400 | ... | 400 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 400 | ...
Russia | 3,100 |   0.2 | [134]2,000 |   0.2 | ... | ... | 1,000 |   0.1 | 63,700 |   5.1 | ... | ... | 64,800 |   5.0 | 61,700 |   5.0 | ... | ...
Spain | 209,200 |  16.8 | ... | ... | 9,900 |   0.8 | 219,100 |  17.4 | ... | ... | 219,100 |  17.5 | ... | ... | ... | ... | 209,200 |  16.7
Sweden | 2,100 |   0.2 | 500 | ... | ... | ... | 1,600 |   0.1 | 1,200 |   0.1 | ... | ... | 2,800 |   0.2 | 700 | ... | ... | ...
Switzerland | ... | ... | ... | ... | ... | ... | ... | ... | 6,400 |   0.5 | ... | ... | 6,400 |   0.5 | 6,400 |   0.5 | ... | ...
Tunis | 31,100 |   2.5 | 31,000 |   2.5 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 31,100 |   2.5
Turkey-in-Asia | 15,300 |   1.2 | ... | ... | ... | ... | 15,300 |   1.2 | ... | ... | 15,300 |   1.2 | ... | ... | ... | ... | 15,300 |   1.2
United States | 411,900 |  33.3 | ... | ... | 13,200 |   1.0 | 425,100 |  33.8 | ... | ... | 10,800 |   0.9 | 414,300 |  32.1 | 2,400 |   0.2 | ... | ...
Other countries | ... | ... | ... | ... | 2,600 |   0.2 | 2,600 |   0.2 | 34,100 |   2.7 | ... | ... | 36,700 |   2.8 | 36,700 |   2.9 | ... | ...
World[135] | 1,245,100 | 100.0 | 227,800 |  18.2 | 239,400 |  19.2 | 1,256,700 | 100.0 | 476,200 |  37.8 | 441,600 |  35.2 | 1,290,500 | 100.0 | 682,700 |  52.9 | 636,500 |  50.9

[130] Процентная доля мирового производства извлекаемого свинца из руд.

[131] Процентная доля мирового производства свинца в слитках на плавильных заводах.

[132] Процент от среднего значения итогов, использованных в a и b.

[133] Общее извлекаемое содержание свинца в заявленной добыче руды за вычетом содержания свинца в австралийской продукции в формах, отличных от свинца в слитках.

[134] Вероятно, представляет собой излишек руды, а не экспорт.

[135] Отсутствие надлежащего баланса в этих итогах указывает на ошибку, неполноту или отсутствие сопоставимости, отчасти из-за задержки в статистических данных, которые, однако, правильно отражают общую ситуацию.

Владение или оперативный контроль над рудниками является второстепенным фактором в коммерческом контроле над свинцовой промышленностью и в целом имеет значение лишь как фактор, определяющий распределение руды на плавильные заводы, конкурирующие в остальном на почти равных условиях. Большинство крупных плавильных интересов занимаются добычей или имеют дочерние компании, занимающиеся добычей, либо имеют достаточные доли в крупных горнодобывающих компаниях, чтобы влиять на свои контракты на плавку. Таким образом, фактическая основа контроля над отраслью часто осуществляется через объединенное владение или контроль над рудниками и перерабатывающими предприятиями.

Владение или контроль над перерабатывающими предприятиями были доминирующим фактором в коммерческом контроле над отраслью. Производство каждой страны в 1913 году, основные свинцовоплавильные заводы мира, а также их аффилированность и контроль обсуждаются ниже.

Соединенные Штаты.

—Контроль над свинцовой промышленностью Соединенных Штатов посредством владения или управления распределен между десятью группами следующим образом:

1. Группа Morgan-Guggenheim, включающая American Smelting & Refining Co.; American Smelters Securities Co.; и их дочерние предприятия: Selby Smelting & Lead Co.; Tacoma Smelting Co.; Garfield Smelting Co.; Consolidated Kansas City Smelting & Refining Co.; Federal Lead Co.; Federal Mining & Smelting Co.; Western Mining Co.; Silver Lake Mining Co.; а также Yak Mining, Milling & Tunnel Co.

2. St. Joseph Lead Co.

3. National Lead Co.; St. Louis Smelting & Refining Co.; United Lead Co.

4. Группа Rockefeller-Ryan, включающая International Smelting Co. (плавильный завод в Туэле, штат Юта) и International Lead Refining Co. (аффинажный завод в Ист-Чикаго, штат Индиана).

5. Группа United States Smelting, Refining & Mining Co., включающая United States Smelting Co. (плавильный завод в Мидвейле, штат Юта); U. S. Metals Refining Co. (электролитический завод по рафинированию свинца в Грасселли, штат Индиана); Needles Mining & Smelting Co. (обогатительная фабрика по переработке цинково-свинцовых руд по заказам в Нидлсе, штат Калифорния); Bingham Mines Co. и другие рудники в штате Юта (Bullion, Beck, Champion, Utah-Apex, Centennial-Eureka и Tintic); рудники Sunnyside и Gold Prince в Силвертоне, штат Колорадо; ранее — доля в 50% в International Metals Selling Co.; а также подразделение Leadville Unit.

6. Группа Day, включающая Northport Smelting & Refining Co.; Pennsylvania Smelting & Refining Co.; Hercules Mining Co.; Tamarack & Custer Mining Co.; а также рудники Amazon-Manhattan и другие.

7. Группа American Metal Co., контролирующая Ohio & Colorado Smelting Co. (владеет 65% акций) и Balbach Smelting & Refining Co. (владеет одной третью акционерного капитала и реализует всю продукцию).

8. Группа Hayden-Stone-Clark-Coolidge, включающая American Zinc, Lead & Smelting Co.; American Zinc Co. of Tennessee; American Zinc Co. of Wisconsin; American Zinc Co. of Illinois; Granby Mining & Smelting Co. of Missouri; а также Butte & Superior Mining Co.

9. Группа Eagle-Picher, включающая Eagle-Picher Lead Co. (Джоплин, штат Миссури) с плавильным заводом в Джоплине, контролирующая Galena Smelting & Manufacturing Co. (Галина, штат Канзас) и Webb City Smelting & Manufacturing Co. (Уэбб-Сити, штат Миссури).

10. Bunker Hill & Sullivan Mining & Concentrating Co., контролируемая интересами Bradley-Crocker и, вероятно, представляющая определенную долю английского капитала.

11. Desloge Consolidated Lead Co., которая ранее эксплуатировала собственный плавильный завод, но в настоящее время перерабатывает свои руды на давальческих началах на заводе Federal Lead Co. и самостоятельно реализует свой свинец.

Все вышеперечисленные компании, насколько известно, принадлежат гражданам США и контролируются ими, за исключением некоторых долей в American Metal Co. и, возможно, в Bunker Hill & Sullivan Mining & Concentrating Co.

American Metal Co. имеет 70 000 акций акционерного капитала, из которых 34 644 акции принадлежали Metallgesellschaft, одной из компаний германского «трио»; 18 620 акций принадлежат немцам, ставшим натурализованными гражданами США и осуществлявшим управление; оставшиеся 16 736 акций принадлежали лондонской фирме Henry L. Merton & Co., находящейся в процессе ликвидации. Управляющий имуществом иностранных граждан (Alien Property Custodian) изъял вышеупомянутые 34 644 акции и продал их на публичном аукционе. Контроль над компанией возложен на трех доверительных управляющих, выбранных по соглашению между Управляющим имуществом иностранных граждан и американскими акционерами.

Компания Vogelstein & Co. одно время связывала группы 5, 7, 8 и 10, главным образом посредством контрактов на сбыт. Vogelstein & Co. владела International Metals Selling Co., ранее занимавшейся реализацией продукции United States Smelting, Mining & Refining Co., но эта связь в настоящее время разорвана. Контракт на продажу всей продукции American Zinc, Lead & Smelting Co. принадлежал L. Vogelstein & Co., частично принадлежавшей Aron Hirsch & Sohn, другому участнику крупного германского металлургического объединения. Компания L. Vogelstein & Co. (Inc.) была изъята Управляющим имуществом иностранных граждан и находилась под контролем пяти директоров, двое из которых были назначены Управляющим. Оперативное управление Bunker Hill & Sullivan Mining & Concentrating Co. возложено на американцев, но сбыт продукции осуществляет Vogelstein & Co. Группы 5 и 8, вероятно, в некоторой степени связаны общими крупными акционерами — Кларком и Кулиджем из Бостона.

Сообщается, что Л. Фогельштейн продал свои доли компании American Metal Co., а впоследствии, в начале 1920 года, приобрел одну пятую долю в этой компании.

В результате деятельности Управляющего имуществом иностранных граждан владение и контроль над практически всеми рудниками и перерабатывающими предприятиями в Соединенных Штатах перешли к гражданам США. Дополнительная информация о деятельности германских интересов в американской торговле металлами приведена в главе о меди, страницы 232–235.

В таблице 54 перечислены важные заводы по плавке и рафинированию свинца в Соединенных Штатах на текущий момент.

Таблица 54.—Заводы по плавке серебряно-свинцовых руд в Соединенных Штатах

Financial
Group
No.
Operating
company
Location
Number
of
furnaces
Annual
capacity
(tons of
charge)

 1 | American Smelters Securities Co. | Selby, Calif. |  3 | 210,000
 1 | American Smelting & Refining Co. | Denver, Colo. |  7 | 510,000
 1 | American Smelting & Refining Co. | Pueblo, Colo. |  7 | 380,000
 1 | American Smelting & Refining Co. | Durango, Colo. |  4 | 210,000
 1 | American Smelting & Refining Co. | Leadville, Colo. | 10 | 510,000
 1 | American Smelting & Refining Co. | Murray, Idaho |  8 | 657,000
 1 | American Smelting & Refining Co. | East Helena, Mont. |  4 | 306,000
 1 | American Smelting & Refining Co. | Omaha, Neb.[137] |  2 | 82,000
 1 | American Smelting & Refining Co. | Perth Amboy, N. J.[137] |  4 | 170,000
 1 | Con. Kansas City Smelting & Refining Co. | El Paso, Texas |  6 | 380,000
10 | Bunker Hill & Sullivan Mining & Concentrating Co. | Kellogg, Idaho |  3 | 600,000
 7 | Ohio & Colorado Smelting Co. | Salida, Colo. |  3 | 200,000
 5 | U. S. Smelting, Refining & Mining Co. | Midvale, Utah |  7 | 530,000
 6 | Northport Smelting & Refining Co. | Northport, Wash. |  2 | 216,000
 6 | Pennsylvania Smelting Co. | Carnegie, Pa. |  2 | 60,000
 4 | International Smelting Co. | Tooele, Utah |  5 | 500,000
| Total |  | 77 | 5,521,000

Также аффинажный завод.

В следующей таблице 55 показана относительная значимость различных финансовых групп, контролирующих производство свинца в Соединенных Штатах.

Таблица 55.—Финансовые группы, контролирующие производство свинца в Соединенных Штатах

Financial group No. | Company | Percentage of production
Oct.-Nov., 1918 | 1917
 1 | American Smelting & Refining Co | 34.1 | 37.7
 3 | National Lead Co. (St. Louis Smelting & Refining Co.) |  5.9 |  9.0
 2 | St. Joseph Lead Co. | 20.1 | 16.4
 4 | International Smelting & Refining Co. |  3.7 |  6.5
 5 | U. S. Smelting Refining & Mining Co. |  5.5 |  8.3
 6 | Pennsylvania Smelting Co. |  6.2 |  7.2
 7 | American Metal Co. |  1.8 |  2.1
 8 | American Zinc, Lead & Smelting Co. |  1.7 |  1.3
 9 | Eagle-Picher Lead Co. |  9.3 |  6.2
10 | Banker Hill & Sullivan Mining & Concentrating Co. |  6.3 |  1.7
11 | Desloge Consolidated Lead Co. |  2.6 |  3.3
| Ontario Smelting Co. |  1.9 |  0.0

American Smelting & Refining Co. благодаря преобладающему объему производства и широкому распределению своих интересов доминирует на внутреннем рынке, хотя ее доля в общем объеме выпуска за последние несколько лет значительно сократилась.

Испания.

—Более 60% чернового свинца, производимого в Испании, поступает с плавильных заводов компании Penarroya (Франция), которая за последние несколько лет поглотила испанские плавильные заводы Escombrera-Bleyberg в Эскомбрере и два плавильных завода Figueroa в Линаресе и Картахене. Это обеспечивает компании Penarroya доминирующее положение в испанской свинцовой промышленности. Английские интересы, E. J. Enthoven & Co., владеют плавильным заводом, производящим около 25 000 коротких тонн свинца ежегодно. Все плавильные компании заключили соглашение о прекращении конкуренции при закупке руды. Испанское правительство взимает пошлину в размере около 1,80 доллара за тонну на экспортируемые свинцовые концентраты.

Австралия.

—Плавильные заводы в Австралии, производящие свинец, имеют мощности, указанные ниже.

Company | Location | 1913 production, short tons pig lead
Broken Hill Associated Smelters | Port Pirie, South Australia |  92,824
Sulphide Corporation | Cockle Creek, New South Wales |  19,660
Total |  | 112,484

The annual capacity of the Port Pirie plant is now 165,000 short tons of pig lead.

Таблица 56.—Заводы по плавке серебряно-свинцовых руд в Мексике

Company
Location
Number of
furnaces
Annual
capacity
tons of
charge

American Smelting & Refining Co. | Monterrey |  7 |  | 410,000
American Smelting & Refining Co. | Aguascalientes |  1 | (lead) | 40,000
American Smelting & Refining Co. | Chihuahua |  7 |  | 400,000
American Smelters Securities Co. | Velardeña |  3 |  | 150,000
Compañia de Minerales y Metales | Cerralvo |  2 |  | 35,000
Compañia de Minerales y Metales | Guadalupe, N. L. |  1 |  | 70,000
Compañia Fundadora y Refinadora de Monterrey (leased to American Metal Co.) | Monterrey |  4 | (or 8?) | 210,000
Compañia Metalurgica Mexicana (Towne) | San Luis Potosi | 10 |  | 250,000
Compañia de Minerales y Metales (reported about to be dismantled) | Torreon |  9 |  | 350,000
Compañia Minera de Peñoles | Mapimi |  6 |  | 350,000
Mazapil Copper Co., Ltd. (English) | Saltillo, Coahuila |  1 |  | 36,000
Total |  | 51 |  | 2,301,000

Мексика.

—Практически все мексиканские плавильные заводы принадлежат американским компаниям и эксплуатируются ими. До войны некоторые из них контролировались германскими интересами через American Metal Co. (зарегистрированную в США), но действия Управляющего имуществом иностранных граждан устранили любой иностранный контроль в этих компаниях, к которым относятся Compañia Minera de Peñoles, Compañia de Minerales y Metales и Compañia Metalurgica de Torreon, оставив под германским контролем только Compañia Fundadora y Refinadora de Monterrey. American Metal Co. обычно контролировала от 60 000 до 75 000 тонн мексиканского свинца, находящегося на таможенном складе, и от 12 000 до 15 000 тонн свинца, выплавленного в Мексике, вместе с более чем тысячей тонн сурьмянистого свинца.

Заводы в Агуаскальентесе и Веларденье являются преимущественно медеплавильными. В Террасасе и Санта-Росалии (штат Чиуауа) имеются небольшие свинцовоплавильные заводы, но они, вероятно, заброшены.

Британские острова.

—Сообщается, что во время войны мощности по плавке свинца в Великобритании были увеличены. До войны большое количество иностранного свинцового слитка из Испании, Бельгии и Германии проходило аффинаж (извлечение серебра) на Британских островах.

Другие страны.

—Плавильные заводы по переработке свинца во Франции избежали разрушения во время войны, находясь вне зоны боевых действий. Мощность завода в Понтибо была значительно увеличена. Все они принадлежат французским владельцам. Самым важным свинцовоплавильным заводом в Италии является завод Societa di Pertusola (Англия), объем производства чернового свинца которого в 1915 году составил 16 625 метрических тонн; другой завод — Societa di Monteponi (Италия) с объемом производства 5 187 тонн. Единственным предприятием по плавке свинца в Греции является Compagnie des Mines de Laurium (Франция).

Единственным важным свинцовоплавильным заводом в Канаде является завод в Трейле, Британская Колумбия, который контролируется канадским правительством. Этот завод включает аффинажный цех, использующий электролитический процесс Беттса.

Единственный свинцовоплавильный завод в Турции контролируется французскими интересами — это завод Société des Mines de Balia-Kara-Aidin в Кара-Айдине. Свинцовоплавильный завод Burma Mines Corporation, Ltd. в Баудвине, Бирма, имеет мощность 22 000 коротких тонн свинца.

В Сибири компания Ridder Mining Co., контролируемая лондонской Irtysh Corporation, построила 165 миль железной дороги, которая вместе с речным транспортом доставляет руду с концессии Риддер и уголь с Экибастузских угольных месторождений на плавильный завод в Ермаке, имеющий мощность 15 000 тонн свинца в год.

Торговые объединения.

—Национальный и даже международный контроль над рынком свинца временами достигался посредством маркетинговых организаций или торговых объединений перерабатывающих заводов, агентств по закупке руды и продаже металлов с перекрестным участием в советах директоров, совместной собственностью и долгосрочными контрактами на руды, концентраты и металлы.

В 1909 году в Париже была сформирована так называемая Свинцовая конвенция, или официально — Международная ассоциация по сбыту. В нее входили германские, испанские и бельгийские производители и агентства по продаже металлов, контролировавшие непосредственно около половины европейского производства. Некоторые компании, формально не входившие в ассоциацию, действовали с ней согласованно. Эта конвенция была возобновлена в 1910 году и снова в 1913 году на три года. В ассоциации доминировали те же интересы, что и в Германском цинковом синдикате — группа Мертона, включавшая Metallgesellschaft, Metallbank и Metallurgische Gesellschaft во Франкфурте и компании Мертона в Лондоне; Beer, Sondheimer & Co., контролировавшая дюжину германских металлургических и химических предприятий, и Aron Hirsch & Sohn в Хальберштадте. Группа Мертона в Лондоне и Франкфурте была торговым агентом ассоциации, а доминирующее «трио» через Australian Metal Co. контролировало свинец, экспортируемый из Австралии в виде металла или концентратов.

В Соединенных Штатах и Мексике весь экспортируемый свинец контролировался American Metal Co., аффилированной с ассоциацией, или American Smelting & Refining Co., действовавшей с ней согласованно. Германское «трио» поддерживало и быстро расширяло и укрепляло свое господство во всем мире через банки, холдинговые компании, связи с синдикатами и картелями, перекрестное участие в советах директоров, совместное владение акциями и покупку полностью или частично рудников и плавильных заводов. Некоторые английские аффинажные заводы были тесно связаны с Конвенцией, и весь свинец, экспортируемый с завода в Порт-Пири, продавался компанией Merton & Co. Ассоциация была способна устанавливать цену на свинец в Европе и тем самым влиять на объем производства и, как утверждалось, манипулировала рынком таким образом, что свинец вне Конвенции контролировался так же эффективно, как и внутри нее. Членство было международным, объединенным корыстными мотивами. То, что самыми сильными и агрессивными интересами были германские граждане, было чисто случайным обстоятельством.

Однако в результате войны производство австралийских свинцовых концентратов и слитков было навсегда выведено из-под германского контроля. Деятельность Управляющего имуществом иностранных граждан была направлена на устранение всех германских интересов в Соединенных Штатах. Большая часть производства свинцовых слитков в Австралии в настоящее время реализуется компанией Broken Hill Associated Smelters, Prop., Ltd., в акционерном капитале которой Broken Hill Proprietary владеет одной третью, а Broken Hill South, Broken Hill North и Zinc Corporation — по две девятых каждая. Завод этой компании в настоящее время является крупнейшим плавильным заводом в мире.

Националистическое движение во Франции привело к формированию торговых ассоциаций, известных как «консорциумы», включающих основного участника в каждой отрасли. Эти «консорциумы» были признаны правительством, и каждый из них стал фактически арбитром в своей конкретной области. Консорциум минеральной промышленности был доведен до совершенства в виде Société Minerais et Metaux, бульвар Осман, 154, Париж. В официальном объявлении говорится, что это общество организовано под эгидой французского правительства с целью объединения французских производителей металлов, работающих как внутри страны, так и за рубежом, в кооперативную ассоциацию для закупки и продажи металлургической продукции.

Участники включают основные компании во Франции, производящие или рафинирующие металлы, а также горнодобывающие и плавильные компании, контролируемые французским капиталом в Испании, Алжире, Тунисе и других зарубежных странах. Таким образом, достигается высокоцентрализованная организация той части минеральной и металлургической промышленности, которая находится под французским контролем, для взаимной защиты и преимуществ в конкуренции с другими национальностями. Члены этой организации будут производить большую часть руды в Алжире и Тунисе и, вероятно, 75% испанских свинцовых слитков. Текущий годовой объем производства участвующих компаний составляет около 200 000 метрических тонн свинца, 50 000 метрических тонн цинка и 40 000 тонн меди, помимо железа, сурьмы, платины и т. д. Ассоциация включает следующие компании: Société Minière et Metallurgique de Penarroya; Société d’Affinage de Metaux; Compagnie des Mines d’Ain-Barbar; Association Minière; Société des Mines de Zinc d’Ain-Arko; Compagnie du Boleo; Compagnie Française des Mines de Bor; Corocoro United Copper Mines, Ltd.; Société des Mines de Fedj-el-Adoum; Société des Mines de Zinc de Guergour; Compagnie des Mines de Huaron; Société Minière du Kanguet; Compagnie des Minerais de Fer Magnetique de Mokta-et-Hadid; Comptoir Lyon Allemand; Société Anonyme des Mines de Malfidano; Compagnie des Mines d’Ouasta et de Desloula; Société des Mines de Parzan; Compagnie Industrielle du Platine; Société Anonyme des Mines et Fonderies de Pontgibaud; Société des Mines d’Antimoine de Rochetrejoux; Société des Anciens Etablissements Sopwith; Société Française d’Etudes et d’Enterprises; Société des Mines du Djebel-Ressas; Société Anonyme Française du Djebel-Hallouf; Société Anonyme des Mines et Usines de Peyrebrune; и Compagnie La Cruz.

Одним из результатов войны стало стимулирование кооперативных предприятий между британскими компаниями, причем это движение поощрялось правительством, которое в некоторых случаях участвовало финансово. Компания British Australian Lead Manufacturers Proprietary, Ltd. была сформирована как консолидация австралийских интересов британских фирм с целью создания индустрии белил в этой стране. В число участников входят: Alexander Ferguson & Co.; Cookson & Co.; Foster, Blockett & Wilson; Locke, Blockett & Co.; Locke-Lancaster; W. W. & R. Johnson & Sons, Ltd.; Mersey White Lead Co., Ltd.; и Walkers Parker & Co.

Синдикат Chloride, включающий Zinc Corporation, Ltd., Burma Mines Corporation и Swansea Vale Smelter, Ltd., проводит экспериментальные работы по процессу Ганлина с целью его совершенствования.

Ричард Тилден Смит, приобретя контрольные пакеты акций в J. H. Enthoven & Sons, Locke-Lancaster, Walkers Parker & Co. и одну треть доли в Burma Mines Corporation, стал сильным связующим звеном между этими важными компаниями и таким образом добился договоренности с Имперским правительством о финансовой помощи новому заводу National Smelting Co., Ltd. в Эйвонмуте в размере 500 000 фунтов стерлингов из общей оценочной стоимости в 750 000 фунтов стерлингов, причем правительство было особенно заинтересовано в производстве побочного продукта — кислоты. National Smelting Co. согласилась принимать 25 000 тонн концентрата Broken Hill ежегодно и не плавить иностранную руду без разрешения правительства. Enthoven & Sons контролируют через владение продукцию одного из испанских плавильных заводов, а через контракты на аффинаж и сбыт — продукцию французской компании Laurium в Греции. Попытка добиться более тесного объединения всех вышеупомянутых английских и австралийских компаний не удалась.

Сообщается, что в 1917 году Vivian, Younger & Bond и Morgan, Grenfeld & Co. сыграли важную роль в создании «Металлического банка» в Лондоне. Говорили, что Broken Hill Associated Smelters Prop. Ltd. и компания Penarroya согласились продавать свою продукцию через этот банк, но вполне вероятно, что эта договоренность так и не была реализована. В Лондоне был сформирован Химико-металлургический банк, среди акционеров которого — Ричард Тилден Смит. Его предполагаемая сфера деятельности не ясна, но он, вероятно, будет стремиться влиять на контроль над свинцом в Соединенном Королевстве.

В 1918 году компаниями Vivian, Younger & Bond, Chas. Tennant Sons & Co., Cookson & Co., British Aluminum Co., Morgan, Grenfeld & Co. и крупными акционерами Rio Tinto Co. была сформирована British Metals Corporation с капиталом 5 000 000 фунтов стерлингов. Имперское казначейство будет представлено в совете директоров. Цели заключаются в финансировании британских компаний по производству цветных металлов, объединении всего производства этих металлов в пределах империи под эгидой одной маркетинговой организации и сохранении британского контроля. Если планы будут успешно реализованы, плавка как в Англии, так и на континенте Европы, если туда будут направляться какие-либо британские концентраты, будет практически осуществляться на давальческих началах, при этом металл останется под контролем Metals Corporation или аффилированного банка.

ПОЛОЖЕНИЕ ВЕЛИКИХ ДЕРЖАВ

В прилагаемой таблице представлены имеющиеся статистические данные о производстве с 1913 года, чтобы показать степень контроля над промышленностью в каждой стране со стороны внутреннего или иностранного капитала, а также предпринята попытка показать степень коммерческого контроля со стороны каждой из великих держав. Такая статистика в лучшем случае является лишь приблизительной; контроль меняется из года в год, а данные трудно получить и проверить.

Таблица 57.—Коммерческий контроль над мировым производством чернового свинца

Country
Recent
pig-lead
production
(short tons)
Year
Per cent.
of
world
Financial control by

Home capital | United States | Great Britain | France | Germany
United States | 612,200 | 1917 |  44.6 | ... | 612,200 |  |  |
Australia | 127,800 | 1913 |   9.4 | ... | ... | 127,800 |  |
British Isles | 12,600 | 1916 |   0.9 | ... | ... | 12,600 |  |
Canada | 20,400 | 1916 |   1.5 | ... | ... | 20,400 |  |
Burma | 20,000 | 1917 |   1.5 | ... | ... | 20,000 |  |
France | 30,800 | 1913 |   2.2 | ... | ... | ... | 30,800 |
Italy | 24,000 | ... |   1.8 | 5,700 | ... | 18,300 |  |
Belgium | 39,400 | 1913 |   2.9 | 15,000 | ... | ... | 24,400 |
Venezuela | 200 | 1917 | ... | ... | ... | ... | ... | 200
Bolivia | 2,400 | 1917 |   0.2 | 400 | ... | ... | 2,000 |
Greece | 12,800 | 1916 |   0.9 | ... | ... | ... | 12,800 |
Japan | 12,300 | 1916 |   0.9 | 12,300 |  |  |  |
Peru | 3,000 | 1917 |   0.2 | 500 | 500 | 2,000 |  |
Russia | 1,100 | 1913 |   0.1 | 1,100 |  |  |  |
Chile | 6,000 | 1917 |   0.4 | 3,000 | ... | 1,000 | ... | 2,000
Mexico | 61,200 | 1913 |   4.4 | ... | 53,200 | 8,000 |  |
Spain | 157,000 | 1917 |  11.4 | 20,000 | ... | 25,000 | 105,000 | 7,000
Sweden | 2,100 | 1915 |   0.1 | 1,100 | ... | ... | ... | 1,000
Germany | 200,000 | 1913 |  14.5 | ... | ... | ... | ... | 200,000
Austria-Hungary | 26,600 | 1913 |   1.9 | 26,600 |  |  |  |
Total | 1,371,900 | ... | 100.0 |  | 665,900 | 235,100 | 175,000 | 210,200
Per cent. of world production. |  |  | 100.0 |  | 48.6 | 17.2 | 12.7 | 16.3

Соединенные Штаты.

—Во время войны Соединенные Штаты продемонстрировали, что их месторождения свинцовых руд способны обеспечить производство, значительно превышающее нормальный уровень. То, что рост не был больше, объясняется главным образом недостаточным стимулом в рыночной цене на свинец, которая не достигла ранней инфляции многих других металлов; а позже, когда цена стала приемлемой, производство было ограничено нехваткой мощностей по рафинированию. Существующие мощности временами не использовались полностью из-за перегруженности железнодорожного транспорта. Месторождения свинцовых руд в Соединенных Штатах имеют большие возможности, но, за исключением вкрапленных свинцовых руд юго-восточного Миссури, разведанные запасы руды обеспечат производство лишь на несколько лет. Контроль над рудниками в Соединенных Штатах возложен почти исключительно на американцев или американские компании, некоторые из которых, однако, имеют иностранных акционеров, главным образом британских или канадских.

Соединенные Штаты импортируют свинцовые руды в объеме небольшого процента от своего общего производства из Мексики, Канады, Южной Америки и Африки. Мексиканская руда в значительной степени импортируется для удовлетворения особых потребностей свинцовоплавильного завода в Эль-Пасо, а не из-за нехватки плавильных мощностей в Мексике. Плавильные мощности Соединенных Штатов всегда превышали фактическую добычу руды и в настоящее время значительно превышают нормальный уровень производства. Владение большинством важных плавильных заводов всегда принадлежало американскому капиталу, и в результате деятельности Управляющего имуществом иностранных граждан все они в настоящее время принадлежат гражданам США и контролируются ими. Значительное количество свинцовых слитков импортируется, главным образом из Мексики, для рафинирования. Большая часть этого объема реэкспортируется. Американский капитал через владение плавильными заводами контролирует большую часть чернового свинца, производимого в Мексике и Перу. Импорт руды и слитков для рафинирования из Канады ограничен правительственной премией на свинец, выплавленный и рафинированный в Канаде. Американский капитал также контролирует значительный процент рудников Мексики и имеет некоторую долю в Burma Mines Corporation и Irtysh Corporation.

Несмотря на расширенные плавильные мощности и возможности производства на американских рудниках, не ожидается, что после периода адаптации после Первой мировой войны будет значительный экспорт отечественного свинца.

Британская империя.

—Страны Британской империи в порядке значимости их производства свинца в 1913 году: Австралия, Британские острова, Канада, Бирма и Египет.

Британский капитал контролирует рудники и плавильные заводы на Британских островах, в Канаде, Австралии, Бирме и на Алтае в Сибири, а также, благодаря владению рудниками и плавильными заводами, около 25 000 тонн свинца ежегодно из Испании и более 70% производства Италии. Благодаря контрактам на аффинаж и сбыт он контролировал большую часть испанской продукции и часть производства Греции. Сообщается также, что он контролирует небольшие объемы руды из Перу и Чили. Ввиду недавнего увеличения мощностей по рафинированию в Испании компанией Penarroya (Франция) и организации всех французских интересов в Société Minerais et Metaux, будущий контроль английского капитала над испанской продукцией сверх 25 000 тонн, производимых английским заводом, сомнителен, хотя сообщалось, что компания Penarroya согласилась продавать свой свинец через новый Металлический банк Лондона. До войны большое количество чернового свинца из Испании, Бельгии и Германии импортировалось, проходило аффинаж и в значительной части реэкспортировалось.

Добыча руды в Британской империи примерно на 25% превышает ее потребление, но недостаточные плавильные мощности вызвали зависимость от свинца, выплавленного за рубежом. Плавильные мощности были увеличены, и дополнительные планируемые мощности сделают общий объем равным потреблению. Империя может стать независимой от остального мира, если будет принята политика «имперских преференций».

Все крупные интересы в свинцовой промышленности Британской империи в период войны проявили сильную тенденцию к сотрудничеству и организации для взаимной защиты и выгоды. Кульминацией этого движения, по-видимому, является формирование British Metals Corporation, призванной сосредоточить маркетинговый контроль над производством всей Британской империи в одной организации под эгидой правительства.

Австралия.

—Австралийское производство свинцовой руды и концентратов, получаемых главным образом из Нового Южного Уэльса, ставит Австралию на второе место в мировом производстве свинцовых руд. В 1913 году немногим более половины продукции экспортировалось в Европу для плавки, остальная часть плавилась в Кокл-Крик и Порт-Пири. Произведенный черновой свинец, за вычетом небольшого местного потребления, также экспортировался.

Австралийские рудники всегда принадлежали британскому и австралийскому капиталу. До войны сбыт концентратов и всех экспортируемых свинцовых слитков контролировался Australian Metal Co., аффилированной с германским металлургическим «трио» во главе с Metallgesellschaft. Однако во время войны правительства Великобритании и Австралии аннулировали долгосрочные контракты на закупку руды и металлов, и производители руды и плавильные заводы организовались для взаимной защиты и сохранения промышленности навсегда под исключительным британским контролем. Мощность перерабатывающих заводов в Порт-Пири была увеличена за счет капитала, внесенного совместно основными горнодобывающими компаниями, и этот завод в настоящее время является крупнейшим свинцовоплавильным заводом в мире.

Британские острова.

—Небольшой объем добычи свинцовой руды в Великобритании получается из нескольких разрозненных месторождений, не имеющих большого значения. Некоторое количество руды импортируется и плавится вместе с продукцией отечественной добычи. Потребление на Британских островах настолько велико, что необходим очень большой импорт чернового свинца, составляющий 14% мирового производства. Все рудники и плавильные заводы на Британских островах, насколько известно, принадлежат британскому капиталу и контролируются им.

Канада.

—Благодаря помощи канадского правительства в виде премий, плавильный завод в Трейле прочно утвердился и является единственным важным производителем свинца в Канаде. Он перерабатывает большую часть руд Британской Колумбии, которые в противном случае пришлось бы отправлять на переработку в Соединенные Штаты. Однако канадское потребление примерно на одну треть превышает производство.

Бирма.

—Хотя производство руды и чернового свинца в Северных Шанских штатах компанией Burma Mines Corporation в 1913 году составляло незначительную часть мирового производства, компания развила свои месторождения так, что стала способна на гораздо больший выход, который в ближайшем будущем может составить 75 000 тонн ежегодно. Эта компания контролируется британским, вероятно, с некоторой долей американского капитала.

Египет.

—Небольшой объем добычи руды в Египте экспортируется для плавки и контролируется французским капиталом.

Германия.

—Германия, крупный производитель свинцовых руд, в 1913 году импортировала для плавки почти 10% мирового производства и, кроме того, импортировала значительное количество чернового свинца, являясь вторым по величине потребителем свинца в мире. Если Германия потеряет Верхнюю Силезию, которая производила почти половину отечественных руд, она станет еще более зависимой от импорта для снабжения своих плавильных заводов. До войны германская свинцовая промышленность была тесно организована, причем большая часть добычи и плавки свинца осуществлялась департаментами правительств земель, хотя некоторые из крупнейших предприятий были частными корпорациями. Германское металлургическое «трио» во главе с Metallgesellschaft через Международную ассоциацию по сбыту контролировало непосредственно около половины европейского производства, включая в эту так называемую Свинцовую конвенцию, помимо германских предприятий, большинство испанских и бельгийских производителей, большую часть свинца, экспортируемого из Соединенных Штатов и Мексики, а также черновой свинец и концентраты, экспортируемые из Австралии. Эта система контроля за пределами Германии в настоящее время навсегда разрушена, и масштабы и организация германской свинцовой промышленности в ближайшем будущем не могут быть предсказаны.

Франция.

—Во Франции добыча свинцовой руды невелика и контролируется, за одним возможным исключением, французским капиталом. Некоторые руды импортируются для плавки, причем Тунис и Алжир способны поставлять даже больше. Чтобы обеспечить большое потребление (Франция занимает четвертое место среди стран-потребителей свинца), импортируется в виде чернового свинца около 7% мирового производства. Недавно плавильные мощности были увеличены. Французский капитал контролирует более половины производства Бельгии через владение плавильными заводами, а через владение рудниками и плавильными заводами контролирует более половины производства Испании и большую часть, если не всю, продукцию Греции. Он также контролирует добычу руды в Египте и большую часть руд, добываемых в Алжире и Тунисе. Под эгидой правительства недавно была осуществлена сильная организация всех металлопроизводящих компаний, контролируемых французским капиталом во Франции и зарубежных странах, под названием Société Minerais et Metaux, которая контролирует продажу всей продукции своих членов, а также выступает в качестве закупочного агента для них.

Бельгия.

—Бельгия не производит руд, но выплавляет около 4,5% мирового производства, почти весь объем которого потребляется внутри ее границ. Чуть менее половины этого производства контролируется бельгийским капиталом, остальная часть — французскими интересами. Бельгийский капитал также в незначительной степени представлен в Испании, Алжире, на Кавказе и в Тунисе. Считается, что часть австралийских концентратов может быть выделена Бельгии для плавки.

Италия.

—Итальянская добыча руды, составляющая около 2% мирового объема, плавится в этой стране. Продукт потребляется вместе с примерно 50% дополнительного объема, импортируемого в виде чернового свинца. Более трех четвертей отечественной продукции контролируется английским капиталом; почти вся остальная часть контролируется итальянским капиталом, но другие английские, французские и бельгийские компании производят незначительные количества руды.

Австро-Венгрия.

—Австро-Венгерская империя в 1913 году производила и плавила руды в объеме около 2% мирового производства и потребляла это количество вместе с примерно 50% дополнительного металла, импортируемого в виде чернового свинца. Несколько районов добычи свинца и плавильных заводов, некоторые из которых принадлежат государствам Австрии и Венгрии, с разделом империи попадают под три или более различных политических юрисдикций, производство свинца ни в одной из которых не будет иметь значения. Один из важных свинцовоплавильных заводов находится в Фиуме.

Испания.

—Испания занимает третье место по содержанию добываемых руд и второе место по производству на плавильных заводах. Поскольку внутреннее потребление незначительно, весь свинец экспортируется. До войны большая часть продукции направлялась в Англию для аффинажа. Однако во время войны мощности по рафинированию в Испании были значительно увеличены, и теперь кажется вероятным, что любой серебряно-свинцовый продукт, который не могут переработать отечественные заводы, будет отправляться во Францию для аффинажа. Более половины испанского производства контролируется французским капиталом, и в меньшей степени — бельгийскими и германскими интересами.

Япония.

—Ресурсы свинцовой руды в Японии скудны. Объем добычи свинцовой руды и производства чернового свинца в 1913 году составлял около 25% внутреннего потребления. С тех пор руды и концентраты импортировались из Китая, Формозы, Кореи, Сибири и Австралии, но импорт чернового свинца все еще оставался необходимым. Японцы стремятся обеспечить контроль над месторождениями руды в Китае и Сибири и поставлять сырье для увеличения своих внутренних плавильных и производственных мощностей. Однако вероятно, что Япония еще много лет будет зависеть от импорта из других источников для получения большей части потребляемого свинца.

РЕЗЮМЕ

Основные виды использования свинца — в виде металла и в форме белил или основного карбоната, в качестве пигмента. Металлический свинец используется для водопроводных труб, оболочек электрических кабелей, футеровки кислотных камер и чанов, а также для изготовления дроби, пуль и шрапнели. Сплавы с различными другими металлами используются в типографском деле, подшипниках и предохранителях. Красные и оранжевые оксиды используются в качестве пигментов. Крупнейшим отдельным видом потребления являются свинцовые белила.

Свинцовые и цинковые руды обычно встречаются вместе и широко распространены по всему миру. Галенит является основным свинцовым минералом, другие рудные минералы, церуссит и англезит, образуются из него в результате окисления. Галенит — устойчивый минерал, встречающийся почти во всех типах месторождений руд. Страны, производящие больше всего руды, в порядке значимости: Соединенные Штаты, Австралия, Испания, Германия и Мексика. Районы первостепенной важности: Брокен-Хилл, Новый Южный Уэльс; юго-восточная Испания; юго-восточный Миссури; и Кер-д’Ален, Айдахо.

Разработки в области селективной масляной флотации, с помощью которой вредное содержание цинка удаляется из комплексных руд и превращается в актив, представляют собой величайшее недавнее достижение в обогащении свинцовых руд. Электролитическое рафинирование — величайшее недавнее достижение в металлургии свинца.

Легкость, с которой свинец восстанавливается из своих руд, и его полезность в качестве собирателя драгоценных металлов при плавке привели к широкому распространению перерабатывающих заводов. Тем не менее, большой процент мирового объема добычи руд транспортируется из стран происхождения в другие страны для переработки вблизи рынка и там, где квалифицированная рабочая сила и топливо более обильны и дешевы.

Страны с наибольшим производством на плавильных заводах: Соединенные Штаты, Испания, Германия и Австралия; страны с гораздо меньшим значением: Мексика, Бельгия, Великобритания, Франция, Австро-Венгрия, Италия, Греция, Канада и, недавно, Бирма. Другие страны имеют малое значение.

Страны с основным потреблением: Соединенные Штаты, Германия, Великобритания и Франция. Соединенные Штаты производят свинец для собственных нужд, но остальные три страны импортируют руды для плавки, а также черновой свинец в больших количествах. Австралия и северная Африка поставляли основную часть руд, а Испания, Австралия и Мексика — большую часть чернового свинца. Это ситуация в конечном анализе, фактическое движение торговли, конечно, гораздо сложнее.

Политический контроль над мировым производством свинца, в пересчете на содержание свинца в рудах, в 1913 году был следующим: Соединенные Штаты — 36,0%; Британская империя — 23,9%; Испания — 6,4%; Германия — 5,9%; Мексика — 5,1%; и Франция — 4,0%. Таким образом, три державы контролируют 76% производства.

Владение рудниками важно главным образом как фактор, определяющий распределение руд по плавильным заводам. Контракты на закупку руды могут изменить или аннулировать эффект политической юрисдикции и владения рудниками. Владение или контроль над перерабатывающими заводами были наиболее эффективной основой для коммерческого контроля над отраслью. В Соединенных Штатах American Smelting & Refining Co. доминирует на рынке, но контролирует непосредственно только одну треть продукции. В Испании французская компания Penarroya контролирует более половины производства. В Германии «трио» во главе с Metallgesellschaft контролировало внутреннюю промышленность до войны и через «Свинцовую конвенцию» распространило свое господство на половину европейского производства и большую часть экспорта Австралии, Мексики и Соединенных Штатов. Этот контроль, однако, никогда не был абсолютным. В Австралии в настоящее время Broken Hill Associated Smelters контролирует сбыт большей части экспортируемого чернового свинца.

Совместный политический и коммерческий контроль был установлен в Британской империи и Франции. Во время войны политическая юрисдикция довольно широко использовалась для изменения или устранения коммерческого контроля, особенно в отношении интересов враждебных иностранных граждан.

Различные объединения британских компаний для обеспечения британского контроля над ресурсами империи, особенно Австралии и Бирмы, завершились формированием British Metals Corporation для продажи продукции. Представитель Имперского казначейства будет в совете директоров, и либо Металлический банк Лондона, либо Химико-металлургический банк могут финансировать его деятельность, если только он не поглотит их функции. Эта организация, несомненно, призвана занять место Metallgesellschaft как доминирующего фактора в свинцовой промышленности мира. Она будет иметь большое влияние, так как британский капитал контролирует все производство Британских островов, Австралии, Бирмы, Канады и, как правило, Сибири, большую часть производства Италии, часть производства Испании и Мексики и, возможно, Греции. Вероятно, Британские острова в будущем не будут проводить аффинаж такого количества иностранного свинца, как раньше, поэтому важность этой основы коммерческого контроля будет значительно снижена.

Société Minerais et Metaux, включающая всех производителей, контролируемых французским капиталом, под эгидой правительства является агентом по продаже и закупке для своих членов и контролирует все французское и большую часть греческого производства, более половины производства Испании и Бельгии, помимо руд северной Африки и Египта.

После устранения активов враждебных иностранных граждан Управляющим имуществом иностранных граждан американский капитал контролирует практически все внутреннее производство и почти все производство Мексики, помимо некоторых руд, импортируемых из Мексики, Канады и Южной Америки. Несмотря на большие запасы руды и перерабатывающие мощности, ожидается, что Соединенные Штаты после периода адаптации будут обеспечивать свои внутренние потребности, но экспортировать мало свинца, как это было до войны.

Положение Германии будет в значительной степени зависеть от договоренностей о поставках иностранной руды. Некоторая часть добычи мексиканской руды может все еще находиться под германским контролем. Бельгия полностью зависит от иностранной руды, которая, по-видимому, будет в значительной степени поступать из Австралии; и, поскольку более половины ее производства контролируется французским капиталом, она будет находиться под британским и французским господством; но она потребляет большую часть продукции своих плавильных заводов. Италия потребляет на 50% больше, чем составляет внутреннее производство, которое в основном контролируется английским капиталом. Ни одно из государств, образованных в результате распада Австро-Венгерской империи, не будет иметь значения в свинцовой промышленности.

Коммерческий контроль над производством свинца на плавильных заводах, рассчитанный по последним имеющимся статистическим данным, составляет примерно следующее: Соединенные Штаты — 48,6%; Британская империя — 17,2%; Германия — 15,3%; и Франция — 12,7%; или всего для четырех держав — 93,8% мирового производства чернового свинца.

ГЛАВА XVI ЦИНК Фредерик Б. Хайдер

ИСПОЛЬЗОВАНИЕ ЦИНКА

Металлический цинк, или спельтер, как часто называют этот коммерческий металл в торговле, главным образом используется в виде катаных листов; при гальванизации; в сплавах, образующих латунь и бронзу; и при аффинаже (извлечении серебра) из свинцовых слитков. Катаные листы используются для крыш, резервуаров, трубопроводов и защитных футеровок. Железные и стальные предметы погружаются в ванны с расплавленным спельтером и покрываются металлом или оцинковываются, тем самым защищаясь от окисляющих агентов. Используются и другие методы нанесения этого защитного покрытия.

Цинк и медь соединяются во всех пропорциях, образуя сплавы, известные как латунь, которые имеют широкое промышленное применение. Существует только один определенный сплав; он соответствует приблизительно CuZn2, содержит 33% меди и 67% цинка, является твердым, хрупким и имеет небольшую практическую ценность. Все остальные латуни можно рассматривать как твердые растворы этого определенного сплава в избытке одного из его компонентов. Используемые латуни варьируются по содержанию цинка от 20 до 85% и сильно различаются по своим свойствам в зависимости от состава. Сплавы цинка и алюминия обладают ценными свойствами, особенно те, которые содержат от 25 до 35% цинка. Другие используемые сплавы содержат, помимо меди и цинка, свинец, олово или никель.

Процесс Паркса по аффинажу свинцовых слитков вытеснил более старые процессы Паттинсона и купелирования, за исключением случаев присутствия висмута, благодаря жадности, с которой цинк извлекает из слитков золото, серебро, медь и теллур. Эта очистка может быть доведена до желаемой степени или только до коммерчески выгодного уровня, обычно до содержания половины унции серебра на тонну свинца.

Среди прочих видов использования цинка: декоративное литье; в гальванических элементах; в фотогравировке; в пластинах, подвешиваемых в котлах для предотвращения образования накипи; осаждение золота в цианидном процессе; в виде порошка, как восстановитель в органической химии, особенно при восстановлении индиго-синего, и в краске для конструкционной стали. Цинк также используется в виде многочисленных солей, таких как хлорид в качестве консерванта для древесины, и сульфат, применяемый в медицине, крашении и производстве клея.

Оксид цинка, производимый как из металла, так и из руд, используется в качестве пигмента как в сочетании со свинцовыми белилами и баритом, так и в качестве их конкурента. Значительные количества оксида также используются в резинотехнической промышленности. Литопон (интимная смесь, полученная путем химического осаждения сульфида цинка и сульфата бария) приобретает все большее значение в качестве пигмента.

Все основные виды использования цинка, включая гальванизацию, катаные листы, производство латуни и аффинаж свинцовых слитков, можно считать важными. Латунь относится вместе со сталью к категории незаменимых материалов современной промышленности. Никакой удовлетворительной замены с точки зрения как физических качеств, так и стоимости не существует для многих важных частей механизмов и производственных целей. Его широкое использование зависит от ряда качеств. Отличные четкие отливки, изготовленные из определенных латуней, легко поддаются механической обработке или другой отделке и гальваническому покрытию, если это необходимо. Электропроводность латуни хорошая. Некоторые латуни легко прокатываются в листы и нарезаются и штампуются в желаемые формы. Смазанные поверхности стали по латуни образуют удовлетворительные и долговечные подшипники.

Другие крупные виды использования цинка зависят от его устойчивости к окислению и возможности прокатки в довольно тонкие листы. Однако по обоим этим качествам он уступает другим металлам, в частности никелю и олову. В сплаве со свинцом он может быть прокаткой превращен в заменитель оловянной фольги. В некоторых случаях это довольно удовлетворительный, дешевый заменитель металлов более высокого качества. Во времена дефицита или высоких цен возможна замена металлами более низкого качества, и во многих случаях от цинка можно временно отказаться вовсе. Его область применения, следовательно, в значительной степени определяется коммерческими условиями предложения и цены, которые в широком смысле определяют общее потребление и особенно проценты, приходящиеся на различные виды использования. Можно предположить, однако, что проценты для внутреннего потребления в Соединенных Штатах в 1910 году приблизительно представляют собой показатели нормального мирного времени. В том году из общего объема потребления 60% использовалось при гальванизации; 20% — при производстве латуни; 11% — в катаных листах; и 1% — при аффинаже свинца; оставляя 8% для прочих видов использования. Во время войны процент, используемый при гальванизации, был значительно снижен, а используемый для производства латуни — значительно увеличен. Использование катаных листов будет расти.

Большая часть европейского производства в нормальное время прокатывается в листы, используемые главным образом для кровли.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

При извлечении цинка из его руд наиболее важными изменениями в практике за последние годы стали адаптация ретортной плавки с целью использования цинковых концентратов из комплексных руд, увеличение производства оксида цинка и литопона за счет применения методов волатилизации при переработке ретортных остатков и рядовых руд, а также электролитические и электротермические процессы извлечения металла.

Наиболее революционным достижением стала разработка методов масляной флотации, электромагнитной и электростатической сепарации для обогащения руд. Эти процессы получают широкое распространение и в сочетании с электролитическим восстановлением особенно хорошо приспособлены для производства цинка высочайшего качества из комплексных руд. Поскольку электролитические и электротермические процессы находят применение только там, где электроэнергия относительно дешева, существует тенденция размещать установки в местах доступности гидроэлектроэнергии, что приводит к перераспределению центров плавки цинка.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Цинк и свинец обычно встречаются вместе в месторождениях полезных ископаемых, иногда в тесной смеси, иногда в такой степени обособленно, что преобладает один из металлов, однако руды одного из них редко бывают полностью свободны от примесей другого. Геологическое и географическое распространение этих двух металлов, следовательно, почти идентично.

Сульфидные руды, главным образом сфалерит или цинковая обманка, являются наиболее важными, но в зоне окисления они часто превращаются в карбонаты — смитсонит, каламин и гидроцинкит. Оксиды — франклинит, виллемит и цинкит — имеют значение только в одном районе штата Нью-Джерси. Карбонаты, хотя и содержат низкий процент цинка, часто встречаются в виде концентрированных рудных тел и легко поддаются металлургической обработке. Поэтому каламин-смитсонитовые руды составляют значительную долю добычи во многих важных районах, но в будущем цинковая обманка будет приобретать все большее значение в мировом производстве.

Цинковые руды встречаются в месторождениях нескольких различных генетических типов. В порядке их значимости это:

(а) Месторождения, сформировавшиеся в осадочных породах без видимой связи с изверженными породами, в виде пластовых залежей, замещающих обычно известняки и доломиты. Руды этого типа обычно содержат минералы свинца (галенит) и железа (пирит или марказит), часто марганца и кадмия, иногда мышьяка, кобальта и никеля, но редко золото, серебро, медь или сурьму. Иногда присутствуют барит и флюорит.

Месторождения этого типа имеют повсеместное распространение. Их большая чистота и простота необходимой обработки, особенно руд в зонах окисления, привели к тому, что они стали эксплуатироваться первыми и наиболее интенсивно и до недавнего времени являлись доминирующим фактором в мировом производстве цинка. К этому типу относятся месторождения долины Миссисипи и Силезии, которые в совокупности обеспечили 34 процента мирового объема добычи в 1913 году.

(b) Жилы, связанные с изверженными породами, и вкрапленные сульфидные замещения в изверженных породах. К этой группе относятся месторождения Бьютта, Ледвилла и Кер-д'Ален, а также вкрапленные месторождения Бодуин (Burma Mines Co.), Риддер (Сибирь) и Салмон-Ривер (Британская Колумбия). Эти руды обычно являются комплексными и включают минералы цинка, свинца, меди, железа, золота и серебра, а часто также мышьяка, сурьмы и других металлов. В одной группе, серебряно-свинцовых месторождениях, цинк кажется второстепенным фактором, но с глубиной он замещает свинец в качестве преобладающего металла. Месторождения этих комплексных руд в последние годы стали важными источниками цинка благодаря выявлению цинковых руд в зонах окисления, тому, что цинк становится доминирующим металлом с увеличением глубины на многих рудниках, и особенно благодаря совершенствованию методов обогащения комплексных руд и извлечения металла из концентратов. Руды этого типа будут приобретать все большее значение в будущем из-за их повсеместного распространения.

(c) Магматогенно-метаморфические месторождения, содержащие франклинит, виллемит, цинкит, немного цинковой обманки и жильную массу из кальцита, родонита, граната, пироксена, роговой обманки, магнетита и тремолита. Этот тип характерен для месторождений Франклина и Адирондака в северо-восточной металлогенической провинции Соединенных Штатов, а также встречается в Магдалене и Хановере, штат Нью-Мексико, и на руднике Хорн-Силвер в Юте.

(d) Метаморфизованные месторождения. Первоначально они могли относиться к любому из предыдущих типов, но в настоящее время изменены региональным метаморфизмом. Лучшим примером является важное месторождение Аммеберг в Швеции. Цинковая обманка там встречается в виде вкрапленности в полосах гнейсовидного гранулита, который также содержит полосы вкрапленного пирротина и арсенопирита.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Основные месторождения цинковых руд в мире находятся в странах, перечисленных в таблице ниже; порядок стран соответствует их значимости в отрасли в 1913 году, насколько это можно оценить по неполным данным.

Тремя основными металлогеническими провинциями мира, согласно текущей эксплуатации, являются Брокен-Хилл (Новый Южный Уэльс), Силезия и долина Миссисипи.

Состояние цинковой промышленности в основных странах в 1913 году показано в Таблице 59.

Соединенные Штаты.

— Цинковые месторождения Соединенных Штатов могут быть отнесены к трем металлогеническим провинциям, которые в порядке их текущей значимости представляют собой: провинцию долины Миссисипи, Западную провинцию и Северо-Восточную провинцию.

Судя по имеющимся знаниям, провинция долины Миссисипи является одной из трех крупнейших цинконосных металлогенических провинций мира. Она занимает территорию, подстилаемую слабо дислоцированными палеозойскими известняками, возраст которых варьируется от ордовикского до нижнекарбонового, и охватывает большую часть великой межконтинентальной долины Миссисипи в штатах Миссури, Арканзас, Оклахома, Канзас, Иллинойс, Кентукки, Висконсин, Айова, а также Теннесси и западную часть Виргинии. Изверженные породы, как правило, отсутствуют. Существуют три основные подпровинции: Озаркская провинция, включающая Миссури, Оклахому, Канзас, Арканзас; верхняя часть долины Миссисипи, включающая Висконсин, северную часть Иллинойса и Айову; а также районы Теннесси и Виргинии.

Таблица 58. — Основные месторождения цинковых руд мира

Approximate
order
Country
Percentage
of world’s
production
in 1913

 1 | United States | 35.0
 2 | Germany | 25.0
 3 | Australia | 15.0
 4 | Italy |  5.0
 5 | Algeria |  3.0
 6 | Japan |  2.0
 7 | Spain |  2.0
 8 | Russia (including Russian Poland) |  2.0
 9 | France |  1.5
10 | Greece |  1.0
11 | Sweden |  1.0
12 | Mexico |  1.0
13 | Austria |  1.0
14 | Tunis |  1.0
15 | Indo-China (Tonkin) |
16 | Great Britain |
17 | China |
18 | Bolivia |
19 | Canada |
20 | India (Burma) |
21 | Egypt |
22 | South Africa |
23 | Peru |

В Озаркской подпровинции наиболее важным является район Джоплин. Руды залегают на трех горизонтах в горизонтально залегающих нижнекарбоновых известняках. В верхнем горизонте, под поверхностью, руда залегает в глинистых кремнистых брекчиях, и преобладает галенит. Средний горизонт, или «пластовая залежь», содержит смесь галенита и цинковой обманки, цементирующую брекчированный кремень. Руда низкосортная, средний выход цинка составляет 1,9 процента. Этот горизонт был наиболее важным источником руды. Третий и самый нижний горизонт, пока еще мало эксплуатируемый, содержит вкрапленные руды. В 1918 году в районе Джоплин работало тридцать обогатительных фабрик. Компания Athletic Mining & Smelting Co. была крупнейшим производителем, эксплуатирующим рудник Athletic в Дуэнвеге, Bertha A. в Уэбб-Сити и Mutual в Ороного. Крупными операторами являются Miami Zinc Syndicate, связанный с Butte & Superior и American Zinc, Lead & Smelting Co.; Commerce Mining & Royalty Co.; Century Zinc Co.; и Tri-State Mining Co. Значительная часть добычи осуществляется арендаторами и мелкими операторами.

Таблица 59. — Цинковая промышленность в 1913 году

Country | Available zinc in ore (short tons) | Spelter (short tons)
Produced | For export | To be imported | Annual con- sumption
Produced | Smelted | Exported | Imported | Primary | Secondary
United States | 305,500 | 310,500 | 8,500 | 13,500 | 310,500 | 50,000 | 21,000 |  | 339,500
Australasia | 206,000 | 4,000 | 202,000 | ... | 4,000 | ... | ... | ... | 4,000
British Isles | 50,000 | 65,000 | ... | 15,000 | 65,000 | 6,000 | ... | 143,500 | 214,500
Canada | 24,000 | ... | 24,000 | ... | ... | ... | ... | 20,000 | 20,000
Burma, Indo China, etc. | 18,000 | ... | 18,000 | ... |  |  |  |  |
France and French Africa | 69,000 | 63,000 | 6,000 | ... | 63,000 | 20,500 | ... | 5,500 | 89,000
Italy | 40,000 | ... | 40,000 | ... | ... | ... | ... | 12,000 | 12,000
Belgium | 11,000 | 218,000 | ... | 207,000 | 218,000 | 3,500 | 7,500 | ... | 84,000
China | 5,000 | 2,500 | 2,500 | ... | 2,500 | ... | ... | 7,500 | 10,000
Greece | 12,000 | ... | 12,000 |  |  |  |  |  |
Japan | 10,000 | 8,000 | 2,000 | ... | 8,000 | ... | ... | 4,000 | 12,000
Russia | 35,000 | 13,000 | 22,000 | ... | 13,000 | ... | ... | 23,500 | 36,500
Holland | ... | 27,000 | ... | 27,000 | 27,000 | 3,000 | 25,500 | ... | 4,500
Mexico | 30,000 | ... | 30,000 |  |  |  |  |  |
Norway | 15,000 | 10,000 | 5,000 | ... | 10,000 | ... | 10,000 |  |
Spain | 50,000 | 15,000 | 35,000 | ... | 15,000 | ... | 8,500 | ... | 6,500
Sweden | 10,000 | 6,000 | 4,000 | ... | 6,000 | ... | 6,000 | ... |
Austria-Hungary | 24,000 | 24,000 | ... | ... | 24,000 | 3,000 | ... | 17,500 | 44,500
Germany | 163,500 | 312,000 | ... | 148,500 | 312,000 | 18,500 | 75,000 | ... | 255,500
Other | ... | ... | ... | ... | ... | 1,500 | ... | 45,000 | 46,500
Total | 1,078,000 | 1,078,000 | 411,000 | 411,000 | 1,078,000 | 106,000 | 283,500 | 278,500 | 1,179,000

В Арканзасе руды имеют схожий характер и условия залегания; они встречаются в той же формации, а также в ордовикском известняке. Lavender Mining & Milling Co. является крупнейшим оператором, и добыча в основном велась по карбонатным рудам.

Верхнемиссисипский район включает месторождения в почти горизонтальных известняках ордовикского возраста. Три четверти добычи в этом районе обеспечивают пять компаний: Mineral Point Zinc Co., дочерняя компания New Jersey Zinc Co., с семью рудниками; Vinegar Hill Zinc Co. с шестью рудниками; Wisconsin Zinc Co., дочерняя компания American Zinc, Lead & Smelting Co., с четырьмя рудниками; Frontier Mining Co. с пятью действующими рудниками; и Cleveland Mining Co. с двумя рудниками. Другими важными компаниями являются Burr Mining Co., Block House Mining Co., M. & A. Mining Co., B. M. & B. Mining Co. и Oliver Mining Co., дочерняя компания U. S. Steel Corporation. Все рудники оснащены обогатительными установками. Добыча в районе демонстрирует устойчивый рост.

Цинковые месторождения юго-западной Виргинии и северо-восточного Теннесси встречаются в виде вкрапленных брекчий замещения вдоль зон дробления и разломов в складчатых кембро-ордовикских известняках, а также в виде окисленных руд в глинах, остаточных продуктах выветривания тех же известняков. Жильная масса состоит из кальцита и доломита. American Zinc Co. является крупнейшим оператором в Теннесси; она обладает мощностью обогащения 3000 тонн в сутки и запасами цинковой обманки более 6 000 000 тонн со средним содержанием цинка от 4 до 5 процентов, из которых производятся 60-процентные концентраты цинковой обманки. Эта компания является дочерним предприятием American Zinc, Lead & Smelting Co.

Западная провинция охватывает большинство западных штатов; она простирается на север в Британскую Колумбию и на юг в Мексику. Основными подпровинциями являются Ледвилл, Бьютт и Кер-д'Ален.

Месторождения Ледвилла встречаются в пластах, возраст которых варьируется от архейского до мелового, прорванных изверженными породами. Руды в основном представляют собой продукты замещения известняка и встречаются в виде крупных масс. Этот район впервые приобрел значение в производстве цинка после обнаружения смитсонита и каламина в крупных массах окисленных руд. В последние годы сульфиды составляют все большую часть добычи, поступая в основном с более глубоких горизонтов. Руды содержат золото, серебро, марганец, медь и иногда висмут. United States Smelting Refining & Mining Co., Empire Zinc Co., дочерняя компания New Jersey Zinc Co., Western Mining Co., Downtown Mines Co., Wellington Mines Co. в Брекенридже и рудник Mary Murphy в Чок-Крик являются крупнейшими операторами в этом регионе.

Руды Бьютта встречаются в виде жил в изверженных породах. Район, в котором преобладают цинковые руды, окружает зону важных медных жил с трех сторон. На границе двух зон в верхних горизонтах преобладают цинково-серебряные руды, а в более глубоких выработках — медные. Многие из нынешних цинковых рудников ранее разрабатывались на серебро. Эти комплексные цинковые руды стали доступными благодаря успешному применению масляной флотации и электролитического осаждения. Рудник Black Rock компании Butte & Superior Mining Co., Elm Orlu компании W. A. Clark & Son, Alice и несколько других рудников Anaconda Copper Mining Co. и North Butte Mining Co. являются одними из важнейших производителей. Двенадцать рудников, добывавших цинк в 1915 году, в совокупности обладают огромными запасами. Все руды содержат свинец и серебро, а также некоторое количество пирита, многие содержат медь и золото.

Подпровинция Кер-д'Ален включает ряд горнодобывающих районов в Айдахо, по крайней мере пять из которых являются производителями цинка. Interstate-Callahan в районе Бивер — самый крупный цинковый рудник в штате. Руда примечательна низким процентом минералов, отличных от сфалерита, при среднем содержании цинка 28 процентов.

Северо-Восточная провинция включает важные месторождения во Франклине, штат Нью-Джерси, и в горах Адирондак в Нью-Йорке, а также другие, менее значимые, в штатах Новой Англии. Она характеризуется месторождениями магматогенно-метаморфического происхождения в докембрийских известняках. Месторождения Франклина в Нью-Джерси состоят главным образом из франклинита, виллемита и цинкита в жильной массе из кальцита, родонита, граната, пироксена, магнетита и роговой обманки. Виллемит отделяется от этих руд магнитным способом и используется для производства цинка очень высокого качества, свободного от свинца и кадмия, и поэтому пользующегося большим спросом для определенных целей. Другие классы руд переплавляются для производства цинковых белил и зеркального чугуна. Эти рудники, принадлежащие и управляемые New Jersey Zinc Co., произвели более 1 500 000 тонн цинка в виде металла и оксида цинка. Район Эдвардс-Балмат в округе Сент-Лоуренс, штат Нью-Йорк, включает территорию шириной две-три мили и длиной пятнадцать миль, сложенную докембрийскими известняками. Руда встречается в виде линз и представляет собой смесь сфалерита, пирита и небольшого количества галенита с жильной массой из доломита. Разделение осуществляется на магнитных столах. Типичная руда содержит: сфалерит — 25,5 процента; галенит — 1,43 процента; пирит — 12,4 процента; барит — 3,9 процента. Запасы руды компании Northern Ore Co., крупнейшего оператора, по имеющимся данным, превышают один миллион тонн.

Германия.

— Имперская Германия включала большую часть одной металлогенической провинции первостепенной важности — Силезии, а также другие районы, ранжируемые следующим образом: Верхняя Силезия, Рейнская Пруссия, Вестфалия, Саксония, Ганновер и Нассау.

Основная часть минеральной провинции Верхней Силезии в 1914 году находилась в границах Германии. Когда-то она была частью Королевства Польского, за исключением частей, включенных в состав старых империй России и Австрии. Довоенная добыча цинковых руд из Российской Польши велась исключительно в этой металлогенической провинции. Месторождения, содержащие свинец и цинк вместе, встречаются в триасовых формациях, залегающих на каменноугольных породах, содержащих важные пласты угля. Такое соседство руды и топлива создало идеальную базу для развития крупной плавильной промышленности и облегчает плавку низкосортных руд. Сообщается, что руды содержат в среднем 17 процентов цинка и 5 процентов свинца. Они поступают из двух рудных горизонтов. Нижний характеризуется цинковой обманкой с небольшим количеством галенита и марказита; верхний, или свинцовый, горизонт включает очень устойчивый пласт галенита толщиной от 0,05 до 0,30 метра, под которым обычно залегает красный каламин. Месторождения цинковой обманки обширны и будут продуктивны еще долгое время.

В Рейнской Пруссии месторождения цинковой руды (смитсонита) встречаются в пластах девонского возраста. Эти месторождения близки к истощению. Основные цинковые месторождения Вестфалии находятся в девонских пластах. Исторические рудники во Фрайберге (Рудные горы) в Саксонии производят небольшое количество цинковой обманки при обогащении свинцовых руд. Цинковая обманка содержит значительное количество железа и серебра, а некоторые ее разновидности — следы олова. Эти рудники находятся под контролем саксонского правительства.

Значительное количество руды цинковой обманки концентрируется как побочный продукт при обогащении свинцовой руды в Верхнем Гарце, Ганновер. Руда Раммельсберга в Нижнем Гарце встречается в пласте, залегающем среди нижнедевонских сланцев и песчаников; она представляет собой тесную смесь цинковой обманки, галенита, пирита, халькопирита, барита, а также некоторого количества кальцита и кварца. Цинк производится как побочный продукт свинцовых руд в долине Лан (Нассау), где в нижнедевонских пластах обнаружена серия мощных жил.

Австралия.

— Цинковые ресурсы Австралийского Союза сосредоточены главным образом в Новом Южном Уэльсе и Тасмании. Первый в прошлом был основным источником цинка, но месторождения Тасмании в настоящее время быстро осваиваются и оснащаются для производства.

Важнейшим источником цинковой руды в Новом Южном Уэльсе является великая жила Брокен-Хилл, где работы начались в 1884 году. Вмещающие породы включают кристаллические сланцы и гнейсы. Между окисленными и первичными сульфидными рудами находилась тонкая зона вторичных сульфидов. Ранние работы в этом районе велись на свинец, и накопились огромные отвалы цинкосодержащих руд, отсортированных при добыче, или цинкосодержащих хвостов от обогащения свинцовых руд. В 1903 году эти отвалы оценивались в 5 687 400 тонн с содержанием 18,6 процента цинка. С ростом спроса на сульфидные цинковые руды и развитием методов масляной флотации для разделения и обогащения эти отвалы стали важными источниками цинковых концентратов, однако многие из них близки к истощению. Сульфидные руды представляют собой тесную смесь галенита и цинковой обманки, содержащую серебро. Существует два класса этих руд, различаемых как руды с силикатной жильной массой и руды с кальцитовой жильной массой. Рудные тела с силикатной жильной массой содержат родонит, гранат и кварц и богаче цинком и серебром, чем руды с кальцитовой жильной массой.

В настоящее время работают восемь горнодобывающих компаний. В порядке значимости их добычи и запасов руды эти компании следующие: Broken Hill South Silver Mining Co.; Broken Hill North Mining Co.; Zinc Corporation; Sulphide Corporation; British Broken Hill Proprietary Co.; Broken Hill Proprietary Co., Block 10; и Broken Hill Proprietary Co., Block 14. Оценочные запасы руды всех рудников составляют примерно 12 000 000 тонн.

Компания Broken Hill South Silver Mining Co. имеет запасы руды, оцениваемые в 3 350 000 тонн, и является крупнейшим производителем. Broken Hill North, Amalgamated Zinc (de Bavay), Zinc Corporation и Barrier South Ltd. контролируются Говеттом и партнерами, группой австралийских капиталистов. Компания Amalgamated Zinc Co. в 1913 году переработала 498 289 тонн хвостов, получив 140 098 тонн цинковых концентратов с содержанием цинка 48,9 процента; а также свинцовые концентраты в количестве 1 584 тонн с содержанием свинца 57,1 процента. Zinc Corporation, компания, созданная Bewick, Moreing Co., имеет запасы руды, оцениваемые в 1 504 211 тонн, со средним содержанием 14,8 процента свинца, 9,2 процента цинка и 2,5 унции серебра на тонну. Рудник Broken Hill Proprietary Co., согласно последним отчетам, почти истощен.

Основными месторождениями Тасмании являются месторождения Primrose, Hercules и Tasmania Copper Mines, все они принадлежат Mount Reed Rosebery Co., аффилированной с Mount Lyell Mining & Railway Co. Геологическая служба штата оценивает запасы в 1 272 500 тонн со средним содержанием 29,79 процента цинка, 8,89 процента свинца, 12,16 унции серебра и 0,17 унции золота на тонну.

Италия.

— Добыча цинка в Италии ведется в районе Иглезиас на Сардинии и в провинции Бергамо. Район Иглезиас находится в юго-восточной части острова Сардиния. Руды являются окисленными и в основном разрабатываются открытым способом. Их добычу и обогащение осуществляют две итальянские компании: Societa di Monteponi и Societa di Pertusola. Руды обычно переплавлялись в Германии, Англии или Бельгии. Рудники Бергамо в провинции Ломбардия разрабатываются английской компанией Crown Spelter Co., которая отправляет руду на плавку в Суонси, Уэльс.

Алжир.

— В 1913 году Алжир добыл 82 256 тонн цинковой руды. Из 78 973 тонн, происхождение которых известно, 31 процент от общего объема был добыт бельгийскими компаниями, а остальная часть — французскими операторами.

Япония.

— Единственным важным цинкодобывающим районом в Японии является провинция Хида. Основными компаниями являются Osaka Zinc Mining & Smelting Co., Takata & Co., Rhuara Mining Co. и Mitsui Mining Co. Крупнейшим производителем является рудник Камиока последней из названных компаний, который ежегодно добывает около 10 000 тонн. Osaka Mining Co. также добывает в Корее (Чосон) около 15 000 тонн руды ежегодно.

Годовая мощность плавильных заводов в Японии, с учетом завершения всего запланированного строительства, оценивается в 300 000 тонн цинковой руды, тогда как внутренняя добыча руды составляет около 50 000 тонн. Разница импортировалась главным образом из Сибири, Китая, Тонкина и Австралии. Ожидается, что в будущем иностранные руды будут поступать в основном из Китая и Сибири. Внутреннее производство цинка достигло около 60 000 тонн в год, а внутреннее потребление — 29 000 тонн.

Испания.

— Цинковые руды добываются в провинциях Сантандер, Мурсия, Теруэль, Бискайя и Гипускоа. Единственным важным районом является Сантандер, где находится цинкоплавильный завод, принадлежащий Compagnie Royale Asturienne des Mines (французской). Часть руды переплавляется во Франции. Большинство испанских руд представляют собой каламин и встречаются почти исключительно в известняках. Восемьдесят процентов испанской добычи приходится на Сантандер и Мурсию. В последней рудники разрабатываются преимущественно на свинец.

Россия.

— Добыча цинка в Российской империи велась в Российской Польше, восточной Сибири, на Алтае в юго-западной Сибири и в северных горах Кавказа. Польские месторождения являются частью Силезского бассейна. Руды в основном представляют собой карбонаты и силикаты. Некоторые рудники и заводы принадлежали российскому правительству, другие, по-видимому, французским компаниям. В восточной Сибири рудник Тютиха имеет рудное тело каламина, содержащее не менее 200 000 тонн со средним содержанием 48 процентов цинка. Часть руды поступала из Уссурийского района. Считается, что Mitsui Mining Co. договорилась об отправке руд из этого района в Японию для переработки.

На Алтае в юго-западной Сибири компания Ridder Mining Co., контролируемая Irtysh Corporation, Ltd. из Лондона, разработала два крупных месторождения в одной и той же минерализованной зоне с запасами руды, оцениваемыми в 1917 году более чем в 3 500 000 тонн. Потенциал этого объекта огромен. Компания приобрела Экибастузские угольные месторождения, построила около 165 миль железной дороги и обеспечила речной транспорт, таким образом соединив руду и уголь на плавильном заводе мощностью 15 000 тонн свинца и 5 000 тонн цинка в год.

В северных горах Кавказа рудник Садон, принадлежащий Société d’Alagir (французской), разрабатывается уже давно. Руды с этого рудника переплавляются на месте.

Другие страны.

— Добыча цинковой руды во Франции ведется в нескольких разрозненных районах. Из 45 929 длинных тонн, зарегистрированных в 1912 году, почти все поступили с шести рудников, которые полностью контролируются французским капиталом, возможно, с некоторым участием бельгийского.

Единственным важным источником цинка в Греции является знаменитое месторождение Лаврион, которое разрабатывалось еще в древности. Древние, однако, по возможности отбрасывали цинковые руды. Эти месторождения в настоящее время контролируются и эксплуатируются французской компанией Compagnie Française des Mines de Laurium, которая также вновь открыла древние выработки Гебель-Росас недалеко от Красного моря в Египте.

Основными цинковыми рудниками Швеции являются Аммеберг, Rylls Wytland и Сала. В Сале огромные кучи хвостов, образовавшиеся за столетия эксплуатации и содержащие значительные количества цинка, теперь могут быть переработаны, так же как и цинконосные участки, оставленные при добыче серебряно-свинцовых руд. Важное месторождение Аммеберг состоит из полос и линз вкрапленной цинковой обманки в гнейсовидном гранулите и эксплуатируется Société de la Vieille Montagne (бельгийской).

Добыча цинка в Мексике велась главным образом в штатах Нуэво-Леон, Чиуауа и Сонора. Различные цинковые месторождения в Нуэво-Леоне разрабатывались на немецкий и американский капитал. Большинство из них находятся в пределах 50 миль от Монтеррея. Цинкодобывающие районы разбросаны по всему штату Чиуауа. В районе Санта-Эулалия компания El Potosi Mining Co., контролируемая американцами, разрабатывает одноименный рудник, в котором карбонатные руды залегают на глубине до 1700 футов. Buena Tierra в том же районе контролируется британским капиталом. Основные рудники в районе Парраль принадлежат американским и британским компаниям, включая American Smelters Securities Co., American Zinc Extraction Co. и San Francisco Mines of Mexico, Ltd. (британскую). Carnegie Lead & Zinc Co. владеет крупнейшим цинковым рудником в Соноре, расположенным недалеко от Кананеи. Calumet & Arizona Co. и Mexican Metal Co. владеют цинковыми месторождениями в районе Ариспе. Все эти компании являются американскими.

Цинковые руды добываются в Австрии в провинциях Каринтия, Штирия, Крайна, Тироль и Галиция. Рудники Райбл и Шнеберг в Каринтии являются государственными, а руды переплавляются на государственных заводах в Цилли. Тирольские руды отправлялись во Франкфурт-на-Майне и Ахен. Штирийские руды отправлялись на плавку в Силезию и Рейнскую Пруссию.

Значительная добыча каламина с некоторым количеством цинковой обманки в Тунисе находится под французским политическим и коммерческим контролем. Основными производителями цинковой руды являются, по-видимому, французские компании, которые в целом выплачивают правительству Туниса роялти в размере 5 процентов от чистой выручки. Общий объем добычи за 1916 год составил 12 544 тонны.

Four districts of Indo-China produce zinc ores with an aggregate total annual output of about 46,000 tons.

Крупнейшим цинковым рудником в Великобритании является Нентхед в Камберленде, разрабатываемый Société de la Vieille Montagne (бельгийской). Вторым по величине производителем является рудник Каршилд в Нортумберленде. За исключением рудника Нентхед, все важные производители, насколько известно, принадлежат британскому капиталу и управляются им.

Основным рудником в Китае является Шуйкоушань, находящийся под контролем Горного управления Хунани. До войны этот рудник находился под доминированием немецкого капитала, который предоставил оборудование и отправлял продукцию в Европу. Японцы усердно и с частичным успехом пытались установить контроль над этим рудником.

Основным цинкодобывающим районом в Боливии является Уанчака, добыча в котором в последнее время сократилась из-за большого притока воды в выработки. Крупнейшим оператором является Compañia Huanchaca de Bolivia, капитал и контроль которой являются французскими. Добыча цинка является сопутствующей, основным металлом является серебро.

Добыча цинка в Канаде ведется главным образом в Британской Колумбии, но небольшое количество добывается в Онтарио и Квебеке. Единственная добыча, имеющая значение, ведется в южной части Британской Колумбии, где наиболее важен район Слокан. Значительный интерес проявляют британский, канадский и американский капитал. В 1915 году рудники района Слокан, по оценкам руководства плавильного завода Трейл, были способны производить от 10 000 до 15 000 тонн руды с содержанием 40–45 процентов цинка. По-видимому, это было в дополнение к возможной добыче на руднике Салливан, принадлежащем Consolidated Mining & Smelting Co., Ltd. (плавильный завод Трейл), который имел доказанные запасы 3 500 000 тонн галенит-сфалеритовой руды. Основные рудники Онтарио и Квебека произвели 580 тонн цинка, или одну тридцатую часть добычи Канады. Они эксплуатируются, по крайней мере частично, на американский капитал, а руды переплавляются компанией Zinc Co., Ltd., принадлежащей американцам.

Основными месторождениями Индии являются месторождения рудника Бодуин, расположенные в Северных штатах Шан (Бирма). На 31 декабря 1917 года оценивалось 4 033 000 тонн свинцово-цинковой руды с содержанием 24,7 унции серебра, 27,4 процента свинца и 19,1 процента цинка. Основными компонентами руд являются галенит и сфалерит с небольшим количеством пирита и халькопирита. Свинцовые и цинковые концентраты пригодны для обычных методов плавки. В Сакохи с помощью индийского правительства строится завод по дистилляции цинка и производству серной кислоты для переработки цинкового концентрата. Компания эксплуатирует свинцовый плавильный завод в Нам-Ту, в 11 милях от рудников. Можно ожидать, что месторождения Бодуин станут важным фактором в мировом производстве цинка в ближайшем будущем. Они принадлежат Burma Mines, Ltd., английской корпорации интересов Р. Тилдена Смита, Говетта и Гувера, в которой участвует некоторый американский капитал.

Единственным примечательным цинковым месторождением в Египте является Гебель-Росас, эксплуатируемое Compagnie Française de Laurium. Это месторождение расположено недалеко от Красного моря и разрабатывалось в древности.

Единственным важным месторождением в Южной Африке является Родезия Брокен-Хилл. Крупные рудные тела, насколько они разведаны, почти полностью окислены. Одно рудное тело оценивается в 250 000 длинных тонн со средним содержанием 26 процентов свинца, 22,5 процента цинка, а другое — в 300 000 длинных тонн со средним содержанием 32 процента цинка, с небольшим количеством свинца, но большим количеством оксида железа и карбоната. Они контролируются британским капиталом. При разработке коммерческого метода переработки возникли значительные трудности.

В Перу французская компания Association Minière имеет интересы в Compagnie des Mines de Huaron.

РАЗВИТИЕ И ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРОСТРАНЕНИИ В БЛИЖАЙШЕМ БУДУЩЕМ

Насколько доступна информация, никаких заметных изменений в темпах добычи в странах Европы и северной Африки не представляется вероятным. Большинство районов в этих странах эксплуатировались в течение длительного периода и прошли свой зенит добычи; многие близки к истощению. Однако снижение в большинстве из них будет постепенным. Наиболее важным изменением в Европе, вероятно, станет переход под польскую юрисдикцию всего Силезского бассейна, что сделает новое государство Польша, если оно будет создано, как предлагается, крупнейшим единичным источником цинковой руды в Европе.

В Соединенных Штатах, которые останутся крупнейшим производителем цинка в мире, наибольшего увеличения относительной значимости можно ожидать от западной металлогенической провинции, особенно на северо-западе, в районах Бьютт и Кер-д'Ален. Район Ледвилл уже прошел зенит добычи и опустился на второе место после Бьютта, который способен на дальнейшее увеличение.

В Австралии можно ожидать, что район Брокен-Хилл будет давать около 450 000 тонн концентратов ежегодно в течение примерно трех лет, после чего добыча должна снизиться до примерно 300 000 тонн. Увеличение добычи в Тасмании будет в значительной степени зависеть от строительства электролитических цинковых заводов, но остров будет фактором производства в ближайшем будущем.

Крупнейшим новым фактором в мировом производстве цинка станут рудники Бодуин в Бирме, которые в течение короткого времени будут оснащены для производства около 300 000 тонн руды ежегодно, или около 75 000 тонн высококачественных цинковых концентратов и 100 000 тонн низкокачественных концентратов или промпродуктов для переработки по процессу Ганлина. Степень, в которой цинковые концентраты из этой руды будут перерабатываться в Индии, будет определяться развитием местного рынка серной кислоты. Остальная часть концентратов будет перерабатываться в Англии.

Недавние разработки на Алтае в юго-западной Сибири доказали наличие огромных тел комплексных цинково-свинцовых руд. Однако масштаб их эксплуатации будет в значительной степени определяться состоянием российского рынка, на который влияют социальные и политические условия. Отмена жестких тарифов на импорт из-за рубежа в производственные центры Варшавы, Петрограда и Москвы может значительно ограничить рынок для продукции этих рудников. Их крайняя географическая изоляция не позволит месторождениям стать важным фактором на мировом рынке в течение длительного периода, несмотря на их большие размеры и отличное качество.

Использование месторождения Родезия Брокен-Хилл в Южной Африке будет задержано из-за трудности разделения окисленных свинцовых и цинковых минералов, нехватки топлива, а также географической и коммерческой изоляции.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Политический контроль над цинковыми ресурсами мира до начала войны в 1914 году, по-видимому, оказывал лишь незначительное влияние на отрасль. Экономические факторы делали неэффективным любой контроль, не имеющий международного масштаба. Очень большой процент цинковых руд мира транспортировался из страны добычи в другую для переработки, в некоторых случаях даже реэкспортируясь, иногда после кальцинации, с целью использования содержания серы в производстве кислоты. Некоторые страны, например, Соединенные Штаты, вводили тарифы на определенные классы цинковых руд. Такие меры имели некоторое влияние на добычу в Мексике и Канаде. Россия ввела высокие импортные пошлины, которые субсидировали внутреннее производство и стимулировали разведку и разработку. Основные европейские страны, импортирующие и переплавляющие цинковые руды, допускали их беспошлинный ввоз.

Однако во время Мировой войны политическая юрисдикция в значительной степени использовалась для восстановления контроля над национальными ресурсами гражданами данной страны или ее союзниками. Это движение было особенно заметно в Британской империи, где в настоящее время существует совместный политический и коммерческий контроль. Иностранные интересы были устранены действиями правительства, и правительство сохраняет долю в контроле через участие в маркетинговых организациях или через финансовое участие в перерабатывающих предприятиях. Канада установила небольшую премию на цинк, произведенный в Канаде из отечественных руд, и оказала финансовую помощь попыткам создания отечественных плавильных и рафинировочных заводов.

В Соединенных Штатах Управляющий имуществом враждебных государств (Alien Property Custodian) активно занимался устранением любого контроля со стороны иностранных враждебных элементов. Его ставленники будут контролировать многие важные компании в течение нескольких лет. Предпринятые действия, по-видимому, не нарушили ту централизацию контроля, которая уже была осуществлена.

См. главу о меди, страницы 232–235, для обсуждения немецких интересов в американской торговле металлами.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Медь, свинец и цинк образуют отдельный класс с точки зрения промышленного использования и объемов производства, занимая место после железа, которое значительно превосходит их, как наиболее важные цветные металлы. Годовое производство каждого из них значительно превышает миллион тонн. Учитывая промышленную важность цинка и тот факт, что латунь, сплав меди и цинка, является незаменимым материалом в современной промышленности, неудивительно, что великие промышленные нации придумали множество уловок в стремлении контролировать цинковую промышленность.

Владение и оперативный контроль над рудниками были второстепенным фактором в коммерческом контроле этой отрасли. Экономические факторы вынуждают размещать ретортные плавильные заводы в промышленных районах, прилегающих к угольным бассейнам, причем наиболее важными факторами являются доступность и стоимость топлива и рабочей силы, а также близость к рынку сбыта цинка. Нехватка топлива и дефицит или высокая стоимость рабочей силы препятствовали плавке в некоторых регионах, производящих значительное количество руды. С другой стороны, плавка, осуществляемая в некоторых странах, была совершенно несоразмерна их добыче руды. Возрождение националистических настроений в результате Мировой войны может сделать владение и оперативный контроль более важным фактором в будущем.

Электролитическое и электротермическое восстановление руд делает возможным экономичное производство цинка там, где это было ранее невозможно, и может привести к некоторой децентрализации отрасли.

Владение или контроль над перерабатывающими заводами были важной основой для контроля над отраслью. Наиболее эффективный контроль осуществлялся через маркетинговые организации или торговые объединения перерабатывающих заводов, агентства по закупке руды и продаже металла, с перекрестным участием в советах директоров, совместным владением и долгосрочными контрактами на руды, концентраты и металлы. В последние годы они приобрели всемирный масштаб и полностью доминировали в отрасли.

Соединенные Штаты.

— Ниже перечислены наиболее важные компании по плавке цинка в Соединенных Штатах, а также процент от общей мощности переработки, который контролирует каждая из них:

| Percentage of production controlled
New Jersey Zinc Co. | 13.4
American Metal Co. | 15.2
Grasselli Chemical Co. | 10.1
Anaconda Copper Mining Co. | 10.0
United States Steel Corporation |  7.7
American Smelting & Refining Co. |  7.2
American Zinc, Lead & Smelting Co. |  5.7
Beer, Sondheimer & Co. |  4.7
L. Vogelstein & Co. |  1.7
Various independents or of unknown affiliation | 24.3

Тесные связи L. Vogelstein & Co., Beer, Sondheimer & Co., American Metal Co. и их дочерних компаний, составляющих 27,3 процента плавильных мощностей, и различных производителей руды, с их контрактами на продажу металла с другими плавильными заводами, позволили им доминировать на американском рынке металлов в интересах немецкого «Трио». Управляющий имуществом враждебных государств взял под контроль все три компании во время войны и устранил всю собственность и контроль со стороны иностранных враждебных элементов, продав акции, принадлежащие немцам, на аукционе.

American Metal Co. полностью владеет American Zinc & Chemical Co., South American Metal Transport Co., Bartlesville Zinc Co. и South American Metal Co.; она имеет крупные пакеты акций в Ohio and Colorado Smelting & Refining Co., Compañia Minera de Peñoles, Compañia de Minerales y Metales, Compañia Metalurgica de Torreon, Compañia Minera Palmo y Cabrillos, Fundicion de Guayacan, Balbach Smelting & Refining Co. и Nichols Copper Co., некоторые из которых работают в Мексике и Южной Америке. Акционерный капитал American Metal Co. составлял 70 000 акций, из которых 34 644 принадлежали иностранцам, связанным с немецким «Трио»; 18 620 акций принадлежали американским гражданам, которые осуществляли контроль над управлением, а остальные принадлежали интересам Мертона из Лондона, которая была реорганизована британским правительством с устранением иностранной собственности. Акции, принадлежавшие иностранцам, были проданы Управляющим имуществом враждебных государств, и контроль над бизнесом на период в пять лет был передан совету из пяти доверенных лиц, назначенных им.

National Zinc Co. принадлежала Beer, Sondheimer & Co., одному из членов немецкого «Трио», которая также владела другими компаниями по производству металлов в Соединенных Штатах и на Кубе.

Оперативный контроль над American Zinc, Lead & Smelting Co. был приобретен Butte & Superior Mining Co., в которой доминирует Hayden, Stone & Co. из Нью-Йорка и Бостона. Крупная доля в American Zinc, Lead & Smelting Co. принадлежала L. Vogelstein & Co., ранее представителю немецкой Metallgesellschaft в Соединенных Штатах. American Zinc, Lead & Smelting Co. контролирует Wisconsin Zinc Co.; American Zinc Co. из Иллинойса; American Zinc Co. из Теннесси; и American Zinc Ore Separating Co.

New Jersey Zinc Co., американская компания, контролирует месторождение в Нью-Джерси и через свою дочернюю компанию Empire Zinc Co. владеет и управляет рядом рудников в западных штатах и Мексике, а также Mineral Point Zinc Co. из Висконсина, одним из трех крупнейших производителей в этом регионе, и четырьмя цинкоплавильными заводами.

Компания Anaconda управляет рядом цинкодобывающих рудников в районе Бьютт и построила электролитические заводы для переработки собственных концентратов: один мощностью 25 тонн в качестве экспериментального завода в Анаконде и завод мощностью 200 тонн в сутки в Грейт-Фолс, штат Монтана. Она перерабатывала часть продукции других компаний, в частности Butte & Superior Mining Co. Это американская компания под американским контролем, но имеющая много европейских акционеров.

Германия.

— Амбиции немецких коммерческих интересов контролировать рынки металлов и ресурсы мира были в большей степени реализованы в случае с цинком, чем с любым другим металлом.

Немецкий цинковый синдикат (Zinkhüttenverband) был организован в 1909 году тремя мощными группами интересов: (1) группой Мертона, включающей Metallgesellschaft, Metallbank и Metallurgische Gesellschaft, все из Франкфурта, и компании Мертона из Лондона; (2) Beer, Sondheimer & Co., которая через акционерное общество Tellus контролировала более десятка металлургических и химических предприятий; и (3) Aron Hirsch & Sohn в Хальберштадте; и к нему немедленно присоединились все важные силезские и рейнско-вестфальские цинковые предприятия. Организаторы стали эксклюзивными торговыми агентами синдиката, и закупки из любых иностранных источников производились сообща. Синдикат немедленно заключил соглашения с австрийскими и бельгийскими производителями, включая Vieille Montagne, которая имеет рудники, заводы и агентства во многих частях мира. К нему также присоединилась голландская компания Zincs de la Campine. Синдикат объединял в общей сложности 18 фирм и регулировал как их выпуск, так и цены. К концу 1912 года этот немецкий синдикат контролировал непосредственно половину мирового производства цинка и три четверти европейского производства.

Два бельгийских и несколько французских заводов сформировали другой синдикат. Третий был сформирован шестью английскими заводами, и конкуренция со стороны фирм Соединенных Штатов вынудила все три объединиться в Международный цинковый синдикат, который просуществовал до апреля 1914 года. Международный синдикат регулировал выпуск продукции своих членов, но не устанавливал точных цен. Через American Metal Co. и аффилированные компании немецкий синдикат быстро становился важным фактором в контроле над добычей цинка в Соединенных Штатах, Мексике и Австралии у источника. Немецкий синдикат сохранял свое доминирование и быстро расширял и укреплял его по всему миру через банки, холдинговые компании, связи с синдикатами и картелями, перекрестное участие в советах директоров и совместное владение акциями.

В результате войны австралийские цинковые концентраты навсегда перенаправлены с немецких перерабатывающих заводов, и весь немецкий контроль устранен. Деятельность Управляющего имуществом враждебных государств способствовала устранению немецких интересов в Соединенных Штатах. Восстановление государства Польша может отобрать у Германии все силезские месторождения и перерабатывающие заводы, оставив только предприятия Рейнско-Вестфальского, Гарцского и Рудногорского регионов, с объемом добычи руды, составляющим лишь одну треть от прежнего внутреннего производства. Польша должна стать в два раза важнее Германии в цинковой промышленности, если только Германия не сможет импортировать руды и концентраты в больших масштабах.

Австралия.

— К началу Мировой войны австралийская цинковая промышленность находилась в тисках великого немецкого цинкового синдиката, описанного более подробно выше в разделе «Германия». Он контролировал мировой рынок цинка, определял объемы производства и цены и манипулировал рынком в интересах Германии. Это было возможно благодаря долгосрочным контрактам на цинковые концентраты, в виде которых почти вся продукция цинка экспортировалась для переработки в Бельгию и Германию. Только 10 процентов концентратов переплавлялись в Порт-Пири или в Англии.

Во время войны эти контракты были аннулированы австралийским и британским правительствами, и была предпринята работа по реорганизации отрасли на чисто австралийской и британской основе. Идея заключалась в том, чтобы по мере возможности обеспечить переработку всей руды в Австралии, чтобы ее можно было продавать в готовом виде. Австралийское правительство сначала создало биржу металлов, через которую должны были проходить для продажи все металлы, произведенные в Австралии. Компания Zinc Producers’ Association Proprietary, Ltd. была зарегистрирована 20 мая 1916 года в штате Виктория, Австралия, для сбыта продукции компаний-членов, производящих цинковые руды, концентраты и металлы в Австралийском Союзе и на Тасмании; все эти компании продали весь свой объем производства ассоциации сроком на пятьдесят лет. Акции в количестве 100 000 штук номиналом по 1 фунту стерлингов каждая принадлежат следующим компаниям: Amalgamated Zinc (De Bavay’s); Broken Hill Proprietary, Block 14; Zinc Corporation; Broken Hill Proprietary; Electrolytic Zinc Smelters; Junction North; North Broken Hill; Sulphide Corporation; British Broken Hill; Broken Hill Associated Smelters; Broken Hill Junction; Broken Hill South Silver; Broken Hill Proprietary, Block 10; Mount Lyell Mining & Railway Co.

Федеральное правительство Австралии, действуя через Zinc Producers’ Association, заключило контракт на продажу британскому правительству всего объема производства цинковых концентратов в Австралии на период войны и десять лет после ее окончания. Ранее премьер-министр заключил контракт на продажу имперскому правительству 100 000 тонн цинковых концентратов и 45 000 тонн электролитического цинка и товарного цинка сроком на десять лет. Соглашение предусматривало, что британское правительство заберет запасы цинковых концентратов, имевшиеся на 31 декабря 1917 года, за вычетом определенного процентного резерва, а затем по 250 000 тонн ежегодно в течение периода войны и по 300 000 тонн ежегодно в течение последующих девяти лет. Также были предусмотрены поставки для нужд австралийских заводов по рафинированию цинка и выполнение японских контрактов в течение периода, охватываемого британским контрактом. В нормальных условиях австралийское производство цинковых концентратов с содержанием цинка от 46 до 48 процентов составляет около 450 000 тонн в год стоимостью 25 000 000 долларов.

Результатом вышеуказанных соглашений является постоянный перевод контроля над австралийской цинковой промышленностью от германских к британским гражданам в рамках системы, сочетающей коммерческие и политические аспекты. Рудники и предприятия всегда находились в собственности британского и австралийского капитала.

Zinc Producers’ Association носит кооперативный характер, гарантируя всем членам равные условия независимо от объема добычи. Содружество представлено в совете директоров. Федеральное правительство также всячески поощряет создание заводов по восстановлению металлов, особенно заводов по производству электролитического цинка. Сообщалось, что Burma Corporation была акционером Zinc Producers’ Association, но это сообщение не получило удовлетворительного подтверждения. Если это правда, ассоциация может в конечном итоге контролировать продажу от 85 до 95 процентов цинковых руд Британской империи. Обладая мощностями по плавке значительной части своей продукции и действуя как единое целое при продаже излишков, австралийские производители цинка в дальнейшем должны занимать сильные позиции в отношениях с германскими, голландскими и бельгийскими плавильными заводами. Плавильные мощности не будут значительно увеличены в ближайшем будущем.

Франция.

— Националистическое движение во Франции во время войны привело к созданию торговых ассоциаций, известных как «консорциумы», включающих основных участников каждой отрасли.

[139] Описание консорциума, охватывающего минеральную промышленность, Société Minerais et Metaux, см. в главе о свинце, страницы 284 и 285.

ПОЛОЖЕНИЕ ВЕЛИКИХ ДЕРЖАВ

После устранения интересов враждебных иностранных государств в American Metal Co., L. Vogelstein & Co. и Beer, Sondheimer & Co., промышленность в Соединенных Штатах контролируется, а рудники и предприятия принадлежат американскому капиталу, который также контролирует часть добычи цинка в Мексике, Канаде и Перу. Будущее производство и потребление, вероятно, будут сбалансированы, как и до войны. В настоящее время существуют избыточные плавильные мощности, но было убедительно доказано, что страна способна обеспечить рудой еще большие мощности. Соединенные Штаты сохранят первое место как производитель. В период адаптации некоторые концентраты могут поставляться в Бельгию и Голландию.

С постоянным перенаправлением австралийских концентратов и вероятной потерей силезских месторождений и заводов по восстановлению металлов Германия потеряет свое второе место в отрасли. Имея в качестве источников отечественных руд только Рейнский, Вестфальский, Гарцский и Рудные горы районы, поставки сократятся до одной трети от объема, производившегося до 1914 года, что составляло лишь две трети всей руды, выплавляемой в стране. Если руды или концентраты не будут импортироваться, Германия станет лишь незначительным фактором в производстве цинка. В то время как в 1912 году у Германии было 50 000 тонн товарного цинка, доступного для экспорта, теперь может потребоваться импорт. В результате мирного договора польская промышленность может оказаться под доминированием французского капитала.

Не более 5 процентов руды, выплавляемой в Бельгии, является продукцией отечественной добычи. Рудники принадлежат французским и германским компаниям. Предприятия принадлежат французам, бельгийцам и немцам примерно в равных пропорциях. Часть австралийских концентратов будет выделена Бельгии для плавки. Крупнейший участник бельгийской промышленности, компания Société de la Vieille Montagne, владела и разрабатывала рудники в Бельгии, Морене (Германия), Швеции, Англии, Алжире и Тунисе, а также заводы по восстановлению металлов в Бельгии, Германии и Франции. Хотя ранее эта компания была членом германской цинковой конвенции, она, по-видимому, контролируется бельгийским капиталом, связанным с сильнейшими бельгийскими финансовыми интересами. Несколько других бельгийских компаний имеют важные интересы во Франции, Испании, Алжире и Тунисе. Между французским и бельгийским капиталом в цинковой промышленности, по-видимому, существует тесная связь, которая, как ожидается, сохранится.

Рассмотрим теперь Британскую империю. Внутренняя добыча цинковых руд на Британских островах незначительна, но плавильные заводы сделали Англию важным фактором в отрасли, хотя до 1914 года они обеспечивали лишь 32 процента потребления цинка в империи. Мощности этих заводов, находящихся в британской собственности, были значительно увеличены, и строятся новые предприятия для переработки концентратов из Австралии и Бирмы, поставки из которых в более чем достаточном количестве обеспечены контрактами имперского правительства с Zinc Producers’ Association Австралии. Имперское правительство заинтересовано в некоторых из этих предприятий. Заводы по восстановлению металлов также будут работать в Австралии, на Тасмании, в Индии и Канаде. Излишки австралийских концентратов будут распределяться между французскими и бельгийскими заводами. При существующей организации британское доминирование в европейской цинковой промышленности кажется неизбежным.

Рудники и предприятия Австралии полностью контролируются английским и австралийским капиталом. Организация, находящаяся под контролем австралийского правительства, стала единственным маркетинговым агентством для производителей. Рудники Индии и Бирмы контролируются англичанами, а плавильный завод, строящийся в Сакчи, частично финансируется индийским правительством. Рудники Канады в основном принадлежат британцам, хотя есть и некоторые американские интересы. Потенциальная мощность рудников велика. Несмотря на государственные субсидии, мощность и будущее заводов по восстановлению металлов остаются неопределенными.

Французский капитал контролирует все отечественные предприятия и рудники Франции, а также предприятия Греции, Индокитая, Туниса, большинство рудников Алжира, где также заинтересован некоторый бельгийский капитал, часть бельгийских и польских рудников и заводов по восстановлению металлов, некоторые испанские рудники и плавильные заводы, а также, вероятно, рудники на Кавказе в России. Франция должна стать важным фактором в отрасли в ближайшем будущем.

Крупнейшие рудники Италии принадлежат итальянским компаниям, и ими же строятся некоторые отечественные заводы по восстановлению металлов. Главная добывающая компания в Северной Италии — английская.

В Японии японскому капиталу принадлежат все отечественные рудники и предприятия, а также предприятия в Чосоне (Корее), и он быстро берет под контроль месторождения Китая и Восточной Сибири. Текущие плавильные мощности превышают внутреннее потребление и значительно превышают внутренние поставки руды. Руда импортируется из Китая, Сибири, Индокитая и Австралии.

Что касается России, то право собственности на месторождения в польских регионах до 1914 года было разделено между русскими и французами, и это положение, по-видимому, будет восстановлено с учетом польского политического контроля. Российские интересы, несомненно, находились под германским влиянием. Регион Алтайских гор контролируется британским капиталом, и его развитие полностью зависит от того, как внутренние социальные и политические условия повлияют на внутренний рынок, к которому продукция этого региона ограничена географической изоляцией. Восточная Сибирь, по-видимому, быстро переходит под коммерческий контроль японцев.

Голландия не имеет рудников, но обладает значительными плавильными мощностями. Она также зависит от своих соседей в поставках угля. Ее будущее трудно предсказать. Рудники и предприятия Испании в значительной степени находятся под французским и бельгийским контролем, что может быть изменено контрактами с английскими интересами. Контроль в Норвегии и Швеции точно не известен. Номинально он осуществляется местным капиталом, но вероятны некоторые английские и германские интересы. Сообщается, что компании Sulphide и Zinc, обе британские, заинтересованы в Hydraulic Power & Smelting Co.

Рудники и предприятия Австрии, которые принадлежали австрийскому правительству и австрийским компаниям, возможно, под германским доминированием, теперь будут распределены между двумя или тремя политическими юрисдикциями. Руда почти не импортируется и не экспортируется, и регион в целом не является важным фактором в отрасли.

Рудники в Мексике в значительной степени принадлежат мексиканцам и американцам. Сообщается, что германский контроль силен и растет. Возможности добычи руды велики.

РЕЗЮМЕ

Основные виды использования цинка: в латуни, сплаве с медью, являющемся незаменимым материалом в современной промышленности; в гальванотехнике в виде катаных листов; и при обессеребливании свинцового сплава. Потребление наиболее велико в гальванотехнике. Количество, используемое в виде катаных листов, будет увеличиваться.

Цинк и свинец обычно встречаются вместе в своих рудах и широко распространены по всему миру, но странами с наибольшей добычей руды являются, в порядке убывания, Соединенные Штаты, Германия и Австралия. Бирма скоро станет важным игроком. Сибирь может добывать много руды в ближайшем будущем, но эксплуатация будет сдерживаться политическими условиями и географической изоляцией. Ожидается, что Канада, Мексика, Чили, Перу и Боливия увеличат объем производства.

Успешное коммерческое применение электромагнитных, электростатических и, особенно, процессов масляной флотации для разделения и концентрации комплексных руд сделало доступными огромные ресурсы, пополнив список регионов добычи руды и существенно повлияв на их относительную значимость.

Экономические факторы, особенно наличие и стоимость топлива и квалифицированной рабочей силы при ретортной плавке, а также рынок сбыта товарного цинка, определяли расположение заводов по восстановлению металлов в густонаселенных промышленных районах, прилегающих к угольным бассейнам. Минеральные ресурсы, однако, во многих случаях находятся в странах, либо неразвитых в промышленном отношении, либо не имеющих обильного и дешевого топлива, и большой процент цинковых руд перевозится из страны-производителя в другую для переработки. В порядке их важности странами, производящими больше всего товарного цинка, являются: Соединенные Штаты, Германия, Бельгия, Великобритания и Франция.

Коммерческий контроль над отраслью основывался главным образом на контроле над заводами по восстановлению металлов, организациями по закупке руды и продаже металлов, а не на владении месторождениями, и для эффективности он неизбежно приобрел международный масштаб. До 1914 года организация, по-видимому, международного характера, но на самом деле доминируемая немцами, благодаря контролю на этой основе достигла командных высот в отрасли, весьма эффективно влияя на объем производства и цены. Однако во время Первой мировой войны политическая юрисдикция в значительной степени использовалась для восстановления контроля над ресурсами страны и отраслями промышленности в пользу граждан этой страны или ее союзников. Это движение было особенно заметно в Британской империи, где сейчас существует совместный политический и коммерческий контроль через Zinc Producers’ Association и контракты, в которых участвуют правительства, а также во Франции, где Société Minerais et Metaux под эгидой правительства объединяет все основные горнодобывающие и металлургические компании, контролируемые французским капиталом, и является арбитром в металлургической промышленности.

Децентрализация отрасли и перераспределение заводов по восстановлению металлов в некоторой степени являются результатом успешного применения электролитического восстановления и распространения знаний о практике ретортной плавки.

Британская империя как единое целое должна быть способна доминировать в отрасли в Европе в ближайшем будущем. Франция, благодаря политическому и коммерческому контролю над Алжиром и Тунисом, а также крупному финансовому контролю в Бельгии, Испании и Польше, будет занимать сильные позиции. Бельгия, с небольшими, но широко распространенными финансовыми интересами в рудниках и предприятиях во Франции, Германии, Англии, Швеции, Испании, Алжире и Тунисе, является важным фактором в европейской ситуации. Ее интересы кажутся тесно связанными с интересами Франции. Соединенные Штаты, обладая большими мощностями по восстановлению металлов и запасами руды, сохраняя при этом свое положение крупнейшего производителя, как ожидается, будут обеспечивать внутреннее потребление, но экспортировать мало, как это было до войны. Положение Германии будет зависеть главным образом от поставок иностранной руды, которую, возможно, придется в значительной степени импортировать из Мексики и Соединенных Штатов.

ГЛАВА XVII ОЛОВО Автор: Джеймс М. Хилл [140]

[140] Автор выражает свою благодарность Адольфу Кнопфу из Геологической службы США и Р. Р. Хорнеру из Бюро горного дела США за их помощь в подготовке этой статьи.

ИСПОЛЬЗОВАНИЕ ОЛОВА

Олово, которое обычно считается одним из второстепенных металлов, тем не менее является металлом первостепенной важности в нынешнем состоянии мирового развития. В 1913 году стоимость мирового производства олова составила 131 000 000 долларов, что превышало стоимость мирового производства свинца или цинка. Без олова весьма сомнительно, чтобы нынешние методы упаковки и распределения продуктов питания могли быть реализованы. Основное использование олова — производство жести, из которой изготавливаются так называемые «консервные банки», известные каждому. Второе по величине потребление олова приходится на сплавы: припой и баббит, изготавливаемые со свинцом, а также латунь и бронзы, изготавливаемые с медью. Незначительные количества олова используются для изготовления тонких металлических трубок, оловянной фольги и складных тюбиков для упаковки таких материалов, как зубные и косметические кремы, художественные краски и т. д. Олово потребляется производителями шелка, главным образом для придания веса и «хруста» их продукции.

В 1917 году потребление олова в Соединенных Штатах составило приблизительно 93 000 тонн [141], из которых 19 000 тонн было получено из лома. Из общего объема потребления 31 000 коротких тонн было использовано для производства жести, 20 400 коротких тонн — для припоя, 13 800 коротких тонн — для антифрикционных сплавов (баббит, бронзы и т. д.) и 27 700 коротких тонн — для многих второстепенных целей, среди которых 1 000 тонн для шелковой промышленности, 5 000 тонн для фольги, 4 000 тонн для складных тюбиков, 3 000 тонн для белого металла.

[141] В этом отчете цифры для тонн относятся к метрическим тоннам (2204 фунта эвердьюпойс), если не указано иное, и приведены в круглых числах, поскольку ошибки в статистике и при конвертации не оправдывают более точных расчетов.

Трудно провести различие между основными и второстепенными видами использования олова в промышленности. Безусловно, жесть необходима, однако некоторая экономия оловянных контейнеров была достигнута во время военного дефицита за счет сокращения использования олова и замены его бумагой и другими веществами для упаковки непортящихся продуктов. Припои, антифрикционные сплавы и бронзы, несомненно, необходимы, но изменение спецификаций сплавов позволило в военный период добиться значительной экономии олова без ущерба для результатов. Фактически, некоторые стандарты, установленные в чрезвычайных условиях, были лучше тех, что использовались ранее. Алюминиевая фольга в некоторой степени заменяет оловянную, но подходящих заменителей олова для производства складных тюбиков, которые являются предметами первой необходимости, не найдено.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Более 70 процентов олова, производимого в мире, добывается из россыпных месторождений, хотя в последние несколько лет эксплуатация оловоносных жил приобрела значительное значение. Оловянные руды тесно связаны с кремнистыми изверженными породами. Практически все известные жильные месторождения находятся либо в кремнистых изверженных породах, таких как гранит, гранит-порфир, кварцевый порфир или монцонитовые типы, либо вблизи них. В Мексике и Соединенных Штатах незначительные оловянные месторождения были найдены в риолите. Только в одном или двух местах в мире известны оловянные жилы, где кремнистые изверженные породы не выходят на поверхность, и в этих местах геологические данные указывают на наличие гранитных пород на небольшой глубине. В главных мировых центрах производства олова — на Малайском полуострове, в Боливии, Австралии, Нигерии, Корнуолле и Южной Африке — гранитные породы повсеместно присутствуют, и оловянные жилы настолько тесно связаны с этими гранитами, что вопрос об их происхождении не возникает.

Фторсодержащие минералы, такие как флюорит и топаз, турмалин и вольфрамовый минерал вольфрамит, встречаются практически во всех оловянных месторождениях. Молибденит и висмутовые минералы присутствуют во многих оловянных месторождениях, хотя их распространение не так повсеместно, как у вышеупомянутых минералов. Сульфиды меди, свинца, цинка и железа (последние часто мышьяковистые) обычны в оловянных жилах, а кварц и полевой шпат являются главными жильными минералами.

Общепризнано, что оловянные жилы образовались ближе к концу интрузивной активности в результате окончательной дифференциации кислых магм. Эти конечные растворы примечательны своим пневматолитовым действием и способностью вызывать глубокое изменение гранита в грейзен, а также формирование станниферных пегматитов и кварцевых жил. Грейзен, продукт изменения гранита, состоит из кварца, слюды и различного количества топаза и турмалина. Он обычно развивается вдоль трещин, и в благоприятных местах большие массы породы могут быть грейзенизированы.

Оловянные месторождения чаще всего встречаются в виде жил, как трещинных, так и пегматитовых, или штокверков, но известны и некоторые сегрегации. Своеобразная трубчатая форма месторождения встречается местами в Трансваале и на Тасмании.

Как правило, оловянные месторождения залегают близко к контакту интрузивных и вмещающих пород и в основном находятся вблизи верхней части интрузивного массива. Отсюда следует, что в глубоко эродированных гранитных массивах вероятность обнаружения жильных оловянных месторождений меньше, чем при поиске в верхней части гранитных интрузий. Также было отмечено, что месторождения во вмещающих породах обычно залегают там, где падение интрузивного контакта пологое, и редко встречаются вдоль крутопадающего интрузивного контакта.

Практически единственным рудным минералом олова является касситерит (оксид олова), который содержит 78,6 процента металла. Касситерит известен в торговле под различными названиями, такими как оловянный камень, черный оксид олова, черное олово или, если он встречается в россыпях, шлиховое олово. Оловянные концентраты от россыпной добычи обычно содержат от 60 до 75 процентов металлического олова, при этом 70 процентов является средним показателем. Концентраты, получаемые на фабриках, перерабатывающих боливийское жильное олово, представляют собой продукт под названием барилья, который содержит в среднем около 62 процентов олова; концентраты, производимые из жил в Корнуолле, содержат в среднем около 65 процентов; а из жил и россыпей Малайского полуострова — около 72 процентов олова.

Во многих частях мира жилы не содержат достаточного количества олова для прибыльной разработки. В Корнуолле и на Тасмании добываются жилы, содержащие около 1 процента олова; но в целом содержание от 1 до 2 процентов олова является нижним пределом для коммерческой жильной добычи. В Боливии оловянные жилы содержат в среднем от 5 до 8 процентов олова, и были вскрыты некоторые рудные тела с содержанием до 40 процентов олова. В местах, где добывались низкосортные оловянные руды, побочные продукты, главным образом мышьяк и вольфрам, помогали покрывать расходы, и большинство этих рудников выгодно расположены по отношению к транспорту и снабжению. В россыпях Малайского полуострова, включая Банку и Биллитон, и Австралии, которые разрабатываются драгами, содержание олова варьируется от половины фунта до 3 фунтов, но в среднем составляет менее фунта касситерита на кубический ярд. Выгодное расположение и дешевая рабочая сила делают эксплуатацию прибыльной.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Как видно из карты, Таблица IX, оловянные месторождения встречаются во всех частях мира, хотя изучение Таблицы 60 и рисунка 9 покажет, что месторождения в пределах Британской империи являются наиболее важными источниками мировых поставок. Боливия и Голландская Ост-Индия были главными производителями олова за пределами Британской империи, хотя Китай и Сиам неуклонно приобретают значение как производители олова.

Британская империя.

— Британская империя имеет оловянные месторождения в Англии, Азии, Австралии и Африке. Крупнейшее производство приходится на месторождения на Малайском полуострове. Африканские месторождения, те, что в Нигерии и Южно-Африканском Союзе, дают второй по величине объем производства империи, австралийские месторождения занимают третье место, а месторождения Корнуолла, ранее крупнейшего производителя олова в мире, теперь занимают четвертое место.

Малайский полуостров.

— Федеративные Малайские Штаты и Британские защищаемые Малайские Штаты занимают южную оконечность Малайского полуострова. Этот регион, который полностью контролируется британцами, в течение многих лет производил половину мирового объема олова, но в последние несколько лет производство неуклонно снижается. Снижение, по-видимому, связано с истощением легко разрабатываемых россыпных месторождений, хотя в 1917 и 1918 годах дополнительной причиной была нехватка рабочей силы.

Таблица IX. — Месторождения олова в мире. Автор: Джеймс М. Хилл.

Рис. 9. — Мировое производство олова, 1913-1918 гг., в метрических тоннах.

Таблица 60. — Мировой объем производства металлического олова, 1913-1918 гг., в метрических тоннах [142] (Металл, получаемый плавкой из концентратов)

Country | 1913 | 1914 | 1915 | 1916 | 1917 | 1918
Cornwall | 5,370 | 5,140 | 5,060 | 4,770 | 4,000 | 4,000
Nigeria | 2,950 | 4,590 | 4,630 | 5,150 | 7,070 | 7,000
Union of South Africa | 2,050 | 2,000 | 2,050 | 1,900 | 1,540 | 1,500
Federated Malay States | 50,930 | 49,820 | 47,520 | 44,570 | 40,470 | 37,970
British Protected Malay States | 1,800 | 2,700 | 4,170 | 4,450 | 4,500 | 4,500
Australia | 8,160 | 5,520 | 5,680 | 5,550 | 4,970 | 4,900
Total British Empire | 71,260 | 69,770 | 69,110 | 66,390 | 62,550 | 59,870
Percentage world total | 52.6 | 54.1 | 53.7 | 52.  | 47.  | 45.8
Banca | 15,940 | 14,630 | 13,660 | 14,460 | 13,540 | 11,000
Billiton and Singkep | 5,300 | 6,090 | 6,760 | 6,780 | 7,300 | 9,200
Total Dutch | 21,240 | 20,720 | 20,420 | 21,240 | 20,840 | 20,200
Percentage world total | 15.4 | 16.1 | 15.4 | 16.7 | 16.  | 15.5
China | 8,390 | 7,120 | 8,000 | 7,630 | 11,800 | 12,000
Siam | 6,660 | 6,740 | 8,520 | 8,960 | 8,600 | 8,600
Bolivia | 26,760 | 22,360 | 21,900 | 21,330 | 28,320 | 28,000
Other countries | 1,400 | 1,500 | 1,500 | 1,700 | 1,800 | 2,000
Total other control | 43,210 | 37,720 | 39,920 | 39,620 | 50,520 | 50,600
Percentage world total | 32.  | 29.8 | 30.9 | 31.3 | 38.  | 38.7
World total | 135,710 | 128,210 | 129,450 | 127,250 | 133,910 | 130,670

[142] Кнопф А., «Олово в 1918 году», Геологическая служба США, «Минеральные ресурсы Соединенных Штатов в 1918 году».

Крупнейшим центром плавки олова в мире является Сингапур, где компании Straits Trading Co. и Eastern Smelting Co., обе британской собственности, а также плавильный завод, принадлежащий китайцам, имеют общую мощность 58 000 метрических тонн металла в год.

Большое количество малайзийских рудников разрабатывается китайцами, хотя значительный английский и австралийский капитал инвестирован в оловодобывающие компании на полуострове, и финансовый контроль над отраслью находится в руках британских подданных. Политический контроль осуществляется посредством запретительной экспортной пошлины (285 долларов за тонну) на всю оловянную руду, экспортируемую для переработки, за исключением поставок в Стрейтс-Сетлментс, Соединенное Королевство или Австралию.

Как видно из Таблицы 60, Федеративные Малайские Штаты производят гораздо больше олова, чем Защищаемые Штаты. Практически все олово на полуострове добывается из россыпных месторождений, некоторые из которых до сих пор разрабатываются ручными методами, хотя часть черного олова теперь добывается драгами.

Хребет Малайского полуострова состоит из гранита, который является интрузивным по отношению к известняку, сланцу и кварциту. Олово было найдено в коренном залегании практически во всех горных породах. Из-за интенсивного выветривания и эрозии оловоносных формаций во всех частях полуострова встречаются большие скопления детрита, более или менее смешанного с глиной, которые содержат касситерит. Первичные месторождения настолько размягчены выветриванием, что их можно разрабатывать гидравлическими методами.

Провинции Перак, Селангор, Паханг и Негри-Сембилан в Федеративных Малайских Штатах производят олово. Следующая таблица показывает их относительную важность.

Таблица 61. — Производство олова в Федеративных Малайских Штатах в 1917 году

| Metric tons
Perak | 25,075
Selangor | 10,595
Pahang |  3,750
Negri Sembilan |  1,055

В Негри-Сембилане кварцевые жилы в разложившемся пегматите разрабатываются гидравлическим способом, а полученный смешанный оловянно-вольфрамовый концентрат дополнительно разделяется на магнитных сепараторах. Основные рудники находятся недалеко от Тити и Серембана.

Паханг, на восточной стороне гор, имеет много широко разбросанных оловянных месторождений, как жильных, так и россыпных. Основные разработки в настоящее время ведутся в горах недалеко от границы с Селангором, в Бентонге, Трасе и Мачи. Некоторая добыча также ведется в различных местах вдоль реки Куантан и ее притоков. Транспортировка является серьезным пунктом расходов при разработке оловянных рудников в Паханге.

Куала-Лумпур является центром наиболее важных оловодобывающих операций в Селангоре. Разрабатываются как разложившийся жильный материал, так и гравий. Рядом с Серендахом разложившийся грейзенизированный гранит разрабатывается с помощью мониторов. Рядом с Танджунг-Малимом, а также на реках Калумпанг и Селангор в северной части штата разрабатываются как гравий, так и разложившийся жильный материал.

Район Кинта в штате Перак является наиболее важным оловодобывающим районом в Федеративных Штатах. Структурная долина, эродированная в мягких известняках между гранитными хребтами, является местом расположения большинства разработок. Долина заполнена глинами и валунными глинами, содержащими олово, а современные русла рек также являются оловоносными. Добыча ведется вокруг 15 или более поселений в этом районе; большая часть добычи ведется открытым способом и драгами, но некоторая жильная добыча ведется в трубках в известняках. Вторым по значимости после Кинты является район Ларут, к северо-западу от первого. Россыпные месторождения являются основным источником олова в районе, но жилы разрабатываются в Селаме и Бланда-Мабок. На юге Перака, в Брусе, штокверки в сланцах разрабатываются гидравлическим способом, давая около трех четвертей фунта на кубический ярд разрабатываемого материала.

Развитие оловянных месторождений в Защищаемых Малайских Штатах сдерживалось транспортными трудностями. До недавнего времени аллювиальное олово добывалось примитивными местными методами. Основная добыча приходится на штаты Джохор, Кедах, Келантан, Перлис и Тренгану.

Рядом с Сетулом, в штате Перлис, для добычи олова использовались своеобразные заполненные гравием пещеры в известняке. Некоторые из этих пещер были пройдены на четыре или пять миль. В штате Тренгану ведется жильная добыча под европейским управлением. Жилы, по-видимому, представляют собой разложившиеся штокверки в граните.

Незначительное количество олова добывается из пляжных месторождений на острове Малакка, Стрейтс-Сетлментс. Олово было получено из сланцев, прорванных гранитом, в которых имеется много оловоносных прожилков.

Африка.

— Как видно из Таблицы 60, основное производство олова в Африке приходится на Британскую Нигерию. Район разрабатывался местными жителями в ранние времена, но значительного производства не было до 1904 года, после подчинения эмира Баучи. Производство в Нигерии неуклонно росло, пока не достигло 8 500 тонн концентратов в 1917 году. По-видимому, все рудники контролируются британским капиталом, и экспорт в основном осуществлялся на плавильные заводы в Англии.

Аллювиальные месторождения Нигерии находятся в долинах плато Баучи. Щелочной гранит и пегматиты, интрузивные в более древние кристаллические породы, по-видимому, являются источником касситерита, который был сконцентрирован современными потоками. Шлюзование является основным методом добычи, хотя некоторые месторождения подходят только для драгирования. Олово также известно в северной Нигерии в холмах Нинги и Бурра, а также в других местах. В южной Нигерии олово было найдено недалеко от Аквы-Ибами, в районе Увет.

Добыча олова в Южно-Африканском Союзе ведется главным образом в районе Уотерберг-Заайплаатс в западном Трансваале, небольшое количество олова добывается в Свазиленде и Капской провинции. Производство варьировалось от 2 950 до 3 450 тонн концентрата в год, большая часть которого до войны шла в Англию для плавки, но с 1915 года — в Стрейтс-Сетлментс. Небольшой плавильный завод мощностью 250 тонн в год был построен в Заайплаатсе в 1917 году; ожидается, что он будет обеспечивать оловом потребности Южной Африки.

Район Уотерберг содержит несколько оловянных месторождений. Оловянные руды встречаются в красном граните и уотербергских фельзитах, песчаниках и конгломератах. В первых руды встречаются в трубках, в неправильных телах измененного гранита, вкраплены в гранит, в виде пропиток вдоль трещин, а также в пегматитах и кварцевых жилах. В серии Уотерберг оловянные руды находятся в жилах, а также в неправильных линзах и карманах, положение которых определяется трещинами или плоскостями напластования.

В районе Потгитерсруст основные рудники — это в основном трубчатые месторождения в красном граните. Эти трубки, которые очень изменчивы по направлению, варьируются от нескольких дюймов до 20 футов в диаметре; некоторые из них были пройдены на 3 000 футов. Заполняющий материал сильно варьируется, от слегка измененного гранита до зеленоватой однородной породы; внешние зоны представляют собой турмалин-кварцевую породу. В меньших трубках касситерит распределен довольно равномерно, но в больших трубках он встречается вблизи внешних краев.

В районе Нилстром основные рудники разрабатывают рудные месторождения в фельзитах и сланцах нижней серии Уотерберг. Месторождения представляют собой брекчированную вмещающую породу, сцементированную кварцем, турмалином, касситеритом и флюоритом.

Месторождение Уормбатс включает несколько рудников, расположенных вдоль стыка красного гранита и фельзитов. Олово встречается в жилах в обоих типах пород, также добывалось некоторое количество аллювиального олова. В месторождении Руберг оловянные месторождения практически все находятся в трещинах в кварците, прорванном красным гранитом. Олово встречается в красном граните в 40 милях к северу от Претории.

В Капской провинции, недалеко от реки Куилс, касситерит встречается в виде вкраплений в граните и в жилах на контакте гранита и сланцев. Большая часть добытого небольшого количества олова была получена из гравия, образовавшегося из этих месторождений.

В северо-западном Свазиленде аллювиальные месторождения разрабатывались в течение ряда лет, производя около 500 тонн концентратов в год. На рифе Форбс сланцы были прорваны гранитом, и оловянные жилы встречаются вблизи контакта двух формаций.

Сообщалось об олове в россыпных месторождениях в районе Виннеба и в пегматитовых дайках в районах Манкофа и Маунт-Манквади на Золотом Берегу. Олово было найдено в россыпных концентратах из ручьев в Ньясаленде. Оловянные месторождения, по-видимому, малой ценности, были найдены в районе Энтерпрайз, к востоку от Солсбери, и в районе Нданга, к востоку от Виктории, в Родезии. Эти месторождения представляют собой станниферные пегматиты, которые встречаются в сланцах вблизи гранита.

Австралия.

— Олово производится в следующих провинциях Австралии: Тасмания, Квинсленд, Новый Южный Уэльс, Западная Австралия, Северная территория, Виктория, названные в порядке их важности. В 1907 году объем производства на Тасмании составлял около 14 000 тонн концентратов, но с тех пор производство неуклонно снижалось, пока не стало почти стабильным на уровне 3 000 тонн ежегодно в последние несколько лет, и считается, что этот объем производства может поддерживаться в течение некоторого времени.

Существуют заводы по плавке олова в Лонсестоне (Тасмания), Вулвиче (недалеко от Сиднея, Новый Южный Уэльс) и Ирвайнбэнке (недалеко от Хербертона, Квинсленд), способные производить более 4 200 тонн металлического олова в год. В последние годы оловянный концентрат отправляется на плавку в Стрейтс-Сетлментс (Сингапур). Экспорт металлического олова из австралийских портов в 1917 году составил около 3 100 тонн.

Практически все горнодобывающие компании контролируются австралийским и английским капиталом, и, поскольку олово плавится либо на месте, либо в Сингапуре, весь австралийский объем производства можно считать находящимся под прямым политическим и коммерческим контролем Англии.

Общий объем производства оловянной руды на Тасмании [143] с 1880 по 1918 год включительно составляет приблизительно 128 200 тонн.

[143] Тасмания, Отчет секретаря по горному делу за год, заканчивающийся 31 декабря 1918 года, стр. 46.

Самым важным оловянным рудником является Маунт-Бишофф, в 45 милях к юго-западу от Эму-Бэй. Месторождения, открытые в 1871 году, имеют общий объем производства около 75 000 тонн оловянной руды. Существует несколько месторождений, представляющих собой мягкие измененные кварцевые порфиры, интрузивные в сланцы. Топаз и касситерит вкраплены в порфиры, а жилы, содержащие олово и вольфрамит, вместе с пиритом и арсенопиритом, встречаются как в порфире, так и в сланцах.

Рудник Шеперд и Мерфи, недалеко от Миддлсекса, находится в зоне метаморфизма на контакте гранита, интрузивного в песчаник и кварцит. Из этой руды добываются олово, вольфрам и висмут. Россыпные оловянные месторождения на реке Рингарума (район Дерби) поставляют около 1 000 тонн оловянных концентратов в год. Основными россыпными рудниками являются Пайонир и Брайсис. Рядом с Глэдстоуном разрабатываются россыпные и жильные месторождения, содержащие олово и вольфрам. На руднике Анкор в районе Блу-Тир разрабатывается оловоносный гранит с содержанием олова в среднем полпроцента, но добыча не была прибыльной. Рудники Ренисон-Белл, Дредноут-Боулдер и Монтана в районе Норт-Дандас находятся в сланцах, прорезанных дайками кварцевого порфира. Сульфиды цинка, свинца и железа важны в жилах. В районе Химскирт, юго-западная Тасмания, оловянные месторождения находятся в граните и в перекрывающих его сланцах и песчаниках. На руднике Федерация руда находится в трубке размером 25 на 15 футов на поверхности, но сужающейся до 1 на 5 футов на глубине 115 футов.

Олово впервые было добыто в Квинсленде в 1872 году, и общий объем производства, включая 1917 год, оценивается примерно в 144 008 тонн. Основными добывающими районами являются Хербертон, Куктаун, Чиллаго (недалеко от порта Кэрнс), Станнхиллс, Кенгуру-Хиллс и Станторп, причем последний находится недалеко от границы с Новым Южным Уэльсом. В районах Хербертон-Куктаун олово встречается в грейзенизированном граните, прорванном сланцами, слюдистыми сланцами и кварцитом; с ним связаны минералы висмута и вольфрама. Россыпные месторождения разрабатываются гидравлическим способом, и местами оловоносный грейзен разрушается гидравлическими мониторами. В месторождении Станнхиллс, недалеко от Кройдона, касситерит встречается в жилах в граните вместе с галенитом, сфалеритом и халькопиритом. Кенгуру-Хиллс, в 100 милях к югу от Хербертона, производит как жильное, так и россыпное олово. В районе Станторп большая часть продукции поступает из россыпных месторождений, некоторые из которых погребены под базальтами.

Олово впервые начали добывать в Новом Южном Уэльсе в 1872 году, и общее производство, включая объем 1917 года, оценивается в 84 230 тонн олова и 34 510 тонн оловянных концентратов.

Основными добывающими районами являются регион Веджитабл-Крик и Эммавилл-Тинга-Инверелл на северо-востоке недалеко от границы с Квинслендом и район Ардлетан, в 40 милях к западу от Теморы, на юге. В регионе Эммавилл-Инверелл эрозия станниферного грейзенизированного гранита, интрузивного в сланцы, привела к широкому распространению оловянных россыпей как в современных руслах рек, так и в том, что считается руслами третичных рек, которые теперь покрыты лавами. Рудники Веджитабл-Крик, недалеко от Эммавилла, типичны для более старых россыпных месторождений. С 1900 года драгирование стало важным, и, по оценкам, объем производства драгами до 1917 года составил 18 854 тонны концентратов. Жильная добыча, хотя и менее важная, велась в этом районе в трубках и штокверках в граните; типичные фторсодержащие жильные минералы обычны, и встречаются минералы вольфрама, висмута, меди и свинца.

Олово было обнаружено в районе Ардлетан в 1912 году в жилах в граните и сланце. Молибден, висмут и вольфрам обычно связаны с оловом в жилах грейзенизированного гранита. Барьерный район в западной части провинции не был крупным поставщиком из-за нехватки воды. Касситерит встречается в дайках крупнокристаллического гранита, интрузивного в грейзен и слюдяной сланец.

В Западной Австралии наиболее важными оловодобывающими районами являются Гринбушес на юго-западе и Пилбара на северо-западе, хотя было очень небольшое извлечение олова на золотом прииске Мерчисон и в Кулгарди. В районе Гринбушес касситерит встречается в пегматитовых и кварц-турмалиновых жилах в граните, но добытое олово поступает из речных отложений и латерита. В месторождении Пилбара аллювиальное олово было получено из пегматитовых даек, которые прорезают гранит и метаморфические породы.

Производство олова на Северной территории составляло около 200 тонн в год, большая часть которого была получена из пегматитовых месторождений в граните в окрестностях Буррунди.

Несколько тонн оловянных концентратов ежегодно сохраняется при эксплуатации золотых россыпей в Северо-Восточном и Гиппслендском подразделениях штата Виктория.

Индия.

— Основной объем производства олова в Индии приходится на районы Мергуи и Тавой в южной Нижней Бирме; районы Тартон и Амхерст в северной Нижней Бирме; и Южные штаты Шан. Производство составляет около 150 тонн металлического олова в год и отправляется на плавку в Стрейтс-Сетлментс.

В районе Мергуи касситерит встречается в аллювиальных отложениях недалеко от гранитных холмов, причем гранит является интрузивным в осадочные породы неопределенного возраста. Оловянная руда также встречается в пегматитовых и кварцевых жилах. В районе Тавой олово получается как побочный продукт добычи вольфрама. Месторождения встречаются в пегматитовых и кварцевых жилах, прорезающих гранит и осадочные породы. В районе Тартон оловоносный аллювий, как говорят, богат, и его развитие ожидается с интересом. Производство олова началось в 1912 году из месторождений штата Бавлаке, Каренни, Южные штаты Шан, и в 1917 году эти месторождения были главными производителями в Индии.

Корнуолл.

— На крайнем юго-западе Англии находится знаменитый оловянный регион Корнуолл, который включает районы Камборн, Сент-Остелл и Лискерд в Корнуолле и район Тависток в Девоне. Рудники производили около 8 000 тонн концентратов в год, но в настоящее время объем производства, по-видимому, уменьшается; в 1915 году производство металлического олова составляло приблизительно 5 000 тонн, но в 1918 году — только около 4 000 тонн.

Добыча олова в Корнуолле восходит к доисторическим временам. В XVI веке рудники производили около 700 тонн олова в год; максимальный объем производства был достигнут в период с 1860 по 1890 год, когда ежегодно производилось около 10 000 тонн. По оценкам, общий объем производства олова в этом районе составляет приблизительно 1 750 000 тонн. Горнодобывающие компании без исключения контролируются британским капиталом.

Вторая по величине мощность по плавке олова в мире находится в районе Корнуолла. Следующие компании: Williams Harvey & Co., Penpoll, Cornish Tin Smelting Co., Copper Pass, Redruth Tin Smelting Co. и London Smelting Co. — эксплуатируют плавильные заводы с общим объемом производства приблизительно 31 100 тонн олова в год.

Оловянные месторождения Корнуолла и Девона залегают около пяти массивов гранита, которые прорывают сланцы (киллас) и зеленые камни. Дайки кварцевого порфира тесно связаны с гранитом, и оловянные жилы встречаются как в сланцах, так и в граните, будучи особенно обильными вблизи интрузивных контактов с пологим падением. Основные жилы представляют собой широкие зоны трещиноватых пород, которые подверглись турмалинизации, а менее важные трещины содержат олово и жильные минералы. Из этих жил добываются минералы меди и вольфрама, а мышьяк является важным побочным продуктом плавки. Жилы в сланцах, как правило, богаче медью, чем в граните, и на глубине жилы содержат большую долю олова, чем ближе к поверхности. Рудники вокруг гранитного массива Камборн дают около 85 процентов добываемого олова, рудники вокруг гранитного массива Лэндс-Энд — 12 процентов, а рудники вокруг Сент-Остелла, Бодмин-Мура и Дартмура — около 1 процента каждый.

Практически все олово, произведенное в последние годы, было получено из жил, но россыпное олово добывалось недалеко от Сент-Остелла. Жилы разрабатывались на глубину 3 000 футов, что, по-видимому, является наибольшей глубиной, на которую распространяется коммерчески выгодная руда. Поскольку значительная часть грунта выше этого уровня остается неразработанной, район должен оставаться продуктивным еще некоторое время.

Другие страны.

— За пределами Британской империи основные оловянные месторождения мира находятся в Боливии, Голландской Ост-Индии, Китае и Сиаме, названные в порядке их важности как производителей в 1918 году. Существуют небольшие объемы производства олова из месторождений в Японии, Испании, Португалии и Соединенных Штатах, а оловянные месторождения известны в Германии, Италии, России, Бельгийском Конго и Юго-Западной Африке.

Боливия.

—Практически вся оловянная руда, вывозимая из Боливии, добывается из жил. Горные работы начались в конце прошлого века. Экспорт осуществляется в виде «барильи» — оловянного концентрата с содержанием олова от 60 до 65% (в среднем около 62%). Объем добычи неуклонно растет, и с 1913 года Боливия является вторым по величине производителем олова в мире. (См. Таблицу 60 и Рисунок 9). Большинство компаний, работающих в Боливии, контролируются чилийским или местным капиталом, хотя до войны в боливийские оловянные рудники были вложены небольшие суммы английского, французского, швейцарского и немецкого капитала. В последнее время интерес к этим месторождениям проявили английские и американские инвесторы.

До войны практически вся «барилья» отправлялась на плавку в Германию и Англию, но в последнее время экспорт идет в Соединенные Штаты и Англию. Недавно в Арике был построен небольшой чилийский плавильный завод с расчетной мощностью 900 тонн в год для переработки концентратов с одного из крупных рудников.

В восточной части центральной Боливии, в провинциях Потоси, Оруро и Ла-Пас, расположены четыре важных оловодобывающих района. Этот регион находится на высокогорном плато (высота 12 000 футов), и основные рудники расположены рядом с горами к востоку от пампы или в самих горах, а не в западном хребте Кордильер. Сланцы, глинистые сланцы и кварциты были прорваны кислыми магматическими породами, и оловянные месторождения встречаются в гранитах, кварцевых порфирах и осадочных породах вблизи контактов. Кварцевые жилы мощные и содержат от 3 до 8% олова на большинстве продуктивных рудников, хотя некоторые рудные тела содержали до 40% олова. Некоторые рудники разрабатывались испанцами ради серебра, но серебряные руды, по-видимому, ограничены верхними зонами, а жилы становятся относительно богаче оловом на глубине. Вольфрамит и висмут добываются как побочные продукты на некоторых рудниках. Пирит, сфалерит, халькопирит и галенит обычно в изобилии присутствуют в оловянных рудах, нередко встречаются турмалин и флюорит.

Боливийские месторождения имеют значительную перспективную ценность. Многие рудники и перспективные участки не были освоены из-за нехватки знаний или финансовых средств; местное управление на большинстве рудников было крайне неудовлетворительным, и считается, что при надлежащем техническом руководстве добычу олова можно значительно увеличить.

Голландская Ост-Индия.

—На островах Банка, Биллитон и Синкеп, к югу от Малайского полуострова, находятся важные оловянные рудники. Как видно из Таблицы 60, добыча олова на этих островах составляла примерно 21 000 тонн в год. Добыча на Банке началась около 1718 года, но месторождения на Биллитоне начали разрабатываться только около 1860 года. Рудники на Банке эксплуатируются правительством, а на Биллитоне и Синкепе месторождения сдаются в аренду частным компаниям, преимущественно голландским. На Банке голландское правительство управляет плавильными заводами с годовой мощностью 16 000 тонн. Концентраты, производимые на Биллитоне и Синкепе, частично отправляются на переработку в Стрейтс-Сетлментс, но часть из них плавится на месте.

Практически все олово, добываемое в Голландской Ост-Индии, поступает из россыпных месторождений, некоторые из которых являются аллювиальными. Однако на Биллитоне ведется небольшая жильная добыча. Касситерит образовался в грейзенизированных гранитах и осадочных породах, и первичные месторождения схожи с месторождениями Малайского полуострова. Небольшое количество вольфрама и золота получается в качестве побочных продуктов при добыче олова.

Китай.

—Оловянные месторождения в районе Мэнцзы, недалеко от Коцю, провинция Юньнань, юго-восточный Китай, разрабатываются уже много лет. В последние годы экспортировалось около 8000 тонн олова, и известно, что значительная часть оловянной руды, добываемой на этих месторождениях, плавится на месте, а металл потребляется в Китае. Экспорт осуществляется через французский порт Хайфон. Горнодобывающая промышленность полностью находится под китайским контролем. Большая часть оловянной руды добывается россыпным и открытым способами из разрушенных гранитных и пегматитовых жил, которые встречаются вблизи контакта гранита, внедрившегося в известняк. Существуют менее значительные оловянные месторождения в районах Фучуань и Тунчуань, причем первый из них дает металл очень высокой чистоты.

Экспортируемые оловянные концентраты направляются в основном в Гонконг и Стрейтс-Сетлментс для переработки, поэтому объем добычи олова в Китае в той или иной степени находится в распоряжении Англии.

Сиам.

—В той части Сиама, которая расположена на Малайском полуострове, разрабатываются оловянные месторождения, схожие по происхождению и условиям залегания с месторождениями в британских провинциях, и, как показано в Таблице 60, они с каждым годом становятся все более значимыми факторами в мировом объеме добычи. Крупнейшие операции ведутся вблизи Ренонга и Тонгки, где активно работают драги британских компаний. Основными добывающими компаниями являются Tongkah Harbor Tin Dredging Co., Tin Benbong, Bangnon Valley, Ronpibon Extended, Beebook Dredging Co. и Katoo Syndicate.

Япония.

—Месторождения олова в Японии расположены вблизи Кагосимы, Сацума, на острове Кюсю; примерно в 50 милях к северу от Кобе в провинции Тадзима; и недалеко от Наеги, провинция Мино, в центре главного острова. Россыпные месторождения вблизи Наеги дали некоторое количество олова, по-видимому, происходящего из пегматитовых жил в граните. Рудник Акинобе в провинции Тадзима разрабатывался как медный рудник, но около 1912 года в руде были обнаружены оловянные и вольфрамовые минералы. Жилы залегают в сланцах и кварцитах, прорванных диоритами. Говорят, что в 1917 году ежедневно добывалось около 40 тонн смешанных оловянно-вольфрамовых руд. Небольшой плавильный завод в Икуно перерабатывает оловянные концентраты и производит около 250 тонн олова в год. Рудник Сусуияма в Сацуме добывает олово из жил в сланцах и песчаниках, которые также содержат свинец и цинк. По-видимому, продукция плавится и используется на месте.

Испания.

—В провинциях Саламанка, Самора, Оренсе, Понтеведра и Ла-Корунья на северо-западе Испании имеются оловянные месторождения. Жильные месторождения встречаются вблизи контакта гранита, внедрившегося в сланцы и гнейсы, а россыпные месторождения разрабатываются с древних времен. Сообщается, что в 1913 году было добыто около 6700 тонн руды, но с тех пор объем добычи составляет около 100 тонн в год.

Португалия.

—В Португалии, к югу от испанской границы, были найдены оловянные жилы в гранитах и сланцах, а в гравийно-песчаных отложениях, прилегающих к жилам, велась добыча из россыпей. Ежегодная добыча на этих месторождениях составляет около 300 тонн. Сообщается, что американский капитал проявляет интерес к некоторым португальским месторождениям олова и вольфрама.

Соединенные Штаты.

—В Соединенных Штатах внутренняя добыча является лишь номинальной и эквивалентна 60–100 тоннам олова в год. Продуктивные месторождения — россыпи, разрабатываемые драгами, — находятся в районе Йорк на полуострове Сьюард, Аляска. Они залегают вблизи контакта гранита, внедрившегося в известняки, в специфических породах контактово-метаморфического происхождения.

Касситерит добывался из гравия, образовавшегося из пегматитовых жил, внедрившихся в докембрийские породы Блэк-Хилс вблизи Тинтона и Хилл-Сити, Южная Дакота, и предпринимались различные попытки разработки жильных месторождений. Эти месторождения представляют скорее научный интерес, чем коммерческую важность. Небольшое количество олова было также добыто на границе Северной и Южной Каролины вблизи Кингс-Маунтин, где касситерит является первичным компонентом пегматитовых жил, внедрившихся в докембрийские сланцы. В Айриш-Крик, округ Рокбридж, Виргиния, известны оловоносные жилы в грубозернистых гранитах. В горах Франклин в 14 милях к северу от Эль-Пасо, Техас, когда-то разрабатывались кварцевые жилы в граните, содержащие касситерит, но в последнее время они не приносят продукции. В горах Темескал, округ Риверсайд, Калифорния, небольшие кварцевые жилы с касситеритом встречаются в кислых гранитных породах, внедрившихся в метаморфизованные осадочные породы. В этой местности значительные работы проводились в 1880–1890 годах, но нерегулярность месторождений и низкое содержание олова не дают больших надежд на будущую добычу.

До войны Соединенные Штаты, будучи крупнейшим потребителем олова в мире, практически не производили оловянной руды и импортировали только металлическое олово, не имея плавильных заводов для переработки оловянной руды. С 1916 года плавильные заводы были построены компаниями American Smelting & Refining Co. и Williams Harvey Corporation, их расчетная мощность составляет 18 000 тонн олова в год. По-видимому, эти заводы должны в значительной степени полагаться на боливийские концентраты.

Германия-Австрия.

—Германия в последние годы практически не производила оловянных руд, хотя в стране существовала плавильная промышленность с расчетной мощностью около 16 000 тонн олова в год, зависящая от иностранных руд. Нормальный импорт оловянной руды до войны составлял 17 000–18 000 метрических тонн в год, большая часть которой поступала из Боливии.

В Рудных горах (Эрцгебирге), на германо-австрийской границе, в районе Альтенберг-Циннвальд, ранее велась добыча олова. Месторождения, представляющие собой типичный грейзен, залегающий вблизи вершин и склонов гранитных тел, внедрившихся в сланцы и гнейсы, в течение нескольких лет практически не дают продукции и считаются истощенными.

Италия.

—В Кампилья-Мариттима, Тоскана, железо и олово добывались из жил в известняке и сланцах. Объем добычи изменчив и на него нельзя полагаться.

Россия.

—В бывшей Российской империи олово было найдено в Забайкальской области, Сибирь, а также на Урале и в Финляндии в европейской части России. Сибирские месторождения представляют собой россыпи в бассейне реки Онон. Перед войной была создана немецкая компания для разработки жильных оловянных месторождений вблизи Оловянной, к юго-западу от Нерчинска, на Урале. Финские месторождения находятся в Питкяранте, к северу от Ладожского озера. Руды представляют собой смесь магнетита, касситерита и халькопирита, залегающих в измененных известняках и сланцах.

Бельгийское Конго (Катанга).

—Аллювиальное олово, происходящее из жил в граните и внедрившихся осадочных породах, было найдено вдоль реки Луалаба и на хребте Бусанга. Записей о добыче нет, но месторождение подает значительные надежды.

Юго-Западная Африка.

—Касситерит встречается в пегматитах, внедрившихся в гранит, в горах Эронго к востоку от Брандберга, также велась разработка некоторых россыпных месторождений олова. В целом регион не кажется особенно перспективным.

ВЕРОЯТНЫЕ ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРЕДЕЛЕНИИ

Представляется вполне вероятным, что Англия в состоянии продолжать добычу значительной части мирового олова в течение некоторого времени, при этом снижение добычи в малайских провинциях будет компенсироваться увеличением производства в африканских колониях. Считается, что Корнуолл и Австралия смогут в течение ряда лет поддерживать довольно стабильный уровень добычи, близкий к нынешнему.

Боливия, несомненно, сможет увеличить добычу олова, и, вероятно, можно ожидать, что в будущем как Сиам, так и Китай будут производить большие количества. Добыча в Голландской Ост-Индии, вероятно, может поддерживаться на нынешнем уровне в течение ряда лет.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Как видно из Таблицы 62 и Рисунка 10, Великобритания политически контролирует более 50% мирового производства олова, поскольку ее политическое влияние является абсолютным в Англии, Африке, Австралии и всех ее колониальных владениях на восточной стороне Индийского океана; и не может быть сомнений в том, что жесткая британская политика в отношении восточных колоний также эффективна в отношении Сиама и Китая.

Рис. 10.—Политический контроль над оловянными месторождениями и плавильными заводами, основанный на оценках за 1918 год.

Голландия контролирует добычу олова в своих ост-индских колониях, где имеются плавильные заводы, которые, по-видимому, способны перерабатывать большую часть добываемой руды. Голландия сама потребляет мало олова и имеет в своем распоряжении примерно 16% мировых запасов. До войны Голландия была крупным дистрибьютором олова, но во время войны олово из ее колоний отправлялось напрямую в Америку и Англию, крупнейшие страны-потребители.

Китай имеет довольно слабый политический контроль над продукцией оловянных рудников Юньнани, но поскольку та часть его продукции, которая достигает остального мира, экспортируется через французскую территорию, в основном через английских посредников, его фактический контроль не особенно велик.

Сиам контролирует некоторые важные оловянные месторождения. Очень сильное британское влияние на Малайском полуострове в сочетании с тем фактом, что сиамская руда плавится в Стрейтс-Сетлментс, по-видимому, указывает на то, что британская политика будет в значительной степени доминировать в оловодобывающей промышленности Сиама.

Боливия, потребляющая мало олова и производящая почти четверть мирового объема, является, по сути, единственным крупным производителем, который может действовать более или менее независимо. Ее рудники в основном контролируются чилийско-боливийским капиталом, и ее рынок — весь мир. Казалось бы, боливийская «барилья» могла бы плавиться на месте, но поскольку в Боливии нет топлива, мощности по плавке олова в Боливии до сих пор практически равны нулю. Ее ближайший рынок в настоящее время — Соединенные Штаты, но будущее покажет, будет ли боливийская руда по-прежнему плавиться в Соединенных Штатах, как в последние несколько лет, или будет отправляться в Англию и Германию, как до войны.

Связь политического контроля над оловянными месторождениями и плавкой олова показана в следующей таблице и схематически на Рисунке 10.

Таблица 62.—Политический контроль над оловянными месторождениями и плавильными заводами на основе оценок за 1918 год

Country
Control of
tin deposits,
annual output
(metric tons)
Percentage
of
world output
Control of
tin smelters,
annual capacity
(metric tons)
Percentage
of
world capacity

Great Britain |  59,900 | 45.5 |  88,300 | 57.3
Holland |  20,200 | 15.2 |  16,000 | 10.2
China |  12,000 |  9.3 |  12,000 |  7.4
Siam |   8,600 |  7.0 |  |
Bolivia |  28,000 | 21.3 |   2,700 |  1.6
Germany | ... | ... |  16,000 | 10.2
France | ... | ... |   1,500 |  0.7
America | ... | ... |  18,000 | 12.4
All others |   2,000 |  1.7 |     500 |  0.2
Total | 130,700 |  | 154,000 |

КОММЕРЧЕСКИЙ КОНТРОЛЬ НАД ОЛОВЯННЫМИ РУДНИКАМИ

Британский капитал является доминирующим контролирующим фактором примерно 57% мирового производства олова, а благодаря связям с капиталом других стран он частично контролирует еще около 15%. Британский капитал доминирует во всех британских владениях и Сиаме, а через закупочные агентства практически контролирует экспорт олова из Китая. Боливийские оловянные рудники — единственные в мире, где британский контроль не ощущается сильно. Большая часть боливийской продукции находится под финансовым контролем чилийских финансистов, при этом местный капитал является вторым по значимости фактором. Французские и немецкие деньги были в ограниченной степени вложены в боливийские рудники.

Недавно фирма Guggenheim Brothers из Нью-Йорка, связанная с американской оловоплавильной промышленностью, приобрела определенные оловянные рудники в Боливии.

КОММЕРЧЕСКИЙ КОНТРОЛЬ НАД ПЛАВКОЙ ОЛОВА

Британский капитал контролирует плавильные заводы с годовой мощностью примерно 88 300 тонн олова в год. Они расположены в Англии, Стрейтс-Сетлментс и Австралии. Оловянные месторождения, находящиеся под несомненным британским контролем, могут дать руду только для производства 62 550 тонн, так что Англия имеет мощности по плавке, превышающие ее собственные запасы на 15 750 тонн в год.

Голландцы контролируют плавильные заводы мощностью 16 000 тонн в своих ост-индских колониях, но годовая добыча руды в этих колониях эквивалентна 20 200 тоннам олова, поэтому излишек в 4 200 тонн должен плавиться в другом месте, и большая его часть направляется на плавильные заводы в Стрейтс-Сетлментс, которые принадлежат англичанам.

Китайский капитал контролирует плавильные заводы, которые, по-видимому, способны перерабатывать весь объем добычи Китая — около 12 000 тонн олова в год.

Американский капитал после войны развил оловоплавильные заводы в Соединенных Штатах и Боливии, которые имеют годовую мощность 18 000 метрических тонн. Эта мощность расширяется и вскоре должна быть способна перерабатывать весь объем добычи боливийского олова при условии получения руды. Но чилийский капитал построил плавильный завод в Арике, который мог бы перерабатывать около 10% боливийской продукции, и если этот завод будет пользоваться поддержкой чилийских владельцев рудников, американские плавильные заводы могут столкнуться с нехваткой руды.

Немецкий капитал заинтересован в оловоплавильных заводах в Германии, имеющих производственную мощность 15 000 тонн в год. Вся перерабатываемая руда должна импортироваться, но вряд ли можно ожидать поступления большого количества руды из внешних источников в течение некоторого времени, поскольку мощности по плавке в мире превышают объем добычи на рудниках.

Мировая мощность по плавке олова составляет примерно 154 000 тонн, тогда как мировое производство оловянной руды эквивалентно примерно 130 700 тоннам. Очевидно, что если не будет достигнуто большего объема добычи, некоторые плавильные заводы будут простаивать, и разумно предположить, что ни британские, ни голландские заводы не будут испытывать недостатка в руде. Соединенные Штаты, благодаря своему благоприятному положению в отношении поставок из Боливии, могут надеяться на то, что значительная часть их плавильных мощностей будет работать, хотя существует вопрос, будет ли доступно достаточно руды для обеспечения максимальной загрузки оловоплавильных заводов в Соединенных Штатах.

ПОЛОЖЕНИЕ СТРАН-ПОТРЕБИТЕЛЕЙ ОЛОВА

Великобритания производит больше олова, чем потребляет, и поэтому находится в положении, позволяющем поставлять олово остальному миру. Из изучения таблиц импорта и экспорта следует, что Англия потребляет около 20 000 тонн олова в год, импортирует около 55 000 тонн и, следовательно, имеет 35 000 тонн для экспорта. Благодаря своему большому политическому и коммерческому контролю над оловянными месторождениями и плавильными заводами она может практически диктовать мировую политику в отношении олова.

Голландские колонии производят около 16% мирового олова, и, поскольку Голландия обычно является очень малым потребителем олова, она поставляла значительную часть олова, используемого в Германии и Соединенных Штатах.

До войны на юге России была создана значительная промышленность по производству жести, зависящая от иностранного олова. Потребление составляло около 8000 тонн олова в год, которые в основном поставлялись Великобританией, Голландией и Германией. Если эта промышленность сохранится, Россия по-прежнему будет вынуждена импортировать значительное количество олова.

Потребители олова в Германии, которые до войны, по-видимому, потребляли около 22 000 тонн олова, должны закупать все поставки у других. До войны основным источником оловянной руды была Боливия, а металлического олова — Голландская Ост-Индия. Представляется разумным, что поставки боливийской руды в Германию могут быть сокращены в будущем, поскольку Соединенные Штаты теперь в состоянии перерабатывать руду, а фрахтовые ставки должны способствовать отгрузке боливийской «барильи» в Соединенные Штаты, а не в Германию. Выживет ли немецкая оловоплавильная промышленность или нет — покажет время.

Франция имеет небольшую оловоплавильную промышленность, перерабатывающую около 1500 тонн в год. Видимое потребление составляет около 7000 тонн олова в год, большая часть которого ранее импортировалась из Британской Индии, Англии и Голландской Ост-Индии.

Соединенные Штаты ежегодно потребляют более 80 000 тонн олова, включая вторичный металл, и производят из отечественных руд около 100 тонн. До войны металлическое олово получали через Англию и Голландию, так как в этой стране не было оловоплавильных заводов. Во время войны была создана оловоплавильная промышленность, которая полностью зависит от иностранной руды, большая часть которой до сих пор поступала из Боливии. Расчетная мощность оловоплавильных заводов в Америке составляет около 18 000 тонн в год, или около 20% от расчетной годовой потребности. Объединение английского, боливийского и американского капитала заинтересовано в одном из этих заводов, а также в боливийских оловянных рудниках, и, вероятно, этот завод может быть обеспечен сырьем. Однако существует значительный вопрос, смогут ли другие заводы получить поставки боливийской руды. Безусловно, они столкнутся с конкуренцией со стороны как английских, так и немецких плавильных компаний, что будет в некоторой степени компенсироваться более дешевым фрахтом в Соединенные Штаты, чем через Атлантику. Эта разница, вероятно, невелика, и кажется, что если американские плавильные заводы хотят получать боливийскую оловянную руду, их издержки должны быть низкими. Более надежным методом удовлетворения их потребностей в руде было бы получение финансового контроля над достаточным количеством месторождений руды в Боливии для обеспечения спроса.

Очевидно, что Соединенные Штаты должны в будущем, как и в прошлом, импортировать значительные количества олова как из Великобритании, так и из Голландии. Следует надеяться, что торговые пути олова, установленные во время войны, могут быть сохранены и что американским потребителям не придется платить дополнительные расходы, вызванные тем, что восточное олово идет в Европу и обратно в Соединенные Штаты.

ГЛАВА XVIII РТУТЬ Ф. Л. Рэнсом

ПРИМЕНЕНИЕ РТУТИ

В нормальных условиях основные виды использования ртути (quicksilver) или ее солей, перечисленные в порядке убывания важности, следующие: в производстве лекарств и химикатов, включая каломель и сулему; в производстве определенных химических веществ, таких как ледяная уксусная кислота, фталевая кислота и фталевый ангидрид, в которые сама ртуть не входит; в качестве гремучей ртути ((C:N.O2)Hg, ¹⁄₂H2O), получаемой путем обработки ртути спиртом и азотной кислотой, которая используется как детонатор для мощных взрывчатых веществ и, хотя и в меньшей степени, чем раньше, в боеприпасах для стрелкового оружия.

Открытие гремучей ртути Говардом в 1799 году привело к изобретению капсюля-детонатора взамен старого кремневого замка, и гремучая ртуть до сих пор остается самым известным и наиболее используемым детонатором для пороха и мощных взрывчатых веществ. Ее часто комбинируют с другими веществами, особенно с абразивом, таким как порошкообразное стекло, для повышения чувствительности, а также с соединениями или смесями, которые сами обладают свойством детонировать, такими как сульфид сурьмы и хлорат калия. В последнее время значительная часть гремучей ртути в детонаторах для современных мощных взрывчатых веществ была заменена пикриновой кислотой, тринитротолуолом или тетранитрометиламином, благодаря чему достигается гораздо более сильный начальный эффект, и одна часть гремучей ртути заставляет детонировать заряд, для которого потребовалось бы в шесть раз больше гремучей ртути при использовании ее в чистом виде. Были найдены другие вещества, которые, по-видимому, могут полностью заменить гремучую ртуть для определенных целей. Одно из них — азид свинца, соль азотистоводородной кислоты. Крупные сухие кристаллы этой соли настолько чувствительны, что взрываются при прикосновении перышком, но более мелкие кристаллы менее чувствительны.

В виде сульфида ртути ртуть образует блестящий красный пигмент — киноварь. Металл широко применяется в электротехнических приборах, включая выпрямители для преобразования переменного тока в постоянный, ртутные лампы и аккумуляторные батареи. При производстве фетровых шляп из кроличьего меха нитрат ртути используется для придания волоскам шероховатости, чтобы они лучше сцеплялись друг с другом, — процесс, технически известный как «карротирование». Металлическая ртуть используется при амальгамации золотых и серебряных руд, хотя в последние годы широкое применение цианидного процесса снизило это использование. Металл также используется в производстве инструментов, термостатов, газовых регуляторов и других приборов. Ртуть входит в состав некоторых противообрастающих красок для днищ судов — современное и в настоящее время быстро растущее применение. Ртуть для этой цели обычно используется в виде красного оксида ртути, эффективность которого зависит от постепенного превращения оксида в ядовитый двухлорид под воздействием хлорида натрия морской воды. Ртуть также используется в определенных соединениях для предотвращения накипи в котлах, в косметике и в стоматологической амальгаме. Нитрат серебра в значительной степени заменил ртуть при серебрении зеркал. Небольшое количество ртути, не более двух-трех колб в год, используется для плавания некоторых типов вращающихся огней в маяках. Ртуть также используется в качестве катода в определенных электролитических процессах для производства хлора и каустической соды из поваренной соли. Оксид ртути легко отдает кислород и является полезным окислителем в определенных химических процессах. Важное современное использование этого свойства — производство ледяной уксусной кислоты путем окисления ацетилена.

Эксперименты по определению возможных преимуществ использования паров ртути вместе с паром в турбинных генераторах энергии, как сообщается, были обнадеживающими, и компания General Electric Co. построила установку мощностью 4000 киловатт для дальнейшего тестирования этого применения. За исключением случайных потерь, используемая таким образом ртуть подлежит восстановлению, но если на практике увеличение мощности будет таким, как показали экспериментальные работы, это, вероятно, приведет к большому потреблению металла.

The production of quicksilver in this country in 1917 was 35,954 flasks (of 75 pounds) and in 1918 it was 32,883 flasks.

ГЕОЛОГИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Руды ртути, как и руды большинства металлов, в целом демонстрируют тесную связь с магматическими породами и зонами трещиноватости. Чаще, чем в случае с другими металлами, за возможным исключением сурьмы, они связаны с вулканизмом, в отличие от плутонической магматической активности, и отлагались сравнительно близко к поверхности. Отсюда следует, что ртутные месторождения, как правило, встречаются в регионах третичной и четвертичной вулканической активности, которые не подвергались длительной и глубокой эрозии, что они с большей вероятностью находятся в более молодых геологических формациях, чем в более древних породах, и что как класс, по сравнению, например, с гипогенными рудами золота или меди, они не распространяются на большую глубину. Однако следует отметить, что существуют некоторые заметные исключения из этих обобщений. Хотя калифорнийские месторождения находятся в регионе поздней вулканической активности и многие из них тесно связаны с активными горячими источниками, рудные тела, которые сейчас являются наиболее продуктивными — те, что в Нью-Идрии (почтовое отделение Идрия), и огромные месторождения в Нью-Альмадене, которые ранее давали столь богатую добычу, — не имеют очевидной связи с вулканизмом. Крупнейший в мире ртутный рудник в Альмадене, Испания, не имеет известной связи с вулканизмом или массивными магматическими породами, разрабатывался на глубину 1150 футов, и было обнаружено, что рудные тела становятся больше и богаче с глубиной. Самый глубокий ртутный рудник в мире — Нью-Альмаден в Калифорнии, разрабатывавшийся на глубину 2200 футов. Часть рудника ниже уровня 600 футов была заброшена в то время, когда цена на ртуть была низкой, но сомнительно, чтобы при любых условиях, которые можно предвидеть сейчас, было выгодно вновь открывать и разрабатывать глубокие горизонты этого рудника.

Хотя большинство известных ртутных месторождений находятся в регионах геологически поздних вулканических извержений, вероятно, что руды ртути отлагались во время или вскоре после эпох подобной магматической активности в более древние геологические периоды, но многие из них были удалены эрозией. Некоторые месторождения в более древних породах, которые, по-видимому, не связаны с третичными или более поздними вулканическими извержениями, могли иметь такое более раннее происхождение.

Ртутные месторождения Адриатического региона в Европе, включая месторождения в Идрии (Австрия), Авале (Сербия) и Монте-Амиата (Италия), как показал Де Лоне, принадлежат к единой металлогенической провинции, характеризующейся третичными извержениями. Аналогичным образом, несколько разбросанные проявления ртути на Аляске, в Вашингтоне, Айдахо, Монтане, Орегоне, Неваде, Юте, Калифорнии, Аризоне, Мексике, Перу и Чили частично совпадают с поясом третичной и четвертичной вулканической активности вдоль западных сторон континентов Северной и Южной Америки. Месторождения в Альмадене (Испания), в Донецком бассейне (Россия), в азиатской части Турции и в Китае представляются изолированными проявлениями, которые в настоящее время нельзя отнести к распознаваемым провинциям эруптивной активности и металлогении.

Ртутные месторождения не ограничиваются породами какого-либо определенного вида или какого-либо определенного геологического возраста.

В Овьедо содержание руды составляет в среднем 0,33% и дает соединения мышьяка в качестве побочных продуктов. В Идрии руда дает 0,65%. Руда Аббадия-Сан-Сальваторе, главного рудника в районе Монте-Амиата в Италии, давала около 0,9% в 1915 году. В Калифорнии немногие рудники имеют руду с содержанием более 2%, а средний выход перерабатываемой руды составляет около 0,5%. Самый низкий выход, который был рентабельно получен в этом штате в 1917 году, составлял 0,185%. Руды, разрабатываемые в Техасе, как правило, более высокого качества, чем те, что добываются в Калифорнии. На главном руднике района Терлингуа, Техас, фактическое содержание руды в 1916 году составляло 2,5%, а в 1917 году — 3,9%.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Европа.

—Крупнейшее и богатейшее известное месторождение ртутной руды находится в Альмадене, в центральной Испании. Там есть три почти параллельных рудных тела, расположенных вертикально бок о бок, каждое из которых состоит из части пласта кварцита силурийского возраста, пропитанного киноварью. Рудные тела разрабатывались на глубину 350 метров. Добыча в 1917 году составила, вероятно, около 25 000 колб. Говорят, что на руднике вскрыта руда, обеспечивающая будущую добычу не менее 40 000 метрических тонн ртути. Другими продуктивными месторождениями в Испании являются месторождения вблизи Овьедо, где руда, содержащая киноварь, пирит, аурипигмент и реальгар, как говорят, содержит в среднем около одной трети 1% ртути, с соединениями мышьяка в качестве побочных продуктов. Согласно отчету вице-генерального консула Г. А. Макбрайда, написанному в Барселоне в 1911 году, основными компаниями, работающими в районах Овьедо, были Oviedo Mercury Mines Co., Ltd. из Лондона, Sociedad Fabrica de Mieres из Овьедо и Sociedad Union Asturiana из Мьереса. Добыча в этом районе в 1915 году составила 608 колб (20,7 метрических тонн). Третья группа месторождений находится на южном склоне Сьерра-Невады в провинциях Гранада и Альмерия, южная Испания. Добыча в Гранаде в 1915 году составила 41 колбу (1,4 метрических тонн).

Небольшое количество ртути было добыто в Португалии в девятнадцатом веке на руднике недалеко от Лиссабона. Киноварь встречается в ряде мест во Франции, а также на Корсике, но месторождения не имеют экономического значения.

В Южной Германии, к северу от Цвайбрюккена, находятся ртутные месторождения, которые имели значительное значение в конце тринадцатого века, но к началу Первой мировой войны рудники были закрыты уже много лет. Цинковые руды, добываемые вблизи Бенсберга, к востоку от Кельна, дают ежегодно около 90 колб ртути, получаемой в качестве побочного продукта при плавке цинка. В бывшей Австрийской империи основное месторождение находится в Идрии, примерно в 28 милях от Триеста. Рудное тело встречается главным образом в виде пропитки триасового доломита и сланца. Добыча в Австрии в 1916 году, вероятно, вся из Идрии, как полагают, составила около 25 000 колб. Известны запасы, способные дать 20 000 метрических тонн, или 587 733 колбы. По последним сообщениям, эти рудники находились во владении Италии. В Ципсе, в северной Венгрии, ртуть получается как побочный продукт из железной руды (сидерита), которая содержит ртутистый тетраэдрит и некоторое количество киновари. Добыча в 1913 году составила 2615 колб.

К западу от Идрии ртутные месторождения, принадлежащие к тому же общему поясу металлогении, простираются в северную Италию. Основным месторождением этого пояса в Венеции является Валлальта. Рудник произвел 9550 колб (325 метрических тонн) в период между 1856 и 1870 годами, но долгое время простаивал. Самыми продуктивными месторождениями ртути в Италии являются месторождения района Монте-Амиата в Тоскане, примерно на полпути между Римом и Флоренцией. Монте-Амиата, по-видимому, является постплиоценовым вулканом, и следы недавней вулканической активности сохранились. Самым продуктивным рудником является Аббадия-Сан-Сальваторе, который дает около 65% добычи района, что в 1917 году составило около 29 300 колб.

На горе Авала, недалеко от Белграда в Сербии, с 1883 года известны месторождения ртутной руды, которые напоминают многие месторождения в Калифорнии. Месторождения Авалы разрабатывались в период между 1889 и 1895 годами, но, по-видимому, в последние годы не были продуктивными.

Единственные значимые ртутные месторождения в европейской части России — это месторождения в Донецком угольном бассейне, южная Россия. Основным минералом является киноварь, сопровождаемая антимонитом и пиритом. Месторождения были открыты в 1879 году, максимальная добыча — 18 102 колбы (616 метрических тонн) — была достигнута в 1897 году, и работы были прекращены в 1911 году, но с тех пор возобновились в небольшом масштабе.

Азия.

—Рудник Конья в южной части центральной Малой Азии находится в окремненном известняке. Ртуть встречается в виде киновари, и большая часть руды содержит от 1 до 2,5% металла. Известные запасы оценивались в 1908 году в 13 000 метрических тонн 1%-ной руды. Добыча в 1911 году составила всего 90 колб по 75 фунтов. Рудник Кара-Бурну, который называют единственным важным ртутным рудником в Турции, расположен к юго-востоку от Смирны. В 1906 и 1907 годах рудник производил около 3000 колб ежегодно, но в последние годы добыча сократилась и в 1912 году составила всего 811 колб (31 метрическая тонна).

Ильдеканский ртутный рудник в юго-восточной Сибири, к востоку от озера Байкал, приобрел печальную известность из-за того, что политические ссыльные были приговорены к добыче руды. Месторождение, по-видимому, имеет незначительное экономическое значение.

То, что ртутные месторождения встречаются в провинции Гуйчжоу, в южной части центрального Китая, известно давно, но эта местность удалена от обычных путей сообщения, и сравнительно мало записей о характере этих месторождений. Рудные тела рудников Ван Сан Чанг разрабатываются наиболее интенсивно. В течение нескольких лет до 1905 года добыча составляла в среднем около 4000 фунтов ртути в месяц. Это было бы эквивалентно примерно 640 колбам ежегодно. Более свежие данные о добыче отсутствуют.

Северная Америка.

—Ртутные месторождения Северной Америки ограничены Кордильерским регионом от Аляски до Центральной Америки. Самые продуктивные месторождения находятся в Калифорнии и западном Техасе. На Аляске минералы, содержащие ртуть, были найдены в ряде районов россыпной добычи, но месторождения в коренном залегании были обнаружены только в центральном регионе Кускоквим. Руда встречается в виде киновари, сопровождаемой антимонитом, кварцем и железистым доломитом. Развитию препятствовали транспортные трудности, и было добыто лишь несколько сотен фунтов ртути для местного потребления. В Вашингтоне ртутные руды были разведаны в различных местах, но добыча пока незначительна. В Орегоне киноварь широко распространена, но только одно месторождение (в Блэкбьют, округ Лейн) в настоящее время является продуктивным. На руднике Блэк-Бьют руда содержит в среднем около 0,25% ртути, и количество, доступное выше 500-футового уровня, оценивается компанией примерно в 150 000 тонн. Добыча в Орегоне в 1917 году составила 388 колб, причем все, кроме 3 колб, были получены на руднике Блэк-Бьют.

В Калифорнии основные месторождения встречаются в Береговых хребтах в пределах пояса, который имеет длину около 400 миль и максимальную ширину около 75 миль. Известных месторождений в пределах этой области множество. Около двадцати пяти из них в настоящее время являются продуктивными, в то время как, вероятно, в три раза больше тех, что когда-то были продуктивными, сейчас простаивают. За немногими исключениями, месторождения этого основного ртутного пояса находятся в породах вероятного юрского возраста или в серпентине, который является продуктом изменения перидотитов. Наиболее заметными исключениями являются месторождения рудника Оушеник, округ Сан-Луис-Обиспо, и рудника Салфер-Бэнк, в округе Лейк. Многие из наиболее продуктивных рудников прошлого годами не давали ртути при подземных работах.

Самым продуктивным рудником в Калифорнии в настоящее время является Нью-Идрия в округе Сан-Бенито, который в 1917 году дал 11 000 колб из общего объема по штату 23 733 колбы и по Соединенным Штатам 35 954 колбы. Руда Нью-Идрии поступает с двух рудников: собственно Нью-Идрия и Сан-Карлос. Нью-Идрия была интенсивно вскрыта на глубину около 1000 футов. В Сан-Карлосе практически вся известная руда залегает в пределах 200 футов от поверхности. Оба рудника внесли почти равный вклад в общий объем добычи в 1917 году, а среднее содержание руды, пригодной для извлечения, в том году составило 0,32%. Было подсчитано, что на двух рудниках имеется 2 400 000 тонн руды со средним содержанием 0,253% ртути.

Рудник Нью-Альмаден находится в округе Санта-Клара. В настоящее время все горизонты ниже 800-футового уровня затоплены, и в последние годы на старом руднике добывалось очень мало руды. Большая часть недавней продукции New Almaden Co., Inc., которая в 1917 году составила 2683 колбы, поступила с рудника Эль-Сенадор, к северо-востоку от старого рудника, а также из ртути, извлеченной из грунта под старыми печами и конденсаторами. В Нью-Альмадене, Эль-Сенадоре и соседнем Нью-Гваделупе, который произвел 3100 колб в 1917 году, руда встречается в виде нерегулярных тел в серпентине. Рядом с рудником, который сейчас разрабатывается компанией New Guadalupe Mining Co. и принадлежит той же компании, находится первоначальный рудник Гваделупе, когда-то высокопродуктивный, но теперь давно простаивающий.

Рудник Оушеник в округе Сан-Луис-Обиспо занимал четвертое место по продуктивности в Калифорнии в 1917 году с объемом добычи 1246 колб. Руда встречается в виде пропитки песчаника. Среднее содержание руды, пригодной для извлечения, в 1917 году составило 0,185%. Другие рудники в Калифорнии, которые дали от 500 до 1000 колб в 1917 году, — это Грейт-Истерн, Кловердейл и Калвер-Бэр, все в округе Сонома. Те, чей объем добычи составлял от 400 до 500 колб, — это Сент-Джонс и Хелен в округе Лейк.

Невада содержит много широко разбросанных месторождений ртутной руды, ни одно из которых еще не разрабатывалось в широком масштабе, хотя некоторые из них были довольно продуктивными в течение коротких периодов. Руды встречаются в риолите третичного возраста и в известняке или связанных осадочных пластах различного возраста от палеозойского до мезозойского. Общий объем добычи в Неваде в 1917 году составил 997 колб, почти половина из которых поступила с рудника Фарнхэм и Дрю, к востоку от Мины, который закрылся из-за нехватки руды ближе к концу года. Следующий рудник по объему добычи, Голдбэнкс в округе Гумбольдт, также в настоящее время не является продуктивным.

В Техасе основные ртутные месторождения находятся в районе Терлингуа, в округе Брюстер. Руда встречается вдоль зон трещиноватости в меловых известняках и сланцах, как правило, в близости к интрузивной породе. Основными рудниками являются Чисос, Марипоса, Биг-Бенд и Даллас.

В Мексике ртутные месторождения в штатах Сан-Луис-Потоси, Герреро и Дуранго, как говорят, дают значительное количество ртути, даже в нынешнем нестабильном состоянии страны. Торговец ртутью, дававший показания на слушаниях Комиссии по тарифам в Сан-Франциско 26 июня 1918 года, сказал, что 400 колб в месяц экспортировалось в Соединенные Штаты, но значительная часть этого, вероятно, была регенерированной ртутью, которая использовалась при амальгамации серебряных руд.

Южная Америка.

—Ртутные месторождения известны в Колумбии, Эквадоре, Боливии, Чили, Бразилии, Аргентине и Перу, но только месторождения в Перу, по-видимому, имеют нынешнее экономическое значение, и добыча в этой стране в 1916 году составила всего 62 колбы (2,1 метрических тонн). Самые известные месторождения в Перу — это месторождения в Уанкавелике, особенно месторождения рудника Санта-Барбара, на восточном фланге западной цепи Анд. Они разрабатываются с 1566 года и, как говорят, дали 46 500 метрических тонн (1 366 480 колб по 75 фунтов) до 1790 года. Добыча в 19-м веке оценивается в 3500 метрических тонн (102 865 колб). Рудные тела многочисленны, нерегулярны и встречаются в стратифицированных породах, которые прорезаны магматическими породами. В 1916 году большая часть ртутьсодержащих земель в районе Уанкавелика была приобретена Э. Э. Фернандини из Лимы, и, по-видимому, есть некоторые перспективы возобновления активной добычи.

ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРЕДЕЛЕНИИ В БУДУЩЕМ

Как и большинство месторождений руд, сформировавшихся позднее отложения или затвердевания вмещающих их горных пород, месторождения ртути, скорее всего, будут обнаружены в регионах эруптивной активности и сложного геологического строения, особенно в районах сравнительно поздних вулканических возмущений. Отсюда следует, что новые месторождения наиболее вероятно будут открыты в пределах областей третичной или посттретичной вулканической активности, как, например, в Кордильерских поясах Северной и Южной Америки, на восточном побережье Азии, в некоторых частях Океании и на побережье Средиземного моря. Аляска, Мексика и западная часть Южной Америки, по-видимому, обладают наибольшими перспективами будущей продуктивности, однако вероятность каких-либо существенных изменений в источниках ртути в ближайшем будущем невелика. Ценность месторождения ртути, как правило, может быть установлена только путем горноразведочных работ, и лишь в очень немногих ртутных рудниках можно сделать надежную оценку «неразведанных» запасов руды. Известные факты не дают надежного основания для прогноза о том, что в ближайшем будущем какой-либо ныне незначительный район в течение следующих десяти лет отберет первенство по добыче у Испании или составит конкуренцию Австрии, Италии, Калифорнии или Техасу. Что касается основных известных источников, то представляется, что пик продуктивности в Калифорнии давно пройден, хотя рудники все еще способны увеличить текущую добычу при достаточном стимулировании. Добыча в Италии в последние годы растет, но неясно, означает ли это открытие новых рудных тел или указывает на более длительный срок эксплуатации района Монте-Амиата. Устойчивое улучшение политической обстановки в Мексике при сохранении нынешних или более высоких цен, вероятно, привело бы к заметному увеличению выхода продукции в этой стране. Существует также некоторая вероятность того, что Перу может вновь стать важным источником ртути.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Ртутная промышленность, скорее всего, претерпит изменения не столько из-за методов добычи, сколько из-за усовершенствований в металлургии. Хотя переработка ртутных руд проста в принципе, из-за подвижности и неуловимости металла как в жидком, так и в парообразном состоянии она сопряжена со многими практическими трудностями.

Крупнокусковая руда обычно перерабатывается в различных типах простых шахтных печей, при этом топливо либо смешивается с шихтой, либо сжигается в топке. Однако мелкокусковая или порошкообразная руда, составляющая большую часть материала на большинстве ртутных рудников, требует иной обработки. В Европе распространенным типом печи для мелкой руды является печь Шпирека, а в Соединенных Штатах — печь Скотта-Хютнера, или, как ее чаще называют, печь Скотта. В обеих печах руда опускается под действием силы тяжести по плиткам из огнеупорной глины, форма и расположение которых позволяют пламени проходить вперед и назад через проходы под плитками, причем эти проходы или дымоходы образуются частично плитками, а частично самой рудой. Из печи насыщенные ртутью пары направляются через ряд конденсационных камер из кирпича, железа, дерева или другого материала, в которых собирается металл.

При грамотной эксплуатации печь Скотта является на удивление экономичной и эффективной; однако ее конструкция дорога и требует специально обученных каменщиков. Кроме того, печь трудно ремонтировать, и после постройки ее невозможно переместить. Это серьезные недостатки для предпринимателя с небольшим капиталом, который разрабатывает новый рудник, и он обычно вынужден прибегать к ретортам, которые дороги в эксплуатации и неудовлетворительны, за исключением случаев переработки относительно небольших количеств богатой руды.

В последние годы в Калифорнии и Техасе предпринимались попытки использовать слегка модифицированные вращающиеся цементные печи для переработки ртутных руд. Это нововведение является многообещающим и, по-видимому, окажется успешным. Такая печь, хотя она, возможно, и не вытеснит печь Скотта при определенных условиях, не требует сложной кирпичной кладки, и ее использование может привести к значительному увеличению добычи на небольших рудниках.

Конденсационные системы, используемые с ртутными печами, сильно различаются, и ни на двух рудниках в Соединенных Штатах они не идентичны. Кирпичные конденсационные камеры, ранее широко применявшиеся с печью Скотта, дороги в строительстве; кроме того, кирпичи плохо проводят тепло и поглощают большое количество ртути. Недавняя тенденция в Калифорнии заключается в замене кирпичных камер большими ящиками или цилиндрическими резервуарами из дерева. Европейская практика, которой следуют один рудник в Орегоне и один в Техасе, отдает предпочтение конденсаторам, изготовленным из труб из витрифицированной керамики. Весь вопрос конденсации ртути требует изучения и квалифицированных экспериментов. Установление стандарта практики увеличило бы производство за счет устранения значительной части потерь и разочарований, возникающих из-за неэффективных индивидуальных попыток собрать ртуть из печных паров и газов наиболее полным и экономичным способом.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Ртутная промышленность предлагает два ярких примера прямого политического контроля над минеральными ресурсами. Рудник Альмаден, объем добычи которого в обычное время определяет рынок ртути, принадлежит испанскому правительству и разрабатывается им с 1645 года, а рудник Идрия до окончания войны принадлежал австро-венгерскому правительству.

Испанское правительство на основе конкурсных предложений заключает контракт с победителем торгов на продажу ртути сроком на десять лет. В течение ряда последовательных периодов контракт присуждался лондонскому дому Ротшильдов, текущий контракт действует с 1 июня 1912 года. Подрядчики обязуются продавать в Лондоне максимально возможное количество ртути, которую они принимают на условиях франко-борт на обогатительной фабрике в Альмадене, по ценам выше 7 фунтов стерлингов за флягу. Они получают комиссионные в размере 1 1/4 процента от суммы продажи; 6 шиллингов за каждую флягу, отправленную из Испании в Лондон; и 10 процентов от суммы, на которую цена продажи превышает 8 фунтов 2 шиллинга за флягу. Испанское правительство резервирует из объема по этому контракту 500 фляг ежегодно для национальных нужд Испании. Благодаря этой договоренности, хотя рудник принадлежит Испании, рынок контролируется из Лондона. Во время войны продажа ртути из Альмадена была взята на себя Адмиралтейством через фирму Ротшильдов. Количество ртути, полученное в Лондоне из Альмадена в 1917 году, составило около 25 000 фляг.

[144] Increased to 10,000 flasks in 1919.

Рудник Конья в Малой Азии вернулся в собственность турецкого правительства в 1912 году, но его добыча, как отмечалось ранее, незначительна.

Ртутные рудники района Монте-Амиата в Италии, хотя и менее очевидно иллюстрируют политический контроль, чем упомянутые выше, возможно, должны быть упомянуты в данной связи. Германский капитал доминировал в их развитии в последние годы перед войной, и, по достоверным сведениям, наиболее продуктивные рудники полностью или частично принадлежали германскому императору. С вступлением Италии в войну они были конфискованы итальянским правительством. Итальянские рудники произвели около 28 000 фляг, из которых от 12 000 до 15 000 фляг были закуплены Британским адмиралтейством.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Согласно современной практике, переработка ртутных руд почти неизменно осуществляется на руднике, причем и рудник, и обогатительные предприятия находятся в одной собственности. Поэтому для целей настоящего исследования их необходимо рассматривать вместе.

Наиболее ярким примером коммерческого контроля является контроль, осуществляемый лондонским домом Ротшильдов, которые не владеют ресурсами, обеспечивающими им это превосходство. Добыча на исключительно богатом руднике Альмаден, годовой объем которой превосходит объем любого другого рудника и в 1916 году превысил объем любой страны, кроме самой Испании (чья руда, даже при небрежной обработке, дает ртуть с низкими затратами, а известные запасы велики), позволяет Ротшильдам в мирное время и при условии соблюдения минимальной фиксированной цены в их контракте определять цену, по которой ртуть будет продаваться на мировых рынках. Еще одним, но гораздо меньшим фактором, делающим Лондон ведущим мировым рынком ртути, является контроль британского капитала над основными рудниками в районе Овьедо на севере Испании.

В Соединенных Штатах, стране, занимающей второе место после Испании по производству ртути, все рудники принадлежат корпорациям или частным лицам, и, насколько известно, в настоящее время не существует официального объединения или соглашения между этими владельцами для контроля над объемом производства или продажами. Несколько лет назад большинство ведущих производителей в Калифорнии сформировали компанию Eureka, которая выступала в качестве торгового агента и в некоторой степени могла контролировать цены. Эта организация, которую посторонние часто называли «ртутным трестом», была распущена после недолгого существования. Фирма Haas Brothers из Сан-Франциско (отличная от Haas Brothers из Нью-Йорка) играла ведущую роль в компании Eureka и после ее роспуска выполняла многие функции, которые должна была выполнять компания. Фирма владеет акциями ведущего рудника на Тихоокеанском побережье и выступает в качестве торгового агента для компании New Idria Quicksilver Mining Co., с которой взимает 1 процент, тогда как с других взимает 2 1/2 процента. Она также закупает металл для себя, обычно у мелких производителей, по ценам, как правило, значительно ниже текущих рыночных котировок, и должна снабжать операторов пустыми флягами, но только при условии, что Haas Brothers будут покупать продукцию или продавать ее на комиссионных началах. Другими брокерами, которые обрабатывают значительные количества ртути на Тихоокеанском побережье, являются Atkins, Kroll & Co. и Braun-Knecht-Hiemann Co., обе из Сан-Франциско. Насколько известно, эти две фирмы не владеют ртутными рудниками и продают только на комиссионных началах.

Эта связь, как сообщается, была разорвана в 1919 году.

Ртутные рудники в Техасе принадлежат американским гражданам или американским корпорациям. Руда с каждого из них разрабатывается независимо, и ртуть продается отдельными производителями.

Ртутные месторождения Мексики принадлежат, насколько известно, коренным мексиканцам. Британский капитал, вероятно, заинтересован в некоторых из более крупных рудников. Ранее продуктивные ртутные рудники в Уанкавелике, Перу, были приобретены Э. Э. Фернандини из Лимы и могут снова внести вклад в мировые поставки.

Насколько известно автору этой статьи, патенты, секретные процессы или торговые соглашения не играют никакой роли в контроле над ртутными ресурсами.

Во время войны Германия и ее союзники контролировали ртутные месторождения Австралии, Сербии, Турции и, вероятно, европейской части России. Важными являются только месторождение Идрия и, возможно, месторождение Зипс в Австрии, и доступный годовой объем поставок для тевтонских союзников составлял, вероятно, от 25 000 до 30 000 фляг. Союзники по Антанте контролировали месторождения Соединенных Штатов, дававшие около 36 000 фляг ежегодно; Италии, дававшие около 28 000 фляг; и контролировали, хотя и не владели, месторождения нейтральной Испании, дававшие от 30 000 до 41 000 фляг ежегодно. Китайские ртутные месторождения, возможно, в некоторой степени использовались Японией, у которой, как и у Британии и Франции, нет собственных месторождений, заслуживающих упоминания.

РЕЗЮМЕ

Основные области применения ртути и ее соединений в общем порядке убывания важности следующие: в производстве лекарств и химикатов, включая каломель, сулему и ледяную уксусную кислоту; в качестве детонатора для мощных взрывчатых веществ; в качестве пигмента киновари; в электротехнических приборах, термостатах, газовых регуляторах и других устройствах; при амальгамации золотых и серебряных руд; в противообрастающих красках для судов; в составах для предотвращения накипи в котлах; в косметике; и в стоматологической амальгаме. Существует сравнительно немного областей применения ртути, где нельзя было бы использовать заменитель, хотя заменитель может быть не таким экономичным или удовлетворительным.

В целом ртутные руды не залегают на больших глубинах и в целом демонстрируют тесную связь с третичными и четвертичными изверженными породами, которые не подвергались длительной и глубокой эрозии. Однако существуют некоторые заметные исключения из этих обобщений. Новые месторождения ртути наиболее вероятно будут обнаружены на восточном побережье Азии, в некоторых частях Океании, на побережье Средиземного моря или в Кордильерских поясах Северной и Южной Америки. Известные факты не дают надежного основания для прогноза о том, что в течение следующих десяти лет произойдет какой-либо заметный сдвиг от нынешних основных источников поставок к какому-либо вновь открытому месторождению.

Самые богатые ртутные месторождения находятся в Альмадене, центральная Испания; в Идрии, Австро-Венгрия; и в районе Монте-Амиата в Италии. Другие продуктивные месторождения расположены недалеко от Овьедо и Гранады, Испания; в Донецком угольном бассейне, Россия; недалеко от Айдына, Турция; в провинции Гуйчжоу, Китай; в Орегоне, Калифорнии, Неваде и Техасе; в Сан-Луис-Потоси, Герреро и Дуранго, Мексика; и в Перу. Многие месторождения, в настоящее время не разрабатываемые, известны в других частях мира.

Политический контроль над ртутными месторождениями по большей части соответствует географическому положению. Богатые месторождения Альмадена в Испании и Идрии в бывшей Австро-Венгрии находятся в государственной собственности. Испанское правительство на основе конкурсных предложений заключает контракт с победителем торгов на продажу ртути сроком на десять лет. Контракт присуждался лондонскому дому Ротшильдов в течение ряда последовательных периодов. Этот контроль над выходом продукции испанских рудников дает Ротшильдам контроль над мировым рынком ртути. Испанское правительство резервирует достаточное количество фляг ежегодно для национальных нужд Испании. Рудник Конья в Малой Азии является собственностью турецкого правительства с 1912 года. Считается, что наиболее продуктивные рудники района Монте-Амиата в Италии полностью или частично принадлежали германскому императору; с вступлением Италии в войну они были конфискованы итальянским правительством. Рудники Соединенных Штатов полностью контролируются корпорациями или частными лицами. Считается, что рудники Мексики принадлежат мексиканским гражданам, хотя британский капитал может быть инвестирован в некоторые из них. Рудники в Уанкавелике, Перу, были приобретены сеньором Э. Э. Фернандини из Лимы.

ГЛАВА XIX БОКСИТЫ И АЛЮМИНИЙ Автор: Дж. М. Хилл

ИСПОЛЬЗОВАНИЕ БОКСИТОВ И АЛЮМИНИЯ

Боксит, оксид алюминия, помимо того, что является основной рудой алюминия, имеет важное применение в производстве искусственных абразивов, которые широко используются во всех металлообрабатывающих отраслях промышленности. Боксит также является основой обширной химической промышленности, будучи сырьевым материалом, из которого производятся квасцы, сульфат алюминия и несколько других химикатов, используемых для очистки воды, крашения и дубления. Быстрорастущей областью применения бокситов является производство бокситового кирпича для футеровки печей. Наиболее важными областями использования бокситов являются производство алюминия и абразивов, хотя представляется сомнительным, чтобы использование бокситов для химической промышленности могло быть сильно ограничено. Использование бокситов для огнеупорных материалов относительно невелико. В 1917 году почти 65 процентов внутреннего производства бокситов пошло на алюминий, почти 13 процентов было потреблено производством солей алюминия, 19 процентов было израсходовано в производстве бокситовых абразивов и 3 процента было использовано производителями бокситовых огнеупоров.

Области применения алюминия бесчисленны, главными из них являются производство деталей двигателей внутреннего сгорания и изготовление промышленной и бытовой утвари.

ИЗМЕНЕНИЯ В ПРАКТИКЕ ПРОИЗВОДСТВА АЛЮМИНИЯ

До сих пор для приготовления глинозема для производства алюминия использовались бокситы с низким содержанием кремнезема (от 2 до 5 процентов SiO2). Многие экспериментаторы пытались использовать низкосортные (с высоким содержанием кремнезема) бокситы или силикаты алюминия для извлечения глинозема. Эти эксперименты показывают, что химически возможно производить глинозем с низким содержанием кремнезема из многих алюминосодержащих материалов, но не на коммерчески выгодной основе. Представляется вполне вероятным, что один или несколько методов обработки низкосортных бокситов или даже силикатов алюминия будут доведены до коммерческой стадии, даже в обычных условиях, в ближайшем будущем. Это событие должно привести к революции в алюминиевой промышленности, поскольку глины и сланцы, содержащие от 25 до 35 процентов Al2O3, встречаются повсеместно. Будет ли это существенно снижать цену на алюминий, более сомнительно, так как производственные затраты возрастут из-за повышенной стоимости переработки низкосортного сырья.

ГЕОЛОГИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Европейские месторождения бокситов находятся в складчатых осадочных породах, главным образом мелового периода. В Соединенных Штатах месторождения бокситов являются поверхностными и возникли в результате изменения либо осадочного каолина (силиката алюминия), либо каолина, полученного в результате выветривания сиенита или доломитовых известняков. В тропических месторождениях, которые до сих пор мало эксплуатировались и, по сути, мало изучены, бокситы, по-видимому, являются поверхностными отложениями, полученными в результате изменения полевошпатовых пород.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Основные месторождения бокситов в Европе находятся в департаментах Вар и Эро на юге Франции, хотя другие месторождения известны в департаменте Буш-дю-Рон и нескольких других южных департаментах. В центральной Италии бокситы добываются уже несколько лет. В Германии низкосортные бокситы добывались в горах Фогельсберг, Гессен, недалеко от Кёнигсвинтера, в районе нижнего Рейна, и известны в Ганновере. В бывшей Австро-Венгерской империи имеются обширные месторождения бокситов в горах Бихор и в провинциях Истрия, Хорватия и Далмация. Бокситы также известны в северо-западной России, примерно в 200 милях к юго-востоку от Петрограда. Бокситы добываются уже много лет из пластов на северо-западе Ирландии.

В Соединенных Штатах бокситы добываются годами в центральном Арканзасе, северо-западной Джорджии, северо-восточной Алабаме и юго-восточном Теннесси, а в последнее время — на месторождении в центральной Джорджии, которое расширяется в западно-центральную часть Джорджии.

В Южной Америке обширные месторождения хороших бокситов были найдены в Британской и Голландской Гвиане, и сообщается, что существуют признаки наличия бокситов в восточной Венесуэле, западной Французской Гвиане и северо-восточной Бразилии.

В Африке сообщается, что бокситы хорошего качества были разведаны недалеко от побережья Французской Гвинеи и найдены в ряде внутренних районов этой колонии. Ходят смутные слухи о больших площадях бокситовых латеритов во многих местах экваториальной Африки.

Латерит — это общее название для породы любого вида, которая находится в полностью размягченном и разложившемся состоянии из-за изменения или выветривания на поверхности.

В литературе по геологии Индии много упоминаний о бокситовых латеритах, и сообщается, что в последнее время некоторые из месторождений бокситов Декана эксплуатируются.

В юго-западной и восточной Австралии некоторые латериты, как сообщается, являются бокситовыми, хотя, насколько известно, ни одно месторождение бокситов не было разработано.

Существует упорный, не подтвержденный слух о том, что бокситы были недавно обнаружены в Китае. Об этом месторождении никакой информации нет.

В приведенной ниже таблице показана мировая добыча бокситов за ряд лет. Хотя цифры дают представление об относительной важности месторождений по отношению к центрам потребления, не считается, что они отражают относительную важность в отношении будущего. Кажется неизбежным сделать вывод, что тропические страны обладают огромными запасами бокситов и что когда-нибудь алюминиевая промышленность будет ближе к тропикам, чем в настоящее время.

Таблица 63. — Мировая добыча бокситов, 1910-1916 гг. (Добыча в тоннах)

Country | 1910 | 1911 | 1912 | 1913 | 1914 | 1915 | 1916
United States | 148,932 | 155,618 | 159,865 | 210,241 | 219,318 | 297,041 | 425,100
France | 192,913 | 250,818 | 254,851 | 304,407 | ([147]) | ([147]) | ([147])
United Kingdom (Ireland) | 3,792 | 6,007 | 5,790 | 6,055 | 8,286 | 11,723 | 10,329
Italy | 4,524 | 5,600 | 6,596 | 6,843 | 3,844 | 6,504 | 8,746
India | 66 | 12 | 950 | 1,184 | 514 | 400 | 750
Total | 350,277 | 418,055 | 428,052 | 528,730 |  |  |

Статистические данные отсутствуют.

The production of bauxite in the United States in 1917 was 568,690 long tons.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Франция и Соединенные Штаты содержат в своих границах крупнейшие месторождения бокситов, которые разрабатывались в прошлом. Англия контролирует через свои колониальные владения большую часть экваториальных районов, которые, вероятно, содержат значительную часть неразведанных бокситов. Франция и Голландия имеют владения в тропиках, где известны бокситы, и представляется вероятным, что бокситы могут быть найдены в колониях Португалии и Бельгии, а также в тех, которые ранее контролировались Германией.

Сообщается, что Англия ввела определенные ограничения на приобретение месторождений бокситов в Индии и Гвиане иностранными физическими или юридическими лицами. Известно, что она ограничила направление экспорта бокситов из Британской Гвианы. По имеющимся сведениям, голландское правительство недавно изучило месторождения бокситов в Голландской Гвиане, вероятно, с целью ограничения приобретения собственности, которая еще не была приобретена. Очевидно, существует некое соглашение между британским, французским и итальянским правительствами, которое позволяет отправлять французские бокситы на алюминиевые заводы как Италии, так и Англии.

Алюминиевые заводы мира в значительной степени находятся под политическим доминированием Соединенных Штатов, Англии, Франции, Германии, Швейцарии, Италии и Норвегии. Производственная мощность различных стран оценивается следующим образом:

Производственная мощность алюминиевых заводов

| Short tons
United States and Canada | 87,500
France | 20,000
Switzerland, Germany and Austria | 20,000
Norway | 16,000
England | 12,000
Italy | 7,000
Japan | 250
Total | 162,750

Хилл, Дж. М., «Бокситы и алюминий в 1916 г.»; Геологическая служба США; «Минеральные ресурсы Соединенных Штатов», часть I, 1917 г., стр. 167.

Фактический выпуск продукции заводами, включенными в приведенную выше таблицу, не представляет собой полную мощность, и кажется более разумным предположить, что производство в настоящее время, вероятно, ближе к 150 000 тонн в год, чем указанный общий объем. Почти не вызывает сомнений, что заводы Соединенных Штатов и Канады производят более половины мирового объема алюминия. Сообщается, что в течение 1917 и 1918 годов расширение британских и итальянских заводов довело их выпуск продукции почти до номинальной мощности заводов.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Можно с уверенностью сказать, что алюминиевая промышленность различных стран в значительной степени контролирует месторождения бокситов в мире. Основными алюминиевыми компаниями являются следующие: Aluminum Company of America, British Aluminum Co., L’Aluminium Française, Aluminum Industries A. G.

Общеизвестно, что до войны соглашения между этими четырьмя компаниями стабилизировали цены на алюминий во всем мире. В настоящее время (1919 г.) перспектива заключается в том, что Aluminum Company of America должна быть в состоянии доминировать в алюминиевой промышленности мира в течение нескольких лет за счет расширения своих электрических станций и своей инициативы в приобретении вновь открытых месторождений исключительно чистых бокситов в Южной Америке. Представляется вполне вероятным, что британские, французские и, возможно, германские интересы могут попытаться скорректировать свои отношения так, чтобы они могли противостоять американскому доминированию.

Соединенные Штаты и Канада.

— Большая часть месторождений бокситов в Соединенных Штатах, по-видимому, контролируется Aluminum Company of America через ее дочерние компании American Bauxite Co. и Republic Mining & Manufacturing Co. Существуют небольшие владения бокситовыми землями, контролируемые National Bauxite Co., дочерней компанией E. I. du Pont de Nemours Co., и Norton Co. из Вустера, штат Массачусетс, производителями искусственных абразивов. Помимо этих более крупных владельцев, существует несколько независимых операторов бокситовых рудников, но их совокупный объем добычи настолько мал, что им можно пренебречь.

Все алюминиевые заводы Соединенных Штатов и Канады контролируются Aluminum Company of America, в которой доминируют банковские интересы Меллонов из Питтсбурга, штат Пенсильвания.

Гвианы.

— Сообщается, что Aluminum Company of America контролирует около 2 030 000 акров бокситовых земель в британских и голландских колониях. В Британской Гвиане право собственности, по-видимому, принадлежит Canadian Bauxite Co. С Aluminum Company of America в британских гвианских владениях связана Merrimac Chemical Co. из Бостона. Также сообщается, что Norton Co. из Вустера, штат Массачусетс, приобрела в Голландской Гвиане небольшие владения бокситовых земель. В Голландской Гвиане нет заводов, использующих бокситы.

Франция.

— До войны некоторые из крупных месторождений высококачественных бокситов в департаменте Вар контролировались «Bauxites de France», германским предприятием, но этот контроль был естественно приостановлен в начале военных действий, и он, вероятно, не будет возобновлен. Французская бокситовая промышленность в значительной степени находится в руках французских производителей алюминия, упомянутых ниже, хотя некоторые месторождения, как говорят, контролируются British Aluminum Co. через ее контроль над компанией Union des Bauxites.

Французская алюминиевая промышленность централизована под управлением одного торгового агента, L’Aluminium Française, в котором участвуют следующие пять компаний:

Compagnie des Produits Chemiques d’Alais et de la Camargue, Société Electro-Metallurgique Française, Société d’Electro-Chemie, Société des Forces Motrices de l’Arve, Société Electro-Metallurgique de Pyrenees.

Говорят, что акции торговой компании принадлежат участвующим компаниям пропорционально их выпуску алюминия, что указывало бы на то, что контроль над l’Aluminium Française принадлежит первым двум компаниям из вышеперечисленных.

Великобритания.

— Месторождения бокситов в графстве Антрим, Ирландия, по-видимому, контролируются исключительно British Aluminium Co. British Aluminium Co. является единственным производителем металла в Англии, управляющим заводами в Фойерсе и Лох-Левене на Британских островах, а также заводами в Норвегии.

Норвегия.

— Все бокситы, используемые алюминиевыми заводами в Норвегии, имеют французское или британское происхождение. В стране нет месторождений бокситов. British Aluminium Co. контролирует алюминиевые заводы в Хайланде и Стрэнгфиорде через Anglo-Norwegian Co. Compagnie des Produits Chemiques d’Alais et de la Camargue (Франция) в значительной степени контролирует Société Norvegienne des Nitrures, которая управляет алюминиевыми заводами в Арендале и Тюсседале. Норвежская компания Norske Aluminum Co. была недавно организована для производства алюминия.

Италия.

— Существует мало информации о собственности на итальянские месторождения бокситов, но, по-видимому, они контролируются производителями алюминия. Основным производителем алюминия является Societa Italiana per la Fabricazione dell’Alluminio, которая находится под итало-французским контролем.

Новая алюминиевая компания L’Allumino Italiano, недавно организованная в Италии, если верить сообщениям, может частично контролироваться германскими и швейцарскими интересами. Поскольку компания была организована во время войны, не кажется разумным предполагать, что германское участие было бы разрешено.

Центральные державы.

— По-видимому, большая часть алюминиевой промышленности этих стран контролируется германо-швейцарской компанией Société Swisse pour l’Industrie de l’Aluminium, или Aluminum Industrie, A. G., которая управляет заводами в Нойхаузене, Чиппесе, Навизансе и Борне в Швейцарии; в Рейнфельдене, Германия, и в Ленде и Раурисе, Австрия. Небольшое количество алюминия также производится германской фирмой Gebrüder Guilini на ее заводе в Мартиньи. Сообщается, что недавно была сформирована Aluminum Fabrik-Martigny, A. G. во главе с Г. Гилини, что, возможно, является реорганизацией прежнего предприятия.

SUMMARY

Безусловно, самое большое и важное использование бокситов — это извлечение алюминия, металла, используемого главным образом в производстве деталей для двигателей внутреннего сгорания и промышленной и бытовой утвари. Бокситы также используются в производстве искусственных абразивов, как источник определенных солей алюминия и в производстве огнеупорного кирпича. Первые два применения, производство алюминия и абразивов, являются наиболее важными, хотя было бы трудно ограничить в какой-либо значительной степени использование в химической промышленности.

Основные месторождения бокситов в мире находятся в департаментах Вар и Эро, южная Франция; в бывшей Австро-Венгерской империи; в Арканзасе, Джорджии и Алабаме; в Британской и Голландской Гвиане; и на северо-западе Ирландии. Незначительные месторождения расположены в Германии, России, Венесуэле, Французской Гвиане, Бразилии, Африке, Австралии и, вероятно, Китае. Считается, что тропические страны обладают огромными запасами бокситов.

Эксперименты показали, что химически возможно производить алюминий из низкосортных (с высоким содержанием силикатов) бокситовых руд. Ни один коммерческий процесс не был доведен до совершенства, но кажется несомненным, что один или несколько методов будут доведены до коммерческой стадии в ближайшем будущем. Однако снижения цены на алюминий в результате этого изменения практики ожидать не следует, так как использование низкосортных материалов, несомненно, увеличит производственные затраты.

Крупнейшие добывающие месторождения бокситов политически контролируются Соединенными Штатами и Францией. Великобритания контролирует большую часть экваториальных регионов, которые, вероятно, содержат большинство неразведанных месторождений. Бокситы также могут быть найдены в колониальных владениях Португалии и Бельгии, а также в тех, которые ранее принадлежали Германии. Алюминиевые заводы мира контролируются Соединенными Штатами, Великобританией, Францией, Германией, Швейцарией, Италией и Норвегией.

Большинство месторождений бокситов в Соединенных Штатах принадлежат Aluminum Company of America, в которой доминируют банковские интересы Меллонов из Питтсбурга и которая контролирует все алюминиевые заводы Соединенных Штатов и Канады. Небольшие владения в Соединенных Штатах контролируются дочерней компанией E. I. du Pont de Nemours Co. и Norton Co. из Вустера, штат Массачусетс. Aluminum Company of America также контролирует через дочерние компании большие площади бокситовых земель в Британской и Голландской Гвиане. До войны некоторые из крупных французских месторождений контролировались германскими интересами. Французская промышленность в значительной степени находится в руках французских производителей алюминия, хотя некоторые из месторождений, как говорят, контролируются британским капиталом. Основные французские компании организовали торговую компанию L’Aluminium Française.

British Aluminium Co. контролирует месторождения в Ирландии и является единственным производителем алюминия в Англии. Британский капитал также контролирует алюминиевые заводы в Норвегии. Основные месторождения бокситов в Италии, вероятно, контролируются Societa Italiana per la Fabricazione dell’Alluminio, итало-французской компанией. По-видимому, большая часть алюминиевой промышленности Центральных держав контролируется германо-швейцарской компанией. Сообщается, что американские интересы исследовали месторождения бокситов во Французской Гвинее, Африка, но, насколько известно, бокситов не добывали.

ГЛАВА XX НАЖДАК И КОРУНД Автор: Фрэнк Дж. Кац

ИСПОЛЬЗОВАНИЕ НАЖДАКА И КОРУНДА

Корунд — это природный (минеральный) кристаллический оксид алюминия. Наждак — это очень мелкозернистое и тесное срастание корунда и других минералов, главным образом магнетита, причем некоторые разновидности содержат также значительные количества гематита, шпинели и хлорита. И наждак, и корунд очень твердые и раскалываются на грубые, острые зерна; поэтому они используются в качестве абразивов для шлифования, обдирки и полировки металлов — главным образом железа и стали — и стекла, а в меньшей степени — камня, дерева и других материалов. Наждак и корунд используются в свободном виде в форме зерен, порошков и муки, а также в виде зерен, спрессованных в твердые круги, цилиндры, бруски и напильники многих форм с помощью большого разнообразия связующих веществ. Основные области применения — работа по железу, стали и стеклу. Более мягкие металлы и другие материалы во многих случаях можно обрабатывать с большей эффективностью с помощью других абразивов, таких как кварц, триполи, гранат и пемза.

Основные операции, для которых используются наждак и корунд, могут выполняться с помощью искусственных карбидных и глиноземистых абразивов. Однако для некоторых работ такие замены, по-видимому, нецелесообразны, поскольку абразивное качество и эффективность как природных, так и искусственных абразивов зависят не только от твердости этих материалов, но и от ряда других факторов: среди них физические качества обрабатываемых материалов; острота краев и углов разбитых частиц абразива; способ разрушения абразива при использовании; способ и материалы, используемые при связывании частиц абразива; а также скорость и давление, с которыми они применяются к работе.

Из различных видов абразивных материалов каждый требует разных сортов и видов абразивов, а также изменения вышеуказанных факторов при использовании этих абразивов для обеспечения наиболее эффективного использования. Следовательно, почти невозможно произвольно определить области применения, для которых необходим каждый из различных абразивных материалов. По крайней мере, одно кажется несомненным — что для финишной обработки и полировки стекла, особенно оптического и листового стекла, до сих пор нет общего согласия относительно того, что существуют удовлетворительные заменители для лучших сортов турецкого и греческого наждака, хотя эксперименты по производству и использованию подходящих искусственных абразивов были успешными.

ГЕОЛОГИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Известные месторождения наждака являются продуктами магматической дифференциации или регионального метаморфизма, или комбинированного контактового и регионального метаморфизма известняка, предположительно глинистого, и глинистых отложений. Изучение некоторых отдельных месторождений, таким образом, позволяет сделать некоторый прогноз относительно будущих поставок в некоторых регионах, особенно тех, в которых месторождения наждака тесно связаны с определенными пластами в метаморфических осадочных формациях в непосредственной близости от изверженных пород. Однако тела наждака, как правило, пятнистые или распределены неравномерно, и надежные оценки запасов затруднены.

Корунд в ряде ассоциаций является первичным компонентом большого разнообразия изверженных пород, таких как перидотиты, анортозиты, сиениты, нефелиновые сиениты и сиенитовые пегматиты. Он также обильно встречается в регионально метаморфизованных породах и в зонах контактового метаморфизма, встречаясь в серпентинитах, слюдяных сланцах, кварцевых сланцах и кристаллических известняках. Третьим важным источником корунда являются аллювиальные отложения. Корунд не является характерным или существенным компонентом ни в одном из этих типов пород и присутствует в аллювиальных отложениях только в ограниченных местностях. Более того, его распределение и концентрация, когда он присутствует, являются нерегулярными и бессистемными, и поэтому не существует геологических ориентиров, по которым можно было бы прогнозировать будущие поставки без интенсивного изучения каждого отдельного случая.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Основные месторождения наждака и корунда в Соединенных Штатах находятся в штатах восточного побережья или Аппалачских штатах.

Месторождения наждака в Честере, штат Массачусетс, находятся в узкой полосе шириной менее 500 футов, которая была прослежена на протяжении почти пяти миль. Месторождения в Честере разрабатывались в разное время с восьмидесятых годов и до 1913 года.

Месторождения наждака недалеко от Пикскилла, штат Нью-Йорк, связаны с изверженными породами на площади от 20 до 25 квадратных миль. Эти месторождения разрабатываются с 1889 года. Часть добываемого материала является настоящим наждаком, то есть тесной смесью корунда и магнетита, но большая его часть представляет собой смесь шпинели и магнетита, которая, хотя и не является настоящим наждаком, представляет собой отличный абразив. В 1916 и 1917 годах годовой объем добычи руды составлял примерно 15 000 тонн.

В окрестностях Уиттла, округ Питтсильвания, штат Вирджиния, в изобилии встречается шпинелевый наждак, несколько похожий на нью-йоркский наждак, но содержащий больше корунда. Месторождения в этом регионе уже дали значительное количество наждака, и на них можно рассчитывать как на крупный источник поставок.

Корунд связан с серпентинитовым поясом, проходящим через округа Ланкастер, Честер, Делавэр, Монтгомери и Бакс в Пенсильвании, а также через прилегающие округа в Делавэре и Мэриленде. Месторождения в этом регионе, по-видимому, не имеют коммерческого значения.

Корунд встречается в большом количестве мест в Северной Каролине. Наиболее важные проявления корунда находятся в перидотитовых массивах или рядом с ними, а также в сланцах и в аллювиальных отложениях. Активные горные работы были впервые начаты в 1871 году и продолжались примерно до 1906 года, когда корунд из Северной Каролины был вытеснен с рынка конкуренцией канадского корунда и искусственных абразивов. Добыча корунда была возобновлена в 1915 году, и три предприятия, работавшие в 1917 году, дали 820 тонн продукции. В этом регионе, несомненно, имеются очень большие запасы корунда, но транспортировка затруднена, а квалифицированная рабочая сила в дефиците, поэтому в ближайшее время нет особых перспектив для крупного развития.

Единственные коммерчески важные месторождения абразивного корунда к западу от Аппалачских гор находятся в центральной части округа Галлатин недалеко от Сейлсвилла, штат Монтана, где корунд встречается в сиените и сиенитовом пегматите. Месторождения разрабатывались тремя компаниями, и до 1903 года, когда работы прекратились, было добыто несколько сотен тонн корунда.

Источники абразивного корунда коммерческого значения в Канаде ограничены корундовыми сиенитами и анортозитами в центральной части Онтарио. Эти месторождения разрабатывались и добывались только на рудниках Берджесс и Крейгмонт. Добыча корунда как отрасль промышленности в Канаде началась в 1900 году. Производство достигло максимума в 1906 году и было меньшим и довольно равномерным с 1907 по 1913 год, в котором работы были практически приостановлены.

Сообщения о находках корунда в Мексике, Центральной и Южной Америке касаются главным образом ювелирных разновидностей. Наждак упоминается в Муско, Колумбия, а обычный корунд, как сообщается, особенно обилен в местностях штата Сан-Паулу, Бразилия.

Единственное месторождение наждака и корунда коммерческого значения в Европе находится на островах Греческого архипелага, в частности на острове Наксос. Месторождения встречаются там в виде линз и масс в известняках и вблизи гранитов. Разведка и разработка были поверхностными, но запасы или будущие поставки там, вероятно, огромны. Ежегодный экспорт в период с 1897 по 1914 год составлял в среднем 6 800 метрических тонн.

В Азии существуют коммерческие месторождения корунда в азиатской части Турции и в Индии.

Месторождения наждака в азиатской части Турции находятся недалеко от Смирны. Турецкий наждак по происхождению и общему характеру похож на греческий наждак, за исключением того, что в Малой Азии не встречается наждака такого превосходного качества, как на Наксосе. Основным источником поставок, по-видимому, до сих пор были детритовые отложения. Кажется почти несомненным, что запасы велики. Наждачные рудники Малой Азии очень старые и ежегодно вносили большие количества в мировые поставки, причем их объем добычи был больше, чем из любого другого региона в мире. Статистика за последние годы отсутствует. Зарегистрированный объем добычи в официальных отчетах турецкого правительства составлял около 62 000 метрических тонн в 1908 году и около 25 000 в 1909 году.

Месторождения корунда в Индии многочисленны и включают не только обычные абразивные разновидности, но и самые высоко ценимые ювелирные разновидности. Коммерчески важные месторождения абразивной разновидности встречаются в президентстве Мадрас. Следующие провинции и туземные штаты также содержат этот минерал в той или иной степени изобилия: Афганистан, Бенгалия, Бирма, Центральные провинции, Пенджаб и Траванкор.

Имеющиеся данные о производстве корунда в Индии указывают на объем добычи от 100 до 500 длинных тонн в год, вплоть до 1915 года включительно. В 1916 году производство составило примерно 2 000 длинных тонн, и с тех пор оно, вероятно, сравнялось с этой цифрой или превысило ее. Ничего определенного о ресурсах корунда в Индии не известно, кроме того, что они, несомненно, велики.

Единственные зарегистрированные месторождения абразивного корунда в коммерческих количествах на континенте Африка находятся в окрестностях Претории, в Трансваале, где корунд, вероятно, изначально встречавшийся в сланцах, концентрируется из остаточного материала на поверхности земли. Мало информации об этих месторождениях корунда доступно, но вероятно, что могут быть разработаны большие запасы. Производство, которое было незначительным или пренебрежимо малым до 1912 года, значительно расширилось в 1917 году до примерно 3 000 длинных тонн.

Корунд, по-видимому, обилен на острове Мадагаскар, где большие количества ювелирного сырья и абразивных материалов были найдены в аллювиальных отложениях. Производство абразивного корунда, которое было очень небольшим в 1910 году, расширилось до примерно 1 100 метрических тонн в 1913 году и примерно 1 000 метрических тонн в 1916 году.

РАЗВИТИЕ И ИЗМЕНЕНИЯ В БЛИЖАЙШЕМ БУДУЩЕМ

Никаких существенных изменений в географическом распределении ресурсов в ближайшем будущем не предвидится. Ни одно из разрабатываемых в настоящее время месторождений не приближается к истощению, и только в отношении наждака в Вирджинии, где можно ожидать несколько большего производства наждака, имеется информация, на основании которой можно прогнозировать изменения в объеме добычи.

Замещение наждака и корунда искусственными абразивами может быть расширено. Эксперименты, проведенные в начале 1918 года с целью разработки искусственного абразива, пригодного для использования в оптической и листовой стекольной промышленности, увенчались успехом, так что, возможно, не останется ни одной промышленной операции, полностью зависящей от наждака и корунда. Однако полное вытеснение природных абразивов будет отчасти зависеть от запасов бокситов, доступных для производства искусственных абразивов. В настоящее время запасов бокситов в Соединенных Штатах достаточно для такого использования.

Спрос в Великобритании и Франции на индийский и южноафриканский корунд, а также на греческий наждак, несомненно, уменьшился бы, если бы французские заводы по производству искусственных абразивов работали на полную мощность. Такое изменение также, вероятно, сократило бы экспорт искусственных абразивов из Соединенных Штатов и соответствующим образом повлияло бы на спрос на наждак и корунд.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Ресурсы наждака и корунда в пределах Соединенных Штатов принадлежат, насколько известно, американским гражданам и никоим образом не контролируются государством.

Греческая промышленность по добыче наждака ранее была монополией, контролируемой греческим правительством, но жители наждачного региона всегда сохраняли за собой исключительное право на его добычу. Это право соблюдалось, а греческое правительство лишь регулировало и управляло продажами и экспортом, взимало высокие роялти, которые время от времени менялись, устанавливало цены и поддерживало высокое качество и единые стандарты наждака для экспорта. Во время войны французское правительство взяло под контроль поставки наждака с Наксоса и, по-видимому, продолжило соблюдать правила греческого правительства. Поставки греческого наждака были доступны только Франции и ее союзникам посредством распределения французским правительством.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

В Соединенных Штатах различные месторождения наждака и корунда находятся в мелких владениях, которые в основном принадлежат местным жителям. Шахты и карьеры, как правило, разрабатывались арендаторами на условиях выплаты роялти. Значительное число операторов работают и работали в нескольких районах, и торговых коалиций не существует. Дробление и сортировка находятся в руках восьми независимых конкурирующих компаний, за исключением тех случаев, когда во время войны они были объединены Советом по военной торговле в торговую ассоциацию с целью распределения под государственным надзором небольшого импорта греческого наждака для нужд важнейших отраслей промышленности.

В Канаде лучшие части месторождений корунда, по-видимому, в значительной степени контролируются одной компанией — Manufacturers Corundum Co., владельцы которой, судя по всему, преимущественно или полностью являются гражданами Канады.

Греческие месторождения наждака, особенно на острове Наксос, считаются неотчуждаемой собственностью семей, проживающих на острове.

Контроль над ресурсами наждака и корунда не осуществляется ни через владение заводами по дроблению, помолу и сортировке, ни через патенты или секретные процессы подготовки. Торговые объединения, влияющие на поставки наждака и корунда, неизвестны. В Соединенных Штатах, Великобритании, Франции и Германии существует ряд помольных компаний, которые конкурируют за мировые поставки сырьевых ресурсов, а компании каждой страны конкурируют друг с другом за рынки сбыта отсортированного, подготовленного материала.

ПОЛОЖЕНИЕ СТРАН

Соединенные Штаты располагают запасами наждака низкого качества и ресурсами корунда, которые недостаточно развиты для удовлетворения спроса на природные абразивные материалы. Во время войны Соединенные Штаты испытывали нехватку наждака и корунда, требуемых потребителями. Однако этот дефицит был компенсирован избыточным предложением искусственных абразивов.

Англия, имея Индию и Южную Африку, обладает запасами корунда, вероятно, более чем достаточными для ее нужд. Англия, вероятно, достаточно хорошо обеспечена этими абразивами, особенно до тех пор, пока она продолжает импортировать из Канады и Соединенных Штатов необходимые искусственные абразивы.

Франция не имеет собственных запасов наждака и корунда, но обладает крупными ресурсами в своей колонии Мадагаскар, а во время войны контролировала поставки греческого наждака. Кроме того, Франция имеет в резерве богатые месторождения бокситов и гидроэлектроэнергию для производства искусственных абразивов.

Германия во время войны зависела от турецкого наждака. Она испытывает нехватку бокситов, но производит большое количество карборунда.

Япония, вероятно, может удовлетворить свои потребности, используя ресурсы индийского корунда и искусственные абразивы из Соединенных Штатов. Во время дефицита поставок в 1917 году некоторое количество материала было экспортировано в Соединенные Штаты из Японии.

РЕЗЮМЕ

Корунд и наждак, причем последний представляет собой тесную ассоциацию корунда с некоторыми другими минералами, используются в качестве абразивов для шлифовки и полировки металлов, стекла, камня и дерева. Многие операции, ранее выполнявшиеся с помощью наждака и корунда, теперь выполняются с использованием искусственных абразивов на основе карбида и глинозема.

Месторождения наждака и корунда немногочисленны, но их продукции достаточно для всех текущих нужд. Коммерчески важные месторождения расположены в Аппалачском регионе Соединенных Штатов; на островах Греческого архипелага, особенно на острове Наксос; в провинции Айдын в Малой Азии; в президентстве Мадрас и провинциях Пенджаб, Бенгалия и Траванкор в Индии; на Мадагаскаре; и в Трансваале недалеко от Претории.

Геологическое строение месторождений наждака и корунда делает невозможной любую точную оценку запасов или какой-либо прогноз будущих открытий.

Политический контроль над мировыми ресурсами наждака и корунда соответствует географическому положению, за исключением месторождений на острове Наксос. Этот остров является греческой территорией, но французское правительство во время войны взяло под контроль наждачную промышленность и распределяло поставки абразива только для нужд промышленности Франции и ее союзников. Месторождения Малой Азии в настоящее время (1920 г.) номинально находятся под контролем Турции, но фактически частично — в прибрежных полосах, захваченных и удерживаемых итальянцами и греками после перемирия. Мадагаскар является французским владением, а Трансвааль и Индия — частями Британской империи.

Месторождения Соединенных Штатов принадлежат ряду мелких независимых операторов, все из которых, насколько известно, являются американцами. Канадские месторождения в значительной степени контролируются одной компанией, Manufacturers Corundum Co., владельцы которой преимущественно или полностью являются канадцами. Греческие месторождения наждака, особенно на Наксосе, считаются неотчуждаемой собственностью семей, проживающих на острове.

Таблица 64.—Добыча наждака и корунда, 1910-1917 гг.

| Emery | Corundum
United States [149] | Greece [149] | Turkey | United States [149] | Canada [149] | India [149] | Mada- gascar [149] | So. Africa [149]

Ore
produced
(long tons)
Ore
shipped
from Syria
(metric tons)

Grains
produced
(long tons)
Grains
shipped
(long tons)
Grains
produced
(long tons)
Grains
or ore
produced
(metric tons)
Grains
or ore
produced
(long tons)

1910 |    940 | 12,939 | [150] | [151] |  1,660 |    218 |     11 | [150]
1911 |    620 |  9,845 | [150] | [151] |  1,270 |    275 |    150 | [150]
1912 |    870 |  7,687 | [150] | [151] |  1,600 |    345 |    496 |     99
1913 |    900 |  1,440 | [150] | [151] |  1,090 |    355 |  1,099 | [150]
1914 |    460 | 10,226 | [150] | [151] |    500 |    105 |    556 | [150]
1915 |  2,840 | [150] | [150] | [152] |    220 |     62 |    327 | [150]
1916 | 14,400 | [150] | [150] | [152] |     60 |  1,868 |    914 | [150]
1917 | 15,400 | [150] | [150] |    770 |    160 | [150] | [151] | [153]4,051

[149] Статистика по Соединенным Штатам — Геологическая служба США; по Канаде — Министерство горнодобывающей промышленности Канады; по Греции — отчеты британских консульств, цитируемые в «Mineral Industry»; по Индии — отчеты Геологической службы Индии; по Мадагаскару — Горное управление Мадагаскара; по Южной Африке — отчеты американских консульств.

[150] Данные отсутствуют.

[151] Добыча не велась.

[152] Небольшое неучтенное количество.

[153] Девять месяцев, янв.-июнь и окт.-дек.

ГЛАВА XXI МАГНЕЗИТ Автор: Р. У. Стоун

ПРИМЕНЕНИЕ МАГНЕЗИТА

Магнезит и продукты его переработки используются в различных отраслях промышленности, наиболее важной из которых, вне всякого сомнения, является металлургия. Благодаря высокой температуре плавления и химической инертности оксида магния магнезит является одним из основных минералов, используемых в металлургической и других отраслях промышленности, где требуются высокоогнеупорные материалы. Для этой цели используется магнезит, обожженный до спекания (dead-burned magnesite), в виде кирпича или зерен. Кирпич и фасонные изделия применяются для футеровки мартеновских сталеплавильных печей, сварочных, нагревательных и плавильных печей, отражательных печей, отстойников и печей для рафинирования свинца, конвертеров для меди и электрических печей. Дробленый или зернистый магнезит используется для футеровки подин мартеновских сталеплавильных печей, а также при изготовлении тиглей и купелей.

В производстве цемента, известного как оксихлоридный или цемент Сореля, количество используемого магнезита уступает только количеству, используемому для огнеупорных целей. Этот цемент широко применяется для санитарных полов и, в меньшей степени, для штукатурки стен, как внутренних, так и наружных. Он также используется вместо портландцемента для некоторых видов наружных строительных работ, где требуется быстрое и прочное схватывание. Магнезит используется в производстве бумаги из древесной массы на Тихоокеанском побережье, в огнестойких красках, в качестве теплоизолятора в покрытиях труб и печей, а также в производстве хлорида магния, легкого карбоната и других продуктов, включая металлический магний.

ГЕОЛОГИЧЕСКОЕ ЗАЛЕГАНИЕ

Месторождения магнезита широко распространены по всему миру и встречаются в двух различных формах: аморфной и кристаллической. Аморфный магнезит, наиболее распространенная форма, является мелкозернистым и плотным; он обычно встречается в виде жил или масс в серпентине, образовавшемся в результате изменения магнезиальных пород семейства перидотитов. К этой группе относятся греческие месторождения, почти все месторождения Калифорнии, а также месторождения в Мексике, Венесуэле и других частях мира. Кристаллический магнезит является средне- или крупнозернистым и встречается в виде масс в известняках, доломитах или сопутствующих осадочных породах, которые подверглись метаморфизму. Основными месторождениями этого класса являются месторождения в Австрии, Венгрии, Квебеке и Вашингтоне.

Считается, что месторождения магнезита возникли тремя способами. Массивная некристаллическая разновидность, такая как в Калифорнии и Греции, как полагают, образовалась в результате разложения серпентина. Месторождения магнезита около Биселла, Калифорния, и на реке Мадди, недалеко от Сент-Томаса, Невада, считаются осадочного происхождения. Австро-венгерские, вашингтонские и квебекские месторождения рассматриваются как результат замещения известковых осадочных пород магнезиальными растворами.

Месторождения магнезита, встречающиеся в виде жил в связи с серпентинизированными магнезиальными породами, вероятно, образовались как в результате разрушения минералов, образующих серпентин, так и из самого серпентина. По-видимому, обычно как серпентин, так и магнезит образуются в процессе распада первичных минералов в перидотитах и родственных им основных породах, и что во время распада серпентина продолжается образование магнезита. В любом случае магнезия или магнезиальный минерал превращается в карбонат, растворяется просачивающейся водой, насыщенной углекислым газом, и осаждается в трещинах и пустотах в виде жил. При таком способе образования магнезит встречается в виде крупных и мелких жил, линз и штокверков, а его распределение и протяженность носят беспорядочный характер. Справедливо предположить, что эти месторождения могут простираться до предела глубины легко циркулирующих поверхностных вод, что в благоприятных условиях может составлять несколько сотен футов. С другой стороны, сбросы с такой же вероятностью могут прервать жилы как по глубине, так и по простиранию. Любая оценка доступного тоннажа магнезита в месторождениях этого типа поэтому необоснованна до проведения разведочных работ.

Осадочные месторождения, такие как месторождения Биселла, Калифорния, и около Сент-Томаса, Невада, по своей природе более регулярны по залеганию, и их тоннаж может быть оценен по обнажениям в естественных выходах и шурфах.

Месторождения замещения, подобные тем, что находятся в Вашингтоне и Квебеке, не столь регулярны, как осадочные месторождения, но более регулярны, чем жилы, и оценки тоннажа могут основываться на поверхностном обнажении и предполагаемой глубине от 50 до 100 футов.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Известное распределение месторождений магнезита выглядит следующим образом:

Северная Америка.

Канада: Квебек, Британская Колумбия и другие места.

Соединенные Штаты: Калифорния, Вашингтон, Невада.

Мексика: Нижняя Калифорния на острове Санта-Маргарита.

Южная Америка.

Венесуэла: остров Маргарита.

Европа.

Австрия, Венгрия, Германия, Греция, Италия, Македония, Норвегия, Швеция, Россия.

Африка.

Трансвааль, Родезия, Португальская Западная Африка.

Азия.

Индия, в Мадрасе и Майсуре.

Австралия.

Квинсленд, Новый Южный Уэльс, Южная Австралия, Тасмания.

Океания.

Новая Каледония.

Следующее описание по странам приведено в порядке, указанном выше:

Северная Америка.

Канада.

— Основные месторождения магнезита в Канаде находятся в округе Гренвилл, графство Аржантей, Квебек, где минерал ассоциирован с серпентином, доломитом и другими минералами. Магнезит в округе Гренвилл представляет собой блестящий кремово-белый, молочно-белый или серый материал, который встречается в виде обширных масс, ассоциированных с полосами или линзами темно-зеленого или светло-желтого серпентина. По всей массе месторождений магнезит и доломит настолько похожи по внешнему виду, что обнаружение доломита затруднительно. Существует значительное количество положительных доказательств в поддержку гипотезы о том, что месторождения образовались путем растворения и замещения кристаллического известняка под воздействием магнезиальных растворов. Выходы месторождений достигают 1000 футов в длину и 300 футов в ширину. По оценкам, в поле зрения находится 686 900 тонн магнезита, содержащего менее 12 процентов CaO, и 483 700 тонн магнезит-доломита, содержащего более 12 процентов CaO.

В горнодобывающем округе Атлин, в Британской Колумбии, были отмечены как магнезит, так и гидромагнезит, но обширные массы гидромагнезита недалеко от города Атлин являются наиболее важными. Эти месторождения представляют собой поверхностные пласты мелкопорошкообразного белого гидромагнезита толщиной от 6 до 8 футов, которые покрывают площади до 18 акров. По оценкам, две группы этих месторождений содержат 180 000 тонн гидромагнезита.

Соединенные Штаты.

— Магнезит в коммерческих количествах встречается в Калифорнии, Неваде и Вашингтоне. Сообщения о пригодных для разработки месторождениях в других штатах не были подтверждены.

В Калифорнии месторождения магнезита находятся во многих местах по всему Береговому хребту и на западном склоне Сьерры, от округов Мендосино и Плейсер на севере до округа Риверсайд на юге. До войны добыча была ограничена несколькими районами, а годовой объем производства составлял около 10 000 тонн, но спрос, вызванный значительным сокращением импорта, стимулировал активную разведку и разработку, в результате чего в 1917 году тринадцать округов дали в общей сложности 211 663 тонны стоимостью 2 116 630 долларов. В девяти округах месторождения крупные, и в четырех округах пока найдены только небольшие месторождения. Наиболее важные месторождения находятся в округах Напа, Санта-Клара, Сан-Бенито и Туларе. В 1917 году 63 процента добытого сырого магнезита было добыто в округе Туларе. Практически все месторождения магнезита в Калифорнии представляют собой нерегулярные жилы в серпентине, образовавшиеся в результате изменения магнезиальных магматических пород.

В штате Вашингтон месторождения кристаллического магнезита были найдены в нескольких местах. Вашингтонский магнезит сильно отличается от калифорнийских месторождений и встречается в виде более крупных масс. Он крупнокристаллический, похожий на мрамор или крупнозернистый доломит, и бывает красного, розового, черного, белого и серого цвета. Магнезит округа Стивенс образовался путем замещения линз доломита в осадочных породах. Перекристаллизация более чистого магнезиального карбоната могла быть вторичной и находиться под влиянием интрузии основной магнезиальной породы, которая в некоторых местах встречается выше и ниже магнезита. Более крупные месторождения имеют толщину 200 или более футов и длину 1000 или более футов. Оценки в один миллион тонн в пределах 100 футов от поверхности являются разумными по крайней мере для трех месторождений. Добыча в Вашингтоне началась в декабре 1916 года с объемом производства 715 тонн. Объем производства в 1917 году составил 105 175 тонн стоимостью 783 188 долларов.

Единственным известным месторождением магнезита в Неваде является обширный осадочный пласт в долине реки Мадди, округ Кларк. Магнезит содержит более 5 процентов извести и более 11 процентов кремнезема. Он не разрабатывался.

Общий объем производства магнезита в Соединенных Штатах в 1915 году составил 30 499 коротких тонн; в 1916 году — 154 974 короткие тонны; в 1917 году — 316 838 коротких тонн; и в 1918 году — 231 605 коротких тонн.

Мексика.

— На острове Санта-Маргарита, в заливе Магдалена, Нижняя Калифорния, находятся обширные месторождения магнезита, из которых осуществлялся экспорт в Соединенные Штаты. Стены каньонов в горах показывают массы магнезита толщиной в несколько футов, а валуны магнезита усеивают русла рек. Большие количества можно получить без добычи, и их нужно только раздробить для отправки. Анализ кальцинированного магнезита с острова Санта-Маргарита показывает практически полное отсутствие кремнезема, извести или железа.

Южная Америка.

— Месторождения на острове Маргарита, Венесуэла, относятся к аморфному или калифорнийскому типу и встречаются в виде жил и штокверков. Информация об их размерах отсутствует, но в 1915 году в Соединенные Штаты было экспортировано 500 тонн.

Европа.

— Месторождения магнезита в Австрии и Венгрии, которые до недавнего времени обеспечивали значительную часть мировых поставок, простираются вдоль северо-восточной линии на несколько сотен миль через обе страны. Минерал встречается в виде линз. Крупное месторождение недалеко от Файтча, Австрия, имеет размеры от 700 до 800 футов от вершины до основания. Руда добывается карьерным способом в виде серии уступов. Еще одно очень крупное месторождение в Австрии находится в Радентайне. Магнезит добывается большими разрезами и опускается под действием силы тяжести к вращающимся печам. Кальцинация производится рядом с шахтой, и отгружаются как зернистый магнезит, так и магнезитовые кирпичи. Собственность принадлежала американцам до войны, и большая часть продукции шла в американские порты.

Магнезит в этих месторождениях является кристаллическим и встречается в доломите, вероятно, каменноугольного возраста, из которого он был получен путем инфильтрации растворов карбоната магния и выщелачивания растворимого карбоната кальция. Он мелко- или крупнокристаллический, желтого или голубовато-белого цвета, содержит от 3 до 4,5 процента оксида железа, менее 2 процентов кремнезема и менее 3 процентов извести. Он легко кальцинируется до состояния спекания и дает удовлетворительный зернистый магнезит и кирпич для огнеупорных целей.

Месторождения магнезита в течение многих лет разрабатывались недалеко от Франкенштейна, Силезия, Германия.

В провинции Сантандер, на севере Испании, крупнокристаллический магнезит, залегающий в нижнемеловых известняках и доломитах, добывался в течение ряда лет. Объем производства в 1915 году составил 1400 тонн.

В Греции магнезит относится к некристаллическому типу и встречается в ассоциации с серпентином в виде жил и масс. Наиболее важные месторождения находятся на острове Эвбея. Эвбейские месторождения расположены близко к морскому побережью, и в нормальных условиях доступна дешевая водная транспортировка на основные рынки магнезита в мире. Производство греческого магнезита в 1914 году находилось в основном в руках трех компаний: Anglo-Greek Magnesite Co., 24 Finsbury Sq., Лондон; Société Hellenique des Mines, Афины; и Hellenic Magnesite Co., Афины. Распределение магнезита контролируется лондонской компанией. Anglo-Greek Magnesite Co. разрабатывает шахты в Галатаки и Афратионе на Эвбее. На шахтах Галатаки вскрытая жила руды имеет длину 1300 футов и ширину от 50 до 60 футов. Société Hellenique des Mines (ныне называемая The Financial Corporation of Greece, Ltd.) контролирует добычу на нескольких шахтах в Мантуди, Лимни, Ларимне и др. Hellenic Magnesite Co. получает большую часть своей руды из поверхностных выработок. В 1912 году производство магнезита несколькими компаниями в Греции (не включая Hellenic Magnesite Co.) было следующим: сырой магнезит — 87 338 тонн; кальцинированный магнезит — 30 645 тонн; магнезит, обожженный до спекания — 3 201 тонна. Это эквивалентно примерно 150 000 тонн сырой руды и не включает продукцию одного из трех крупнейших производителей.

Магнезит из Греции и магнезит из Калифорнии практически идентичны по физическим и химическим характеристикам, но до 1915 года калифорнийский материал не мог конкурировать с греческим на нью-йоркском рынке из-за того, что трансконтинентальный тариф на перевозку был слишком высоким по сравнению с океанским фрахтом на материал, перевозимый в качестве балласта.

Магнезит встречается в больших количествах в Македонии, залегая в виде жил в серпентине.

Месторождения магнезита, которые ранее разрабатывались, встречаются в Италии в районе Турина и на острове Эльба. Ни одно из месторождений, по-видимому, не является крупным. Анализ магнезита с острова Эльба показывает более 8 процентов кремнезема, следы железа и от 1 до 3,5 процента извести.

Магнезит встречается в Норвегии в виде небольших жил в серпентине, но, в отличие от другого магнезита в серпентине, он является кристаллическим. Он примечателен тем, что не содержит извести, но содержит более 4 процентов железа и 9 процентов кремнезема. Его кальцинируют и делают из него кирпич.

Месторождения, подобные тем, что находятся в Норвегии, встречаются в Швеции, но из-за их расположения, которое влечет за собой высокие эксплуатационные и транспортные расходы, сомнительно, что они когда-либо смогут конкурировать с более дешевым европейским магнезитом.

Магнезит добывался в Оренбургской губернии, Россия. Одна шахта дала 26 320 метрических тонн в 1906 году. Магнезит встречается также на северном склоне Кавказских гор.

Африка.

— Обширные месторождения магнезита встречаются в Трансваале в виде жил, толщина которых достигает 4 футов. Порода используется для производства углекислого газа и оксихлоридного цемента. Сообщается о крупных месторождениях магнезита в Португальской Западной Африке. Месторождения находятся рядом с горячими источниками или связаны с ними.

Азия.

— Наиболее важное месторождение магнезита в Индии, по-видимому, находится в президентстве Мадрас, в южной части полуострова Индостан, где минерал встречается в виде переплетающихся жил. Основные месторождения давали более 2000 тонн в год.

Кристаллический магнезит встречается в известняках в горах Маньчжурии и добывается в Дайсецукё для огнеупорных целей.

Сообщается о наличии магнезита в Азиатской Турции примерно в 75 километрах от Смирны.

Австралия.

— Месторождения магнезита в Квинсленде настолько малы, что, вероятно, не имеют коммерческой ценности. Округлые блоки чистого белого магнезита выходят на поверхность в одном месте в Новом Южном Уэльсе, где многие тысячи тонн доступны при небольших затратах. Анализ показывает 99,01 процента карбоната магния и отсутствие извести. Сообщается о крупных месторождениях магнезита в Южной Австралии. Обширные месторождения также встречаются на северной оконечности западного побережья Новой Каледонии. Небольшое количество было экспортировано.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Месторождения магнезита, играющие заметную роль в мировой экономике, расположены в Канаде, Соединенных Штатах, Австро-Венгрии и Греции.

Соединенные Штаты.

— Основные месторождения магнезита в штате Вашингтон принадлежат Northwest Magnesite Co., Спокан, Вашингтон; Valley Magnesite Co., Спокан, Вашингтон; и American Mineral Production Co., Чикаго, Иллинойс. Northwest Magnesite Co. является крупнейшим производителем в Вашингтонском поле и, вероятно, сделала крупнейшие инвестиции. American Mineral Production Co. имеет завод в Вэлли, Вашингтон; Valley Magnesite Co. имеет месторождение недалеко от Вэлли, но не разрабатывает его.

Основными производителями магнезита в Калифорнии летом 1918 года были Tulare Mining Co. с шахтой недалеко от Портервилла; Porterville Magnesite Co. of California с шахтой в Портервилле; Western Magnesite Development Co. с шахтой на Ред-Маунтин; и Фрэнк Р. Суизи, разрабатывающий шахту Уайт-Рок, Поуп-Вэлли, округ Напа.

Австрия.

— Veitscher Magnesite Co. из Вены и Magnesite Co., Ltd. из Будапешта сформировали объединение или картель с пониманием или соглашением о том, что все продажи магнезита за пределами Австрии и Венгрии должны осуществляться через Carl Spater & Co., немецкую фирму в Кобленце, Германия. Фирма Carl Spater & Co. ранее владела заводами Veitscher Magnesite Co., но продала их и получила бессрочное агентство по продажам, когда была сформирована акционерная компания. Harbison-Walker Refractories Co., Питтсбург, Пенсильвания, как говорят, была американским представителем Spater & Co.

Austro-American Magnesite Co., чье месторождение и заводы в Радентайне, Австрия, представляют собой инвестиции в размере 1 800 000 долларов, принадлежат американцам. Весь акционерный капитал абсолютно контролируется основными акционерами American Refractories Co., или так контролировался до войны. Austro-American Magnesite Co., как утверждается, до войны фактически осуществляла 95 процентов бизнеса по магнезиту в Англии и около 65–70 процентов бизнеса в Соединенных Штатах. Эта компания имеет мощность 150 000 тонн кальцинированного магнезита в год.

Когда выяснилось, что Carl Spater & Co., которые занимаются как магнезитом, так и магнезитовым кирпичом, произведенным Veitscher Magnesite Co. и Magnesite Co., Ltd., не будут продавать магнезит английским производителям огнеупорного кирпича, Austro-American Magnesite Co. сформировала торговую компанию в Англии под названием Anglo-Austrian Magnesite Co., Шеффилд, Англия. Английская компания продавала магнезит с заводов Austro-American Magnesite Co. в Радентайне, Австрия, всем производителям огнеупорного кирпича в Англии и фактически забрала всю английскую торговлю у немцев.

General Magnesite Co. из Будапешта имеет месторождение магнезита и завод в Хизонвиче (Hisnyoviz?), Венгрия. Акции этой компании, как полагают, принадлежат в основном акционерам General Refractories Co., 111 Бродвей, Нью-Йорк. Остальная часть акций, как полагают, около 40 процентов, принадлежит некоторым венграм из Будапешта, которых представляет г-н Ганст из Будапешта, президент компании.

Согласно Министерству торговли Соединенных Штатов [154], в Греции семь компаний эксплуатируют магнезит: Anglo-Greek Magnesite Co., Ltd. с головными офисами в Лондоне, Англия; Société Financière de Grèce, улицы Солон и Ликабеттус, Афины; The Internationale Magnesite Werken с головными офисами в Роттердаме, Нидерланды; Л. Карамбелас, Лимни, Эвбея; Н. Папантонатос, Лимни, Эвбея; Г. А. Георгидадес, Афины (эксплуатирующий концессию от имени General Magnesite & Magnesia Co. из Филадельфии); и Алексиу, Дафнопотамос, Эвбея. У большинства производителей в 1917 году было изобилие заказов на магнезит для использования в сталелитейной промышленности Франции и Англии.

[154] Commerce Reports, 1 мая 1917 г.

РЕЗЮМЕ

Основное и самое важное использование магнезита — в металлургии, в качестве огнеупорного материала для футеровки печей. Магнезит также используется в производстве цемента Сореля и бумаги из древесной массы, в огнестойких красках, в качестве теплоизолятора в покрытиях труб и печей, а также в производстве хлорида магния, легкого карбоната и других продуктов, включая металлический магний.

Магнезит встречается в двух формах: аморфной и кристаллической, и месторождения возникают тремя способами: в результате разложения серпентина, в виде осадочных месторождений и путем замещения известковых осадочных пород магнийсодержащими растворами. До проведения разведочных работ невозможно сделать надежные оценки доступного тоннажа первого типа, но можно сделать довольно точные оценки месторождений второго и третьего типов.

Разработанные месторождения магнезита, которые в свое время были продуктивными, расположены в Калифорнии и Вашингтоне; в Квебеке и Британской Колумбии, Канада; на острове Санта-Маргарита, Нижняя Калифорния; на острове Маргарита, Венесуэла; в Австро-Венгрии, Германии, Испании, Греции, Македонии, России, Норвегии, Трансваале и Индии. Другие месторождения, некоторые из которых давали небольшие количества, расположены в Неваде, Онтарио, Нью-Брансуике, на острове Седрос, Нижняя Калифорния; в Малой Азии, Швеции, Родезии, Португальской Западной Африке, Австралии, Тасмании и Новой Каледонии. Нет оснований полагать, что в ближайшем будущем произойдет какой-либо заметный сдвиг в важных источниках поставок. В 1916 и 1917 годах добыча на месторождениях Тихоокеанского побережья Соединенных Штатов увеличивалась очень быстро, но с января 1918 года наблюдается резкий спад производства в Калифорнии.

Месторождения магнезита в Калифорнии и Вашингтоне принадлежат ряду компаний, все из которых американские. Считается, что американские производители огнеупоров заинтересованы в некоторых канадских месторождениях. Месторождения на островах Санта-Маргарита и Седрос, Нижняя Калифорния, по-видимому, принадлежат или эксплуатируются в основном жителями Калифорнии. Месторождения у побережья Венесуэлы принадлежат филадельфийской компании. Две крупные магнезитовые компании Австро-Венгрии договорились осуществлять все свои продажи за пределами Австро-Венгрии через немецкую фирму в Кобленце. Две другие компании, Austro-American Magnesite Co. и General Magnesite Co., принадлежат в основном американцам. Месторождения магнезита в Греции контролируются семью компаниями, одна из которых английская, одна американская, одна голландская, а остальные, по-видимому, греческие. Другие месторождения магнезита в мире в настоящее время не имеют большого значения.

ГЛАВА XXII ГРАФИТ Авторы: Х. Г. Фергюсон, Фрэнк Ф. Граут и Джордж Д. Даб

ПРИМЕНЕНИЕ ГРАФИТА

Графит производится в нескольких сортах, которые адаптированы для различных целей. Аморфный графит — это торговый термин, применяемый к некристаллическому или очень мелкозернистому графиту различной степени чистоты. Если кристаллический графит производится в виде хлопьев или чешуек, это чешуйчатый графит; но если он добывается из жил, он может иметь другие формы и называться жильным графитом. Кусковой, чипсовый и пылевидный графит относятся к продуктам из более крупных кристаллов цейлонского жильного графита, более или менее разбитых при добыче и обработке. Все эти три вида называются кристаллическими. Искусственный графит, изготовленный из угля или другого углеродистого вещества, напоминает аморфную разновидность.

Графит для использования в тиглях должен быть высокого качества, либо кусковой, либо чипсовый, либо чешуйчатый, содержать не менее 85 процентов графитового углерода и быть свободным от флюсующих примесей. Жильный графит считается особенно желательным для этого использования. Возможно, расширение использования электрических печей в сталелитейной промышленности и в цветной металлургии уменьшит спрос на тигли. Как кристаллический, так и аморфный графит используются в качестве смазочных материалов. Для этой цели графит должен быть свободен от кварца или других абразивных примесей. Для литейных покрытий в основном используются аморфный графит и цейлонская пыль; материал высокого качества не требуется. Для лучших сортов карандашей нужны смеси кристаллического и высококачественного аморфного графита; для более низких сортов используется только аморфный. Графит, используемый в качестве полировки для взрывчатых веществ, является аморфным. Это использование не потребляет больших количеств. Для производства электродов наиболее подходящим считается искусственный графит. Графит, используемый в качестве наполнителя для сухих батарей, может быть аморфным, искусственным или кристаллическим. Требуется чистый материал, но размер зерна не является фактором.

Аморфный графит используется в составах для котлов для предотвращения образования твердой накипи; чистый материал не является обязательным. Для красок можно использовать как аморфный, так и кристаллический графит, и они не обязательно должны быть высокого качества.

Для полировки печей и обуви в основном используется аморфный графит; имперский графит используется в качестве фальсификата в удобрениях, чтобы придать желаемый темный цвет.

Вместо аморфного графита и пыли можно использовать искусственный графит. Для кристаллического графита, используемого в производстве тиглей, хорошей замены нет. Однако использование электрических печей или печей с открытым пламенем в цветной металлургии может уменьшить потребность в тиглях. Для смазки слюда используется примерно так же, как графит, но она намного хуже. Многие другие составы для котлов служат той же цели, что и графит. В красках заменителем является сажа. Тальк используется в сочетании с графитом и в качестве частичного заменителя графита в литейном производстве. Графит из доменных печей, или «киш», предлагает возможности в качестве заменителя чешуйчатого графита для смазочных целей. Разработки в этом направлении, однако, не продвинулись достаточно далеко, чтобы быть окончательными.

ГЕОЛОГИЧЕСКОЕ ЗАЛЕГАНИЕ

Аморфный графит может встречаться везде, где угольные или другие углеродистые пласты подверглись региональному или магматическому метаморфизму. Кристаллический графит имеет два основных геологических залегания: в виде чешуек в сланцах и в виде более крупных кристаллов в жилах. Чешуйчатый графит в сланцах обычно ассоциируется с гранитными интрузиями, которые, по-видимому, способствовали перекристаллизации первичного углеродистого материала в осадочных породах. Жильный графит в коммерческих количествах встречается довольно редко. Он находится в ассоциации с гранитными интрузивами и, как правило, с графитовыми осадочными породами, содержащими чешуйчатую разновидность. Такие породы в большинстве частей мира не были достаточно разведаны, чтобы убедиться, что все важные тела графита обнаружены.

МИРОВАЯ МОЩНОСТЬ ПО ПРОИЗВОДСТВУ ГРАФИТА

В порядке их важности в следующей таблице перечислены различные страны, которые производят графит или в которых были обнаружены месторождения графита:

1. Кристаллический графит

А. Жильный графит

Ceylon—could produce up to 35,000 short tons per year, all grades.

Соединенные Штаты — небольшая добыча из Монтаны.

Канада — небольшое количество, произведенное недавно.

Б. Чешуйчатый графит

Madagascar—could produce up to nearly 50,000 short tons per year.

Бавария — в среднем 12 000 тонн за несколько довоенных лет, и значительно увеличила производство во время войны. Произвела 40 000 метрических тонн в 1917 году.

United States—could readily produce 4,000 tons of flake exclusive of dust.

Canada—could probably produce 1,200 tons of flake exclusive of dust.

Испания — месторождения разрабатываются.

Норвегия — сообщается о новых разработках.

Румыния — недавно сообщалось о важных месторождениях.

Япония — не производила очень много.

Швеция — очень небольшое производство.

Трансвааль — очень небольшое производство, потребляемое на месте.

Гренландия, Бразилия — сообщается о крупных месторождениях. Очень мало разработок.

Германская Восточная Африка (бывшая) — сообщается о месторождениях предположительно большого размера.

2. Аморфный графит

Германская Австрия, Чехословакия — давно производят большое количество графита ежегодно.

Chosen—could probably produce 12,000 tons per annum.

Italy—could probably produce 12,000 tons per annum.

Mexico—could probably produce 6,000 tons per annum.

United States—could readily produce 6,000 tons natural and 6,000 tons artificial amorphous graphite.

Spain—could probably produce 1,000 tons annually.

France—could probably produce 1,000 tons annually.

Сибирь — большое количество доступно, но не разработано.

Родезия — местное снабжение.

Бразилия — запасы не разработаны.

Квинсленд — запасы не разработаны.

БУДУЩИЕ РАЗРАБОТКИ

Хотя точных данных нет, считается, что Цейлон не сможет производить графит еще долго при нынешних темпах, и возможно, что фактическое истощение месторождений не за горами. Мадагаскар способен значительно увеличить производство. Сомнительно, что американские месторождения с содержанием графита менее 5 процентов смогут выдержать свободную конкуренцию с Мадагаскаром, где более 20 процентов добываемой породы составляет графит. Слишком мало известно о гренландских и бразильских месторождениях, чтобы строить догадки об их будущей важности, но сообщается, что в Гренландии существуют огромные запасы. Немецкие чешуйчатые месторождения вряд ли выдержат свободную конкуренцию с Мадагаскаром, если не будут внедрены современные методы. Аморфный графит, вероятно, будет по-прежнему производиться в основном Австрией, Богемией, Мексикой и Чосеном. Мексика и Чосен, скорее всего, будут поставлять большую часть карандашного графита в мире. Увеличение производства искусственного графита может уменьшить спрос на аморфный графит. В 1918 году в немецкой технической прессе появились сообщения об открытии огромных месторождений чешуйчатого графита в Румынии. Они должны были разрабатываться совместно немецким и австрийским правительствами по 75-летней концессии от румынского правительства. Исход войны, конечно, аннулировал эту договоренность.

Жильный графит (то есть цейлонский графит) предпочтителен для производства тиглей, но все большее количество чешуйчатого графита успешно используется. Европейские производители, по-видимому, используют почти исключительно чешуйчатый графит; и американские производители, несомненно, найдут это возможным, если потребуется. Все большее количество аморфного графита используется для различных промышленных целей, главным образом для литейных покрытий. Развитие электрических сталеплавильных печей, за счет сокращения использования тиглей, может в некоторой степени способствовать уменьшению разницы в стоимости между кристаллическим и аморфным графитом.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Аморфный графит настолько широко распространен, что ни одна из великих коммерческих наций вряд ли столкнется с серьезными трудностями в удовлетворении своих жизненно важных потребностей. Мексиканский графит является основным источником хорошего материала для карандашей. Интерес сосредоточен на материале, пригодном для изготовления тиглей.

Графит для тиглей в прошлом производился в основном на Цейлоне. Его зернистая форма (характерная для жильного графита) считалась производителями тиглей лучшей. Месторождения на Цейлоне разрабатываются в основном мелкими местными владельцами, а объем производства контролируется британцами через государственный суверенитет и судоходство. Контроль через владение и эксплуатацию с современным оборудованием был предпринят английской компанией, но встретил сопротивление со стороны местного населения до нескольких лет назад.

В последнее время чешуйчатый графит с Мадагаскара в значительной степени заменил цейлонский материал в европейской практике. Это месторождение находится под французским суверенитетом, и французы осуществляют высокую степень коммерческого контроля. Чешуйчатый графит Соединенных Штатов еще не достиг высокого уровня развития. Существуют большие запасы сланцев с содержанием графита около 5 процентов. Баварский материал является кристаллическим, хотя и не такого хорошего качества. Он находится под немецким контролем. До войны методы добычи и помола были примитивными, а продукт — соответственно низкого качества. Канада, Норвегия, Швеция, Гренландия, Бразилия и, возможно, другие страны имеют запасы чешуйчатого графита в своих границах. Япония имеет небольшое производство чешуйчатого графита и контролирует поставки в Чосене.

Американский контроль над мексиканскими шахтами направляет весь мексиканский объем производства в эту страну для рафинирования и реэкспорта. Одна из крупных канадских шахт также принадлежит Соединенным Штатам.

Когда британские поставки на Цейлоне сократились, а производство на Мадагаскаре увеличилось, британцы, которые всегда контролировали основные мировые поставки, не спешили отказываться от контроля. Они скупили большую часть продукции Мадагаскара и имеют на острове завод по обогащению. Morgan Crucible Co. из Лондона работает на острове как французская компания «Graphites Maskar», но это дочерняя компания лондонской фирмы, и контроль полностью британский. Однако это не единственный завод, работающий на острове. Одна крупная компания до войны имела главный офис в Гамбурге, Германия, один в Антверпене, и было несколько французских компаний. Некоторые австрийские шахты до войны принадлежали бельгийским компаниям, а английские интересы владеют частью итальянских месторождений.

Во время войны французы и британцы, успешно освоив мадагаскарский графит, по-видимому, заключили соглашение, согласно которому эти поставки должны были использоваться в Европе, в то время как цейлонский графит направлялся преимущественно в Соединенные Штаты. Контроль был возможен только благодаря объединению усилий британцев и французов, что, по всей видимости, было скорее коммерческим, нежели политическим вопросом, хотя и подлежало государственному регулированию.

По-видимому, среди производителей мадагаскарского графита существует объединение, о чем свидетельствует заявление консула в Тананариве в ноябре 1918 года о том, что «Union des Producteurs de Graphite» может ежегодно поставлять в эту страну 15 000–20 000 тонн 85-процентного графита по фиксированной цене франко-борт Таматаве. Цель этого объединения, судя по всему, заключается в защите производителей от недобросовестных действий со стороны покупателей.

В некоторых источниках упоминается «Коломбо Графит Юнион» (Colombo Graphite Union) как местное объединение, вероятно, связанное с Цейлонской торговой палатой. Оно не проявляло активности в совершенствовании методов добычи и обогащения, а также возражало против модернизации за счет внешнего капитала.

Ассоциация производителей графита Алабамы была организована в 1917 году, и ее целью было содействие интересам графитодобытчиков штата. Были предприняты усилия по честному отбору проб и анализу поставок, чтобы помочь устранить наиболее серьезные возражения производителей против использования местного чешуйчатого графита — ненадежность продукта.

ПОЛОЖЕНИЕ СТРАН

В Соединенных Штатах в изобилии имеется низкосортный аморфный графит. Во многих штатах и на Аляске есть запасы, которые практически не разрабатывались. В больших количествах доступен превосходный сорт материала из Мексики, что делает масштабную внутреннюю разработку нерентабельной, за исключением случаев, когда месторождения расположены очень выгодно. Самое продуктивное мексиканское месторождение принадлежит компании United States Graphite Co. из Сагино, штат Мичиган. Искусственный графит производится в больших количествах в Ниагара-Фолс, что делает страну независимой в вопросе поставок электродов.

Эта страна еще не является независимой в вопросе тигельного графита. Производители тиглей настаивают на использовании цейлонского графита в объеме около 15 000 тонн или более в год. Единственным источником аналогичного графита в стране является очень небольшое месторождение в Монтане. Однако в Алабаме, Пенсильвании, Нью-Йорке, на Аляске, в Техасе и, возможно, в других штатах имеются неплохие запасы чешуйчатого графита. До 1919 года производилось около 3500 тонн в год. Он больше напоминает мадагаскарский, чем цейлонский графит, хотя чешуйки у него мельче. Американские производители тиглей не спешат его использовать, хотя есть свидетельства того, что он мог бы вполне подойти. Если спрос на тигельный графит сохранится, то, вероятно, сохранится и спрос на импорт.

Наши месторождения не настолько высокосортны и не так выгодно расположены, чтобы успешно конкурировать с месторождениями Цейлона и Мадагаскара.

Канадские компании, производящие чешуйчатый графит, аналогичный американскому, частично принадлежат американскому капиталу.

Поставки чешуйчатого графита для производителей тиглей в обычное время могут осуществляться с Мадагаскара, но в случае необходимости мы можем быть достаточно независимыми, если будем готовы стимулировать добычу внутри страны.

Англия контролирует графит с Цейлона. Однако существует общее мнение, что добыча на Цейлоне, вероятно, будет сокращаться, если контроль не перейдет в руки тех, кто внедрит современные эффективные методы добычи. Англия обычно разрешает около двух третей цейлонской продукции поставлять в Соединенные Штаты. Собственные запасы тигельного графита Англии сейчас в основном поступают с Мадагаскара, где на острове работает компания, принадлежащая англичанам и находящаяся под их контролем. Аморфный графит поступает из Италии и Кореи. Лондонская компания ведет деятельность в Квебеке, производя некоторое количество чешуйчатого графита и графитовой пыли. Английский капитал инвестирован в итальянские месторождения графита, а по-видимому, также и в испанские.

Благодаря своему суверенитету над Мадагаскаром Франция, вероятно, контролирует лучшие в мире будущие запасы чешуйчатого графита. Месторождения крупные, удобно расположенные и удивительно богатые — 20 процентов графита или более. Они способны обеспечить значительно увеличенный объем добычи. Объем производства уже превышает показатели любой другой страны, хотя месторождения были освоены лишь недавно. Франция имеет небольшую местную добычу аморфного графита и получает некоторое количество из Италии.

Германия в настоящее время главным образом зависит от баварского чешуйчатого графита для производства тиглей. Усилия, предпринятые во время войны для получения цейлонского графита через Голландию и Швейцарию, указывают на то, что баварские запасы не вполне удовлетворительны. Аморфный графит поставляется из Австрии. Перепроизводство временами позволяло продавать продукцию в Америке ниже себестоимости.

Япония производит некоторое количество чешуйчатого графита. Корея обладает обильными запасами аморфной разновидности. В Корее были недавние открытия кристаллического графита, которые могут иметь значение.

На рисунке 11 показаны изменения в годовом объеме добычи графита в основных странах-производителях, а на рисунке 12 показана доля тигельных графитов, производимых основными источниками поставок.

РЕЗЮМЕ

Графит встречается в природе в двух формах: кристаллической и аморфной, каждая из которых имеет свои специфические области применения. Кристаллический графит используется в производстве тиглей, в качестве смазки и в красках. Аморфный графит используется в качестве смазки, для литейных форм, в карандашах, красках, как полироль для взрывчатых веществ, в составах для котлов, в электродах, сухих батареях, как средство для чистки печей и обуви, а также как наполнитель для удобрений. Большинство вышеперечисленных видов использования являются важными и их нелегко исключить. Искусственный графит, изготовленный из угля или других углеродистых материалов, может быть заменен природным аморфным графитом.

Рис. 11. — Годовой объем добычи графита в основных странах-производителях, 1902–1918 гг. Сплошные линии обозначают кристаллический графит; пунктирные линии — преимущественно аморфный графит.

Рис. 12. — Доля тигельного графита, производимого основными источниками поставок, 1907–1917 гг. Данные по Баварии с 1913 года сомнительны, но после завершения графика было обнаружено, что объем производства в 1917 году был значительно выше показанного.

Аморфный графит может встречаться везде, где угольные или другие углеродистые пласты подверглись региональному или магматическому метаморфизму. Кристаллический графит, как чешуйчатый, так и жильный, обычно встречается в ассоциации с гранитными интрузиями. Поскольку такие породы не были тщательно изучены во всех частях мира, вероятно, будут обнаружены важные новые месторождения графита, особенно в Канаде, Сибири и частях Южной Америки и Африки.

Цейлон является основным источником поставок лучших сортов кристаллического графита, а именно жильного графита. Кристаллический графит, получаемый на Мадагаскаре, в Баварии и в небольших количествах в Соединенных Штатах, Канаде, Норвегии, Швеции, Японии и Корее, в основном относится к чешуйчатой разновидности, и по этой причине производители считают его менее качественным, чем тот, что добывается на Цейлоне. Сообщается о крупных неразработанных месторождениях в Гренландии и Бразилии. Открытие крупных месторождений чешуйчатого графита в Румынии было зарегистрировано некоторое время назад. Время от времени поступают сообщения об открытиях в других местах, но их значимость сомнительна, главным образом потому, что месторождения обычно расположены в труднодоступных местах. Считается, что цейлонские месторождения прошли пик своей добычи, и если бы удалось найти месторождения жильного графита равного качества и богатства, цейлонские производители могли бы оказаться в трудном положении. За последние несколько лет Мадагаскар стал ведущим производителем кристаллического графита, и влияние этого потенциального источника должно оказать стабилизирующее воздействие на цены цейлонского графита.

Австрия, Корея, Мексика, Италия и Соединенные Штаты являются основными производителями аморфного графита; Корея и Мексика поставляют большую часть графита для карандашей в мире.

Развитие электропечей, несомненно, снизит спрос на тигли в сталелитейном производстве.

Великобритания через суверенитет над Цейлоном и Канадой, а Франция через суверенитет над Мадагаскаром политически контролируют самые важные в мире месторождения кристаллического графита. Япония контролирует месторождения Кореи.

Американский капитал контролирует месторождения Соединенных Штатов, месторождения Мексики и частично месторождения Канады. Цейлонские месторождения разрабатывались в основном мелкими местными владельцами, которые до недавнего времени противились попыткам английской компании получить контроль путем строительства и эксплуатации современного завода. Компания Graphites Maskar, владеющая частью мадагаскарских месторождений, является дочерним предприятием британской компании Morgan Crucible Co. Другая крупная мадагаскарская компания до войны имела свой главный офис в Гамбурге, Германия. Другие компании контролируются бельгийским и французским капиталом. Британские интересы владеют частью итальянских и, вероятно, частью испанских месторождений.

ГЛАВА XXIII СЛЮДА Автор: Дюран А. Холл

ПРИМЕНЕНИЕ СЛЮДЫ

Две разновидности слюды имеют особое экономическое значение: мусковит, или белая слюда, и флогопит, или янтарная слюда. Три другие разновидности — лепидолит, циннвальдит и биотит — находят эпизодическое коммерческое применение.

Слюда продается в виде листовой или блочной слюды, слюдяных пластин (расщепленной слюды), тонких листов, расщепленных главным образом из кусков блочной слюды меньшего размера, а также скрапа или молотой слюды. Области применения листовой или блочной слюды зависят от размера, толщины и формы куска, который можно из нее вырезать, а также от качества самого материала. Факторы, влияющие на качество слюды: наличие или отсутствие пятен, вкраплений, трещин или проколов; гибкость и эластичность; твердость; степень деформации листов; прозрачность и диэлектрическая прочность.

Важной областью применения листового или блочного мусковита являются электротехнические работы; из слюды изготавливают конденсаторы для радиооборудования, магнето и определенного телефонного оборудования; также в меньшей степени для резонаторов в звуковых коробках. Эта слюда также используется при изготовлении свечей зажигания, особенно для двигателей с высокой степенью сжатия, для намотки сердечников и в качестве шайб вместо фарфора. Эти области применения были значительно расширены во время войны для удовлетворения потребностей автомобильного транспорта, авиации и радиооборудования.

Большое количество этой разновидности слюды используется для других изоляционных целей. Существует огромное разнообразие применений, таких как листы, шайбы и диски в динамо-машинах, патронах для электрических ламп, защитные элементы в реостатах, распределительных коробках, телефонах и т. д.

Листовой или блочный флогопит используется для общей электрической изоляции — особенно там, где требуется слюда мягче мусковита.

Слюдяные пластины как мусковита, так и флогопита используются для производства «щипаной слюды» (built-up mica), которая широко применяется для электрической изоляции во многих различных формах, таких как листы, трубки, чашки и т. д. Слюдяной картон, изготовленный из пластин флогопита, широко используется для изоляции между медными сегментами коллекторов.

Среди менее важных областей применения листовой или блочной слюды (главным образом мусковита) — окна для передних панелей печей и духовок; дымоходы и абажуры для ламп и фонарей; а также многие другие цели, где требуется прозрачный, негорючий, небьющийся материал. Она также используется для теплоизоляции в различных электрических нагревательных приборах.

Молотая слюда также используется для теплоизоляции, например, в покрытиях для труб и котлов и т. д.; а также в качестве запатентованного кровельного материала, как в виде покрытия для предотвращения слипания при сворачивании в рулоны, так и в качестве наполнителя в самой кровле. Она также используется при отжиге стали и в качестве смазки для деревянных подшипников.

Среди второстепенных областей применения слюды, для которых известны удовлетворительные заменители, — использование листовой или блочной слюды для мембран фонографов и в декоративных целях, главным образом в Индии. На аналогичной основе базируется использование молотой слюды (смешанной с маслом) в качестве смазки для металлических подшипников; в качестве наполнителя для резиновых изделий и т. д.; а также в декоративных целях — в обоях, декоративных красках, отделочном камне и т. д.

Заменители.

— Никакое другое вещество не обладает сочетанием эластичности, прочности, гибкости, прозрачности, способности выдерживать чрезмерный нагрев и резкие перепады температуры, высокой диэлектрической прочности, плоскостности и способности расщепляться на тонкие пленки, которое присуще слюде.

Для огромного разнообразия электрооборудования, в котором используется слюда, удовлетворительного заменителя не найдено. В производстве некоторых низковольтных конденсаторов вместо слюдяных пленок использовались листы промасленной бумаги, но попытки более широкого использования этого материала не увенчались успехом. Согласно одному отчету, в Германии во время войны был разработан спрессованный бумажный продукт под названием «Пертинакс», который, как утверждается, является «наиболее удовлетворительным» для всех электрических целей, даже для производства высоковольтных конденсаторов. Однако тот факт, что Германия платила 75 долларов за фунт слюды из Норвегии и продолжала использовать слюду в производстве конденсаторов для авиационных магнето, указывает на то, что полная замена была невозможна.

Для многих целей остекления можно использовать жаропрочные или небьющиеся разновидности стекла.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Из-за характера месторождений слюды было мало стимулов для применения каких-либо методов добычи, кроме довольно грубых и простых. Эти методы оказывались достаточными до тех пор, пока оставались новые и легкодоступные месторождения. В настоящее время в Индии, Канаде и Соединенных Штатах наблюдается тенденция к применению более научных методов разведки и добычи там, где существует угроза истощения легкодоступных месторождений.

Сортировка, очистка, классификация, обрезка и резка слюды для рынка — это по существу ручные процессы, и в силу характера продукта они таковыми и останутся. По этой причине производящие регионы, обладающие обильной дешевой рабочей силой, имеют явное преимущество перед теми, где рабочая сила дорога и дефицитна. В одном важном направлении были предприняты попытки применить механическое устройство к процессу, который всегда требовал ручного труда. Это касается производства слюдяных пластин, широко используемых в производстве «щипаной слюды». Эти изобретения еще не доказали свою коммерческую успешность в широком масштабе.

Слюда все чаще используется в электрических целях. Война создала большой спрос, особенно на лучшие сорта материала для производства магнето, радиоконденсаторов и свечей зажигания, и многие из этих областей применения будут продолжать требовать много слюды. Однако использование слюды для остекления, особенно в передних частях печей, сокращается. Это связано с уменьшением производства того типа печей, в которых используется слюда.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

По оценкам, слюда составляет около 4 процентов изверженных пород мира. Сегрегация в месторождения промышленного размера, содержащие слюду коммерческого размера и качества, встречается сравнительно редко. Слюдяные рудники разрабатываются ради небольшого процента листовой или блочной слюды, которую они содержат, а большое количество отходов слюды используется только там, где наличие готового рынка оправдывает помол.

Отдельные месторождения как мусковита, так и флогопита характеризуются крайней нерегулярностью, поэтому любые прогнозы относительно запасов являются неопределенными. Этот факт объясняет грубые методы добычи, которые так долго почти повсеместно применялись. Объем добычи в районе в целом складывается из множества мелких рудников, а не из одного крупного.

Важным соображением в геологическом распространении слюды с экономической точки зрения является степень динамического метаморфизма, которому подвергался регион во время или после формирования слюдоносных месторождений. Это связано с тем, что ценность листовой слюды зависит, среди многих других факторов, от отсутствия деформации листов.

Мусковитовая слюда в коммерческих количествах неизменно встречается в дайках и линзах пегматита, которые считаются представляющими собой сегрегации определенных частей гранитных интрузий. Основными сопутствующими минералами являются кварц и полевой шпат, оба из которых обычно значительно преобладают над слюдой. Дайки или линзы пегматита могут находиться внутри самого гранита или в других вмещающих породах, которые могут казаться не связанными с материнской интрузией. Сланцы или гнейсы образуют вмещающую породу пегматита в большинстве коммерческих месторождений.

Флогопит встречается гораздо реже, чем мусковит, и находится в месторождениях, структурно сходных с гранитными пегматитами. Важными сопутствующими минералами являются пироксен, апатит и кальцит, хотя в некоторых месторождениях масса почти полностью состоит из слюды. Канадские месторождения, которые наиболее известны, состоят из жил и карманов в пироксенитовых дайках, а вмещающей породой обычно является известняк, что является важным фактом в отношении происхождения месторождений.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Индия, Канада и Соединенные Штаты производят около 98 процентов листовой слюды в мире. Продукция Индии и Соединенных Штатов — это исключительно мусковит, тогда как канадское производство почти полностью состоит из флогопита. Бразилия и Аргентина стали важными производителями за последние два года, а Германская Восточная Африка приобретала значительное значение непосредственно перед войной. Южная Африка, Гватемала, Цейлон, Мадагаскар и Австралия производили небольшие количества слюды и могут рассматриваться как потенциальные источники поставок.

Индия производит около 65 процентов листовой слюды в мире и является самым важным источником высококачественного мусковита. Двумя основными производящими регионами являются округ Хазарибаг в провинции Бихар и Орисса в Бенгалии, а также округ Неллор в Мадрасском президентстве.

Продукция Канады практически полностью состоит из флогопита, или янтарной слюды, основным источником которой в мире является эта страна. Важные производящие районы находятся к северу от города Оттава, в провинции Квебек, и в центральной части провинции Онтарио. Рудник Лейси в Онтарио в течение многих лет был крупнейшим производителем янтарной слюды в Канаде.

Соединенные Штаты производят около 15 процентов листового мусковита в мире. В стоимостном выражении около 70 процентов американской продукции поступает из Северной Каролины и 23 процента — из Нью-Гэмпшира. Другие районы незначительны: 3 процента поступает из Вирджинии, 1 процент — из Южной Дакоты и 3 процента — из Джорджии, Алабамы, Айдахо и Колорадо вместе взятых.

Основными источниками слюды в Бразилии являются штаты Баия, Сан-Паулу, Гояс и Минас-Жерайс. Два последних особенно важны. Месторождения широко разбросаны по большой территории.

Добыча слюды в Аргентине до самого недавнего времени была случайной, а развитие — незначительным. Месторождения многочисленны, но особое значение имеют месторождения в провинциях Кордова, Сан-Луис и Сан-Хуан. Насколько известно, мусковит является единственной производимой слюдой.

Значительная активность в добыче слюды наблюдалась в Гватемале, и поставки в эту страну осуществлялись довольно регулярно. Однако слюда низкого качества и не нашла признания на американских рынках.

Добыча в бывшей Германской Восточной Африке ограничивается исключительно мусковитовой слюдой, найденной в районах гор Улугуру и соседних хребтов. Значительные количества высококачественного материала экспортировались в Германию до войны. Слюдяные рудники в Германской Восточной Африке во время войны работали под руководством британского Министерства боеприпасов. Этот район важен как будущий источник высококачественного мусковита.

Основная местность в Южной Африке находится недалеко от Лейдерсдорпа, в Северном Трансваале. Сообщается о наличии в этом районе как мусковита, так и янтарной слюды.

Небольшие количества высококачественной янтарной слюды поставлялись с Цейлона в Англию.

Известно о существовании месторождений слюды отличного качества в хребте Макдональд в Южной Австралии, откуда эпизодически поступали небольшие партии. Это единственный район, где была отмечена лепидолитовая, или литиевая, слюда в листах коммерческого размера.

В Китае сообщается о крупных месторождениях мусковитовой слюды в окрестностях залива Киао-Чау, а также в Шаньдуне, но коммерческого освоения не проводилось, и считается, что месторождения бесполезны как источник листовой слюды.

До 1914 года попытки добывать слюду в Норвегии в коммерческих масштабах не увенчались успехом, и о месторождениях мало что известно. Острая потребность в слюде в Германии во время войны стимулировала производство в Норвегии, за материал платили огромные цены.

ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРОСТРАНЕНИИ В БЛИЖАЙШЕМ БУДУЩЕМ

Наиболее важное изменение в известном географическом распространении слюды в ближайшем будущем касается расширения разработки южноамериканских месторождений. Во время войны бразильская слюда получила значительное признание как в этой стране, так и в Европе, а лучшие сорта считаются равными лучшей индийской слюде. Импорт слюды из Бразилии имел большое значение для удовлетворения огромных потребностей Соединенных Штатов в слюде высокого качества для нужд правительства. Из-за характера месторождений слюды в целом делать оценки относительно запасов небезопасно. Это особенно верно в отношении Бразилии, где отрасль молода, а тщательная разведка и разработка еще не зашли далеко. Судя по большому количеству известных месторождений и быстроте, с которой отрасль отреагировала на военные нужды, несмотря на трудности с транспортировкой от рудников до побережья, представляется, что бразильская слюда будет играть все более важную роль на рынках слюды в мире, особенно в Соединенных Штатах. Однако, какими бы высокими ни были достоинства рудников того или иного района, если слюда не подготовлена тщательно, не классифицирована по размеру и качеству, а поставки не стандартизированы, она не может рассчитывать на постоянное признание среди потребителей в этой стране или в Европе.

Меньше известно о будущих возможностях Аргентины как важной слюдодобывающей страны. Известно много месторождений, и значительные партии поставлялись в Соединенные Штаты и Европу. Полученный здесь материал не был равен индийской или бразильской слюде.

Есть все основания ожидать, что Индия сохранит свою позицию самой важной слюдодобывающей страны. Большое количество месторождений предлагает почти каждый сорт мусковита, требуемый в торговле. Отрасль хорошо развита, а условия труда чрезвычайно благоприятны для производства товара, требующего такого большого количества ручного труда, прежде чем он будет готов к продаже. Однако верно и то, что самые богатые и легкодоступные месторождения были выработаны, и для сохранения прежнего уровня добычи необходимо применять научные методы.

Сомнительно, что в ближайшем будущем произойдет какое-либо важное изменение в положении Соединенных Штатов как производителя слюды. Хотя запасы страны в целом, вероятно, велики, месторождения невелики, а процент высококачественной слюды невелик. Производство значительных объемов слюды среднего качества будет продолжаться. Условия труда не способствуют дешевому производству товара, значительная часть стоимости которого определяется подготовкой и тщательной сортировкой.

Научные методы применялись при добыче и подготовке значительной части канадской продукции. Запасы велики, и Канада, несомненно, сохранит на многие годы свою позицию основного источника янтарной слюды.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Британская империя через государственный суверенитет контролирует 75 процентов текущего мирового производства листовой слюды. В Бразилии и Аргентине, которые имеют важные потенциальные ресурсы слюды, и в Соединенных Штатах политический контроль определяется государственным суверенитетом.

По большей части владение рудниками и концессиями в Индии находилось в руках местных жителей. В округе Хазарибаг английская фирма F. F. Christen & Co. владеет правами на большие участки земли за пределами государственных лесов и ведет добычу в значительных масштабах. К началу войны Германия через коммерческие интересы получила значительную степень контроля над многими индийскими рудниками. S. O. Fillion & Co. из Нью-Йорка — единственная американская фирма, которая, как известно, работает на рудниках в Индии.

Самый важный производящий рудник флогопита в Канаде, в Сиденхэме, Онтарио, принадлежит и управляется General Electric Co. из Скенектади, Нью-Йорк. Та же компания владеет несколькими другими объектами в этом районе и имеет крупный завод по производству слюды в Оттаве, Онтарио. Другие мелкие интересы принадлежат главным образом Канаде.

Davol & Co. из Нью-Йорка — единственная иностранная фирма, которая, как известно, в настоящее время активно разрабатывает слюдяные рудники в Бразилии.

Слюдяные рудники в Соединенных Штатах, насколько известно, все принадлежат американцам.

ПОЛОЖЕНИЕ ВЕДУЩИХ СТРАН

Соединенные Штаты до войны были крупнейшим в мире потребителем слюды всех видов. Развитие ее электротехнической промышленности зависит от поставок слюды, большая часть которой импортируется из Индии и Канады. Производство в этой стране было значительным, но оказалось далеко не достаточным для удовлетворения спроса, особенно спроса на более высокие сорта слюды для использования в магнето, радиоконденсаторах и свечах зажигания, а также на слюдяные пластины, используемые при изготовлении «щипаной слюды».

Большой спрос и высокие цены, созданные войной, не увеличили внутреннее производство настолько, чтобы оправдать веру в то, что эта страна может стать независимой в отношении листовой слюды при любых условиях, кроме самых искусственных. Производитель защищен 25-процентной импортной пошлиной на необработанную (грубую или обрезанную ножом) слюду и 30-процентной пошлиной на резаную слюду, пластины и другие обработанные формы. Производство в этой стране в значительной степени находится в руках отдельных лиц и небольших компаний, которые финансово не способны увеличивать выпуск продукции скачкообразно даже при очень благоприятных условиях. Более того, многие потребители имеют твердую предубежденность в пользу импортной слюды.

Если Соединенные Штаты хотят занять доминирующее положение в электротехнической промышленности мира, необходимо обеспечить адекватные поставки слюды. Самым многообещающим полем для развития таких поставок, несомненно, является Южная Америка. Это особенно верно, поскольку значительное развитие электротехнической промышленности в Англии во время войны ставит эту страну в доминирующее положение, которое ранее занимали Германия и Австрия. Это развитие потребует значительной части индийской слюды, ранее доступной для экспортной торговли.

Британская империя обладает в Индии самым важным источником мусковитовой слюды в мире, а в Канаде — единственным важным источником янтарной слюды. Несмотря на огромное преимущество Англии в отношении сырья, Германия благодаря своему важному положению в электротехнической промышленности и значительной степени контроля, приобретенного над индийскими рудниками, угрожала доминировать на мировом рынке слюды к началу войны. С начала войны Англия закрепила свое положение не только как контролирующий центр для сырой слюды, но и как главная производящая нация электрооборудования. Лондон является мировым распределительным центром индийской слюды, и лондонские цены регулируют рынок. Во время войны индийская слюда контролировалась британским Министерством боеприпасов, а распределение между ассоциированными странами осуществлялось по фиксированным ценам.

В развитии южноамериканских месторождений заключается лучшая возможность для мира уменьшить свою зависимость от Англии в отношении этого важнейшего сырья.

Франция полностью зависит от внешних источников поставок слюды. До войны ее потребности не были большими и удовлетворялись индийской слюдой.

Хотя Германия до войны полностью зависела от внешних источников слюды, ее ведущее положение в электротехнической промышленности позволило ей получить контроль над значительной частью индийской продукции. Каждой возможностью пользовались в полной мере, и в 1914 году, по словам британского министра боеприпасов, мировой рынок слюды был на грани перемещения из Лондона в Гамбург. Месторождения Германской Восточной Африки активно эксплуатировались, а немецкие коммерческие интересы распространялись на Южную Америку.

Хотя в 1914 году Германия, вероятно, обладала очень большими запасами, во время войны она очень остро ощущала нехватку слюды. Норвегии платили высокие цены за продукцию этой страны, но этот источник, вероятно, совершенно неспособен удовлетворить нормальные потребности Германии.

РЕЗЮМЕ

Листовая слюда необходима для производства огромного разнообразия электрооборудования и поэтому должна быть классифицирована как одно из важных видов сырья в мире. Магнето, такой жизненно важный фактор в современном транспорте на суше, в воздухе и на море, зависит от слюды в своей конструкции, а слюдяные конденсаторы незаменимы в современном радиооборудовании.

Индия, Канада и Соединенные Штаты в настоящее время являются самыми важными слюдодобывающими странами. Месторождения будущего значения, из которых добыча до сих пор не была значительной, известны в Германской Восточной Африке, Бразилии, Аргентине и Трансваале; из нескольких других частей мира сообщается о более спорадической добыче.

В отличие от развития многих других видов сырья, производство слюды не было повсеместно предпринято в больших масштабах, и научные методы не применялись к ее добыче. Это было в значительной степени связано с нерегулярным характером месторождений и их разбросанным положением внутри района, что делает значительные капиталовложения в добычу особенно рискованным предприятием. Поэтому торговые интересы играли важную роль в контроле производства и рынков.

Британская империя, имея в своих границах большую часть важных слюдодобывающих районов, в настоящее время доминирует в ситуации политически. Британский коммерческий контроль, которому угрожало ведущее положение Германии в электротехнической промышленности и широкие интересы в индийских рудниках к началу войны, теперь прочно восстановлен, и Великобритания заняла место в электротехнической промышленности, которое ранее занимали Германия и Австрия.

Соединенные Штаты, крупнейший потребитель слюды среди стран мира, полагались на импорт для обеспечения значительной части потребления и, вероятно, будут продолжать делать это в будущем, хотя можно ожидать устойчивого развития внутренних источников поставок. Бразилия предлагает наиболее многообещающее иностранное поле для развития независимого источника поставок для американских рынков.

ГЛАВА XXIV АСБЕСТ Автор: Оливер Боулз

ПРИМЕНЕНИЕ АСБЕСТА

Асбест полезен благодаря своей негорючести, изоляционным качествам и волокнистой структуре. Высококачественный асбест прядут или ткут в веревки и ткани, ткани используются для многих целей, таких как защитные занавесы, маты, матрасы, обивка, костюмы и перчатки пожарных. В последние годы много высококачественного асбеста использовалось для фрикционных накладок в тормозах и для уплотнений. Низкосортный асбест используется для множества целей, которые можно разделить на три группы: строительные, изоляционные и прочие.

В строительных целях асбест применяется во многих отношениях. Смесь асбеста и цемента используется для изготовления огнеупорной черепицы или шифера. Асбест также используется с портландцементом для создания защитной поверхности на металлической обшивке; асбестовая бумага используется для защиты от атмосферных воздействий и звукоизоляции, а также для целей противопожарной защиты. Он широко используется для штукатурки, которая не только огнеупорна, но и улучшает акустические свойства аудиторий, церквей и т. д. Асбест также используется для напольной плитки и в производстве красок. Асбестовый лесоматериал и плиты используются для многих конструктивных целей.

Асбестоцемент, смесь асбестового волокна и глины, широко используется в качестве покрытия для котлов и паровых труб для предотвращения теплового излучения. Другие покрытия изготавливаются из смеси асбеста и магнезии. Разновидности асбеста с низким содержанием железа полезны для целей электрической изоляции.

Некоторые из многих прочих применений асбеста — это огнеупорный кирпич, кислотные фильтры, коллекторы свинцовых паров, маты для печей, футеровка кухонной утвари и т. д.

Наиболее важными из вышеперечисленных применений являются те, в которых используется длинноволокнистый асбест. Для огнеупорных веревок и тканей ничто не может его заменить. Его использование во фрикционных накладках для тормозов является важным во всех автотранспортных средствах.

Области применения низкосортного асбеста можно рассматривать как менее важные, и их можно было бы исключить в случае необходимости, хотя такое исключение, несомненно, повлекло бы за собой много серьезных трудностей. Пожарный риск при этом увеличился бы, а многие котлы и отопительные установки стали бы менее эффективными и более расточительными, хотя эти трудности можно было бы в некоторой степени преодолеть с помощью использования заменителей.

Заменители.

— Шлаковата или минеральная вата — это огнеупорный материал и хороший непроводник тепла и звука. Она также обладает высокой пористостью, а следовательно, полезна как абсорбент. Поэтому ее можно в некоторой степени использовать в качестве заменителя асбеста для теплоизоляции и огнезащиты. Однако, поскольку она хрупкая и ее нельзя ткать так же легко, как асбест, ее нельзя считать удовлетворительным заменителем для более высоких сортов. Тальк может применяться в производстве огнеупорных и коррозионностойких красок, а также в качестве футеровки для печей и каминов. Инфузорная земля в некоторой степени используется как заменитель асбеста для изоляции и огнезащиты. Но важно отметить, что ни один из вышеупомянутых заменителей не может заменить высококачественное прядильное волокно.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Как было указано, существует вероятность увеличения спроса на асбест. Широкое использование автотранспортного оборудования требует большого количества высококачественного волокна для тормозных накладок, в то время как растущее использование парового оборудования, а также электрического оборудования и приборов требует все больше материала как для электрических, так и для теплоизоляционных целей. Хотя для более низких сортов могут использоваться заменители, для прядильных сортов асбеста, на которые сейчас самый сильный спрос, заменители неизвестны. Следовательно, нет никаких изменений в практике, которые уменьшили бы спрос на асбест.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Асбест происходит по большей части из пород, состоящих в основном из оливина, таких как перидотиты или дуниты, или из пород, состоящих в основном из пироксена. Следовательно, только в измененных породах такого рода следует ожидать асбест обычных типов. Распространены два различных типа изменения: изменение оливина или пироксена в серпентин с развитием хризотила в некоторых местах; и изменение оливина или пироксена в амфибол с развитием антофиллита (разновидность амфибола) и родственных форм. Оба типа изменения хорошо представлены в великом североамериканском поясе асбестоносных перидотитов, который простирается от центральной Алабамы вдоль плато Пидмонт до полуострова Гаспе в Квебеке, на расстояние более 1600 миль. В северной части пояса, в Вермонте и Квебеке, изменение происходило в серпентин с хризотиловым асбестом в некоторых местах, в то время как в южной части изменение происходило главным образом в амфиболит с развитием антофиллитового асбеста и талька.

Хризотиловый асбест (квебекский тип), как он представлен в большинстве месторождений, образуется путем серпентинизации с последующей призматической кристаллизацией в трещинах, при этом образовавшиеся таким образом жилы представляют собой перекристаллизацию вдоль стенок и, следовательно, являются жилами замещения, а не жилами выполнения трещин. Контактовый метаморфизм, очевидно, играет важную роль в этом процессе, поскольку в большинстве регионов с месторождениями связаны интрузивные дайки, которые, очевидно, оказали определенное влияние на развитие коммерческого продукта. Поскольку серпентинизация является глубоким процессом, хризотиловые месторождения могут встречаться на значительной глубине.

Антофиллитовый асбест (грузинский тип) является результатом изменения перидотитов или пироксенитов в амфибол, давая волокнистый антофиллит и родственные формы. Этот тип асбеста не встречается в жилах, а составляет большую часть массы породы.

Хотя отмеченные выше способы изменения объясняют большинство известных месторождений асбеста, существуют два важных исключения — крокидолит, или синий асбест, из Южной Африки и хризотиловые месторождения Аризоны, оба из которых встречаются в осадочных породах. Крокидолит залегает в яшме и железняке, а аризонский хризотил является результатом изменения кремнистого известняка под влиянием в некоторой степени действия диабазовых интрузий.

Как было указано в обсуждении применений, для различных избранных целей антофиллит не может быть использован в качестве заменителя хризотила прядильного сорта. Поскольку области применения антофиллита таким образом ограничены, а запасы, по-видимому, достаточны на многие годы вперед, проблема поставок сосредоточена вокруг месторождений высококачественного хризотила.

Месторождения серпентинизированных основных пород отнюдь не редки, и даже развитие волокнистой структуры является обычным явлением, но во всех хризотилсодержащих месторождениях лишь небольшая часть серпентина является волокнистой, и из волокнистой части лишь небольшой процент может быть использован в качестве высококачественного асбеста. Ценность месторождений большинства руд зависит в значительной степени от процента металла и присутствующих примесей, и мало внимания нужно уделять физическому характеру руды. Ценность асбеста, однако, зависит не только от чистоты состава, но и от очень определенных физических свойств, таких как длина волокна, гибкость и прочность на разрыв. Такие свойства являются результатом сочетания благоприятных условий кристаллизации, условий, которые в настоящее время мало изучены.

Большое тело серпентинизированной основной породы, следовательно, не дает никакой уверенной гарантии поставок асбеста, хотя может предложить стимул для разведки. Высококачественное волокно, очевидно, образуется при специфическом сочетании геологических условий, которые включают присутствие определенных типов первичных пород, их изменение во вторичные минералы и перекристаллизацию последних в жилах, причем такая перекристаллизация вызывается сочетанием метаморфических агентов. Хотя, следовательно, вполне вероятно, что будут открыты новые месторождения, нет никакой вероятности обильных поставок.

Важным моментом, который следует учитывать в связи с будущими поставками, является то, что для большинства применений асбеста практически нет восстановления скрапа; то, что однажды использовано, по большей части ушло безвозвратно. Поэтому мудро придерживаться консервативного взгляда на запасы асбеста, ибо, хотя есть свидетельства запасов в канадских месторождениях и в других местах, которых хватит на многие годы, вероятность того, что месторождения высококачественного материала ни многочисленны, ни обширны.

Общий объем добычи и оценочные запасы прядильного асбеста в важных производящих странах показаны на рисунке 13.

Рис. 13. — Общий объем добычи и оценочные запасы прядильного асбеста.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Соединенные Штаты.

— Асбест в Соединенных Штатах бывает двух типов: хризотил и антофиллит. Хризотиловая разновидность встречается в Аризоне, Вермонте, Вайоминге и Калифорнии, а антофиллит — в Джорджии, Вирджинии, Мэриленде, Массачусетсе, Коннектикуте, Род-Айленде и Айдахо.

Хризотиловый асбест.

— Асбестовые месторождения Аризоны необычны тем, что представляют собой поперечно-волокнистые хризотиловые жилы в кремнистом известняке и, таким образом, совершенно отличаются по происхождению от квебекских месторождений. Асбестоносные пласты тонкие, и некоторые из них почти недоступны.

Асбест был впервые обнаружен в Аризоне в двух точках в Гранд-Каньоне Колорадо, к западу от устья реки Литл-Колорадо. Минерал встречается в одном пласте толщиной от 12 до 14 дюймов, жилы параллельны напластованию. В некоторых местах жилы имеют толщину 4 дюйма, но обычно они не превышают 2,5 дюйма. Видимые запасы, следовательно, невелики, и, поскольку район труднодоступен, добыча была незначительной. Асбест также встречается в каньоне Эш-Крик недалеко от Глоуба. Добыча началась в 1914 году и с тех пор значительно увеличилась. Асбест содержит только 0,5 процента оксида железа, в то время как канадский асбест содержит от 2,2 до 2,6 процента оксида железа. Аризонский материал, следовательно, превосходит канадский асбест для электрической изоляции. По оценкам, при благоприятных условиях регион может поставлять 1000 тонн ежегодно на многие годы вперед, но объем добычи никогда не будет большим по сравнению с Канадой. В 1914 году месторождение асбеста, подобное месторождениям Эш-Крик, было зарегистрировано недалеко от почтового отделения Янг. Оно находится в 80 милях от ближайшей железнодорожной станции и, вероятно, будет недоступным в течение многих лет. Рядом с вершиной горы Бейкер, к северу от водохранилища Рузвельт, в 1917 году был открыт рудник, производящий хороший хризотил. Асбест встречается в поперечно-волокнистых жилах в известняке.

Асбестовые месторождения Вермонта расположены в Лоуэлле, в той же формации, что и квебекские месторождения. Асбест встречается в многочисленных нерегулярных жилах, запасы, вероятно, велики, и некоторые из них сравнимы с канадским продуктом. В прошлые годы добыча была значительной, но после 1912 года карьеры простаивали. Запасы низкосортной породы, вероятно, велики.

Основные месторождения Вайоминга находятся к югу от Каспера в изверженных архейских породах. Минерал представляет собой хризотиловый асбест, в основном поперечно-волокнистого типа, хотя присутствует и некоторое количество продольно-волокнистого (slip-fiber). Утверждается, что вайомингский асбест обладает лучшими жаростойкими качествами, чем канадское волокно. Однако очень небольшая часть волокна относится к прядильному сорту.

Месторождения хризотилового асбеста были отмечены во многих частях Калифорнии, разбросанных по 13 округам. Месторождения кажутся небольшими, и до сих пор добыча не превышала нескольких тонн в год. Небольшая добыча зарегистрирована за 1917 год в округах Невада и Иньо. В 1918 году объем производства увеличился, составив в общей сложности 229 тонн. Некоторое количество прядильного волокна № 1 было получено в округе Невада.

Антофиллитовый асбест.

Месторождения антофиллитового асбеста в штате Джорджия обеспечивают самый высокий уровень добычи среди всех штатов Союза. Этот материал не относится к прядильным сортам и практически полностью используется для огнезащиты и изоляции. Тем не менее, на такой материал существует значительный спрос, и отрасль имеет прочную основу. Примечательной особенностью месторождений Джорджии является то, что около 95 процентов добываемой породы составляет волокнистый антофиллит товарного качества, тогда как в Квебеке можно использовать лишь около 6¹⁄₂ процентов добываемого материала.

Месторождения антофиллитового асбеста встречаются в штате Виргиния, недалеко от Бедфорда. Материал низкосортный, и его количество, вероятно, невелико. Небольшое его количество расходуется при производстве «тенакса» — препарата, используемого стоматологами. Амфиболовый асбест с тонкими волокнами в последнее время добывается в небольших масштабах в штате Мэриленд, недалеко от Пайлсвилла. Он используется для фильтров. Несколько лет назад была зафиксирована небольшая добыча в Далтоне, штат Массачусетс, и Нью-Хартфорде, штат Коннектикут.

Антофиллитовый асбест встречается в штате Айдахо, недалеко от Камии. Он не относится к прядильным сортам, обладает низкой прочностью на разрыв и уступает всем сортам хризотила, за исключением самых низких. Месторождение, очевидно, крупное, но добыча практически ничтожна.

Канада и Ньюфаундленд.

Наиболее важными в мире месторождениями асбеста являются месторождения в провинции Квебек, Канада, главным образом в районе Тетфорда и Бротона. Асбест встречается в серпентинах кембрийского периода; область, в которой расположены важные рудники, простирается от южного Вермонта до Гаспе в провинции Квебек. Серпентин залегает в виде трех заметных поясов. Серпентиновый пояс Данвилл-Истмен-Вермонт имеет протяженность около 62 миль. Разрозненные выходы, вероятно, связаны между собой под мощными наносами и лесными массивами. Перспективные участки разрабатывались в шести местах, но достигнутый объем добычи невелик. Этот пояс представляет собой неопределенную величину, которая дает неплохие перспективы для крупных поставок в будущем.

Район Тетфорд-Блэк-Лейк является важной областью Квебека и в настоящее время самым продуктивным асбестовым районом в мире. В 1917 году в этом районе действовало 17 рудников. В 1918 году количество добытой породы составило 2 445 745 тонн, а общий объем добычи асбеста — 159 225 тонн стоимостью 9 053 945 долларов. Месторождения Бротона, а также центрального и восточного Тетфорда в основном представлены асбестом с тонкими волокнами. Месторождения в Западном Тетфорде, Южном Ирланде и северном Тауншипе Корейн образуют пояс жильного волокна, который дает высококачественный прядильный асбест, пользующийся мировой репутацией.

Сообщается о наличии серпентиновых пород, содержащих хризотил-асбест, недалеко от Порт-о-Пор на Ньюфаундленде, что, вероятно, представляет собой продолжение Квебекского пояса. Возможность промышленной разработки остается неопределенной.

Мексика, Центральная и Южная Америка.

Сообщалось о месторождениях асбеста в Бразилии, но, помимо этого, в Южной Америке не было отмечено месторождений промышленного значения.

Сведений о месторождениях асбеста в Мексике или Центральной Америке нет.

Европа.

Месторождения асбеста в России, вероятно, занимают второе место после канадских. Основные рудники находятся в 57 милях к северу от Екатеринбурга, на Урале. Карьеры могут разрабатываться только с мая по ноябрь каждого года. Транспортировка осуществляется по Пермской железной дороге, а продукция экспортируется через Ригу. Волокно того же типа, что и канадское, — хризотил-асбест, преимущественно поперечно-волокнистого типа. Самая богатая руда дает от 42 до 55 фунтов асбеста на кубический ярд. О добыче также сообщала компания «Южно-Уральское асбестовое общество», работающая в Орском районе Оренбургской губернии. Говорят, что российский асбест более жесткий, чем канадский, и менее пригоден для прядения, однако было произведено большое количество высококачественного волокна, и Россия, вероятно, станет важным источником асбеста в будущем.

Асбест в Италии относится к антофиллитовой разновидности. Существует три основных района: месторождения в долине Суза, недалеко от французской границы, которые находятся на высоте от 6000 до 10 000 футов над уровнем моря и поэтому труднодоступны; месторождения в долине Аоста, обширные по площади, с длинноволокнистым, прочным и мылким продуктом; и месторождения в Ломбардии, также весьма обширные. Итальянский асбест может в некоторой степени использоваться в качестве заменителя канадского волокна или для смешивания с ним, но запасы высококачественного волокна невелики, а его добыча сложнее и дороже, чем канадского материала. Крупнейшим производителем является компания United Asbestos Co. из Лондона, Англия.

На острове Кипр известны крупные месторождения асбеста. Материал происходит из серпентина и относится к амфибол-антофиллитовому типу. Большая его часть — коротковолокнистая, но некоторая часть может использоваться для смешивания с канадским волокном.

Хороший прядильный асбест был обнаружен в центральной Финляндии, но добыча до настоящего времени практически ничтожна.

Месторождения асбеста были отмечены в Англии, Шотландии, Ирландии, Франции, Португалии, Испании, Швейцарии, Германии, Норвегии, Греции и Турции, но все вышеперечисленные месторождения, как говорят, состоят из грубого и хрупкого материала, имеющего небольшую коммерческую ценность. Сообщается о крупном месторождении хорошего асбеста на острове Корсика.

Азия.

Месторождения известны в различных районах Индии. Асбест также обнаружен в Афганистане. Индийский асбест обладает низкой прочностью на разрыв, а отсутствие разработок делает его неопределенным ресурсом.

Геологическая служба США в 1912 году сообщила, что три асбестовых рудника работали в 45 милях к северо-востоку от Аньдуна, Китай. Продукт, который отправлялся в Маньчжурию, относится к амфиболовому (антофиллитовому) типу и довольно хрупок. О хризотил-асбесте хорошего качества сообщается к югу от озера Байкал, в Монголии. Он никогда не добывался, и из-за своей удаленности вряд ли будет разрабатываться. Месторождения, дающие небольшую добычу, отмечены в нескольких других провинциях.

Месторождения асбеста встречаются в нескольких местностях Японии. Продукция низкого качества и смешивается с импортным материалом для асбестовой набивки. Компания Japan Asbestos Co. из Осаки является главным производителем асбестовых изделий.

Месторождения были открыты в Минусинске, на реке Енисей, в Сибири, но добыча зафиксирована только за 1905 год. Транспортировка затруднена.

Африка.

Асбест Капской колонии — это крокидолит, или синий асбест; он относится к амфиболовому типу и не выдерживает высоких температур, вероятно, из-за содержания железа, но он длиннее, прочнее, тоньше и эластичнее хризотила. Благодаря своей низкой температуре плавления он полезен при электросварке. Минерал встречается в трех важных районах и выходит на поверхность во многих точках от реки Оранжевой на севере до Бечуаналенда. Правительственные инженеры сообщают, что это самая большая асбестоносная область в мире. Основные месторождения находятся в Кугасе, где компания Cape Asbestos Co., Ltd. в 1916 году произвела около двух третей от общего количества асбеста, добытого в Южной Африке. Синий асбест завоевывает популярность на внешних рынках, и этот факт, в сочетании с большой протяженностью месторождений, указывает на то, что они являются важным фактором мировых поставок.

Крупные и, вероятно, обширные месторождения хризотил-асбеста высочайшего качества встречаются в Трансваале. В этом районе недавно работали три компании. Добыча, которая началась около 1914 года (в этом году было зарегистрировано 30 тонн), увеличилась до 407 тонн в 1916 году.

Новым и важным направлением является добыча длинноволокнистого амфиболового асбеста, известного как «амозит».

В течение нескольких лет сообщалось о небольшой добыче асбеста в Натале; однако волокно невысокого качества, и увеличение добычи маловероятно.

Важные месторождения встречаются в Южной Родезии. Геологическая служба Южной Родезии сообщает, что имеются разведанные запасы на несколько лет при добыче 200 тонн в месяц без углубления более чем на 60 футов. Запасы «вероятной руды» очень велики. Было заявлено, что родезийское волокно — это единственный класс хризотил-асбеста, который может успешно конкурировать с лучшим сортом канадского волокна.

Австралазия.

Хризотилсодержащий серпентиновый пояс занимает значительную площадь в Квинсленде. Месторождение находится недалеко от Рокуэлла, Южная Австралия. Компания Australia Asbestos Manufacturing Co. произвела небольшое количество материала, похожего на итальянский асбест. Также было найдено небольшое количество хризотила. Утверждается, что месторождение хризотила, разведанное в Новом Южном Уэльсе, имеет самое длинное асбестовое волокно в мире. О добыче не сообщалось. В районе Пилбара, Западная Австралия, имеется хризотил-асбест прядильного сорта, который, как говорят, превосходит как российский, так и итальянский продукт. Несколько лет назад рудник разрабатывался на значительную глубину компанией Pilbarra Asbestos Co. из Лондона, Англия, но в последние годы добыча была почти ничтожной. В Новой Зеландии хризотил-асбест прядильного сорта встречается в провинции Нельсон. Компания Australasian Asbestos Co. из Сиднея недавно провела разведку серпентинового пояса Тасмании, который содержит как хризотиловый, так и антофиллитовый асбест.

РАЗВИТИЕ И ИЗМЕНЕНИЯ В РАСПРЕДЕЛЕНИИ РУДНИКОВ

Соединенные Штаты лидируют среди всех стран в производстве асбестовых изделий, а крупные запасы асбеста в Квебеке легкодоступны. Поэтому мало шансов на какие-либо радикальные изменения в географическом распределении американских асбестовых рудников. Однако, поскольку всегда существует вероятность таких изменений, полезно рассмотреть контролирующие факторы.

Что касается будущего месторождений Квебека, нынешнего источника поставок, то имеется мало определенной информации. Тот факт, что серпентинизация является глубоким процессом, привел канадских геологов к выводу, что товарное волокно может образовываться на всю глубину исходной перидотитовой породы. Однако для всех практических целей глубина месторождения ограничена глубиной, на которой асбест можно добывать с прибылью. Один рудник сейчас работает на глубине 300 футов, а буровые скважины, пробуренные еще на 400 футов, указывают на мощность не менее 700 футов хорошей волокноносной породы. Циркель заявил, что в одном из карьеров Блэк-Лейк имеется 44 377 500 тонн асбестовой породы, видимой над железнодорожными путями, готовой к немедленной эксплуатации. Вычет 50 процентов на пустую породу оставит 22 000 000 тонн фабричной руды, или достаточно, чтобы обеспечить в течение 22 лет завод, способный производить 4000 тонн в день. Поскольку это включает только видимую руду, можно сделать вывод, что резерв очень велик. Циркель оценивает общую площадь продуктивного жильного волокна в 12 420 акров, из которых 1100 акров в настоящее время находятся в разработке. Геолог, который провел два лета, изучая геологию региона, утверждает, что волокно второго сорта очень распространено, а высококачественные месторождения истощены не более чем на 25 процентов. Таким образом, в течение многих лет не предвидится никаких изменений в географическом распределении действующих рудников из-за истощения нынешних месторождений.

В течение 1916 и 1917 годов добыча высококачественного волокна в Соединенных Штатах неуклонно росла, но все еще далека от удовлетворения внутреннего спроса, так как общий объем добычи в США в 1917 году составлял лишь одну восьмидесятую от объема импорта. Наиболее важное развитие произошло в районах высококачественного хризотила в Аризоне, но эти новые месторождения не дают надежды на обильные поставки, и маловероятно, что они станут доминирующим фактором в американском производстве.

Законодательство может оказать глубокое влияние на разработку месторождений. Высокая экспортная пошлина на сырой асбест, установленная страной, которая в настоящее время производит его в больших количествах, привела бы к поощрению разведки в других странах и разработке месторождений, которые могли бы поставлять заменители. В этой связи интересно отметить, что Торговая палата восточных тауншипов Квебека предложила меры по защите экспорта сырого асбеста, чтобы принудить к производству асбестовых изделий в Канаде. Бюллетень Канадского института горного дела (август 1916 г.) указал на опасности таких действий, поскольку другие страны немедленно начали бы искать месторождения асбеста в других местах, и, поскольку хороший асбест встречается в России, Южной Африке, на Кипре и в других местах, заменители канадского материала, вероятно, могли бы быть найдены. Таким образом, очевидно, что Канада не контролирует поставки, но до тех пор, пока канадское волокно доступно по разумным ценам, нет сильного стимула для разработки новых месторождений.

В Старом Свете ситуация менее стабильна, чем в Америке. Европейские страны импортируют значительное количество материала из Канады, а остаток их потребностей покрывается из различных источников, главным образом из России, Кипра, Италии, Южной Африки и Австралии. Высококачественные месторождения асбеста существуют в различных странах и по большей части разрабатываются в незначительной степени. Факторы, определяющие изменения в производстве, несколько отличаются от тех, что были описаны для Америки. Отсутствие сильного центрального правительства сильно затрудняет производство в любой стране. Так, в условиях недавней ситуации в России объем добычи упал с почти 20 000 тонн в 1913 году до около 9 000 в 1916 году. Стабилизация условий и более эффективные правительства способствовали бы увеличению добычи в ряде восточных стран. Самым важным фактором, способствующим медленному развитию месторождений Старого Света, является плохая транспортная инфраструктура. Российский асбест для английского рынка должен оплачивать транспортные расходы в размере 25–30 долларов за тонну. Важные месторождения крокидолита в Южной Африке также страдают от плохой транспортировки. Мало того, что дороги плохие, самые важные месторождения в Кугасе находятся в 18 милях от проезжей дороги, а другие месторождения — примерно в 100 милях от дорог. Этот недостаток в некоторой степени компенсируется дешевой рабочей силой.

Нынешние политические потрясения в Европе, связанные с формированием новых государств и новых форм правления, могут оказать значительное влияние на разработку месторождений асбеста, но до тех пор, пока не будут созданы прогрессивные правительства и не будут проведены значительные улучшения в транспортной сфере, значительное увеличение производства невозможно.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Значительная часть месторождений асбеста в мире, будучи расположенной в британских колониальных владениях, находится под политическим контролем Великобритании. Месторождения Кипра в настоящее время находятся под британским политическим контролем, но это может быть не навсегда. До войны Кипр номинально был турецким, хотя управлялся Великобританией; в 1914 году Великобритания официально аннексировала остров. Кипр был предложен Греции в обмен на ее помощь в войне, но предложение не было принято.

Из имеющейся информации очевидно, что правительства России и Италии в прошлом не накладывали серьезных ограничений на развитие своих асбестовых объектов ни за счет внутреннего, ни за счет иностранного капитала.

Ниже изложен коммерческий контроль над месторождениями асбеста в мире по странам в следующем порядке: Соединенные Штаты, Канада, Россия, Южная Африка, Италия, Кипр и Австралия.

В районе Глоуб в Аризоне, США, прядильный асбест производится компанией Johns-Manville Co., разрабатывающей собственность Snell & Fisk, и компанией American Ores & Asbestos Co. Компания Sierra Asbestos Co., недалеко от Невада-Сити, Калифорния, произвела прядильное волокно в 1918 году. Насколько известно, все компании, работающие в Соединенных Штатах, принадлежат американцам.

Асбестодобывающая промышленность в Канаде ограничена восточными тауншипами провинции Квебек. Крупнейшей компанией является Asbestos Corporation of Canada, Ltd. с головным офисом в Монреале. Эта компания управляет рудниками Kings и Beaver в Тетфорд-Майнс, рудником British Canadian в Блэк-Лейк и рудником Frazer в Ист-Бротоне. Компания контролируется английским, канадским и американским капиталом. Компании Bell Asbestos Mines Co., Asbestos & Asbestic Corporation и Manville Asbestos Co. полностью или в значительной степени принадлежат США. Остальные компании в основном контролируются английским или канадским капиталом, хотя интересы США представлены в некоторых из них. Очевидно, таким образом, что собственность компаний разделена между английским, канадским и американским капиталом, причем британские интересы, вероятно, преобладают.

Самыми важными из екатеринбургских рудников в России являются Вознесенский и Зое-Анонский, недалеко от Баженова. Около одной трети от общего объема добычи на Урале приходилось на эти рудники в 1916 году. Сообщается, что до войны немецкий синдикат контролировал несколько российских рудников, которые в общей сложности производили более 80 процентов всей российской добычи. Германия и Австрия были главными покупателями российского асбеста до войны.

В Южной Африке крокидолит Капской колонии добывается в основном компанией Cape Asbestos Co., британской фирмой с рудниками в Кугасе и Вестерберге, имеющей фабрики в Англии, Турине и Гамбурге. Сестринская компания во Франции, Compagnie Française de l’Amiante du Cap, в 1916 году обрабатывала около двух третей от общего объема добычи в Южной Африке и была главным производителем изделий из синего асбеста. В Трансваале асбест добывается тремя компаниями: The Transvaal Asbestos Syndicate, ныне поглощенной Consolidated Gold Fields; South African Minerals Option Syndicate, дочерней компанией Bechuanaland Exploration Co., и Anglo-Swiss Asbestos Co. Преобладает британский капитал. Rhodesia Asbestos Co., Ltd. была главным родезийским производителем до недавнего времени, но в 1917 году была организована Rhodesia and General Asbestos Corporation с капиталом 400 000 фунтов стерлингов для принятия в управление действующих рудников. Таким образом, коммерческий контроль является британским.

Главным производителем в Италии является компания United Asbestos Co. из Лондона, Англия.

До войны месторождения Кипра разрабатывались австрийской корпорацией Cyprian Mining Co. Поскольку концессии на добычу полезных ископаемых получаются от британского правительства в аренду на основе роялти, вполне вероятно, что договор аренды к настоящему времени аннулирован.

Месторождения в Австралазии практически полностью контролируются английским или австралийским капиталом.

Рудники, не имеющие обогатительного оборудования, могут производить сырое волокно, которое может быть обработано на производственных предприятиях. Различные сорта фабричного волокна могут быть произведены только там, где фабрики расположены на рудниках или рядом с ними. Поскольку использование всех сортов может быть осуществлено только с помощью фабрик, такие фабрики необходимы для эффективной добычи. Следовательно, при прочих равных условиях рудники с близлежащими фабриками имеют явное коммерческое преимущество перед рудниками, производящими только сырое волокно. Хотя фабрики не являются существенными факторами в асбестодобывающей промышленности, они оказывают вторичное влияние на коммерческий контроль за счет повышения эффективности добычи, которую они делают возможной. Для месторождений, удаленных от центров производства, фабрики малоэффективны, так как волокно ниже прядильного сорта не выдержит высоких транспортных расходов. Большинство рудников США и Канады имеют фабрики для обработки породы, содержащей короткое волокно. Несколько российских рудников оснащены аналогичным образом, но в других частях мира обогащение практически не проводится.

Ряд крупных производителей асбестовых изделий в Соединенных Штатах являются владельцами или имеют тесные торговые соглашения с крупными канадскими асбестовыми рудниками, а также с некоторыми внутренними рудниками. Следовательно, в отношении коммерческого контроля Соединенные Штаты практически обеспечены поставками сырья.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ ДЕРЖАВ

Хотя Соединенные Штаты являются крупнейшим производителем асбестовых изделий в мире, в 1917 году менее 1 процента сырья было добыто в этой стране. Таким образом, страна в значительной степени зависит от иностранных источников поставок. Обильные месторождения Квебека, Канада, удобно расположены рядом, и до тех пор, пока сохраняются нынешние дружественные отношения с Канадой, достаточные поставки кажутся обеспеченными. В 1916 году Соединенные Штаты использовали 86 процентов канадской добычи. В течение 1916 и 1917 годов наблюдалась заметная активность в разработке месторождений высококачественного хризотила в Аризоне. Хотя пока нет доказательств обильных поставок, материал является важным дополнительным источником поставок из-за своего качества.

Хотя на Британских островах не добывается коммерческий асбест, британские колониальные владения контролируют около 88 процентов ежегодной мировой добычи асбеста и приблизительно 70 процентов мировых запасов. Таким образом, хотя поставки внутри Британской империи достаточны, внутренние потребности страны могут быть удовлетворены только при благоприятных условиях судоходства, так как весь необходимый материал должен транспортироваться на несколько тысяч миль.

Россия является вторым по величине производителем асбеста в мире и, по-видимому, обладает большими запасами. Поскольку в стране мало что производится, практически вся продукция экспортируется. Будучи независимой в отношении собственных потребностей в сыром асбесте, Россия требует только поддержания активного внешнего рынка для обеспечения постоянной отрасли.

Неизвестно о существовании месторождений коммерческого асбеста в Германии. До войны асбест импортировался главным образом из России и Канады. Говорят, что главные российские рудники контролировались немецким капиталом.

Италия имеет крупные месторождения амфиболового (антофиллитового) асбеста, некоторые из которых относятся к прядильному сорту, но поскольку добыча всегда была небольшой и, за исключением незначительных колебаний, оставалась неизменной в течение последних 18 лет, маловероятно, что месторождения могут обеспечить внутренние потребности в высококачественном волокне. Небольшое количество экспортировалось для использования в фильтрах, для чего итальянский асбест хорошо подходит. Поскольку главный рудник управляется британской компанией, значительное количество итальянского асбеста отправляется в Англию.

Во Франции месторождения асбеста не разрабатываются. Поставки осуществляются из России, Канады и Южной Африки. Франция является ведущей страной в производстве изделий из синего асбеста.

В Японии встречается несколько месторождений асбеста, но все они низкого качества. Добываемый материал смешивается с импортным волокном для производства асбестовой набивки.

РЕЗЮМЕ

Асбест — уникальный минерал по той причине, что он сочетает в себе негорючесть и изоляционные качества с волокнистой структурой, что делает возможным его переработку в ткани, войлок и аналогичные изделия. Наибольшим спросом пользуются прядильные сорта асбеста, и проблема поставок во многом зависит от месторождений высококачественного хризотила. Такой материал используется для производства канатов, защитных занавесов, матов, набивок и фрикционных накладок в тормозах. Более низкие сорта используются для изготовления огнеупорной черепицы и других строительных материалов, для изоляции, а также для огнеупорного кирпича, кислотных фильтров и т. д. Хотя для низких сортов можно найти некоторые заменители, для прядильного волокна заменителей не известно.

Асбест встречается в трех основных типах: хризотил, крокидолит и антофиллит; первый и второй обеспечивают большую часть прядильного волокна, а третий почти полностью состоит из непрядильного качества. Самое важное месторождение хризотил-асбеста находится в Квебеке, Канада, но крупные месторождения разрабатываются в России и Родезии. Крокидолит добывается только в Капской колонии, Южная Африка. Крупные месторождения антофиллита встречаются в Соединенных Штатах, Италии и на Кипре.

Соединенные Штаты являются, безусловно, крупнейшим производителем асбестовых изделий в мире, но производят лишь малую часть необходимого сырья; они практически обеспечены достаточными поставками этого материала, поскольку крупнейшие месторождения в мире находятся в соседней провинции Квебек, Канада. Месторождения Аризоны обеспечивают отличное качество волокна и представляют собой многообещающий дополнительный источник поставок, хотя предполагаемые запасы невелики. Британская империя занимает доминирующее положение, контролируя около 88 процентов ежегодной мировой добычи асбеста и приблизительно 70 процентов предполагаемых запасов. Канада далеко опережает все страны, поставляя около 85 процентов мировой добычи. Россия до революции была второй после Канады по объему добычи; из-за стоимости транспортировки основной продукцией является прядильное волокно. Южная Африка обладает большими запасами хорошего волокна, но добыча затруднена плохой транспортировкой.

Истощение основных источников поставок вряд ли произойдет в течение многих лет, как и нет непосредственной перспективы какого-либо существенного сдвига в центрах производства, хотя с улучшением транспортировки возможен сдвиг в сторону Южной Африки. Спрос на высококачественный асбест, вероятно, будет расти стабильными темпами.

Все асбестовые карьеры в Соединенных Штатах, по-видимому, принадлежат американцам. Канадские месторождения контролируются канадским, английским и американским капиталом, причем британские интересы, вероятно, преобладают. Британские компании, очевидно, удерживают исключительный контроль над текущей добычей в Южной Африке, Австралазии и Италии. До войны российская добыча в значительной степени контролировалась немецким синдикатом, а добыча на Кипре — австрийской компанией.

ГЛАВА XXV ФОСФАТНАЯ ПОРОДА Автор: Р. У. Стоун

ИСПОЛЬЗОВАНИЕ ФОСФАТНОЙ ПОРОДЫ

Фосфатная порода главным образом используется после обработки серной кислотой в качестве ингредиента искусственных удобрений. Небольшое количество тонко измельчается и используется непосредственно в качестве удобрения. Меньшие количества используются для производства фосфорной кислоты и фосфора. Фосфор играет важную роль в военных операциях, используя для зажигательных пуль и дымовых завес. Фосфор также является обычным ингредиентом спичек и терочной поверхности на коробках безопасных спичек, и он входит в небольшой пропорции в фосфористую бронзу, фосфористую медь и фосфористое олово.

Заменители.

Заменители фосфатной породы можно разделить на природные и искусственные. Природные заменители — это фосфатный известняк; другие фосфатсодержащие минералы, такие как апатит, нельсонит и вавеллит; гуано; мергель; экскременты животных и кости. Искусственные заменители включают томасшлак и промышленные соединения, такие как фосфат аммония.

ГЕОЛОГИЧЕСКОЕ ЗАЛЕГАНИЕ

Фосфатная порода — это осадочное отложение, содержащее фосфат извести. Она встречается в виде твердой породы, переслаивающейся с пластами песчаника, сланца или других осадочных пород; в виде аморфных конкреций или гальки в речных отложениях; и в виде остаточного продукта разложения фосфатного доломита или известняка, или других пород, содержащих фосфат извести. Другой тип месторождений, обычно классифицируемый как фосфатная порода, — это пористый коралловый или другой известняк тропических островов, который был пропитан фосфатом, выщелоченным из гуано.

Фосфатные месторождения западных Соединенных Штатов, Алжира, Туниса и Египта представляют собой пласты твердых пород первого типа. Аморфные конкреционные отложения встречаются в Южной Каролине, части Флориды, Уэльсе, Англии, Бельгии, северо-центральной и восточной Франции и России. Месторождения в Теннесси, Кентукки и некоторые во Флориде являются остаточными. Выщелоченные отложения гуано встречаются на островах Аруба, Кюрасао и Сомбреро в Вест-Индии, а также на островах Рождества, Оушен, Макатеа, Ангаур и других островах в Индийском и южной части Тихого океана.

Запасы в Соединенных Штатах довольно хорошо известны и оцениваются в 6 000 000 000 тонн. Запасы высококачественной породы в Алжире и Тунисе оцениваются в 300 000 000 тонн. Информации о количестве фосфатной породы в Египте или Европе нет, за исключением того, что Россия, как полагают, имеет 80 000 000 тонн в одном из своих месторождений. Месторождения на островах южной части Тихого океана оцениваются в 70 000 000 тонн. До войны мировая добыча фосфатной породы составляла около 6 000 000 тонн ежегодно, из которых около половины добывалось в Соединенных Штатах. Следующее по величине производство осуществляется в Северной Африке.

Фосфорная кислота также получается из апатита, фосфата кальция, который встречается в жилах. Апатит добывался в провинции Квебек, Канада, и в Испании.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

В Западном полушарии фосфатная порода добывается в Соединенных Штатах, Канаде, Нидерландских Антильских островах и Французской Гвиане, а также встречается в Перу и Чили.

Соединенные Штаты.

Основные месторождения фосфатной породы в Соединенных Штатах находятся во Флориде, Южной Каролине, Теннесси, Кентукки, Арканзасе, Монтане, Айдахо, Вайоминге и Юте. Хотя самые крупные месторождения находятся в западных штатах, они дают менее 1 процента от общего объема из-за отсутствия крупного близлежащего рынка и высоких фрахтовых ставок на сырую породу. Это не является общеизвестным фактом, но, тем не менее, это факт, что западные месторождения фосфатной породы настолько обширны, что практически неисчерпаемы, даже если бы весь мир зависел от них в своих поставках фосфатов.

Фосфатные месторождения Флориды, которые являются наиболее широко разрабатываемыми в Соединенных Штатах, включают три класса фосфатов: твердая порода, сухопутная галька и речная галька. Первая — самого высокого качества, вторая производится в наибольшем количестве, а третья в настоящее время не добывается. Месторождения твердой породы лежат узкой полосой вдоль западной части полуострова Флорида от округа Суванни до округа Паско, на расстоянии около 100 миль. Область фосфатной сухопутной гальки, к востоку от Тампы, имеет длину около 30 миль и ширину 10 миль. Продажи фосфатов Флориды значительно сократились после 1913 года из-за ограничений на экспорт, вызванных войной. В 1913 году продажи составили 2 500 000 тонн стоимостью 9 500 000 долларов, а в 1915 году добыча составила 1 350 000 тонн стоимостью 3 700 000 долларов.

Южная Каролина производит сухопутный фосфат в окрестностях Чарльстона. Речная фосфатная галька встречается в той же области, но не добывается. Часть продукции Южной Каролины ежегодно экспортировалась. Продажи сократились со 169 000 тонн в 1911 году до 83 000 в 1915 году, а стоимость за те же годы — с 673 000 до 311 000 долларов.

Месторождения фосфатной породы в Теннесси находятся в западно-центральной части и крайнем северо-восточном углу штата; последние в последнее время не разрабатывались. Признаны три типа, известные по своим цветам как коричневая, синяя и белая порода; последняя в последнее время не добывалась. Коричневая порода продается с гарантией 70–80 процентов трикальцийфосфата; синяя порода значительно варьируется по содержанию фосфатов. Продажи фосфатов Теннесси в 1914 году составили 483 000 тонн стоимостью 1 823 000 долларов; к 1915 году они упали до 390 000 тонн стоимостью 1 328 000 долларов.

Кентукки в последние годы был незначительным производителем фосфатной породы. Месторождения фосфатов в Арканзасе находятся в северо-центральной части штата. Объем добычи невелик.

Четыре западных штата обладают огромными месторождениями высококачественной фосфатной породы, но их добыча пока незначительна, составляя всего 3000–5000 тонн в год. Производящими штатами являются Айдахо, Юта и Вайоминг. Монтана не является производителем, хотя содержит обширные месторождения, легкодоступные и близкие к железнодорожному транспорту.

Айдахо имеет неограниченные запасы высококачественных фосфатов в юго-восточной части штата. Небольшое количество добывается в округе Беар-Лейк. Месторождения Юты находятся к востоку от Большого Соленого озера, в хребтах Уосатч и Юинта, и к востоку от озера Беар-Лейк. Эти месторождения обширны, но порода беднее, чем обычный фосфат Айдахо, в среднем ближе к 60 процентам, чем к 80 процентам трикальцийфосфата. Западный Вайоминг также богат фосфатной породой, месторождения находятся в основном в хребтах Оул-Крик, Уинд-Ривер, Грос-Вентр и Солт-Ривер. Некоторые пласты толстые, содержат 80 процентов трикальцийфосфата и простираются на многие мили. Они составляют резервный запас, который можно назвать неисчерпаемым. Небольшой местный спрос на удобрения и отсутствие дешевого транспорта могут на несколько лет замедлить развитие великих и богатых западных месторождений.

Оценка количества фосфатной породы, доступной в Соединенных Штатах, была сделана несколько лет назад и не требует пересмотра с учетом того, что было добыто в промежутке. Она повторяется здесь:

Запасы фосфатной породы в Соединенных Штатах

| Long tons
Florida | 227,000,000
Tennessee | 88,000,000
South Carolina | 9,000,000
Kentucky | 1,000,000
Arkansas | 20,000,000
| 345,000,000
Western States: Montana, Idaho, Utah, and Wyoming | 5,367,082,000
Total | 5,712,082,000

Канада.

Основной фосфатной породой в Канаде является апатит, который встречается в пригодном для разработки количестве в двух основных районах — один в провинции Онтарио, другой в провинции Квебек. Эти месторождения, которые разрабатывались в основном карьерным способом, в настоящее время практически заброшены. Фосфатная порода встречается в тонком пласте недалеко от Банфа, Альберта, но не используется.

Южная Америка.

На Арубе и Кюрасао, островах Нидерландских Антильских островов, у побережья Венесуэлы, находятся месторождения фосфатной породы, из которых небольшое количество добывается и отправляется в Европу. Сообщается, что добыча в 1914 году составила около 100 000 тонн, в среднем 85–90 процентов фосфата кальция.

В Перу, в департаменте Ика, находится месторождение конкреционного фосфата извести, которое не используется из-за местного предпочтения гуано.

Крупное, богатое месторождение фосфатов обнаружено в Чили, примерно в 300 милях к северу от Вальпараисо, но пока не разрабатывалось.

Фосфатные месторождения встречаются на острове Салю и на островах Коннетабль, недалеко от побережья Французской Гвианы. Порода экспортируется.

Европа.

Высококачественные фосфатные месторождения Бельгии истощены, остались только низкосортные месторождения. Порода встречается в слоях и карманах и содержит от 25 до 65 процентов костяного фосфата. Добыча с 1911 по 1913 год составляла в среднем более 200 000 тонн ежегодно.

Основные месторождения во Франции находятся в бассейнах Соммы и Уазы. Лучшие французские месторождения выше по качеству, чем бельгийские, так как они содержат 50–80 процентов костяного фосфата, но они почти истощены, остались только низкосортные материалы. Добыча с 1910 по 1914 год составляла около 300 000 тонн ежегодно.

Важные месторождения фосфатной породы в России можно разделить на северную, центральную и южную группы. Месторождения южной группы были единственными, которые эксплуатировались до войны. Их добыча составляла около 25 000 тонн в год — очень мало по сравнению с размером месторождений, которые, по оценкам, содержат более 1 500 000 000 тонн. Часть породы высокого качества, содержит до 75 процентов трикальцийфосфата, но нормальный сорт составляет около 50 процентов.

Единственные месторождения, которые широко разрабатываются в Испании, — это апатитовые жилы в провинции Касерес. После многолетнего простоя эти месторождения были вновь открыты и дали 28 000 тонн в 1917 году.

Низкосортный фосфат в виде пластов конкреций встречается в Англии и Уэльсе. Добыча была незначительной, потому что месторождения слишком малы для промышленной эксплуатации.

Африка.

Основные месторождения фосфатной породы в Тунисе — это поля Гафса в южной половине страны. Там фосфат встречается в пластах толщиной в несколько футов, но эксплуатируются только те, которые содержат более 58 процентов фосфата извести. Месторождения можно проследить на несколько сотен миль, и они составляют резерв в сотни миллионов тонн. Тунис сейчас производит больше фосфатов, чем любая другая зарубежная страна, его ежегодная добыча составляет от 1 500 000 до 2 000 000 тонн, большая часть которых идет в Южную Европу.

Месторождения фосфатной породы в Алжире являются продолжением месторождений в Тунисе, важные горнодобывающие районы находятся в восточном Алжире. Добыча составляет более 500 000 тонн в год, а экспортируемая порода содержит 58–68 процентов фосфата извести.

Обширные месторождения фосфатов встречаются в Египте, недалеко от Красного моря, в тонких и нерегулярных пластах того же геологического возраста (эоцен), что и месторождения в Тунисе и Алжире. Лучшие месторождения содержат в среднем 70 процентов фосфата извести, а добыча в 1916 году составила 125 000 тонн. Есть рудники в 20 милях от Порт-Сафаги и концессии в 12 милях вглубь страны от Коссейра, а также в Себае, на восточном берегу Нила между Кеной и Асуаном. Пласты фосфатов найдены в других районах по обе стороны долины Нила. Практически вся добываемая сырая фосфатная порода содержит 65 процентов или более трикальцийфосфата и экспортируется в основном в Японию.

Месторождения фосфатов встречаются в 80–120 километрах от города Триполи в пластах толщиной более 1 метра. Эти пласты, вероятно, являются продолжением фосфатных месторождений в южном Тунисе.

Месторождения фосфатов отмечены в Марокко в 125 километрах к юго-юго-западу от Касабланки на западном побережье и в 70 километрах от конца железной дороги. Говорят, что эти месторождения сопоставимы с полем Гафса в Тунисе.

Сообщается, что в Дилоре, в Сенегале, примерно на широте Зеленого Мыса, самой западной точки африканского побережья, есть фосфатный пласт толщиной 2 метра на глубине 64 метра. Порода содержит только 50 процентов трикальцийфосфата, поэтому она не пригодна для разработки в нынешних условиях, особенно ввиду обилия высококачественной породы в Алжире и Тунисе.

Фосфаты были найдены в Натале, недалеко от Винена, Ледисмита и Бернетауна, в виде фосфатных сланцев и конкреций. Процент трикальцийфосфата в фосфатных сланцах слишком низок для использования при производстве суперфосфатов; фосфатные конкреции более высокого качества, но недостаточно обильны, чтобы иметь ценность.

Азия и Австралазия.

В Уральской области, в юго-западной Сибири, граничащей с северной оконечностью Каспийского моря, по сообщениям, находится 600 000 000 тонн фосфатной породы. Говорят, что большая часть этого материала содержит 17–20 процентов фосфорной кислоты, что эквивалентно 36–43 процентам трикальцийфосфата. Тургайская область, граничащая с Уральской областью на востоке, по сообщениям, содержит 67 000 000 тонн фосфатной породы, большая часть которой содержит 18–19 процентов фосфорной кислоты, или около 40 процентов трикальцийфосфата. Самый высококачественный материал, о котором сообщается, содержит 24 процента фосфорной кислоты, что эквивалентно примерно 52 процентам трикальцийфосфата. Таким образом, весь фосфат низкосортный. О добыче ни в одной из этих местностей не сообщается.

Низкосортная фосфатная порода в осадочных пластах значительной протяженности и высококачественные жильные месторождения отмечены в Палестине, на восточной стороне Иордана. Осадочные месторождения встречаются также на западной стороне Иордана. Известные запасы составляют около 3 500 000 тонн. Осадочные месторождения содержат в среднем около 48 процентов, а жильные месторождения — 77 процентов трикальцийфосфата. Поскольку жильный материал пригоден для экспорта, эти месторождения были исследованы французской компанией, но имеющаяся информация указывает на то, что добычи не было.

Острова в северной части Тихого океана.

После открытия фосфатной породы на острове Раса, в 500 милях к востоку от Формозы, несколько лет назад была сформирована японская компания для эксплуатации месторождений. Порода богатая, содержит 75 процентов фосфата извести, а запасы оцениваются в 2 800 000 тонн. В 1915 году остров Раса дал 50 000 тонн. Бывший немецкий источник фосфатов находится на острове Ангаур, в группе Пелау, к востоку от южной оконечности Филиппин. Запасы на этом острове оцениваются в 2 000 000–4 000 000 тонн фосфатной породы, в основном высокого качества. Германия увеличила добычу с 45 000 тонн в 1910 году до 90 000 тонн в 1913 году. Япония удерживает этот остров с октября 1914 года и добывает 30 000 тонн или более фосфатов ежегодно.

Месторождения фосфатов, состоящие из замещений доломитового кораллового известняка и фосфатного гуано, отмечены на нескольких других островах Океании, таких как острова Бейкер и Фаннинг в Полинезии и остров Фаис на западных Каролинских островах. Вероятно, на других островах есть коммерческие месторождения, еще не открытые.

Острова в Индийском и южной части Тихого океана.

К северу от Аделаиды, в Австралии, находятся кармановые месторождения фосфатов; они не имеют регулярной стратификации и разного качества. Ежегодная добыча составляла 4000–6000 тонн в течение нескольких лет. В районе Отаго, недалеко от Кларендона, Новая Зеландия, пласты фосфатов толщиной от 3 до 12 футов залегают в карманах в известняке. Добыча была очень незначительной, если вообще была.

На острове Рождества (Стрейтс-Сетлментс), расположенном в Индийском океане в 190 милях к югу от Явы, добывается порода, содержащая 80 процентов костяного фосфата, которая затем отправляется в Австралию и Японию. Месторождения, по-видимому, носят нерегулярный характер, однако, по оценкам, содержат несколько миллионов тонн породы очень высокого качества. Остров принадлежит правительству Сингапура. Эксплуатация месторождений британцами началась в 1900 году. В 1913 году экспорт составил 150 000 тонн.

Фосфориты высокого качества добываются на острове Ошен, входящем в архипелаг Гилберта, расположенном между Маршалловыми островами и Соломоновыми островами, к востоку от Новой Гвинеи и к северу от Новой Зеландии. На этом и других так называемых коралловых островах в экваториальном поясе, которые на протяжении веков служили лежбищами морских птиц, выщелачивание гуано пропитало известняк, образовав фосфориты мощностью во много футов. Месторождения на этом острове, как говорят, составляют многие миллионы тонн и являются одними из самых богатых в мире. Их добывают с 1901 года, при этом объем добычи достигал 300 000 тонн в год. В 1916 году объем добычи составил 70 000 тонн породы, содержащей около 85 процентов трикальцийфосфата. Остров является британским владением.

Еще одним британским владением в архипелаге Гилберта, содержащим фосфориты, является остров Плезант, также известный как остров Науру или Нгару. Месторождения схожи с месторождениями на островах Ошен и Рождества, отличаясь очень высоким содержанием фосфата кальция и низким содержанием железа и глинозема. Ранее этот остров принадлежал Германии, но в 1917 году он был захвачен британцами.

По оценкам, на острове Макатеа, недалеко от Таити в архипелаге Острова Общества, содержится 10 000 000 тонн фосфоритов очень высокого качества, неравномерно распределенных между рифами и доломитовыми пиками. Месторождения начали разрабатываться лишь в 1910 году и до 1917 года дали более 300 000 тонн. Часть породы содержит 85 процентов фосфата извести. Остров является французским владением.

НЕДАВНИЕ ИЗМЕНЕНИЯ И РАЗВИТИЕ

С началом Мировой войны экспорт фосфоритов из Соединенных Штатов, обычно составлявший около 1 000 000 тонн в год, был прекращен, и годовое производство в Соединенных Штатах упало с 3 000 000 до 1 800 000 тонн. В отечественной промышленности наблюдается сильное восстановление, и если условия труда и транспортировки улучшатся, то вскоре годовой объем производства должен составить почти 3 000 000 тонн для внутреннего потребления, или столько же фосфоритов для нашего собственного использования, сколько ранее производилось для нас самих и для крупной экспортной торговли.

Предполагается, что в будущем Северная Африка будет давать большие количества, чем в довоенный период. Производство в Алжире, Тунисе и Египте, вероятно, стимулировалось во время войны из-за значительного сокращения количества американской породы, отправляемой в Европу.

Япония, несомненно, обеспечит большой объем добычи на германских месторождениях в Полинезии, которые перешли в ее владение в начале войны.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Право собственности на месторождения фосфатов в Соединенных Штатах в основном является внутренним; некоторые из месторождений твердых пород Флориды принадлежат французским и (до войны) германским компаниям. Месторождения, принадлежавшие Германии, были переданы Управляющему имуществом враждебных государств и, несомненно, перешли в другие руки. Месторождения фосфатов на Кюрасао, Нидерландские Антильские острова, разрабатываются компанией Curacao Phosphate Mining Co., которая отправляет продукцию в Англию и Германию. Месторождения фосфатов в Алжире и Тунисе эксплуатируются французскими компаниями. Некоторые компании работают на условиях аренды. В качестве участников в этих областях упоминались La Compagnie des Phosphates de Paris и La Compagnie Algerienne des Phosphates. Месторождения на нижнем Ниле и Красном море разрабатываются Egyptian Phosphate Co., британским предприятием, и Societa Egiziana per l’Estrazione de il Commercio dei Phosphati, компанией, управляемой итальянцами. Сообщается, что значительная часть продукции идет в Японию. Компания Pacific Phosphate Co., Ltd. из Лондона эксплуатирует на правах концессии месторождения фосфатов на островах Ошен и Плезант. Японские компании добывают фосфаты на островах Раса и Ангаур.

ПОЛОЖЕНИЕ ВЕДУЩИХ СТРАН

Соединенные Штаты обладают крупнейшими известными месторождениями фосфоритов в мире и, как и до войны, могут удовлетворять потребности других стран, а также свои собственные. С начала добычи было извлечено около 55 000 000 тонн, что составляет менее 1 процента запасов. Великобритания обладает фосфатами в Египте и на островах Рождества, Ошен и Плезант, и импортировала их из Соединенных Штатов и, вероятно, из Северной Африки. Франция и другие средиземноморские страны имеют достаточные запасы в Алжире и Тунисе. Германия ранее владела богатыми месторождениями фосфатов на острове Ангаур в группе островов Пелеу, Полинезия, а также на островах Плезант и Ошен, но, насколько известно, в настоящее время не имеет источника снабжения. Япония располагает большими запасами высококачественных фосфатов на островах Раса и Ангаур.

РЕЗЮМЕ

Основным применением фосфоритов является использование в качестве ингредиента удобрений. Меньшие количества потребляются при производстве фосфорной кислоты, фосфора, используемого в военных операциях, при производстве спичек и в металлургии. Для многих видов использования фосфоритов доступны как натуральные, так и искусственные заменители.

Фосфорит — это осадочное отложение, содержащее фосфат извести. Он встречается в виде твердой породы между пластами песчаника или сланца, в виде аморфных конкреционных фосфатов в аллювиальных отложениях и в виде остаточного продукта разложения фосфатоносных доломитов, известняков и других фосфатоносных пород. Пористый известняк тропических островов, пропитанный фосфатами, выщелоченными из гуано, обычно классифицируется как фосфорит.

Месторождения фосфоритов, имеющие в настоящее время коммерческое значение, расположены в Соединенных Штатах, Алжире, Тунисе, Египте и на островах Индийского и южной части Тихого океанов, причем Соединенные Штаты обладают, безусловно, самыми большими запасами. Меньшие месторождения, либо неразработанные, либо почти истощенные, находятся в Канаде, Венесуэле, Чили, Бельгии, Франции, России, Англии, Испании, Южной Австралии и Новой Зеландии.

Во время войны экспорт фосфоритов из Соединенных Штатов значительно сократился. Однако с возвращением к нормальным условиям Соединенные Штаты должны без особых трудностей снова стать основным источником фосфоритов.

Основные месторождения фосфоритов находятся под политическим контролем Соединенных Штатов, Франции (Алжир и Тунис) и Великобритании (Египет). Ряд фосфатоносных островов в Тихом океане принадлежал Германии до войны, но был захвачен Великобританией и Японией.

Коммерческий контроль над месторождениями Соединенных Штатов находится в основном в руках американцев, хотя германские (до войны) и французские интересы владеют некоторыми из месторождений твердых пород Флориды. Месторождения Алжира и Туниса контролируются французскими компаниями. Египетские месторождения контролируются двумя компаниями: одной британской и другой итальянской.

Германия останется без источника снабжения под собственным контролем теперь, когда она потеряла свои колонии.

ГЛАВА XXVI. КАЛИЙНЫЕ СОЛИ. Авторы: Хойт С. Гейл и А. У. Стокетт

ПРИРОДА И ПРИМЕНЕНИЕ КАЛИЙНЫХ СОЛЕЙ

Термин «калийные соли» обычно используется для обозначения любых солей элемента калия, особенно тех, которые растворимы в воде и широко используются в сельском хозяйстве и промышленности. Элемент калий широко распространен как компонент горных пород, почв, а также растительных и животных веществ, но большие количества солей калия в формах, пригодных для использования человеком, были найдены лишь в немногих местах. Древесная зола, которая ранее была основным источником калийных солей в торговле, сейчас поставляет незначительную часть мировых потребностей. С 1860 года основным, по сути, почти единственным коммерческим источником калийных солей являются огромные месторождения в Северной Германии. Сырые соли калия, получаемые из этих месторождений в процессе добычи, используются либо в качестве удобрения в том виде, в котором они извлекаются из земли, либо очищаются путем кристаллизации или перерабатываются в различные соединения калия, необходимые как для сельского хозяйства, так и для других промышленных нужд.

Использование в сельском хозяйстве в качестве ингредиента так называемых искусственных или химических удобрений составляет 90 процентов или более мирового потребления. Калий является не только одним из десяти или более химических элементов, необходимых для жизни растений, но и одним из трех, которые часто настолько отсутствуют в почвах, что урожайность сельскохозяйственных культур становится нерентабельной. Даже если калий присутствует в почвах, он может находиться и часто находится в форме, нелегко доступной для использования растениями, поэтому внесение свежих, легко растворимых в воде солей калия дает быстрый эффект, стимулируя рост урожая. В общем смысле считается, что калийные соли обеспечивают необходимое питание растений, которое укрепляет стебель и наполняет зерна растущего растения. Также существует общее мнение, что некоторые разрушительные болезни растений, такие как фитофтороз и ржавчина хлопка и картофеля, в значительной степени способствуются неправильным питанием, а также плохим физическим состоянием почвы, для чего калийные соли, по-видимому, являются специфическим средством. Таким образом, так называемая калийная промышленность, под которой понимается добыча и сбыт основных или наиболее распространенных соединений калия, основана главным образом на использовании в сельском хозяйстве.

Другие виды использования солей калия многочисленны и разнообразны. Большинство солей калия обладают свойствами, схожими с соответствующими солями натрия, и для большинства промышленных целей соли этих двух элементов могут быть взаимозаменяемыми, что, однако, в какой-либо степени не относится к сельскохозяйственному применению калия. Некоторые промышленные предпочтения в пользу соли калия зависят от более благоприятных физических свойств калия по сравнению с солью натрия, таких как меньшая склонность соли калия поглощать влагу из воздуха. Другие предпочтения зависят от незначительных химических различий, как, например, несколько большая растворимость, что облегчает очистку соли калия. Во время дефицита и высоких цен в военный период было сделано много замен, которые либо напрямую, либо путем некоторой модификации практики сейчас оказываются настолько удовлетворительными, что, вероятно, будут продолжены.

Один из самых насущных спросов на калийные соли исходит от производителей спичек. Хлорат калия является важным ингредиентом большинства спичек, и это использование потребляет удивительно большое количество калийных солей. Некоторые виды стекла, особенно столовая посуда из хрусталя (флинтглас) и некоторые виды оптического стекла, изготавливаются из калийных солей, обычно в форме, известной как карбонат для производства стекла. Большинство видов мыла изготавливается из соды, но калийные соли (в виде едкого кали или гидроксида) используются для некоторых более тонких сортов, таких как мыло для бритья, туалетное мыло и шампуни, особенно в жидкой форме. Едкое кали нашло значительное применение в прачечных, а также для промывки или стирки шерсти. Старая форма черного пороха изготавливалась из калийных солей в виде нитрата калия или селитры; отсюда и общепринятое мнение о военном значении калийных солей. Черный порох, хотя сейчас в значительной степени вытеснен современными порохами высокой взрывчатости, все еще имеет относительно небольшое, но тем не менее важное применение в современной войне. Существуют и другие виды использования, которые, хотя и требуют небольшого общего количества, включают некоторые важные потребности, среди которых медицинские или фармацевтические, кожевенные, красильные, фотографические, гальванотехнические и металлургические нужды.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Великие месторождения калийных солей в Северной Германии залегают под обширной территорией в прусских провинциях Саксония, Ганновер, а также в герцогствах Ангальт и Брауншвейг. Наиболее важные горнодобывающие районы лежат в области, практически опоясывающей горы Гарц, в 75–150 милях к юго-западу от Берлина и в 100–150 милях к югу — юго-востоку от Гамбурга. Эта область более точно обозначена на прилагаемой обзорной карте (рис. 14).

Месторождение, первоначально открытое в Штассфурте, с тех пор было исследовано глубоким бурением и освоено путем проходки шахтных стволов, в результате чего были намечены предполагаемые запасы в 20 000 000 000 метрических тонн сырых калийных солей, которых при нынешнем уровне мирового потребления должно хватить почти на 2000 лет. Таким образом, для всех практических целей месторождение можно считать неисчерпаемым.

Рис. 14. — Распространение месторождений калийных солей в Северной Германии.

В 1904 году в результате бурения в долине реки Рейн в южном Эльзасе было обнаружено еще одно важное и обширное месторождение водорастворимых калийных солей. Эльзас, находившийся тогда во владении Германии, теперь возвращен Франции. Месторождение состоит из двух по существу непрерывных пластов, залегающих на доступной глубине под площадью 70–80 квадратных миль плоских низинных земель долины Рейна. По оценкам, пласты содержат около 1 500 000 000 метрических тонн сырых калийных солей, которые в среднем значительно богаче калием, чем продукция северогерманских месторождений, и, будучи более простыми по химическому составу, легче поддаются очистке. Шахты, открывающие эти месторождения, легко доступны для водного транспорта по реке Рейн и каналам долины Рейна. Расстояние до океанских портов значительно больше, чем от северогерманских месторождений, составляя около 375 миль по сравнению со 150 милями по каналам и речным судам от последних, но объем погрузочно-разгрузочных работ, необходимых для транспортировки аналогичных грузов из этих двух районов, по-видимому, примерно одинаков. Месторождение в Эльзасе находится в эллиптической области, центр которой расположен примерно в 5 милях к северо-западу от города Мюлуз.

Некоторое количество калийных солей было добыто на месторождении в Галиции, недалеко от Калуша, к югу от Лемберга, из месторождений, которые, как сообщается, относятся к типу, схожему с месторождениями Северной Германии, но этот район никогда не давал даже достаточного количества калийных солей для удовлетворения местного спроса и считается небольшим.

Во время войны относительно небольшие объемы калийных солей были получены из многих независимых источников в Соединенных Штатах, Абиссинии, Тунисе и других странах. Под давлением военных нужд и полного прекращения других поставок эти объемы в совокупности составили значительную величину. Большая часть разработок, вероятно, не будет постоянной, когда возобновится строгая конкуренция с калийными солями из более доступных источников, но каждое из этих месторождений и, несомненно, многие другие содержат возможности развития, которые могут в любой момент придать мировой ситуации новый аспект. Главным среди наиболее непосредственных перспектив для важного развития является довольно обширное месторождение в восточной Испании, недалеко от Барселоны. Это месторождение еще не начало добычу в коммерческих масштабах. Одна из оценок запасов в испанском месторождении утверждает наличие доказанной площади в 13,5 квадратных миль, содержащей 200 000 000 тонн оксида калия.

Нитратные месторождения Чили содержат небольшой процент калийных солей, и они извлекаются отдельно от нитрата натрия на нескольких нефтеперерабатывающих заводах. Было подсчитано, что из этого источника можно ежегодно получать в общей сложности 240 000 тонн оксида калия.

Многие различные источники в Соединенных Штатах дают калийные соли. Крупнейшее известное месторождение растворимых калийных солей в довольно концентрированной форме находится на озере Серлс, Калифорния. Это высохшее соленое озеро, представленное сейчас пластом кристаллических солей с большим количеством насыщенного рассола, богатого калийными солями. Тело солей, несущее рассол, залегает под площадью около 25 квадратных миль и простирается на среднюю глубину 70 футов. По оценкам, только рассол в этом месторождении содержит почти 20 000 000 тонн оксида калия, чего было бы достаточно для удовлетворения потребностей страны в течение примерно 60 лет при нынешнем нормальном уровне. Многочисленные небольшие озера в западной Небраске содержат рассолы, исключительно богатые калийными солями, и они сейчас дают значительный объем производства калийных удобрений. Удовлетворительной оценки запасов в этом районе нет.

При нынешних условиях эксплуатации около одной трети годовых потребностей Соединенных Штатов может быть извлечено на цементных заводах. Около 380 000 коротких тонн калийных солей, большая часть которых улетучивается, ежегодно загружается в доменные печи страны. Лучшие доступные оценки показывают, что около 30 000 тонн калийных солей ранее пропадали в отходах мелассных винокуренных заводов и около 8 000 тонн — в сточных водах процесса Штеффена на свеклосахарных заводах страны. Келп и алунит доступны в количествах, достаточных для продолжения обеспечения существенного производства. Огромные количества лейцитовой лавы, содержащей 10 процентов калийных солей в нерастворимой силикатной форме; глауконитовый песок, содержащий от 6 до 7 процентов нерастворимых калийных солей; серицит с содержанием от 7 до 12 процентов и полевой шпат с аналогичным содержанием доступны в качестве сырья для производства, если могут быть разработаны удовлетворительные коммерческие процессы. Таким образом, потенциальные запасы калийных солей в Соединенных Штатах практически неисчерпаемы. Будущее американской калийной промышленности, следовательно, зависит от разработки процессов или методов разделения, достаточно экономичных, чтобы позволить отечественному продукту конкурировать с импортными калийными солями.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Месторождения калийных солей в Северной Германии залегают посреди серии формаций, известных как Цехштейн, геологический возраст которых — пермский. Как эльзасские, так и испанские месторождения встречаются в олигоценовых третичных породах, хотя месторождения не обязательно были строго синхронными по происхождению. Галицийские месторождения описываются как имеющие нижнемиоценовый (третичный) возраст. Это основные известные пластовые месторождения калийных солей в мире, для которых, как для класса, различие по геологическому возрасту, по-видимому, имеет особое значение. Ассоциация калийных солей с крупными месторождениями солей и гипса в мире, по-видимому, по какой-то причине была исключительной в геологической истории. Но определение того, что эти несколько аналогичные проявления сформировались в разное время и в разных местах, является хорошим основанием для ожидания того, что подобные месторождения могут быть еще обнаружены в других местах.

ИЗМЕНЕНИЯ В КОММЕРЧЕСКОЙ ПРАКТИКЕ

До войны мировое потребление калийных солей практически было мерилом германского производства, статистика которого доступна в значительных деталях. В круглых цифрах Германия производила около 10 000 000 метрических тонн калийных солей, содержащих в среднем около 10 процентов K2O, из которых она использовала более 60 процентов внутри страны и экспортировала около 25 процентов в Соединенные Штаты. В течение двух лет очень небольшое производство из Эльзаса было объединено с остальным. Вскоре после начала войны германское правительство наложило эмбарго на экспорт калийных солей, предположительно в надежде нанести тем самым ущерб производству сельскохозяйственных культур союзников, и, возможно, из-за того небольшого военного значения, которое они имеют. Производство калийных солей в Германии, однако, продолжалось практически на том же уровне, что и до войны, при этом часть, ранее экспортировавшаяся, распределялась для использования в качестве удобрений внутри страны. Это, естественно, дало огромный стимул усилиям других стран по развитию источников калийных солей. Хотя огромных природных ресурсов, сопоставимых с уже известными месторождениями, обнаружено не было, усилия тем не менее имели разумный успех, так что мир не пострадал каким-либо жизненно важным образом из-за лишения калийных солей. Стоимость калийных солей в Соединенных Штатах и странах-союзниках увеличилась до десяти раз по сравнению с довоенной ценой, но предложения было достаточно для удовлетворения всех самых насущных потребностей. Было открыто много возможностей для производства из различных источников, для которых еще слишком рано предсказывать окончательный результат. По-видимому, ряд этих новых предприятий вошел в эту область на постоянной основе, хотя в период реконструкции неизбежно будет некоторая неопределенность.

Уступка Эльзаса Франции, которая обсуждается в последующем параграфе, несомненно, влечет за собой самое большое и значительное изменение в коммерческой ситуации в отношении мирового рынка калийных солей. Возможность производства из месторождений в восточной Испании имеет схожее, хотя и более отдаленное значение.

ИСТОЧНИКИ ПРОИЗВОДСТВА

Объем производства калийных солей в 1917 году, суммированный по странам в соответствии с лучшими доступными данными, выглядит следующим образом:

Таблица 65. — Мировое производство калийных солей в 1917 году

Country
Source of data
Production
(short tons)
Average
content
K₂O
(per cent.)

Germany | Kalisyndikat statistics. | 9,853,171 | 11.2 |
Alsace | (Included under Germany.) |  |  |
United States | U. S. Geological Survey. | 126,961 | 25.6 |
India | Rec. Geol. Surv. India, vol. 49, part 2, p. 71. | 23,838 | 40.0 | [155]
Tunis | Jour. Soc. Chem. Ind., vol. 37, p. 294 T. | 20,000 | 40.0 |
Galicia | “Kali,” vol. 7, p. 9. | 10,000 | 10.0 |
Russia | War Industrial Comm. of Russia report. | 5,000 |  |
Abyssinia | Com. Fertilizer, Jan. 18, 1918, p. 44. | 5,000 | ? |
Japan | Commerce Rept., Dec. 1, 1916, p. 830. | 4,000 | ? |
Chile | U. S. imports potassium nitrate. | 1,750 | 25.0 | [155]
China | Commerce Rept., Nov. 27, 1918, p. 790. | 1,000 |  |
France | Saline-de-Giraud. | 300 |  |
Mexico | U. S. imports saltpeter. | 115 | 40.0 | [155]
England | Kelp and blast furnace recoveries. | ? | ? |
Spain | ... | No production
Total |  | 10,051,135 |  |

[155] Оценка по указанным данным.

ПОЛИТИЧЕСКИЙ И КОММЕРЧЕСКИЙ КОНТРОЛЬ

Германия.

— Сообщается, что калийная промышленность в Германии представляла собой инвестиции в размере 500 000 000 марок (119 000 000 долларов). В 1918 году насчитывалось 209 шахт, способных к производству, как указано в списке Kalisyndikat, распределяющем квоты на ожидаемое производство от отдельных шахт на год.

Большинство этих шахт находятся в частной собственности в соответствии с различными законами в отдельных германских землях и провинциях. Первоначально разработки, как говорят, велись в соответствии с различными местными правилами; например, в Ганновере права на добычу принадлежали владельцам собственности, в Саксонии права на разведку были свободными, а концессии на добычу принадлежали первому открывателю месторождений без учета владельца поверхности почвы, а в Ангальте добыча сначала была объявлена государственной монополией, которая позже была передана по контракту нескольким частным компаниям. Некоторые объекты, однако, принадлежат государству и эксплуатируются им. Прусское правительство владеет шахтами в Штассфурте, Блейхероде и Виненбурге; герцогство Ангальт имеет крупные предприятия в Леопольдсхалле; а герцогство Брауншвейг имеет долю в некоторых калийных объектах.

Известны два случая участия американских предприятий в германской промышленности. International Agricultural Corporation, американская компания, организованная в 1909 году, некоторое время была владельцем всего акционерного капитала Sollstedt Works в Германии. Позже половина доли в этой американской корпорации была передана Kaliwerke Aschersleben, другому германскому предприятию, на условиях, которые, по-видимому, усложнили вопрос собственности. Virginia-Carolina Chemical Co. из Ричмонда, Вирджиния, как сообщается, приобрела контрольный пакет акций Einigkeit Works, предположительно в результате прямой денежной сделки.

Согласно закону германского рейхстага, известному как закон о калийных солях от 25 мая 1884 года, был предписан обязательный контроль над калийной промышленностью в Германии. Был создан общий орган, известный как Kalisyndikat, представляющий все шахты, с полномочиями контролировать открытие новых шахт, объем производства каждой шахты и продажные цены на калийные соли. Таким образом, промышленность стала трестом, поддерживаемым германским правительством, хотя частная собственность на отдельные объекты сохраняется. Этот синдикат отличается от американского синдиката тем, что он сформирован на ограниченный период времени, в данном случае 5 лет, и его оборотный капитал невелик, достаточен только для обеспечения фактических рабочих нужд организации. Цель синдиката — предотвратить катастрофическую конкуренцию, обеспечить соответствие предложения спросу и получение разумной прибыли производителями.

Шахты или предприятия, составляющие калийный синдикат, как и большинство горнодобывающих синдикатов в Германии, могут быть либо с ограниченной ответственностью, акции которых не подлежат оценке, либо те, чей акционерный капитал разделен на акции, называемые «kuxe», которые подлежат оценке в любое время и имеют неограниченную ответственность. Акции обоих видов торгуются на биржах в крупных городах Германии.

Каждая компания, являющаяся членом германского синдиката, имеет своего представителя в совете управления треста, и этот совет устанавливает квоту производства, разрешенную каждой шахте, и в целом управляет делами всего объединения в соответствии с его уставом и правилами (statuten). [156] Устав и правила должны быть подписаны каждым предприятием, вступающим в синдикат, и содержащиеся в них положения должны строго соблюдаться под угрозой штрафов, взыскиваемых в судебном порядке.

[156] Выдержка из Daily Consular and Trade Reports, № 265, том 4, 11 ноября 1911 г., стр. 760.

Слабым местом в этой форме организации являются разногласия, которые часто возникают по поводу квот, разрешенных различным членам. Каждая компания хочет получить как можно большую долю. По истечении срока действия синдиката всегда существует неопределенность относительно того, будет ли он продлен, из-за конкуренции между различными входящими в него фирмами.

До войны, согласно условиям контрактов пяти крупных компаний по производству удобрений с германским калийным синдикатом, половина максимально допустимой скидки вычиталась из суммы счета-фактуры, покрывающего каждую поставку, а остаток выплачивался покупателю в конце каждого полугодия при условии, что он предоставил синдикату письменное заявление о том, что он закупил все свои потребности в калийных солях у синдиката. Таким образом, допуская максимальные скидки для крупных покупателей и не позволяя им иметь дело с калийными солями из любого источника, кроме синдиката, это положение было направлено на подавление развития любых конкурентных источников снабжения.

Эльзас.

— Месторождения калийных солей в Эльзасе разрабатывались в соответствии с германским законом о горном деле для Эльзас-Лотарингии от 16 декабря 1843 года, измененным 14 июля 1908 года, с особым упоминанием калийных солей. После перемирия германские шахты эксплуатировались в режиме секвестра под руководством французских военных властей, направляемых министерством промышленной реконструкции Франции. Теперь, когда мирный договор ратифицирован Германией, Эльзас можно считать формально и окончательно перешедшим во владение Франции, а вместе с этим, естественно, и политический и коммерческий контроль над эльзасскими месторождениями калийных солей. Поэтому французскому парламенту предстоит определить, каково будет окончательное распоряжение бывшей германской собственностью на эти объекты, и такие вопросы, как национализация или франко-эльзасский контроль, обсуждались летом 1920 года.

Хотя большинство концессий на эльзасском калийном месторождении были предоставлены германским интересам, развитие было начато эльзасцами, и две из концессий находятся во франко-эльзасской собственности. Они не были и, вероятно, не будут изменены, если только они не вступят в какое-либо добровольное объединение.

В Соединенных Штатах было организовано агентство по продаже и распределению эльзасских калийных солей, и, по крайней мере в настоящее время, продукт вступает в прямую конкуренцию с солями из старых германских шахт.

Испания.

— Месторождения калийных солей, недавно обнаруженные в провинциях Барселона и Лерида в Каталонии, в восточной Испании, подлежат специальным правилам испанского правительства. Большая площадь концессий, уже предоставленных частным интересам, охватывает значительную часть поля, намеченного разведочными бурениями. Операции на этих концессиях разрешены, но государство оставляет за собой право подчинить эксплуатацию интересам страны и наложить особые условия в пользу потребления калийных солей, произведенных в Испании. Недавно неисследованные государственные земли были открыты королевским указом для торгов на разведку и аренду. Схема в целом следует плану государственного контроля над германской калийной промышленностью. Согласно ей, все концессии на разработку и продажу солей подлежат во многих деталях государственному контролю. Среди прочих условий, работа должна быть непрерывной, за исключением определенных исключительных обстоятельств; государство ежегодно устанавливает внутренние и экспортные цены, а также максимальную и минимальную квоту для каждой шахты.

Другие страны.

— До войны австрийский калийный синдикат, состоявший из австрийского правительства и группы капиталистов, контролировал месторождения недалеко от Калуша в Галиции. О каких-либо специальных государственных правилах для второстепенных операций, связанных с производством калийных солей в других странах, не сообщается.

РЕЗЮМЕ

Более 90 процентов калийных солей, используемых в мировой торговле, применяются в качестве удобрений. Остальное используется в качестве химического вещества в различных отраслях промышленности, главными из которых являются производство спичек, определенных видов стекла и мыла, а также лучших сортов черного пороха. Виды использования, специально упомянутые в этом параграфе, являются существенными, так как удовлетворительные заменители неизвестны.

До 1914 года практически все калийные соли, используемые в мире, поступали из месторождений в Северной Германии, которые по существу неисчерпаемы. Следующими по важности являются месторождения Эльзаса, которые содержат достаточно калийных солей для удовлетворения текущих мировых потребностей почти на 300 лет. Другие ресурсы известны в Испании, Галиции, Абиссинии, нитратных пластах Чили и в месторождениях в Соединенных Штатах, но еще слишком рано с уверенностью предсказывать, какую роль они будут играть в расширении калийной промышленности.

Германия больше не сможет поддерживать мировую монополию на рынке калийных солей. Переход контроля над важными ресурсами в Эльзасе от Германии к Франции предвещает конкуренцию со стороны признанных адекватных источников снабжения. Существует много других возможностей, одни лишь потенциальные возможности которых достаточны, чтобы сдержать любую тенденцию к необоснованному вымогательству со стороны тех, кто контролирует германские месторождения. Более того, внимание было настолько направлено на желательность развития независимых источников, и так много способных технических талантов сейчас посвящается тому, чтобы привести к успешному результату многие предпринимаемые начинания, что очень маловероятно, что эта страна или любая другая будет в будущем зависеть от одной или двух произвольно управляемых монополий.

ГЛАВА XXVII. АЗОТ. Автор: Честер Г. Гилберт

ИСПОЛЬЗОВАНИЕ АЗОТА

Растительная жизнь требует азота и получает его в нормальном цикле событий. Но когда возникает необходимость стимулировать рост растительной жизни путем питания, другими словами, путем внесения удобрений в почву, азот в доступной форме становится незаменимым. Далее по каналам снабжения продовольствием он выполняет другую и не менее важную функцию, обеспечивая химическое вещество (аммиак), на котором построена современная практика охлаждения. Точно так же химия взрывчатых веществ — это, по сути, химия соединений азота. И это еще не все, поскольку химические операции в целом — а следовательно, исследования и промышленная химия в целом — включают использование соединений азота. Таков, вкратце, его статус. По каждому из трех основных пунктов — интересы производства продовольствия, распределения продовольствия и национальной обороны — он незаменим; и не менее важным является ряд менее заметных агентов, служащих интересам химии на каждом шагу.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Развитие источников связанного азота обусловлено тремя простыми химическими фактами. Имея в виду эти три простых факта, остальное следует в значительной степени как вопрос вывода. Факты таковы:

Что при всех обычных условиях температуры и давления свободный азот является газом.

Что он чрезвычайно инертен и не склонен участвовать с другими элементами в образовании химических соединений.

Что такие соединения, когда они все же возникают, характерно растворимы.

Вследствие этих трех руководящих принципов, наряду с его связью с органическим веществом, как упоминалось в предыдущем заголовке, азот имеет четыре способа проявления, которые стоит рассматривать как по крайней мере потенциальные источники снабжения.

Атмосферный азот.

— Будучи не склонным участвовать в химических соединениях, азот в ходе мировой эволюции был в значительной степени предоставлен самому себе; и поскольку в свободном состоянии он обычно является газообразным, он обосновался в атмосфере. Таким образом, получается, что атмосфера сегодня примерно на четыре пятых состоит из газообразного азота, и в конечном итоге атмосфера неизбежно будет составлять великий источник, к которому мы должны обращаться за нашими запасами. С источником, столь безгранично вездесущим, вопрос снабжения на первый взгляд кажется достаточно простым. Но атмосферный азот, следует помнить, — это азот несвязанный, а спрос существует не на сам азот, а на азотсодержащие соединения. Однажды в состоянии соединения он может оставаться таковым бесконечно, и форма соединения может быть более или менее легко изменена в соответствии со спросом. Однако прежде чем его можно будет использовать, его нужно побудить отказаться от своей газообразной свободы и закрепиться в каком-либо таком состоянии соединения. Свободный азот должен стать связанным азотом — отсюда термины «связанный азот», «фиксация азота» и тому подобные, находящиеся в общем употреблении. Для этого его нужно побудить сделать то, что он не счел нужным делать по своей собственной воле, и сама черта отчужденности, ответственная за неисчерпаемые ресурсы атмосферного азота, стоит как препятствие, противостоящее их использованию. Препятствие не оказалось непреодолимым, как будет показано позже; но оно является достаточно источником проблем даже по сей день, так что ситуацию со связанным азотом можно с особой уместностью охарактеризовать как отчетливо «висящую в воздухе».

Месторождения нитратных руд.

— Склонность азота обосноваться в атмосфере имеет очевидный результат в минимизации развития минеральных нитратов. Атмосферный азот, однако, не является полностью застойным. Природные процессы постоянно работают, осуществляя существенную фиксацию. Процессы не являются навязчиво энергичными, как в случае с атмосферным кислородом, чьи процессы фиксации составляют вездесущие явления окисления. Тем не менее, различными способами, наиболее заметным среди которых, несомненно, является форма бактериального действия, нитрификация и создание нитратных минералов повсюду в почве тихо продвигаются вперед, и их концентрацию в месторождениях руд более или менее обильного распространения следует, таким образом, ожидать в естественном ходе геологических событий. Пытаясь проследить их дальнейший путь, мы, однако, с самого начала сталкиваемся с принципом растворимости. Нитратные минералы по своей природе являются растворимыми солями. Они выщелачиваются из непосредственной среды, в которой образуются, точно так же, как и растворимые минералы в целом. В основном последние переносятся в растворе в океан, добавляясь к его солености; но при исключительных условиях топографии, где дренаж питает замкнутые бассейны, вода оказывается в ловушке без выхода, кроме как через испарение. Здесь соли накапливаются, концентрируются и, наконец, дают начало месторождениям.

Это, в общих чертах, путь, установленный для растворимых минеральных солей как класса, и именно по этому пути мы должны ожидать проследить развитие месторождений нитратных руд. Но океан с его 3,5-процентной соленостью имеет лишь следы нитратных минералов; то же самое верно и для вод замкнутых бассейнов на всех различных стадиях концентрации. Их растворимость такова, что они не могли избежать существенной формы по пути. Можно сделать только один вывод. Очевидно, присущая черта отчужденности не теряется азотом, когда он все же соединяется. Соединения не выживают в течение какого-либо длительного времени, но подвергаются диссоциации, высвобождая свой азот и возвращая его в атмосферу, даже когда другие процессы медленно извлекают его из атмосферы.

С этим вечный цикл для азота замыкается, и замыкается без видимого обеспечения какого-либо значительного отвода, который потребовался бы при создании месторождений руд. Столько о правиле; теперь об исключениях: в основном они имеют второстепенное значение. Карманообразные обогащения в почве обычны. Накопления имеют тенденцию образовываться в пещерах и могут даже вырасти до значительных размеров в небольшом масштабе, как во время Гражданской войны, когда они существенно помогли облегчить азотные проблемы блокированной Конфедерации. В засушливой местности они также нередко приобретают достаточную известность, чтобы представлять интерес, особенно в руках промоутера. Наконец, существуют чилийские нитратные поля, которые, будучи далеко не второстепенными, переходят в другую крайность, обслуживая потребности всего мира.

Эти проявления, особенно последнее названное, послужили поддержанию надежды на то, что другие, имеющие экономическое значение, ждут своего открытия. Чилийские месторождения единственные среди всех заслуживают большего, чем мимолетного внимания. Происхождение этих месторождений окутано неопределенностью. Почему или как природные силы, которые в других местах, как предмет всеобщего наблюдения, противостояли как образованию азотных солей, так и накоплению тех, которые все же умудряются образоваться, должны были потерпеть неудачу в этом конкретном случае, остается полностью гипотетическим. Убедительное объяснение имело бы величайшую ценность при определении вероятности подобных проявлений в других местах. Но ничего не было предложено, и ничего нельзя выиграть для нынешней цели, останавливаясь, чтобы исследовать правдоподобность различных попыток, которые были предприняты. Перед нами, с одной стороны, свидетельства установленного азотного цикла, по-видимому, не дающего никакой видимой лазейки для накопления обширных месторождений; с другой стороны, стоит голый факт огромного отложения. Этот факт существования, несомненно, несет в себе возможность дублирования в других местах. Однако факт проявления лишь предполагает возможность, но не определяет шансы на повторение. Они записаны в распространенности условий, необходимых для обширного отложения. В случае с азотом они уникальны сверх всякого понимания, и перспектива повторения в точно такой же степени маловероятна. Соответственно, для всех практических целей обзор мировых месторождений нитратных руд, как реальных, так и потенциальных, сводится к обзору чилийского проявления.

Чилийские нитратные поля лежат в засушливой долине бассейна к востоку от высокого берегового хребта и чуть южнее нынешней пограничной линии с Перу. Они не встречаются как единая обширная область отложения, а как месторождения, разбросанные здесь и там вдоль пустынной земли у подножия горных склонов. Формация состоит из конгломерата или брекчии горного материала с прилегающих склонов, сцементированного смесью растворимых солей, в которой доминирующим членом является хлорид натрия, поваренная соль, а нитрат натрия занимает второе место. Формация называется каличе. Она залегает по большей части чуть ниже поверхности земли и варьируется от нескольких футов до многих футов в толщину. Только в разбросанных участках каличе достаточно высока по содержанию нитрата натрия, чтобы оправдать обработку. Эти участки разыскиваются и раскапываются, а отобранная руда загружается в тележки, которые перевозят ее на экстракционный завод для обработки. Здесь растворимые соли в целом извлекаются в растворе, а нитрат, в свою очередь, отделяется от других солей путем кристаллизации. Помимо перевозки, повсюду используется ручной труд.

Каличе, рассматриваемая как стоящая обработки, содержит не менее 10 процентов нитрата и варьируется до 25 процентов и более, со средним значением около 18 процентов. Продукт, поступающий на рынок, бывает двух общих сортов — обычный, указанный как 95-процентный нитрат, и очищенный, гарантированный 96-процентный нитрат, с низким содержанием хлорида натрия. Месторождения разрабатывались более или менее последовательно, с постоянно растущим объемом добычи, примерно с 1830 года. Их важность в схеме снабжения азотом можно понять из рисунков 16–18.

Органический азот.

— Еще один источник связанного азота вырастает из его связи с жизненными процессами и является следствием самых требований организованного общества, которые ранее он призван был помогать удовлетворять. Другими словами, связанный азот участвует в материальном цикле жизни. Он входит в материальные потребности жизни в пище и отдается среди материальных отходов, доступных для поглощения. Все виды остатков, как животных, так и растительных, дают по крайней мере потенциальный источник снабжения связанным азотом. Некоторые из них находятся в эксплуатации; другие по той или иной причине — нет. Среди тех, что в первом классе, выделяются экскременты животных, так называемый танках из заводов по переработке животных, отходы скотобоен, рыбная мука и отходы нефтеперерабатывающих заводов растительных продуктов. Наиболее заметными среди тех, что все еще в значительной степени потенциальны, являются канализация и утилизация мусора.

Азот из этих органических источников не появляется на рынке как таковой. Вместо этого продукты входят в массе в состав удобрений. Они имеют разнообразный характер, и только часть того, что вносится, собирается, чтобы пройти через промышленные каналы, где его поток может быть измерен. Промышленный поток фиксируется, и записи доступны, но даже здесь содержание азота никогда систематически не вычислялось, поэтому запись неадекватна. Что касается остального, той части, которая не достигает каналов промышленности, нет абсолютно никаких данных, на которые можно было бы опереться. В целом, таким образом, значение ресурсов органического азота в значительной степени гипотетично. Это прискорбно. Приблизительные цифры, охватывающие использование органического азота, были бы ценны в различных связях, как в интересах разумного распределения во времена нехватки азота, как помощь в определении степени, в которой растущие требования сельского хозяйства, связанные с ростом населения, могут быть дисконтированы из-за последующего расширения возможностей сбора отходов, или как предоставление основы для оценки весьма значительного влияния моторизации на увеличение спроса на химически приготовленные удобрения.

В нынешнем положении все такие вопросы взаимосвязи ведут только к бесплодным спекуляциям. Даже относительная важность органических источников в целом в экономике снабжения азотом неопределенна. То, что они могут предложить из неразработанных запасов, принимающих сейчас форму расточительной санитарной процедуры, будет рассмотрено позже. При существующих условиях, вероятно, справедливо предположить, что 40–50 процентов азота, обычно используемого в Соединенных Штатах, органически связано.

Карбониферные месторождения.

— Азот в своих органических связях связан с углеродом, из которого в значительной степени состоит органическое вещество, и связь между ними полностью разрывается только тогда, когда сам углерод теряет свою материальную форму через окисление. Вследствие этого прочного союза азот характерно присутствует в карбониферных месторождениях, форма проявления, дающая начало еще одному, четвертому типу азотного ресурса. Уголь и нефтеносные сланцы вырисовываются как выдающиеся представители этого класса. В каждом из них содержание азота варьируется, но составляет 1 процент или более. При столь низком проценте азота само собой разумеется, что ни один из них не следует рассматривать как возможный источник прямого снабжения. Стоимость была бы запретительной даже под давлением самой крайней чрезвычайной ситуации. Азот в угольном пласте или формации нефтеносных сланцев так же бесполезен, как железо в любой обычной породе. Но уголь имеет другие применения, как и нефтеносные сланцы, или, по крайней мере, скоро будет иметь. Азот не нужно извлекать; он высвобождается попутно, и когда его высвобождение осуществляется при условиях, которые предотвращают его утечку, результатом является продуктивный азотный ресурс. Азот из этого типа ресурса находится в форме аммиака, относительная важность которого показана на рисунках 16–18 и в таблице 66.

ОБЩИЕ АСПЕКТЫ КОНТРОЛЯ

Такова природа азотных ресурсов. Ситуация с ресурсами в целом представлена графически на рисунке 15. Ни один другой не может сравниться с ним по всеохватности. Его источники — животные, растительные, минеральные и атмосферные, что означает универсальные; и из этого беспрецедентного разнообразия выросло промышленное развитие, столь же сложное, сколь и диверсифицированное, и, кстати, ввиду его влияния на снабжение продовольствием и боеприпасами, столь же важное, сколь и сложное. Ситуацию в лучшем случае можно понять лишь несовершенно, ибо она была недостаточно изучена. Нарушая все установленные правила проявления ресурсов, она нарушает пределы, установленные для организованного расследования. Геологи изучили одну фазу ситуации, электрохимики — другую, эксперты по санитарии — третью и так далее; а различные вовлеченные коммерческие интересы позаботились о том, чтобы дать гласность там, где гласность принесла бы наибольшую пользу.

Таблица 66. — Статистика производства азота

Year | Organic nitrogen | Chemical nitrogen
Dried blood; tankage; guano; fish scrap; cotton seed cake and meal; etc. | Sodium nitrate | Fixation compounds | By-product ammonium sulphate
World’s production, tons | Domestic production, tons | Imports, tons | World’s production | Domestic production, tons | Imports, tons | World’s production, tons | Domestic production, tons | Imports, tons

Ammon.
sulph.
(Haber),
tons
Calcium
nitrate
(Arc),
tons
Cyanamid,
tons

1900 | Data for organic nitrogen indefinite, but probably about equal to the total for chemical nitrogen. | ... | ... | ... | ... | ... | ... | ... | ... |   540,000 |    27,600 |     8,411
1901 | 1,328,664 | ... |   203,960 | ... | ... | ... | ... | ... |   580,000 |    29,279 |    14,486
1902 | 1,349,300 | ... |   205,245 | ... | ... | ... | ... | ... |   600,000 |    36,124 |    18,146
1903 | 1,485,279 | ... |   272,947 | ... | ... | ... | ... | ... |   640,000 |    41,873 |    16,777
1904 | 1,559,091 | ... |   228,012 | ... | ... | ... | ... | ... |   650,000 |    54,664 |    16,667
1905 | 1,754,605 | ... |   321,231 | ... | ... | ... | ... | ... |   694,575 |    65,296 |    15,288
1906 | 1,800,500 | ... |   372,222 | ... | ... |       386 | ... | ... |   778,365 |    75,000 |     9,182
1907 | 1,846,036 | ... |   364,610 | ... | ... |     1,874 | ... | ... |   906,255 |    99,300 |    30,114
1908 | 1,970,974 | ... |   310,713 | ... | ... |     2,767 | ... | ... |   970,200 |    83,400 |    38,238
1909 | 2,110,961 | ... |   428,429 | ... |    45,450 |    12,734 | ... | ... |   987,840 |   106,500 |    42,914
1910 | 2,465,415 | ... |   529,172 | ... | ... |    22,596 | ... |       764 | 1,104,705 |   116,000 |    92,342
1911 | 2,521,023 | ... |   544,878 | ... | ... |    59,479 | ... |     5,617 | 1,206,135 |   127,000 |    94,633
1912 | 2,585,850 | ... |   486,352 | ... | ... |   115,688 | ... |     7,134 | 1,356,075 |   165,000 |    59,542
1913 | 2,772,254 | ... |   625,862 |    20,000 |   181,800 |   173,026 | ... |    14,656 | 1,532,475 |   195,000 |    65,775
1914 | 2,463,356 | ... |   541,715 |    60,000 | ... |   208,070 | ... |    29,536 | 1,320,000 |   183,000 |    75,010
1915 | 1,755,291 | ... |   772,190 |   150,000 | ... |   845,388 | ... |    20,564 | 1,690,000 |   249,000 |    36,370
1916 | 2,912,893 | ... | 1,218,423 |   300,000 | ... | 1,053,439 | ... |    38,023 | 2,000,000 |   285,000 |    12,962
1917 | 2,950,000 | ... | 1,555,839 |   500,000 |   300,000 |   954,765 | ... |    44,146 | ... |   325,000 |
1918 | 2,900,000 | ... | 1,845,192 | ... | ... | ... | ... |    43,070 |  |  |

Рис. 15. — Источники азота и циклы его использования.

Рис. 16. — Развитие производства азота в военное время. Цифры указаны в тысячах тонн.

Однако исследование, основанное только на геологии, не способно справиться с ситуацией; так же, как и исследование, основанное только на технологии, органической химии или бактериологии; или же исследование, готовое использовать любые или все эти средства, но лишь для достижения какой-то частной цели. И снова, разноголосица множества преследуемых интересов не создает шума, из которого можно было бы извлечь адекватное понимание. Ситуация с азотом рассматривалась неадекватно, потому что она неадекватно изучалась. Ее изучали по частям, всегда с помощью ограниченных средств или с какой-то особой целью. Это не ряд технических проблем в геологии, бактериологии, фиксации, снабжении боеприпасами и тому подобном. Это вопрос сложной экономической структуры, создаваемой для обеспечения зависимости общества как в мирное, так и в военное время. Пока ситуация не будет рассматриваться как таковая, ее потребности неизбежно будут удовлетворяться неадекватно, а контроль над ней останется делом опасной неопределенности. Настоящее обсуждение не претендует на устранение этого недостатка или на что-либо большее, чем демонстрация степени его существования.

Рисунок 15 призван показать не столько масштаб ресурсов, сколько их совокупное функционирование в системе азотного снабжения. Влияние географии на контроль над столь повсеместно доступными ресурсами неизбежно будет второстепенным. Правда, это позволяет Чили осуществлять монопольный контроль над поставками минеральных нитратов, но оставляет путь открытым для развития других источников; и, признавая полноту нашей зависимости, как показано на рисунках 16–18 и в таблице 66, мы не должны упускать из виду тот факт, что это происходит не по необходимости, а потому, что мы довольствовались таким положением, вместо того чтобы предпринять попытки развить собственные запасы. Так же обстоит дело и с политическим контролем; то, что выигрывается в одном направлении, по крайней мере потенциально, компенсируется возможностями, открывающимися в других. Контроль над морем дает контроль над поставками минеральных нитратов, столь же абсолютный, как и территориальная монополия Чили. Тем не менее в недавней великой войне Германия, чье судоходство было уничтожено в самом начале, не была вынуждена существенно страдать от нехватки азота. Господство Британии на море оказалось тщетным. В годы перед войной сила, призванная в свое время осуществлять контроль над поставками нитратов, служила лишь стимулом для развития внутренних потенциальных возможностей, в результате чего, когда наступило испытание, оборудование Германии на деле оказалось более эффективным.

Так оно и идет. Контроль над самими азотными ресурсами невозможен. Они слишком повсеместно доступны. Их единственная подверженность контролю заключается в формировании их развития. Это слишком важный вопрос, чтобы безнаказанно игнорировать его и оставлять развиваться без руководства. Современная нация, которая поступает так, навлекает на себя неотвратимую катастрофу нации, находящейся в состоянии войны, но лишенной средств не только для ведения войны, но и для поддержания продовольственного снабжения. Из рисунка 16 можно судить о качестве внимания, уделяемого вопросу внутренних поставок различными странами непосредственно перед войной и во время нее. Германия, как можно заметить, прислушалась к призыву уделить этому вопросу особое внимание еще до войны и имела готовую независимую систему снабжения, опирающуюся на азот из атмосферы и продуктов переработки угля, с результатами, которые уже были зафиксированы. Великобритания не игнорировала важность азота, но полагалась на свое господство на море и почти не уделяла внимания формированию курса развития. Не осталась незамеченной его важность и в других странах за рубежом, и плацдарм, завоеванный для фиксации во Франции, Италии, Австрии, России и Японии, можно с уверенностью сказать, был не совсем автоматическим. Соединенные Штаты были единственной среди великих держав, которая до начала военных действий в Европе в 1914 году пренебрегла принятием каких-либо особых мер предосторожности.

Рис. 17. — Развитие азотной промышленности в Соединенных Штатах. 1. Расширение мощностей в военное время для производства боеприпасов. 2. Сфера конкурентных возможностей для чилийской селитры, фиксации атмосферного азота, усовершенствованных методов использования угольного топлива, аммиака из сланцевой нефти, бактериальной фиксации, улучшения санитарии и т. д. 3. Сфера возможностей, зарезервированная для коксохимического производства. 4. Развитие, намеченное для коксохимического производства.

Рис. 18. — Развитие азотной промышленности в мире, 1900–1918 гг.

Война, когда она началась, далеко превзошла все ожидания по своим масштабам, и, как следствие, возрос спрос на специально разработанные азотные ресурсы. Чтобы справиться с чрезвычайной ситуацией, часть азота можно было отвлечь из сельскохозяйственных каналов, но это было далеко не то, что требовалось, поскольку продовольствие было столь же важно, как и боеприпасы. Органические источники не предложили никакой помощи. Скорее, они были помехой; ибо органический азот, говоря в широком смысле, является побочным продуктом санитарии и как таковой развивается как результат достижений цивилизации. Был заметный отклик со стороны каменноугольных источников, но их нельзя было заставить удовлетворить чрезвычайную потребность, поскольку, будучи побочными продуктами, их объем определяется не спросом на азот, а спросом на основные продукты. Зависимость от природного минерального источника в Чили была исключена или, по крайней мере, была ненадежной для любой страны, кроме Великобритании. Соответственно, из четырех великих источников именно атмосферному азоту предстояло справиться с чрезвычайной ситуацией. Таким образом, война, решительно выдвинув азотную проблему на первый план, передала практически всю тяжесть своего огромного импульса развитию в одном направлении — фиксации. Результат показан на рисунке 18.

Встревоженные кошмаром войны в 1914 году, даже Соединенные Штаты осознали опасности, если не реальные потребности внутренней ситуации. Поразительным и весьма значимым фактом является то, что, несмотря на фундаментальную важность азота, пробуждение застало нас абсолютно без какой-либо сформулированной программы действий, даже военной или сельскохозяйственной, не говоря уже о чем-то всеобъемлющего экономического масштаба. Последовала истерическая попытка импровизировать программу. Мы еще не вступили в войну, и общественный интерес был лишь доведен до доверчивой стадии. Возможность личной наживы на государственных милостях была слишком многообещающей, чтобы ее упустить. Единственная открывающаяся перспектива лежала в направлении развития фиксации, а фиксация в руках промоутера — одно из самых привлекательных предложений, которые только можно себе представить. Ее основные требования — азот и энергия. Поскольку первый неисчерпаемо присутствует в воздухе, а вторая неисчерпаемо доступна в растрачиваемых водных ресурсах страны, казалось бы, ничто не могло сулить больших перспектив. Добавьте к этому соображение, что дешевый азот означает дешевые удобрения, а дешевые удобрения означают снижение стоимости продуктов питания, и предложение, транслируемое по всей стране, готово. Из путаницы интересов — общественных, политических и частных — после нашего вступления в войну наконец была разработана программа, призывающая к строительству ряда заводов по фиксации с совокупной производственной мощностью около 85 000 тонн связанного азота в год. На данный момент достаточно сказать, что война закончилась до того, как любой из них достиг стадии производства, и Соединенные Штаты, как и Великобритания, зависели от импорта.

Графики, составляющие рисунок 16, показывают влияние войны на развитие азотной промышленности в распределении по соответствующим странам. Скандинавские разработки, хотя и были продиктованы сугубо коммерческими мотивами, находились под таким сильным влиянием политически стимулируемого рынка, что их вполне можно включить в этот общий класс политически контролируемых разработок. То же самое верно и для нейтральных стран в целом. Рисунок 18, основанный на наилучшей доступной информации, призван выявить коллективное влияние войны на вклад в мировые запасы. Органический азот не учитывается как потому, что он связан со слишком многими неопределенностями, так и потому, что акцент в военное время был сделан исключительно на химический азот. Этот рисунок учитывает только фактическое производство и оставляет в стороне то, что находилось в процессе строительства, когда война закончилась. Соответственно, хотя в одном отношении он переоценивает эффект войны, включая чисто коммерческие операции, которые вполне могли произойти и без нее, в другом он недооценивает ситуацию, игнорируя такие разработки, как в нашей стране. Лучшее, что можно сделать, — это считать, что они уравновешивают друг друга, что, учитывая все обстоятельства, вероятно, достаточно справедливо для всех практических целей. Исходя из этого, можно заметить, что чистый эффект войны заключался в увеличении производства связанного азота примерно на 40–50 процентов по сравнению с цифрами, указанными для нормального темпа роста.

Так оно и идет. Таким образом, нехватка военного времени была восполнена; но все это история. Теперь, когда война окончена, возникает вопрос, предстоит ли миру столкнуться с обратной ситуацией. Готовясь к войне и, наконец, удовлетворяя ее требования, не создал ли мир 50-процентное перепроизводство сверх потребностей мирного времени? На первый взгляд, ответ кажется утвердительным, но это не тот вопрос, на который можно ответить с ходу. Сельское хозяйство способно поглотить неопределенное количество азота, и война вызвала длительные изменения в сельскохозяйственной ситуации. Изменившиеся сельскохозяйственные условия создают возможности для значительной, возможно, для всей, прибавки к производству азота. Однако развитие не может поддерживаться на нынешней произвольной преференциальной основе политической целесообразности. Меньше всего оно может поддерживаться на этой основе в нашей стране. Обычно мы не мыслим и не можем быть заставлены мыслить категориями войны. Причина достаточно очевидна, и ее повторяющаяся сила уже заметна. Как бы неприятен ни был этот факт в некоторых крайностях его применения, единственный рациональный подход — принять его и сформировать наши меры экономической готовности так, чтобы нормальная деятельность мирного времени поддерживала наши экономические силы в тонусе и в готовности к испытанию войной. Еще до войны было признано, что без гарантированного источника азотного снабжения наша система обороны была пустой; но нам не удалось создать никаких средств снабжения в непосредственном ответ на политические нужды. Нам удалось неплохо начать во время войны, но еще предстоит увидеть, в какой степени это искусственно подпитываемое развитие способно выдержать предстоящую ожесточенную конкурентную борьбу.

КОММЕРЧЕСКИЕ АСПЕКТЫ КОНТРОЛЯ НАД АЗОТОМ

Свободный азот, как мы помним, не имеет экономического значения. Чтобы быть доступным для промышленного использования, он должен находиться в состоянии химического соединения. Форма соединения имеет второстепенное значение, поскольку она может быть более или менее легко изменена в соответствии с потребностями, но его ценность обусловлена его доступностью в виде азотных соединений. В результате различные источники промышленно классифицируются по трем направлениям:

Природные соединения — азот, встречающийся в природе в виде товарных соединений.

Побочные соединения — азот, становящийся доступным попутно в ходе операций, направленных на другие цели.

Соединения фиксации — азот, доступность которого зависит от специальной обработки фиксации.

Природные соединения.

— Чилийская селитра является выдающимся представителем природных соединений. Гуановая промышленность, или то, что от нее осталось, и несколько других мелких производств из органических источников также относятся сюда, но их совокупный объем выпуска настолько относительно мал, что чилийская промышленность представляет собой не что иное, как монополию на природные ресурсы. Однако она не управляется как таковая, а находится в руках частного капитала, который владеет и управляет офисинами (заводами), выплачивая чилийскому правительству роялти или экспортный налог в размере около 11,20 доллара за тонну. Британские и чилийские интересы делят примерно поровну большую часть инвестированного капитала. Остальная часть в значительной степени принадлежит немцам и американцам. Общая капитализация в 1909 году составляла примерно 134 000 000 долларов, что представляло фактическую оценку около 30 000 000 долларов. Различные попытки со стороны вовлеченных коммерческих интересов осуществить объединения с целью стабилизации производства предпринимались, но не были полностью успешными, и общая тенденция все время была направлена в сторону перепроизводства.

Операции, как уже было описано на странице 424, являются примитивными, и стоимость производства соответственно высока, составляя около 25–30 долларов за тонну в порту, включая экспортный налог в 11 долларов. Селитра реализуется в основном через комиссионные дома. Американская ситуация находится в основном в руках трех компаний: W. R. Grace & Co., E. I. du Pont de Nemours Powder Co. и Wessel, Duval & Co. Масштабы чилийской промышленности в целом и ее относительная важность показаны на рисунках 16–18 и в таблице 66.

Побочные соединения.

— К этому классу соединений относятся, за немногими незначительными исключениями, уже отмеченными, азотистые продукты органического происхождения в целом, а также продукты из каменноугольных источников, таких как уголь и горючие сланцы. Из первых поступает множество органических отходов, образующихся в результате деятельности, связанной с продуктами животного, растительного и рыбного происхождения, и содержащих азот в форме органических аммиакатов, обычно оставляемых в таком виде для использования в сельском хозяйстве. Из последних извлекаемый азот является полностью химическим азотом в форме аммиака или солей аммония, в основном сульфата аммония, и доступен для всех видов использования.

Органическое производство невозможно проанализировать с какой-либо определенной точки зрения. Отсутствие систематически составленных записей, а за этим — разнородный, в значительной степени децентрализованный характер выпуска, наряду с тем фактом, что производственные затраты по большей части неразличимы, оставляет слишком много места для воображения. Большая часть поставок происходит из связей с санитарией, особенно местной санитарией, такой как сельская практика, для которой нет никаких измерений. Другим важным источником поставок является так называемый танках (отходы переработки животных), отходы от заводов по переработке животных; но и здесь вопрос теряется в разбросанности производства, неопределенности состава и в том факте, что не весь продукт используется как источник азота, часть его идет на приготовление кормов для животных. То же самое верно для хлопчатникового шрота и различных других менее заметных форм органических отходов, возникающих в результате промышленной деятельности. Рыбная мука и отходы скотобоен от мясопереработки также вносят заметный и в то же время более определенный вклад в поставки сельскохозяйственного азота; но даже здесь адекватные цифры недоступны. Федеральная торговая комиссия предприняла попытку проанализировать потребление 1913 года, результаты которой приведены в следующей таблице:

Оценочное потребление азота в коммерческих удобрениях за 1913 год

Materials | Fertilizing substance | Consumption (tons) | Content (per cent.) | Units consumed [157]
Nitrate of soda | Ammonia | 260,000 | 18.0 |  4,680,000
Sulphate of ammonia | Ammonia | 130,000 | 25.0 |  3,250,000
Cyanamid | Ammonia |  15,488 | 18.0 |    278,784
High-grade tankage | Ammonia | 210,000 | 10.5 |  2,205,000
Concentrated | Ammonia |  18,351 | 14.5 |    266,090
Dried blood | Ammonia |  40,000 | 17.0 |    680,000
Dried fish scrap | Ammonia |  50,000 | 11.0 |    550,000
Cottonseed meal | Ammonia | 660,000 |  7.5 |    950,000
Total | ... | ... | ... | 16,859,874

[157] Единица — это 1 процент от тонны, или 20 фунтов.

Эта оценка, однако, учитывает только более строго промышленные источники, оставляя сельскую санитарию и тому подобное вне расчетов.

Помимо переработки органических аммиакатов, которая практикуется в больших масштабах лишь в нескольких случаях, в частности в парижской системе канализации, четыре общих типа промышленных операций более или менее фигурируют в производстве побочного аммиака. Они включают перегонку угля, карбонизацию костей, перегонку горючих сланцев и доменные операции. Американское производство, однако, полностью происходит из первых двух типов. Оба других являются активными производителями за рубежом, особенно в Шотландии, но ни один из них еще не получил распространения в этой стране. Американское извлечение в связи с карбонизацией костей имеет второстепенное значение. Практически весь объем поставок поступает от газовых заводов и операций по производству побочного кокса. Рисунок 17, в заштрихованной области с обозначением «производство сульфата аммония», показывает масштаб и тенденцию производства из года в год с 1900 года.

Органический азот, извлекаемый во всех различных побочных связях вместе взятых, вероятно, составляет 40–50 процентов от общего объема поставок. Аммиак из продуктов переработки угля в этой стране добавляет еще 12–15 процентов. Таким образом, более половины наших поставок приходится на побочные продукты. Внутренний выпуск дополняется в случае органической формы значительным импортом из Южной Америки, и, пока не вмешалась война, небольшие количества сульфата аммония ежегодно импортировались из Европы. По сути, однако, поставки побочных продуктов имеют внутреннее происхождение. Несмотря на свои масштабы, они занимают аномальное положение в промышленности. Они извлекаются попутно, ради того, что они стоят, и продаются за то, что за них можно получить. Стоимость производства в значительной степени списывается на основные операции, с которыми связано их извлечение, а доходы зачисляются в соответствии с этим как экономия на стоимости основных операций. Это одинаково верно независимо от того, идет ли речь о домашнем животном на ферме, коксовой печи или мясокомбинате.

Промышленный выпуск строится как следствие промышленной концентрации. Это подтверждается по всей линии, особенно в выпуске аммиака из коксовых печей в сталелитейной промышленности и в выпуске органических аммиакатов в мясоперерабатывающей промышленности. Именно это влияние скоординированной промышленной концентрации, наряду с потребностью в основных операциях, контролирует поставки побочного азота; поэтому развитие и обработка промышленного выпуска естественным образом оказываются в значительной степени в руках торговых объединений. Таким образом, ситуация с аммиаком из продуктов переработки угля в значительной степени находится в распоряжении Barrett Co., танках и другие аммиакаты животного происхождения собираются для реализации в руках мясоперерабатывающих интересов, а азотные удобрения из семян хлопчатника по большей части подготавливаются и реализуются интересами, дочерними по отношению к Cotton Oil Co.

Вовлеченные производственные интересы занимаются прежде всего производством не азотных продуктов. Извлеченный побочный азот должен конкурировать за свой рынок с тем, что поступает из двух других промышленных классов поставок, и его цена опускается ровно настолько, чтобы позволить ему это делать. Пределы, установленные случайным характером выпуска, не оставляют особого стимула для дальнейшего ценового соревнования. Любая дополнительная широта преимуществ в отношении стоимости производства, которой он обладает, идет не на содействие дальнейшему снижению цены на азот, а на снижение затрат в отношении основной темы производства. Газовый аммиак, например, влияет на рынок азота не столько, сколько на стоимость газа, а органические аммиакаты, извлеченные в связи с мясопереработкой, не столько снизили стоимость удобрений, сколько сдержали стоимость мяса для потребителя. Таким образом, класс побочных поставок, хотя и является ведущим по масштабам и самым дешевым в производстве, мало влияет на определение цены на азот. Продажная цена побочного азота определяется ценой, которую приносит продукт из конкурирующих источников. В этой стране она контролируется ценой чилийской селитры, а не, как обычно приписывают, торговыми объединениями, которые развивают и обрабатывают выпуск.

Соединения фиксации.

— Азот имеет пять общих привычек соединения: с кислородом, порождая азотную кислоту и ее свиту нитратных солей; с водородом, давая аммиак и соли аммония; с углеродом, образуя циан и цианиды; с основными элементами, давая нитриды; и органически, в форме органических аммиакатов. Были выдвинуты различные проекты по использованию их для фиксации атмосферного азота. По большей части они встретили мало или никакого практического успеха, но есть исключения из правила неудачи во всех пяти направлениях.

Прямое окисление — дуговая фиксация.

— Азот окисляется совсем не охотно при любых обычных условиях, но его естественное нежелание соединяться с кислородом может быть преодолено путем пропускания смеси двух газов через электрическую дугу. Атмосфера предоставляет азот и кислород уже смешанными, поэтому все, что нужно в плане сырья, — это обильное снабжение энергией. Дуговая фиксация была разработана в Норвегии, где возможности в плане гидроэлектроэнергии дают лучшие условия, которые можно найти где-либо в мире. Попытки внедрить ее в других местах привели к неудовлетворительным результатам, и дуговая фиксация добилась относительно небольшого прогресса, что можно вывести из таблицы 66 и рисунка 18. Причина двояка. До сих пор использование энергии оказывалось неэкономичным, а продукт — неудовлетворительным. Первое из этих двух возражений зависит от спроса на энергию, но последнее является более решающим. Непосредственным конечным продуктом является азотная кислота, которую трудно транспортировать и которая ограничена в использовании. Чтобы быть готовой к сельскохозяйственному использованию, она должна быть нейтрализована в форме нитратной соли. Известняк — единственный дешевый нейтрализующий агент. Это дает соль, нитрат кальция, который поглощает влагу, слеживается и, таким образом, не подходит для американской сельскохозяйственной практики машинного бурения. Экспериментальный завод недалеко от Сиэтла, штат Вашингтон, стремится преодолеть эту трудность, выпуская свой дуговой продукт в форме нитрата натрия, но проект не имеет коммерческого значения в том виде, в котором он существует.

Аммиачная фиксация.

— Азот не более склонен соединяться по своей воле с водородом, чтобы дать аммиак, чем с кислородом, чтобы дать азотную кислоту. В случае процесса Габера, единственного процесса синтетического аммиака, который выдержал испытание промышленным применением, врожденное нежелание соединяться преодолевается путем подвергания правильно пропорционированной смеси двух газов воздействию тепла и давления в присутствии катализатора. Этот процесс был внедрен в Германии незадолго до начала войны и, как показано на рисунке 16 и в таблице 66, с тех пор неуклонно развивался. Мало что известно об эффективности немецкой практики Габера. По-видимому, для получения результатов необходима тщательная манипуляция. Это означает квалифицированное внимание, которое несовместимо с механическим массовым производством и, таким образом, не подходит для американской практики. То, что стремится быть адаптацией к американским условиям, было разработано General Chemical Co., и завод с номинальной мощностью 60 000 фунтов безводного аммиака в день был спроектирован в Шеффилде, штат Алабама, по инициативе правительства. Завод был завершен, но до того, как его можно было настроить на фактическое производство, война закончилась.

Цианидная фиксация.

— Азот, проходя через раскаленную смесь мелкодисперсной кальцинированной соды, кокса и железа, реагирует с натрием и углеродом, давая цианид натрия. Этот принцип фиксации активно экспериментируется, но не был развит коммерчески, за исключением небольшого завода с номинальной суточной мощностью 10 тонн цианида натрия в Солтвилле, штат Вирджиния.

Цианамидная фиксация.

— Горячий карбид кальция поглощает азот, образуя соединение кальция, углерода и азота по формуле CaCN2, известное как цианамид. Цианамидный процесс, основанный на этой реакции, был широко развит, гораздо больше, чем любой другой из различных процессов, что видно при обращении к рисунку 16 и таблице 66. На первый взгляд, он выглядит наиболее адаптируемым и, следовательно, наиболее многообещающим из всех коммерчески. В этой связи, однако, интересно изучить несколько графиков его роста в воюющих странах, приведенных на рисунке 16. Ни на одном из них показатели не свидетельствуют о сильном, здоровом развитии. Хуже всего обстоит дело в Германии, с контрастом, предлагаемым на графиках Габера и цианамида. До войны производство цианамида не могло получить конкурентоспособную опору в Соединенных Штатах, хотя небольшой завод работал на Ниагарском водопаде в Канаде в течение нескольких лет. Проблема, с которой он столкнулся, аналогична той, что уже была описана для дуговой фиксации, в том, что он сильно зависит от энергии при подготовке необходимого карбида, а стоимость энергии в этой стране была запретительной. Однако под давлением спроса на азот в военное время правительство заключило контракт на строительство трех заводов — одного в Масл-Шолс, штат Алабама, одного недалеко от Толедо, штат Огайо, и одного недалеко от Цинциннати, штат Огайо, с общей номинальной мощностью 220 000 тонн нитрата аммония в год. Работы на всех трех были в самом разгаре, но ни один из заводов не достиг стадии производства, когда подписание перемирия положило конец нитратной деятельности Военного министерства.

Нитридная фиксация.

— Единственный процесс, имеющий некоторую известность и направленный на фиксацию азота в форме нитрида, — это процесс, разработанный Aluminum Company of America. Его рабочий принцип заключается в том, что смесь глинозема и углерода при сильном нагревании поглощает азот, реагируя с образованием нитрида алюминия. Нитрид при нагревании с каустической содой дает конечный продукт в форме чистого аммиака. Выдающаяся трудность, с которой сталкиваются при коммерческом применении этого процесса, по-видимому, заключается в обеспечении печи, способной выдержать температурные требования. Во всяком случае, процесс не преуспел в промышленном отношении.

Бактериальная фиксация.

— Искусственные попытки фиксации были направлены почти исключительно на использование химических принципов. Учитывая возникшие трудности и неопределенную ценность результатов в целом, интересно и, возможно, весьма значимо задуматься о том, что, в конце концов, как показано на рисунке 15, неорганические химические принципы, по-видимому, мало связаны с развитием природных запасов, вероятно, из-за деятельности нитрифицирующих бактерий. Этим возможностям уделялось мало внимания. Это вполне естественно, насколько это касается коммерчески мотивированных исследований, поскольку они не ведут в определенном направлении патентных прав; но неспособность организовать адекватное правительственное расследование можно объяснить только отсутствием понимания масштабов азотной проблемы, как это показано в разделе «Общие аспекты контроля» на страницах 425–433. Предмету было уделено ровно столько внимания, чтобы показать, что бактериальная фиксация представляет собой огромную область грубо игнорируемых возможностей.

НЕДАВНИЕ РАЗРАБОТКИ И ИЗМЕНЕНИЯ В ПРАКТИКЕ

Весь вопрос фиксации должен рассматриваться как находящийся в процессе развития. Правда, он был начат около пятнадцати или двадцати лет назад и вырос до крупнейшего производственного источника химического азота, с операциями практически во всех важных промышленных странах мира и при ответственной финансовой поддержке. Но никто не может изучить графики на рисунке 16, не признав преждевременного, грибовидного качества роста, вызванного прежде всего в ответ на политические условия, ведущие к войне и проходящие через нее. Это особенно верно для американской ситуации. Когда разразилась война, фиксация здесь, по общему признанию, все еще находилась на зависимой стадии своего развития, неспособная в каждой предпринятой попытке стоять самостоятельно в промышленном отношении. В основном, разработки, которые произошли впоследствии, следовали по уже существующим линиям. Поскольку они это делали, им не следует придавать большого фактического экономического значения. Что касается остального, новых разработок, все, что можно сказать на данном этапе, — это то, что они разочаровывающе скудны.

Только одно достижение военного времени, окисление аммиака, выделяется как имеющее несомненно ясную ценность. Азотная ситуация, как мы помним, имеет два аспекта: военный и сельскохозяйственный. Военный фокус сосредоточен на азотной кислоте и наиболее доступных средствах обеспечения поставок; сельскохозяйственный фокус сосредоточен на аммонийных соединениях или их эквиваленте в нейтральных азотных солях и наиболее экономичных средствах снабжения. Здесь, следовательно, происходит расхождение путей к целесообразности, и именно на этом этапе, когда военные влияния вышли на первый план, азотные разработки последних нескольких лет были уведены на неэкономичный путь военного контроля. Бюро горной промышленности, однако, взяв на себя работу других, усовершенствовало простой, эффективный способ окисления аммиака до азотной кислоты. Это, вне всякого сомнения, самый важный вклад дня. Его значение, возможно, лучше всего может быть показано графически на прилагаемом эскизе.

Окисление аммиака, как можно заметить из вышеприведенного эскиза, дает средство обеспечения военных потребностей с прямой линии сельскохозяйственной эффективности. С чисто военной точки зрения, оно имеет возражение в виде окольного пути. Пунктирная линия прямого военного процесса, однако, не имеет функции в мирное время и, следовательно, не может поддерживаться в мирное время в готовности к войне, а должна вместо этого создаваться специально для удовлетворения потребностей военного времени. У нас была иллюстрация того, что это означает в плане времени и денег, и этого одного должно быть достаточно. Сельскохозяйственный канал, однажды построенный на основе экономической эффективности, открыт во все времена. В крайнем случае, все, что требуется, — это следить за чрезвычайными потребностями в плане оборудования для окисления, что является относительно простым делом. Таким образом, вместо ненадежной процедуры доверия к удаче, которая характеризовала наше довоенное отношение к азоту с одной стороны, или попытки невозможного в плане поддержания военной программы промышленного процесса в мирное время с другой, все, что нужно, — это конструктивная программа, посвященная исключительно интересам экономической эффективности.

ПЕРСПЕКТИВЫ АЗОТА

На азот нет импортной пошлины, и вряд ли она будет, ибо азот является важным винтиком в механизме продовольственного снабжения, а акцент мирного времени, меняя порядок военного времени, делается прежде всего на дешевизне и лишь во вторую очередь на месте происхождения. Соответственно, заглядывая вперед, рыночные условия Америки, как только мировая торговля будет полностью восстановлена, должны отражать мировые условия. Как показано на рисунке 18, внезапное окончание войны с отменой военных требований, которые неуклонно росли даже до начала военных действий в 1914 году, оставило мир с производственной мощностью на 30–40 процентов выше нормальной. В какой степени это кажущееся перепроизводство, составляющее около полумиллиона тонн азота, окажется реальным, предсказать невозможно; конечно, не все из него, ибо под стимулом нехватки продовольствия кривая нормального потребления, несомненно, изогнется вверх. С другой стороны, однако, необходимо принять во внимание производственную мощность заводов, еще не введенных в эксплуатацию. Какова бы ни была способность сельского хозяйства поглощать излишки, нельзя ожидать, что оно примет их полностью немедленно или без особого стимула. Из этого следует вывод, что цена и производство снизятся, чтобы стимулировать и скоординироваться с ростом спроса. Где будет точка встречи между кривой спроса вверх и кривой производства вниз, предсказать невозможно. Однако интересно рассмотреть в обзоре, как три типа промышленных источников — природный, побочный и фиксационный — оснащены для совершенно очевидной борьбы конкуренции, подразумеваемой в этой ситуации.

С развитием фиксации появилось множество необоснованных заявлений о том, что дни чилийской селитры проходят. Всякий раз, когда на первый план выходит синтетическая разработка, предаются особому заблуждению в рассуждениях, которое игнорирует факт присущей природной ценности, пренебрегает неизбежной стоимостью ее дублирования и рассматривает синтетическое достижение как дающее «сезам, откройся» к природному сокровищу. В качестве обоснования в случае с азотом, стоимость производства чилийской селитры высока, составляя около 30 долларов за тонну. Этому, однако, в значительной степени способствуют несистематизированная примитивность операций, высокий экспортный налог и перекапитализация. Но это, как можно заметить, переменные факторы, поддающиеся неопределенной модификации в соответствии с потребностью. Чилийская селитра никогда не претендовала на конкуренцию с побочным азотом, с его преимуществами в виде низких сопутствующих производственных затрат и близости к рынку. Расхождение между поставками побочных продуктов и общим спросом на азот все время составляло поле возможностей, открывающееся для чилийской селитры. В этом ее единственный заслуживающий внимания конкурент — индустрия фиксации.

Источники фиксации невозможно проанализировать на определенной основе затрат. Вовлечено слишком много переменных факторов и неопределенностей. Повторяющиеся попытки предпринимались, но все, что они послужили выявить, — это то, что при определенных условиях, как, например, снабжение энергией, и для определенных специальных целей, одна форма проекта имеет очевидный запас преимуществ перед другой, и наоборот для других условий; но что в лучшем случае стоимость производства, если не фактически запретительная, опасно близка к нормальной довоенной цене связанного азота. За всем этим стоит тот факт, что фиксация должна иметь дело с проблемой преодоления природной химической инерции азота, и проблема еще не решена сколько-нибудь убедительно. Всегда выдвигаемое решение требовало некоторой особой меры облегчения от промышленной конкуренции, будь то естественной, как в случае со скандинавским снабжением энергией, или политической, как в случае с американскими и немецкими проектами.

Фиксация широко рекламировалась в последние годы как призванная не только освободить мир от зависимости от чилийского источника, но и существенно снизить стоимость азотных удобрений, следовательно, стоимость производства продуктов питания, к заметному улучшению условий жизни. В своем обещании политического и экономического улучшения в одном, она привлекла внимание всех. Однако заявление об особом экономическом преимуществе, исходящее от отрасли, едва ли, если вообще, способной удовлетворить условия даже в том виде, в котором они есть, было преувеличено.

Это не означает, что фиксацию в испытании конкуренцией ждет только неудача. У нее есть возможности развития в нечто коммерчески и экономически, а также политически стоящее, но существующий тепличный порядок роста, несомненно, должен быть значительно сокращен, и многое из того, что бесполезно, так же определенно должно уйти. Американские разработки имеют особенно неблагоприятную экономическую обстановку в преобладающей шкале затрат. Единственной спасительной альтернативой для них, по-видимому, была бы та или иная форма федерального обеспечения их постоянной поддержки на какой-то такой основе, на которой они были спроектированы, и это маловероятно, ибо нет очевидной причины. Правда, снижение затрат на азот имеет тенденцию к снижению стоимости продуктов питания, но так же, если на то пошло, было бы снижение стоимости сельскохозяйственных орудий, и любые аргументы, которые применимы в случае с азотом, применимы в равной степени для поташа, для фосфатов, для сельскохозяйственных орудий, для угля — фактически для промышленности в целом.

Что касается побочного азота, ситуация совсем иная. В целом, источники побочных продуктов имеют такой порядок, что они не были существенно затронуты войной в ту или иную сторону и, следовательно, не должны быть существенно затронуты в процессе перестройки, за исключением случая аммиака из коксовых печей, где временный спад в сталелитейной промышленности приведет к временному спаду, вероятно, на 15–20 процентов от выпуска 1918 года. Особое значение в связи с тем, что лежит впереди для побочного производства азота, имеет его связь с прогрессом промышленной координации. Вся текущая тенденция индустриализма, представленная в интеграции, массовом производстве и тому подобном, движима интересами координации и преодоления потерь движения; и азот получает важную долю в этих разработках.

Что касается органической группы соединений, перспективы на будущее столь же неопределенны, как и фактические условия сегодняшнего дня. Централизованное развитие мясопереработки, предприятий по переработке животных и хлопкоочистки породило в свое время весьма важные извлечения азотистых отходов; но с прогрессом разработок это использование, в свою очередь, уступает место более продвинутому порядку. Хлопчатник как удобрение уступает место индустрии продуктов из хлопчатника; танках как удобрение уступает место искусственному составлению кормов для животных; лошади, важный вкладчик сельскохозяйственного азота в прошлые времена, уступают большую часть своего места под солнцем автомобильному двигателю. Тем временем, с фактором разбавления, который нужно преодолеть, наша канализация используется для загрязнения рек и уничтожения рыбных запасов, вместо того чтобы быть направленной на полезные цели. Так оно и идет. Разработки ведутся в обоих направлениях, и невозможно сказать, как изменится баланс. Вероятно, лучшее предположение состоит в том, что относительно, по крайней мере, он будет скорее вниз, чем вверх.

Перспективы для побочного аммиака более определенны. Аммиак — это конечная точка материального рафинирования; поэтому здесь азотные разработки сохраняют все, что получают, вместо того чтобы снова терять в дальнейшем рафинировании использования, как в случае с органической группой. Выпуск увеличивался последовательно и быстро благодаря переходу от ульевых к побочным коксовым операциям, к прогрессу централизации и координации; другими словами, в отношении производства кокса. Даже сейчас менее половины коксуемого угля обрабатывается в ретортной печи; но ульевая печь находится вне линии прогресса и должна быть полностью вытеснена. Кроме того, отрасль все еще расширяется по мере того, как процесс перехода, с его отдельной потенциальностью для удвоения текущего выпуска аммиака из продуктов переработки угля, идет вперед.

До сих пор извлечение побочных продуктов в связи с использованием угля ограничивалось одним направлением — производством кокса, наряду с аналогичной процедурой производства газа. Но развитие, которое таким образом началось в коксовой промышленности, на этом не остановится. Потеря движения, возникающая из-за отсутствия координации в использовании угля, столь же велика в других направлениях, как и в производстве кокса, и преимущества интегрального использования могут с уверенностью ожидаться, что проявят себя. Уже проекты такого рода попадают под серьезное рассмотрение в предложениях, таких как поставка газа городам, использование побочных операций, расположенных на шахте, в поддержку убывающего снабжения природным газом, и интегрированные проекты тепла, света и энергии, работающие на угле с извлечением побочных продуктов. Тем временем ситуация с моторным топливом наводит на мысли об интересных разработках впереди. Есть все основания полагать, что нефтяные ресурсы не могут продолжать удовлетворять растущий спрос, фактически, что повод для поддержки уже настал. Какова бы ни была природа этих поддерживающих разработок, принимают ли они форму индустрии сланцевой нефти или что-то еще, кажется определенным, что они откроют важный источник побочного азота.

Рисунок 17 суммирует американскую ситуацию в отношении химического азота, как и рисунок 18 в менее детальном виде — для мира. Органический азот опущен, отчасти из-за недостатка информации, отчасти потому, что проблемы, более непосредственно вовлеченные в ситуацию в том виде, в котором она есть, — это проблемы химического азота.

РЕЗЮМЕ

Азот сам по себе является инертным газом, не имеющим особого применения, но азотистые соединения необходимы для сельского хозяйства, охлаждения, производства боеприпасов и для применений химии в целом. В природном газообразном состоянии он составляет около четырех пятых атмосферы, а в связанном виде встречается как нитратные минералы, как органические соединения и в каменноугольных отложениях. Атмосферный азот полезен только после того, как он был искусственно соединен или зафиксирован, что является предложением, которое природная инертность азота делает трудным и дорогим. Единственные минеральные отложения, имеющие значение, — это те, что составляют нитратные поля северного Чили. Органические ресурсы включают все виды животных и растительных отходов. Аммиак из каменноугольной смолы от ретортно-коксового и газового производства, наряду с некоторым количеством аммиака из сланцевой нефти, составляет практически весь объем поставок, полученных из каменноугольных источников. Этот диапазон ассоциаций, включая животные, растительные, минеральные и атмосферные источники, нарушает все установленные правила возникновения ресурсов и, следовательно, все регулярно проводимые исследования. В результате азотные ресурсы и их потребности во внимании никогда не исследовались всесторонне. Это стало поразительно очевидным, когда война, угрожающая быстрой катастрофой под видом нехватки азота, показала, что мы совершенно лишены какой-либо систематической азотной программы, и спровоцировала истерическую попытку разработать вместо нее импровизированную. Было обнаружено, что атмосфера обеспечивает единственный независимый источник снабжения, доступный по чрезвычайному рейтингу; поэтому, следуя примеру европейских стран, несколько заводов по фиксации атмосферного азота были спроектированы правительственно.

В промышленном отношении азотные источники могут быть классифицированы как природные, побочные и фиксационные. Природные поставки почти полностью представлены в форме нитрата натрия из чилийских нитратных месторождений. Они контролируются и эксплуатируются британским, чилийским, немецким и американским капиталом. Американский импорт в значительной степени обрабатывается тремя компаниями, чья система контроля осуществляется посредством судоходных и складских мощностей.

Побочные источники включают почти весь используемый органический азот, а также азот из угля и горючих сланцев. Поставки регулируются по величине прогрессом промышленной координации посредством централизации при подготовке продуктов животного, растительного и угольного происхождения. Таким образом, развитие и маркетинг побочных поставок имеют естественную тенденцию собираться в промышленные объединения. Это, однако, естественные разработки, а не разработки, искусственно созданные в интересах контроля цен. Цена побочного азота контролируется не торговыми объединениями, а ценой продукта из других источников, что означает ценой чилийской селитры. Помимо этого, преимущества, возникающие в виде низких производственных затрат, идут не полностью на коммерческую прибыль, а на экономию затрат в отношении основного производства, как, например, в случае с аммиаком газовых заводов, который вносит свой главный вклад в снижение цены на газ для потребителя. Быстрое развитие фиксации объясняется в значительной степени политическими влияниями, активированными условиями, ведущими к войне и проходящими через нее. Существует ряд проектов по фиксации азота, но только три имеют какую-либо подлинную меру промышленных достижений на своем счету: дуговая фиксация в Норвегии, синтетическая аммиачная фиксация Габера в Германии и цианамидная фиксация в ряде мест. Три из четырех крупных американских заводов относятся к последнему названному порядку; другой — это проект синтетического аммиака. Все четыре были законтрактованы правительством, и насколько можно сказать, что фиксация получила промышленную опору в Соединенных Штатах, это полностью в ответ на диктат политического контроля.

Вероятно, несколько менее половины потребляемого азота связано органически, и несколько более половины его химически соединено. Практически весь органический азот и около одной четверти химического азота имеют внутреннее побочное происхождение. До сих пор остаток поставлялся из чилийской селитры, дополненной небольшим импортом гуано, животных отходов, побочного аммиака и цианамида из-за рубежа.

Нет очевидной вероятности того, что эта корректировка будет существенно затронута как непосредственный результат разработок в отношении фиксации. Они показали себя имеющими величайшее политическое значение как предоставляющие неограниченный, независимый источник азотного снабжения. Их подлинное экономическое значение на нынешней стадии принудительного расширения, однако, сомнительно. В этой стране, особенно, шкала затрат дает неперспективную обстановку. Побочные источники, вырастающие из централизованной промышленной координации, находятся в соответствии с тенденцией современного индустриализма и могут рассматриваться как обеспечивающие устойчивый рост выхода, особенно если процесс промышленной эволюции в направлении скоординированной экономической эффективности адекватно культивируется, вместо того чтобы ему мешать. В этой же связи наиболее значимое достижение, зафиксированное для азота, заключается в разработке средства для окисления побочного аммиака, тем самым делая растущие побочные поставки доступными для полного спектра азотных применений.

Что касается экономических и политических аспектов перспектив впереди, все остальное затмевается и теряется из виду в насущной потребности в конструктивной программе, разработанной на всеобъемлющей основе, в соответствии с всеобъемлющим характером самих ресурсов, с помощью которой можно заменить неэкономичную импровизированную программу, возникшую в результате войны. Требуемая программа — это та, которая рассчитана на то, чтобы выявить и выявить скоординированно лучшее, что есть в бактериальной, а также химической фиксации, в промышленных побочных источниках органического и химического азота и в области санитарии.

ГЛАВА XXVIII ПИРИТ И СЕРА Автор: А. Г. Уайт

ИСПОЛЬЗОВАНИЕ ПИРИТА И СЕРЫ

Пирит и сера тесно связаны в своих наиболее существенных применениях, и один материал во многих случаях может быть заменен другим. Самое большое и наиболее важное использование этих минералов — в производстве серной кислоты, которая является важным материалом, необходимым для самого широкого спектра целей, включая производство кислого фосфата для удобрений, производство современных взрывчатых веществ большой мощности, переработку нефти, травление железа и стали и для огромного числа химических производств. Конкуренция между пиритом и серой для этой цели прошла через несколько стадий. С развитием итальянских месторождений в больших масштабах сера широко использовалась для производства кислоты. По мере того как цены на серу повышались, стало дешевле использовать пирит, который во многих местностях затем вытеснил серу для этой цели. С быстрым расширением американского производства и, в частности, с огромным увеличением мощности заводов по производству серной кислоты для военных целей, сера снова стала очень широко использоваться для производства кислоты. Перспективы после окончания войны таковы, что из-за огромной мощности серных рудников Соединенных Штатов сера может продолжать конкурировать с пиритом в этом использовании.

Вероятно, вторым по значимости направлением использования этих материалов является производство сульфитной древесной целлюлозы. В Европе для этой цели в основном используется пирит, тогда как в Соединенных Штатах и Канаде основным материалом является сера. При соблюдении оптимальной технологии на каждую тонну произведенной сульфитной целлюлозы требуется около 250 фунтов серы. В Соединенных Штатах и Канаде ежегодно для этой цели расходуется около 175 000 тонн серы, что составляет около 50 процентов от общего потребления серы в этих странах. Существует также ряд других важных областей применения, где используется сера, а не пирит; наиболее значимыми из них являются производство сельскохозяйственных опрыскивателей и инсектицидов, а также вулканизация каучука. Сера является основным компонентом черного пороха, и значительные ее количества до сих пор используются для этой цели. Хотя для производства большинства взрывчатых веществ, применяемых в современной войне, требуется серная кислота, сера в них не используется в элементарной форме. Существует множество других второстепенных химических способов применения.

Заменители серы и пирита.

— Из-за наличия крупных доступных месторождений серы, а также масштабов и широкого распространения месторождений пирита и дешевизны обоих этих материалов, адекватных коммерческих заменителей для них не существует. Увеличение объемов получения побочной кислоты на медеплавильных и цинкоплавильных заводах, а также, возможно, на никелевых заводах в Садбери, можно считать наиболее важными факторами, способствующими вытеснению пирита и серы. В целом, определяющими факторами являются стоимость и транспортировка, а не какой-либо текущий или вероятный дефицит материалов.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ ПИРИТА

Хотя пирит является очень широко распространенным минералом, существует относительно немного месторождений, имеющих достаточное значение для мировой торговли. Это, как правило, связано с относительно низкой стоимостью содержания серы в тонне руды, обычно составляющей от 40 до 45 процентов извлекаемой серы; это означает, что требуется почти 2¹⁄₂ тонны пирита, чтобы соответствовать одной тонне серы, которая конкурирует с ним во многих областях применения. Следовательно, пирит редко перевозится на большие расстояния, если только он не находится в таком месте, где можно воспользоваться дешевыми балластными тарифами при отсутствии других грузов для судов, или если он не содержит значительных примесей меди или золота, которые можно извлечь после использования серы. Многие известные месторождения, например, в Мексике и западной части Соединенных Штатов, остаются неосвоенными из-за удаленности от рынков сбыта. В таких странах, как Россия, Франция, Италия, Германия, Швеция, Япония и восточная часть Соединенных Штатов, добыча поглощается местным рынком. Испания и Португалия, являющиеся важнейшим источником мировых поставок, выгодно расположены для отгрузки в близлежащие европейские страны или для получения дешевых балластных тарифов при отправке в Соединенные Штаты; кроме того, значительная часть руды содержит несколько процентов меди.

Норвегия занимает второе место по экспорту, поставляя высококачественный пирит с содержанием меди, который отправляется в Швецию или через Балтийское море в близлежащие страны. Канада поставляет значительное количество пирита на близлежащие рынки Соединенных Штатов, причем продукт из Квебека содержит медь, а продукт из Онтарио перевозится водным транспортом по Великим озерам.

Испания и Португалия.

— Месторождения Испании и Португалии являются крупнейшими и важнейшими в мире, обеспечивая примерно две трети мировых поставок. Этот район по сути представляет собой единое целое, а основные месторождения залегают в зоне, простирающейся от Рио-Тинто в Испании до Сан-Доминго в Португалии. Совокупная годовая добыча железного и медного колчедана в этих двух странах обычно составляет почти 4 миллиона метрических тонн, 90 процентов из которых приходится на Испанию и 10 процентов — на Португалию. Около двух третей общего объема добычи содержит медь, которую можно извлечь до или после обжига пирита для получения серы. Когда медь извлекается на руднике, руду выщелачивают, раскладывая ее слоями на открытом воздухе и часто перемешивая и смачивая. Медь переходит в раствор и осаждается на железном ломе, образуя цементную медь. Процесс занимает около 3 лет, а остаток пирита отгружается как промытая руда. Руда плотная, мелкокристаллическая и содержит от 48 до 51 процента серы. Консервативные оценки запасов руды в этом районе составляют от 300 до 400 миллионов тонн, чего достаточно для обеспечения добычи в течение ста лет при нынешнем уровне производства. Следовательно, этому району суждено еще долго оставаться главным мировым центром добычи пирита.

Компания Rio Tinto Co. является основным производителем, обеспечивающим около одной трети общего объема добычи во всем районе (Испания-Португалия). Она принадлежит британскому и французскому капиталу. Добыча ведется преимущественно открытым способом, и компания насчитывает 25 000 сотрудников. Руда содержит около 2 процентов меди, что делает эту компанию крупнейшим европейским производителем этого металла. Запасы оцениваются в 250–300 миллионов тонн, что составляет большую часть запасов всего района. Rio Tinto Co. обеспечивает около 60 процентов из 1 000 000 тонн испанского пирита, обычно импортируемого Соединенными Штатами.

Вторым основным производителем является компания Tharsis Sulphur and Copper Mines (британская), на долю которой приходится около одной восьмой общего объема добычи. В районе в целом преобладает британский капитал, остальная часть принадлежит Франции и Испании. Уэльва (Испания) является основным пунктом экспорта, расположенным в 30–40 милях от рудников. В нормальных условиях пирит перевозится по дешевым балластным тарифам и продавался по цене от 6 до 7 долларов за длинную тонну (12–16 центов за единицу серы) с доставкой в порты Соединенных Штатов. Обычно этот испано-португальский район экспортировал одну четверть своей продукции в Соединенные Штаты, одну восьмую — в Англию, одну восьмую — в Голландию, одну восьмую — в Германию, а большую часть остального — во Францию и Бельгию.

Норвегия и Швеция.

— Норвегия производит от 400 до 500 тысяч тонн пирита в год (около 8 процентов от мирового объема), и ее добыча неуклонно растет. Руда обычно содержит от 1 до 3 процентов меди и от 42 до 49 процентов серы и не содержит мышьяка. Семь восьмых продукции экспортируется в Швецию, Германию, Англию и Россию. Когда во время войны импорт серы в Швецию (около 40 000 тонн) был прекращен, она переоборудовала свои целлюлозные заводы для сжигания пирита вместо серы и стала потреблять около половины норвежской продукции, поскольку собственная добыча пирита в Швеции (около 30 000 тонн) имела второстепенное значение.

Норвежские месторождения широко распространены от юга Бергена до самой северной оконечности полуострова. Руда представляет собой преимущественно массивный медьсодержащий пирит, залегающий в виде плоских линз в хлоритовых сланцах в зонах регионального метаморфизма. Около 250 000 тонн добывается в районе Тронхейма, где крупнейшими производителями являются рудники Лёккен компании Orkla Mine Co.

Северный район занимает второе место по значимости с годовой добычей около 150 000 тонн, в основном на руднике Сулитьельма на шведской границе, недалеко от Полярного круга. В восточном районе компания Fodal Copper & Sulphur Co. имеет объем добычи от 75 000 до 100 000 тонн. Норвегия располагает достаточными известными запасами, чтобы обеспечить добычу в течение тридцати лет при нынешнем уровне производства, а вероятно, и гораздо дольше. Крупнейшие запасы находятся в районе Тронхейма. Сообщается также, что Швеция обладает большими запасами, хотя до сих пор они почти не разрабатывались.

Коммерческий контроль над рудниками осуществляется преимущественно английскими и норвежскими интересами. Сообщалось, что рудники с большими запасами недалеко от Нарвика принадлежали германским интересам, но во время войны были выкуплены шведскими интересами.

Франция.

— В течение многих лет Франция производила около 300 000 тонн пирита в год, или около 5 процентов мирового объема. Основные месторождения находятся в Сен-Бель, недалеко от Лиона, в департаменте Рона. Продукт отличается высоким содержанием серы. Известные запасы составляют, вероятно, от десяти до двенадцати миллионов тонн. Продукция используется для внутреннего потребления, а в прошлом дополнялась импортом испанского пирита, а также сицилийской и американской серы.

Италия.

— В дополнение к крупному производству серы Италия добывала значительное количество пирита, который использовался на местах для производства серной кислоты. Добыча пирита составляла около 300 000 тонн до войны и увеличилась до 400 000 тонн в 1916 году, так что Италия производит около 6 процентов мирового объема. Пирит содержит около 45 процентов серы, а небольшая его часть содержит медь. Основная добыча ведется в районе недалеко от Флоренции, хотя ряд более мелких рудников широко разбросан по стране.

Россия.

— Россия обладает крупными месторождениями пирита, расположенными в поясе, параллельном восточному склону Уральских гор. Основной объем добычи обеспечивают Кыштымский и Сысертский районы. Отчеты указывают на высокое качество пирита с большим содержанием серы. Добыча находилась на уровне около 150 000 тонн, или около 2 процентов от мирового объема. До момента экономического коллапса России добыча неуклонно росла, но была ограничена из-за удаленности месторождений от главных центров потребления — Петрограда, Москвы и Одессы. Следует ожидать, что Россия, после того как она восстановит равновесие, продолжит импортировать пирит в значительных объемах, как она делала это в прошлом.

Германия, Австрия и Венгрия.

— Довоенная добыча пирита в Германии составляла от 200 000 до 250 000 тонн в год, или около 4 процентов мирового объема. Около двух третей продукции поступает с месторождений близ Меггена. Содержание серы в пирите оценивается примерно в 43 процента. Сообщается, что во время войны добыча пирита значительно увеличилась, так как Германия импортировала от 800 000 до 1 000 000 тонн пирита. Она продолжала импортировать некоторое количество норвежского пирита, который особенно ценится из-за возможности извлечения из него меди. Германия получает значительное количество серной кислоты в качестве побочного продукта на цинкоплавильных заводах, что помогло восполнить дефицит ее серных ресурсов.

Hungary normally produces about 100,000 tons of pyrite per annum, chiefly from the deposits of Schemnitz.

Кипр.

— Важное месторождение медьсодержащего пирита находится в стадии разработки в старом меднорудном районе на северо-западном побережье Кипра. Сообщается о наличии нескольких миллионов тонн руды с высоким содержанием серы и меди. Разработка ведется в крупных масштабах корпорацией Cyprus Mines Corporation, представляющей американский капитал, и можно ожидать, что она станет важным фактором в экспорте пирита.

Соединенные Штаты.

— Довоенная добыча в Соединенных Штатах составляла около 350 000 длинных тонн, или 6 процентов мирового производства, по сравнению с импортом около 1 000 000 тонн. Около 40 процентов общего объема добывалось в Вирджинии и в основном продавалось для использования на заводах по производству суперфосфата от Мэриленда до Джорджии; около 25 процентов добывалось в Калифорнии и использовалось для местного производства кислоты в окрестностях Сан-Франциско; около 15 процентов добывалось в штате Нью-Йорк; остальная часть была рассредоточена, поступая в качестве побочного продукта с угольных шахт в Огайо, Иллинойсе и Индиане, а также из района добычи цинка в южном Висконсине. Во время войны добыча увеличилась примерно на 50 процентов, но не было сделано открытий, которые обещали бы значительно увеличить постоянную добычу в стране. В целом месторождения не отличаются очень высоким качеством, содержание серы в среднем составляет около 40 процентов. Очень большие запасы пирротина находятся в западной Вирджинии и восточном Теннесси, но они не получили широкого использования. Крупные запасы пирита существуют в Колорадо, Аризоне, Юте и других западных штатах, но они слишком удалены от заводов по производству кислоты, расположенных на Востоке и Юге, чтобы конкурировать. В целом, слабое развитие добычи пирита в Соединенных Штатах объясняется конкуренцией со стороны высококачественного испанского пирита, поступающего в атлантические порты по дешевым балластным тарифам; импортом канадского пирита либо в близлежащие пункты Новой Англии, либо в порты Великих озер; крупным производством дешевой серы в Луизиане и Техасе, которая монополизировала торговлю сульфитной целлюлозой; а также получением побочной кислоты на медеплавильных и цинкоплавильных заводах. Значительный рост производства серы во время и после войны, весьма вероятно, еще больше сократит рынок для пирита. Добыча пирита находится в руках американских компаний, причем несколько более крупных предприятий контролируются фирмами, занимающимися производством кислоты или удобрений.

Канада.

— Добыча пирита в Канаде быстро росла, особенно во время войны, достигнув около 300 000 тонн. Это связано с увеличением экспорта в Соединенные Штаты, главным образом на заводы по производству серной кислоты. Основными районами добычи в Канаде являются: (1) Район в Квебеке, недалеко к северу от границы с Вермонтом, где работают два рудника и имеется ряд перспективных участков. Там имеются большие запасы руды, которая содержит значительное количество меди. Основные рудники контролируются американским капиталом. (2) Район Гудро, расположенный примерно в 40 милях к северу от Су-Сент-Мари, обладает большими запасами руды, но довольно низкого качества. До сих пор основным производителем является американская компания. (3) Район Норт-Пайн недалеко от Грэма, Онтарио, значительно западнее Порт-Артура, является крупным производителем пирита хорошего качества. Основным производителем была дочерняя компания General Chemical Co.

Существуют большие запасы пирротина, оцениваемые примерно в 50 000 000 тонн, многие из которых содержат в среднем более 25 процентов серы, связанные с никелевыми месторождениями Садбери. В настоящее время они не имеют коммерческого значения. В различных частях Британской Колумбии имеются значительные месторождения пирита, но они не имеют коммерческого значения из-за удаленности от доступных рынков сбыта. Большая часть канадской продукции контролируется американскими интересами, главным образом American Chemical Co., штаб-квартира которой находится в Нью-Йорке. Значительная часть канадской продукции импортируется в Соединенные Штаты через Чикаго, Кливленд и Буффало, а также по железной дороге через Вермонт, Бостон и в Нью-Йорк.

Куба.

— Важное пиритовое месторождение разрабатывается примерно в двадцати милях от Сьенфуэгоса, провинция Санта-Клара, Куба. Сообщается, что оно содержит несколько миллионов тонн руды хорошего качества, которая в среднем содержит не менее 40 процентов серы и может содержать извлекаемую медь. Разработка ведется на американский капитал интересами, связанными с Davison Chemical Corporation из Балтимора, штат Мэриленд, которые являются одними из крупнейших производителей серной кислоты на Атлантическом побережье. Это месторождение обещает стать важным близлежащим источником пирита для Соединенных Штатов.

Мексика.

— Известно о существовании важных месторождений пирита в Мексике, но в настоящее время они не имеют коммерческого значения из-за труднодоступности, высоких транспортных тарифов и нестабильной политической обстановки. Сообщается о крупном месторождении примерно в 30 милях вглубь страны в штате Герреро, содержащем несколько миллионов тонн высококачественного пирита с содержанием серы около 48 процентов, не содержащего мышьяка.

Нет никаких перспектив того, что Мексика будет иметь какое-либо непосредственное значение в мировой ситуации с пиритом.

Япония.

— Япония имеет небольшую добычу пирита в объеме от 75 000 до 100 000 тонн в год, или около 1¹⁄₂ процента мирового объема. Большая часть руды содержит медь. Добыча ведется в нескольких разбросанных местах. Государство сохранило за собой право собственности на первоначальные права на недра, а операторы, которым они были сданы в аренду, по-видимому, являются исключительно японцами. Япония потребляет свой пирит для местных нужд, а большую часть своей серы экспортирует.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ СЕРЫ

Италия и Сицилия.

— Италия практически монополизировала мировые поставки серы до 1904 года, когда началось крупномасштабное производство в Соединенных Штатах. Значение серы как мирового минерального ресурса началось с использования пороха в XIV веке. Значительная экспортная торговля развилась рано и приобретала все большее значение с 1830 года. Девяносто процентов итальянской добычи приходилось на остров Сицилия.

Серный район Сицилии представляет собой центральный пояс, пересекающий остров, простирающийся примерно на 100 миль с востока на запад и на 50 миль с севера на юг. Более богатые месторождения разбросаны в виде неправильных линз или чашеобразных тел на этой обширной территории. Месторождения, имеющие коммерческую ценность, относятся к осадочному типу и встречаются в виде пластовых залежей или слоев в известняке, ассоциированных с гипсом и битуминозным мергелем. Обычно имеется три или четыре сероносных слоя, разделенных несколькими футами пустой породы. Средняя мощность серных пластов составляет от 10 до 15 футов, хотя в некоторых местах она достигает нескольких сотен футов. Сера встречается в виде корок, карманов или тонких прослоев, тесно связанных с известняком. Среднее содержание серы в добываемой руде составляет от 20 до 25 процентов, варьируясь от 8 до 50 процентов; а в некоторых местах достигает 90 процентов. Оценки запасов руды сильно разнятся, но, по-видимому, указывают на то, что имеется от 40 до 60 миллионов тонн еще не добытой руды, которая в среднем содержит около 23 процентов серы.

Добыча велась в основном вручную, руду выносили на спинах рабочих. На нескольких рудниках имелись современные подъемные механизмы и вагонетки. Нехватка рабочей силы во время войны способствовала внедрению современных приспособлений на некоторых новых рудниках. С увеличением глубины стоимость добычи возросла до такой степени, что американская сера может конкурировать на европейских рынках.

Методы извлечения серы из руды также были крайне примитивными и расточительными, но за последние несколько лет были установлены более совершенные типы печей, обеспечивающие гораздо более высокий выход за счет улучшенной дистилляции и использования перегретого пара для плавления серы.

Серная промышленность Сицилии служит ярким примером попытки коммерческого контроля, которая переросла в государственный контроль над отраслью. Недавняя история отрасли делится на три периода. Первый охватывает период с 1875 по 1895 год и характеризуется быстрым ростом производства с 200 000 до 400 000 тонн в год при соответствующем снижении продажной цены с 25 долларов за тонну до 12 долларов за тонну. Это был период перепроизводства, обусловленный легкостью ведения добычи на малых глубинах и обилием дешевой рабочей силы. Эти условия привели к созданию большого количества мелких рудников, конкуренция между которыми снизила цены. Второй период, с 1896 по 1906 год, начинается с образования Anglo-Sicilian Sulphur Co., финансируемой английским капиталом, которая заключила пятилетнее соглашение с основными производителями, позже продленное еще на пять лет. Это была прежде всего маркетинговая организация, созданная путем объединения итальянских и английских интересов для контроля производства, стабилизации отрасли и поддержания цен. В конечном итоге она контролировала от 75 до 85 процентов отрасли. Вся сера закупалась примерно по 16 долларов за тонну франко-борт судна, и продажная цена оставалась практически стабильной в течение десятилетнего периода, в среднем составляя от 18 до 19 долларов за тонну. Несмотря на усилия по ограничению производства, годовой объем выпуска достигал 550 000 тонн в течение большей части этого периода. В то же время более высокие цены на серу стимулировали использование пирита в качестве заменителя. Чтобы поддерживать цены в этих условиях, излишки продукции приходилось закупать и складировать, так что к 1906 году на Сицилии накопился запас серы объемом более 500 000 тонн. К концу этого периода началось крупномасштабное производство в Соединенных Штатах (1904 г.). В 1903 году Соединенные Штаты производили менее 10 000 тонн серы и были лучшим клиентом Италии, закупив в том году более 170 000 тонн. В течение трех лет Соединенные Штаты производили более чем достаточно для удовлетворения собственных нужд и накапливали большой резервный запас. Внезапная потеря американского рынка и угроза конкуренции на других рынках вызвали кризис в сицилийской промышленности, который усугублялся большим количеством (30 000) людей, занятых в отрасли. По истечении соглашения с Anglo-Sicilian company (31 июля 1906 г.) итальянское правительство предприняло шаги по контролю над ситуацией. Третий период, с 1906 года по настоящее время, — это период государственного вмешательства и контроля над отраслью. Все производители были обязаны вступить в компанию под названием «Consorzia Obbligatoria per l’Industria Solfiefera Siciliana», организованную в соответствии с законом, принятым итальянским парламентом. Организация управлялась комиссией, назначенной правительством, и имела полный контроль над экспортом и ценами. Вся сера должна была продаваться этой организации по фиксированной цене. Гарантировался минимальный процент на вложенный капитал; были снижены местные тарифы на перевозку серы для экспорта; запасы серы, накопленные Anglo-Sicilian company, были взяты под контроль; и была начата кампания по снижению цен на американском рынке, что привело к снижению продажной цены серы на несколько долларов за тонну. Вскоре было достигнуто рыночное соглашение, и цены восстановились. Ряд мелких рудников закрылся, и был принят закон, контролирующий и ограничивающий предоставление новых концессий. В 1913 году производство снизилось до 350 000 тонн. К началу войны основной производитель в Соединенных Штатах готовился вступить в более активную конкуренцию с итальянской серой, особенно на французских рынках. В результате войны итальянское производство упало до 180 000 тонн в 1917 году, главным образом из-за нехватки рабочей силы; около половины излишков запасов было израсходовано, оставив лишь 160 000 тонн на конец 1917 года; цены выросли так, что рафинированная сера продавалась примерно по 80 долларов за тонну, а низшие сорта — по 55 долларов за тонну франко-борт сицилийских портов. Растущая стоимость добычи серы из-за увеличения глубины шахт и роста затрат на рабочую силу затруднит конкуренцию на европейских рынках с значительно расширившимся производством более дешевого американского продукта.

Сера добывалась в нескольких районах на Апеннинском полуострове, в частности в Романье, Марке, Кампании и Калабрии. Добыча в этих районах в последние годы снижалась и обычно составляла лишь от 25 000 до 30 000 тонн. Содержание серы в рудах варьируется от 20 до 30 процентов. Месторождения имеют ограниченные размеры и разрабатываются на больших глубинах. Продукция в основном использовалась для местных сельскохозяйственных нужд, в препаратах для борьбы с болезнями винограда.

Соединенные Штаты.

— До 1904 года добыча серы в Соединенных Штатах составляла значительно менее 10 000 тонн в год, и основная часть наших потребностей должна была покрываться за счет импорта из Сицилии. С 1904 по 1914 год Соединенные Штаты производили достаточно для собственных нужд, а к концу этого периода поставляли серу в Канаду, начали активно выходить на французский и германский рынки, а кроме того, накопили резервный запас в руках производителей в объеме около одного миллиона длинных тонн. Цифры, недавно обнародованные в связи с судебными разбирательствами по патентным правам, показывают, что половина этого запаса была накоплена за один год, 1912-й, когда производство достигло 790 000 длинных тонн, из которых только 300 000 тонн было реализовано, а остальные 490 000 тонн пошли на хранение. Производство в Соединенных Штатах превышает производство Италии с 1912 года, хотя продажи были меньше, поскольку сера изымалась из запасов в Италии, в то время как запасы в Соединенных Штатах увеличивались. Чистым результатом войны стало четырехкратное увеличение объема серы, проданной в Соединенных Штатах, без какого-либо сокращения запасов; в то время как в Италии производство упало на 50 процентов, а имеющиеся запасы сократились на тот же процент.

От 98 до 99 процентов производства в Соединенных Штатах приходится на регион побережья Мексиканского залива в штатах Луизиана и Техас. Ряд других местностей в западном Техасе, Колорадо, Вайоминге, Айдахо и Неваде имеют поверхностные месторождения, обычно ограниченные по размеру, которые разрабатывались в небольших масштабах, но утратили свое значение с освоением более качественных и доступных месторождений региона побережья Мексиканского залива.

Залегание серы в регионе побережья Мексиканского залива связано с особой формацией, известной как «соляные купола» или «холмы». Было обнаружено более двадцати таких куполов, разбросанных на территории длиной 200 миль, простирающейся через западную Луизиану и восточный Техас, и, как правило, в пределах 50 миль от Мексиканского залива. Коммерческие месторождения нефти, серы и соли были разработаны в связи с этими куполами, но до сих пор в одном куполе не разрабатывалось более одного минерала в коммерческих масштабах. Сера была обнаружена при бурении на нефть. К настоящему времени для добычи серы были освоены три купола, а именно: принадлежащий Union Sulphur Co. в Салфере, штат Луизиана (1903 г.), принадлежащий Freeport Sulphur Co. во Фрипорте, штат Техас (1912 г.), и купол Texas-Gulf Sulphur Co. недалеко от Матагорды, штат Техас (1919 г.). Еще два купола находятся в стадии разведки, и ряд других, возможно, содержат серу.

Сера залегает на глубине от 300 до 1200 футов, ассоциирована с известняком и подстилается гипсом. Площадь поверхности продуктивных куполов варьируется от 200 до 1500 акров. Разведка проводится путем бурения стоимостью от 200 000 до 300 000 долларов, а стоимость комплектного завода составляет несколько миллионов долларов. Сера не может добываться шахтным способом из-за плывунов и встречающихся ядовитых газов. Месторождение в Салфере, штат Луизиана, оставалось нетронутым почти 40 лет после его открытия, прежде чем был разработан удовлетворительный процесс его добычи. Он известен как «процесс Фраша» и заключается в бурении скважин к серному месторождению, каждая из которых обсажена трубой диаметром от 10 до 12 дюймов. Внутри помещаются трубы меньшего диаметра, чтобы перегретая вода могла контактировать с серной рудой, которая плавится и вытесняется на поверхность сжатым воздухом. Сера при охлаждении готова к продаже и имеет чистоту более 99 процентов. Каждый из трех работающих заводов оснащен котельной мощностью более 20 000 л.с. для перегрева воды и требует около полутора миллионов баррелей мазута в год. Считается, что происхождение этих куполов связано с глубокими магматическими интрузиями, приведшими к изменению гипса и кристаллизации соли и серы, что вызвало выгибание пластов вверх. Из-за природы формации и нерегулярности месторождений невозможно точно оценить запасы серы.

С добавлением двух новых заводов с 1912 года Соединенные Штаты теперь имеют мощности по производству серы около 1¹⁄₄ миллиона тонн в год, что в четыре раза превышает нормальные продажи до войны. Если необходимо найти выход для этой избыточной серы, она должна конкурировать с пиритом на внутреннем рынке или с сицилийской серой на европейских рынках. Во второй половине 1919 года котировались цены от 14 до 15 долларов за тонну франко-рудник, что указывало на попытку захватить часть рынка кислоты, на котором ранее использовался пирит.

В серной промышленности Соединенных Штатов нет элемента политического контроля, за исключением временных мер, принятых во время войны при лицензировании экспорта и распределении потребления. Коммерческий контроль полностью находится в руках американских компаний. Union Sulphur Co. пыталась предотвратить использование усовершенствованного «процесса Фраша» другими компаниями, которые конкурируют с ней. Если претензия о нарушении патентных прав будет удовлетворена, это даст компании Union контроль над ситуацией, аналогичный тому, который она имела до развития двух более новых компаний, и может привести к ограничению выпуска и поддержанию цен.

Япония.

— Япония занимает третье место по добыче серы, хотя она имеет второстепенное значение по сравнению с Соединенными Штатами или Италией. Добыча серы в Японии медленно росла с 15 000 длинных тонн в 1900 году до 60 000 тонн в 1913 году, или около 7 процентов мирового объема. Внутреннее потребление очень мало, и около 90 процентов продукции экспортировалось, главным образом в Австралию, на западное побережье Соединенных Штатов и Канады, а также в Китай и Индию. Во время войны объем выпуска увеличился до максимума около 100 000 тонн, но в 1918 году добыча была значительно сокращена из-за резкого роста фрахтовых ставок в Австралию, которая закупала около половины японской продукции.

Сера встречается в поверхностных месторождениях ограниченного размера и редко достигает 100 футов в мощности. Месторождения, как правило, относятся к сольфатарному типу и встречаются в многочисленных районах вулканической активности. Большинство продуктивных площадей имеют почти круглые очертания, что указывает на их образование путем отложения в кратерных озерах. В некоторых случаях они стратифицированы и перекрыты мелкозернистым коричневым глинистым или туфогенным материалом, полученным частично из окружающих пород, а частично из самой серы. Другие месторождения второстепенного значения могли образоваться путем пропитки. Добываемая руда содержит от 50 до 60 процентов серы. Месторождения с содержанием серы менее 40 процентов разрабатываются редко.

Примерно две трети добычи приходится на юго-западную часть острова Хоккайдо. Четыре рудника производят в среднем около 10 000 тонн каждый в год, а остальная часть добычи поступает с 10–12 более мелких предприятий, расположенных от окрестностей горы Дайтон на Тайване (Формоза) до Курильских островов.

Точной оценки запасов руды нет. Один из самых важных рудников, по оценкам, содержит несколько миллионов тонн 50-процентной руды. Запасов, вероятно, достаточно для поддержания нынешнего уровня добычи в течение многих лет. Отсутствие судоходных мощностей препятствует производству, и мало шансов, что относительное значение Японии в серной промышленности значительно возрастет.

Все серные рудники управляются японцами. Государство сохраняет за собой право первоначальной собственности на все минералы, за исключением нескольких россыпных месторождений. Право на разработку предоставляется японским компаниям или частным лицам в порядке очередности подачи заявок. Однако горное законодательство признает права любой корпорации, организованной иностранцами в соответствии с японским законодательством.

Великобритания.

— Великобритания имеет оценочный годовой объем извлечения побочной элементарной серы от 30 000 до 40 000 тонн. Процесс извлечения известен как процесс Чанса-Клауса и применяется в связи с процессом Леблана по производству соды. Он основан на разложении сульфата кальция в отходах чанов с помощью диоксида углерода и извлечении серы из образующегося сероводородного газа.

Другие страны.

— Добыча серы за пределами Соединенных Штатов, Италии и Японии имеет второстепенное значение.

Северная Чили имеет небольшую добычу серы на вулканах Такора и Чупикина. Запасы оцениваются как довольно большие, но большая высота (14 000–20 000 футов) и плохая транспортная доступность ограничили добычу местным использованием в винодельческих районах Чили. Добыча, согласно отчетам, постепенно увеличилась до 6 000 тонн в 1913 году и, как сообщается, удвоилась с тех пор.

Испания производит около 10 000 тонн серы ежегодно из низкосортных месторождений, расположенных в окрестностях Альмерии. Большие цифры, часто приводимые в отчетах, относятся к добытой низкосортной руде.

Австрии приписывают добычу от 10 до 15 тысяч тонн сырой серной руды, что, вероятно, составляет лишь 2 или 3 тысячи тонн чистой серы.

Крупнейший серный рудник в Мексике расположен в Серритосе, в 25 милях к югу от Гуадалькасара, Сан-Луис-Потоси. Пятнадцать лет назад он был приобретен американской компанией Virginia-Carolina Chemical Co. Позже он был сдан в аренду германским интересам. Небольшой объем продукции в несколько тысяч тонн отгружался в Германию до войны. В Сан-Луис-Потоси есть ряд месторождений в дополнение к месторождению в Серритосе.

Несколько раз сообщалось, что британская компания собирается разрабатывать серные месторождения мексиканского вулкана Попокатепетль, недалеко от Мехико. Заявления относительно месторождений в вулкане противоречивы, но исследования показывают, что их масштаб был сильно преувеличен. Многие другие месторождения встречаются в связи с местными вулканическими районами, но до сих пор они имеют небольшую экономическую ценность из-за труднодоступности.

Существует ряд месторождений серы на Алеутских островах (Аляска), вероятно, содержащих значительное количество серы, но частично покрытых ледниками и труднодоступных. Сомнительно, что их можно было бы разрабатывать в условиях конкуренции с дешевой серой из района прибрежной равнины Соединенных Штатов.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

В ближайшем будущем вряд ли произойдут какие-либо далеко идущие изменения в практике. Истощение поверхностных месторождений серы в Италии и необходимость глубокой добычи делают необходимым улучшение и внедрение там более современных методов. Также внедряются усовершенствованные методы рафинирования серы, благодаря которым потери при старом методе «калькароне» будут в значительной степени устранены. Потребление серы для сульфитной древесной целлюлозы может быть значительно сокращено за счет повсеместного использования усовершенствованной практики, которая уже применяется на лучших заводах. В местностях, где доступен пирит, этот материал может использоваться в целлюлозной промышленности для замены серы. В случае возникновения конкуренции между тремя крупными серными компаниями в Соединенных Штатах и значительного снижения цены на серу, это может привести к более широкому использованию этого материала в производстве серной кислоты. Серные горелки могут быть установлены гораздо быстрее и дешевле, чем печи, необходимые для обжига пирита, и после установки количество труда и заботы, требуемых при их эксплуатации, меньше. Увеличение извлечения серной кислоты в качестве побочного продукта на медеплавильных и цинкоплавильных заводах, вероятно, будет представлять собой растущий фактор конкуренции с кислотой, производимой либо из пирита, либо из серы. Дальнейшее увеличение этого источника в Соединенных Штатах затруднено расположением многих медеплавильных заводов на западе, на больших расстояниях от рынка сбыта серной кислоты, который находится преимущественно в восточных и южных штатах. Проводятся эксперименты с новыми процессами производства элементарной серы из этих сернистых газов. Если они будут успешными в больших масштабах, материал из этого источника может обеспечить любые будущие рынки, расположенные на западе, и может конкурировать с японской серой, которая ранее импортировалась в наши штаты на Тихоокеанском побережье.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ НАД СЕРОЙ И ПИРИТОМ

Политический контроль над важными месторождениями серы в мире в первую очередь соответствует странам, в которых они расположены. В случае Соединенных Штатов месторождения контролируются частными компаниями. В качестве строго военной меры осуществлялся контроль над распределением продукции. В Италии правительство взяло на себя контроль над производством и сбытом серы. Это было в значительной степени вызвано конкуренцией со стороны американской серы и последовавшим за этим спадом в итальянской промышленности. В 1906 году была организована так называемая Consorzia Obbligatoria в соответствии с законом, принятым итальянским парламентом, который предусматривал, что эта компания должна управляться королевским комиссаром, назначенным итальянским правительством. Согласно этому закону, производители были обязаны продавать свою продукцию этой компании, которая контролировала цены и экспорт. В 1910 году были введены ограничения на предоставление новых концессий. Аргументами, недавно представленными в пользу продолжения государственного контроля, были растущая иностранная конкуренция, значительный рост производства в Соединенных Штатах во время войны, незначительный рост производства в Японии и возможности разработок в северной Африке. Цель этого государственного контроля над отраслью состоит в том, чтобы объединить и регулировать усилия отдельных производителей для эффективного противостояния будущей конкуренции.

КОММЕРЧЕСКИЙ КОНТРОЛЬ НАД СЕРОЙ И ПИРИТОМ

До 1906 года итальянские месторождения в значительной степени контролировались Anglo-Sicilian Sulphur Co., представлявшей английский капитал, но с того времени, когда итальянское правительство взяло на себя контроль над отраслью, коммерческий контроль стал преимущественно итальянским.

В Соединенных Штатах коммерческий контроль над производством серы находится в руках трех компаний, одна из которых начала производство как раз во время начала европейской войны, а другая начала производство только в 1919 году. Насколько известно, между этими тремя интересами нет объединения. Union Sulphur Co., которая была первым и основным производителем, контролирует определенные патенты на «процесс Фраша». В период войны было заключено соглашение, по которому предполагаемое нарушение патентов не преследовалось. После окончания войны остается увидеть, в какой степени затронутые патентные права могут повлиять на производство двух других компаний, Freeport и Texas Gulf, которые в целом используют аналогичный процесс.

Производство серы в Японии коммерчески контролируется японскими интересами.

Американская компания Virginia-Carolina Chemical Co. владеет серным месторождением в Мексике, которое до войны было сдано в аренду германским интересам. Сообщалось, что ряд других месторождений в Мексике и Южной Америке контролировались германскими интересами, но до сих пор добыча из всех этих источников имела относительно второстепенное значение, и нет никаких непосредственных перспектив каких-либо больших изменений.

Значимым фактором коммерческого контроля в ситуации с пиритом являются крупные инвестиции британского капитала в испанские месторождения и, в меньшей степени, инвестиции французского капитала. Американский капитал контролирует основные разработки пирита в Канаде, на Кубе, в Мексике и на Кипре. Английский, французский и шведский капитал инвестирован в Норвегию.

ПОЛОЖЕНИЕ ОСНОВНЫХ ДЕРЖАВ

Соединенные Штаты наиболее благоприятно расположены среди всех стран по своим запасам серы. В годы, предшествовавшие европейской войне, они производили около половины мирового объема. С того времени их производство увеличилось в несколько раз, и теперь они являются доминирующим фактором в мировой ситуации.

Относительное положение Италии, которая ранее была равна по значимости Соединенным Штатам, ухудшается. Стоимость ее производства растет, и американская сера вступит в острую конкуренцию на европейских рынках. Ресурсы Японии сравнительно невелики, и большая часть ее продукции экспортировалась. Послевоенные условия, вероятно, сократят рынки для японской серы, и нет никаких шансов на усиление позиций Японии. Англия, Франция и Германия должны в первую очередь полагаться на другие страны в своих поставках как пирита, так и серы. Англия получает часть своих поставок серы из побочного источника, известного как процесс Чанса-Клауса, который производит от 30 до 40 тысяч тонн ежегодно. Кроме того, она получает большие объемы пирита из Испании. Франция производит некоторое количество местного пирита, но импортирует большие количества этого материала из Испании; а до начала войны получала растущие объемы серы из Соединенных Штатов. Германия и Австрия имеют некоторые ресурсы пирита и, вероятно, имели значительные запасы серы к началу войны. Было заявлено, что для обеспечения своих потребностей в этих материалах Германия была вынуждена использовать дорогостоящие процессы, снижать содержание серы в гипсе, расширять добычу пирита и увеличивать выпуск кислоты на заводах. В нормальных условиях ей, вероятно, придется вернуться к импорту пирита из Норвегии и Швеции или серы из Соединенных Штатов и Италии.

ГЛАВА XXIX ЗОЛОТО Автор: Джон Э. Орчард

ИСПОЛЬЗОВАНИЕ ЗОЛОТА

Физические свойства золота и трудности, связанные с его получением, сделали золото во все времена одним из самых драгоценных металлов. Благодаря своему блеску, цвету и неразрушимости первобытный человек придавал ему форму колец, браслетов и других украшений. Эти же свойства, вместе с его делимостью, рано привели к использованию золота в качестве торгового эквивалента, и во всех, кроме самых примитивных обществ, оно рассматривалось как мера стоимости и средство обмена. Самое раннее известное упоминание о золоте касается его использования в торговле и содержится в указе Менеса Египетского (возможно, 3800 г. до н. э.), устанавливающем соотношение стоимости золота к серебру как 2¹⁄₂ к 1.

В качестве средства обмена золото используется в различных формах. Первобытный торговец принимал и отдавал золотые украшения в обмен на товары. В шахтерских лагерях золотой песок и самородки были средством обращения. В оседлом обществе при правительстве, пользующемся доверием управляемых, золото, отчеканенное правительством в монеты удобных номиналов, принимается без вопросов во всех сделках. Для расчетов по балансам в международной торговле используется золотой слиток, стоимость которого определяется весом. Сегодня практически все страны находятся на золотом стандарте, и даже те, кто использует серебряный стандарт во внутренней торговле, приняли золотой стандарт для внешней торговли.

Но золото, хотя и обладает многими превосходными качествами, является одним из самых тяжелых металлов, и носить его при себе неудобно, особенно в количествах, достаточных для крупных сделок. Кроме того, при постоянном обращении золото стирается, а монеты теряют в стоимости. Соответственно, большая часть монет или золотых слитков хранится в национальной казне или в банковских хранилищах, а в качестве средства обращения используется та или иная форма бумажной валюты. На этом золотом резерве, который видят лишь немногие сотрудники правительства или банка, не имеющие на него прав собственности, построена сложная система кредитов и торговли.

Правда, в реальном обращении находится мало золота и для внутренней торговли все чаще используются средства обмена, обеспеченные золотом лишь частично. Даже международный обмен больше не находится на золотом стандарте, но эта ситуация, несомненно, временная, и с улучшением финансовых условий в Европе золото будет восстановлено в своем положении основы торговли и финансов, как национальной, так и международной. Средство обращения, какова бы ни была его природа, должно быть свободно конвертируемым, а кредит, чтобы оставаться надежным, должен основываться на адекватном золотом резерве.

Согласно официальным оценкам, в период с 1492 по 1894 год мировая добыча золота составила около 8 000 000 000 долларов. Из этой суммы чуть менее 4 000 000 000 долларов хранилось в виде золотого резерва в 1894 году, а остальная часть была утрачена или поглощена промышленным использованием или производством ювелирных изделий. С 1894 года потребление золота в промышленности составляло от 50 000 000 до 100 000 000 долларов ежегодно, что за 27 лет составило около 2 100 000 000 долларов из общего объема добычи в 9 000 000 000 долларов — почти 25 процентов.

Дженнингс, Хеннен: «Золотая промышленность и золотой стандарт», 1919 г.

ГЕОЛОГИЧЕСКИЕ УСЛОВИЯ ЗАЛЕГАНИЯ

Золото широко распространено как географически, так и геологически. Оно встречается примерно в 60 странах во всех частях света и присутствует в породах всех возрастов, от архейских до четвертичных, часто в ассоциации с другими металлами, такими как серебро, медь, теллур, свинец и железо.

Месторождения золота можно в широком смысле классифицировать как коренные и россыпные. Коренные месторождения также известны как жильные или кварцевые месторождения; в них золото встречается вместе с кремнеземом или кварцем в виде неправильных масс, прожилков, чешуек, пластин и кристаллов, или, что чаще, в виде микроскопических частиц в сульфидных минералах или пустой породе. Для извлечения руды используются практически те же методы, что и при добыче серебра, свинца или цинка.

Россыпные или аллювиальные месторождения представляют собой осадочные слои гравия или песка, в которых частицы золота, вымытые из коренной жилы, были сконцентрированы под воздействием воды. Большинство россыпных месторождений залегают открыто, вдоль русла реки, но некоторые из них покрыты слоем лавы или другой непродуктивной породы. Золото встречается в виде чешуек, зерен, слитков или самородков. Было найдено немало крупных самородков, самым крупным из которых является австралийский «Welcome Stranger» («Желанный незнакомец»), весящий 2520 унций и оцениваемый примерно в 42 000 долларов. Однако обычно частицы золота очень мелкие.

Россыпные месторождения разрабатываются одним из следующих методов, в зависимости от характера и богатства аллювия: промывка в шлюзах, гидравлический способ, дражная разработка или подземная разработка (дрифтовый метод).

В первые годы того, что называют современной эрой золотодобычи, начавшейся с открытия золота в Калифорнии в 1848 году, большая часть мировой ежегодной добычи приходилась на россыпные месторождения. Де Лоне оценивает, что с 1848 по 1875 год россыпи обеспечивали 87 процентов добычи. В более поздние годы, по мере истощения легко обнаруживаемых и легко разрабатываемых россыпных месторождений, эта доля снизилась и в настоящее время составляет, вероятно, не более 10 процентов. Сегодня крупнейшие золотые рудники мира — это коренные месторождения. Самый глубокий золотой рудник в мире достиг вертикальной глубины 5900 футов.

Сделав все поправки на будущие открытия, исследователи данного вопроса придерживаются мнения, что мировая добыча золота уже достигла своего зенита и следует ожидать ее снижения.

Приведенное выше обсуждение геологических условий залегания золота основано главным образом на работе «Золотая промышленность и золотой стандарт» и других статьях Хеннена Дженнингса, инженера-консультанта Бюро горной промышленности США.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Коммерчески важные рудники встречаются на каждом континенте, и на земной поверхности мало регионов, которые не содержали бы месторождений, разрабатываемых сейчас или ранее. Распределение золота сыграло важную роль в заселении новых земель, особенно Калифорнии, западной Канады, Аляски, Мексики, Австралии и Южной Африки, и, несомненно, будет оказывать большое влияние на будущие перемещения народов. И все же, хотя золото распределено так широко, 323 950 000 долларов, или более 75 процентов от общего количества золота, добытого в 1917 году, поступило из четырех стран: Трансвааля, США, Австралии и России.

Объемы добычи основных стран-производителей приведены в Таблице 67 и на Рисунке 19.

Северная Америка

Соединенные Штаты.

— Хотя в настоящее время США уступают Трансваалю, ранее они лидировали в мире по добыче золота. По оценкам, эта страна с 1792 года внесла около 3 913 000 000 долларов в мировые запасы золота, что составляет чуть менее 25 процентов от общего объема добычи, и этот показатель выше, чем у любой другой страны. Соединенные Штаты впервые стали важным производителем в 1850 году после открытия золота в Калифорнии. До этого времени некоторое количество золота добывалось в штатах Аппалачского региона, причем общая сумма, вероятно, достигала 50 000 000 долларов.

Отчет комитета, назначенного Министром внутренних дел для изучения ситуации с золотом.

В 1915 году объем добычи в Соединенных Штатах составил 101 035 000 долларов, что является самым высоким показателем, достигнутым на тот момент. С того года наблюдается ежегодное падение добычи примерно на 8 000 000 долларов. Объем добычи в 1918 году составил 68 646 700 долларов, а в 1919 году — 58 488 800 долларов.

За последние четыре года восемь штатов — Калифорния, Колорадо, Аляска, Южная Дакота, Невада, Аризона, Монтана и Юта — произвели более 90 процентов золота, добытого в Соединенных Штатах.

Таблица 67. — Добыча золота в основных странах-производителях, 1880-1917 гг.

Year | United States | Australasia | Transvaal [162] | Russia- Siberia | Rhodesia [162] | Mexico | Canada | British India | World [163]
1880 | $36,000,000 | $28,765,000 | $1,993,800 | $28,551,028 |  | ... | $989,160 |  | $815,089 | ... | $106,436,800
1881 | 34,700,000 | 30,690,000 | 1,993,800 | 24,371,343 | ... | 858,909 | 1,094,926 | ... | 103,023,100
1882 | 32,500,000 | 31,955,017 | 1,993,800 | 23,867,935 | ... | 936,223 | 1,094,926 | ... | 101,996,600
1883 | 30,000,000 | 27,150,000 | 717,000 | 20,119,000 | ... | 951,000 | 954,000 | ... | 95,392,000
1884 | 30,800,000 | 28,284,000 | 830,000 | 21,874,000 | ... | 1,183,000 | 954,000 | ... | 101,729,000
1885 | 31,801,000 | 27,439,000 | 1,384,000 | 25.338,000 | ... | 867,000 | 1,116,000 | $135,000 | 108 435,000
1886 | 34,869,000 | 26,425,000 | 1,438,000 | 20,518,000 | ... | 614,000 | 1,330,442 | 421,600 | 106,163,000
1887 | 33,136,000 | 27,327,600 | 1,919,600 | 20,092,000 | ... | 824,000 | 1,178,637 | 320,000 | 105,774,900
1888 | 33,167,000 | 28,560,660 | 4,500,000 | 21,302,000 | ... | 974,000 | 1,111,959 | 685,720 | 110,196,000
1889 | 32,967,000 | 33,086,700 | 7,788,372 | 23,905,600 | ... | 700,000 | 1,295,000 | 1,502,600 | 123,489,200
1890 | 32,845,000 | 29,808,000 | 10,438,356 | 25,484,000 | ... | 767,000 | 1,666,000 | 2,000,000 | 118,848,700
1891 | 33,175,000 | 31,399,000 | 14,885,639 | 24,162,500 | ... | 1,000,000 | 930,666 | 2,495,000 | 130,650,000
1892 | 33,015,000 | 34,159,000 | 23,220,108 | 24,806,200 | ... | 1,129,200 | 907,600 | 3,318,300 | 146,651,500
1893 | 35,955,000 | 35,688,600 | 28,293,831 | 27,808,200 | ... | 1,305,300 | 927,200 | 3,813,600 | 157,494,800
1894 | 39,500,000 | 41,760,800 | 39,696,330 | 24,133,400 | ... | 4,500,000 | [164] | 1,042,100 | 3,882,900 | 181,175,600
1895 | 46,610,000 | 44,798,300 | 43,893,300 | 28,894,400 | ... | 6,000,000 | [164] | 1,910,900 | 4,656,200 | 198,763,600
1896 | 53,088,000 | 45,181,900 | 43,779,669 | 21,535,800 | ... | 8,331,700 | [164] | 2,810,200 | 6,130,500 | 202,251,600
1897 | 57,363,000 | 52,665,700 | 57,633,861 | 23,245,700 | ... | 7,500,000 | [164] | 6,089,500 | 7,247,200 | 236,083,700
1898 | 64,463,000 | 64,860,800 | 79,213,953 | 25,463,400 | 444,617 | 8,500,000 | [164] | 13,838,700 | 7,781,500 | 286,879,700
1899 | 71,053,400 | 79,321,600 | 71,384,561 | 22,167,100 | 1,129,773 | 8,500,000 | [164] | 21,324,300 | 8,658,800 | 306,724,100
1900 | 79,171,000 | 73,498,900 | 6,124,226 | 20,145,500 | 1,158,815 | 9,000,000 | [164] | 27,880,500 | 9,435,500 | 254,576,300
1901 | 78,666,700 | 76,880,200 | 5,333,994 | 22,850,900 | 2,974,943 | 10,284,800 |  | 24,128,500 | 9,395,900 | 260,992,900
1902 | 80,000,000 | 81,578,800 | 34,901,140 | 22,533,400 | 3,366,561 | 10,153,100 | 21,336,700 | 9,588,100 | 296,737,600
1903 | 73,591,700 | 89,210,100 | 61,454,439 | 24,632,200 | 4,065,489 | 10,677,500 | 18,834,500 | 11,428,900 | 327,702,700
1904 | 80,464,700 | 87,767,300 | 78,004,559 | 24,803,200 | 4,794,208 | 12,605,300 | 16,462,500 | 11,722,900 | 347,377,200
1905 | 88,180,700 | 85,926,500 | 101,489,199 | 22,291,600 | 7,337,211 | 16,107,100 | 14,610,400 | 11,950,200 | 380,288,700
1906 | 94,373,800 | 82,391,400 | 119,618,507 | 19,496,500 | 10,082,747 | 18,534,700 | 12,023,900 | 12,087,700 | 402,503,000
1907 | 90,435,700 | 75,677,700 | 133,361,943 | 26,684,300 | 11,199,181 | 18,681,100 | 8,382,800 | 10,383,600 | 412,966,600
1908 | 94,560,000 | 73,327,300 | 145,862,971 | 28,052,200 | 13,022,460 | 22,371,200 | 9,842,100 | 10,598,500 | 442,476,900
1909 | 99,673,400 | 71,007,900 | 150,799,880 | 32,381,300 | 13,223,955 | 23,842,900 | 9,382,200 | 10,358,600 | 454,059,100
1910 | 96,269,100 | 65,470,600 | 155,597,202 | 35,579,600 | 13,590,658 | 24,910,600 | 10,205,800 | 10,718,400 | 455,239,100
1911 | 96,890,000 | 60,184,200 | 170,566,159 | 32,151,600 | 13,823,733 | 24,880,100 | 9,762,100 | 11,054,100 | 461,939,700
1912 | 93,451,500 | 54,509,400 | 188,293,100 | 22,199,000 | 14,226,900 | 24,500,000 | 12,648,800 | 11,055,700 | 466,136,100
1913 | 88,884,400 | 53,113,200 | 181,885,300 | 26,508,700 | 14,274,700 | 19,308,800 | 16,598,900 | 12,178,000 | 459,941,100
1914 | 94,531,800 | 47,569,023 | 173,559,940 | 28,586,392 | 17 663,686 | 4,788,175 | 15,983,004 | 11,378,400 | 439,078,260
1915 | 101,035,700 | 49,397,797 | 188,033,156 | 26,322,745 | 18,915,324 | 6,559,275 | 18,977,901 | 11,522,457 | 468,724,918
1916 | 92,315,363 | 38,213,328 | 192,182,900 | 22,300,000 | 19,232,200 | 7,690,700 | 19,235,000 | 11,206,500 | 454,176,500
1917 | 84,456,600 | 35,275,000 | 186,254,256 | 18,000,000 | [164] | 14,988,600 | 9,000,000 | [164] | 15,449,426 | 10,756,800 | 423,590,200

Составлено по отчетам Директора монетного двора, 1880-1917 гг.

До 1898 года добыча в Родезии и Мозамбике включалась в отчетность Трансвааля.

Общая мировая добыча, 1492-1917 гг., 16 916 735 394 доллара.

Оценочно.

Рис. 19. — Добыча золота в основных странах-производителях, 1880-1917 гг., на основе отчетов Директора монетного двора.

С открытием золота в мельничном канале в Коломе, округ Эльдорадо, Калифорния, Дж. А. Маршаллом в 1848 году началась история современной золотодобычи. За этим последовала великая «золотая лихорадка» в Калифорнии, и штат стал ведущим золотодобывающим регионом мира. Объем добычи в 1860 году составил 45 320 000 долларов по сравнению с общим объемом добычи всего в 1 000 000 долларов для остальных штатов. В течение многих лет добыча золота в Калифорнии снижалась, и общий объем в 1917 году составил всего 20 000 000 долларов, что на 2 000 000 долларов меньше, чем в 1916 году. Около трех пятых добычи приходится на коренные рудники, а остальная часть — на россыпи.

В течение ряда лет Колорадо был ведущим золотодобывающим штатом, главным образом благодаря добыче в Криппл-Крик, округ Теллер, который с 1893 по 1908 год был ведущим центром золотодобычи в Соединенных Штатах. В последнее время объем добычи упал ниже уровня Калифорнии. Более половины добычи штата в 1916 году пришлось на округ Теллер.

Первое открытие золота на Аляске произошло, вероятно, около 1849 года вдоль берегов залива Кука. В 1879 году были открыты золото-кварцевые жилы возле Ситки, а год спустя — россыпи Джуно. Открытие золотых россыпей в долине Юкона произошло в 1886 году, а в Клондайке — в 1896 году. Большая часть добычи на Аляске получается из россыпных месторождений, самыми богатыми из которых являются месторождения на полуострове Сьюард возле Нома и в бассейне Юкона. Крупнейшими коренными рудниками были рудники возле Джуно; из них «Тредвелл» долгое время был величайшим золотым рудником в мире, но сейчас он неактивен. В течение последних нескольких лет разработка крупных низкосортных вкрапленных месторождений типа «Тредвелл» возле Джуно велась в масштабах, ранее немыслимых, но пока эти предприятия (рудники «Аляска Голд» и «Аляска Джуно») не были финансово успешными.

Золотодобывающий район Южной Дакоты ограничен площадью менее 100 квадратных миль, расположенной в Блэк-Хилс. Гравий в ущельях Уайтвуд и Дедвуд впервые начали промывать в 1875 году, а в 1876 году были открыты знаменитые жилы «Хоумстейк». В настоящее время около 94 процентов общего объема добычи штата контролируется одной компанией, «Хоумстейк Майнинг Компани», крупнейшей добывающей компанией в Соединенных Штатах.

После истощения знаменитой жилы «Комсток», открытой в 1851 году, Невада не имела большого значения как золотодобывающий штат до открытия богатых месторождений Тонопа в 1900 году. В настоящее время практически все золото, добываемое в штате, поступает из жильных месторождений Тонопа и Голдфилда. Дивайд — это недавно освоенный лагерь между ними.

В Аризоне есть три основных золотоносных района: окрестности Бисби и Томстоуна, округ Кочис; район Оатман, округ Мохаве; и район Верде, округ Явапай. Аризона была одним из немногих штатов, показавших больший объем добычи в 1917 году, чем в 1916 году. Рудник «Юнайтед Истерн», новое предприятие, открытое в 1913 году в районе Оатман округа Мохаве, дало значительную добычу и стало причиной этого роста. Добыча золота в округах Кочис и Явапай осуществляется в основном из медной руды.

В шестидесятых и семидесятых годах Монтана уступала только Калифорнии по добыче россыпного золота. Самыми известными россыпями были месторождения Баннак и Алдер-Галч, а позже Хелена. Большая часть текущей добычи получается как побочный продукт при переработке медных руд.

Немногие рудники в Юте разрабатываются исключительно ради содержания золота, большая часть добычи штата извлекается из медных и свинцовых руд.

Золото также добывается в Айдахо, Нью-Мексико, Орегоне и Вашингтоне. Небольшие количества были добыты в 1917 году в ряде штатов Аппалачского региона. До открытия золота в Калифорнии практически все золото, чеканившееся на монетном дворе Соединенных Штатов, поступало с рудников Вирджинии, Мэриленда, Алабамы, Джорджии и Каролин, но после Гражданской войны их добыча не имела большого значения. Добыча золота на Филиппинских островах в 1917 году составила 1 404 000 долларов.

Канада.

— Общий объем добычи золота в Канаде в 1900 году составил 28 000 000 долларов, но с истощением россыпных месторождений он снизился до 8 382 000 долларов в 1907 году. С развитием жильных месторождений добыча неуклонно росла с этой низкой точки и достигла 19 235 000 долларов в 1916 году и 15 272 992 долларов в 1917 году, что поставило Канаду на шестое место в списке производителей золота. Три провинции — Онтарио, Британская Колумбия и территория Юкон — дают большую часть золота, остальные провинции производят менее 1 процента от общего объема.

Более половины канадской добычи приходится на район Поркьюпайн в Темискаминг, Онтарио, освоенный в 1912 году. Другими добывающими районами, хотя и меньшего значения, являются Киркленд-Лейк и тауншип Манро, также в Темискаминг, и Лонг-Лейк, недалеко от Нотона, район Садбери.

«Добыча меди, золота, свинца, никеля, серебра, цинка и других металлов в Канаде, 1916 г.». Министерство горной промышленности Канады, Горный департамент, 1917 г.

Одно время большая часть добычи золота в Британской Колумбии была получена из россыпей, главным образом в районах Атлин и Карибу, но в 1917 году из этого источника было получено менее 5 процентов. Основными районами коренной добычи являются Западный Кутеней и Йель в южной части провинции. Добыча золота в 1917 году составила около половины от общего объема за 1916 год.

«Добыча меди, золота, свинца, никеля, серебра, цинка и других металлов в Канаде, 1917 г.». Министерство горной промышленности Канады, Горный департамент, 1919 г.

Золото известно на территории Юкон с 1869 года, и месторождения активно разрабатываются с 1881 года. Большая часть россыпей реки Форти-Майл и все россыпи реки Сиксти-Майл находятся под юрисдикцией Канады. В 1897 году произошло открытие Клондайка. Добыча золота достигла своего пика на территории Юкон в 1900 году, когда объем составил 1 077 649 чистых унций стоимостью 22 000 000 долларов. Практически вся добыча 1917 года была получена из россыпных месторождений.

Золото добывалось в Квебеке еще в 1823 году, но Канада не имела большого значения как золотодобывающий регион до открытия россыпей в Британской Колумбии в 1857 году. Золотые месторождения, имеющие небольшую экономическую ценность, до сих пор разрабатываются в Квебеке, Нью-Брансуике, Новой Шотландии и Ньюфаундленде. Геологоразведочные и подготовительные работы в Манитобе, Саскачеване и Альберте указывают на то, что эти провинции могут стать важными производителями золота.

Мексика.

— В течение многих лет Мексика занимала четвертое место среди золотодобывающих стран мира, уступая только Трансваалю, Соединенным Штатам и Австралазии. Революции и бандитские налеты серьезно мешали горным работам с 1911 года, и объем добычи золота в 1917 году составил немногим более одной трети от нормального годового объема. С установлением стабильного правительства, способного защитить иностранные инвестиции, Мексика, несомненно, вернет себе прежние позиции.

Большая часть добычи золота в Мексике получается как побочный продукт при переработке свинцовых, серебряных, цинковых и медных руд. Единственным настоящим золотодобывающим районом является район Эль-Оро в штатах Мехико и Мичоакан. Основными добывающими рудниками являются «Эсперанса», «Эль-Оро», «Мехико Майнз оф Эль-Оро» и «Дос Эстреллас». В 1906 году «Эсперанса» считался, как по фактической добыче, так и по полученной прибыли, самым продуктивным золотым рудником в мире. С тех пор его превзошли рудники Соединенных Штатов и Трансвааля. Другой знаменитый золотой рудник Мексики, «Долорес», расположенный в западной Чиуауа, дает руду, содержание серебра в которой по стоимости почти равно золоту. Нижняя Калифорния, Сонора, Дуранго, Идальго, Сан-Луис-Потоси, Гуанахуато и Чьяпас — все это золотодобывающие штаты.

Центральная Америка.

— Во времена открытия Америки испанцев привлек регион, ныне входящий в состав государств Центральной Америки, сообщениями о сказочно богатых рудниках и богатствах индейцев. Было отправлено несколько экспедиций на поиски золота, и были открыты и разрабатывались некоторые богатые рудники. Золото до сих пор добывается в Центральной Америке, но общее количество невелико, составляя менее 1 процента от мирового объема в 1913 году. Гондурас является самым богатым из этих государств по добыче, а Никарагуа занимает второе место; основные центры золотодобывающей промышленности находятся в департаментах Матагальпа и Чонталес, а также в районе Кабо-Грасиас и Принсаполька.

Торговые отчеты США, Приложение 34a, 1915 г., стр. 4.

Южная Америка

Южная Америка также была важным источником золота в годы, последовавшие за открытием Америки. Ранние завоеватели получали золото, грабя храмы, церкви и даже могилы туземцев. После завоевания испанцы с помощью своих рабов систематически обыскивали большую часть континента в поисках золотых месторождений. Около 15 процентов (2 266 000 000 долларов) всего золота, добытого в период с 1492 по 1917 год, поступило из Южной Америки.

Сегодня Южная Америка имеет небольшое значение как производитель золота, совокупный объем добычи всех стран в 1913 году составил около 2,5 процента от мирового объема. Большая часть добычи в Южной Америке до сих пор приходилась на аллювиальное золото. С установлением более стабильных правительств и улучшением транспортных условий вполне вероятно, что добыча в Южной Америке увеличится.

Согласно Макларену, золотые месторождения Южной Америки расположены в трех довольно четко разделенных областях. Основная область — это та, что тянется вдоль Анд от Панамского перешейка до центральной части Чили и включает месторождения Колумбии. Вторая область находится в хорошо выраженной петрографической и металлогенической провинции, простирающейся через внутренние районы Гвианы и включающей также рудники Венесуэлы и северной Бразилии. Третья область находится в провинции Минас-Жерайс, Бразилия. Некоторое количество золота добывается в Чили, Аргентине, Боливии, Перу, Эквадоре и Уругвае. Основными золотоносными районами Колумбии являются Чоко, департамент Антьокия и район, лежащий между реками Каука и Магдалена. Довольно богатые месторождения были также найдены в Колумбии недалеко от границы с Эквадором.

Макларен, Дж. Малкольм: «Золото: его геологические условия залегания и географическое распределение, 1908 г.», стр. 619.

Торговые отчеты США, Приложение 42b, 1915 г., стр. 12.

Основными рудниками Бразилии являются рудник «Сент-Джон-дель-Рей» и рудники, принадлежащие компании «Оуро Прето Голд Майнз оф Бразил, Лтд.», оба в штате Минас-Жерайс. Первый рудник считается самым глубоким в мире.

Европа

Хотя Европа в прошлом играла важную роль в добыче золота, в настоящее время добывается очень мало. До открытия Америки большая часть используемого золота поступала из Альп и Венгрии. Месторождения также разрабатывались в Англии, Ирландии, Уэльсе, Испании и Германии.

Единственные золотые рудники в Европе, имеющие в настоящее время экономическое значение, находятся в бывшей империи Австро-Венгрии, Франции и на Урале в России. На юге Франции золото добывалось вдоль рек, текущих с Пиренеев, а также в восточных провинциях. В настоящее время работают только три рудника, которые в 1911 году произвели 2554 килограмма золота. Венгерские месторождения очень старые, так как они разрабатывались римлянами 2000 лет назад. Большинство действующих сегодня рудников находятся в Трансильвании. Россия, как считается, произвела 5,8 процента от мирового объема в 1913 году. Небольшая часть этой добычи пришлась на Урал в европейской части России, главным образом как побочный продукт из других руд, но большая часть была получена в Сибири. Сибирские месторождения обсуждаются ниже, в разделе об Азии.

Азия

После снижения добычи в Мексике Россия занимает четвертое место среди золотодобывающих стран. Большая часть добычи приходится на Сибирь, которая долгое время была источником золота, а рудники Алтайских гор считаются одними из старейших в мире. Добыча золота в Сибири с 1830 года по настоящее время оценивается российскими властями примерно в 1 000 000 000 долларов.

Макларен разделил золотоносные области страны на два отдельных региона: восточный и западный. Около четырех пятых добычи страны приходится на первый регион, который простирается одним довольно узким золотоносным поясом от озера Байкал до юго-западного побережья Охотского моря.

Макларен, Дж. Малкольм: «Золото: его геологические условия залегания и географическое распределение», стр. 210.

В Уральском районе эксплуатировалось несколько драг. Самым перспективным объектом является Ридерлинский, к востоку от Омска. На Южном Урале большинство рудников производят медь, пирит или цинк, а золото в качестве побочного продукта обеспечивает прибыль. Риддерский рудник в Алтайских горах — самый известный коренной рудник в Сибири.

Россыпи расположены вдоль Маньчжурской границы на реках Онон и Амур. Они являются одними из самых важных в Сибири и дали более 100 000 000 долларов золотом. Месторождения Иркутска вдоль реки Лены являются самыми важными месторождениями, эксплуатируемыми до сих пор в Сибири, и, вероятно, самыми богатыми россыпями из когда-либо открытых. Район дает около одной трети сибирской добычи. Россыпи в настоящее время практически выработаны как подземные рудники, но продолжат давать продукцию при установке драг.

Многие инженеры считают, что Сибирь — самый богатый из оставшихся потенциальных источников золота в мире. По оценкам, страна произведет в будущем, скажем, в ближайшие 30 или 40 лет, около 6 000 000 000 долларов. Нестабильные политические условия сильно помешали добыче. Многие рудники были захвачены большевиками, и хотя маловероятно, что будут предприняты попытки систематической добычи, они, вероятно, будут разграблены в части более богатой вскрытой руды, прежде чем владельцы смогут их вернуть.

Индия долгое время считалась страной богатств. Филологи доказали, к собственному удовлетворению, что Офир, источник запасов золота Соломона, находился там. В пустынях северной Индии жили золотодобывающие муравьи, описанные греческими историками и более поздними авторами, что до сих пор не нашло объяснения. Современные факты не подтверждают легенды и предания. В 1913 году Индия внесла лишь 2,6 процента от общего мирового объема добычи золота, что едва ли соразмерно размерам страны. Земля предлагает старателю крайне непривлекательное поле деятельности. Она была тщательно исследована, и ее месторождения усердно разрабатывались по крайней мере двадцать пять веков людьми, обладающими большим терпением и значительным горным мастерством. Основные современные золотодобывающие рудники Индии находятся в районе Колар, где главная жила несет пять крупных рудников вдоль своего простирания.

Макларен, Дж. Малкольм: «Золото: его геологические условия залегания и географическое распределение», стр. 238-240.

Япония была одним из главных поставщиков золота, хлынувшего в Европу в XVI веке. Португальские и голландские торговцы приходили на острова, чтобы обменять европейские товары на золото, добываемое тысячами туземцев. Японцы в конце концов восстали против этого доминирования в их торговле и изгнали последних португальцев в 1624 году. Некоторым голландцам было разрешено остаться и торговать через определенные порты, но на самых унизительных условиях. По оценкам, в период с 1601 по 1764 год из Японии было вывезено около 3 763 572 унций золота. В настоящее время ежегодная добыча золота в Японии, включая Формозу, составляет около 6 000 000 долларов.

Большинство золото-кварцевых жил Японии разрабатывались на протяжении многих поколений, и остались только более бедные сульфидные зоны.

Остров Формоза, который был приобретен Японией в 1895 году, описывался ранними европейскими путешественниками как сокровищница неисчислимых богатств. Только в 1890 году были вновь открыты места старых разработок, а обнаружение чешуек золота во время строительства железной дороги спровоцировало приток китайских старателей на остров.

«Горное дело в Японии, прошлое и настоящее», Бюро горной промышленности, Министерство сельского хозяйства и торговли, Япония, 1909 г., стр. 17 и 64.

Общий объем добычи золота в Чосоне (Корее) в 1914 году составил около 5 000 000 долларов, но в настоящее время добыча снижается из-за аномального роста цен на химикаты и материалы, необходимые для добычи. Объем добычи за 1918 год, вероятно, не превысит 3 500 000 долларов, 60 процентов из которых будет получено на трех рудниках, эксплуатируемых иностранным капиталом. Основные золото-кварцевые рудники Чосона включены в американскую концессию в Унсане в провинции Северный Пхёнан, северо-западная Корея. С этих рудников получается около половины ежегодной добычи золота в Чосоне. Корея также содержит большое количество россыпных месторождений, в основном небольших, которые широко разрабатывались корейцами. Россыпные месторождения района Унсан еще не разрабатывались, но месторождения района Чиксан эксплуатируются японцами.

Торговые отчеты США, 26 февраля 1914 г.

Небольшие, разбросанные золотые месторождения Китая, как жильные, так и россыпные, разрабатываются почти исключительно китайцами, так как не было обнаружено ни одного месторождения, достаточно богатого, чтобы привлечь иностранный капитал. На острове Хайнань, к юго-востоку от материка, китайское правительство эксплуатирует рудники.

Геологоразведочные работы, проводимые в Китае до настоящего времени, не указывают на то, что страна когда-либо станет важным производителем золота. Даже в провинциях, обеспечивающих большую часть текущей добычи — Маньчжурии, Юньнани и Сычуани — золотодобывающая промышленность дает мало надежд на рост. В течение 1911, 1912 и 1913 годов в последних двух провинциях было обследовано 700 рек, и золото было найдено в 430, но ни в одном случае в количестве, достаточном для окупаемости работ.

Существует много слухов о золотых месторождениях обширной и неисследованной территории Тибета с самых первых экспедиций в эту страну, но эта область до сих пор закрыта для современного предпринимательства и даже для тщательного научного исследования. Несмотря на предыдущие сообщения, геолог, сопровождавший британскую экспедицию около 10 лет назад, заявил, что минеральная ценность Тибета не является легко очевидной. Рядом с границей штата Бутан есть много колоний золотоискателей. Тибетское золото встречается в виде самородков, а также в виде блесток и пыли, но говорят, что тибетцы стараются оставлять самородки нетронутыми или заменять их, если они были потревожены, полагая, что они живые и являются родителями блесток и пыли, или корнями, из которых растет новое золото, которое исчезло бы, если бы комки были удалены.

Торговые отчеты США, 26 февраля 1914 г.

Сиам, Бирма, Индокитай и Федеративные Малайские Штаты в настоящее время вносят лишь небольшую часть в добычу золота в Азии. Исследования и разведка ведутся активно, и результаты на сегодняшний день благоприятны. Будущие разработки могут подтвердить утверждения древних писателей и картографов о том, что в этом регионе было много золота. Известно, что золото и другие минералы существуют в Афганистане, но, за исключением золотого рудника недалеко от Кандагара, находящегося под управлением европейца, минеральные ресурсы почти полностью не освоены.

Африка

С 1905 года Южная Африка, включая Трансвааль, Капскую колонию и Наталь, является ведущим производителем золота в мире, позиция, которая была бы достигнута на несколько лет раньше, если бы не помешала Англо-бурская война. В 1917 году было добыто золота на сумму 186 255 000 долларов, или почти половина мирового объема, причем большая часть была получена из Витватерсранда, или Ранда, недалеко от Йоханнесбурга, Трансвааль. Добыча в 1918 году упала до 174 068 000 долларов.

Золото было впервые обнаружено в Трансваале в 1870 году, но добыча не имела большого значения до открытия золота на ферме Ланглаагте, Витватерсранд, в 1885 году. Рудники разбросаны вдоль пояса, простирающегося примерно на 62 мили от Рандфонтейна на западе до Холфонтейна на востоке. Этот пояс содержит крупнейшее месторождение золота, которое когда-либо было найдено в одном месте, и его содержание золота, вероятно, равно содержанию всех остальных известных золотых месторождений мира вместе взятых. Руда не является исключительно высокосортной, но может экономично перерабатываться в больших количествах. По оценкам, месторождение может представлять от 3 000 000 000 до 4 000 000 000 долларов с площади около 40 квадратных миль, из которых около половины было добыто к 1916 году.

Золото встречается как в жильных, так и в россыпных месторождениях в Натале и Капской колонии, но объем добычи невелик.

Родезия, занимавшая седьмое место в 1913 году, в последние годы быстро развивалась как производитель золота и сейчас превосходит Мексику. Согласно португальским записям, золото добывалось в Родезии еще в 1788 году. Открытие в 1866 году древних руин и древних золотых рудников в Зимбабве породило гипотезу о том, что Родезия была библейским Офиром. Хотя предпринимались многочисленные попытки открыть золотые месторождения, никакого успеха не было достигнуто до 1891 года, и только в нынешнем столетии был признан истинный характер родезийских золото-кварцевых жил. Заселение страны и развитие рудников — результат усилий Сесила Родса и «Чартер Компани».

Золото широко распространено, и большинство рудников небольшие. Будущее страны как производителя золота, по-видимому, зависит от разработки низкосортных рудных тел крупными компаниями. Рудник «Шамва» — яркий пример.

Западная Африка, особенно Золотой Берег, является единственным регионом Африки, помимо Трансвааля и Родезии, производящим золото в значительных количествах. Объем добычи британских колоний в Западной Африке в 1917 году составил около 7 500 000 долларов. Нездоровый климат региона, вероятно, будет препятствовать в течение нескольких лет любым масштабным горным операциям со стороны белых людей.

Золотые рудники также разрабатываются в Абиссинии, Бельгийском Конго, Египте, Французской Экваториальной Африке, бывшей Германской Восточной Африке, на Мадагаскаре и в Судане, но общая ежегодная добыча всех этих стран составляет немногим более 2 000 000 долларов. Наскальные рисунки и иероглифы Древнего Египта указывают на то, что северная Африка и регион вдоль реки Нил были важными источниками золота древнего мира.

Австралазия

В течение многих лет Австралазия была близким соперником Соединенных Штатов как производителя золота, часто превосходя эту страну. С 1903 года наблюдается быстрое снижение, и добыча в Австралазии в 1917 году составила менее половины добычи Соединенных Штатов. Однако Австралазия по-прежнему занимает третье место и произвела 11,3 процента от мирового объема в 1913 году и около 8,3 процента в 1917 году.

Австралия.

— Золото было обнаружено в Австралии в 1839 году, а возможно, даже еще в 1823 году. Опасаясь дестабилизирующего эффекта золотоискательства на прогресс колонии, правительственные власти держали эти ранние открытия в секрете в течение ряда лет. Однако в 1851 году старатель, недавно вернувшийся из Калифорнии, обнаружил золото возле Батерста в Новом Южном Уэльсе, и началась «золотая лихорадка», подобная калифорнийской. За этим последовали открытия в других частях страны. Жильные месторождения Австралии встречаются в двух отдельных областях, хорошо разделенных как географически, так и геологически. Первая включает золотые месторождения запада и северо-запада, а другая лежит вдоль великого Восточного Кордильерского хребта Австралии и простирается на север от Тасмании через Викторию, Новый Южный Уэльс и Квинсленд.

В течение многих лет Виктория, самый маленький из штатов, была крупнейшим производителем золота и к 1908 году произвела около половины общего объема добычи содружества. Среди ранних находок были одни из самых крупных известных самородков. С открытием в 1892 году сенсационного месторождения Кулгарди в Западной Австралии, штате, который ранее считался лишенным минеральных богатств, Виктория опустилась на второе место. Калгурли — главный город и центр золотодобывающего района в Западной Австралии.

Квинсленд занимает место после Виктории. В 1858 году произошла катастрофическая «золотая лихорадка», и от 15 000 до 20 000 человек остались голодать на берегах реки Фицрой. Людей спасли пароходы, отправленные правительствами Нового Южного Уэльса и Виктории. Несколько лет спустя аллювиальное золото было найдено возле Пик-Даун, Клермонт, который до сегодняшнего дня является основным россыпным районом Квинсленда. Чартерс-Тауэрс, нынешнее ведущее месторождение штата, было открыто в 1872 году. Рудник «Маунт-Морган» — это изолированный рудник, расположенный недалеко от места злополучной «лихорадки» 1858 года. Это, безусловно, самый продуктивный рудник Квинсленда, как по золоту, так и по меди. Новый Южный Уэльс, хотя и был первым австралийским штатом, давшим золото в сколько-нибудь значительных количествах, сейчас занимает четвертое место. Тасмания и Южная Австралия производят лишь небольшое количество золота.

Новая Зеландия.

— В 1852 году, через год после богатых открытий в Австралии, золотой песок и золото в кварце были найдены в Новой Зеландии, примерно в 40 милях от Окленда, но это открытие оказалось малозначительным. Десять лет спустя были открыты богатые россыпи Габриэльс-Галли, открытие, которое привлекло «лихорадку» с австралийских месторождений. Золотые месторождения Новой Зеландии можно разделить на три четко определенных и хорошо разделенных района: золотое месторождение Хуараки, которое содержит ценные жильные месторождения, но не содержит россыпей; район Западного побережья, в котором жильные и аллювиальные проявления имеют равное значение; и район Отаго, в котором золотоносные аллювиальные гравии важны, а немногие известные кварцевые жилы имеют небольшую экономическую ценность.

Некоторое количество золота добывается в других частях Австралазии, особенно в Британской и Голландской Ост-Индии, а также в Британской Новой Гвинее. Месторождения, не имеющие большого значения, отмечены в Новой Каледонии, на островах Фиджи и в бывшей Германской Новой Гвинее.

ВЕРОЯТНЫЕ ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРЕДЕЛЕНИИ В БЛИЖАЙШЕМ БУДУЩЕМ

Конкретные прогнозы относительно изменений в географическом распределении источников мирового золота кажутся бесполезными. В течение последних нескольких лет добыча золота на основных месторождениях снизилась. Помимо любого снижения, связанного с войной и сопутствующей нехваткой рабочей силы и высокими затратами на добычу, представляется вероятным, что мировая добыча золота достигла своего зенита и следует ожидать дальнейшего снижения, если только к известным запасам не будут добавлены новые рудные тела или не будет открыт какой-либо революционный метод извлечения золота из низкосортных руд.

Хотя ведущие месторождения — Южная Африка, Соединенные Штаты и Австралия — по-видимому, достигли или прошли свой период наибольшей добычи, существует ряд месторождений в нестабильных и неисследованных регионах мира, от которых можно ожидать увеличения добычи. О возможностях Сибири уже упоминалось, и многие инженеры придерживаются мнения, что этот регион в конечном итоге составит конкуренцию Южной Африке. Южная Америка произвела огромное количество золота, главным образом аллювиального, и ожидается, что в будущем она даст увеличенный объем добычи. Будущее Южной Африки проблематично.

В течение последнего полувека значительно возросшая добыча золота была обусловлена главным образом эксплуатацией низкосортных объектов, что стало возможным благодаря улучшениям в горном деле и металлургии. Кажется, однако, что это развитие достигло точки, когда чрезмерные затраты на рабочую силу препятствуют использованию руд еще более низкого качества.

В целом, следовательно, можно ожидать, что мировая добыча золота останется на прежнем уровне или снизится, по крайней мере до тех пор, пока уровень цен не изменится настолько, что станет выгодным расходовать капитал на разведку и освоение до сих пор неисследованных регионов.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Политический контроль можно резюмировать следующим образом:

Country | Percentage of 1913 production
British Empire | 62.9 
United States | 19.3 
Russia and Siberia |  5.8 
Japan |  1.8 
France |  1.4 
Belgium |  0.2 
Central Power |  0.55
Mexico |  4.2 
Other Countries |  3.7 

Великобритания политически контролировала 62,9 процента добычи 1913 года через государственный суверенитет над Трансваалем, Австралией, Родезией, Канадой и Индией. Другими британскими владениями, вносящими небольшие количества в мировой объем добычи, являются Британский Гондурас, Британская Гвиана, Британская Западная Африка, Британская Новая Гвинея, Новая Зеландия, Британская Ост-Индия, Египет и Британские острова. Все золото, добытое в Британской империи, должно отправляться в Англию.

Соединенные Штаты политически контролировали 19,3 процента добычи 1913 года, практически вся она поступила из континентальной части Соединенных Штатов. Филиппинские острова и Пуэрто-Рико произвели небольшие количества.

Россия является одним из основных поставщиков мировых запасов золота, производя 5,8 процента от объема 1913 года. Большая часть этих 5,8 процента поступила с рудников Сибири, и политический контроль над этим регионом до сих пор не урегулирован. Мексика, с объемом добычи, равным 4,2 процента от мирового итога, была крупнейшим производителем среди нейтральных держав во время войны. Франция контролировала 1,4 процента мирового итога, треть поступила с рудников во Франции, а остальная часть — из французских колоний в Южной Америке и Африке. Япония контролировала 1,8 процента, 1 процент поступил с японских островов и Формозы, а остальная часть — из Кореи. Остальная часть добычи 1913 года, составляющая около 4 процентов, была широко разбросана и контролировалась рядом стран Южной Америки, Европы и Азии.

Следует отметить, что, хотя Великобритания и Соединенные Штаты политически контролируют важные добывающие месторождения настоящего времени, все из которых, по-видимому, достигли своего максимального объема добычи, контроль над месторождениями, которые, как ожидается, станут важными производителями в будущем, находится в других руках.

Во время войны, особенно в ее последние месяцы, большинство воюющих стран и некоторые нейтральные страны ввели ограничения на экспорт золота, как в слитках, так и в виде изделий. В нормальное время золоту разрешено свободно перемещаться между странами по мере необходимости для урегулирования международных торговых балансов.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Коммерческий контроль над золотыми ресурсами мира показан в Таблице 68 и на Рисунке 20. При изучении таблицы и диаграммы читатель должен помнить, что цифры и проценты в лучшем случае являются лишь оценками. Большинство золотых рудников принадлежат компаниям, чьи акции являются акциями на предъявителя; они покупаются и продаются на фондовых рынках многих финансовых центров. Сегодня контроль может быть в руках одной группы, завтра — в руках другой. Из-за этой постоянно меняющейся собственности трудно определить национальность коммерческого контроля, особенно когда есть попытки скрыть национальность инвестированного капитала. Однако считается, что таблица и диаграмма приблизительно верны. Информация, на которой они основаны, была получена из горнодобывающих справочников, отчетов горнодобывающих компаний, отчетов консульских агентов в различных странах и путем личных интервью с горными инженерами.

Рис. 20. — Политический и коммерческий контроль над добычей золота в мире.

Таблицу 68 можно резюмировать следующим образом:

Коммерческий контроль над золотыми ресурсами

Country | Percentage of 1917 production
British Empire | 63.0 
United States | 23.0 
France |  5.6 
Russia |  2.1 
Japan |  1.7 
China |  0.84
Belgium |  0.5 
Brazil |  0.07
Germany |  0.81
Mexico |  0.21
Unclassified |  1.9 

Интересно отметить, что политический контроль и коммерческий контроль практически идентичны в случае Британской империи и Соединенных Штатов. Французский контроль гораздо важнее коммерчески, чем политически. В других странах доступно мало внутреннего капитала, и политический контроль гораздо сильнее коммерческого.

Коммерческий контроль, если он отличается от политического, вступает в проверку сил с ним в периоды чрезвычайных ситуаций или беспорядков, в результате чего более сильный подавляет более слабого. Что касается правительств, которые достаточно сильны и стабильны, недавняя война показала, что устранение иностранного капитала, инвестированного в страну, легко. Соединенные Штаты и Великобритания, в частности, взяли под контроль большое количество компаний, ранее принадлежавших немецким интересам. Однако там, где правительство не столь сильно, коммерческий контроль, подкрепленный во многих случаях более энергичными правительствами стран, откуда поступает инвестированный капитал, побеждает, и таким образом определяются политические события, вплоть до свержения более слабого правительства. Так, свержение бурского правительства и рождение Британской Южной Африки стало результатом столкновения между британским коммерческим контролем и бурским политическим контролем.

Вопрос контроля над запасами золота обсуждается в отчете золотого комитета Министерства внутренних дел. Контроль над запасами в 1916 году показан графически на Рисунке 21 и обсуждается более подробно в следующем разделе: «Положение ведущих коммерческих наций».

Отчет комитета, назначенного Министром внутренних дел для изучения ситуации с золотом.

Золотые рудники Соединенных Штатов контролируются в основном американским капиталом. Несколько рудников преимущественно британские, и акции других горнодобывающих компаний, несомненно, удерживаются в Лондоне, но общая добыча, контролируемая Великобританией, невелика. По оценкам, в последние годы 95 процентов ежегодного объема добычи контролировалось американцами, а остальная часть — британцами.

Более половины золота, добываемого в Канаде, поступает из провинции Онтарио, главным образом из района Поркьюпайн. В 1917 и 1918 годах рудник «Холлинджер», принадлежащий компании «Холлинджер Голд Майнз, Лтд.», был основным производителем. Это один из величайших золотых рудников в мире, выплативший более 9 000 000 долларов дивидендов к концу 1918 года. Контроль над компанией удерживается в Соединенных Штатах. Другим важным рудником в районе Поркьюпайн является «Макинтайр», принадлежащий компании «Макинтайр Поркьюпайн Майнз, Лтд.», также американской. В провинции Британская Колумбия крупнейшим добывающим лагерем является Россленд, эксплуатируемый компанией «Консолидейтед Майнинг энд Смелтинг Ко.», контролируемой капиталом Соединенных Штатов и Канады. По оценкам, около двух третей золотых рудников Канады контролируются капиталом Соединенных Штатов, а оставшаяся одна треть — британским капиталом, включая канадский.

Table 68.—Financial Control of the Gold Production of the World, 1917
(Percentages are only approximate)

Country | Production 1917 (in dollars) | 1917 Production controlled financially by— | Remarks
United States | United Kingdom | France | Belgium | Japan | China | Russia | Brazil | Total Allies | Germany | Mexico | Unclassified
North America: |  |  |  |  |  |  |  |  |  |  |  |  |  |
United States | $83,750,700 | $79,563,165 | $4,187,535 | ... | ... | ... | ... | ... | ... | $83,750,700 | ... | ... | ... | 95 per cent. by United States capital; 5 per cent. by British.
Canada | 15,200,000 | 10,000,000 | 5,200,000 | ... | ... | ... | ... | ... | ... | 15,200,000 | ... | ... | ... | 66 per cent. by United States capital; 33 per cent. by British.
Mexico | 9,000,000 | 2,700,000 | 3,600,000 | $900,000 | ... | ... | ... | ... | ... | 7,200,000 | $900,000 | $900,000 | ... | Capital control: British 40 per cent.; United States 30 per cent.; French 10 per cent.; German 10 per cent. and Mexican 10 per cent.
Central America | 3,122,000 | 750,000 | 750,000 | ... | ... | ... | ... | ... | ... | 1,500,000 | ... | ... | $1,622,000 | 50 per cent. by natives; 25 per cent. each by United States and Great Britain.
South America: |  |  |  |  |  |  |  |  |  |  |  |  |  |
Argentina | 4,600 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 4,600 |
Bolivia | 115,000 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 115,000 |
Chile | 200,000 | 200,000 | ... | ... | ... | ... | ... | ... | ... | 200,000 | ... | ... | ... |
Brazil | 2,958,000 | ... | 2,662,200 | ... | ... | ... | ... | ... | $295,800 | 2,958,000 | ... | ... | ... | 90 per cent. by British capital.
Colombia | 6,200,000 | 620,000 | 3,000,000 | 900,000 | $620,000 | ... | ... | ... | ... | 5,140,000 | ... | ... | 1,060,000 | Capital control: 50 per cent. British; 15 per cent. French; 10 per cent. Belgian; 10 per cent. United States; and 15 per cent. local.
Guiana: |  |  |  |  |  |  |  |  |  |  |  |  |  |
British | 600,000 | ... | 600,000 | ... | ... | ... | ... | ... | ... | 600,000 | ... | ... | ... |
Dutch | 400,000 | ... | 125,000 | 125,000 | ... | ... | ... | ... | ... | 250,000 | ... | ... | 150,000 |
French | 1,500,000 | ... | ... | 1,500,000 | ... | ... | ... | ... | ... | 1,500,000 | ... | ... | ... |
Peru | 1,300,000 | 1,300,000 | ... | ... | ... | ... | ... | ... | ... | 1,300,000 | ... | ... | ... |
Other S. America | 1,357,000 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 1,357,000 |
Europe: |  |  |  |  |  |  |  |  |  |  |  |  |  |
Austria-Hungary | [176]2,179,000 | ... | ... | ... | ... | ... | ... | ... | ... | ... | [176]2,179,000 | ... | ... |
France | 700,000 | ... | ... | 700,000 | ... | ... | ... | ... | ... | 700,000 | ... | ... | ... |
Germany | [176]135,600 | ... | ... | ... | ... | ... | ... | ... | ... | ... | [176]135,600 | ... | ... |
Great Britain | 5,000 | ... | 5,000 | ... | ... | ... | ... | ... | ... | 5,000 | ... | ... | ... |
Italy | 2,000 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 2,000 |
Russia and Siberia | 18,000,000 | ... | 9,000,000 | ... | ... | ... | ... | $9,000,000 | ... | 18,000,000 | ... | ... | ... | Large part of Russian production probably controlled by German capital. Situation uncertain.
Serbia | [176]328,000 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | [176]328,000 |
Sweden | 10,000 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 10,000 |
Turkey | [176]500 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | [176]500 |
Asia: |  |  |  |  |  |  |  |  |  |  |  |  |  |
China | $3,600,000 | ... | ... | ... | ... | ... | 3,600,000 | ... | ... | 3,600,000 | ... | ... | ... | Probably controlled largely by Japanese and other foreign capital.
Chosen (Korea) | 4,444,000 | $2,500,000 | ... | ... | ... | $1,944,000 | ... | ... | ... | 4,444,000 | ... | ... | ... | Part of production credited to Japan controlled by British.
Dutch East Indies | 2,818,000 | ... | $2,100,000 | ... | ... | ... | ... | ... | ... | 2,100,000 | ... | ... | 718,000 |
Federated Malay States | 342,300 | ... | 342,300 | ... | ... | ... | ... | ... | ... | 342,300 | ... | ... | ... |
French Indo-China | 50,000 | ... | ... | $50,000 | ... | ... | ... | ... | ... | 50,000 | ... | ... | ... |
Japan and Formosa | 5,595,200 | ... | ... | ... | ... | 5,595,200 | ... | ... | ... | 5,595,200 | ... | ... | ... |
India and British Indies | 10,756,800 | ... | 10,756,800 | ... | ... | ... | ... | ... | ... | 10,756,800 | ... | ... | ... |
Australasia | 35,945,500 | ... | 35,945,500 | ... | ... | ... | ... | ... | ... | 35,945,500 | ... | ... | ... | Before war considerable capital controlled by Germans. Small blocks now owned by Dutch and Belgians.
Africa: |  |  |  |  |  |  |  |  |  |  |  |  |  |
Belgian Congo | 2,000,000 | 500,000 | ... | ... | 1,500,000 | ... | ... | ... | ... | 2,000,000 | ... | ... | ... | 25 per cent. by American capital.
Egypt and Sudan | 150,000 | ... | 150,000 | ... | ... | ... | ... | ... | ... | 150,000 | ... | ... | ... |
German East Africa | [176]253,200 | ... | ... | ... | ... | ... | ... | ... | ... |  | [176]253,200 | ... | ... |
Madagascar | 1,000,000 | ... | ... | 1,000,000 | ... | ... | ... | ... | ... | 1,000,000 | ... | ... | ... |
Rhodesia | 14,988,600 | ... | 14,988,600 | ... | ... | ... | ... | ... | ... | 14,988,600 | ... | ... | ... |
Transvaal | 186,254,256 | ... | 167,629,256 | 18,625,000 | ... | ... | ... | ... | ... | 186,254,256 | ... | ... | ... | Before war controlled in large part by German interests. At present: British, 90 per cent.; French, 10 per cent.
West Africa (British) | 7,435,488 | ... | 7,435,488 | ... | ... | ... | ... | ... | ... | 7,435,488 | ... | ... | ... | Probably all controlled by British capital.
Undistributed | 2,785,656 | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | ... | 2,785,656 |
Total (1917) | $422,590,100 | $98,133,165 | $268,477,679 | $23,800,000 | $2,120,000 | $7,539,200 | $3,600,000 | $9,000,000 | $295,800 | $412,965,844 | $3,467,800 | $900,000 | $8,152,756 |
Total (including 1913 figures) | $425,486,400 |  |  |  |  |  |  |  |  |  |  |  |  |
Per cent. of world production | 100 | 23 | 63 | 5.6 | 0.5 | 1.7 | 0.84 | 2.1 | 0.07 | 96.81 | 0.81 | 0.21 | 1.9 |

[176] Добыча в 1913 г. Более поздние данные отсутствуют.

Золотые рудники Мексики принадлежат британскому, американскому и французскому капиталу в указанном порядке. Основными горнодобывающими компаниями округа Эль-Оро, ведущего золотодобывающего района республики, являются El Oro Mining & Railway Co., Ltd., Esperanza, Ltd. и Dos Estrellas Mining Co. Британский капитал контролирует El Oro Mining & Railway Co., Ltd. и 51 процент акций Esperanza, Ltd., остальные 49 процентов контролируются американцами. В последние годы французы приобретают контроль над горнодобывающими предприятиями в округе Эль-Оро. В настоящее время им принадлежат Dos Estrellas Mining Co. и Mexico Mines of El Oro, Ltd. Обе компании ранее контролировались из Лондона. Рудник Долорес в западной части штата Чиуауа, один из знаменитых золотых рудников Мексики, принадлежит Mines Company of America, американской корпорации.

Рис. 21. — Запасы золота в банках, государственных казначействах и в обращении в основных странах мира в 1916 г.

В штате Дуранго золотые рудники, большинство из которых также добывают серебро, принадлежат American Smelting & Refining Co. (американская), Bacis Gold & Silver Mines Co. (британская) и Inde Gold Mining Co. (американская). Большинство золото-серебряных рудников штата Гуанахуато были освоены американским капиталом. Штат Синалоа становится золотодобывающим регионом; рудники Пальмарито в округе Мокорито и Минас-де-Тахо в Росарио принадлежат американским интересам. Золото встречается в медных рудах Соноры. Большинство рудников округа контролируется американцами.

Рудники Чиуауа, Идальго и Сакатекаса являются преимущественно серебряными, но их руды содержат некоторое количество золота. В Чиуауа, вероятно, преобладает американский капитал, за которым следует британский. В последние годы германские интересы через American Metal Co. и ее дочерние предприятия приобретают контроль над собственностью в Чиуауа и других частях Мексики. Германский капитал также инвестирован в Сакатекас, причем основная компания контролируется A. Goerz & Co., Ltd. Рудники штата Идальго, ведущего серебродобывающего округа Мексики, принадлежат американскому, британскому и мексиканскому капиталу.

Золотые рудники Центральной Америки [177] в настоящее время имеют некоторое значение, и добыча в будущем может несколько возрасти. Рудники по большей части принадлежат американскому и британскому капиталу в указанном порядке. Дочерние компании United Fruit Co. и Tonopah Mining Co., обе американские, эксплуатируют предприятия в Коста-Рике и Никарагуа.

[177] «Инвестиции в Латинской Америке и на Британских Антильских островах», серия «Специальный агент» № 169, Бюро внешней и внутренней торговли, Министерство торговли США, 1918 г.

В Колумбии, ведущей золотодобывающей стране Южной Америки, большинство крупных компаний являются британскими, наиболее важными из которых являются Pato Mines, Nechi Mines, а также Frontino and Bolivia Mines. Бельгийская компания Platinum & Gold Concessions of Colombia, Ltd. и французская компания San Antonio Gold Mines Co., Ltd. недавно приобрели концессии на добычу золота. Американский капитал также инвестирован в эту отрасль.

Две наиболее важные горнодобывающие компании Бразилии, St. John del Rey Mining Co., Ltd. и Ouro Preto Gold Mines of Brazil, Ltd., находятся под британским управлением. Некоторый французский капитал заинтересован в последнем предприятии. Большинство рудников Французской Гвианы контролируется французскими компаниями. В остальных южноамериканских странах добыча золота имеет сравнительно небольшое значение. Добыча в значительной степени контролируется британским и американским капиталом.

Иностранный капитал, инвестированный в рудники Сибири и России, является преимущественно британским, хотя известно, что Германия проявляла большой интерес к этой отрасли. Некоторый российский капитал, особенно предоставленный крупными российскими банками, был инвестирован в сибирские горнодобывающие предприятия. Горное законодательство старой Российской империи предусматривало, что минеральные ресурсы могут находиться во владении как иностранных, так и российских компаний на основании концессий или договоров аренды, предоставленных короной, или на основании аренды у российских землевладельцев. Во многих случаях иностранные капиталисты создавали холдинговые компании для приобретения контрольного пакета акций российской компании, от имени которой велось владение и эксплуатация предприятия. Большинство этих холдинговых компаний имели свои главные офисы в Лондоне, и большинство директоров были британскими подданными. Контроль, по-видимому, был британским. Однако акции компаний были на предъявителя и широко торговались на Петроградской бирже.

Самый важный золотодобывающий округ Сибири находится в Иркутской губернии, на реке Лене. Российская компания «Ленское золотопромышленное товарищество» эксплуатирует основные предприятия этого округа с 1863 года. Директорами компании являются российские евреи. Британская компания Lena Goldfields, Ltd. владела 70 процентами акций Ленского товарищества, но в 1917 году завершила продажу 51 000 акций петроградской группе, включая Imperial Foreign Corporation, Ltd. и Русско-Английский банк. Lena Goldfields, Ltd. в настоящее время владеет менее чем 10 процентами акций Ленского товарищества.

Пирито-медный рудник, приносящий достаточно золота в качестве побочного продукта для обеспечения прибыли, расположен в Пермской губернии, в южном районе Уральских гор, и принадлежит Кыштымским горным заводам — российской компании, контролируемой Kyshtim Corporation, Ltd. из Лондона. Компания владеет крупной концессией, включающей леса, фермы и минеральные земли. Контроль над Kyshtim Corporation, по-видимому, является британским.

Tanalyk Corporation контролируется практически теми же интересами, что и Kyshtim Corporation, и была организована для приобретения полного контроля над Южно-Уральским горнопромышленным и плавильным обществом. Собственность компании, расположенная в Орском уезде Оренбургской губернии на Южном Урале, является лишь перспективным участком и не была полностью освоена. Она включает общую площадь 28 350 акров лесных и минеральных земель. Руда содержит медь, золото и серебро, причем содержание меди является наиболее ценным. В течение 1917 года акции, удерживаемые в Кыштымских горных заводах и Южно-Уральском горнопромышленном и плавильном обществе, были переданы Canadian Development Corporation, Ltd., компании, зарегистрированной в Канаде, вероятно, с целью уклонения от высоких британских подоходных налогов. Передача не повлекла за собой изменения контроля, поскольку две британские холдинговые компании, Kyshtim Corporation и Tanalyk Corporation, Ltd., контролируют канадскую компанию.

Колчанский россыпной прииск в Охотском горном округе Восточной Сибири был взят в аренду британской компанией Orsk Goldfields, Ltd. у Русско-Азиатского банка с выплатой роялти, основанного на валовой добыче золота. Orsk Goldfields, Ltd. первоначально контролировала золотодобывающее предприятие в Оренбургской губернии на Южном Урале, но отказалась от аренды и опциона.

В Сибири добывается большое количество золота в качестве побочного продукта медных, свинцовых и цинковых рудников. Контроль над этими рудниками во многом совпадает с контролем над вышеупомянутыми золотыми предприятиями — британский с российскими акционерами, главным образом представителями российских банков.

Японский контроль расширяется, особенно в Восточной Сибири. В японской прессе в ноябре 1918 года сообщалось, что специальная финансовая миссия Японии планирует создание японо-российского партнерского предприятия, аналогичного Японо-Китайской промышленной ассоциации, с целью получения от российских властей прав на горнодобывающие и лесные районы Сибири и эксплуатации природных ресурсов Сибири. Предлагалось, чтобы среди инвесторов партнерства были российские капиталисты, Южно-Манчжурская железная дорога, East Asia Development Co., Японо-Китайская торговая ассоциация и капиталисты стран Антанты.

Практически вся добыча Индии поступает с рудников рифа Колар в Майсуре. Существует шесть крупных добывающих компаний: Champion Reefs Mining Co., of India, Ltd.; Gold Fields of Mysore and General Exploration, Ltd.; Mysore Gold Mining Co., Ltd.; Nundydroog Co., Ltd.; Balaghat Gold Mining Co., Ltd.; и Ooregum Gold Mining Co. of India, Ltd. Все эти компании являются британскими и принадлежат тесно связанным интересам. Другими действующими компаниями в Индии являются Hutti (Nizam’s) Gold Mines, Ltd. в Хайдарабаде (Южная Индия), а также Northern Anantapur Gold Mines, Ltd. и Jibutil (Anantapur) Gold Mines, Ltd. в президентстве Мадрас; все они являются британскими компаниями.

В Японии государство оставляет за собой право первоначальной собственности на все руды и предоставляет отдельным лицам или компаниям право на разработку месторождений. Согласно закону 1890 года, иностранец не имел права работать на руднике и не мог стать членом горнодобывающего предприятия, поэтому право на разработку рудников было исключительно зарезервировано за японскими подданными. Согласно поправке к горным правилам 1900 года, деловым предприятиям, организованным японцами или иностранцами, или и теми и другими, теперь разрешено разрабатывать рудники при условии, что такие предприятия подчиняются японским законам. Недавно в японский парламент был внесен законопроект, предлагающий предоставить иностранцам привилегии на добычу полезных ископаемых и имущественные права. Японский капитал имеет почти полный контроль над золотыми рудниками империи.

Основные золотые рудники принадлежат следующим компаниям: Tanak Chobei (Формоза), Mitsubishi & Co. (Садо), Shimadzu Tadashige (Сацума), Fujita & Co. (Рикутю и Формоза), Kimura Kintaro (Формоза) и Ushio Gold Mine Co. (Сацума).

Наиболее ценные минеральные концессии Чосена (Кореи), включая золото, находятся в руках иностранных компаний, большинство из которых — американские. Oriental Consolidated Mining Co., американская компания, контролирует рудники Унсан в провинции Северная Пхёнан на северо-западе Кореи, самое важное золотодобывающее предприятие страны. Концессия включает 600 квадратных миль на реке Анджу и действует около 21 года с правом продления на 15 лет. Эксплуатирующая компания ежегодно выплачивает 15 000 долларов корейскому правительству. Запасы руды на 1 июля 1916 года оценивались в 852 000 тонн стоимостью 4 823 000 долларов.

Рудники Чиксан в провинции Южная Чхунчхон также управляются американским капиталом. Рудники Суан в провинции Хванхэ первоначально контролировались британской компанией, но были сданы в аренду американской компании. Итальянская компания владеет рудниками в провинции Северная Пхёнан, а британская компания ведет деятельность в провинции Северная Чхунчхон. Германская компания владела рудниками, не находящимися в полной эксплуатации, в провинции Северная Пхёнан, но эти предприятия, несомненно, были конфискованы японским правительством. Японские и корейские горняки владеют и эксплуатируют небольшие рудники страны, добыча на которых значительно сократилась в последние годы.

Хотя добыча золота в Китае в 1917 году составила 3 600 000 долларов, месторождения невелики, широко разбросаны и принадлежат и эксплуатируются почти исключительно местными горняками. Некоторые из более крупных рудников финансировались правительствами провинций. В некоторых провинциях владельцам горнодобывающей собственности не разрешается искать инвестиции иностранного капитала, если они не в состоянии финансировать предприятие в пределах провинции. В последние годы во многих частях страны проводились геологоразведочные работы, но не было обнаружено месторождений, достаточно перспективных для привлечения иностранных инвесторов. Учитывая их активность в освоении других природных ресурсов Китая, вполне вероятно, что японцы попытаются взять отрасль под свой контроль, если будут обнаружены какие-либо важные месторождения.

В Трансваале все минералы принадлежат государству, а не владельцам поверхности земли. Когда золото или любой другой минерал обнаружен, часть территории (менее половины) резервируется за владельцем земли, другая часть — за первооткрывателем минерала, а остальная часть открыта для подачи заявок. В настоящее время право собственности на минеральные земли сохраняется за государством. Право на эксплуатацию минеральных богатств предоставляется в аренду лицу, предложившему наивысшую цену, при этом ставки основаны на проценте от прибыли, дифференцированном в зависимости от эксплуатационных расходов и качества руды. Налог в размере 10 процентов на прибыль, с учетом амортизации капитала, взимается со всех золотодобывающих предприятий.

До войны практически все золотые рудники Витватерсранда контролировались британским и германским капиталом. Первая американская компания вышла на рынок в 1917 году, также был инвестирован некоторый французский капитал. Позиции Германии были сильны, так как германские компании контролировали половину, а возможно, и больше капитала, инвестированного в золотые рудники. Отчет южноафриканского куратора по делам вражеской собственности, опубликованный в начале 1918 года, показал, что не менее 26 000 вражеских акционеров в золотодобывающих, угольных и других горнодобывающих предприятиях Союза владели акциями совокупной номинальной стоимостью 37 500 000 долларов. Поскольку золото является, безусловно, самым важным минералом Трансвааля, вероятно, что большая часть этого германского капитала была инвестирована в золотые рудники. Вражеские фирмы были ликвидированы или перешли в добровольную ликвидацию, а вражеские акции в горнодобывающих корпорациях номинальной стоимостью 24 000 000 долларов были взяты под контроль куратором по делам вражеской собственности. [178]

[178] «Engineering and Mining Journal», 11 мая 1918 г., стр. 888.

Контроль над золотыми рудниками Трансвааля сосредоточен в следующих шести компаниях: Central Mining & Investment Corporation, Consolidated Mines Selection Co., Johannesburg Consolidated Investment Co., Consolidated Goldfields of South Africa, Union Corporation (ранее Ed Goerz & Co.) и General Mining & Finance Corporation. Последние две компании до войны были полностью германскими. Central Mining & Investment Corporation контролирует, вероятно, 50 процентов добычи округа. Американский капитал заинтересован в Consolidated Mines Selection Co. Другая американская компания, Anglo-American Corporation of South Africa, Ltd., была зарегистрирована в Претории 25 сентября 1917 года с выпущенным капиталом в 1 000 000 фунтов стерлингов. Непосредственной целью корпорации является участие в торгах на аренду определенных золотодобывающих площадей на Дальнем Восточном Ранде. [179]

[179] U. S. Commerce Reports, 15 декабря 1917 г., стр. 1033.

Сообщалось, что французский капитал контролирует около 10 процентов годовой добычи. В течение многих лет большинство горных инженеров в Трансваале были американцами.

Немцы не только приобрели значительный контроль посредством инвестирования капитала в горнодобывающие предприятия, но и осуществляли контроль через торговлю горношахтным оборудованием. Компания Orenstein-Arthur Koppel Co. наладила важную торговлю рельсами, шахтными вагонетками и аналогичными припасами и продолжала вести бизнес даже после начала войны. Вскоре после потопления «Лузитании» толпа разрушила офисы компании в Йоханнесбурге и сожгла запас крайне необходимых припасов. С началом войны возникли опасения, что могут возникнуть серьезные препятствия для нормального хода золотодобывающей промышленности из-за возможных трудностей с получением достаточного количества цианида, ртути и цинка, используемых при извлечении золота, большая часть которых ранее поставлялась Германией. Однако необходимые материалы были получены из других источников.

Родезия контролируется British South African Co., организованной Сесилом Джоном Родсом, в честь которого была названа колония. Компания является полностью британской; она является правительством, взимает налоги, администрирует законы и контролирует горнодобывающую промышленность. Компаниям и частным лицам разрешено регистрировать горные отводы почти так же, как в Калифорнии. Goldfields Rhodesian Development Co., имеющая крупные родезийские горнодобывающие интересы, является ответвлением Consolidated Goldfields of South Africa. Можно с уверенностью сказать, что золотые рудники Родезии принадлежат и эксплуатируются полностью британским капиталом. Процентный налог взимается с добычи золотых рудников.

В Австралии до войны существовали почти те же условия, что и в Южной Африке. Крупные золотодобывающие компании были, по-видимому, британскими; их штаб-квартиры находились либо в Австралии, либо в Лондоне, а их директора и управляющие были британцами. Однако несомненно, что значительная часть германского капитала была инвестирована в эти компании. Среди важных добывающих компаний — Associated Gold Mines of Western Australia, Great Boulder Proprietary Mines, Ltd., Golden Horseshoe Estates Co., Ltd., Ivanhoe Gold Corporation, Ltd., все из Западной Австралии; Mount Morgan Gold Mining Co. из Квинсленда; Mount Boppy Gold Mining Co. и Mount Lyell Mining & Railway Co., Ltd. из Тасмании.

Благодаря энергичным действиям премьер-министра Австралии Уильяма М. Хьюза германский капитал был изгнан в начале войны из всех отраслей промышленности Содружества, включая золотые, свинцовые и цинковые рудники, плавильные и аффинажные заводы, а также закупочные организации. В январе 1916 года, чтобы обезопасить финансовое положение Содружества, премьер-министр издал указы, предусматривающие, что никакие новые выпуски акций компаний или увеличения капитала существующих компаний не будут разрешены без согласия казначея Содружества; что компании, зарегистрированные в Австралии, будут иметь три месяца на прекращение владения их акциями лицами вражеской национальности или происхождения, независимо от того, натурализованы они или нет; и что в будущем передача акций лицам вражеской национальности или происхождения не будет разрешена. [180]

[180] U. S. Commerce Reports, 21 февраля 1916 г., стр. 733.

Остальные страны мира имеют малое значение как производители золота; следовательно, обсуждение коммерческого контроля над их рудниками имело бы небольшую ценность. В большинстве из них горнодобывающие предприятия принадлежат и эксплуатируются отечественным капиталом, за исключением бывшей Австро-Венгерской империи. До войны британский капитал контролировал золотые рудники в Трансильвании.

Владение плавильными и обогатительными заводами мало влияет на коммерческий контроль над золотодобывающей промышленностью. Большинство крупных золотодобывающих компаний имеют собственные аффинажные заводы на рудниках, и поэтому контроль над плавильными заводами идентичен контролю над рудниками. Некоторое количество золота производится как побочный продукт при плавке свинца, серебра и меди, особенно в Соединенных Штатах, где плавильные заводы почти полностью контролируются американским капиталом. Дальнейшее обсуждение коммерческого контроля над плавильными и аффинажными заводами можно найти в главах XIV, XV и XXX.

Контроль над секретными процессами и патентами имеет меньшее значение в коммерческом контроле над золотодобывающей промышленностью, чем в любой другой минеральной отрасли. Отрасль своеобразна тем, что цена на золото всегда фиксирована и нет конкуренции за рынок. Контроль над усовершенствованным методом извлечения или аффинажа золота может позволить одной компании снизить затраты на добычу и переработку и тем самым обеспечить большую прибыль, но передача усовершенствованного процесса второй компании не обязательно приведет к снижению прибыли компании, которая его открыла.

ПОЛОЖЕНИЕ ВЕДУЩИХ КОММЕРЧЕСКИХ НАЦИЙ

Соединенные Штаты контролировали политически через государственный суверенитет 19,3 процента добычи золота в 1913 году, занимая место вслед за Великобританией. Коммерческий контроль был несколько выше, составляя примерно 23 процента добычи 1917 года. Рудники Соединенных Штатов принадлежат почти исключительно американцам, и американский капитал инвестирован во многие зарубежные месторождения. Более половины, возможно, до двух третей рудников Канады принадлежат корпорациям Соединенных Штатов. Крупнейшие корейские компании принадлежат или управляются американским капиталом. Две американские компании были недавно созданы в Трансваале. Вероятно, от 30 до 40 процентов золота, добываемого в Мексике в нормальное время, поступает с рудников, принадлежащих Соединенным Штатам. Добыча в Центральной и Южной Америке, хотя в настоящее время относительно незначительна, в значительной степени контролируется американцами.

Хотя Соединенные Штаты уступают по объему добычи Великобритании, они контролируют, безусловно, самые большие запасы золотых монет и слитков среди всех наций. В 1916 году в банках, национальных казначействах и в обращении в Соединенных Штатах находилось 2 299 454 000 долларов, что почти вдвое превышает сумму, которой обладает любая другая нация. В 1918 году эта сумма увеличилась до 3 050 000 000 долларов. Денежный резерв, вероятно, превышает общую добычу золота в Соединенных Штатах с момента начала ведения статистики добычи.

Учитывая тот факт, что государственный долг Соединенных Штатов невелик по сравнению с долгами других основных наций, финансовая система этой страны находится на относительно прочной основе. Когда придет время погашать непогашенные облигации и другие формы задолженности, накопленные во время войны, Соединенные Штаты, несомненно, будут в более выгодном положении, чем любая из других воюющих сторон.

Запасы золота в основных золотодобывающих странах в 1916 году показаны на диаграмме на рисунке 21.

Великобритания является ведущей золотодобывающей нацией мира. Британская империя контролировала политически 62,9 процента добычи 1913 года, а британский коммерческий контроль составлял приблизительно 63 процента. Незначительное количество золота добывается на Британских островах, но империя включает таких важных производителей золота, как Южная Африка, Австралия, Родезия, Индия и Канада. Британский капитал также контролирует золотые рудники в Сибири, Мексике, Южной Америке и Соединенных Штатах.

Несмотря на большой политический и коммерческий контроль, осуществляемый британцами, золотые запасы Британской империи были намного меньше, чем у Соединенных Штатов, и в 1916 году были превзойдены запасами Франции.

Земли, находящиеся под французским контролем, производят мало золота, добыча в 1913 году составила всего 1,4 процента от общемировой. Менее 0,5 процента поступило из самой Франции, а остальное было получено из Французской Гвианы и Мадагаскара. Однако французский капитал не ограничивался национальными границами и был инвестирован во многие основные месторождения, что подтверждается тем фактом, что коммерческий контроль составил 5,6 процента добычи 1917 года. В Мексике по меньшей мере 10 процентов капитала, контролирующего золотые рудники, является французским, и эта доля неуклонно растет. В Южной Америке — особенно в Колумбии, а также в Голландской и Французской Гвиане — некоторые крупные компании являются французскими, но большая часть золота, контролируемого коммерчески французами, поступает из Трансвааля. По оценкам, французские интересы контролируют около 10 процентов добычи Южной Африки с тех пор, как был устранен германский контроль. Золотой резерв Франции был велик до войны и занимал второе место после резерва Соединенных Штатов в 1916 году. Сейчас (1920 г.) он сократился до очень малых размеров.

Хотя Россия вместе с Сибирью является одним из самых перспективных потенциальных источников будущего предложения золота и произвела 5,8 процента от общего объема в 1913 году, российский капитал, по-видимому, контролирует лишь малую часть мировой добычи золота. Британцы наиболее активны в Сибири, и известно, что французские интересы приобрели там собственность. Насколько известно, российские капиталисты не контролируют золотые месторождения в зарубежных странах. В 1916 году золотой резерв в российских банках, казначействах и в обращении составлял 1 058 000 000 долларов, но неизвестно, что стало с этим запасом с тех пор, как большевики находятся у власти. В настоящее время общая сумма, вероятно, намного меньше.

Япония контролирует лишь малую часть мировой добычи золота, как политически, так и коммерчески. Некоторое количество золота добывается в Японии и на Формозе, и все оно, вероятно, находится под японским финансовым контролем. Добыча в Корее, на которую японцы претендуют как на часть своей империи с 1910 года и которая в настоящее время пытается добиться независимости, контролируется американцами и представителями других национальностей. Небольшие рудники принадлежат японцам, но более крупные концессии были предоставлены иностранцам старым корейским правительством до 1910 года. Золотые запасы Японии оценивались в 143 128 000 долларов в 1916 году. К 26 декабря 1918 года они увеличились до 225 820 000 долларов. Кроме того, японцы имели на депозитах в Лондоне, Нью-Йорке и Париже в общей сложности около 550 000 000 долларов.

Добыча золота, контролируемая политически или коммерчески Германией и странами бывшей Австро-Венгерской империи, относительно незначительна, составляя в обоих случаях менее 1 процента. Германия ежегодно производила на своей европейской территории чуть более 100 000 долларов, и ее единственной колонией, дававшей заметное количество, была Германская Восточная Африка, потерянная во время войны. Рудники Австро-Венгрии были важны в прошлом, но сейчас они очень старые и в 1913 году дали лишь 0,5 процента от общемировой добычи. По имеющимся сведениям, одна из крупнейших действующих компаний в Трансильвании до войны была британской.

РЕЗЮМЕ

Основными и наиболее важными способами использования золота являются использование его в качестве меры стоимости и средства обмена. Золото также используется в стоматологии и в искусстве для изготовления ювелирных изделий, позолоты и других видов украшений. В чрезвычайных ситуациях другие материалы могут быть заменены для последних целей, но любая значительная замена для основных целей повлекла бы за собой радикальные изменения в нашей денежно-финансовой системе.

Золото встречается в породах всех геологических эпох от архейской до четвертичной, а также в ничтожных количествах в океанской воде. Только более концентрированные месторождения могут разрабатываться с прибылью. Считается, что добыча из нынешних основных месторождений достигла своего зенита, но дальнейшие важные открытия, вероятно, будут сделаны в арктических регионах, в тропиках или в других регионах, до сих пор не исследованных человеком. Сибирь, Южная Америка и, возможно, Китай являются наиболее перспективными регионами, так как более освоенные земли уже тщательно разведаны.

Золото широко распространено географически. Оно встречается во всех частях мира, и коммерчески важные рудники разрабатываются на каждом континенте. Более 75 процентов от общего годового объема мировой добычи приходится на четыре страны: Трансвааль, Соединенные Штаты, Австралию и Россию. Другими важными производителями являются Родезия, Мексика, Канада, Индия, Западная Африка и Новая Зеландия. Мало золота добывается в Европе или Южной Америке. Месторождения первого континента, когда-то важные, истощаются. Ожидается, что с улучшением транспортных условий и дальнейшими геологоразведочными работами добыча в Южной Америке существенно возрастет.

Великобритания контролирует политически более 60 процентов годовой мировой добычи золота через государственный суверенитет над Южной Африкой, Австралазией, Родезией, Канадой и Индией. Соединенные Штаты занимают второе место, контролируя около 20 процентов. Россия контролирует около 6 процентов, а Мексика — 4 процента. Остальные 10 процентов контролируются многими странами, среди которых Япония, Франция, Бельгия и Центральные державы.

Степень британского политического и коммерческого контроля почти идентична: британские интересы контролируют более 60 процентов добычи и владеют, помимо рудников в империи, собственностью в Сибири, Южной и Центральной Америке, Мексике и Соединенных Штатах. Интересы Соединенных Штатов финансово контролируют около 23 процентов мировой добычи. Корейские месторождения преимущественно принадлежат американцам. Капитал Соединенных Штатов также инвестирован в Канаду, Мексику, Центральную и Южную Америку, а в последнее время — в Трансвааль. Хотя золото, контролируемое политически Францией, имеет небольшое значение, французские интересы коммерчески контролируют около 5,6 процента от общего годового объема добычи, владея рудниками в Трансваале, Мексике, а также в Центральной и Южной Америке.

До войны германские интересы имели обширные активы в Южной Африке и Австралии.

ГЛАВА XXX СЕРЕБРО Ф. У. Пейн

ИСПОЛЬЗОВАНИЕ СЕРЕБРА

Основным и важным использованием серебра являются деньги. Эта форма потребления происходит главным образом в Индии и Китае, где серебро служит основой для расчетов по внешнеторговым балансам. В Китае серебро является денежным стандартом страны. В Индии используется золотой стандарт, но с незапамятных времен местные жители накапливали серебро и вкладывали свои сбережения в серебряные монеты и украшения, а не пользовались банками, облигациями или другими ценными бумагами. Серебро используется для разменной монеты во всех странах, но такие монеты в Европе и Соединенных Штатах обычно могут быть в значительной степени заменены бумажными, так как они обращаются по стоимости, превышающей их внутреннюю стоимость. В Мексике, Перу и других серебродобывающих странах широко используются серебряные деньги.

Большое количество серебра используется в искусстве. В небольшой степени такое потребление идет на фотографические или химические работы, но главным образом на производство ювелирных изделий и предметов роскоши для дома. Использование серебряных украшений в Индии тесно связано с накоплением серебра, банковским балансом местных жителей. Однако такие накопления сейчас в основном состоят из монет, потому что монета стала более стабильной по стоимости, чем украшения, с тех пор как Индия приняла золотой стандарт. До 1914 года, по оценкам директора Монетного двора США, две трети нового ежегодно добываемого серебра шло в искусство. Однако в 1912 году чеканка монет поглотила более половины из 224 310 000 унций, произведенных в мире. Во время войны оплата союзниками товаров, закупленных на Востоке, направила огромные запасы серебра в Индию и Китай. В Европе в условиях войны требовалось большее количество серебряной монеты. Более того, крупные выпуски бумажных денег делают желательными соответствующие увеличения количества серебряных монет. В 1915 году только 20 процентов мирового серебра использовалось в искусстве; в 1916 году — 15 процентов, остальное было пущено на чеканку.

Важность серебра для основных нужд во время войны лучше всего подтверждается тем фактом, что старые неиспользуемые запасы серебряной монеты, доллары США в Казначействе, манильские доллары и т. д. должны были быть призваны на службу. Стадия, до которой не дошли, — это переплавка серебряной посуды и украшений. Эта стадия была достигнута в Германии в случае с золотом и, вероятно, с серебром, точно так же, как Соединенные Штаты начали принимать такую программу для получения платины. В течение 1916 года наш экспорт серебра превысил 210 000 000 долларов, превзойдя на 58 000 000 долларов общий экспорт меди за тот же период.

Пока не изменятся многовековые обычаи Индии и Китая, серебро должно считаться наравне с золотом важным денежным металлом внутренней и международной торговли.

Широкое использование серебра в искусстве в период с 1900 по 1914 год, использование, которое естественно считается чисто роскошью, приводит к акценту на неважном характере потребления серебра в целом. Когда разразилась европейская война, цены на серебро, как и на большинство металлов и других товаров, снизились. Но серебро не выросло в цене несколько месяцев спустя, как это сделали цветные металлы. Только к концу 1915 года серебро продавалось так же дорого, как до войны, а в начале войны оно продавалось так дешево, что производители чувствовали себя обескураженными и рассматривали серебро, в основном, как предмет роскоши.

С другой стороны, факт заключается в том, что чеканка серебра в Европе колоссально возросла в 1914 и 1915 годах, хотя это, по-видимому, не полностью компенсировало сокращение производства серебряной посуды и ювелирных изделий. Эта потребность в чеканке продолжалась во время войны ускоренными темпами, точно так же, как и спрос на боеприпасы и людей. «Серебряная пуля» была важна в Европе, но еще более важна для доставки припасов с Дальнего Востока на фронты. Этот факт подтверждается ростом цены на серебро практически вдвое по сравнению с довоенной котировкой, и если бы цена тогда не была зафиксирована, рост был бы, вероятно, больше. Нормальная годовая добыча серебра в мире составляет около 159 000 000 унций, тогда как фактический спрос на серебро в течение 1918 года превысил 500 000 000 унций.

Все серебро, используемое в искусстве, отнюдь не представляет собой потребление в предметах роскоши. Серебро в значительной степени входит в важные химическую и фотографическую отрасли промышленности. По крайней мере одна треть серебра, потребляемого в искусстве до войны, приходилась на ювелирные изделия, используемые в Индии, и это использование является гораздо более формой инвестиций местных жителей, чем в Европе и Соединенных Штатах.

Министерство финансов Соединенных Штатов было очень обеспокоено снижением добычи золота. Во время войны золотодобывающей промышленности были предоставлены приоритеты, чтобы поставить ее в положение привилегированной военной отрасли. Серебро нельзя считать находящимся в ином положении, хотя производители серебра получили приоритеты скорее как производители цветных металлов и золота, чем только серебра.

Кредиту и финансам мира очень помогает максимальная добыча золота, но не менее важным является большой запас серебра, ибо, хотя золото стало общим денежным стандартом, серебро все еще остается, как и на протяжении всей истории человечества, одним из двух драгоценных или денежных металлов. Это, по крайней мере, костыль, помогающий золоту.

Во многих частях мира серебро стоит наравне с золотом или считается более важным в качестве денежного стандарта. В других местах, в странах, где бумажная валюта свободно принимается продавцами, оно не является важным денежным металлом, например, в Соединенных Штатах. Однако серебро вместе с золотом помогает поддерживать кредит и положение бумажных денег в Европе сегодня, а в странах с менее сложными финансовыми системами оно напрямую заменяет и, таким образом, сберегает золото.

Таким образом, серебро считается важным металлом мировых финансов, торговли и промышленности. Оно относится к группе жизненно важных минеральных сырьевых ресурсов и не может быть отнесено к алмазам или другим неважным минеральным продуктам.

Неограниченная добыча и производство серебра не могут рассматриваться как самоцель, что Испания обнаружила во времена конкистадоров. Но нынешняя добыча серебра не превышает реальных потребностей. На самом деле можно ожидать большого дефицита капитала из-за огромных разрушительных последствий мировой войны. Добыча серебра увеличивает запас денег, повышает доверие к финансовым условиям и обеспечивает, вместе с золотом и в качестве дополнения к нему, основу для кредита. В ближайшем будущем максимальная добыча серебра может иметь такое же или даже большее значение для мира, чем когда-либо прежде.

ГЕОЛОГИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Около половины мировой добычи серебра получается в качестве побочного продукта при добыче других металлов, прежде всего свинца и меди. Такая добыча происходит из месторождений всех геологических эпох. Серебро, получаемое из высококачественных серебряных руд, ассоциированных с небольшими количествами золота или цветных металлов, в настоящее время извлекается главным образом из третичных месторождений. Докембрийские месторождения имеют некоторое значение, например, Кобальт, Онтарио; но третичные отложения являются основным источником серебряных руд.

Мексиканские рудники, которые являются, безусловно, самыми важными производителями серебряных руд, связаны с третичными вулканическими породами. Подобная ассоциация встречается к югу, в Центральной Америке, Перу и Боливии. Месторождения Соединенных Штатов, Невады, Колорадо, Юты и Монтаны встречаются в аналогичных условиях. Это также верно для главных отработанных месторождений недавней истории добычи серебра — Комсток-Лоуд.

В прошлом в Европе добывалось большое количество серебра, главным образом из богатых серебряных месторождений, которые сейчас в значительной степени истощены. Геологические условия здесь неясны, потому что добыча была завершена так давно.

В будущем Мексика и Кордильеры Скалистых гор — Анд будут главным регионом для добычи богатых серебряных руд. Докембрийские районы Канады могут продолжать иметь некоторое значение.

ГЕОГРАФИЧЕСКОЕ РАСПРОСТРАНЕНИЕ

Обобщенная таблица нормальных объемов добычи выглядит следующим образом:

Таблица 69. — Текущая нормальная добыча серебра

Country | By-product silver | Straight silver deposits | Notes
Western Hemisphere: |  |  |
Mexico and Central America | 12,000,000 | 60,000,000 | Tertiary
Peru and Bolivia | 10,000,000 | 5,000,000 | Tertiary
Chile | 2,000,000 | ... | Miscellaneous
United States | ... | 23,000,000 | Tertiary
United States lead ores | 24,000,000 | ... | Miscellaneous
United States copper ores | 23,000,000 | ... | Miscellaneous
Canada | ... | 21,000,000 | Pre-Cambrian
Canada | 4,000,000 | ... | Miscellaneous
Total Western Hemisphere | 75,000,000 | 109,000,000 |
Eastern Hemisphere: |  |  |
Spain | ... | 4,500,000 |
Austria and Turkey | ... | 3,000,000 |
India | 5,000,000 | ... | Burma
Australia | 16,000,000 | ... | Broken Hill
Japan | 7,000,000 | ... |
Miscellaneous | 2,000,000 | 1,500,000 |
Total Eastern Hemisphere | 30,000,000 | 9,000,000 |

Резюме

| Total output, ounces | Percentage of total output
Rich silver mines | 118,000,000 |  53
By-product silver | 105,000,000 |  47
Total | 223,000,000 | 100

Мексика, великий центр богатых серебряных рудников, в настоящее время производит менее половины своей нормальной добычи из-за нестабильных политических и социальных условий. В 1907 году мексиканская добыча снизилась до 31 000 000 унций, что составляет потерю более 50 процентов. Следовательно, в 1917 году мировая добыча серебра составила всего 170 000 000 унций; и из этого количества более половины было получено в качестве побочного продукта при аффинаже других металлов.

Поразительной особенностью распределения серебряных месторождений является большое количество крупных добывающих районов в Мексике и западной части Соединенных Штатов. Таким образом, обозначена аргентоносная металлогеническая провинция, что хорошо показано в следующей таблице:

Таблица 70. — Географическое распределение серебряных месторождений по регионам

Region | Proportion from Rocky Mountain- Andes region | Normal output (ounces) | Percentage of world total
1. | Rocky Mountain-Andes Region: |  |  |
| United States | 99 per cent. of total | 70,000,000 |
Mexico | All | 70,000,000 |
Central America | All | 2,000,000 |
Peru and Bolivia | All | 15,000,000 |
Chile | All | 2,000,000 |
Canada | 16 per cent. of total | 4,000,000 |
Total | ... | 163,000,000 |  73   
2. | Cobalt, Ontario | ... | 21,000,000 |   9.45
3. | India and Australia (2 mines) | ... | 21,000,000 |   9.45
4. | Japan | ... | 7,000,000 |   3.1 
5. | Miscellaneous | ... | 11,000,000 |   5.0 
| Total for world | ... | 223,000,000 | 100.00

Относительный геологический возраст серебряных месторождений представлен в таблице ниже:

| Probable future output (ounces) | Future percentage of total | Present proportion
Tertiary | 170,000,000 | 76 |  73.0 
Japanese copper (largely Tertiary) | 5,000,000 |  2 |   3.1 
India and Australia (age of deposits not stated) | 25,000,000 | 11 |   9.45
Pre-Cambrian | 15,000,000 |  7 |   9.45
Unknown | 10,000,000 |  4 |   5.0 
Total | 225,000,000 | 100 | 100.0 

Изучение приведенных выше данных показывает, что подавляющая часть мирового серебра встречается в великой петрографической и металлогенической провинции, которая образует граничащую зону вокруг Тихого океана и является наиболее продуктивной в западных Кордильерах Северной и Южной Америки.

ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРЕДЕЛЕНИИ В БЛИЖАЙШЕМ БУДУЩЕМ

Снижение может произойти в Кобальте (Онтарио) и в Японии; в Кобальте из-за истощения руды, в Японии из-за снижения добычи меди и свинца, если цены на эти металлы упадут. Добыча в регионе Скалистых гор — Анд должна поддерживаться относительно на уровне, показанном выше, при условии возвращения Мексики к нормальному состоянию. Вся эта добыча в регионе Скалистых гор — Анд, или практически вся, связана с третичными изверженными породами.

Приведенные выше цифры частично учитывают увеличение добычи в Индии с новых рудников в Бирме.

ИЗМЕНЕНИЯ В ПРАКТИКЕ

Сомнительно, что добыча серебра существенно возрастет в ближайшие несколько лет за счет улучшения металлургических, обогатительных или горнодобывающих методов. Добыча серебра, возможно, уникальна тем, что большая часть продукции, производимой в качестве побочного продукта, поступает на рынок по ставке, определяемой скорее объемом добычи свинца и меди, чем текущими котировками на серебро. Также богатые серебряные рудники при обнаружении могут эксплуатироваться с большой прибылью на унцию. Однако высокие цены на серебро будут стимулировать ту часть добычи, которая поступает с собственно серебряных рудников.

Мировая добыча увеличилась более чем на треть в период с 1904 по 1913 год. В то же время цены снизились даже ниже показателей 1893-1894 годов. Увеличение добычи было обусловлено производством в Соединенных Штатах и Канаде.

Независимо от цены, открытие в Кобальте выбросило серебро на рынок. Независимо от цены, увеличение добычи свинца и меди в Соединенных Штатах выбросило побочное серебро на рынок.

Кажется ясным, что открытия новых серебряных месторождений или расширенные и улучшенные операции по добыче цветных металлов — это факторы, которые будут влиять на добычу серебра. Изменения в методах извлечения серебра и даже измененные цены на серебро не имеют огромного эффекта. Даже большое падение цен на серебро в начале девяностых годов не сопровождалось снижением добычи серебра. Вместо этого произошло увеличение.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Мировая добыча серебра распределена между различными политическими группами, как показано в Таблице 71:

Таблица 71. — Добыча серебра в 1917 и 1913 гг.

Country | 1917 production (ounces) | 1913 production (ounces) | 1913 percentage of total
United States | 71,740,000 |  | 66,801,000 |  30.0 
British Empire (chiefly Canada and Australia) | 34,001,000 | 50,429,000 |  22.6 
France | 235,000 | 521,000 |   0.2 
Italy | 450,000 | 424,000 |   0.2 
| 106,426,000 | 118,175,000 |  53.0 
Japan | 6,922,000 | 4,716,000 |   2.1 
Peru | 11,000,000 | 8,351,000 |   3.7 
Central America | 2,369,000 | 2,135,000 |   1.0 
Bolivia | 2,434,000 | 2,410,000 |   1.1 
Russia, Greece, etc. | 1,000,000 | 1,000,000 |   0.4 
Mexico | 31,214,000 | 70,704,000 |  31.7 
Chile | 1,673,000 | 2,000,000 |   0.9 
Spain | 4,500,000 | 4,232,000 |   1.9 
Germany, Austria | 1,500,000 | plus | 7,195,000 |   3.2 
Turkey |  |  | 1,509,000 |   0.7 
Miscellaneous | 1,700,000 | 700,000 |   0.3 
Total | 170,038,000 | 223,126,000 | 100.00

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Через владение рудниками.

— Добыча серебра в Соединенных Штатах полностью контролируется капиталом Соединенных Штатов. Одна треть контролируется интересами по добыче свинца, одна треть — интересами по добыче меди, а оставшаяся треть — добытчиками серебра. Более того, капитал Соединенных Штатов владеет мексиканской горнодобывающей собственностью, обычно способной производить более половины добычи этой страны. Добыча в Центральной Америке и побочное серебро Перу контролируются аналогичным образом. Около четверти канадской добычи поступает с предприятий, принадлежащих Соединенным Штатам. В целом, капитал Соединенных Штатов контролирует более половины ежегодной добычи серебра во всем мире.

Большая часть канадского и все австралийское, индийское и африканское серебро контролируется британским капиталом, как и четверть мексиканской добычи и некоторая часть из Боливии, Перу и Чили. В целом Великобритания контролирует треть мировой добычи.

Германия, вероятно, контролирует около 10 процентов мировой добычи серебра. Часть этого производится на месте, но основной германский контроль находится в Мексике, причем рудники, принадлежащие мексиканцам, в основном считаются германской собственностью.

Рудники, принадлежащие японскому, испанскому, французскому или чилийскому капиталу, обеспечивают практически все оставшиеся 5 процентов мировой добычи серебра.

Финансовый контроль через владение рудниками

Capital | 1913 output, percentage controlled
United States |  52
British |  33
German |  10
Japanese |   2
Spanish |   2
French, etc. |   1
| 100

Через владение обогатительными заводами.

— Как и следовало ожидать, исходя из географического расположения серебряных месторождений, Соединенные Штаты и Мексика являются центрами плавки и аффинажа серебра. Важные интересы по плавке серебра следующие:

Company | Situation of smelters
The American Smelting & Refining Co. | United States and Mexico
The United States S., R. & M. Co. | United States and Mexico
The International Smelting Co. | United States
Anaconda Copper Mining Co. | United States
Consolidated Mining & Smelting Co. | Canada
Compañia Metalurgica Mexicana. | Mexico
Compañia Metalurgica de Torreon. | Mexico
Compañia Minera de Peñoles. | Mexico

Через владение обогатительными заводами Соединенные Штаты осуществляют контроль над несколько большей долей мирового серебра, чем через владение рудниками. Большая часть канадской и мексиканской, а также большая часть южно- и центральноамериканской добычи серебра поступает в Соединенные Штаты либо в виде аффинированных слитков, либо в виде руды и черновых слитков.

По оценкам, контроль через обогатительные заводы распределяется примерно следующим образом:

Соединенные Штаты — ⁴⁄₇; Мексика — ¹⁄₇; Канада — ¹⁄₁₄; Европа и Азия — ³⁄₁₄.

Что касается серебра, этот тип контроля совсем не является мощным. Серебросодержащие материалы могут выдерживать высокую стоимость транспортировки, как только завершен первый процесс отделения от пустой породы. Следовательно, владение рудниками, а не обогатительными заводами, является жизненно важным фактором контроля над серебряными ресурсами, насколько это касается добычи.

Через торговые объединения.

— Мировая добыча серебра контролируется лондонским рынком. В небольшой степени это может быть связано с торговым объединением; в значительной степени это связано с отношениями лондонского рынка с потребителями.

Лондонский рынок серебра формируют четыре фирмы. Цены на серебро устанавливаются в Лондоне ежедневно, и эта «фиксированная» котировка определяет цену на металл в каждом крупном финансовом центре по всему миру.

В Лондоне действуют три аффинажных завода, которые перерабатывают практически всё серебро в слитках, поступающее на лондонский рынок. Никакое серебро не может быть куплено или продано в Лондоне, если оно не прошло пробирный анализ у одного из четырех официальных пробиреров Монетного двора, Банка Англии и т. д. Исключение составляют серебро, обработанное лондонскими аффинажными заводами, и некоторые слитки с европейских государственных аффинажных заводов.

Лондонские аффинажные заводы производят серебро пробы ⁹⁹⁶⁄₁₀₀₀ для нужд индийского рынка. Другое серебро, обращающееся на лондонском рынке, имеет пробу ⁹⁹⁹⁄₁₀₀₀.

По словам Бенджамина Уайта: «Забота о сохранении репутации лондонского рынка серебра, высокий авторитет фирм, составляющих его, и доверие, завоеванное методами и практиками, принятыми для защиты интересов как покупателя, так и продавца, служат надежной гарантией того, что в будущем, как и в прошлом, серебро будет находить свой деловой центр в Лондоне».

Через отношения с потребителями — контроль Англии над серебром.

— Как уже отмечалось, Индия и Китай являются крупнейшими потребителями серебра. За пять лет, предшествовавших 1914 году, из Лондона в эти две страны было отправлено не менее 40 процентов мировой добычи серебра; эти страны с совокупным населением более 700 000 000 человек представляют собой покупательную сторону мирового рынка серебра, точно так же, как Северная Америка представляет сторону продавцов.

С 1914 года способность этих стран поглощать серебро неуклонно росла, и в 1918 году вопрос заключался главным образом в том, где можно получить этот металл. Текущего производства было недостаточно для удовлетворения спроса, и старые запасы драгоценного металла были вынужденно выброшены на рынок.

Мировой бизнес по торговле серебром заключается в доставке металла из Америки на Восток. Зачем отправлять его через Лондон, подвергая драгоценный металл повышенным морским рискам и теряя проценты во время транспортировки? Основная причина заключается в том, что главная торговля Китая и Индии с западными странами ведется с Англией, а крупные банковские дома, финансирующие эту торговлю, находятся в Лондоне. Эти банки покупают серебро в Лондоне для выравнивания торгового баланса. Средства для покупки такого серебра обычно поступают из Лондона, будь то векселя на Лондон, кредиты лондонских банков или иные источники. Кроме того, Лондон был центром мировых финансов и внешней торговли, а также центром, из которого исходили почтовые пароходы — самые быстрые и дешевые маршруты к основным потребителям серебра.

Когда подводные лодки стали представлять угрозу, Соединенные Штаты начали отправлять серебро напрямую из Сан-Франциско в Индию и Китай. Таким образом, значительная часть добычи Соединенных Штатов была отвлечена от Лондона, и в 1918 году экспорт серебра из Лондона был значительно ниже нормы. Однако представители American Smelting & Refining Co., компании, перерабатывающей более трети мировой добычи серебра, заявляют, что не ожидают сохранения этих условий. Устоявшийся бизнес лондонской торговли серебром и, что более важно, отношения между коммерческим Лондоном и странами-потребителями серебра, несомненно, быстро восстановят нормальный статус Лондона как импортера американского серебра и экспортера серебра, необходимого на Дальнем Востоке.

Американский аффинажер или производитель серебра рад иметь устойчивый и широкий рынок сбыта для своего серебра, какой предоставляют четыре лондонские фирмы. Плавильные предприятия и рудники могут сбывать свою продукцию через Лондон; в противном случае им пришлось бы иметь дело с брокерами или банками на Дальнем Востоке. Лондонские фирмы поддерживают тесную связь с крупными торговцами слитками в Бомбее, Калькутте и других городах, которые являются центрами распределения серебра по всей Индии. Однако серебро для индийской имперской чеканки закупается правительством в Лондоне.

Через закон Питтмана в Соединенных Штатах.

— Вышеуказанная схема движения торговли серебром недавно (в 1920 году) была существенно изменена программой правительства Соединенных Штатов по закупке внутреннего серебра по цене 1 доллар за унцию. Если мировая цена на серебро останется ниже этой отметки, все американское серебро будет поглощаться правительством в течение примерно четырех лет, или до тех пор, пока не будут выкуплены 207 000 000 унций, указанные в законе Питтмана. Если же цена на серебро поднимется выше 1 доллара, движение на рынок, как описано выше, возобновится.

Положение Китая и Японии.

— Курсы иностранной валюты в Китае в значительной степени зависят от цены на серебро. Все импортеры или экспортеры, ведущие дела с Китаем, должны работать на рынке серебра. Хотя медная монета «кэш» является основой китайской денежной системы, серебро служит стандартным законным платежным средством для сделок, связанных с крупными суммами, а весовые единицы серебра используются в качестве расчетных единиц. Проба и вес китайских монет подвергаются манипуляциям, поэтому монеты, выпущенные государствами-производителями серебра, например, мексиканские доллары (двух разновидностей), британские доллары, испанские доллары и т. д., ценятся китайцами, поскольку они имеют единообразную стоимость.

Япония производит значительное количество серебра, большая часть которого поступает с ее электролитических медеплавильных заводов. Золото является денежным стандартом, а серебро не используется широко в прикладном искусстве. Следовательно, Япония производит больше серебра, чем необходимо для удовлетворения местного потребления. Правительство осознает важность серебра в связи со всеми сделками с Китаем. В 1918 году японские банки скупали китайские запасы серебра, выплачивая цены, превышающие цены всех остальных торговцев. Считается, что американское серебро поступало в Японию через Китай и что Япония стремится контролировать китайский рынок серебра. В Японии создается крупный резерв серебра. Учитывая международную важность всей китайской проблемы, следует отметить активность Японии на рынке серебра.

РЕЗЮМЕ

Серебро используется как в качестве денег, так и в прикладном искусстве, причем первое использование является более важным и существенным. В некоторых странах, особенно в тех, которые производят серебро в больших количествах, оно является денежным стандартом, либо само по себе, либо вместе с золотом. В других странах, находящихся на золотом стандарте, серебро используется для разменной монеты. В Индии и Китае оно используется для расчетов по балансам внешней торговли. Обычно около двух третей ежегодно добываемого серебра используется в прикладном искусстве, главным образом для производства ювелирных изделий и предметов роскоши для дома, хотя часть потребляется в фотографической, химической и других важных отраслях промышленности. Во время войны на чеканку монет уходило больше серебра, а на прикладное искусство — меньше, чем раньше, поскольку крупные выпуски бумажных денег делали желательным соответствующее увеличение количества серебряных монет. Большие объемы были экспортированы на Дальний Восток. Война показала, что серебро по-прежнему следует считать важнейшим металлом мировых финансов и торговли, несмотря на растущие объемы, потребляемые в некритически важных целях.

Около половины мировой добычи серебра получается как побочный продукт при добыче других металлов, прежде всего свинца и меди, из месторождений всех геологических эпох. Высокосортные серебряные руды происходят главным образом из третичных отложений, и вполне вероятно, что в будущем Мексика и регион Скалистых гор и Анд будут основными источниками руд этого типа.

Из общего объема мировой добычи серебра более 80 процентов приходится на рудники Западного полушария. В течение многих лет Мексика была ведущей страной по добыче серебра в мире, но нестабильные политические условия настолько помешали горным работам, что добыча в 1917 году составила менее половины от уровня 1911 или 1912 годов. Соединенные Штаты, занимавшие второе место после Мексики в дореволюционные годы, сейчас занимают лидирующую позицию. Канада, а также страны Центральной и Южной Америки также производят значительные количества серебра. В Восточном полушарии ведущим производителем серебра является Австралия. Меньшие объемы поставляют Испания, Австрия, Турция, Индия и Япония.

Изменения в практике извлечения серебра и даже цены на серебро мало влияют на его добычу. Она будет стимулироваться скорее открытием новых месторождений серебра или расширением и совершенствованием операций по обогащению цветных металлов.

Основные месторождения серебра в мире находятся под политическим контролем Соединенных Штатов, Мексики и Великобритании; эти три страны контролировали около 85 процентов всей добычи в 1913 году. Американский капитал контролирует всю добычу серебра в Соединенных Штатах, а также рудники, производящие половину мексиканской добычи, четверть канадской добычи и значительную часть добычи стран Центральной и Южной Америки — в общей сложности чуть более половины нормальной мировой добычи серебра. Великобритания контролирует, вероятно, одну треть мировой добычи, главным образом в Канаде, Австралии, Индии, Африке и Мексике. Германскому капиталу принадлежит, вероятно, одна десятая часть, расположенная частично в Германии, но главным образом в Мексике. Остальные месторождения серебра в мире принадлежат японскому, испанскому и французскому капиталу. Владение перерабатывающими заводами не является мощной формой контроля в случае с серебром. Соединенные Штаты владеют около четырех седьмых общей мировой мощности по плавке и аффинажу, а остальные три седьмых контролируются в основном германским, британским и мексиканским капиталом.

Хотя большая часть серебра, производимого каждый год, поступает из Северной и Южной Америки, мировой рынок серебра находится в Лондоне из-за тесных отношений между английскими деловыми интересами и Индией и Китаем — главными потребителями этого металла.

Правительство Соединенных Штатов, однако, будет (в 1920 году) закупать все предлагаемое американское серебро по цене 1 доллар за унцию, в объеме до 207 000 000 унций.

ГЛАВА XXXI ПЛАТИНА Автор: Джеймс М. Хилл

ПРИМЕНЕНИЕ ПЛАТИНЫ

В прошлых дискуссиях о применении платины возникала некоторая путаница из-за непонимания того, что вся коммерческая платина не является чистым металлом. Чистый металл требуется для химических работ любого рода, но для других целей используются сплавы с иридием. Электротехническая платина содержит от 15 до 50 процентов иридия, в среднем 25 процентов, а ювелирная платина содержит около 10 процентов иридия. Палладий, еще один металл платиновой группы, также важен, главным образом в виде палладиево-золотых сплавов, которые могут использоваться для замены платины в стоматологической и ювелирной промышленности. Родий, один из более редких элементов сырой платины, имеет ограниченное применение в электрических пирометрах. Осмий и рутений, остальные члены платиновой группы, по-видимому, имеют мало применений, хотя осмий при правильном использовании может применяться в качестве заменителя иридия для упрочнения платиновых сплавов.

Основные области применения металлов платиновой группы — это химическая и электротехническая промышленность, и, вероятно, стоматологическую промышленность следует отнести к числу важнейших. Чистая платина требуется в химической промышленности для катализаторов при производстве серной кислоты (в настоящее время в Соединенных Штатах используется около 75 000 унций) и при производстве азотной кислоты из аммиака. Для производства серной кислоты основным материалом, содержащим платину, является хлорид платины. Асбест или безводный сульфат магния, пропитанный хлоридом платины, а затем прокаленный для удаления хлора, образует так называемую «контактную массу», которая загружается в камеры контактных установок для производства кислоты. Очень тонкая платиновая сетка используется в качестве катализатора на заводах по производству азотной кислоты. Некоторая сетка, используемая для этой цели, имеет армирующий край из платино-иридиевой проволоки. Чистые платиновые инструменты различных видов, включая тигли, чаши, щипцы и треугольники, требуются в каждой химической лаборатории. Можно заменить некоторые инструменты палладиево-золотыми сплавами или даже золотом, никелем, нихромом и кремнеземом, но до сих пор не найдено заменителей, которые могли бы полностью заменить платиновую химическую посуду.

Платино-иридиевые сплавы широко используются в электротехнической промышленности, но постоянно разрабатываются заменители. Вольфрамовые, молибденовые и никель-хромовые сплавы являются основными заменителями, используемыми до сих пор, но их использование не устранило необходимость в платине в этой отрасли. Основное применение платино-иридиевых сплавов в электротехнике — это контактные точки, и доля иридия, необходимая в сплавах, напрямую зависит от силы тока, проходящего через контакты, и скорости движения контактов. Вероятно, самое большое потребление платинового сплава приходится на производство телефонного и телеграфного оборудования, включая передающие и принимающие инструменты, коммутаторы и реле. Также велико потребление платины для контактов в магнето, используемых для различных видов двигателей внутреннего сгорания. Однако производители автомобилей разрабатывают системы запуска, не требующие платины, поэтому мы можем надеяться на снижение будущего спроса с этой стороны.

Платина имеет важное применение в стоматологии, хотя в экстренных случаях в качестве заменителей использовались палладиево-золотые сплавы. По-видимому, однако, заменители не вполне удовлетворительны, и может возникнуть необходимость вернуться к платине для определенных стоматологических целей. Основное применение — это штифты для коронок, штифты для крепления искусственных зубов к пластинам и фольга для изготовления форм полостей, в которых обжигаются фарфоровые пломбы. На данный момент можно использовать палладиево-золотые заменители, и, возможно, они будут усовершенствованы настолько, что использование чистой платины в будущем может не потребоваться.

Некритически важное использование металлов платиновой группы — это ювелирное дело, и кажется очевидным, что это нецелевое использование платиновых металлов должно быть прекращено, чтобы промышленное развитие могло продолжаться. По оценкам, в течение ряда лет 50 процентов платины, потребляемой в мире, шло на ювелирные изделия. Большая часть платиновых ювелирных изделий находится в частной собственности, и, поскольку стоимость металла в ювелирном изделии составляет примерно 35 процентов от общей стоимости, очевидно, что в случае необходимости было бы трудно, если не невозможно, извлечь более чем малую часть того огромного количества платины, которое находится в форме ювелирных изделий.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ

Об относительной важности стран-производителей платины в мире лучше всего судить по прошлым объемам добычи, которые показаны в следующей таблице [181] и графически на диаграмме.

[181] Хилл, Дж. М.: «Платина и сопутствующие металлы», Геологическая служба США, «Минеральные ресурсы, 1916», ч. 1, 1917, стр. 3.

Платиновое месторождение России находится на Урале, к северу от Екатеринбурга. В Колумбии, Южная Америка, основная добыча платины ведется в верховьях реки Сан-Хуан, которая впадает в Тихий океан недалеко от Буэнавентуры; некоторое количество платины найдено в верховьях реки Атрато, которая впадает в Карибское море недалеко от восточной оконечности Панамы. Небольшое количество платины и осмистого иридия было получено из Нового Южного Уэльса, а некоторое количество осмистого иридия — из Тасмании. Некоторые россыпи на юго-западе Орегона и севере Калифорнии содержат платину наряду с золотом. Платина недавно была обнаружена в концентратах из нескольких мест на Аляске и в Канаде, а также известна в некоторых россыпях на Борнео и в Индии.

Таблица 72. — Оценочная мировая добыча сырой платины, 1909–1917 гг. (в тройских унциях)

Country | 1909 | 1910 | 1911 | 1912 | 1913 | 1914 | 1915 | 1916 | 1917
Borneo and Sumatra | 500 | 200 | ... | ... | 200 | [182] | [182] | [182] | [182]
Canada | 30 | 30 | 30 | 30 | 50 | 30 | 100 | 60 | 80
New South Wales and Tasmania | 440 | 332 | 470 | 778 | 1,500 | 1,248 | 303 | 222 | [182]
Russia | 264,000 | 275,000 | 300,000 | 300,000 | 250,000 | 241,200 | 124,000 | 63,000 | 50,000
United States | 672 | 390 | 628 | 721 | 483 | 570 | 742 | 750 | 605
Totals | 271,642 | 285,952 | 313,128 | 313,529 | 267,233 | 260,548 | 143,145 | 89,932 | 82,685

[182] Нет основы для оценки.

ГЕОЛОГИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ ПЛАТИНЫ

Практически все металлы платиновой группы, добытые в мире на сегодняшний день, были получены из россыпных месторождений, хотя небольшое количество платины и палладия было получено в качестве побочного продукта при электролитическом аффинаже медного и никелевого штейна.

Платиновые россыпи в мире настолько определенно связаны с интрузивными основными магматическими породами, включая пироксениты, перидотиты и дуниты, что вопрос о происхождении металла практически не вызывает сомнений. Фактически, в Британской Колумбии, Испании и России платина была найдена в коренном залегании в этих типах пород, и сообщается, что из-за высокой стоимости платины в настоящее время в России планируется проект по дроблению и промывке некоторых тел дунита.

Платина встречается не во всех россыпях, образованных из основных пород, но, насколько известно, она редко встречается в россыпях, образованных из других типов пород. Поиск платиновых россыпей, следовательно, сводится прежде всего к поиску месторождений гравия, образованного в значительной части из пироксенита, перидотита и дунита. Хромит является характерным тяжелым компонентом платиноносных песков и в некоторых месторождениях может быть извлечен в качестве побочного продукта при добыче. Оливин также присутствует в значительных количествах. Магнетит и ильменит обычно присутствуют в концентратах из платиновых россыпей, но они более характерны для россыпей, в которых золото является наиболее ценным компонентом.

В России и Испании было проведено большое количество геологоразведочных работ, основанных на теории происхождения, изложенной выше. Большая часть этих работ привела к обнаружению платиноносных россыпей, но многие из этих недавних открытий, по-видимому, не имеют коммерческой ценности. Невозможно предсказать, будут ли россыпи, образованные из основных магматических пород, продуктивными. Максимум, что можно сказать, это то, что некоторые россыпи, образованные из этих пород, представляют наибольшую перспективу для искателя платины. Платина — настолько редкий металл и встречается в таких малых количествах в материнской породе, что для прогнозирования коммерческих месторождений необходимо наличие определенных физиографических условий. Самым важным из этих условий является чрезвычайно длительное или очень быстрое выветривание первичных месторождений. В российском месторождении выветривание пород происходило в течение огромного геологического времени; с другой стороны, в Колумбии, Южная Америка, период выветривания, по-видимому, был относительно коротким, но настолько быстрым, что был достигнут тот же результат.

Обычно платина не встречается в коммерческих количествах в гравиях, которые не подвергались переотложению, и более богатые месторождения в мире, по-видимому, являются результатом многократного переотложения платиносодержащего материала. Сырая или россыпная платина не является чистым металлом, а содержит, помимо других металлов платиновой группы, большее или меньшее количество железа, никеля и меди. Российская сырая платина обычно продается исходя из предположения, что она содержит 83 процента металлов платиновой группы; колумбийская сырая платина — 85 процентов металлов платиновой группы. Некоторая так называемая россыпная платина содержит большую долю осмистого иридия. Так, сырая платина из Орегона и Калифорнии содержит от 25 до 45 процентов иридия, а тасманийская платина на самом деле почти чистый осмистый иридий.

Следующие анализы российской [183], колумбийской [184] и американской [184] платины служат для иллюстрации широкого расхождения в содержании металлов в сырой платине.

Таблица 73. — Анализы сырой платины из различных частей мира

North America[183] | South America[183]
| California | California | Oregon | British Columbia | Colombia | Colombia | Colombia
Pt |  85.50 |  63.30 |  51.45 |  72.07 |  86.20 |  86.16 |  80.00
Ir |   1.05 |   0.70 |   0.40 |   1.14 |   0.85 |   1.09 |   1.55
Rh |   1.00 |   1.80 |   0.65 |   2.57 |   1.40 |   2.16 |   2.50
Pd |   0.60 |   0.10 |   0.15 |   0.19 |   0.50 |   0.35 |   1.00
Os | ... | ... | ... | ... | ... |   0.97 |
Io₃[186] |   1.10 |  22.55 |  27.30 |  10.51 |   0.95 |   1.19 |   1.40
Au |   0.80 |   0.30 |   0.85 | ... |   1.00 | ... |   1.50
Fe |   6.75 |   6.40 |   4.30 |   8.59 |   7.80 |   8.03 |   7.20
Cu |   1.40 |   4.25 |   2.15 |   3.39 |   0.60 |   0.40 |   0.65
Sand |   2.95 | ... |   3.00 |   1.69 |   0.40 | ... |   4.35
| 101.15 |  99.40 | 100.25 | 100.15 | 100.25 | 100.35 | 100.15

Oceania[185] | Russia[187]
| Borneo | N. S. W. | Australia Tasmania? | Taguil | Iso | Kamenonchy | Koswinsky | Kanjakowaky
Pt |  82.60 |  75.90 |  61.40 |  76.16 |  80.10 |  82.46 |  83.50 |  60.39
Ir |   0.66 |   1.30 |   1.10 |   2.68 |   1.38 |   1.79 |   2.74 |   6.90
Rh | ... |   1.30 |   1.85 |   0.54 |   0.30 |   0.69 |   0.62 |   0.80
Pd | ... | Trace |   1.80 |   0.27 |   0.30 |   0.18 |   0.28 |   0.19
Os |  |  |  |  |  |  |  |
Io₃[186] |   3.80 |   9.30 |  26.00 |   1.50 |   4.47 |   4.99 |   0.79 |  20.21
Au |   0.20 | ... |   1.20 | ... |   0.09 |   0.27 |   0.07 |
Fe |  10.67 |  10.15 |   4.55 |  14.72 |   7.68 |   9.49 |  11.05 |  11.16
Cu |   0.13 |   0.41 |   1.10 |   3.39 |   0.63 |   0.54 |   1.14 |   0.49
Sand | ... |   1.22 |   1.20 |  |  |  |  |
|  98.06 |  99.58 | 100.20 |  99.26 |  94.95 | 100.41 | 100.19 | 100.04

[183] Дюпарк, Луи: «Le Platine et les gîtes platiniferes de l’Oural»: Soc. des Eng. Civ. de France. Bull. янв.-март, 1916.

[184] Кемп, Дж. Ф.: «Геологическая связь и распределение платины и сопутствующих металлов»: Бюллетень Геологической службы США 193.

[185] Анализы, цитируемые Кемпом.

[186] Io3 — сокращение, используемое для осмистого иридия.

[187] Анализы, цитируемые Дюпарком.

ГЕОГРАФИЧЕСКОЕ РАСПРЕДЕЛЕНИЕ ПЛАТИНЫ

Об относительной важности стран-производителей платины в мире лучше всего судить по прошлым объемам добычи, которые показаны в следующей таблице [188] и графически на Рисунке 22.

[188] Хилл, Дж. М.: «Платина и сопутствующие металлы»: Геологическая служба США «Минеральные ресурсы, 1916», ч. I, 1917, стр. 3.

Таблица 74. — Оценочная мировая добыча сырой платины, 1909–1917 гг. (Тройские унции)

| 1909 | 1910 | 1911 | 1912 | 1913 | 1914 | 1915 | 1916 | 1917
Borneo and Sumatra | 500 | 200 | ... | ... | 300 |  |  |  |
Canada | 30 | 30 | 30 | 30 | 50 | 30 | 100 | 60 | 80
Colombia | 6,000 | 10,000 | 12,000 | 12,000 | 15,000 | 17,500 | 18,000 | 25,000 | 32,000
New South Wales and Tasmania | 440 | 332 | 470 | 778 | 1,500 | 1,248 | 303 | 222 |
Russia | 264,000 | 275,000 | 300,000 | 300,000 | 250,000 | 241,000 | 125,000 | 63,900 | 50,000
United States | 672 | 390 | 628 | 721 | 483 | 570 | 742 | 750 | 605
| 271,642 | 285,952 | 313,128 | 313,529 | 267,233 | 260,548 | 143,145 | 89,932 | 82,685

Рис. 22. — Источники сырой платины, добытой с 1909 по 1917 год.

Россия.

— Российские россыпные месторождения обеспечивали примерно 95 процентов мировой добычи платины. Основные россыпные месторождения, богатые платиной, находятся на Среднем Урале, в Пермской губернии, недалеко от Нижнего Тагила, Нижней Туры и Верхотурья. Более богатые месторождения находятся на восточном склоне гор, главным образом на притоках Иса и Вия реки Туры бассейна Оби. Несколько важных россыпей обнаружено на западном склоне гор в верховьях рек Чусовой и Камы бассейна Волги. Вблизи Нижнего Тагила платиноносные россыпи встречаются как на Мартьяне, притоке Оби, так и на Мартьяне, реке в верховьях бассейна Волги. В этих россыпях платина является преобладающим металлом, но встречается и золото. Большая часть добычи в прошлом велась ручной промывкой, но в последние годы значительная часть площадей была переработана драгами, хотя все еще можно с уверенностью сказать, что более 75 процентов добычи приходится на ручной труд. Вряд ли целесообразно в отчете такого рода подробно обсуждать отдельные месторождения, даже если бы информация была под рукой. Лучшую доступную информацию можно резюмировать следующим образом: большая часть платины, несомненно, возникла в результате разрушения дунитовых, пироксенитовых или перидотитовых пород. Период выветривания был очень долгим, и произошло много изменений в речных системах, которые к настоящему времени достигли зрелости. Уклоны рек небольшие; рельеф междуречий относительно невелик. Платина, вероятно, многократно переотлагалась и в настоящее время добывается главным образом из современных долинных гравиев, хотя продуктивные пласты не всегда следуют за современными руслами рек. Отрабатываются некоторые террасовые отложения, представляющие собой старые русла рек, особенно в Нижнетагильском районе. Продуктивные гравии обычно залегают на коренных породах, хотя концентрация на глинистых пластах, образующих ложное коренное ложе, встречается довольно часто. Мощность продуктивного пласта варьируется от нескольких дюймов до 6 футов. В нем мало крупных валунов, но во многих местах много глины. Вскрыша варьируется от 2 до 16 футов по мощности, в среднем 8–10 футов. Она состоит из толстой базальной части, состоящей практически из пустых гравия и песка, или линз глины и песка, перемежающихся с гравием, которые перекрыты 2–3 футами глинистого песка и растительных остатков, подобных «муку» на рудниках Аляски.

На неглубоких участках, до 3 футов глубиной, добыча ведется открытым способом; на более глубоких участках применялись шахты и штольни. Для месторождений в руслах рек использовались и до сих пор используются примитивные ручные драги для подъема гравия. Около 35 более или менее современных драг были заняты на добыче платины до войны. Глина настолько часто встречается в гравиях, что для сохранения платины использовались специально разработанные машины, а новые драги имеют специальные устройства для решения этой проблемы.

Колумбия.

— Платиновый район Колумбии охватывает верховья рек Атрато и Сан-Хуан в районе Чоко на северо-западе Колумбии. Платина известна на севере до Бете, на реке Атрато, и во многих притоках реки Сан-Хуан, которые впадают с востока. Большая часть платины, экспортируемой из Колумбии, поступает из реки Кондото, притока реки Сан-Хуан. Утверждается, что в этой реке платина составляет около 75 процентов драгоценного металла в гравии. На реке Атрато содержание платины ниже и варьируется от 5 до 15 процентов. Платина и осмистый иридий также встречаются в реках к югу от бассейна Сан-Хуан, которые впадают непосредственно в Тихий океан, хотя достоверных данных о них мало.

По словам доктора Тулио Оспины [189], директора Горной школы в Медельине, Колумбия, платина широко распространена в конгломератах, которые покрывают обширную территорию в бассейнах рек Атрато и Сан-Хуан. Металл был переотложен в современных руслах рек, из которых поступает основная часть добычи платины. Согласно заявлениям различных наблюдателей, существуют места на междуречных пространствах, в которых платина была сконцентрирована. Эти области, по всем данным, являются старыми руслами рек. Первичные месторождения платины, очевидно, следует искать на западном склоне западного хребта Анд, хотя литературы, дающей подробную информацию о геологии этого хребта, не найдено. Перидотит, дунит и другие основные магматические породы представлены в платиноносных гравиях.

[189] Труды Второго Панамериканского научного конгресса, том 8, 1917.

Почти нет информации, на которой можно было бы основывать оценку возможных запасов платины в Колумбии. Мало что было опубликовано по этому вопросу, что давало бы хорошие данные о геологии страны, но, судя по всему, можно с уверенностью предположить, что Колумбия обладает большими перспективами и должна быть более тщательно разведана. Более 90 процентов платины, добываемой в Колумбии, добывается местными жителями, в основном женщинами, которые поднимают гравий в калабасах (calabaches) и промывают его в батеасах (bateas). Используется сухой сезон, так как тогда низкие места в реке более доступны. В настоящее время в Колумбии работает одна драга, хотя предпринимались попытки и других дноуглубительных работ, которые по разным причинам не увенчались успехом.

Канада.

— Небольшое количество платины производится каждый год в результате россыпных работ на реке Туламиен в Британской Колумбии. Металл был получен из массива перидотита и дунита, который выходит на поверхность к западу от основного водораздела. Гравии этого района, по-видимому, очень глубокие, но платина встречается в верхних 8–20 футах, частично сконцентрированная на ложном коренном ложе. Последняя информация указывает на возможность драгирования значительной площади гравиев на реке Туламиен в районе Принстона. В 1917 году ходили слухи об открытии платиноносных россыпей дальше на север в Канадских Скалистых горах, но никакой определенной информации о размере или ценности месторождений нет.

Безусловно, большая часть ежегодной добычи платины и палладия канадского происхождения является побочным продуктом аффинажа никелевых руд района Садбери, Онтарио. То, что возможна гораздо большая добыча обоих металлов из этого источника, было показано Королевской никелевой комиссией Онтарио.

Соединенные Штаты.

— Сырая платина добывается в Калифорнии, Орегоне и Вашингтоне. Драги у подножия гор Сьерра-Невада в Калифорнии производят большую часть россыпной платины в Соединенных Штатах, главным образом из-за огромного объема перерабатываемого грунта, а не из-за какой-либо особой концентрации платины в гравиях, полученных из пояса «Материнской жилы» (Mother Lode). В северной Калифорнии реки Кламат и Тринити, особенно приток Хэй-Форк реки Тринити, содержат платиноносные гравии. На юго-западе Орегона платиноносные гравии были найдены в нескольких местах на реках Иллинойс и Роуг. Вдоль пляжа от Бэндона, Орегон, до Юрики, Калифорния, платина встречается вместе с черными песками и добывалась на ряде рудников, расположенных как на современной береговой линии, так и на древних поднятых пляжах. В Голубых горах восточного Орегона и в хребте Строберри к югу от реки Джон-Дэй разрабатывалось несколько россыпей, содержащих платину. В Вашингтоне, особенно на южном рукаве реки Льюис, недалеко от Яколта, была найдена платина, и сообщается о ее наличии на пляжах от пролива Хуан-де-Фука на юг.

Все платиноносные россыпи в Соединенных Штатах тесно связаны с хромистым серпентином, полученным из перидотитов или пироксенитов. Концентрация платины была невелика, и исходное количество было небольшим, поэтому ни один из районов не кажется способным к значительной добыче. Большая часть сырой платины из россыпей Тихоокеанского побережья содержит значительное количество осмистого иридия. Как уже говорилось, основная масса платины, добываемой в Соединенных Штатах, поступает с дражных полей у подножия гор Сьерра-Невада от округа Бьютт до округа Станислаус. Гравии на этих полях являются результатом нескольких переотложений, но их содержание платины нельзя считать высоким. Практически во всех других районах речных россыпей гравии не подвергались такому обширному переотложению, и в некоторых местах платину содержат современные гравии. Пляжные отложения являются результатом многократной концентрации. Платина и золото чрезвычайно мелкие, чешуйчатые и их трудно отделить от тяжелых песков; они сконцентрированы в темных полосах песка, образованных приливной и волновой концентрацией. Линзы редко превышают один фут в толщину и выклиниваются на коротких расстояниях. Следовательно, точные оценки запасов практически невозможны.

За последние несколько лет небольшое количество платины было добыто в широко разбросанных местах на Аляске, главным образом в россыпях Дайм, Беар и Свипстейк-Крик на востоке полуострова Сьюард; россыпях Буб-Крик, район Толстой, Нижний Юкон; и пляжных отложениях острова Кадьяк. Платина также встречается в верховьях реки Кахилтна, к северу от Анкориджа.

Медные руды, богатые палладием, добываются на руднике Рэмблер, Вайоминг, на руднике Солт-Чак, Аляска, и на руднике Босс, в Неваде. На двух первых рудниках руда ассоциирована с основными магматическими породами; на последнем руднике рудные тела находятся в доломите. Часто повторяющиеся сообщения о наличии платины в некоторых песчаниках, обнажающихся возле тропы Брайт-Энджел в Гранд-Каньоне реки Колорадо, Аризона, и в некоторых сланцевых пластах в округе Честер, Пенсильвания, не были подтверждены, хотя в июне 1918 года была организована United States Platinum Co. для разработки месторождений в Аризоне.

Австралия.

— Платина и осмистый иридий добывались в небольших количествах в Квинсленде, Новом Южном Уэльсе и Тасмании. О наличии платины также сообщается в Новой Зеландии. Большая часть добычи приходилась на гравии, содержащие осмистый иридий, в бассейне реки Сэвидж в горнодобывающем районе Болд-Хиллс в северо-западной части Тасмании. Мало что было опубликовано о масштабах этих гравиев, которые образовались в результате выветривания серии осадочных пород, прорванных основными магматическими породами.

В Новом Южном Уэльсе пляжные отложения, очень похожие на отложения Калифорнии и Орегона, встречаются от Бичи-Хед на север мимо рек Кларенс и Ричмонд до Квинсленда. Коммерческая эксплуатация этих месторождений, по-видимому, имела свои взлеты и многие падения, как и подобные предприятия на нашем Западном побережье. Некоторое количество платины было получено из старого погребенного русла в районе Платина или Файфилд в центральной части Нового Южного Уэльса, где продуктивный гравий мощностью 6–10 футов залегает под вскрышей мощностью от 20 до 80 футов. Водоснабжение было недостаточно обильным, чтобы оправдать крупномасштабные операции. Русло кажется небольшим и было отработано настолько, насколько это коммерчески возможно.

Испания.

— То, что может оказаться коммерческими россыпными месторождениями, было найдено в Сьерра-Ронда, на юге Испании, примерно в 50 милях к северо-западу от порта Малага. Месторождения были довольно подробно описаны Дюпарком [190]. По-видимому, гравии не были многократно переотложены природой, концентрация платины невелика, и проблематично, будет ли оправдана их обширная разработка.

[190] Дюпарк, Луи, и Гроссет, Огюстен: «Etude comparée des gîtes platiniferes de la Sierra de Ronda et de l’Oural»: Soc. Phys. et Hist. Nat. Geneve, Mem., т. 38, fasc. 5, 1916.

Другие страны.

— Небольшое количество платины производится в качестве побочного продукта на золотых драгах на реке Иравади в Индии и на оловянных драгах в Голландской Ост-Индии. Поступили неподтвержденные сообщения об открытиях платины в южной Сибири, в различных местах в Мексике и из нескольких мест в Эквадоре и Перу. Известно, что платина встречается в некоторых реках, а также в некоторых золотых месторождениях района Минас-Жерайс в Бразилии.

На юго-западе Борнео платина встречается в районе Танат-Лаут. Несколько русских авторов предоставили информацию об этом регионе.

ВЕРОЯТНЫЕ ИЗМЕНЕНИЯ В ИЗВЕСТНОМ ГЕОГРАФИЧЕСКОМ РАСПРЕДЕЛЕНИИ В БЛИЖАЙШЕМ БУДУЩЕМ

В настоящее время российские платиновые месторождения практически бездействуют. Драги по большей части не работают, и промышленность дезорганизована. Потребуются значительные расходы и несколько месяцев времени, чтобы восстановить российскую платиновую промышленность. Известные месторождения российского района истощаются, и запасы известных платиноносных гравиев, по словам Дюпарка, имеют срок жизни 12 лет, исходя из довоенного уровня добычи; или, иначе говоря, известные месторождения способны произвести от 3 000 000 до 3 600 000 унций платины, прежде чем они будут исчерпаны.

Колумбия, по-видимому, обладает большими запасами неосвоенных платиносодержащих земель, хотя доступно так мало подробной информации, что небезопасно предсказывать их будущее. Однако можно с уверенностью отметить, что все отчеты указывают на то, что тщательная разведка в районе Чоко, вероятно, будет вознаграждена открытием значительных площадей платиносодержащих земель.

Канадские месторождения содержат некоторые перспективы для будущей добычи. Несколько недавних открытий платины вдоль Скалистых гор в Британской Колумбии, от Туламиена до Стикина, указывают на то, что дальнейшие поиски могут быть вознаграждены. Если сообщения верны, то на реках Туламиен, Уиллоу и Пис есть значительная площадь, которую можно драгировать для добычи золота и платины. Самые важные канадские запасы платины находятся в никелевых месторождениях Садбери, но нынешнюю металлургическую практику придется изменить, чтобы получить максимальный выход платины и палладия из этих руд.

В Соединенных Штатах, по-видимому, нет надежды на значительное увеличение добычи платины; фактически, может случиться так, что добыча будет существенно меньше, когда в Канаде будут завершены новые аффинажные заводы для переработки руд Садбери. Россыпные месторождения, содержащие платину, по большей части относительно невелики; многие из тех, что находятся в северной Калифорнии и Орегоне, не могут разрабатываться экономически, и лишь немногие доступны для драгирования. По мере того как золотодобывающие поля вдоль подножия Сьерры будут истощаться, добыча платины в этой стране будет пропорционально снижаться, если не будут открыты новые земли и месторождения гравия, более богатые платиной, чем те, что известны сейчас.

Различные австралийские месторождения платины не кажутся особенно многообещающими в отношении добычи, за возможным исключением дражного поля Болд-Хилл в Тасмании. Месторождения Файфилд, по-видимому, почти истощены, а пляжные отложения в Новом Южном Уэльсе и Квинсленде слишком низкого качества, а распределение ценных минералов слишком беспорядочно, чтобы представлять большой коммерческий интерес.

Испанские месторождения еще не были достаточно исследованы, чтобы определить их масштаб, но опубликованные отчеты, по-видимому, не указывают на то, что они окажутся очень большими или особенно богатыми.

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ

Как показывает Таблица 74, Россия имеет политический контроль над примерно 90 процентами мировых запасов платины. Представляется вероятным, что Канада, благодаря никелевой руде района Садбери и известным россыпям в районах Туламиен и Баркерсвилл, контролирует третий по величине запас платины. Месторождения, находящиеся под политическим контролем Соединенных Штатов на Аляске и на Тихоокеанском побережье, относительно незначительны. Великобритания, естественно, контролирует платину в своих колониальных владениях: Австралии, Тасмании и Индии. Добыча в Голландской Ост-Индии, на Борнео и Суматре, относительно невелика, хотя существует вероятность того, что добыча в этих странах может быть увеличена. Испания, возможно, контролирует небольшую добычу платины, хотя не кажется вероятным, что добыча в этой стране когда-либо будет большой. Обширная территория в горах Сьерра-Ронда была выделена правительством для дальнейшей разведки под эгидой правительства, и кажется разумным полагать, судя по общей минеральной политике Испании, что в случае подтверждения коммерческих месторождений они будут разрабатываться под эгидой правительства, а не частными лицами.

Хотя месторождения в Колумбии политически контролируются этой страной, они, тем не менее, в значительной степени принадлежат американским интересам.

КОММЕРЧЕСКИЙ КОНТРОЛЬ

Через владение рудниками.

— До войны французские коммерческие интересы практически доминировали в платиновой промышленности России через операции Compagnie Internationale du Platine. Эта компания не только имела обширные горнодобывающие активы, но и имела контракты с двумя крупнейшими независимыми российскими производителями платины, а именно компаниями Шувалова и Демидова, на весь их объем добычи. Контракты были приостановлены французской компанией вскоре после объявления войны и, возможно, не будут возобновлены. Однако существуют две российские компании, которые более или менее независимы от французского контроля, и есть большое количество мелких старателей и крестьян, которые не подчиняются какой-либо конкретной закупочной организации. По-видимому, по крайней мере 75 процентов добычи платины в России контролируется (или контролировалось до большевистского господства) следующими компаниями: Compagnie Internationale du Platine (французская), компания Шувалова (российская), компания Демидова (российская), Николо-Павдинская компания (российская) и компания «Платина» (российская). В течение 1914 года эти компании эксплуатировали около 35 драг на платиновых месторождениях, хотя, согласно лучшим доступным сейчас отчетам, не похоже, чтобы более двух или трех драг работали в течение 1917 года. Читатель должен, однако, осознавать, что добыча драгами всегда была относительно небольшой по сравнению с объемом, полученным другими методами. По оценкам, около 80 процентов платины, добываемой из российских россыпей, извлекается ручным трудом арендаторов (старателей), которые заключают контракты на продажу своей продукции компаниям, владеющим землей, и платят роялти за право работы. После войны крестьяне и старатели фактически контролируют все рудники, и первоначальные операторы имеют мало отношения к эксплуатации или управлению.

Самые важные платиноносные россыпи в Колумбии контролируются американскими финансовыми интересами. General Development Co. из Нью-Йорка через две дочерние компании контролирует обширную территорию в верховьях реки Сан-Хуан, особенно на реке Кондото. Недавно эти интересы организовали South American Gold & Platinum Co. Quito Mining Co. контролирует значительную площадь на реке Кито между Кибдо и Истиминой. Существуют и другие небольшие американские владения в районе Негуа, в бассейне Атрато, и на реках Тамана и Сипи в бассейне Сан-Хуан. В конце 1917 года была организована британская компания для разработки обширных владений на реке Опогодо в верховьях бассейна Сан-Хуан. Если нынешние условия не будут изменены специальным законодательством в Колумбии, представляется, что американские финансовые интересы будут продолжать доминировать в колумбийском платиновом районе.

Платиновые месторождения Соединенных Штатов, по-видимому, в значительной степени находятся в руках мелких владельцев, которые являются гражданами этой страны. Несколько крупных драг в Калифорнии, которые производят платину в качестве побочного продукта, частично принадлежат британскому капиталу.

По-видимому, пляжные отложения в Австралии (в Новом Южном Уэльсе и Квинсленде) разрабатываются в небольшом масштабе местным капиталом, как и месторождения возле Платины и Файфилда. Тасманийские месторождения контролируются местным капиталом.

Что касается Канады, то считается, что большая часть гравийной площади реки Туламиен, недалеко от Принстона, Британская Колумбия, контролируется американским капиталом. Несколько заявок на верхнем Туламиене контролируются канадским капиталом. Недавно была организована американская компания с целью эксплуатации некоторых перспективных районов в регионе Баркерсвилл, в северо-центральной части Британской Колумбии, и считается, что канадский капитал имеет довольно обширные владения на реке Пис, в северной части Британской Колумбии, которые, как сообщается, содержат значительные количества платины. Никелевые месторождения Онтарио, которые имеют значительную перспективную ценность как производители платины и палладия, эксплуатируются Mond Nickel Co. под британским контролем и International Nickel Co. под американским контролем. Однако канадское правительство регулирует деятельность обеих этих компаний.

Через владение перерабатывающими заводами.

— Любопытный факт: хотя большая часть российской сырой платины продается через французскую компанию, тем не менее Англия аффинировала большую часть добычи России. Johnson Matthey Co. из Лондона является крупнейшим аффинером платины в Англии. До войны эта компания, как говорят, аффинировала около 70 процентов российской добычи платины.

В Германии главным аффинером платины является W. C. Heraeus из Ханау. Эта компания, как говорят, принадлежит главным образом доктору Хереусу и наследникам Генриха Хереуса. Фирма F. Eisennad & Co. в Оффенбахе, небольшой аффинер платины, была приобретена интересами Хереуса непосредственно перед войной. G. Seibert из Ханау также аффинирует платину, операции финансируются братьями Зейберт и Deutsche Gold und Silberscheidenanstalt из Франкфурта. Согласно российским данным, около 25 процентов российской добычи аффинировалось Германией, и, по-видимому, большая часть работы выполнялась Хереусом. Интересы Хереуса, без сомнения, преобладают в платино-аффинажной промышленности Германии.

Главным аффинером платины во Франции является Quenessen, de Belmont, Legendre et Cie., которая контролируется наследниками MM. Десмути и Ламера. Другие небольшие аффинажные заводы — это Lyon Allemand, Credit Lyonnais, Herique Marrett & Bonnin и Hesse Fils, все из Парижа. По-видимому, первая компания является контролирующим фактором во французской промышленности.

В Соединенных Штатах платиновая промышленность контролируется Baker & Co., American Platinum Works, Irvington Smelting & Refining Works, Hanovia Chemical Co. и Чарльзом Энглехардом. В Соединенных Штатах есть несколько независимых аффинеров платины, хотя их совокупная добыча составляет менее четверти отечественной промышленности. Это J. Bishop & Co., Малверн, Пенсильвания; Wilson Co., Ньюарк, Нью-Джерси; Belais & Cohn, Нью-Йорк; Kastenhuber & Lehrfeld, Нью-Йорк, и Goldsmith Bros., Smelting & Refining Co., Нью-Йорк и Чикаго, которые финансово управляются американским капиталом. Rossler & Hasslacher Chemical Co. из Нью-Йорка также аффинирует некоторое количество платины.

До войны интересы компаний Johnson and Matthey (Лондон), Quenessen (Париж), Heraeus (Ханау) и Baker & Co. (Нью-Йорк) были в той или иной степени взаимосвязаны. Общепризнано, что до войны компания Heraeus фактически контролировала американские активы, в настоящее время находящиеся под управлением Englehard. Однако после объявления войны эти компании в результате обмена акциями были разделены, и теперь представляется, что германский капитал более не заинтересован в английской, французской или американской платиновой промышленности. Тем не менее вероятно, что английская и французская компании по-прежнему владеют акциями американской компании, хотя контроль над американскими активами в настоящее время принадлежит Чарльзу Энглхарду посредством владения контрольным пакетом акций вышеупомянутых компаний.

Сообщается, что до войны в России существовало два государственных платиноперерабатывающих завода, хотя, по-видимому, они перерабатывали лишь незначительную часть платины, добываемой в России, и не принимали платину из каких-либо зарубежных стран.

ПОЛОЖЕНИЕ В МИРЕ В ОТНОШЕНИИ ПЛАТИНЫ

Как было объяснено выше, благодаря расположению основных регионов добычи платины Россия являлась источником практически всей мировой платины, хотя коммерческий контроль над сбытом основной части российской продукции осуществляли французы. С 1914 года экспорт платины практически прекратился, а те незначительные объемы, которые все же вывозились, поступали преимущественно в Соединенные Штаты. Ситуацию в различных странах можно резюмировать следующим образом:

Россия в обычное время потребляла мало собственной платины, экспортируя ее в Англию, Германию и Францию. В стране практически отсутствовали мощности по аффинажу платины, а отрасль контролировалась французским и российским капиталом при более или менее заметном германском влиянии. После начала войны платиновые прииски не разрабатывались в широких масштабах, и фактически их добыча значительно сократилась. Любые накопленные запасы платины, которые могли находиться в России, вероятно, попали в Германию и страны союзников.

До войны Германия рафинировала около 25 процентов российской добычи платины; собственных месторождений на ее территории нет. Она создала мощную химическую и электротехническую промышленность, требовавшую больших запасов платины, и, вероятно, к моменту объявления войны находилась в достаточно устойчивом положении в отношении этого металла. Представляется вероятным, что в настоящее время в Германии ощущается нехватка платины для сколько-нибудь значительного расширения химической или электротехнической промышленности.

Франция, благодаря контролю над основной частью российской добычи, имела возможность накопить значительные запасы платины, и о том, что она это сделала, свидетельствует тот факт, что правительство не предпринимало никаких мер по регулированию платиновой промышленности до начала 1918 года, и не похоже, чтобы возникла необходимость в каком-либо значительном расширении основных отраслей, требующих платины.

Около 70 процентов российской, вероятно, половина колумбийской и вся австралийская и индийская платина до войны продавались в Англии. Считается, что не вся она рафинировалась в Англии, поскольку значительные объемы сырой платины экспортировались из Англии в Соединенные Штаты; тем не менее к моменту объявления войны в Англии имелись большие запасы платиновых металлов. Во время войны Англии пришлось создавать мощную химическую промышленность, и она быстро израсходовала имевшиеся резервы, поэтому правительство еще в начале войны осознало необходимость контроля над использованием платиновых металлов.

Соединенные Штаты зависели и будут продолжать зависеть от иностранной платины. В настоящее время вся колумбийская платина поступает в эту страну. Когда мы вступили в войну, запасы платины в Соединенных Штатах составляли около 50 процентов от нормы, и, поскольку нам пришлось создавать крупные химические и электротехнические предприятия, эти запасы были быстро исчерпаны.

В Колумбии нет платиноперерабатывающих заводов; по-видимому, у нее нет потребности в использовании продукции своих приисков. До войны ее сырая платина отправлялась на аффинаж в Англию и Соединенные Штаты, но в настоящее время вся она поступает в Соединенные Штаты.

РЕЗЮМЕ

Около 90 процентов ежегодно добываемой сырой платины поступало с Уральских гор, Россия. Следующие по значимости месторождения расположены в Колумбии, Южная Америка. Небольшие количества добываются в Канаде (главным образом в качестве побочного продукта при рафинировании никелевой руды), в Новом Южном Уэльсе, на Тасмании, в Соединенных Штатах, Голландской Ост-Индии, Индии и Испании.

Политический контроль над мировыми месторождениями платины соответствует их географическому распределению. Россия и Колумбия контролируют основные месторождения, а Соединенные Штаты, Великобритания, Голландия и Испания — второстепенные.

До войны французская компания владела обширными активами в России, а кроме того, имела контракты с двумя российскими производителями платины на весь объем их добычи. Эти контракты были расторгнуты вскоре после объявления войны. Оставшиеся месторождения на российских приисках контролируются двумя независимыми российскими компаниями и большим числом мелких старателей. В настоящее время крестьяне и старатели фактически контролируют прииски, а владельцы почти не участвуют в их эксплуатации или управлении.

Основные платиноносные россыпи Колумбии контролируются американскими интересами. Недавно была организована британская компания для разработки активов в верховьях бассейна реки Сан-Хуан. За исключением нескольких крупных драг в Калифорнии, частично принадлежащих британскому капиталу, платиновые месторождения Соединенных Штатов принадлежат американским гражданам. Платиновые месторождения Австралии, вероятно, по большей части находятся в руках британского капитала.

Американский капитал контролирует значительную часть платиноносных гравийных площадей в Британской Колумбии. Несколько участков контролируются канадцами. Компании, эксплуатирующие никелевые месторождения в Онтарио, из которых платина извлекается как побочный продукт, являются американскими и британскими.

Около 75 процентов российской платины рафинировалось в Англии, а большая часть остального объема — в Германии. До войны существовала взаимосвязь интересов аффинеров платины Соединенных Штатов, Германии и Великобритании, которая была разрушена в той части, что касается Германии.

ГЛАВА XXXII КТО ВЛАДЕЕТ ЗЕМЛЕЙ? Джозайя Эдвард Спурр

Давайте бегло рассмотрим предыдущие исследования одно за другим и увидим, какие характерные черты содержит каждое из них.

ТОПЛИВНЫЕ МИНЕРАЛЬНЫЕ РЕСУРСЫ

Нефть

имеет огромное значение в настоящее время, а ее будущее значение будет еще больше. В последнее время 98 процентов мировой добычи обеспечивали следующие страны в порядке убывания значимости: Соединенные Штаты, Россия, Мексика, Голландская Ост-Индия, Румыния, Индия, Персия и Галиция. Считается, что регион вокруг Карибского моря и Мексиканского залива будет приобретать все большее значение, так же как и персидские и месопотамские месторождения.

Капитал Соединенных Штатов занимает господствующее положение в коммерческом контроле над нефтяной промышленностью в Западном полушарии, в то время как британские и британско-голландские интересы легко доминируют в нефтяной ситуации в Восточном полушарии.

Коммерческий контроль над нефтью определяется главным образом через владение эксплуатирующими компаниями землями, договорами аренды или концессиями. Государственная собственность встречается редко, хотя в Аргентине нефтяная промышленность принадлежит государству и управляется им. Британское правительство контролирует путем прямого владения большинством голосующих акций компанию Anglo-Persian Oil Co., что дает ей монополию на персидском месторождении через концессию на территорию площадью 500 квадратных миль, предоставленную Персией компании, и закрывает доступ к этому месторождению для предприятий Соединенных Штатов или других стран; более того, через разветвленную структуру этой компании британское правительство расширяет свое влияние на другие части мира.

В Соединенных Штатах коммерческий контроль над нефтяной промышленностью находится в руках «группы Standard Oil». Британские и британско-голландские компании в Соединенных Штатах контролируют добычу около 11 000 000 баррелей в год из общего объема в 335 000 000. В важном регионе Мексики, который сейчас занимает второе место по добыче, коммерческий контроль полностью находится в руках иностранцев: американские интересы контролируют 65 процентов, а британские и голландские — 32 процента.

В Восточном полушарии продуктивный район Голландской Ост-Индии находится под абсолютным контролем британско-голландских интересов — синдиката Royal Dutch-Shell. Лицензии на разведку и концессии предоставляются только голландским подданным и голландским компаниям, и это, наряду с экономической монополией контролирующих британско-голландских интересов, препятствует деятельности иностранных предприятий.

Абсолютный и исключительный контроль британского правительства над крупными нефтяными месторождениями Персии и Месопотамии будет подтвержден и расширен за счет распространения власти Британской империи на те части Турецкой империи, которые она завоевала силой оружия.

В России коммерческий контроль над крупной нефтяной промышленностью, по-видимому, является британским, причем преобладающими интересами являются британские, франко-британские и британско-голландские (синдикат Royal Dutch-Shell). Основные добывающие районы в России находятся или до недавнего времени находились под британским военным контролем.

Добыча в Индии (Бирма) полностью находится в британских руках.

«Общая политика Британской империи, по-видимому, заключается в контроле над всей разработкой нефти и ограничении операций иностранного капитала». Подобные ограничения правительственными постановлениями существуют в Австралии, Канаде, Индии, Барбадосе, Британской Гвиане, Британском Гондурасе, Тринидаде и других колониях.

Таким образом, в нефтяной промышленности мы наблюдаем примечательное и поразительное разделение мирового богатства между двумя великими англосаксонскими нациями — Америкой и Великобританией. Ни один минеральный ресурс не поддается так легко транспортировке, а следовательно, и коммерческому контролю, как нефть. Согласно текущим объемам добычи, американские интересы значительно превосходят остальные. Однако британский контроль над крупными месторождениями Восточного полушария, многие из которых лишь частично освоены, вместе с растущим влиянием в Западном полушарии указывает на вероятность того, что британский захват мировых нефтяных ресурсов и добычи в будущем может стать преобладающим.

Поразительными аспектами ситуации являются то, что в случае с Великобританией правительство и нефтяные монополии объединены, так что по всем намерениям и целям контроль осуществляется непосредственно британским правительством; в то время как в Соединенных Штатах контроль находится в руках чисто коммерческих интересов, действующих без контроля, помощи или поддержки со стороны правительства. Американские компании не могут владеть и эксплуатировать нефтяные земли в Британской империи, во французских владениях или голландских колониях, но в Соединенных Штатах нет никаких ограничений на иностранное владение или эксплуатацию.

Политика Великобритании, обеспечивающая ее нефтью и бункеровочными станциями по всему миру и гарантирующая ей контроль над морями, будет в дальнейшем неизмеримо увеличивать ее и без того обширное мировое господство.

У Соединенных Штатов нет такой программы имперской экспансии, но у них есть доктрина Монро, которая в мягкой форме является предполагаемым протекторатом над Западным полушарием.

Уголь.

— Далее давайте перейдем к углю, одному из самых важных среди всех минеральных ресурсов — источнику энергии, света и тепла, а также средству плавки железа и других металлов. Здесь снова, как и в случае с нефтью, мы обнаруживаем, что Соединенные Штаты удивительно одарены природой. Им приписывают запасы в 3 527 000 миллионов тонн из общего мирового объема в 7 909 000 миллионов, или практически половину всех мировых запасов. Поскольку мировые запасы угля велики, первостепенное значение имеют высококачественные сорта, расположенные так, чтобы иметь дешевую транспортировку. Великобритания имеет такой уголь недалеко от побережья, и поэтому до войны контролировала экспортную торговлю по всему миру. Промышленность Америки оставляет ей мало угля для экспорта, и ее уголь находится дальше от побережья. Усилия Германии до войны по созданию экспортной торговли углем сдерживались длительными железнодорожными перевозками; и эти месторождения сейчас передаются Франции. Помимо Франции, Великобритании и Соединенных Штатов, только Канада, Австралия и Китай имеют достаточные запасы для обширной экспортной торговли. Из этих стран Китай является наиболее вероятным кандидатом на увеличение экспорта из-за близости к побережью и хорошего качества угля.

Хотя уголь Соединенных Штатов находится не так близко к побережью, как в Англии, он не только составляет, как было сказано выше, самые большие запасы, но и является наиболее доступным в ближайшей перспективе благодаря небольшой глубине залегания и хорошим возможностям железнодорожного транспорта.

Ни одно природное вещество не используется так повсеместно и не является столь необходимым каждому человеку, как уголь, и поэтому каждый человек чувствует естественное право на него и полагает, что он должен быть доступен по минимальной цене. Это привело в ряде стран к национализации угольной промышленности, как в некоторых частях Чили, Болгарии, Пруссии и Австралии. В других странах, как в некоторых частях Соединенных Штатов, правительство сохраняет право собственности на угольные земли, сдавая их в аренду частным операторам. В Англии нынешние условия указывают на национализацию угольной промышленности. Во Франции угольные земли принадлежат правительству, которое предоставляет концессии на их разработку и получает роялти или арендную плату и процент от чистой прибыли оператора.

Хотя Соединенные Штаты занимают выдающееся положение среди мировых держав в отношении угля, Англия имеет преимущество в виде наличия адекватных запасов, разбросанных по всему миру, в ее колониях: Австралии, Канаде, Индии, Новой Зеландии, Южной Африке, Родезии и на Борнео.

В отличие от нефти, уголь — это минеральный ресурс, который не поддается легко контролю со стороны коммерческих объединений. Добыча и сбыт угля — простое дело, требующее относительно мало навыков или оборудования, поэтому это бизнес, открытый для всех; а обширность угольных земель обеспечивает множество владельцев. Поэтому влияние контроля над углем на мировую торговлю и историю является почти полностью вопросом политического контроля. Организация среди производителей существует в различных странах, как в случае с антрацитовой промышленностью Соединенных Штатов, но это, как правило, не распространяется на централизованную собственность и обычно не распространяется на зарубежные страны.

Таким образом, в угле, как и в нефти, мы обнаруживаем, что двумя доминирующими нациями являются великие англосаксонские державы — Англия и Соединенные Штаты. Соединенные Штаты добывают около 40 процентов, или две пятых мировой годовой добычи, в то время как Британские острова производят одну пятую, занимая второе место после Соединенных Штатов. Ни в том, ни в другом случае соответствующие правительства в прошлом не пытались контролировать добычу и продажу угля, но в Англии, по крайней мере, вероятно, что появится какая-то форма совместного контроля с участием правительства и шахтеров.

Методы добычи, необходимые для максимального производства на британских угольных шахтах во время войны, привели к тому, что шахты оказались в настолько плохом состоянии, что потребуется год или два, прежде чем они смогут обеспечить весь прежний объем британской экспортной торговли. Требования британских рабочих о сокращении рабочего дня (приводящие к снижению добычи) еще больше затруднят возобновление крупных экспортных поставок. Одной из важных сторон этого, как для Англии, так и для Америки, является торговля с Южной Америкой. Англия всегда снабжала этот рынок, но Соединенные Штаты, вероятно, будут делать это в настоящее время, и должны позаботиться о том, чтобы делать это, если они желают торговать с Южной Америкой, и исходя из коммерческой теории доктрины Монро. До недавнего времени Соединенные Штаты экспортировали морским путем лишь около 4 процентов своей добычи, тогда как Англия отправляла 25 процентов. Наша собственная расширяющаяся промышленность обеспечила достаточный рынок.

Помимо Америки и Англии, нет доминирующего фактора в будущем контроле над угольной промышленностью в странах, окружающих Атлантический океан. Германия была сильным фактором до войны, но потеря Францией Саарского угольного района и возможная потеря Польшей Домбровского месторождения в Силезии лишат ее значимости; а раздел этих ресурсов между несколькими нациями не позволит ни одной из них стать мировым фактором в угольной торговле.

Однако в странах вокруг Тихого океана наиболее важным будущим фактором являются угольные месторождения Китая. Ни одна страна, кроме Соединенных Штатов, не имеет больших запасов высококачественного угля, готовых к разработке и находящихся недалеко от морских путей. Вероятно, японцы могут попытаться осуществить эту разработку и содействовать развитию экспортной торговли на Востоке. Высококачественные угли Соединенных Штатов удалены от Тихого океана и могут быть доступны для тихоокеанской торговли только по длинному маршруту через Панамский канал. Поэтому не исключено, что китайский уголь в будущем может поставляться в наши собственные тихоокеанские порты японцами по более низкой цене, чем американский уголь, и что благодаря этому развитию Япония сможет доминировать в тихоокеанской торговле, как Англия доминировала в торговле Атлантического и Тихого океанов в прошлом.

МИНЕРАЛЬНЫЕ РЕСУРСЫ ДЛЯ СТАЛИ И ФЕРРОСПЛАВОВ

Железо.

— Поставки железа для мирового потребления осуществлялись главным образом из четырех стран: Соединенных Штатов, Германии, Франции и Великобритании. Более одной трети общего объема добычи приходилось на Соединенные Штаты, и около 85 процентов американской продукции поступало из района озера Верхнее, который один ежегодно производит более 30 процентов мирового объема. Следующими по значимости после Соединенных Штатов были Германия и Франция, и около 80 процентов добычи этих двух стран приходилось на месторождения Лотарингии на границе. Ежегодный объем добычи этих месторождений составлял 25 процентов мирового производства, или почти столько же, сколько в районе озера Верхнее.

Будучи связанной с угольной промышленностью, попыток создания мировых или даже национальных монополий на железную руду не предпринималось. Крупнейшей отдельной коммерческой организацией в мире является United States Steel Corporation с общей годовой мощностью (в 1913 году) более 17 миллионов тонн чугуна, или около половины общего объема американского производства. Но эта организация не является монополией, и существует большое количество мощных независимых компаний. Во Франции и Германии доминирующих организаций не отмечено. В Англии до начала войны железная промышленность контролировалась посредниками, а производители были недостаточно организованы. Чтобы исправить это положение (стр. 86), Комитет Совета по торговле Великобритании рекомендовал консолидацию интересов в черной металлургии.

Расширение коммерческого контроля доминирующими железодобывающими нациями на запасы руды и на железную промышленность зарубежных стран, создающее тем самым ту коммерческую полутень империи, которая так склонна углубляться в фактический суверенитет, однако гораздо более заметно в случае с железом, чем с углем, хотя и менее значимо, чем в случае с нефтью. Контроль со стороны Англии и Соединенных Штатов над крупными железорудными месторождениями в Южной Америке и расширение японского контроля над запасами железной руды в Китае являются наиболее значимыми чертами этой ситуации. Во Франции еще до войны Германия контролировала более одной трети бизнеса по производству железа и стали. С переходом германской Лотарингии к Франции вероятно, что значительная часть германского капитала останется.

Япония имеет промышленность по производству железа и стали, которая, хотя и невелика по сравнению с промышленностью Соединенных Штатов, Германии и Великобритании и других ведущих стран-производителей железа и стали, быстро расширяется. Доменные печи, сталеплавильные печи и сталепрокатные заводы строятся в Японии, а также в Корее, Маньчжурии и Китае японскими интересами. Япония все еще очень далека от обеспечения собственного потребления железа и стали, которое составляет полтора миллиона тонн ежегодно.

Короче говоря, что касается мирового производства железа и стали, Соединенные Штаты занимают значительно преобладающее положение, которое они будут стремиться упрочить, с желательной тенденцией к более тесному сближению Северной и Южной Америки. В Европе Франция и Германия странным образом объединены в контроле над второй по величине сталелитейной промышленностью в мире. На будущей великой арене Тихого океана Япония терпеливо строит свою сталелитейную промышленность с далеко идущим восточным видением. Угольные шахты и доменная печь включены в германские «права», недавно приобретенные Японией. Вернет ли Япония Шаньдун? Вернула ли Германия Эльзас-Лотарингию? В своих перспективных планах у Японии есть два национальных соперника — Англия и Америка. У нее есть обширное плодородное поле для работы, за исключением этих (особенно Англии) — вся восточная Азия. У нее есть великая дезорганизованная нация, которая больше не является соперником, а является полем, на котором можно кормиться и становиться сильнее — Сибирь и Россия.

Вслед за сталью, и сразу после проблем угля и железа, идут несколько менее известных и менее распространенных металлов — ферросплавы, металлы, которые сплавляются с железом для получения сталей особой твердости или вязкости, или с какими-то другими особыми качествами. Относительно незаметные, они незаменимы в промышленности.

Марганец.

— Марганец — это нечто гораздо большее, чем просто ферросплав. Он необходим при производстве всей стали мартеновским и бессемеровским способами, на долю которых приходится 99 процентов общего объема производства в Соединенных Штатах, поскольку он действует как удалитель углерода, который создает разницу в качестве между сталью и чугуном. Для этой цели он смешивается с железом в виде сплавов. Один из них богат марганцем — ферромарганец, а другой беден — зеркальный чугун (шпигель).

Основные марганцевые месторождения — это месторождения России, Индии и Бразилии, которые настолько велики и легко доступны для эксплуатации и транспортировки на рынки, что мало шансов, что они будут вытеснены в качестве основных источников мировых поставок в течение многих лет. В отличие от ситуации с другими важными минеральными ресурсами, большинство марганцевых месторождений по всему миру принадлежит жителям тех стран, в которых они находятся. Это объясняется поверхностным и нерегулярным характером оксидных месторождений (единственных, как правило, достаточно высокого качества, чтобы найти рынок сбыта) и простым характером добычи и промывки руд, что не требует больших капиталовложений.

Соединенные Штаты плохо обеспечены высококачественными марганцевыми рудами, и поэтому всегда были и всегда будут крупным импортером. До войны поставки в основном осуществлялись из России и Индии; а во время войны — из Бразилии, в дополнение к увеличению внутреннего производства под влиянием высоких военных цен. Англия, Франция и Германия — фактически весь промышленный мир — имеют одни и те же источники поставок. Нет особой необходимости в острой конкуренции, ведущей к коммерческим объединениям, или в строгом государственном контроле, поскольку производственная мощность основных месторождений очень велика и намного превышает мировой спрос на производство стали.

Хромит.

— Следующим по важности в группе металлов-ферросплавов является хром, встречающийся в природе в коммерческих масштабах только в виде оксида хромита. Хром широко используется в сталелитейной и кожевенной промышленности — в первой для производства стали особой вязкости (а также огнеупорной футеровки для железных печей); во второй — для дубления.

Хромит встречается во многих странах, но в большинстве (как в Соединенных Штатах и Канаде) в виде небольших и разбросанных месторождений, легко истощаемых. Самые крупные и важные источники поставок находятся во французской колонии Новая Каледония в южной части Тихого океана; в Родезии в Африке; в Малой Азии; и на Уральских горах, Россия. До 1830 года Уральский регион снабжал мир хромом; с 1830 по 1870 год главным источником стали восточные штаты Соединенных Штатов (Мэриленд и Пенсильвания); с 1870 по 1900 год центр основной активности переместился в Малую Азию; а с тех пор на мировых рынках доминируют новокаледонские и родезийские руды. Новокаледонская руда добывается с использованием дешевой рабочей силы, а месторождения находятся недалеко от побережья; родезийские месторождения велики и богаты. Высокие цены во время войны из-за нехватки судоходства привели к значительному увеличению добычи в тихоокеанских штатах Соединенных Штатов; но с возвращением к нормальным условиям этот регион не сможет выдержать конкуренцию, если не будет специально защищен законодательством.

В обычное время Соединенные Штаты потребляют более одной трети мирового годового потребления хромита, но зависят от иностранных источников — Родезии и Новой Каледонии. Во время войны использовались месторождения ограниченного размера в Бразилии и на Кубе, а также канадские и отечественные руды. Однако, насколько известно, Западное полушарие относительно бедно месторождениями хромита. Хромовая промышленность в Соединенных Штатах сильно централизована: компания Electrometallurgical Company обладает почти абсолютной монополией в феррохромовой промышленности и, вероятно, является крупнейшим производителем феррохрома в мире, а компания Mutual Chemical Company имеет значительное преобладание в химической хромовой промышленности.

Таким образом, мировые поставки хромита в настоящее время по существу являются монополией, контролируемой британско-французским капиталом, а крупные запасы находятся в колониях Англии и Франции.

Никель.

— Положение никеля довольно необычно, поскольку месторождения, пригодные для разработки, встречаются редко, а месторождения большого значения ограничены несколькими местами. Единственными действительно коммерчески важными месторождениями являются месторождения Садбери в Канаде и Новой Каледонии; хотя небольшие месторождения пригодной для разработки руды добывались в Норвегии, а никеленосная и хромистая железная руда встречается на Кубе.

Месторождения Садбери относительно гораздо важнее, чем месторождения любого другого района. Поэтому Великобритания (через Канаду) обладает, безусловно, самыми крупными и важными никелевыми месторождениями, что практически равносильно исключительному контролю. Ранее американский капитал осуществлял доминирующий коммерческий контроль над никелевой промышленностью благодаря владению крупнейшими запасами руды и контролю над плавильными и рафинировочными заводами в Соединенных Штатах. Одна из этих американских компаний также имеет вторые по величине активы в Новой Каледонии. Британское правительство явно приняло меры для преодоления этого коммерческого доминирования. В Садбери начала деятельность крупная компания, в которой британское правительство имеет контрольный пакет акций. Правительство также добилось перевода операций по рафинированию компании International Nickel Company из Нью-Джерси в Онтарио, так что вся отрасль будет сосредоточена в Канаде.

Вольфрам.

— Крупнейшим вольфрамодобывающим регионом является восточная Азия; регион Соединенных Штатов и Мексики — второй; регион Боливии и соседних стран в Южной Америке — третий; и четвертое место занимают Португалия, Испания и Италия. По-видимому, не существует очень крупных и концентрированных вольфрамовых месторождений; и почти все разрабатываемые подают признаки того, что их легко истощить. Поэтому в будущем может возникнуть мировая нехватка вольфрама. Возможно, Боливия окажется самым долговечным месторождением.

Что касается коммерческого контроля, то он полностью находится в британских руках, и это благодаря активной политике британского правительства. Фактический контроль осуществляется через производителей ферровольфрама, к которым руды поступают для обработки. На этой основе коммерческий контроль в 1917 году распределялся так: британский — 14 606 тонн; американский — 9 479 тонн; японский — 1 165 тонн; французский — 1 057 тонн; и германский — 360 тонн.

Американский капитал контролирует вольфрамовые месторождения в пределах своих границ и в Мексике, а также в значительной степени заинтересован в Боливии и Китае. До войны Германия контролировала, вероятно, половину добычи вольфрама, а другая половина была разделена между Соединенными Штатами, Англией и Францией. В настоящее время контроль через владение шахтами и плавильными заводами распределяется следующим образом: Великобритания — 54 процента; Соединенные Штаты — 35 процентов; Япония — 4 процента; Франция — 4 процента; и Германия — 1 процент.

Ванадий.

— Ванадий — важный металл для ферросплавов. Ванадиевая сталь обладает большой вязкостью и прочностью на кручение и используется в деталях автомобилей, стволах орудий и тому подобном. Хромованадиевые стали имеют обширный рынок сбыта.

Самые крупные и важные месторождения ванадия в мире находятся в Перу, и до недавнего времени они контролировались American Vanadium Company (американской фирмой), имеющей концессию от перуанского правительства. В остальном наиболее важные месторождения находятся на юго-западе Колорадо и до недавнего времени контролировались Primos Chemical Company из Пенсильвании. American Vanadium Company обладала абсолютной мировой монополией на продукты ванадия и феррованадий до выхода на рынок компании Primos. Совсем недавно активы обеих этих компаний были поглощены Vanadium Corporation, связанной с Bethlehem Steel Corporation.

Сурьма.

— Сурьма имеет относительно ограниченное использование в мирное время, но война создает (для производства шрапнели) значительно возросший спрос. В нормальных условиях предложение намного превышает спрос. Китай долгое время был самым важным источником поставок и, вероятно, останется таковым. Франция и Алжир также являются производителями, как и Мексика; другие страны производят под влиянием высоких цен. Соединенные Штаты, как и Канада, имеют относительно небольшие запасы и обычно небольшую добычу. Однако в начале европейской войны, в 1915 и 1916 годах, такие страны, как Боливия, Мексика, Австралия, Соединенные Штаты, Перу, Бирма и Испания, внесли важный вклад; но ни одна из них не будет важным фактором при обычных низких ценах.

До войны Англия была главным центром плавки сурьмы в мире. Руды со всего мира обрабатывались там, и британские марки считались более чистыми, чем другие, и практически монополизировали мировые рынки, включая рынки Соединенных Штатов. Во время высокого спроса в 1915 и 1916 годах британские интересы полностью контролировали боливийскую промышленность. До 1914 года одна из главных английских компаний имела контракты на продукцию Wah Chang Company, самого важного производителя сурьмы в Китае; но в 1914 году эта компания создала независимое торговое агентство в Соединенных Штатах. Это способствует переносу контроля над рынком сурьмы из Англии в Китай. Обладая всеми своими обширными минеральными ресурсами, Китай смог занять важное положение на мировых рынках лишь в отношении немногих металлов. Из них сурьма является наиболее ярким примером. С 1908 года более 50 процентов общего мирового производства сурьмы поступает из Китая.

Молибден.

— Использование молибдена в сталелитейном производстве пока находится почти на экспериментальной стадии, но, вероятно, станет важным. Он ценен в электротехнике.

Примерно до 1916 года практически вся молибденовая руда (молибденит, сульфид молибдена) поступала из Австралии и Норвегии. Вскоре после начала войны молибденит в Канаде стал заметным; а позже Соединенные Штаты вышли на передний план как производитель. В настоящее время Соединенные Штаты могут производить, вероятно, столько же, если не больше молибдена, чем весь остальной мир вместе взятый, главным образом благодаря крупным недавно открытым месторождениям в Клаймаксе, штат Колорадо. До этого развития Великобритания была крупнейшим производителем в Австралии и Канаде. Как британское, так и канадское правительства были очень заинтересованы в развитии канадского молибдена, и канадское правительство построило завод для концентрации руд. До войны контролируемая Германией American Metal Company, филиал германского «металлического спрута», получила через дочернюю компанию большую долю в контроле над месторождениями Клаймакса; а Primos Chemical Company, которая до войны имела прочные германские связи, производила ферромолибден из руды со своего собственного рудника в Эмпайре, Колорадо. Это, вместе с большим интересом, проявляемым Германией и германским капиталом к молибдену в других местах, привело к слухам о попытке германского контроля над американским молибденом.

Уран.

— Уран ценен для производства специальной стали, хотя используется только в небольших количествах. Он представляет чрезвычайный интерес из-за своей связи с радием, причем оба они получаются главным образом из минералов карнотита и уранинита (включая настуран). Радий используется в медицине и для светящейся краски. Единственными регионами, которые до сих пор производили большие количества радия и урана в коммерческих масштабах, являются Соединенные Штаты и Австрия. В настоящее время Соединенные Штаты производят в несколько раз больше, чем все остальные страны вместе взятые.

Цирконий.

— Цирконий используется в электрическом освещении, и проводились эксперименты с циркониевой сталью. Во время войны его одно время считали необычайно ценным в качестве ферросплава. Цирконий встречается в природе в виде смешанного оксида и силиката, бадделеита, и в виде силиката циркона. Месторождения бадделеита, имеющие более высокий процент циркония, вероятно, станут основным источником металла. Он встречается в коммерческих количествах только в Бразилии. Месторождения циркона находятся в Бразилии, а также в Индии; и месторождение второстепенного значения встречается в Соединенных Штатах (Флорида).

Торий и мезоторий.

— С цирконием необходимо рассматривать монацит, минерал, который является источником тория и мезотория. Нитрат тория используется в производстве калильных сеток Вельсбаха для газовых горелок; мезоторий является побочным продуктом его производства из монацита и представляет собой радиоактивное вещество, используемое в качестве заменителя радия при изготовлении светящихся красок и в терапевтических целях. Минералы циркона и монацит обычно встречаются вместе в речных или пляжных песках. Как и минералы циркония, монацит поступает главным образом из Бразилии и Индии; хотя в прошлом его успешно добывали в Соединенных Штатах, сейчас эта отрасль исчезла.

Промышленность нитрата тория в Соединенных Штатах тесно контролируется двумя компаниями: American Welsbach Company и Lindsay Light Company. Во время войны они поставляли нитрат тория также в Англию и Францию, осуществляя таким образом мировой контроль.

ОСНОВНЫЕ ЦВЕТНЫЕ МЕТАЛЛЫ

Медь.

— Соединенные Штаты выделяются как главный мировой производитель меди, производя в 1917 году 60 процентов мирового объема. Ни одна другая страна не производит и одной шестой того, что производят Соединенные Штаты. Американский капитал контролирует (частично через контроль над рафинированием) 78 процентов мирового производства.

Германия была одним из крупнейших потребителей меди, хотя и не крупным производителем. Из-за этого германские интересы в прошлом обеспечили значительный контроль над поставками меди, а также свинца, цинка и других металлов через контракты на рафинирование и продажу с горнодобывающими компаниями. Такой контроль, как правило, не распространяется на владение шахтами или плавильными заводами. Так, в течение многих лет компании, связанные с крупным германским металлическим синдикатом (Metallgesellschaft), имели влияние в медном бизнесе Соединенных Штатов. В Соединенных Штатах было три таких компании: American Metal Company, L. Vogelstein & Co. и Beer-Sondheimer & Co. Недавно первые две объединились; и все они были американизированы во время войны.

Коммерческий контроль над медью в мире, основанный на владении шахтами, в круглых цифрах составляет: американский капитал — 69 процентов (полностью в Западном полушарии); британский капитал — 13 процентов (в обоих полушариях, но главным образом в Восточном); японский — 8 процентов (полностью внутренний); германский — 6 процентов; и французский — 2 процента. Следует отметить, что из текущей добычи три четверти поступает из Западного полушария (Северная и Южная Америка) и только одна четверть — из остального мира. Вероятно, это справедливый показатель относительного богатства. Будущая добыча в Южной Америке, вероятно, будет расти быстрее, чем в Северной Америке, которая была освоена раньше. Для постоянного контроля над ситуацией с медью со стороны Соединенных Штатов необходимо, чтобы американский капитал продолжал занимать ведущее место в развитии Южной Америки.

Свинец.

— Соединенные Штаты являются крупнейшим производителем свинца в мире и обладают большими ресурсами. После Соединенных Штатов, в указанном порядке, идут Австралия, Испания, Германия и Мексика. Три державы — Соединенные Штаты, Британская империя и Испания — производят 76 процентов общего объема; из них Соединенные Штаты и Великобритания производят 60 процентов.

Наиболее поразительной особенностью свинцовой промышленности является тот факт, что по мере разрушения германской системы далеко идущего коммерческого контроля под эгидой правительства — через плавку, рафинирование и продажу — эта система была немедленно принята британцами и французами. Другими словами, они обнаружили, что германский план был настолько эффективным, что они не только заблокировали его навсегда в том, что касается их собственных стран, но и организовали аналогичные коммерческо-политические объединения, которые должны были не только заботиться обо всем их собственном свинцовом бизнесе, но и, подобно германской организации, распространяться на другие страны. Германское объединение остается активным за пределами территории бывших союзников.

Из всех великих свинцоводобывающих держав Соединенные Штаты — единственная, которая не обладает контролируемой правительством свинцовой монополией. Угрожающие мировые коммерческие монополии на свинец, как и на другие минеральные ресурсы, поэтому, благодаря возрождению националистического духа из-за войны, уступили место национально-коммерческим монополиям трех держав (Германии, Франции и Великобритании), каждая из которых призвана стать как можно более глобальной и, таким образом, конкурировать друг с другом и с чисто коммерческими организациями американской свинцовой промышленности. В Англии это движение приняло форму British Metals Corporation (охватывающей не только свинец, но и другие металлы). Британское казначейство представлено в Совете директоров.

Во Франции националистическое движение привело к формированию консорциумов или торговых монополий для каждой отрасли, организованных под эгидой правительства. Отрасль минеральных ресурсов представлена обществом Société Minerais et Metaux. Официальное объявление гласит, что это общество организовано под эгидой французского правительства для объединения французских производителей металлов, работающих как внутри страны, так и за рубежом, в кооперативную ассоциацию для покупки и продажи металлургической продукции.

В Америке основным коммерческим фактором является American Smelting & Refining Co., доминирующая на рынке благодаря контролю над перерабатывающими заводами, хотя она напрямую контролирует только одну треть добычи.

Цинк.

— Цинк и свинец обычно связаны в минеральных месторождениях, поэтому их геологическое и географическое распределение почти идентично. Из мирового производства цинка Соединенные Штаты производят 35 процентов, Германия — 25 процентов, Австралия — 15 процентов и Италия — 5 процентов.

До начала войны в 1914 году положение цинка было исключительным среди металлов в том смысле, что политический контроль или государственный суверенитет оказывали лишь незначительное влияние на отрасль. «Экономические факторы, — говорит наш автор, — делали неэффективным любой контроль, не имеющий международного масштаба. Очень большой процент цинковых руд в мире транспортировался из страны производства в другую для обработки, в некоторых случаях даже будучи реэкспортированными». Однако во время войны политический контроль в значительной степени использовался для укрепления и восстановления коммерческого контроля для главных воюющих наций. Это движение было особенно заметно в Британской империи, где теперь существует, как было отмечено выше в параграфах, обсуждающих свинец, совместный политический и коммерческий контроль. Иностранные интересы были устранены действиями правительства, и правительство сохранило долю в контроле через участие в маркетинговых организациях или финансовое участие в перерабатывающих предприятиях.

В цинковой промышленности, как и в промышленности ее тесно связанных металлов, меди и свинца, владение или контроль над перерабатывающими заводами, и более конкретно маркетинговыми организациями, были более важными в определении коммерческого контроля, чем государственный суверенитет или коммерческое владение шахтами. В последние годы маркетинговые организации стали глобальными и полностью доминировали в отрасли. Амбиции германских коммерческих интересов контролировать рынки металлов и ресурсы мира были более близки к реализации в случае с цинком, чем с любым другим металлом.

Во Франции, как отмечалось выше в случае со свинцом, была сформирована контролируемая правительством организация по маркетингу металлов для той же цели — защиты и преимущества в конкуренции. Однако британское доминирование в европейской цинковой промышленности кажется несомненным. Только американская промышленность остается нетронутой тесной организацией под эгидой правительства. Если Германия потеряет Силезию, она, вероятно, станет небольшим фактором в цинковой промышленности. Поскольку так много дверей закрыто перед ней британскими и французскими политическими и коммерческими объединениями, американскому правительству следует принять правительственные меры предосторожности, чтобы она не восстановила свои позиции в Соединенных Штатах, а также, насколько это возможно (следуя логическому завершению доктрины Монро), в остальной части Северной и Южной Америки.

Заметьте, что в цинковой промышленности, как и в любой другой отрасли, Япония быстро расширяется, и, достигнув предела своих собственных ресурсов, ее поле роста находится в Корее, Китае и Сибири. Нынешняя мощность Японии по плавке цинка больше, чем ее внутреннее потребление, и намного больше, чем внутренние поставки руды; руда импортируется из Китая, Сибири, Индокитая и Австралии.

Олово.

— Олово относится к группе минеральных ресурсов, которые можно классифицировать вместе по тому факту, что они не имеют широкого распространения, а встречаются в действительно коммерческих количествах только в нескольких точках земного шара, и тем не менее абсолютно необходимы для нашей индустриальной цивилизации. Таковы также хром, платина, соли калия, нитраты и никель. Из этой политико-коммерческой группы олово является важным членом. Примечательно для этой группы, что Соединенные Штаты не являются счастливым обладателем главного приза ни в одном из этих случаев. В случае с хромом это главным образом французские и британские колонии, в случае с платиной — Россия и Колумбия, в случае с солями калия — Германия, в случае с нитратами — Чили, в случае с никелем — опять же британские и французские колонии, а в случае с оловом — юго-восточная Азия и Боливия.

Соединенные Штаты производят менее одной пятой 1 процента своих потребностей, и их контроль над иностранными оловянными ресурсами через владение шахтами ничтожен. С другой стороны, Соединенные Штаты потребляют более половины олова в мире и являются крупнейшим производителем и дистрибьютором оловянной продукции. Оловодобывающая и плавильная промышленность мира доминируется Великобританией.

Олово используется в производстве жести, припоя, латуни и во многих других важных целях, и удовлетворительной замены ему нет. В войне, как и в мире, консервные банки так же необходимы, как винтовки. Алюминий является наиболее вероятным возможным заменителем олова в контейнерах, и Соединенные Штаты контролируют алюминиевую промышленность. Около 68 процентов олова в настоящее время производится в юго-восточной Азии и на соседних островах, 21 процент — в Боливии, 4 процента — в Нигерии и Южной Африке и 3 процента — в Англии. Боливийская добыча, вероятно, будет иметь тенденцию к росту.

Ртуть.

Ртуть, или жидкое серебро, является минералом определенной значимости, хотя и далеко не входит в число четырех последних, рассмотренных выше. Она полезна для производства лекарств и химикатов; в качестве детонатора для бризантных взрывчатых веществ; как пигмент; для обработки золотосодержащих и серебряных руд; а также для многих других целей. Крупнейшие месторождения ртути в мире находятся в Испании. Соединенные Штаты занимают второе место. Важный рудник Идрия близ Триеста, ранее австрийский, но по последним данным находящийся во владении Италии, занимает третье место. Добыча в остальном мире невелика. Таким образом, Испания, Италия и Соединенные Штаты разделяют добычу и контроль посредством государственного суверенитета. Крупнейший рудник Испании, Альмаден (величайший в мире), также принадлежит испанскому правительству и разрабатывается им. Испанское правительство заключает контракты на основе конкурсных предложений с победителем торгов на продажу ртути сроком на десять лет. В течение ряда последовательных периодов контракт присуждался Ротшильдам из Лондона. Благодаря этой договоренности рынок контролируется в Лондоне; а во время войны продажа была взята на себя британским правительством. Контроль над сбытом продукции этого рудника позволяет тем, кто его осуществляет, устанавливать цену на ртуть на мировых рынках.

Алюминий.

Важным металлом в настоящее время, который со временем станет еще более значимым, является алюминий. Хотя он является одним из основных компонентов всех горных пород в форме силикатов, его извлечение из этого соединения настолько затруднительно, что эта задача не была решена в промышленных масштабах. Поскольку в земных соединениях алюминия гораздо больше, чем железа, дефицита не будет, если не принимать во внимание стоимость. Промышленный алюминий производится из оксида — боксита. Боксит также используется непосредственно в качестве абразива и огнеупорного материала. Крупнейшие месторождения бокситов политически контролируются Соединенными Штатами и Францией, при этом Британская империя находится в благоприятном перспективном положении. Алюминиевые заводы мира контролируются Великобританией, Францией и Германией, а также Швейцарией, Италией и Норвегией. Алюминиевая промышленность Соединенных Штатов и Канады практически находится в руках одной компании, Aluminum Company of America, которая также владеет долями в Южной Америке и других странах. Французские производители алюминия создали централизованную организацию путем учреждения сбытовой компании L’Aluminium Française. British Aluminium Company является единственным производителем в Англии и контролирует ирландские месторождения.

НЕМЕТАЛЛИЧЕСКИЕ МИНЕРАЛЫ

Наждак и корунд.

Абразивы необходимы и важны в промышленности. Пожалуй, главными в группе природных абразивов являются наждак и корунд, которые превосходят по твердости другие абразивы, такие как кварц, триполи, гранат и пемза. Они используются при шлифовке и полировке металлов — главным образом железа и стали — и стекла. Промышленно важные месторождения наждака и корунда расположены в Аппалачском регионе Соединенных Штатов, на островах Греческого архипелага (особенно Наксос), в Малой Азии, Индии, на Мадагаскаре и в Южной Африке. Контроль над ними практически отсутствует, за исключением того, что присуще государственному суверенитету.

Магнезит.

Магнезит — минерал определенной значимости, используемый главным образом в металлургических операциях и в качестве огнеупорного материала для футеровки печей; также для производства цемента для напольных покрытий. Магнезит не является редким минералом, и месторождения широко распространены. Продуктивные и коммерческие месторождения расположены в Соединенных Штатах (Калифорния и Вашингтон), Канаде, Мексике (Нижняя Калифорния), Венесуэле, Австрии, Германии, Испании, Греции и других странах. Не будучи достаточно редким, чтобы стать объектом крупных объединений, интересной международной особенностью торговли является та, что сосредоточена в Соединенных Штатах. До недавнего времени крупные месторождения магнезита в Соединенных Штатах не были известны, но за последние несколько лет были разработаны обширные месторождения в Калифорнии и Орегоне. До войны месторождения Австрии в основном использовались потребителями в восточной части Соединенных Штатов, а во время войны в основном использовался канадский магнезит. Американские фирмы владеют значительными долями в месторождениях Австрии и, вероятно, в некоторых месторождениях Канады, Мексики и Венесуэлы.

Графит.

Графит используется для изготовления тиглей для выплавки стали и латуни, для литейных красок, карандашей, крема для обуви, в качестве смазки и т. д. Для тиглей используется только кристаллический графит. Снабжение им для американского потребления было одной из проблем войны. Считается, что из месторождений кристаллического графита месторождения французской колонии Мадагаскар благодаря своей богатству — если конкуренция будет свободной — вытеснят американские и немецкие месторождения; месторождения Цейлона считаются истощающимися. Аморфный графит, вероятно, будет поступать из Австрии, Мексики и Кореи. Месторождения Соединенных Штатов обширны, но низкого качества.

Слюда.

Слюда является важным минералом, особенно в электротехнических работах. Будучи одним из самых распространенных минералов почти всех горных пород, она становится ценной только тогда, когда встречается в кристаллах или листах большого размера, которые встречаются сравнительно редко, находясь только в определенных пегматитовых жилах. Индия, Канада и Соединенные Штаты производят около 98 процентов листовой слюды в мире. Бразилия, Аргентина и бывшая Германская Восточная Африка становятся важными производителями. Индия обеспечивает 65 процентов общего мирового производства; Соединенные Штаты — только 15 процентов. Ожидается, что бразильская слюда будет иметь гораздо большее значение в будущем, чем в прошлом, хотя Индия, несомненно, сохранит свое положение как наиболее важный производитель.

Британская империя контролирует 75 процентов производства листовой слюды. До войны Германия получила значительную степень коммерческого контроля над индийскими рудниками и благодаря своему доминирующему положению в электротехнической промышленности угрожала установлением контроля над мировым рынком слюды. Соединенные Штаты в настоящее время являются крупнейшим потребителем; но поскольку значительное развитие электротехнической промышленности в Англии во время войны поставило ее в положение, ранее занимаемое Германией и Австрией, ей требуется большее количество слюды из Индии, и это может привести к постоянному британскому контролю. Лондон является распределительным центром для индийской слюды, и лондонские цены регулируют рынок. Во время войны индийская слюда контролировалась британским правительством и распределялась между союзными странами по фиксированным ценам. Постоянная британская монополия на рынке слюды, вероятно, лучше всего может быть предотвращена развитием бразильского месторождения американскими электротехническими компаниями.

Асбест.

Асбест является важным минералом благодаря своей негорючести и изоляционным качествам, а также волокнистой структуре, которая позволяет прясть или ткать из него веревки и ткани; по этой причине он имеет широкое и разнообразное применение. Минералогически существует три вида асбеста — хризотил, крокидолит и антофиллит, причем последний, как правило, не пригоден для прядения. Хризотил является наиболее ценным в коммерческом отношении: крокидолит, или голубой асбест, не выдерживает высоких температур, как другие разновидности, и из-за своей низкой температуры плавления полезен для электросварки. Поэтому основная проблема асбеста сосредоточена вокруг месторождений высококачественного хризотила, тем более что запасы антофиллитового асбеста обильны и, учитывая его ограниченное применение, достаточны на неопределенный период. Наиболее важные месторождения хризотил-асбеста находятся в Квебеке, Канада, но крупные месторождения также разрабатываются в России и Родезии.

Соединенные Штаты являются, безусловно, крупнейшим производителем асбестовых изделий в мире, но производят лишь малую часть необходимых материалов. Однако наличие месторождений в Канаде обеспечивает американскую промышленность достаточным снабжением. Британские компании обладают исключительным контролем над добычей в Южной Африке, Австралазии и Италии: из них Южная Африка включает родезийские месторождения хризотила, которые являются одними из самых важных в мире. В целом Британская империя занимает доминирующее положение, контролируя около 88 процентов ежегодной добычи асбеста в мире и примерно 70 процентов оценочных запасов. Канада лидирует среди всех стран, обеспечивая около 85 процентов мирового производства. Если британская политика в отношении других минеральных отраслей будет осуществлена в случае с асбестом, мы можем ожидать действий со стороны британского или канадского правительства по переносу центра производства асбеста из Соединенных Штатов в Канаду или Англию.

МИНЕРАЛЫ ДЛЯ УДОБРЕНИЙ

Выше мы затронули четыре большие группы минералов — топливные минералы, минералы для производства стали и ферросплавов, основные цветные минералы и неметаллические минералы. Далее следует отдельная группа — минералы для удобрений или элементарные вещества, главными среди которых являются фосфориты, калий, нитраты, а также сера и серная кислота. Все они представляются необходимыми для восстановления почвы по мере изъятия последовательных урожаев, и, таким образом, для обеспечения постоянства ее первоначальной продуктивности.

Фосфориты.

Фосфориты — это природное вещество, которое используется главным образом в качестве ингредиента удобрений, будучи мелко измельченным и используемым непосредственно. Большие количества также используются для производства фосфорной кислоты и фосфора, последний из которых используется в спичках и т. д. Фосфориты представляют собой пластовое или осадочное месторождение, содержащее фосфат извести; фосфат извести также встречается в виде конкреций в руслах рек. Другой тип месторождения, обычно классифицируемый как фосфориты, представляет собой пористый коралловый или известняковый материал тропических островов, пропитанный фосфатом, выщелоченным из гуано. Месторождения фосфоритов, имеющие в настоящее время коммерческое значение, расположены в Соединенных Штатах, Алжире, Тунисе и Египте, причем Соединенные Штаты обладают, безусловно, самыми большими запасами. Соединенные Штаты также имеют крупнейшую добывающую промышленность. Политически основные месторождения контролируются Соединенными Штатами, Францией (Тунис и Алжир) и Великобританией (Египет). Коммерческий контроль над месторождениями Соединенных Штатов находится в основном в руках американцев, хотя немецкие и французские интересы владеют некоторыми месторождениями твердых пород. Месторождения Алжира и Туниса контролируются двумя компаниями, одной британской и другой итальянской. Германия останется без источника снабжения под своим собственным контролем теперь, когда ее колонии были конфискованы.

Из вышесказанного видно, что нет никакой вероятности мирового контроля или монополии на фосфаты. Соединенные Штаты находятся в положении, позволяющем диктовать условия на рынке, если только в различных странах не будет принято националистическое законодательство для защиты и развития их собственных отраслей.

Калий.

Калий является важнейшим удобрением, более 90 процентов всего используемого калия применяется именно так, остальная часть идет на производство взрывчатых веществ и стекла, а также в химическую промышленность.

До 1914 года практически весь мировой запас калия поступал из великих природных месторождений каменной соли в Штасфурте, Германия. Вторыми по значимости являются месторождения Эльзаса, содержащие достаточное количество для удовлетворения текущих мировых потребностей в течение 300 лет. Крупные неразработанные месторождения существуют в северо-восточной Испании. Германия активно и практически использовала свое природное калийное богатство, создав государственную монополию, которая снабжала весь мир. Это преимущество широко использовалось в ее планах дальнейшего политического и коммерческого завоевания, а также в трудах тщеславных тевтонцев. Они открыто хвастались, что в калии у них есть всемогущее коммерческое оружие, которое заставит другие нации поставлять в обмен такое сырье, в котором нуждалась Германия, например, хлопок и медь из Соединенных Штатов. Однако с ее политическим крахом исчезла и ее коммерческая калийная монополия. Обширные месторождения эльзасского калия отошли к Франции, и хотя немецкий калий, возможно, все еще может производиться и продаваться дешевле, эльзасские месторождения будут служить сдерживающим фактором. Коммерческое объединение между ними, включающее испанские месторождения, однако, отнюдь не исключено. Калий является одним из самых распространенных элементов на земле, и в Соединенных Штатах имеются обильные запасы, но они в основном находятся в форме силикатов, поэтому их труднее и дороже извлекать, чем из растворимых природных солей Германии.

Нитраты.

Нитраты необходимы в чрезвычайной степени, различными способами: в качестве удобрения, и поэтому необходимы для продовольствия и жизни; как источник аммиака, и поэтому необходимы для современной системы охлаждения продуктов питания; как важный ингредиент взрывчатых веществ, и, таким образом, незаменимы для национальной обороны. Точно так же, как калий является одним из самых распространенных элементов земли, азот является одним из самых распространенных элементов воздуха, в котором он составляет четыре пятых. Поэтому его не должно быть трудно получить; но выделить его и уловить в пригодной для использования форме — в технических терминах, «связать» его — трудно, медленно и дорого. Природа не сделала многого для «связывания» азота в своих минеральных запасах; и хотя он постоянно «связывается» в животных и растительных организмах, он в значительной степени вскоре возвращается в атмосферу в виде аммиака или в других формах, или, будучи в форме растворимых солей, выщелачивается из почвы и уносится, чтобы либо снова превратиться в атмосферу, либо, редко, накапливаться в засушливых условиях путем испарения в минеральные отложения. По какой-то до сих пор не объясненной причине только в Чили таким образом образовались минеральные месторождения, имеющие значение; и чилийские месторождения до недавнего времени снабжали весь мир, давая Чили даже гораздо более исключительное положение в отношении нитратов, чем то, которое занимала Германия в отношении калия; но никогда не было никакого монопольного контроля над чилийскими запасами нитратов. Помимо этого минерального источника и получения азота из воздуха путем фиксации, важные источники азотных удобрений содержатся в органических веществах — отходах растительных или животных остатков или экскрементах животных, — а также в угле, как побочном продукте производства кокса.

До войны Германия предвидела лишение чилийских нитратов путем развития процессов фиксации и побочных продуктов, с помощью которых она снабжала себя во время войны. Другие страны не были столь основательны. Во время войны опасность того, что Соединенные Штаты будут отрезаны от поставок чилийских нитратов в результате немецкой подводной кампании, привела к тому, что правительство спроектировало и начало строительство четырех крупных и дорогостоящих заводов по фиксации азота. Они были не закончены, когда война закончилась.

Около пяти восьмых или менее потребляемого азота поступало из различных органических источников, включая побочное производство при коксовании. Побочный азот в Соединенных Штатах оценивается примерно в одну восьмую от общего объема поставок. Оставшиеся три восьмых в значительной степени обеспечивались чилийскими нитратами.

ДРАГОЦЕННЫЕ МЕТАЛЛЫ

Золото.

В группе драгоценных металлов золото имеет наибольшее значение, главным образом как освященная временем и незаменимая мера стоимости и средство обмена. Это положение оно иногда разделяло с серебром, но ни одна страна никогда не отказывалась признавать золото таким образом.

Золото встречается по всему миру, но Британская империя производит 60 процентов его, в то время как Соединенные Штаты производят 20 процентов. Политический и коммерческий контроль почти идентичны в случае с золотом, которое легко восстанавливается до металлического состояния и с тех пор находится в обращении, не требуя сбытовых агентств. Благодаря торговле, вызванной войной, Соединенные Штаты в настоящее время имеют больший золотой запас, чем любая другая страна.

Серебро.

«Серебро», — говорит наш автор, — «используется как для денег, так и в искусстве, причем первое использование является более важным и более существенным. В некоторых странах, особенно в тех, которые производят серебро в больших количествах, оно является денежным стандартом, либо само по себе, либо вместе с золотом. В других странах, находящихся на золотом стандарте, серебро используется для разменной монеты. В Индии и Китае оно используется для расчетов по балансам внешней торговли».

В странах со сложными финансовыми системами, где бумажная валюта свободно принимается, как в Соединенных Штатах и Европе, оно не является таким важным денежным металлом; но в других странах оно напрямую заменяет и сберегает золото. По этой причине серебро не является предметом роскоши, а является предметом первой необходимости. Чеканка серебра увеличилась в Европе по мере продолжения войны и была необходима для доставки припасов с Дальнего Востока на фронты. В то время как нормальная ежегодная добыча серебра составляет около 159 000 000 унций, спрос в 1918 году превысил 500 000 000 унций. Добыча серебра увеличивает запас денег, повышает доверие к финансовым условиям и обеспечивает, вместе с золотом и в качестве дополнения к нему, основу для кредита. Около половины мирового объема добычи серебра является побочным продуктом добычи других металлов, в частности свинца и меди; и, соответственно, добыча серебра в значительной степени не зависит от цены.

Из общего мирового объема добычи серебра более 80 процентов поступает с рудников Западного полушария. В течение многих лет Мексика была ведущим производителем, пока все ее отрасли не были дезорганизованы революцией. Соединенные Штаты, всегда занимавшие второе место, сейчас находятся на лидирующей позиции. Канада, Центральная Америка и Южная Америка являются важными производителями. В Восточном полушарии Австралия является ведущим производителем.

Основные месторождения серебра в мире политически контролируются Соединенными Штатами, Мексикой и Великобританией, причем эти три страны контролировали 85 процентов общего объема добычи в 1913 году.

Платина.

Платина контролируется главным образом Россией, в остальном добываясь в значительных количествах только в Колумбии. Американские интересы преобладают в Колумбии. До войны существовало переплетение интересов платиноперерабатывающих предприятий Соединенных Штатов, Германии и Великобритании, причем немецкое влияние было очень заметным.

Рис. 23. — Контроль в соответствии с политическим суверенитетом (территориальной принадлежностью) над мировым производством минералов. (Напротив страницы 540)

ПОЛИТИЧЕСКИЙ КОНТРОЛЬ (ТЕРРИТОРИАЛЬНЫЙ)

ЖЕЛЕЗО 1913 191 978 750 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 37% БРИТАНСКАЯ ИМПЕРИЯ 11% ФРАНЦИЯ 14% ЛОТАРИНГИЯ 10% ОСТАЛЬНАЯ ГЕРМАНИЯ 6% АВСТРО-ВЕНГРИЯ 3% ИСПАНИЯ 6% РОССИЯ 5% ВСЕ ОСТАЛЬНЫЕ 6%

УГОЛЬ 1913 1 478 000 000 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 39% БРИТАНСКАЯ ИМПЕРИЯ 26% ФРАНЦИЯ 3% ГЕРМАНИЯ 21% АВСТРО-ВЕНГРИЯ 4% ВСЕ ОСТАЛЬНЫЕ 7%

PETROLEUM 1917
502,980,600 Barrels
UNITED STATES 67% BRIT. EMP. 2% RUSSIA 14% MEXICO 11% ALL OTHERS 6%

COPPER 1917
1,604,472 Short Tons
UNITED STATES 60% BRIT. EMP. 8% JAPAN 8% CHILE 5% CENTRAL POWERS 3% ALL OTHERS 13%

ZINC 1913
1,095,686 Short Tons
UNITED STATES 32% BRITISH EMPIRE 6% FRANCE 7% BELGIUM 30% GERMANY 28% ALL OTHERS 7%

СВИНЕЦ В СЛИТКАХ [191] 1 371 900 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 45% БРИТАНСКАЯ ИМПЕРИЯ 13% ФРАНЦИЯ 2% ИСПАНИЯ 11% ГЕРМАНИЯ 14% АВСТРО-ВЕНГРИЯ 2% ВСЕ ОСТАЛЬНЫЕ 13%

GOLD 1917
425,486,400 Dollars
UNITED STATES 19% BRITISH EMPIRE 64% RUSSIA 4% JAPAN 2% ALL OTHERS 11%

SILVER 1913
223,127,000 Ounces
UNITED STATES 30% BRITISH EMPIRE 23% CENTRAL POWERS 3% MEXICO 32% ALL OTHERS 12%

NICKEL 1913
32,016 Short Tons
BRITISH EMPIRE 85% FRANCE 11% HUNGARY 2% ALL OTHERS 2%

ГРАФИТ 1913 139 283 коротких тонн БРИТАНСКАЯ ИМПЕРИЯ 22% ФРАНЦИЯ 6% ИТАЛИЯ 9% ГЕРМАНИЯ 9% АВСТРО-ВЕНГРИЯ 39% ЯПОНИЯ 8% ВСЕ ОСТАЛЬНЫЕ 4%

MERCURY 1913
4,725 Short Tons
UNITED STATES 16% ITALY 23% SPAIN 33% AUSTRIA-HUNGARY 21% ALL OTHERS 5%

TIN 1917
137,199 Short Tons
BRITISH EMPIRE 50% NETHERLANDS 14% BOLIVIA 21% CHINA 8% ALL OTHERS 9%

MANGANESE 1913
2,607,483 Short Tons
BRITISH EMPIRE 35% RUSSIA 55% BRAZIL 5% ALL OTHERS 5%

POTASH 1913
1,247,992 Short Tons
GERMANY (STASSFURT) 93% GERMANY ALSACE 5% ALL OTHERS 2%

ВОЛЬФРАМ 1917 26 783 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 17% БРИТАНСКАЯ ИМПЕРИЯ 34% ЦЕНТРАЛЬНЫЕ ДЕРЖАВЫ 1% ЯПОНИЯ 7% БОЛИВИЯ 16% КИТАЙ 6% ВСЕ ОСТАЛЬНЫЕ 19%

PLATINUM 1913
267,233 Troy Ounces
RUSSIA 93% COLOMBIA 6% ALL OTHERS 1%

SULPHUR 1916
1,100,000 Short Tons
UNITED STATES 65% ITALY 23% JAPAN 10% ALL OTHERS 2%

ASBESTOS 1913
158,016 Short Tons
BRITISH EMPIRE 87% RUSSIA 12% ALL OTHERS 1%

Prepared by: John E. Orchard,
Assistant Mine Economist,
U.S. Bureau of Mines, May 1, 1919

[191] Недавние

Рис. 24. Контроль в соответствии с коммерческой или финансовой собственностью над мировым производством минералов. (Вставка после рис. 23)

КОММЕРЧЕСКИЙ КОНТРОЛЬ (ФИНАНСОВЫЙ) (Проценты являются оценочными)

ЖЕЛЕЗО 1913 191 978 750 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 37% БРИТАНСКАЯ ИМПЕРИЯ 12% ФРАНЦИЯ 11% ГЕРМАНИЯ 27% АВСТРО-ВЕНГРИЯ 3% ВСЕ ОСТАЛЬНЫЕ 10%

УГОЛЬ 1913 1 478 000 000 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 35% БРИТАНСКАЯ ИМПЕРИЯ 24% ФРАНЦИЯ 3% ГЕРМАНИЯ 21% АВСТРО-ВЕНГРИЯ 4% ВСЕ ОСТАЛЬНЫЕ 13%

PETROLEUM 1917
502,980,600 Barrels
UNITED STATES 72% BRITISH EMPIRE 9% NETHERLANDS 75% GERMANY 2% ALL OTHERS 10%

COPPER 1917
1,604,472 Short Tons
UNITED STATES 69% BRITISH EMPIRE 13% FRANCE 2% GERMANY 6% ALL OTHERS 10%

ZINC 1913
1,098,686 Short Tons
UNITED STATES 32% BRIT. EMP. 6% FRANCE 12% BELGIUM 10% GERMANY 34% ALL OTHERS 6%

PIG LEAD[192] 1,371,900 Short Tons
UNITED STATES 49% BRITISH EMPIRE 17% FRANCE 13% GERMANY 15% ALL OTHERS 6%

GOLD 1917
425,486,400 Dollars
UNITED STATES 23% BRITISH EMPIRE 63% FRANCE 6% CENTL. POWERS 1% ALL OTHERS 7%

SILVER 1913
223,127,000 Ounces
UNITED STATES 52% BRITISH EMPIRE 33% GERMANY 10% ALL OTHERS 5%

NICKEL 1913
32,016 Short Tons
UNITED STATES 51% BRITISH EMPIRE 39% FRANCE 6% GERMANY 4%

ГРАФИТ 1913 139 283 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 11% БРИТАНСКАЯ ИМПЕРИЯ 25% ФРАНЦИЯ 4% ИТАЛИЯ 7% ГЕРМАНИЯ 10% АВСТРО-ВЕНГРИЯ 36% ВСЕ ОСТАЛЬНЫЕ 7%

РТУТЬ 1913 4 725 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 16% БРИТАНСКАЯ ИМПЕРИЯ 35% ИТАЛИЯ 11% ГЕРМАНИЯ 13% АВСТРО-ВЕНГРИЯ 21% ВСЕ ОСТАЛЬНЫЕ 4%

ОЛОВО 1917 137 199 коротких тонн БРИТАНСКАЯ ИМПЕРИЯ 67% ФРАНЦИЯ 1% ГЕРМАНИЯ 1% НИДЕРЛАНДЫ 14% ЧИЛИ 11% БОЛИВИЯ 7% КИТАЙ 7% ВСЕ ОСТАЛЬНЫЕ 2%

МАРГАНЕЦ 1913 2 607 483 коротких тонн СОЕДИНЕННЫЕ ШТАТЫ 4% БРИТАНСКАЯ ИМПЕРИЯ 31% ФРАНЦИЯ 3% ГЕРМАНИЯ 17% АВСТРО-ВЕНГРИЯ 2% РОССИЯ 36% ВСЕ ОСТАЛЬНЫЕ 7%

POTASH 1913
1,247,982 Short Tons
GERMANY (STASSFURT) 93% GERMANY (ALSACE) 5% ALL OTHERS 2%

TUNGSTEN 1917
26,783 Short Tons
UNITED STATES 35% BRITISH EMPIRE 55% FRANCE 4% GERMANY 1% ALL OTHERS 3%

PLATINUM 1913
267,233 Troy Ounces
UNITED STATES 4% BRITISH EMPIRE 2% FRANCE 74% RUSSIA 15% ALL OTHERS 2%

SULPHUR 1916
1,100,000 Short Tons
UNITED STATES 65% ITALY 23% JAPAN 10% ALL OTHERS 2%

ASBESTOS 1913
158,016 Short Tons
UNITED STATES 24% BRITISH EMPIRE 64% CENTRAL POWERS 10% ALL OTHERS 2%

Prepared by John E. Orchard
Assistant Mine Economist
U.S. Bureau of Mines, May 1, 1919

[192] Недавние

Кому принадлежит Земля?

— Ответ на наш вопрос в заголовке этой главы «Кому принадлежит Земля?» содержится в этих сводках и далее изложен в прилагаемых диаграммах, одна из которых показывает политический (или, скорее, в данном случае, строго территориальный) контроль, а другая — коммерческий контроль, рис. 23 и 24. Исходя из территориального и коммерческого контроля над фундаментальными минералами, представляется, что Земля принадлежит двум великим англосаксонским нациям, Соединенным Штатам и Британской империи: первая — по судьбе и удаче, без политического плана или политики, поскольку такой огромный запас минеральных богатств был найден в великой малонаселенной пустыне Америки, которую она заняла; вторая — благодаря имперской политике Британии, развивавшейся сотни лет из-за необходимости расширения торговли и флага в далекие земли, чтобы заменить скудные ресурсы своих собственных ограниченных островов. Из этих двух Соединенные Штаты скорее лидируют и владеют и контролируют больше мировых минеральных богатств, чем любая другая нация; но Великобритания идет следом.

Однако в наши дни происходят быстрые изменения, и будущее должно быть изучено. Имперская политика экспансии и усиления политического контроля стала традицией и инстинктом Великобритании; она научилась после потери своих американских колоний предоставлять полную автономию своим более разумным колониям, так что она укрепляет свое господство тем самым и настойчиво продолжает свой путь, помещая все больше и больше земли под британский флаг. Богатство и ресурсы Соединенных Штатов настолько превышают их потребности, что внешние проблемы свелись к случайным вопросам самозащиты; и из этого состояния возникла непосредственно вытекающая теория невмешательства в остальной мир. Подобно Китаю, мы объявляем себя в стороне от мира и просто просим оставить нас в покое, в обмен на что мы соглашаемся оставить мир в покое. Наша доктрина Монро в том виде, в каком она возникла, является частью этой теории — мы хотели, чтобы мир оставил в покое всю Америку, но не брали на себя никакой ответственности за Америку в остальном — эгоистичная и односторонняя позиция.

То, как мы цепляемся за эту доктрину, глупо и неэффективно: хотя мы понимали ее только как применимую к военному или политическому посягательству, мы упустили из виду современную фазу коммерческого завоевания. Тем самым мы вызываем подозрение у наших латиноамериканских соседей, которые, соответственно, более охотно приветствуют европейский или японский, а не американский капитал; и таким образом мы поощряем те самые посягательства, которые мы думали предотвратить. Мы должны либо полностью отказаться от доктрины Монро, либо определить ее также в терминах политического контроля.

Поэтому, что касается наших великих отраслей промышленности и, более конкретно, наших минеральных отраслей, у нас никогда не было никакой определенной политики; наши беды и проблемы были чисто внутренними, и усилия правительства были в значительной степени направлены на предотвращение такой солидарности любой одной отрасли, чтобы ее власть не была слишком велика, хотя американский организационный гений первым успешно развил эти колоссальные деловые объединения, возникшие без государственной поддержки. Англия, как и Франция, с их демократическими традициями, стремились сопротивляться подавляющей власти крупных деловых организаций, как ведущей к разрушению равных возможностей и угрожающей власти государства. Оставалось Германии, нагло стремящейся к завоеванию мира, увидеть преимущество объединения сил государства с силами деловых монополий как средства регулирования промышленности внутри страны и подавления других наций. Таким образом, старый вопрос о союзе или отделении Церкви от Государства становится вопросом Бизнеса и Государства.

Успех этого плана немецкого проникновения был наиболее ясно и неприятно доведен до британского сознания, а также до французского и американского восприятия войной, и во время войны Англия взяла под государственный контроль свои минеральные отрасли более определенно и систематически, чем мы. Более того, осознав успех немецкой системы как средства проникновения и как метода против конкурентов, она приняла его, поскольку существует поразительная тенденция ставить свои ключевые отрасли под синдикаты, союзы, картели или тресты, контролируемые непосредственно государством.

Система государственного социализма таким образом занимает место свободы индивидуальной конкуренции. Что касается минеральных отраслей, то почти такие же действия были предприняты Францией. Но в Америке, отбросив все проблемы и полувыученные уроки войны, мы возвращаемся к status quo ante. Если эта разница сохранится, несомненно, что британский контроль над землей — под чем мы подразумеваем ее минералы — в конечном итоге будет преобладать. Что касается нас, мы, возможно, предпочли бы видеть его в руках Великобритании, чем любой другой державы, но не должны ли мы определить наш собственный курс как богатая и густонаселенная нация все более тесного, но бурлящего и еще не организованного земного шара?

Наши государственные деятели, газеты и финансисты провозглашают миру, что мы намерены взять львиную долю мирового судоходства и торговли. Англия ничего не говорит, но ставит свое правительство непосредственно за свои собственные отрасли, в то время как американское правительство все еще держится от них в стороне. Национализм был возрожден в Европе, и особенно в Англии и Франции, в результате борьбы за преобладание над интенсивным немецким националистическим духом, который едва не подчинил себе мир, дрейфующий в сторону интернационализма. Это, возможно, шаг назад, реверсия, но какую позицию должна занять Америка? Британский и французский национализм не должны беспокоить нас так сильно, как японский, еще более интенсивный и целенаправленный, работающий теми же немецкими инструментами (не изобретенными в Германии, а в Америке, но, как и большинство немецких искусств, успешно скопированными и использованными), теперь принятыми Англией и Францией в целях самообороны. Америка также пережила возрождение национализма, вполне необходимое в сложившемся положении дел.

В нынешнем положении Соединенные Штаты в значительной степени преобладают в нефтяной промышленности, имея 71 процент мирового производства в 1917 году; Англия, далеко позади, находится на пути к тому, чтобы обогнать нас гигантскими шагами в рамках своей новой системы. В основных потребностях, таких как уголь и железо, Соединенные Штаты также лидируют. Второе место в сталелитейной промышленности, занимаемое Германией, было предположительно потеряно в результате войны и, вероятно, переходит к Англии, уже занимающей второе место по углю и имеющей свои железорудные отрасли под управлением контролируемого государством синдиката в целях защиты и расширения.

По меди Соединенные Штаты далеко впереди, с Англией на втором месте, и по свинцу также, с половиной мирового производства, с Англией на втором месте. До войны Англия и Германия были примерно равны за второе место, и последняя быстро вырывалась вперед благодаря своим контролируемым государством коммерческим методам; но война сильно отбросит ее назад. По цинку Соединенные Штаты имели наибольшее производство (32 процента) до войны, немного больше, чем Германия (28 процентов), но немецкие методы дали ей преобладание фактического коммерческого контроля. Результат войны восстановит коммерческое превосходство Соединенных Штатов, и значение Англии возрастет. По серебру Соединенные Штаты сейчас лидируют в производстве и как в территориальном, так и в коммерческом контроле, и благодаря своему коммерческому контролю над мексиканской добычей контролируют половину мирового объема, при этом Великобритания является сильным коммерческим вторым номером, имея почти 40 процентов его.

В производстве важного минерала, серы, Соединенные Штаты далеко опережают мир, имея 65 процентов мирового производства в 1916 году. Италия на втором месте, Япония на третьем, а Англия практически не представлена. Фосфориты доминируют, как территориально, так и коммерчески, Соединенными Штатами, но есть другие запасы для Англии, и Франция имеет изобилие на своей собственной территории. Ванадий коммерчески контролируется Соединенными Штатами, хотя территориально — Перу. Молибден совсем недавно стал контролироваться Соединенными Штатами, при этом Великобритания, ранее занимавшая первое место, теперь вторая. По урану и радию Соединенные Штаты также занимают первое место, с Австрией на втором месте. Алюминиевая промышленность наиболее сильна в Соединенных Штатах, хотя очень важна также во Франции.

В следующем, однако, Великобритания имеет контроль: важная «ключевая отрасль» олова, где ее территориальный контроль составляет половину, а коммерческий контроль абсолютен, тогда как Соединенные Штаты не представлены; в важной никелевой промышленности, благодаря территориальному контролю в 80 процентов и коммерческому контролю, который сейчас, вероятно, преобладает над сильными американскими интересами, в результате активной государственной политики; по вольфраму, где она контролирует территориально наибольшую добычу (34 процента) и где она имеет коммерческое превосходство, контролируя 54 процента (1917), Соединенные Штаты на втором месте, с коммерческим контролем в 35 процентов (хотя их территориальный контроль составляет только 17 процентов, примерно равный контролю Боливии).

По марганцу Россия номинально лидирует с 36 процентами коммерческого контроля (55 процентов мирового производства в 1913 году); но при нынешних условиях эффект заключается в том, что Англия получает лидерство, а Соединенные Штаты находятся в положении второстепенной важности. По хрому Великобритания и Франция контролируют через синдикат, в котором британский интерес находится в большинстве, а Соединенные Штаты занимают подчиненное положение по отношению к обеим этим странам. В добыче золота Британская империя контролирует 63 процента; Соединенные Штаты — 23 процента. По графиту в 1913 году Британская империя была второй после Австро-Венгрии. Теперь она займет первое место, а Соединенные Штаты будут конкурентом. По асбесту Британская империя производит 87 процентов и контролирует коммерчески 63 процента от общего мирового объема, Соединенные Штаты незначительны в производстве, но вторые в коммерческом контроле (над канадским асбестом). Ртуть территориально находится в основном в руках Испании, но отрасль фактически доминируется Англией в рамках торговых соглашений. Сурьма долгое время контролировалась Англией, но контроль может вернуться к Китаю, что означает возможность того, что она станет японской. Слюда, необходимая для электротехнических работ, контролируется Великобританией.

Осталось лишь несколько минералов, в которых большая часть промышленности не находится в руках Соединенных Штатов или Англии: калий, ранее бывший немецкой монополией, а теперь разделенный между Германией и Францией, причем Германия, вероятно, преобладает; и минеральные нитраты на чилийской территории, без заметного национального коммерческого контроля, кроме контроля Чили.

И Америка, и Англия крепко держат в своих руках мировые минеральные отрасли — Англия гораздо сильнее, чем до войны, и с вновь поставленной целью расширяться. Объединение этих двух стран означало бы практический мировой контроль над минералами, а вместе с Францией — еще более сильный контроль. Это все на данный момент, но неопределенные величины вырисовываются в судьбе России, будущем Азии и прогрессе Японии. Япония намеренно встала на путь к доминированию в Азии, политически и коммерчески. Ее нынешнее положение не так значительно, как рассмотрение ее быстрого прогресса, знание богатого поля, на котором ей предстоит работать, и изучение ее милитаристских методов, которые напоминают методы Германии. Япония не держится ни за одного союзника, который не будет (временно) помогать ей в ее марше вперед, и в слабости России, Китая и Кореи она видит свою возможность. Война для нее была абсолютным благом. Она не рисковала и захватила огромные преимущества.

Существуют три великие фигуры наций, которые, по-видимому, были предназначены в наше время играть критически важную роль для Соединенных Штатов: в прошлом — Германия, в настоящем — Великобритания, в будущем — Япония. Германский вопрос был решен единственно возможным способом; для Англии единственным разумным решением является более тесный союз, а для Японии — бдительность и дружественные намерения.

УКАЗАТЕЛЬ

Африка

Asbestos in, 394

Bauxite and aluminum in, 350

Chrome in, 114

Copper in, 246

Copper, exports to United States, 249; copper production, 246, 249

Восточная Африка

Mica in, 383

Emery and corundum in, 359

Gold in, 473

Magnesite in, 368

Северная Африка

Copper in, 248

Phosphate in, 405

Южная Африка

Gold in, 473; gold, financial control, 488

Mica in, 384

Tin in, 323

Западная Африка

Copper in, 248

Gold in, 474

Аляска. См. Соединенные Штаты.

Алжир

Antimony in, 185

Iron ores of, 71

Lead in, 273

Phosphate in, 406

Zinc in, 303

Сплавы

сурьмяные, 172; хромовые, 109; марганцевые, 90; молибденовые, 191; никелевые, 129; платиновые и иридиевые, 506; вольфрамовые, 142; ванадиевые, 163; циркониевые, 210

Эльзас. См. Франция и Германия.

Petroleum control in, 16

Potash control in, 418

Алюминий (бокситы)

Changes in practice, 349

Chapter on, 349

Алюминий

Коммерческий контроль над алюминием, 352; во Франции, 353; в Германии и Австрии, 354; в Великобритании, 353; в Италии, 354; в Норвегии, 353; в Гвиане, 353; в Соединенных Штатах и Канаде, 352

Географическое распределение, 350; в Африке, 350; в Австралии, 350; в Китае, 351; в Южной Америке, 350; в Соединенных Штатах, 350; в Европе, 350; в Индии, 350

Summary, 354

Uses of, 349

Works, capacity, 352

World’s output, 351

Сурьма

Alloys of, 172

Chapter on, 172

Географическое распределение, 173, 174, 175; в Африке, 185; в Алжире, 185; в Азии, 182; в Австралии, 186; в Австрии и Венгрии, 179; в Боливии, 178; на Борнео, 182; в Канаде, 177; в Китае, 182, 183; в Европе, 179; во Франции, 179; в Германии, 180; в Великобритании, 180; в Индии, 184; в Индокитае, 184; в Италии, 181; в Японии, 184; в Мексике, 177; в Северной Америке, 176; в Перу, 179; в Португалии, 182; в России, 182; в Сербии, 182; в Южной Африке, 185; в Южной Америке, 178; в Испании, 182; в Турции, 184; в Соединенных Штатах, 176

Положение Англии, 187; положение Франции, 188; положение Германии, 188; положение Японии, 188; положение Соединенных Штатов, 187

Production of world, 186

Recent industrial conditions, 188

Summary, 189

Uses of, 172

World situation, 530

Аргентина

Copper in, 245

Petroleum control in, 16

Асбест

в Африке, 394; в Азии, 394; в Канаде и Ньюфаундленде, 393; в Европе, 393; в Италии, 393; в Мексике, Центральной и Южной Америке, 393; в Соединенных Штатах, 391

Anthophyllite, in United States, 392

Changes in practice, 389

Chapter on, 388

Chrysolite, in United States, 391

Control in Canada, 398; in South Africa, 398; in United States, 397

Control, political and commercial, 397

Future changes, 395

Geographical distribution, 391

Geological distribution, 389

Position of Great Britain, 399; position of the United States, 399

Substitutes for, 389

Summary, 400

Uses of, 388

World situation, 537

Азия

Antimony in, 182

Asbestos in, 394

Chrome in, 115

Coal in, 27

Copper in, 253

Emery and corundum in, 358

Gold in, 471

Graphite in, 374

Iron in, 74-77

Magnesite in, 368

Manganese in, 99

Mercury in, 341

Monazite in, 217

Petroleum in, 9

Phosphate in, 406

Tin in, 319, 323, 327, 329, 330

Tungsten in, 149

Zinc in, 303, 305, 306

Малая Азия

Chrome in, 115

Magnesite in, 368

Mercury in, 341

Австралазия

Asbestos in, 395

Chrome in, 111

Copper in, 249

Gold in, 474

Lead in, 268, 269

Manganese in, 101

Nickel in, 134, 135

Phosphate in, 406

Tin in, 325, 326, 329

Tungsten in, 149

Zinc in, 302, 303

Австралия

Antimony in, 186

Bauxite and aluminum in, 350

Coal position, 31

Copper, production in 1917, 250

Gold in, 475

Gold, political and commercial control, 490

Iron in, 80

Lead in, 268

Lead, commercial control, 282

Lead position, 288

Magnesite in, 368

Manganese in, 101

Mica in, 384

Molybdenum in, 191; molybdenum, commercial control, 197

Platinum in, 514

Radium in, 207

Tin in, 325

Tungsten, future of, 149

Uranium in, 207

Zinc in, 302; commercial control, 311

Австрия

Copper in, 258

Lead position, 290

Magnesite control, 369

Mercury in, 340

Radium resources, 206; uranium resources, 206

Zinc in, 305

Австрийская империя

Chrome in, 118

Mercury in, 340

Австрия и Венгрия

Antimony in, 179

Iron, political and commercial control, 70; iron position, 87

Manganese in, 96

Балканский полуостров

Chrome in, 118

Бокситы

Chapter on, 349

Geographical distribution, 350

Geological distribution, 350

Uses of, 349

World control, 351

Бельгийское Конго

Copper in, 246, 247

Manganese in, 101

Бельгия

Coal in, 24, 26

Iron position, 87

Lead in, 276; lead position, 290

Manganese in, 96

Zinc position, 313

Боливия

Antimony in, 178

Copper in, 245

Lead in, 276

Silver in, 498, 501

Tin in, 328; tin control, 333

Tungsten in, 150

Zinc in, 306

Борнео

Antimony in, 182

Manganese in, 101

Боулз, Оливер

Chapter on Asbestos, 388

Бразилия

Chrome in, 120

Coal position, 31

Gold in, 470, 480

Iron, control, 78

Manganese in, 94

Mica in, 383

Monazite in, 217; monazite, commercial control, 218, 219, 220

Zirconium in, 212, 213; zirconium, political control, 213

Британская империя. См. Великобритания.

Британская Гвиана

Gold in, 480

Petroleum control in, 17

Болгария

Iron in, 77

Lead in, 276

Бирма

Lead in, 274; lead position, 289; lead smelters, 283

Petroleum in, 15

Tungsten, future of, 149

Калифорния

Chrome in, 119

Gold in, 466

Magnesite in, 365

Mercury in, 342

Platinum in, 513

Канада

Aluminum control in, 352

Antimony in, 177

Asbestos in, 393; asbestos control in, 398

Chrome in, 118

Copper, commercial control, 238

Emery and corundum in, 358

Gold in, 468

Iron, commercial control, 73

Lead in, 273; lead position, 289; lead smelters, 283

Magnesite in, 365

Manganese in, 94

Mica in, 382

Molybdenum in, 193; molybdenum, commercial control, 197

Nickel in, 133

Petroleum control in, 16

Phosphate in, 405

Platinum in, 513; platinum ownership, 518

Pyrite in, 452

Zinc in, 306

Капская колония, Африка

Asbestos in, 394

Copper in, 248

Gold in, 473

Центральная Америка

Chrome in, 120

Copper in, 239

Gold in, 469; gold control, 485

Petroleum in, 17

Чили

Coal position, 31

Copper control, 241; copper, commercial control, 242; copper, United States control, 243

Iron, control, 78

Manganese in, 96

Nitrate ores, 423; nitrate, outlook for, 441

Sulphur in, 458

Китай

Antimony in, 182

Coal position, 31, 47

Copper in, 255

Gold in, 473; gold, financial control, 488

Iron position, 88

Lead in, 273

Mica in, 384

Petroleum control in, 17

Silver position, 504

Tin in, 329; tin control, 332

Tungsten, future of, 149

Zinc in, 306

Китай и Маньчжурия

Iron, control of, 74

Хром (хромит)

Alloys of, 109

in Australasia, 111

Chapter on, 109

Chief producing countries, 528

Commercial control of, 111-114; in France, 125, 126; in Great Britain, 124; in the United States, 122, 123, 124

Control, commercial and political, 127

Geographical distribution, 111, 112

Геологическое распределение, 110; в Африке, 114; в Азии, 115; в Малой Азии, 115; в Австрийской империи, 118; на Балканском полуострове, 118; в Бразилии, 120; в Канаде, 118; в Центральной Америке, 120; в Колумбии, 120; на Кубе, 120; в Европе, 118; в Греции, 118; в Индии, 117; в Японии, 117; в Македонии, 118; в Новой Каледонии, 111; в Северной Америке, 118; в Родезии, 114; в России, 117; в Сербии, 118; в Южной Америке, 120; в Турции, 115; в Соединенных Штатах, 119; в Венесуэле, 120

Положение Франции, 125; Германии, 126; Великобритании, 124; ведущих стран, 121; России, 127; Соединенных Штатов, 122

Production of, 113

Uses of, 109

World situation, 528

Уголь

Asia and Australia, statistics for, 53

Changes in practice, 23

Chapter on, 22

Commercial control, 33

Control in Germany, 35; in Great Britain, 36; in the United States, 36, 37

Control, political, 33

Domination by Great Britain and the United States, 525

Europe, statistics for, 1913, 49, 50

Exports, and imports, 1913, 52, 53, 54

Geographical distribution, 25

Geological distribution, 23; in Africa, 26; in Europe, 24; in North America, 24; in South America, 24

Imports, 1913, 52, 53, 54; in the United States, 524

Положение Австралии, 31; Бразилии, 31; Чили, 31; Китая, 31, 47; Франции, 46, 47; Германии, 30, 46; Великобритании, 30, 44; Италии, 47; Японии, 47; России, 47; Южной Америки, 31; Соединенных Штатов, 43; мира, 32

Добыча, 1913 г., 49, 50, 51; добыча основных стран, 26; мировая добыча, 27, 28; будущая добыча, 32

Reserves of world, 28

Situation as effected by World War, 39, 40, 41

South America, statistics for, 1913, 52; trade, probable changes in, 42

Summary of control, 524

United States, statistics for 1913, 49

Uses of, 22

Колумбия

Chrome in, 120

Petroleum control in, 17

Platinum in, 512; platinum ownership, 517

Медь

in Africa, Katanga district, 246, 249

Chapter on, 223

Деловой контроль, 225; географический и финансовый контроль, 224; в Канаде, коммерческий контроль, 238; в Чили, коммерческий контроль, 242; контроль Соединенных Штатов, 243; на Кубе и в Карибском бассейне, коммерческий контроль, 239; в Европе, контроль, 257; контроль, сводка, 531, 532

in Europe, production, 257

Географическое распределение, 227; в Африке, 246; в Аргентине, 245; в Азии, 253; в Австралазии, 249; в Капской колонии, 248; в Чили, 241; в Китае, 255; в Европе, 256; в Германии, 258; в Индии, 256; в Японии, 253; в Корее, 255; в Новом Южном Уэльсе, 252; в Северной Америке, 228; в Северной Африке, 248; в Норвегии, 256; в Перу, 244; в Португалии, 256; в Квинсленде, Австралия, 251; в Родезии, 248; в России, 258; в Южной Америке, 241; в Юго-Западной Африке, 248; в Испании, 256; в Швеции, 256; в Тасмании, 252; в Трансваале, 248; в Соединенных Штатах, 228; в Венесуэле, 245

in Japan, production and exports, 253

in Mexico, commercial control, 239

in Peru, commercial control, 244

Reserve of world, 226

in Russia, production, 259; reserves, 259

Summary of, 260

в Соединенных Штатах, контроль со стороны германских интересов, 232–235; контроль через владение рудниками, 228; контроль через владение плавильными и рафинировочными заводами, 230

in United States, leading financial groups, 228, 229

in United States, ore reserves, 236

in United States, ownership and capacity of refineries, 231

in United States, porphyry copper reserves, 236

United States, shipments from Africa, to, 249

World situation, 531

Корбетт, К. С.

Chapter on Nickel, 129

Корнуолл

Tin in, 327

Корунд и наждак

Chapter on, 356

Uses of, 356

World situation, 535

Коста-Рика

Manganese in, 94

Petroleum control in, 17

Куба и Карибский бассейн

Copper, commercial control, 239

Куба

Chrome in, 120

Iron control in, 71

Manganese in, 94

Nickeliferous iron in, 135

Pyrite in, 452

Кипр

Pyrite in, 451

Чехословакия

Iron ores, 70

Lead in, 272

Даб, Джордж Д.

Chapter on Graphite, 372

Голландская Ост-Индия

Petroleum control in, 14

Tin in, 329

Эддингфилд, Ф. Т.

Chapter on Iron, 55

Египет

Lead in, 275; lead position of, 289

Manganese in, 101

Petroleum control in, 16

Phosphate rock in, 406

Zinc in, 306

Наждак и корунд

Chapter on, 356

Control, commercial, 360; control, political, 360

Future developments, 359

Geographical distribution, 357

Геологическое распределение, 357; в Африке, 359; в Азии, 358; в Канаде, 358; в Европе, 358; в Соединенных Штатах, 357

Position of England, 361; of France, 361; of Germany, 361; of Japan, 361; of the United States, 361

Production of, 362

Summary, 361

Uses of, 356

World situation, 535

Англия

См. Великобритания.

Европа

Antimony in, 179

Asbestos in, 393

Bauxite and aluminum in, 350

Chrome in, 118

Coal in, 24-26

Copper in, 256

Copper production and control in, 257

Emery and corundum in, 358

Gold in, 470

Iron in, 57-60

Lead in, 269, 271

Magnesite in, 366

Manganese in, 96

Mercury in, 339

Petroleum in, 8, 9

Phosphate in, 405

Pyrite, exports and imports in, 258

Silver in, 498

Tungsten, future of, 151

Zinc in, 303, 305

Фергюсон, Х. Г.

Chapter on Antimony, 172

Chapter on Graphite, 372

Ferro-Alloy Minerals, 526

Ferromanganese, 90

Fertilizer Minerals, 537

Флорида

Phosphate rock in, 403

Франция

Aluminum control in, 353

Antimony in, 179; antimony position, 188

Chrome position, 125

Coal position, 46; coal control, 36

Copper control in Chile, 243; copper control in Mexico, 240

Emery and corundum position, 361

Gold position, 492

Graphite position, 377

Iron-ore production, 1911-1913, 65; iron, political and commercial control, 64; iron position, 86

Lead in, 274; lead position, 290; lead smelters, 283

Manganese in, 96; manganese position in, 107

Mica, position of, 386

Molybdenum position, 198

Nickel position, 141

Petroleum position, 19

Phosphate rock in, 405

Pyrite in, 450

Tin position of, 335

Tungsten, control of, 156

Zinc, commercial control, 313

Fuel Minerals, 522

Гейл, Хойт С.

Chapter on Potash, 411

Галиция

Petroleum control in, 15

German Austria, lead in, 272

Германия

Antimony in, 180; antimony position of, 188

Chrome position, 126

Coal control, 35; coal position, 30, 46

Copper in, 258; copper control in Australasia, 250; in Chile, 243; in Mexico, 240

Emery and corundum position, 361

Gold position, 492

Graphite position, 377

Iron position, 84; iron, political and commercial control, 63

Lead in, 270, 271; lead position, 289

Magnesite in, 367

Manganese in, 96; manganese position, 107

Mercury in, 340

Mica position, 387

Molybdenum position, 198

Nickel position, 141

Petroleum control in, 518

Potash in, 412; potash control in, 417

Radium in, 207

Tin position of, 335

Tungsten control, 159

Uranium in, 207

Zinc in, 301; zinc, commercial control, 311; zinc, position of, 313

Германия, Австрия и Венгрия

Pyrite in, 450

Гилберт, Честер Г.

Chapter on Nitrogen, 421

Золото

Australia, control of, 490

Chapter on, 462

Коммерческий контроль, 477; контроль в Центральной и Южной Америке, 485; в Китае, 488; в Индии, 487; в Японии, 487; в Сибири, 486; в Сибири и России, 485; в Южной Африке, 488; в Соединенных Штатах и Канаде, 479; политический и коммерческий контроль, 478; политический контроль, 476; финансовый контроль в мире, 480–483; будущие изменения в распределении, 476

Географическое распространение, 464; в Азии, 471; в Австралазии, 474; в Австралии, 475; в Центральной Америке, 469; в Китае, 473; в Европе, 470; в Индии, 471; в Японии, 472; в Корее, 472; в Мексике, 469; в Новой Зеландии, 475; в Северной Америке, 464; в Родезии, 474; в Сибири, 471; в Южной Африке, 473; в Южной Америке, 469; в Соединенных Штатах, 464; в Западной Африке, 474

Geological occurrences, 463; in Mexico, financial control, 484; in Transvaal, financial control, 488, 489

Положение Франции, 492; Германии, 492; Великобритании, 491; Японии, 492; России, 492; Соединенных Штатов, 491

Production in world, 480-483; production of world 1880-1917, 465, 466

Rhodesia, financial control, 489

Summary, 493

Uses of, 462

World situation, 540

Графит

Chapter on, 372

Control, political and commercial, 375; future developments, 374

Geographical distribution, 373

Geological occurrence, 373; in Madagascar, control, 375

Position of England, 377; of France, 377; of Germany, 377; of Japan, 377; of the United States, 376

Production of, 378; production, world capacity, 373

Summary, 377

Uses of, 372

World situation, 536

Великобритания

Aluminum control in, 353

Antimony in, 180; antimony position, 187

Asbestos position, 399

Chrome position, 124

Coal control, 36; coal position, 30, 44, 525

Control of minerals, 542

Copper control in Mexico, 240

Emery and corundum, position, 361

Gold position, 491

Graphite position, 377

Iron, political and commercial control, 66; iron-ore production, 66; iron position, 85

Lead in, 272; lead position, 288, 289; lead smelters, 283

Manganese in, 97; manganese position, 106

Mica position, 386

Molybdenum position, 198

Nickel position, 141

Petroleum interests in Mexico, 14; petroleum policy, 523; petroleum position, 18

Radium resources, 207

Silver market control, 503

Sulphur in, 458

Tin in, 319; tin control, 332; tin position, 335

Tungsten, control of, 154

Uranium resources, 207

Zinc in, 305; zinc position, 314

Греция

Chrome in, 118

Emery in, 358

Iron in, 73

Lead in, 273; lead smelters, 283

Magnesite in, 367

Manganese in, 97

Граут, Фрэнк Ф.

Chapter on Coal, 22

Chapter on Graphite, 372

Гвианы

Aluminum control in, 353

Gold in, 470

Холл, Дюран А.

Chapter on Antimony, 172

Chapter on Mica, 380

Ганновер

Petroleum control in, 16

Хардер, Э. К.

Chapter on Chromium, 109

Chapter on Iron, 55

Хесс, Фрэнк Л.

Chapter on Tungsten, 142

Хьюитт, Д. Ф.

Chapter on Manganese, 90

Хилл, Джеймс М.

Chapter on Bauxite and Aluminum, 349

Chapter on Platinum, 506

Chapter on Tin, 317

Голландия

Tin control, 332; tin position, 335

Венгрия

Iron position, 87

Lead in, 276; lead position, 290

Mercury in, 339

Хайдер, Фредерик Б.

Chapter on Lead, 261

Chapter on Zinc, 294

Айдахо

Lead in, 266

Phosphate in, 404

Индия

Bauxite and aluminum in, 350

Chrome in, 117

Copper in, 256

Gold in, 471; gold, financial control, 487

Iron, control of, 75

Manganese in, 99

Mica in, 383

Monazite in, 217; monazite, commercial control, 220

Petroleum control in, 15

Tin in, 327

Zinc in, 306

Zirconium in, 213; zirconium, political control, 214

Индокитай

Coal in, 24

Zinc in, 305

Иридий

Uses of, 506

Железо

Chapter on, 55

Коммерческий контроль, 61; контроль в Австрии и Венгрии, 70; контроль в Индии, 75; контроль в Японии и Корее, 76; контроль на Кубе, 71; контроль во Франции, 64, 65; контроль на Ньюфаундленде, 71; контроль в России, 68, 69; контроль в Соединенных Штатах, 61, 62, 63; политический контроль, 61

Four chief producing countries, 526

Geographical distribution, 57

Геологическое распределение, 55; железо в Австралии, 80; в Бразилии, 78; в Болгарии, 77; в Канаде, 73; в Чили, 78; на Кубе, 71; в Чехословакии, 70; в Греции, 73; в Италии, 72; в Югославии, 71; в Мексике, 79; на Ньюфаундленде, 71; в Новой Зеландии, 80; в Норвегии, 72; в Польше, 77; в Португалии, 77; в Южной Африке, 80; в Тунисе, 71; в Турции, 77

Iron-ore and pig-iron production and movement, 1913, 60

Ore reserves in United States, 61

Pig-iron manufacture, statistics, 59

Положение Австрии, 87; Бельгии, 87; Китая, 88; Франции, 86; Германии, 84; Великобритании, 85; Венгрии, 87; Японии, 88; России, 86; Соединенных Штатов, 82

Production of the world, 1910-1917, 58

Италия

Antimony in, 181

Asbestos in, 393

Coal position, 47

Iron ores of, 72; iron, commercial control, 73

Lead in, 272; lead position, 290; lead smelters, 283

Manganese in, 97

Mercury in, 339

Petroleum control in, 17

Pyrite in, 450

Sulphur in, 453

Zinc in, 303

Япония

Antimony position, 188

Coal position, 47

Chrome in, 117

Copper in, 253, 254; copper production, 254

Emery and corundum position, 361

Gold in, 472; gold, financial control, 487; gold position, 492

Graphite position, 377

Iron control, 76; iron position, 88

Lead in, 275; lead position, 291

Manganese in, 100, 101

Molybdenum position, 198

Petroleum control in, 16; petroleum position of, 20

Pyrite in, 452

Silver position, 499

Sulphur in, 457

Tin in, 330

Tungsten control, 156

Zinc in, 303; zinc position, 314

Ява

Manganese in, 103

Югославия

Iron ores, 71

Район Катанга, Африка

Copper in, 246, 249

Кац, Фрэнк Дж.

Chapter on Emery and Corundum, 356

Корея

Copper in, 255

Gold in, 472; gold, financial control, 487

Свинец

Changes in practice, 262

Chapter on, 261

Control in Australia, 282; in Mexico, 282, 283; in Spain, 282

Control, commercial, 277

Control, commercial, of pig-lead output, 287; in United States, 279

Control, political, 277

Control through trade combinations, 283, 284, 285, 286

Consumption, 1913, 278

Географическое распределение, 264; в Алжире, 273; в Австралии, 268; в Бельгии, 276; в Боливии, 276; в Болгарии, 276; в Бирме, 274; в Канаде, 273; в Китае, 273; в Колорадо, 267; в Чехословакии, 272; в Египте, 275; во Франции, 274; в Германской Австрии, 272; в Германии, 270, 271; в Великобритании, 272; в Греции, 273; в Венгрии, 276; в Айдахо, 266; в Италии, 272; в Японии, 275; в Мексике, 271; в Миссури, 265; в Новом Южном Уэльсе, 268; в Польше, 270; в Перу, 274; в Португалии, 276; в Квинсленде, 269; в Родезии, 276; в России, 275; в Сибири, 275, 283; в Юго-Западной Африке, 273; в Испании, 269; в Швеции, 276; в Тасмании, 269; в Тунисе, 272; в Турции, 273; в Соединенных Штатах, 265; в Верхней Силезии, 270; в Юте, 267; в Западной Австралии, 269

Geological occurrence, 263

Положение Австралии, 288; Австрии, 290; Бельгии, 290; Британской империи, 288; Британских островов, 289; Бирмы, 289; Канады, 289; Египта, 289; Франции, 290; Германии, 289; Венгрии, 290; Японии, 291; Испании, 291; Соединенных Штатов, 287

Lead-silver smelters, Mexico, 282; lead-silver smelters, United States, 281

Production, 1913, 264, 278; production, future changes, 276

Smelted in 1913, 278

Плавильные заводы в Бирме, 283; в Канаде, 283; во Франции, 283; в Великобритании, 283; в Греции, 283; в Италии, 283; в Турции, 283

Summary, 291

United States, financial groups, 281

World situation, 532

Македония

Chrome in, 118

Мадагаскар

Graphite control, 375

Магнезит

Chapter on, 363

Control, political and commercial, 368; control in Austria, 369; control in the United States, 368

Географическое распределение, 364; в Африке, 368; в Азии, 368; в Австралии, 368; в Калифорнии, 365; в Канаде, 365; в Европе, 366; в Германии, 367; в Греции, 367; в Мексике, 366; в Северной Америке, 365; в Южной Америке, 366; в Соединенных Штатах, 365; в Вашингтоне, 366

Geological occurrence, 363

Summary, 370

Uses of, 363

World situation, 536

Малайский полуостров

Tin in, 319; tin production, 1917, 321

Марганец

Changes in practice, 91

Chapter on, 90

Control, commercial, 103; control, political and commercial, 103

Географическое распределение, 93, 104; в Африке, 101; в Азии, 99; в Австралазии, 101; в Австралии, 101; в Австрии и Венгрии, 96; в Бельгийском Конго, 101; в Бельгии, 96; на Борнео, 101; в Бразилии, 94; в Канаде, 94; в Чили, 96; в Коста-Рике, 94; на Кубе, 94; в Египте, 101; в Европе, 96; во Франции, 96; в Германии, 96; на Золотом Берегу Западной Африки, 101; в Великобритании, 97; в Греции, 97; в Индии, 99; в Италии, 97; в Японии, 100; на Яве, 103; в Мексике, 94; в Новой Зеландии, 101; в Северной Америке, 93; в Панаме, 94; на Филиппинских островах, 101; в Португалии, 97; в России, 97, 98; в Южной Африке, 101; в Южной Америке, 94; в Испании, 99; в Швеции, 99; в Тунисе, 101; в Уругвае, 96

Geological distribution, 91, 92

Position of England, 106; of France, 107; of Germany, 107; of the United States, 106

Principal sources of, 527

Production of, 102

Summary, 108

Uses of, 90

World situation, 527

Ртуть

Changes in distribution, 343

Changes in practice, 344

Chapter on, 337

Control, commercial, 346; control, political, 345

Географическое распределение, 339; на Аляске, 341; в Азии, 341; в Малой Азии, 341; в Австрийской империи, 340; в Калифорнии, 342; в Европе, 339; в Германии, 340; в Венгрии, 340; в Италии, 340; в Мексике, 343; в Неваде, 343; в Северной Америке, 341; в Португалии, 340; в России, 341; в Сербии, 341; в Южной Америке, 343; в Техасе, 343

Geological distribution, 338

Summary, 347

Uses of, 337

World situation, 535

Мезоторий

Uses of, 216

World situation, 531

Мексика

Antimony in, 177

Coal in, 28

Copper in, commercial control, 239

Gold in, 469; gold, financial control, 484

Iron, control, 79

Lead in, 271; lead, commercial control, 282, 283

Magnesite in, 366

Manganese in, 94

Mercury in, 343

Molybdenum in, 195; molybdenum, commercial control, 197

Petroleum, commercial control, 14

Pyrite in, 452

Sulphur in, 458

Tungsten, future of, 151

Zinc in, 305

Слюда

Changes in practice, 381

Chapter on, 380

Control, political and commercial, 385

Future developments, 384

Географическое распределение, 383; в Австралии, 384; в Бразилии, 382; в Канаде, 382; в Китае, 384; в Восточной Африке, 382; в Индии, 382; в Южной Африке, 384; в Соединенных Штатах, 382

Geological distribution, 382

Position of Germany, 387; position of Great Britain, 386; of France, 386; of the United States, 386

Substitutes for, 381

Summary, 387

Uses of, 380

World situation, 536

Минералы

World control of, 541

Миссури

Lead in, 265

Zinc in, 298, 300

Молибден

Chapter on, 191

Control, commercial, 197; in Australia, 197; in Canada, 197; in Mexico, 197; in Norway, 197; in United States, 197

Control, political, 196

Географическое распределение, 191, 199; в Австралии, 191; в Канаде, 193; в Мексике, 195; в Северной Америке, 193; в Норвегии, 191; в Соединенных Штатах, 193

Geological distribution, 191

Position of France, 198; of Germany, 198; of Great Britain, 198; of the United States, 198

Reserves, 196

Summary, 200

Treatment of ores, 196

Uses of, 191

World situation, 530

Монацит

Chapter on, 216

Control, commercial, 218, 219, 220, 221

Control, political, 218

Geographical distribution, 216; in Brazil, 217; in India, 217; in the United States, 216

Geological distribution, 216

Position of the United States, 221

Treatment practice, 218

Uses of, 216

Мур, Р. Б.

Chapter on Molybdenum, 191; Chapter on Monazite, Thorium, and Mesothorium, 216; Chapter on Vanadium, 163

Марокко

Iron ores, 71

Phosphate in, 406

Моррис, Х. К.

Chapter on Zirconium, 209

Невада

Mercury in, 343

Новая Каледония

Chrome in, 111

Nickel in, 134; nickel, commercial control, 139

Ньюфаундленд

Iron ores, 71

Новый Южный Уэльс

Copper in, 252

Lead in, 268

Platinum in, 514

Tin in, 326

Zinc in, 302

Новая Зеландия

Gold in, 475

Iron in, 80

Manganese in, 101

Petroleum control, 17

Никель

Alloys, 129

Changes in practice, 130

Chapter on, 129

Commercial control, 138

Control, commercial, in New Caledonia, 139; in Sudbury district, Canada, 138, 139

Control, political, 138

Future of, 136

Garnierite and lateritic type deposits, 134

Geographical distribution, 132; nickel in Canada, 133

Geological distribution, 131; in Norway, 134; in United States, 134

Position of France, 141; of Germany, 141; of Great Britain, 141; of the United States, 141

Production, 136

Sudbury district, Canada, 133

Sulphide type deposits, 133

Veins, 135

World situation, 528

Nickeliferous iron, Cuba, 135

Нигерия

Tin in, 323

Нитраты

By-product, outlook for, 443

Fixation, outlook for, 442

Ore deposits in Chile, 422

Summary, 444, 445

World situation, 539

Азот

Ammonia fixation, 437

Arc fixation, 437

Atmospheric, 421

Bacterial fixation, 439

By-product compounds, 434

Chapter on, 421

Consumption for fertilizers, 435

Control, commercial aspects, 433; general aspects, 425

Cyanamid fixation, 438

Cyanide fixation, 438

Fixation compounds, 437

Geological distribution, 421; in carboniferous deposits, 425

Natural compounds, 434

Nitride fixation, 438

Organic, 424

Outlook for, 440

Production statistics, 426; production, world developments, 428

Recent developments and changes, 439

Sources, 427

United States, developments in, 430

Uses of, 421

Utilization cycles, 427

World situation, 431

Non-ferrous Metals, 531

Non-metallic Minerals, 535

Северная Америка

Antimony in, 176

Chrome in, 118

Coal in, 24, 25

Copper in, 228

Gold in, 464

Iron in, 57, 61, 62, 63

Magnesite in, 365

Manganese in, 93

Mercury in, 341

Molybdenum in, 193

Petroleum in, 5-8

Silver in, 501

Tungsten, future of, 150

Нортроп, Джон Д.

Chapter on Petroleum, 1

Норвегия

Aluminum control in, 353

Copper in, 256

Iron ores, 72

Molybdenum in, 191; molybdenum, commercial control, 197

Nickel in, 134

Pyrite in, 449

Орчард, Джон Э.

Chapter on Gold, 462

Орегон

Platinum in, 513

Осмиридий

in Canada, 513; in Colombia, 512; in the United States, 513

Осмий

Uses of, 506

Пейн, Ф. У.

Chapter on Copper, 223

Chapter on Silver, 495

Палладий

in Canada, 513

in platinum ores, 510

Uses of, 506

Панама

Manganese in, 94

Petroleum control in, 17

Пенроуз, Р. А. Ф.-младший

Chapter on Radium and Uranium, 201

Перу

Antimony in, 179

Copper in, 244

Lead in, 274

Tungsten, future of, 150

Vanadium in, 165

Zinc in, 307

Нефть

Changes in operating and refining practices, 4

Chapter on, 1

Коммерческий контроль, 11, 12; в Эльзасе, 16; в Аргентине, 16; в Британской Гвиане, 17; в Канаде, 16; в Китае, 17; в Колумбии, 17; в Коста-Рике, 17; в Голландской Ост-Индии, 14; в Египте, 16; в Галиции, 15; в Ганновере, 16; в Индии, 15; в Италии, 17; в Японии, 16; в Мексике, 14; в Новой Зеландии, 17; в Панаме, 17; в Персии, 17; на Тринидаде, 16; в Венесуэле, 17; в Соединенных Штатах, 12, 13

Control, political, 9

Future developments, 6

Geographical distribution, 6

Geological distribution, 5

Policy of Great Britain, 523

Position of France, 19; of Germany, 19; of Great Britain, 18; of Japan, 20; of the United States, 17

Production of, 10

Substitutes for, 3

Summary, 20

Summary of control, 522

Uses of, 3

Персия

Petroleum control in, 17

Филиппинские острова

Manganese in, 101

Фосфориты

Changes and developments, 408

Chapter on, 402

Control, commercial, 408

Географическое распространение, 403; фосфаты в Африке, 405; в Алжире, 406; в Азии и Австралазии, 406; в Канаде, 405; в Египте, 406; в Европе, 405; во Флориде, 403; во Франции, 405; в Айдахо, 404; в Марокко, 406; в Сибири, 406; в Южной Америке, 405; в Южной Каролине, 403; в Теннесси, 404; в Тунисе, 405; в Соединенных Штатах, 403; в Юте, 404; в Вайоминге, 404

Geological occurrence, 402

Position of leading nations, 409; of the United States, 409

Summary, 409

United States reserves, 404

Uses of, 402

World situation, 538

Платина

Chapter on, 506

Коммерческий контроль, 517; контроль канадской платины, 518; колумбийской платины, 517; контроль со стороны Германии, 518; со стороны Соединенных Штатов, 519

Control, political, 516

Control through ownership of mines, 517

Control through ownership of reduction plants, 518

Crude analyses of, 509; purity of, 509

Future changes in distribution, 515

Географическое распределение, 507, 510; платина на Аляске, 514; в Австралии, 514; в Калифорнии, 513; в Канаде, 513; в Колумбии, 512; в Новом Южном Уэльсе, 514; в Орегоне, 513; в России, 510; в Испании, 515; в Тасмании, 514; в Соединенных Штатах, 513; в Вашингтоне, 514; в Вайоминге, 514

Geological distribution, 508

Production of world, 1909-1917, 508

Russian control, 516; Russian ownership, 517

Sources of crude, 1909-1917, 511

Summary, 521

Uses of, 506, 507

World situation, 519, 540

Польша

Coal in, 49, 50

Iron in, 77

Lead in, 275

Zinc in, 304

Португалия

Antimony in, 182

Copper in, 256

Iron in, 77

Lead in, 276

Manganese in, 97

Mercury in, 340

Pyrite in, 448

Tin in, 330

Tungsten, future, 151

Поташ

Alsatian control, 418

Changes in commercial practice, 415

Chapter on, 411

Control, commercial and political, 417

Geographical distribution, 412; in Germany, 412; in the United States, 414

Geological distribution, 415

German control, 417

Nature of, 411

Production of world, 1917, 416

Spanish control, 419

Summary, 419

Uses of, 411

World situation, 538

Precious Metals, 540

Пирит и сера

Chapter on, 447

Control, commercial, 460; control, political, 459

in Europe, exports, and imports, 258

Географическое распределение, 448; в Канаде, 452; на Кубе, 452; на Кипре, 451; во Франции, 450; в Германии, Австрии и Венгрии, 450; в Италии, 450; в Японии, 452; в Мексике, 452; в Норвегии и Швеции, 449; в России, 450; в Испании и Португалии, 448; в Соединенных Штатах, 451

Substitutes for, 448

Uses of, 447

Квинсленд (Австралия)

Copper in, 251

Gold in, 475

Lead in, 269

Tin in, 326

Tungsten in, 148

Ртуть

Chapter on, 337

См. Ртуть.

Радий

Chapter on, 201

Future prospects, 208

Geographical and geological distribution, 203; in Australia, 207; in England, 207; in Germany, 207

Ores of, 202

Production, United States, 205

United States resources, 204

Uses of, 201

Рэнсом, Э. Л.

Chapter on Mercury, 337

Родезия (Африка)

Chrome in, 114

Copper in, 248

Gold in, 474; gold, financial control, 489

Lead in, 276

Родий

Uses of, 506

Райс, Джордж С.

Chapter on Coal, 22

Румыния

Petroleum control in, 15

Россия

Antimony in, 182

Chrome in, 117

Chrome position, 127

Coal position, 47

Copper in, 258

Copper production and reserves, 259

Gold control, 485; gold position, 492

Iron ore reserves, 68; iron, political and commercial control, 68

Iron position, 86

Lead in, 275

Manganese in, 97, 98

Mercury in, 341

Petroleum control in, 13

Platinum in, 510; platinum control in, 516; platinum ownership, 517

Pyrite in, 450

Tin position, 335

Zinc position, 315

Рутений

Uses of, 506

Сербия

Antimony in, 182

Chrome in, 118

Mercury in, 341

Сланцевая нефть

Future of, 4

Сиам

Tin control, 333

Tin in, 329

Tungsten in, 148

Сибирь

Gold in, 471

Gold control, 485, 486

Lead in, 275, 283

Mercury in, 341

Phosphate in, 406

Силезия

Lead in, 270

Серебро

By-product, proportion of output, 498

Changes in practice, 500

Chapter on, 495

Chinese and Japanese position, 504

Coinage, 496

Control, by England, 503

Control, commercial, 500

Control, financial, 501

Control, political, 500

Control, territorial, 501

Control through relations to consumers, 503; control through trade combinations, 502

Control through ownership of mines, 500

Control through ownership of reduction plants, 501

Future changes in, 499

Geographical distribution, 498, 499

Geological age of deposits, 497, 499

Production, in world, 498

Rich mines, proportion of output, 498

Summary, 504

Uses of, 495

World situation, 540

Южная Африка

Antimony in, 185

Asbestos, control in, 397

Coal in, 24, 25, 26

Gold, financial control, 488

Gold in, 473

Iron in, 80

Manganese in, 101

Tin in, 324

Zinc in, 306

Южная Америка

Antimony in, 178

Asbestos in, 393

Bauxite and aluminum in, 350

Chrome in, 120

Coal position, 31

Copper control, 241

Gold in, 469; gold control, 485

Magnesite in, 366

Manganese in, 94

Mercury in, 343

Phosphate in, 405

Tungsten, future of, 150

Южная Каролина

Phosphate in, 403

Юго-Западная Африка

Lead in, 273

Испания

Antimony in, 182

Copper in, 256

Iron, political and commercial control, 67

Lead in, 269; commercial control, 282; lead position, 291

Manganese in, 99

Platinum in, 515

Potash in, 419

Pyrite in, 448

Tin in, 330

Tungsten, 148

Zinc in, 304

Spiegeleisen, 90

Спурр, Дж. Э.

Chapter by, 522

Chapter on petroleum, introduction to, 1

Steel and the Ferro-Alloy Minerals, 526

Стокетт, А. У.

Chapter on Potash, 411

Стоун, Р. У.

Chapter on Magnesite, 363

Chapter on Phosphate Rock, 402

Сера

Changes in practice, 459

Географическое распределение, 453; в Чили, 458; в Италии и на Сицилии, 453; в Японии, 457; в Мексике, 458; в Соединенных Штатах, 455

Position of the principal powers, 461; position of the United States, 461

Сера и пирит

Chapter on, 447

Control, commercial, 460

Control, political, 459

Substitutes for, 448

Uses of, 447

Швеция

Copper in, 256

Iron, political and commercial control, 69

Lead in, 276

Manganese in, 99

Pyrite in, 449

Zinc in, 305

Тасмания

Copper in, 252

Lead in, 269

Nickel in, 134

Platinum, in, 514

Tin in, 325

Zinc in, 303

Теннесси

Phosphate in, 404

Техас

Mercury in, 343

Нефть в, см. Соединенные Штаты

Sulphur in, 455

Торий

Chapter on, 216

Uses of, 216

World situation, 531

Олово

Chapter on, 317

Control, commercial, of mines, 333; of smelting, 334

Control, political, 332, 333

Географическое распределение, 319, 320; в Африке, 323; в Австралии, 325; в Австрии, 331; в Бельгийском Конго (Катанга), 331; в Боливии, 328; в Британской империи, 319; в Британской Нигерии, 323; в Китае, 329; в Корнуолле, 327; в Голландской Ост-Индии, 329; в Германии, 331; в Индии, 327; в Италии, 331; в Японии, 330; на Малайском полуострове, 319; в Новом Южном Уэльсе, 326; в Португалии, 330; в Квинсленде, 326; в России, 331; в Сиаме, 329; в Южной Африке, 324; в Юго-Западной Африке, 331; в Испании, 330; в Тасмании, 325; в Соединенных Штатах, 330

Geological distribution, 318

Положение Франции, 335; Германии, 335; Великобритании, 335; Голландии, 335; России, 335; Соединенных Штатов, 335

Мировая добыча, 1913–1918 гг., 321; добывающие районы мира, 320; добыча, будущие изменения, 332; добыча на Малайском полуострове, 322

Uses of, 317

World situation, 534

Трансвааль, Африка

Copper in, 248

Gold, financial control, 489

Тринидад

Petroleum control, 16

Вольфрам

Alloys of, 142

Changes in practice, 143

Chapter on, 142

Коммерческий контроль, 152; британский контроль, 154; французский контроль, 156; германский контроль, 159; японский контроль, 156; контроль Соединенных Штатов, 156, 159

Control, political, 152

Будущее Азии, 149; Австралии, 149; Боливии, 150; Бирмы, 149; Китая, 149; Европы, 151; Мексики, 151; Северной Америки, 150; Перу, 150; Португалии, 151; Южной Америки, 150; Соединенных Штатов, 150

Geographical distribution, 146

Geological distribution, 145

Production, 147, 148, 152

Substitutes for, 142

United States imports, 157

Uses of, 142

World situation, 529

Тунис

Iron ores in, 71

Lead ores in, 272

Manganese in, 101

Phosphate in, 405

Турция

Chrome in, 115

Iron in, 77

Lead in, 273

Соединенные Штаты

Aluminum, control of, 352

Antimony in, 176; antimony position, 187

Asbestos in, 391; asbestos control, 397; asbestos position, 399

Bauxite and aluminum in, 350

Chrome in, 119; chrome position, 122

Coal control, 36, 37, 524; coal position, 43

Control of minerals, 542

Copper, control of, 228

Copper control in Chile, 241-243; in Mexico, 239

Copper in, 228

Copper shipments from Africa, 249

Emery and corundum in, 357, 358; emery and corundum position, 361

Gold in, 464; gold control, 477, 478; gold position, 491

Graphite position, 376

Iron, political and commercial control, 61

Iron-ore reserves, 61; iron position, 82

Свинец в, 265; свинец, коммерческий контроль, 279; свинец, финансовые группы, 281; положение свинца, 287; свинцово-серебряные плавильные заводы, 281

Magnesite in, 365; magnesite control, 368

Manganese position, 106

Mica in, 383; mica position, 386

Molybdenum in, 193; molybdenum, commercial control, 197; molybdenum, position of, 198

Monazite in, 216; monazite, commercial control, 218-221; monazite position, 221

Nickel in, 134; nickel position, 141

Nitrogen developments in, 430, 432

Petroleum position, 17

Phosphate in, 403; phosphate position, 409

Platinum in, 513; control of platinum, 519

Potash in, 414

Pyrite in, 451

Radium resources, 204

Silver in, 498, 501

Sulphur in, 455

Tin in, 330; tin position, 335

Tungsten control, 156, 160; future of tungsten, 150; imports of tungsten, 157; tungsten, proposed tariff, 161

Uranium resources, 204

Vanadium in, 166

Zinc in, 297; zinc, commercial control, 309; zinc position, 313

Zirconium in, 213

Уран

Chapter on, 201

Future prospects, 208

Geographical and geological distribution, 203; in Australia, 207; in England, 207; in Germany, 207

Ores of, 202

Production, Austria, 206; production, Europe, 206; production, United States, 205

United States resources, 204

Uses of, 202

World situation, 531

Уругвай

Manganese in, 96

Ванадий

Alloys of, 163

Changes in practice, 164

Chapter on, 163

Control, commercial, 165, 170

Control, political, 170

Future developments, 170

Географическое распределение, 165, 169; в Аризоне, 166; в Калифорнии, 166; в Колорадо, 166; в Перу, 165; в Соединенных Штатах, 166

Geological distribution, 165

Position of leading nations, 170

Uses of, 163

World situation, 529

Венесуэла

Chrome in, 120

Copper in, 245

Gold in, 470

Petroleum control in, 17

Вашингтон

Magnesite in, 366

Platinum in, 514

Уайт, А. Г.

Chapter on Pyrite and Sulphur, 447

Кому принадлежит Земля?

Chapter by J. E. Spurr, 522; Who owns the earth? 541

World Control of Minerals, 541

Вайоминг

Phosphate in, 404

Platinum in, 514

Цинк

Australia, commercial control, 311

Changes in practice, 295

Chapter on, 294

Control, commercial, 308; in Australia, 311; in France, 313; in Germany, 311; in the United States, 309

Control, political, 308

Deposits of world, 298

Географическое распределение, 297; цинк в Алжире, 303; в Австралии, 302; в Австрии, 305; в Боливии, 306; в Канаде, 306; в Китае, 306; в Египте, 306; во Франции, 304; в Германии, 301; в Великобритании, 305; в Греции, 304; в Индии, 306; в Индокитае, 305; в Италии, 303; в Японии, 303; в Мексике, 305; в Новом Южном Уэльсе, 302; в Перу, 307; в России, 304; в Южной Африке, 306; в Испании, 304; в Швеции, 305; в Тасмании, 303; в Соединенных Штатах, 297

Geological distribution, 296

Germany, commercial control, 311

Industry in 1913, 299

Положение Бельгии, 313; Германии, 313; Великобритании, 314; Японии, 314; России, 315; Соединенных Штатов, 313

Production, 1913, 299; future changes in production, 307

Summary, 315

United States, commercial control, 309

Uses of, 294

World situation, 533

Цирконий

Alloys, 210

Baddeleyite or brazilite, 211

Chapter on, 209

Control of, 213,

Geographical distribution, 211; in Brazil, 212, 213; in India, 213; in the United States, 213

Geological distribution, 211

Production, 215

Refractory uses of, 209

Summary, 215

Uses of, 209

World situation, 531

Zircon, 212

Примечания транскрибатора

В зависимости от используемых для чтения этого текста аппаратных и программных средств и их настроек, не все элементы могут отображаться должным образом. Некоторые таблицы могут быть нечитаемыми на маленьких экранах или в узких окнах. Иллюстрации можно увеличить, открыв их в новой вкладке или окне.

Орфография, использование заглавных букв и дефисов соответствуют исходному документу (включая ошибки и несоответствия в названиях компаний, географических и собственных именах, названиях публикаций и т. д.) и не были исправлены или стандартизированы, за исключением случаев, указанных в разделе «Внесенные изменения» ниже. Результаты расчетов в таблицах приведены в этом тексте так, как они представлены в исходном документе, даже если они, по-видимому, содержат случайные ошибки в расчетах и/или округлении или основаны на неполных или противоречивых данных.

Стр. 50, Таблица 7, строка таблицы «Австрия»: примечание в последнем столбце может больше подходить для строки «Венгрия».

Стр. 278, Сноска [132] «Процент от среднего значения итогов, использованный в a и b»: a и b относятся к столбцам со сносками [130] и [131] соответственно.

Стр. 508 и 510, Таблицы 72 и 74: эти таблицы (почти) идентичны и в исходном документе.

Внесенные изменения

Таблицы и иллюстрации были вынесены из текстовых абзацев; сноски были перенумерованы последовательно и перемещены непосредственно под абзац, в котором на них есть ссылка.

В нескольких таблицах данные были выровнены более последовательно, чем в исходном документе. Многостраничные таблицы из исходного документа были объединены в единые таблицы в этом тексте.

Некоторые очевидные незначительные опечатки и ошибки пунктуации были исправлены без уведомления.

Текст в пунктирной рамке — это текст, который как таковой не встречается в исходном документе, но был транскрибирован с прилагаемой иллюстрации.

Стр. ix: «Платина, автор Джеймс Х. Хилл» изменено на «Платина, автор Джеймс М. Хилл».

Стр. 35: «Dorfmund» изменено на «Dortmund».

Стр. 45: «Alden» изменено на «Aden».

Стр. 50, Таблица 7: Ссылки на стр. 49 (Австрия, Венгрия) заменены на «см. выше», ср. с другими записями.

Стр. 148: в заголовок таблицы вставлен якорь сноски [78].

Стр. 224, Таблица 35: заголовок столбца «Западное полушарие» перемещен в отдельную строку; строка «Итого по Восточному полушарию»: значения 1 113 000, 212 750, 98 000, 31 000 и 125 000 перемещены в строку «Мировой итог».

Стр. 278, Таблица 53: первый столбец «Процент» под заголовком «Первичный свинцовый пигмент, производство плавильных заводов» (значения 0,2, 4,5 и т. д.) считается предназначенным для второго столбца под заголовком «Импорт, извлекаемое содержание свинца в рудах и концентратах».

Стр. 432: «... and the latter in, exhaustibly available ...» изменено на «... and the latter inexhaustibly available ....»

Стр. 509–510: якорь сноски [186] вставлен после обоих вхождений IO₃.